*202*
*68*
*15MB*

*English*
*Pages 564
[573]*
*Year 2014*

Table of contents :

Contents

Preface to the second edition

1.1. Introduction to the properties of tensors

1.2. Representations of crystallographic groups

1.3. Elastic properties

1.4. Thermal expansion

1.5. Magnetic properties

1.6. Classical linear crystal optics

1.7. Nonlinear optical properties

1.8. Transport properties

1.9. Atomic displacement parameters

1.10. Tensors in quasiperiodic structures

1.11. Tensorial properties of local crystal susceptibilities

2.1. Phonons

2.2. Electrons

2.3. Raman scattering

2.4. Brillouin scattering

3.1. Structural phase transitions

3.2. Twinning and domain structures

3.3. Twinning of crystals

3.4. Domain structures

List of terms and symbols used in this volume

Author index

Subject index

Contents

Preface to the second edition

1.1. Introduction to the properties of tensors

1.2. Representations of crystallographic groups

1.3. Elastic properties

1.4. Thermal expansion

1.5. Magnetic properties

1.6. Classical linear crystal optics

1.7. Nonlinear optical properties

1.8. Transport properties

1.9. Atomic displacement parameters

1.10. Tensors in quasiperiodic structures

1.11. Tensorial properties of local crystal susceptibilities

2.1. Phonons

2.2. Electrons

2.3. Raman scattering

2.4. Brillouin scattering

3.1. Structural phase transitions

3.2. Twinning and domain structures

3.3. Twinning of crystals

3.4. Domain structures

List of terms and symbols used in this volume

Author index

Subject index

- Author / Uploaded
- A. Authier (Ed.)

- Similar Topics
- Chemistry
- Physical Chemistry

INTERNATIONAL TABLES FOR CRYSTALLOGRAPHY

Volume D PHYSICAL PROPERTIES OF CRYSTALS

Edited by A. AUTHIER Second Edition

Published for

THE INTERNATIONAL UNION OF C RYSTALLOG RAPHY by

2014

Contributing authors A. Authier: Institut de Mine´ralogie et de Physique des Milieux Condense´s, 4 Place Jussieu, 75005 Paris, France. [1.1, 1.3] P. Bocˇek: Institute of Information Theory and Automation, Academy of Sciences of the Czech Republic, Pod voda´renskou veˇzˇı´ 4, 182 08 Praha 8, Czech Republic. [3.1.6, GI?KoBo-1]

M. Kenzelmann: Paul Scherrer Institute, CH-5232 Villigen PSI, Switzerland. [1.5] A. Kirfel: Steinmann Institut der Universita¨t Bonn, Poppelsdorfer Schloss, Bonn, D-53115, Germany. [1.11] H. Klapper: Mineralogisch-Petrologisches Institut, Universita¨t Bonn, D-53113 Bonn, Germany. [3.2, 3.3]

A. S. Borovik-Romanov†: P. L. Kapitza Institute for Physical Problems, Russian Academy of Sciences, Kosygin Street 2, 119334 Moscow, Russia. [1.5] B. Boulanger: Institut Ne´el CNRS Universite´ Joseph Fourier, 25 rue des Martyrs, BP 166, 38042 Grenoble Cedex 9, France. [1.7] E. Courtens: Laboratoire des Verres, Universite´ Montpellier 2, Case 069, Place Euge`ne Bataillon, 34095 Montpellier Cedex, France. [2.4]

V. Kopsky´: Institute of Physics, Academy of Sciences of the Czech Republic, Na Slovance 2, 182 21 Prague 8, and Department of Physics, Technical University of Liberec, Ha´lkova 6, 461 17 Liberec 1, Czech Republic. [3.1.3, 3.1.6, GI?KoBo-1] W. F. Kuhs: GZG Abt. Kristallographie, Goldschmidtstrasse 1, 37077 Go¨ttingen, Germany. [1.9] H. Ku¨ppers: Institut fu¨r Geowissenshaften, Universita¨t Kiel, Olshausenstrasse 40, D-24098 Kiel, Germany. [1.4]

K. G. Cox†: Department of Earth Sciences, University of Oxford, Parks Roads, Oxford OX1 3PR, England. [1.6]

G. D. Mahan: Department of Physics, 104 Davey Laboratory, Pennsylvania State University, University Park, Pennsylvania, USA. [1.8]

V. E. Dmitrienko: A. V. Shubnikov Institute of Crystallography, Leninsky pr. 59, Moscow 119333, Russia. [1.11] G. Eckold: Institut fu¨r Physikalische Chemie, Universita¨t Go¨ttingen, Tammannstrasse 6, D-37077 Go¨ttingen, Germany. [2.1] M. Ephraı¨m: Advisory Engineering Agency PROMIS, PO Box 854, 1180 AW Amstelveen, The Netherlands. [1.2.7, Tenar]

E. N. Ovchinnikova: Faculty of Physics, M. V. Lomonosov Moscow State University, Leninskie Gory, Moscow 119991, Russia. [1.11] J. Prˇı´vratska´: Department of Mathematics and Didactics of Mathematics, Technical University of Liberec, Ha´lkova 6, 461 17 Liberec 1, Czech Republic. [3.4]

A. M. Glazer: Department of Physics, University of Oxford, Parks Roads, Oxford OX1 3PU, England. [1.6] I. Gregora: Institute of Physics, Academy of Sciences of the Czech Republic, Na Slovance 2, CZ-18221 Prague 8, Czech Republic. [2.3] H. Grimmer: Labor fu¨r Neutronenstreuung, ETH Zurich, Switzerland, and Paul Scherrer Institute, CH-5232 Villigen PSI, Switzerland. [1.5] Th. Hahn: Institut fu¨r Kristallographie, Rheinisch–Westfa¨lische Technische Hochschule, D-52056 Aachen, Germany. [3.2, 3.3] A. Janner: Institute for Theoretical Physics, University of Nijmegen, 6525 ED Nijmegen, The Netherlands. [1.2.7, Tenar]

K. Schwarz: Institut fu¨r Materialchemie, Technische Universita¨t Wien, Getreidemarkt 9/165-TC, A-1060 Vienna, Austria. [2.2] J. F. Scott: Earth Sciences Department, University of Cambridge, Downing Street, Cambridge CB2 3EQ, England. [3.1.5] A. Thiers: AT Computing, Toernooiveld 104, 6525 EC Nijmegen, The Netherlands. [1.2.7, Tenar] J.-C. Tole´dano: Ecole Polytechnique, Route de Saclay, 91128 Palaiseau Cedex, France. [3.1.1, 3.1.2, 3.1.4] R. Vacher: Laboratoire des Verres, Universite´ Montpellier 2, Case 069, Place Euge`ne Bataillon, 34095 Montpellier Cedex, France. [2.4] A. Zarembowitch: Laboratoire de Physique des Milieux Condense´s, Universite´ P. et M. Curie, 75252 Paris Cedex 05, France. [1.3]

V. Janovec: Institute of Physics, Academy of Sciences of the Czech Republic, Na Slovance 2, CZ-18221 Prague 8, Czech Republic. [3.1.3, 3.2, 3.4] T. Janssen: Institute for Theoretical Physics, University of Nijmegen, 6524 ED Nijmegen, The Netherlands. [1.2, 1.10, Tenar]

J. Zyss: Laboratoire de Photonique Quantique et Mole´culaire, Ecole Normale Supe´rieure de Cachan, 61 Avenue du Pre´sident Wilson, 94235 Cachan, France. [1.7]

† Deceased.

v

Contents PAGE

Preface (A. Authier) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

xi

Preface to the second edition (A. Authier) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

xii

PART 1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

3

1.1.1. The matrix of physical properties .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

3

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

5

1.1. Introduction to the properties of tensors (A. Authier)

1.1.2. Basic properties of vector spaces

1.1.3. Mathematical notion of tensor .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

7

1.1.4. Symmetry properties .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

10

1.1.5. Thermodynamic functions and physical property tensors .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

31

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

32

1.2. Representations of crystallographic groups (T. Janssen) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

34

1.2.1. Introduction

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

34

1.2.2. Point groups

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

35

1.2.3. Space groups

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

46

1.2.4. Tensors .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

51

1.1.6. Glossary

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

53

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

56

1.2.7. Introduction to the accompanying software Tenvar (M. Ephraı¨m, T. Janssen, A. Janner and A. Thiers) .. .. .. .. .. ..

62

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

70

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

72

1.3.1. Strain tensor

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

72

1.3.2. Stress tensor

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

76

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

80

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

86

1.2.5. Magnetic symmetry 1.2.6. Tables 1.2.8. Glossary

1.3. Elastic properties (A. Authier and A. Zarembowitch)

1.3.3. Linear elasticity

1.3.4. Propagation of elastic waves in continuous media – dynamic elasticity

.. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

89

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

92

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

95

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

98

1.4. Thermal expansion (H. Ku¨ppers) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

100

1.3.5. Pressure dependence and temperature dependence of the elastic constants 1.3.6. Nonlinear elasticity

1.3.7. Nonlinear dynamic elasticity 1.3.8. Glossary

1.4.1. Definition, symmetry and representation surfaces .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

100

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

101

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

102

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

104

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

105

1.5. Magnetic properties (A. S. Borovik-Romanov, H. Grimmer and M. Kenzelmann) .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

106

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

106

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

110

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

117

1.5.4. Domain structure .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

126

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

128

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

132

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

133

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

139

1.5.9. Magnetostriction .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

145

1.4.2. Gru¨neisen relation

1.4.3. Experimental methods

1.4.4. Relation to crystal structure 1.4.5. Glossary

1.5.1. Introduction

1.5.2. Magnetic symmetry

1.5.3. Phase transitions into a magnetically ordered state 1.5.5. Weakly non-collinear magnetic structures 1.5.6. Reorientation transitions 1.5.7. Piezomagnetism

1.5.8. Magnetoelectric effect

vii

CONTENTS .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

148

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

149

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

153

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

153

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

153

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

155

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

157

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

169

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

175

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

176

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

179

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

181

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

181

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

181

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

186

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

215

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

217

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

219

1.8. Transport properties (G. D. Mahan) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

223

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

223

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

223

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

223

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

227

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

229

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

230

1.9. Atomic displacement parameters (W. F. Kuhs) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

231

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

231

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

231

1.9.3. Site-symmetry restrictions

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

235

1.9.4. Graphical representation

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

235

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

245

1.10. Tensors in quasiperiodic structures (T. Janssen) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

246

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

246

1.10.2. Symmetry .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

248

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

252

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

253

1.10.5. Tables .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

262

1.11. Tensorial properties of local crystal susceptibilities (V. E. Dmitrienko, A. Kirfel and E. N. Ovchinnikova) .. .. .. .. .. .. ..

269

1.11.1. Introduction .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

269

.. .. .. .. .. .. .. .. .. .. .. .. ..

270

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

272

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

274

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

275

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

275

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

281

1.5.10. Connection between Gaussian and SI units 1.5.11. Glossary

1.6. Classical linear crystal optics (A. M. Glazer and K. G. Cox) 1.6.1. Introduction

1.6.2. Generalized optical, electro-optic and magneto-optic effects 1.6.3. Linear optics

1.6.4. Practical observation of crystals 1.6.5. Optical rotation

1.6.6. Linear electro-optic effect

1.6.7. The linear photoelastic effect 1.6.8. Glossary

1.7. Nonlinear optical properties (B. Boulanger and J. Zyss) 1.7.1. Introduction

1.7.2. Origin and symmetry of optical nonlinearities 1.7.3. Propagation phenomena

1.7.4. Determination of basic nonlinear parameters 1.7.5. The main nonlinear crystals 1.7.6. Glossary

1.8.1. Introduction

1.8.2. Macroscopic equations 1.8.3. Electrical resistivity 1.8.4. Thermal conductivity 1.8.5. Seebeck coefficient 1.8.6. Glossary

1.9.1. Introduction

1.9.2. The atomic displacement parameters (ADPs)

1.9.5. Glossary

1.10.1. Quasiperiodic structures

1.10.3. Action of the symmetry group 1.10.4. Tensors

1.11.2. Symmetry restrictions on local tensorial susceptibility and forbidden reflections 1.11.3. Polarization properties and azimuthal dependence

1.11.4. Physical mechanisms for the anisotropy of atomic X-ray susceptibility 1.11.5. Non-resonant magnetic scattering

1.11.6. Resonant atomic factors: multipole expansion 1.11.7. Glossary

viii

CONTENTS

PART 2. SYMMETRY ASPECTS OF EXCITATIONS .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

286

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

286

2.1.2. Fundamentals of lattice dynamics in the harmonic approximation .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

286

2.1. Phonons (G. Eckold) 2.1.1. Introduction

2.1.3. Symmetry of lattice vibrations .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

294

2.1.4. Conclusion .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

311

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

311

2.2. Electrons (K. Schwarz) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

314

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

314

2.2.2. The lattice .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

314

2.2.3. Symmetry operators .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

314

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

315

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

317

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

317

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

318

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

319

2.1.5. Glossary

2.2.1. Introduction

2.2.4. The Bloch theorem

2.2.5. The free-electron (Sommerfeld) model 2.2.6. Space-group symmetry

2.2.7. The k vector and the Brillouin zone 2.2.8. Bloch functions

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

319

2.2.10. Density functional theory .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

320

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

321

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

323

2.2.9. Quantum-mechanical treatment 2.2.11. Band-theory methods

2.2.12. The linearized augmented plane wave method

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

324

2.2.14. Characterization of Bloch states .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

325

2.2.15. Electric field gradient tensor .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

327

2.2.16. Examples .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

330

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

332

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

334

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

334

2.3.2. Inelastic light scattering in crystals – basic notions .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

334

2.3.3. First-order scattering by phonons .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

335

2.3.4. Morphic effects in Raman scattering .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

342

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

345

2.3.6. Higher-order scattering .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

346

2.2.13. The local coordinate system

2.2.17. Conclusion

2.3. Raman scattering (I. Gregora) 2.3.1. Introduction

2.3.5. Spatial-dispersion effects

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

347

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

348

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

349

2.4.1. Introduction

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

349

2.4.2. Elastic waves

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

349

2.3.7. Conclusions 2.3.8. Glossary

2.4. Brillouin scattering (R. Vacher and E. Courtens)

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

350

2.4.4. Brillouin scattering in crystals .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

350

2.4.5. Use of the tables .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

351

2.4.6. Techniques of Brillouin spectroscopy .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

351

2.4.3. Coupling of light with elastic waves

PART 3. SYMMETRY ASPECTS OF PHASE TRANSITIONS, TWINNING AND DOMAIN STRUCTURES .. .. .. .. .. .. .. .. .. .. ..

358

3.1.1. Introduction (J.-C. Tole´dano) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

358

3.1.2. Thermodynamics of structural transitions (J.-C. Tole´dano) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

360

3.1. Structural phase transitions (J.-C. Tole´dano, V. Janovec, V. Kopsky´, J. F. Scott and P. Bocˇek)

.. .. .. ..

370

.. .. .. .. .. .. .. .. .. .. .. .. ..

381

3.1.3. Equitranslational phase transitions. Property tensors at ferroic phase transitions (V. Janovec and V. Kopsky´) 3.1.4. Example of a table for non-equitranslational phase transitions (J.-C. Tole´dano)

ix

CONTENTS 3.1.5. Microscopic aspects of structural phase transitions and soft modes (J. F. Scott) .. .. .. .. .. .. .. .. .. .. .. .. .. ..

381

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

392

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

394

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

397

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

397

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

398

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

399

3.3. Twinning of crystals (Th. Hahn and H. Klapper) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

413

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

413

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

414

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

418

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

419

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

423

3.1.6. Group informatics and tensor calculus (V. Kopsky´ and P. Bocˇek) 3.1.7. Glossary

3.2. Twinning and domain structures (V. Janovec, Th. Hahn and H. Klapper) 3.2.1. Introduction and history

3.2.2. A brief survey of bicrystallography 3.2.3. Mathematical tools

3.3.1. Crystal aggregates and intergrowths

3.3.2. Basic concepts and definitions of twinning

3.3.3. Morphological classification, simple and multiple twinning 3.3.4. Composite symmetry and the twin law

3.3.5. Description of the twin law by black–white symmetry

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

423

3.3.7. Genetic classification of twins .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

436

3.3.8. Lattice aspects of twinning .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

440

3.3.6. Examples of twinned crystals

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

446

3.3.10. Twin boundaries .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

450

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

469

3.3.12. Domain structures (V. Janovec) .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

477

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

477

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

484

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

484

3.4.2. Domain states .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

486

3.4.3. Domain pairs: domain twin laws, distinction of domain states and switching .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

505

3.3.9. Twinning by merohedry and pseudo-merohedry 3.3.11. Effect of twinning in reciprocal space 3.3.13. Glossary

3.4. Domain structures (V. Janovec and J. Prˇ´ıvratska´) 3.4.1. Introduction

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

528

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

539

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

545

Author index

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

549

Subject index

.. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. .. ..

555

3.4.4. Domain twins and domain walls 3.4.5. Glossary

List of terms and symbols used in this volume

x

Preface to the second edition By Andre´ Authier

chapter (Chapter 1.11) deals with the tensor properties of local crystal properties. It considers the impact of symmetry on local physical properties. The symmetry and physical phenomena that allow and restrict forbidden reflections excited at radiation energies close to X-ray absorption edges of atoms are described; reflections caused by magnetic scattering are also discussed. Part 2 is devoted to the symmetry aspects of excitations in reciprocal space: phonons, electrons, Raman scattering and Brillouin scattering. Part 3 deals with the symmetry aspects of structural phase transitions and twinning. Chapter 3.3, Twinning of crystals, has been considerably updated with a large new section on the effect of twinning in reciprocal space, and a section on the relations between twinning and domain structure, the topic of Chapter 3.4, which has also been entirely updated, with new tables and new figures. It is a pleasure to thank all the authors who have updated their contributions and the authors of the new chapter. I am particularly grateful to the Technical Editor, Nicola Ashcroft, who incorporated all the corrections, sometimes quite complicated, to the existing chapters, and who edited the new chapter and the new sections with speed, highly professional efficiency and good humour.

The first edition of Volume D appeared in 2003. This second edition includes a new chapter and eight chapters have been updated, three of them extensively, with entirely new sections included. Volume D deals with the influence of symmetry on the physical and tensor properties of crystals and on their structural phase transitions. It is an up-to-date account of the physical properties of crystals, with many useful tables, aimed at a wide readership in the fields of mineralogy, crystallography, solid-state physics and materials science; it brings together various topics that are usually to be found in quite different handbooks but that have in common their tensor nature and the role of crystallographic symmetry. The overall structure of the volume has remained unchanged. Part 1 introduces the mathematical properties of tensors and group representations, and gives their independent components for each of the crystallographic groups. Several examples of tensor properties are described: elastic properties, thermal expansion, magnetic properties, linear and nonlinear optical properties, transport properties, atomic displacement parameters, and local electric susceptibility. A new section presenting multiferroics, a field which has seen big progress in recent years, has been added to Chapter 1.5 on magnetic properties. A new

xii

International Tables for Crystallography (2013). Vol. D, Chapter 1.1, pp. 3–33.

1.1. Introduction to the properties of tensors By A. Authier

not the case in an anisotropic medium: a sphere cut in an anisotropic medium becomes an ellipsoid when the temperature is varied and thermal expansion can no longer be represented by a single number. It is actually represented by a tensor of rank 2. (ii) Dielectric constant. In an isotropic medium of a perfect dielectric we can write, in SI units,

1.1.1. The matrix of physical properties 1.1.1.1. Notion of extensive and intensive quantities Physical laws express in general the response of a medium to a certain inﬂuence. Most physical properties may therefore be deﬁned by a relation coupling two or more measurable quantities. For instance, the speciﬁc heat characterizes the relation between a variation of temperature and a variation of entropy at a given temperature in a given medium, the dielectric susceptibility the relation between electric ﬁeld and electric polarization, the elastic constants the relation between an applied stress and the resulting strain etc. These relations are between quantities of the same nature: thermal, electrical and mechanical, respectively. But there are also cross effects, for instance: (a) thermal expansion and piezocaloriﬁc effect: mechanical reaction to a thermal impetus or the reverse; (b) pyroelectricity and electrocaloric effect: electrical response to a thermal impetus or the reverse; (c) piezoelectricity and electrostriction: electric response to a mechanical impetus; (d) piezomagnetism and magnetostriction: magnetic response to a mechanical impetus; (e) photoelasticity: birefringence produced by stress; (f) acousto-optic effect: birefringence produced by an acoustic wave; (g) electro-optic effect: birefringence produced by an electric ﬁeld; (h) magneto-optic effect: appearance of a rotatory polarization under the inﬂuence of a magnetic ﬁeld. The physical quantities that are involved in these relations can be divided into two categories: (i) extensive quantities, which are proportional to the volume of matter or to the mass, that is to the number of molecules in the medium, for instance entropy, energy, quantity of electricity etc. One uses frequently speciﬁc extensive parameters, which are given per unit mass or per unit volume, such as the speciﬁc mass, the electric polarization (dipole moment per unit volume) etc. (ii) intensive parameters, quantities whose product with an extensive quantity is homogeneous to an energy. For instance, volume is an extensive quantity; the energy stored by a gas undergoing a change of volume dV under pressure p is p dV. Pressure is therefore the intensive parameter associated with volume. Table 1.1.1.1 gives examples of extensive quantities and of the related intensive parameters.

P ¼ "0 e E D ¼ "0 E þ P ¼ "0 ð1 þ e ÞE ¼ "E; where P is the electric polarization (= dipole moment per unit volume), "0 the permittivity of vacuum, e the dielectric susceptibility, D the electric displacement and " the dielectric constant, also called dielectric permittivity. These expressions indicate that the electric ﬁeld, on the one hand, and polarization and displacement, on the other hand, are linearly related. In the general case of an anisotropic medium, this is no longer true and one must write expressions indicating that the components of the displacement are linearly related to the components of the ﬁeld: 8 < D1 ¼ "11 E1 þ "21 E2 þ "31 E ð1:1:1:1Þ D2 ¼ "21 E1 þ "22 E2 þ "32 E : 3 D ¼ "31 E1 þ "32 E2 þ "33 E: The dielectric constant is now characterized by a set of nine components " ji ; they are the components of a tensor of rank 2. It will be seen in Section 1.1.4.5.2.1 that this tensor is symmetric (" ji ¼ "ij ) and that the number of independent components is equal to six. (iii) Stressed rod (Hooke’s law). If one pulls a rod of length ‘ and cross section A with a force F, its length is increased by a quantity ‘ given by ‘=‘ ¼ ð1=EÞF=A; where E is Young’s modulus, or elastic stiffness (see Section 1.3.3.1). But, at the same time, the radius, r, decreases by r given by r=r ¼ ð=EÞF=A, where is Poisson’s ratio (Section 1.3.3.4.3). It can be seen that a scalar is not sufﬁcient to describe the elastic deformation of a material, even if it is isotropic. The number of independent components depends on the symmetry of the medium and it will be seen that they are the components of a tensor of rank 4. It was precisely to describe the properties of elasticity by a mathematical expression that the notion of a tensor was introduced in physics by W. Voigt in the 19th century (Voigt, 1910) and by L. Brillouin in the ﬁrst half of the 20th century (Brillouin, 1949).

1.1.1.2. Notion of tensor in physics Each of the quantities mentioned in the preceding section is represented by a mathematical expression. Some are direction independent and are represented by scalars: speciﬁc mass, speciﬁc heat, volume, pressure, entropy, temperature, quantity of electricity, electric potential. Others are direction dependent and are represented by vectors: force, electric ﬁeld, electric displacement, the gradient of a scalar quantity. Still others cannot be represented by scalars or vectors and are represented by more complicated mathematical expressions. Magnetic quantities are represented by axial vectors (or pseudovectors), which are a particular kind of tensor (see Section 1.1.4.5.3). A few examples will show the necessity of using tensors in physics and Section 1.1.3 will present elementary mathematical properties of tensors. (i) Thermal expansion. In an isotropic medium, thermal expansion is represented by a single number, a scalar, but this is Copyright © 2013 International Union of Crystallography

Table 1.1.1.1. Extensive quantities and associated intensive parameters The last four lines of the table refer to properties that are time dependent.

3

Extensive quantities

Intensive parameters

Volume Strain Displacement Entropy Quantity of electricity Electric polarization Electric displacement Magnetization Magnetic induction Reaction rate Heat ﬂow Diffusion of matter Electric current

Pressure Stress Force Temperature Electric potential Electric ﬁeld Electric ﬁeld Magnetic ﬁeld Magnetic ﬁeld Chemical potential Temperature gradient Concentration gradient Potential gradient

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES (iv) Expansion in Taylor series of a ﬁeld of vectors. Let us consider a ﬁeld of vectors uðrÞ where r is a position vector. The Taylor expansion of its components is given by i 2 i @u @u j 1 ui ðr þ drÞ ¼ ui ðrÞ þ dx dx j dxk þ . . . þ 2 @u j @u j @uk ð1:1:1:2Þ

temperature and the associated extensive parameters: S strain, P electric polarization, B magnetic induction, entropy, respectively. Matrix equation (1.1.1.4) may then be written: 10 1 0 1 0 T CS CSE CSH CS T S B P C B CT CE CH C CB C B C B P P P P CB E C ð1:1:1:6Þ CB C: B C¼B T @ B A @ CB CBE CBH CB [email protected] H A CT CE CH C

using the so-called Einstein convention, which implies that there is automatically a summation each time the same index appears twice, once as a superscript and once as a subscript. This index is called a dummy index. It will be shown in Section 1.1.3.8 that the nine partial differentials @ui [email protected] j and the 27 partial differentials @2 ui =ð@x j @xk Þ are the components of tensors of rank 2 and 3, respectively.

The various intensive and extensive parameters are represented by scalars, vectors or tensors of higher rank, and each has several components. The terms of matrix (C) are therefore actually submatrices containing all the coefﬁcients Cpq relating all the components of a given extensive parameter to the components of an intensive parameter. The leading diagonal terms, CST , CPE , CBH , C , correspond to the principal physical properties, which are elasticity, dielectric susceptibility, magnetic susceptibility and speciﬁc heat, respectively. The non-diagonal terms are also associated with physical properties, but they relate intensive and extensive parameters whose products do not have the dimension of energy. They may be coupled in pairs symmetrically with respect to the main diagonal: CSE and CPT represent the piezoelectric effect and the converse piezoelectric effect, respectively; CSH and CBT the piezomagnetic effect and the converse piezomagnetic effect; CS and CT thermal expansion and the piezocaloriﬁc effect; CPT and CE the pyroelectric and the electrocaloric effects; CPH and CBE the magnetoelectric effect and the converse magnetoelectric effect; CH and CB the pyromagnetic effect and the magnetocaloriﬁc effect. It is important to note that equation (1.1.1.6) is of a thermodynamic nature and simply provides a general framework. It indicates the possibility for a given physical property to exist, but in no way states that a given material will exhibit it. Curie laws, which will be described in Section 1.1.4.2, show for instance that certain properties such as pyroelectricity or piezoelectricity may only appear in crystals that belong to certain point groups.

Remark. Of the four examples given above, the ﬁrst three (thermal expansion, dielectric constant, stressed rod) are related to physical property tensors (also called material tensors), which are characteristic of the medium and whose components have the same value everywhere in the medium if the latter is homogeneous, while the fourth one (expansion in Taylor series of a ﬁeld of vectors) is related to a ﬁeld tensor whose components vary at every point of the medium. This is the case, for instance, for the strain and for the stress tensors (see Sections 1.3.1 and 1.3.2). 1.1.1.3. The matrix of physical properties Each extensive parameter is in principle a function of all the intensive parameters. For a variation diq of a particular intensive parameter, there will be a variation dep of every extensive parameter. One may therefore write dep ¼ Cpq diq :

ð1:1:1:3Þ

The summation is over all the intensive parameters that have varied. One may use a matrix notation to write the equations relating the variations of each extensive parameter to the variations of all the intensive parameters: ðdeÞ ¼ ðCÞðdiÞ;

ð1:1:1:4Þ 1.1.1.4. Symmetry of the matrix of physical properties

where the intensive and extensive parameters are arranged in column matrices, (di) and (de), respectively. In a similar way, one could write the relations between intensive and extensive parameters as ) dip ¼ Rqp deq ð1:1:1:5Þ ðdiÞ ¼ ðRÞðdeÞ:

If parameter ep varies by dep, the speciﬁc energy varies by du, which is equal to du ¼ ip dep : We have, therefore ip ¼

Matrices (C) and (R) are inverse matrices. Their leading diagonal terms relate an extensive parameter and the associated intensive parameter (their product has the dimensions of energy), e.g. the elastic constants, the dielectric constant, the speciﬁc heat etc. The corresponding physical properties are called principal properties. If one only of the intensive parameters, iq , varies, a variation diq of this parameter is the cause of which the effect is a variation,

@u @ep

and, using (1.1.1.5), Rqp ¼

@ip @2 u ¼ : @eq @ep @eq

Since the energy is a state variable with a perfect differential, one can interchange the order of the differentiations:

dep ¼ Cpq diq

Rqp ¼

(without summation), of each of the extensive parameters. The matrix coefﬁcients Cpq may therefore be considered as partial differentials:

@iq @2 u ¼ : @eq @ep @ep

Cpq ¼ @ep [email protected] :

Since p and q are dummy indices, they may be exchanged and the last term of this equation is equal to Rpq. It follows that

The parameters Cpq that relate causes diq and effects dep represent physical properties and matrix (C) is called the matrix of physical properties. Let us consider the following intensive parameters: T stress, E electric ﬁeld, H magnetic ﬁeld,

Rqp ¼ Rpq : Matrices Rqp and Cpq are therefore symmetric. We may draw two important conclusions from this result:

4

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS x ¼ x0i e0i :

(i) The submatrices associated with the principal properties are symmetric with respect to interchange of the indices related to the causes and to the effects: these properties are represented by symmetric tensors. For instance, the dielectric constant and the elastic constants are represented by symmetric tensors of rank 2 and 4, respectively (see Section 1.1.3.4). (ii) The submatrices associated with terms that are symmetric with respect to the main diagonal of matrices (C) and (R) and that represent cross effects are transpose to one another. For instance, matrix (CSE ) representing the converse piezoelectric effect is the transpose of matrix (CPT ) representing the piezoelectric effect. It will be shown in Section 1.1.3.4 that they are the components of tensors of rank 3.

ð1:1:2:2Þ

If A ji and Bij are the transformation matrices between the bases ei and e0j , the following relations hold between the two bases: ) ei ¼ A ji e0j ; e0j ¼ Bij ei ð1:1:2:3Þ xi ¼ Bij x0j ; x0j ¼ A ji xi (summations over j and i, respectively). The matrices A ji and Bij are inverse matrices: A ji Bkj ¼ ki

ð1:1:2:4Þ

(Kronecker symbol: ki ¼ 0 if i 6¼ k; ¼ 1 if i ¼ k).

1.1.1.5. Onsager relations Important Remark. The behaviour of the basis vectors and of the components of the vectors in a transformation are different. The roles of the matrices A ji and Bij are opposite in each case. The components are said to be contravariant. Everything that transforms like a basis vector is covariant and is characterized by an inferior index. Everything that transforms like a component is contravariant and is characterized by a superior index. The property describing the way a mathematical body transforms under a change of basis is called variance.

Let us now consider systems that are in steady state and not in thermodynamic equilibrium. The intensive and extensive parameters are time dependent and relation (1.1.1.3) can be written Jm ¼ Lmn Xn ; where the intensive parameters Xn are, for instance, a temperature gradient, a concentration gradient, a gradient of electric potential. The corresponding extensive parameters Jm are the heat ﬂow, the diffusion of matter and the current density. The diagonal terms of matrix Lmn correspond to thermal conductivity (Fourier’s law), diffusion coefﬁcients (Fick’s law) and electric conductivity (Ohm’s law), respectively. Non-diagonal terms correspond to cross effects such as the thermoelectric effect, thermal diffusion etc. All the properties corresponding to these examples are represented by tensors of rank 2. The case of second-rank axial tensors where the symmetrical part of the tensors changes sign on time reversal was discussed by Zheludev (1986). The Onsager reciprocity relations (Onsager, 1931a,b)

1.1.2.2. Metric tensor We shall limit ourselves to a Euclidean space for which we have deﬁned the scalar product. The analytical expression of the scalar product of two vectors x ¼ xi ei and y ¼ y j ej is x y ¼ xi ei y j ej : Let us put ei ej ¼ gij :

The nine components gij are called the components of the metric tensor. Its tensor nature will be shown in Section 1.1.3.6.1. Owing to the commutativity of the scalar product, we have

Lmn ¼ Lnm express the symmetry of matrix Lmn . They are justiﬁed by considerations of statistical thermodynamics and are not as obvious as those expressing the symmetry of matrix (Cpq ). For instance, the symmetry of the tensor of rank 2 representing thermal conductivity is associated with the fact that a circulating ﬂow is undetectable. Transport properties are described in Chapter 1.8 of this volume.

gij ¼ ei ej ¼ ej ei ¼ gji : The table of the components gij is therefore symmetrical. One of the deﬁnition properties of the scalar product is that if x y ¼ 0 for all x, then y ¼ 0. This is translated as xi y j gij ¼ 0

[The reader may also refer to Section 1.1.4 of Volume B of International Tables for Crystallography (2008).]

ðgij Þ 6¼ 0:

1.1.2.1. Change of basis Let us consider a vector space spanned by the set of n basis vectors e1, e2 , e3 ; . . . ; en . The decomposition of a vector using this basis is written x ¼ x ei

8xi ¼) y j gij ¼ 0:

In order that only the trivial solution ðy j ¼ 0Þ exists, it is necessary that the determinant constructed from the gij ’s is different from zero:

1.1.2. Basic properties of vector spaces

i

ð1:1:2:5Þ

This important property will be used in Section 1.1.2.4.1. 1.1.2.3. Orthonormal frames of coordinates – rotation matrix An orthonormal coordinate frame is characterized by the fact that

ð1:1:2:1Þ

gij ¼ ij

using the Einstein convention. The interpretation of the position of the indices is given below. For the present, we shall use the simple rules: (i) the index is a subscript when attached to basis vectors; (ii) the index is a superscript when attached to the components. The components are numerical coordinates and are therefore dimensionless numbers. Let us now consider a second basis, e0j . The vector x is independent of the choice of basis and it can be decomposed also in the second basis:

ð¼ 0

if i 6¼ j and ¼ 1 if i ¼ jÞ:

ð1:1:2:6Þ

One deduces from this that the scalar product is written simply as x y ¼ xi y j gij ¼ xi yi : Let us consider a change of basis between two orthonormal systems of coordinates: ei ¼ A ji e0j : Multiplying the two sides of this relation by e0j, it follows that

5

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES ei

e0j

¼

A ji e0k

e0j

¼

A ji g0kj

¼ A ji kj (written correctly),

which span the space En ðj ¼ 1; . . . ; nÞ. This set of n vectors forms a basis since (1.1.2.12) can be written with the aid of (1.1.2.13) as

which can also be written, if one notes that variance is not apparent in an orthonormal frame of coordinates and that the position of indices is therefore not important, as ei

e0j

¼

A ji

x ¼ xj e j :

The xj ’s are the components of x in the basis e j. This basis is called the dual basis. By using (1.1.2.11) and (1.1.2.13), one can show in the same way that

(written incorrectly):

The matrix coefﬁcients, A ji , are the direction cosines of e0j with respect to the ei basis vectors. Similarly, we have

ej ¼ gij e j :

Bij ¼ ei e0j

where

T

A ¼ BT ;

or

indicates transpose. It follows that A ¼ BT and A ¼ B1

so that AT ¼ A1 BT ¼ B1

) )

AT A ¼ I BT B ¼ I:

ð1:1:2:7Þ 1.1.2.4.2. Reciprocal space Let us take the scalar products of a covariant vector ei and a contravariant vector e j :

The matrices A and B are unitary matrices or matrices of rotation and ðAÞ2 ¼ ðBÞ2 ¼ 1 ) ðAÞ ¼ 1:

ei e j ¼ ei g jk ek ¼ ei ek g jk ¼ gik g jk ¼ ji

ð1:1:2:8Þ

[using expressions (1.1.2.5), (1.1.2.11) and (1.1.2.13)]. The relation we obtain, ei e j ¼ ji , is identical to the relations deﬁning the reciprocal lattice in crystallography; the reciprocal basis then is identical to the dual basis ei .

If ðAÞ ¼ 1 the senses of the axes are not changed – proper rotation. If ðAÞ ¼ 1 the senses of the axes are changed – improper rotation. (The right hand is transformed into a left hand.) One can write for the coefﬁcients A ji A ji Bkj ¼ ki ;

ð1:1:2:15Þ

It can be shown that the basis vectors e j transform in a change of basis like the components x j of the physical space. They are therefore contravariant. In a similar way, the components xj of a vector x with respect to the basis e j transform in a change of basis like the basis vectors in direct space, ej ; they are therefore covariant: ) e j ¼ B jk e0k ; e0k ¼ Akj e j ð1:1:2:16Þ xi ¼ A ji x0j ; x0j ¼ Bij xi :

so that A ji ¼ Bij

ð1:1:2:14Þ

A ji Akj ¼ ki ; 1.1.2.4.3. Properties of the metric tensor In a change of basis, following (1.1.2.3) and (1.1.2.5), the gij ’s transform according to 0 gij ¼ Aki Am j gkm ð1:1:2:17Þ g0ij ¼ Bki Bm j gkm :

giving six relations between the nine coefﬁcients A ji . There are thus three independent coefﬁcients of the 3 3 matrix A. 1.1.2.4. Covariant coordinates – dual or reciprocal space 1.1.2.4.1. Covariant coordinates Using the developments (1.1.2.1) and (1.1.2.5), the scalar products of a vector x and of the basis vectors ei can be written xi ¼ x ei ¼ x j ej ei ¼ x j gij :

Let us now consider the scalar products, ei e j , of two contravariant basis vectors. Using (1.1.2.11) and (1.1.2.13), it can be shown that

ð1:1:2:9Þ

ei e j ¼ gij :

The n quantities xi are called covariant components, and we shall see the reason for this a little later. The relations (1.1.2.9) can be considered as a system of equations of which the components x j are the unknowns. One can solve it since ðgij Þ 6¼ 0 (see the end of Section 1.1.2.2). It follows that x j ¼ xi gij

ð1:1:2:10Þ

In a change of basis, following (1.1.2.16), the gij ’s transform according to gij ¼ B ik B jm g0km ð1:1:2:19Þ g0ij ¼ Aik A jm gkm :

ð1:1:2:11Þ

The volumes V 0 and V of the cells built on the basis vectors e0i and ei , respectively, are given by the triple scalar products of these two sets of basis vectors and are related by

with gij gjk ¼ ik :

V 0 ¼ ðe01 ; e02 ; e03 Þ ¼ ðBij Þðe1 ; e2 ; e3 Þ

The table of the gij ’s is the inverse of the table of the gij ’s. Let us now take up the development of x with respect to the basis ei :

¼ ðBij ÞV;

x ¼ xi ei : Let us replace xi by the expression (1.1.2.10): x ¼ xj gij ei ;

ð1:1:2:20Þ

where ðBij Þ is the determinant associated with the transformation matrix between the two bases. From (1.1.2.17) and (1.1.2.20), we can write

ð1:1:2:12Þ

ðg0ij Þ ¼ ðBki ÞðBm j Þðgkm Þ:

and let us introduce the set of n vectors e j ¼ gij ei

ð1:1:2:18Þ

ð1:1:2:13Þ

6

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS TðxÞ ¼ ti x j If the basis ei is orthonormal, ðgkm Þ and V are equal to one, Pðx; yÞ ¼ pij xi y j ¼ ti xi sj y j ¼ ti sj xi y j : ðBj Þ is equal to the volume V 0 of the cell built on the basis SðyÞ ¼ sj yi vectors e0i and One deduces from this that ðg0 Þ ¼ V 02 : ij

pij ¼ ti sj :

This relation is actually general and one can remove the prime index: ðgij Þ ¼ V 2 :

It is a tensor of rank 2. One can equally well envisage the tensor product of more than two spaces, for example, En Fp Gq in npq dimensions. We shall limit ourselves in this study to the case of afﬁne tensors, which are deﬁned in a space constructed from the product of the space En with itself or with its conjugate En. Thus, a tensor product of rank 3 will have n3 components. The tensor product can be generalized as the product of multilinear forms. One can write, for example, Pðx; y; zÞ ¼ Tðx; yÞ SðzÞ ð1:1:3:1Þ p jik xi yj zk ¼ t ji xi yj sk zk :

ð1:1:2:21Þ

In the same way, we have for the corresponding reciprocal basis ðgij Þ ¼ V 2 ; where V is the volume of the reciprocal cell. Since the tables of the gij ’s and of the gij ’s are inverse, so are their determinants, and therefore the volumes of the unit cells of the direct and reciprocal spaces are also inverse, which is a very well known result in crystallography.

1.1.3.2. Behaviour under a change of basis A multilinear form is, by deﬁnition, invariant under a change of basis. Let us consider, for example, the trilinear form (1.1.3.1). If we change the system of coordinates, the components of vectors x, y, z become

1.1.3. Mathematical notion of tensor 1.1.3.1. Deﬁnition of a tensor For the mathematical deﬁnition of tensors, the reader may consult, for instance, Lichnerowicz (1947), Schwartz (1975) or Sands (1995).

xi ¼ Bi x0 ;

1.1.3.1.1. Linear forms A linear form in the space En is written

yj ¼ Aj y0 ;

zk ¼ Bk z0 :

Let us put these expressions into the trilinear form (1.1.3.1): Pðx; y; zÞ ¼ p jik Bi x0 Aj y0 Bk z0 :

TðxÞ ¼ ti xi ;

Now we can equally well make the components of the tensor appear in the new basis:

where TðxÞ is independent of the chosen basis and the ti ’s are the coordinates of T in the dual basis. Let us consider now a bilinear form in the product space En Fp of two vector spaces with n and p dimensions, respectively:

0 0 0 Pðx; y; zÞ ¼ p0 x y z :

Tðx; yÞ ¼ tij xi y j :

As the decomposition is unique, one obtains j i k p0 ¼ p ik B Aj B :

The np quantities tij ’s are, by deﬁnition, the components of a tensor of rank 2 and the form Tðx; yÞ is invariant if one changes the basis in the space En Fp. The tensor tij is said to be twice covariant. It is also possible to construct a bilinear form by replacing the spaces En and Fp by their respective conjugates En and F p . Thus, one writes

ð1:1:3:2Þ

One thus deduces the rule for transforming the components of a tensor q times covariant and r times contravariant: they transform like the product of q covariant components and r contravariant components. This transformation rule can be taken inversely as the deﬁnition of the components of a tensor of rank n ¼ q þ r.

Tðx; yÞ ¼ tij xi y j ¼ t ji xi yj ¼ t ij xi y j ¼ tij xi yj ;

Example. The operator O representing a symmetry operation has the character of a tensor. In fact, under a change of basis, O transforms into O0 :

where tij is the doubly contravariant form of the tensor, whereas t ji and tji are mixed, once covariant and once contravariant. We can generalize by deﬁning in the same way tensors of rank 3 or higher by using trilinear or multilinear forms. A vector is a tensor of rank 1, and a scalar is a tensor of rank 0.

O0 ¼ AOA1 so that

1.1.3.1.2. Tensor product Let us consider two vector spaces, En with n dimensions and Fp with p dimensions, and let there be two linear forms, TðxÞ in En and SðyÞ in Fp . We shall associate with these forms a bilinear form called a tensor product which belongs to the product space with np dimensions, En Fp :

O0ij ¼ Aik Okl ðA1 Þlj : Now the matrices A and B are inverses of one another: O0ij ¼ Aik Okl Blj : The symmetry operator is a tensor of rank 2, once covariant and once contravariant.

Pðx; yÞ ¼ TðxÞ SðyÞ: This correspondence possesses the following properties: (i) it is distributive from the right and from the left; (ii) it is associative for multiplication by a scalar; (iii) the tensor products of the vectors with a basis En and those with a basis Fp constitute a basis of the product space. The analytical expression of the tensor product is then

1.1.3.3. Operations on tensors 1.1.3.3.1. Addition It is necessary that the tensors are of the same nature (same rank and same variance).

7

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES D ¼ "E: 1.1.3.3.2. Multiplication by a scalar This is a particular case of the tensor product. If the medium is anisotropic, we have, for one of the components, 1.1.3.3.3. Contracted product, contraction D1 ¼ "11 E1 þ "12 E2 þ "13 E3 : Here we are concerned with an operation that only exists in the case of tensors and that is very important because of its applications in physics. In practice, it is almost always the case that This relation and the equivalent ones for the other components tensors enter into physics through the intermediary of a can also be written contracted product. Di ¼ "ij E j ð1:1:3:3Þ (i) Contraction. Let us consider a tensor of rank 2 that is once covariant and once contravariant. Let us write its transformation using the Einstein convention. in a change of coordinate system: The scalar product of D by an arbitrary vector x is ti0j ¼ A jp Bqi t pq : Di xi ¼ "ij E j xi : Now consider the quantity ti0i derived by applying the Einstein The right-hand member of this relation is a bilinear form that is convention ðti0i ¼ t101 þ t202 þ t303 Þ. It follows that invariant under a change of basis. The set of nine quantities "ij ti0i ¼ Aip B qi t pq ¼ qp t qq constitutes therefore the set of components of a tensor of rank 2. Expression (1.1.3.3) is the contracted product of "ij by E j. ti0i ¼ t pp : A similar demonstration may be used to show the tensor nature of the various physical properties described in Section This is an invariant quantity and so is a scalar. This operation can be carried out on any tensor of rank higher than or equal to 1.1.1, whatever the rank of the tensor. Let us for instance 1.1.4.4.3). The two, provided that it is expressed in a form such that its consider the piezoelectric effect (see Section i components of the electric polarization, P , which appear in a components are (at least) once covariant and once contravariant. medium submitted to a stress represented by the second-rank The contraction consists therefore of equalizing a covariant index and a contravariant index, and then in summing over this tensor Tjk are index. Let us take, for example, the tensor ti0jk . Its contracted form P i ¼ d ijk Tjk ; is ti0ik, which, with a change of basis, becomes ti0ik ¼ Akp t qp q :

Example. Let us take again the operator of symmetry O. The trace of the associated matrix is equal to

where the tensor nature of Tjk will be shown in Section 1.3.2. If we take the contracted product of both sides of this equation by any vector of covariant components xi, we obtain a linear form on the left-hand side, and a trilinear form on the right-hand side, which shows that the coefﬁcients d ijk are the components of a third-rank tensor. Let us now consider the piezo-optic (or photoelastic) effect (see Sections 1.1.4.10.5 and 1.6.7). The components of the variation ij of the dielectric impermeability due to an applied stress are

O11 þ O22 þ O33 ¼ Oii :

ij ¼ ijkl Tjl :

The components t ik i are those of a vector, resulting from the contraction of the tensor t jk i . The rank of the tensor has changed from 3 to 1. In a general manner, the contraction reduces the rank of the tensor from n to n 2.

It is the resultant of the contraction of the tensor O. It is a tensor of rank 0, which is a scalar and is invariant under a change of basis.

In a similar fashion, consider the contracted product of both sides of this relation by two vectors of covariant components xi and yj , respectively. We obtain a bilinear form on the left-hand side, and a quadrilinear form on the right-hand side, showing that the coefﬁcients ijkl are the components of a fourth-rank tensor.

(ii) Contracted product. Consider the product of two tensors of which one is contravariant at least once and the other covariant at least once:

1.1.3.5. Representation surface of a tensor 1.1.3.5.1. Deﬁnition Let us consider a tensor tijkl... represented in an orthonormal frame where variance is not important. The value of component 0 in an arbitrary direction is given by t1111...

j k p jk i ¼ t iz :

If we contract the indices i and k, it follows that p jii ¼ t ji zi :

0 t1111... ¼ tijkl... Bi1 B j1 Bk1 Bl1 . . . ;

The contracted product is then a tensor of rank 1 and not 3. It is an operation that is very frequent in practice. (iii) Scalar product. Next consider the tensor product of two vectors:

where the Bi1, B j1 ; . . . are the direction cosines of that direction with respect to the axes of the orthonormal frame. The representation surface of the tensor is the polar plot of 0 t1111... .

t ji ¼ xi y j : After contraction, we get the scalar product: t ii ¼ xi yi :

1.1.3.5.2. Representation surfaces of second-rank tensors The representation surfaces of second-rank tensors are quadrics. The directions of their principal axes are obtained as follows. Let tij be a second-rank tensor and let OM ¼ r be a vector with coordinates xi. The doubly contracted product, tij xi x j , is a scalar. The locus of points M such that

1.1.3.4. Tensor nature of physical quantities Let us ﬁrst consider the dielectric constant. In the introduction, we remarked that for an isotropic medium

8

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS i j

xi ¼ gik xk and y j ¼ g jl yl :

tij x x ¼ 1 It follows that

is a quadric. Its principal axes are along the directions of the eigenvectors of the matrix with elements tij. They are solutions of the set of equations

t ij ¼ gik g jl xk yl :

tij xi ¼ x j ;

xk yl is a tensor product of two vectors expressed in the dual space:

where the associated quantities are the eigenvalues. Let us take as axes the principal axes. The equation of the quadric reduces to

xk yl ¼ tkl : One can thus pass from the doubly covariant form to the doubly contravariant form of the tensor by means of the relation

t11 ðx1 Þ2 þ t22 ðx2 Þ2 þ t33 ðx3 Þ2 ¼ 1:

t ij ¼ gik g jl tkl :

If the eigenvalues are all of the same sign, the quadric is an ellipsoid; if two are positive and one is negative, the quadric is a hyperboloid with one sheet; if one is positive and two are negative, the quadric is a hyperboloid with two sheets (see Section 1.3.1). Associated quadrics are very useful for the geometric representation of physical properties characterized by a tensor of rank 2, as shown by the following examples: (i) Index of refraction of a medium. It is related to the dielectric constant by n ¼ "1=2 and, like it, it is a tensor of rank 2. Its associated quadric is an ellipsoid, the optical indicatrix, which represents its variations with the direction in space (see Section 1.6.3.2). (ii) Thermal expansion. If one cuts a sphere in a medium whose thermal expansion is anisotropic, and if one changes the temperature, the sphere becomes an ellipsoid. Thermal expansion is therefore represented by a tensor of rank 2 (see Chapter 1.4). (iii) Thermal conductivity. Let us place a drop of wax on a plate of gypsum, and then apply a hot point at the centre. There appears a halo where the wax has melted: it is elliptical, indicating anisotropic conduction. Thermal conductivity is represented by a tensor of rank 2 and the elliptical halo of molten wax corresponds to the intersection of the associated ellipsoid with the plane of the plate of gypsum.

This result is general: to change the variance of a tensor (in practice, to raise or lower an index), it is necessary to make the contracted product of this tensor using gij or gij , according to the case. For instance, tkl ¼ g jl tlk ;

t ijk ¼ gkl t ijl :

Remark gij ¼ gik gkj ¼ ij : This is a property of the metric tensor. 1.1.3.6.3. Examples of the use in physics of different representations of the same quantity Let us consider, for example, the force, F, which is a tensor quantity (tensor of rank 1). One can deﬁne it: (i) by the fundamental law of dynamics: F ¼ mC;

with F i ¼ m d2 xi =dt2 ;

where m is the mass and C is the acceleration. The force appears here in a contravariant form. (ii) as the derivative of the energy, W: Fi ¼ @[email protected] ¼ @i W: The force appears here in covariant form. In effect, we shall see in Section 1.1.3.8.1 that to form a derivative with respect to a variable contravariant augments the covariance by unity. The general expression of the law of dynamics is therefore written with the energy as follows:

1.1.3.5.3. Representation surfaces of higher-rank tensors Examples of representation surfaces of higher-rank tensors are given in Sections 1.3.3.4.4 and 1.9.4.2.

m d2 xi =dt2 ¼ gij @j W:

1.1.3.6. Change of variance of the components of a tensor 1.1.3.6.1. Tensor nature of the metric tensor Equation (1.1.2.17) describing the behaviour of the quantities gij ¼ ei ej under a change of basis shows that they are the components of a tensor of rank 2, the metric tensor. In the same way, equation (1.1.2.19) shows that the gij ’s transform under a change of basis like the product of two contravariant coordinates. The coefﬁcients gij and gij are the components of a unique tensor, in one case doubly contravariant, in the other case doubly covariant. In a general way, the Euclidean tensors (constructed in a space where one has deﬁned the scalar product) are geometrical entities that can have covariant, contravariant or mixed components.

1.1.3.7. Outer product 1.1.3.7.1. Deﬁnition The tensor deﬁned by ^ x y¼xyyx is called the outer product of vectors x and y. (Note: The symbol is different from the symbol ^ for the vector product.) The analytical expression of this tensor of rank 2 is ^ x ¼ xi ei ¼) x y ¼ ðxi y j yi x j Þ ei ej : y ¼ y j ej

1.1.3.6.2. How to change the variance of the components of a tensor Let us take a tensor product

The components pij ¼ xi y j yi x j of this tensor satisfy the properties

t ij ¼ xi y j :

pij ¼ p ji ;

We know that

pii ¼ 0:

It is an antisymmetric tensor of rank 2.

9

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.1.3.7.2. Vector product Consider the so-called permutation tensor of rank 3 (it is actually an axial tensor – see Section 1.1.4.5.3) deﬁned by 8 < "ijk ¼ þ1 if the permutation ijk is even " ¼ 1 if the permutation ijk is odd : ijk if at least two of the three indices are equal "ijk ¼ 0

1.1.3.8.2. Generalization Consider a ﬁeld of tensors t ji that are functions of space variables. In a change of coordinate system, one has t ji ¼ Ai Bj t0 : Differentiate with respect to xk : 0 0 @t ji j j @t @x ¼ @ t ¼ A B k i i @xk @x0 @xk j j @k t i ¼ Ai B Ak @ t0 :

and let us form the contracted product zk ¼ 12 "ijk pij ¼ "ijk xi yj :

ð1:1:3:4Þ

It is easy to check that 8 < z1 ¼ x2 y3 y2 x3 z ¼ x3 y1 y3 x1 : 2 z3 ¼ x1 y2 y2 x1 :

It can be seen that the partial derivatives @k t ji behave under a change of axes like a tensor of rank 3 whose covariance has been increased by 1 with respect to that of the tensor t ji . It is therefore possible to introduce a tensor of rank 1, r (nabla), of which the components are the operators given by the partial derivatives @[email protected] .

One recognizes the coordinates of the vector product.

1.1.3.8.3. Differential operators If one applies the operator nabla to a scalar ’, one obtains

1.1.3.7.3. Properties of the vector product Expression (1.1.3.4) of the vector product shows that it is of a covariant nature. This is indeed correct, and it is well known that the vector product of two vectors of the direct lattice is a vector of the reciprocal lattice [see Section 1.1.4 of Volume B of International Tables for Crystallography (2008)]. The vector product is a very particular vector which it is better not to call a vector: sometimes it is called a pseudovector or an axial vector in contrast to normal vectors or polar vectors. The components of the vector product are the independent components of the antisymmetric tensor pij . In the space of n dimensions, one would write vi3 i4 ...in ¼

grad ’ ¼ r ’: This is a covariant vector in reciprocal space. Now let us form the tensor product of r by a vector v of variable components. We then have rv¼

@v j e e j: @xi i

The quantities @i v j form a tensor of rank 2. If we contract it, we obtain the divergence of v: div v ¼ @i vi :

1 i1 i2 2 "i1 i2 ...in p :

Taking the vector product, we get The number of independent components of pij is equal to ðn2 nÞ=2 or 3 in the space of three dimensions and 6 in the space of four dimensions, and the independent components of pij are not the components of a vector in the space of four dimensions. Let us also consider the behaviour of the vector product under the change of axes represented by the matrix 0 1 1 0 0 @ 0 1 0 A: 0 0 1

curl v ¼ r ^ v: The curl is then an axial vector. 1.1.3.8.4. Development of a vector function in a Taylor series Let uðrÞ be a vector function. Its development as a Taylor series is written ui ðr þ drÞ ¼ ui ðrÞ þ

This is a symmetry with respect to a point that transforms a right-handed set of axes into a left-handed set and reciprocally. In such a change, the components of a normal vector change sign. Those of the vector product, on the contrary, remain unchanged, indicating – as one well knows – that the orientation of the vector product has changed and that it is not, therefore, a vector in the normal sense, i.e. independent of the system of axes.

2 i @ui j 1 @ u dx þ dx j dxk þ . . . : ð1:1:3:5Þ 2 @xj @xj @xk

The coefﬁcients of the expansion, @ui [email protected] j , @2 ui [email protected] j @xk ; . . . are tensors of rank 2; 3; . . .. An example is given by the relation between displacement and electric ﬁeld: Di ¼ "ij E j þ ijk E j Ek þ . . . (see Sections 1.6.2 and 1.7.2). We see that the linear relation usually employed is in reality a development that is arrested at the ﬁrst term. The second term corresponds to nonlinear optics. In general, it is very small but is not negligible in ferroelectric crystals in the neighbourhood of the ferroelectric–paraelectric transition. Nonlinear optics are studied in Chapter 1.7.

1.1.3.8. Tensor derivatives 1.1.3.8.1. Interpretation of the coefﬁcients of the matrix – change of coordinates We have under a change of axes: x0i ¼ Aij x j :

1.1.4. Symmetry properties For the symmetry properties of the tensors used in physics, the reader may also consult Bhagavantam (1966), Billings (1969), Mason (1966), Newnham (2005), Nowick (1995), Nye (1985), Pauﬂer (1986), Shuvalov (1988), Sirotin & Shaskol’skaya (1982), and Wooster (1973).

This shows that the new components, x0i , can be considered linear functions of the old components, x j , and one can write Aij ¼ @x0i [email protected] j ¼ @j x0i : It should be noted that the covariance has been increased.

10

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS 1.1.4.1. Introduction – Neumann’s principle

The symmetry of the indicatrix is identical to that of the medium if the crystal belongs to the orthorhombic holohedry and is higher in all other cases. This remark is the basis of the generalization of the symmetry principle by P. Curie (1859–1906). He stated that (Curie, 1894): (i) the symmetry characteristic of a phenomenon is the highest compatible with the existence of the phenomenon; (ii) the phenomenon may exist in a medium that possesses that symmetry or that of a subgroup of that symmetry; and concludes that some symmetry elements may coexist with the phenomenon but that their presence is not necessary. On the contrary, what is necessary is the absence of certain symmetry elements: ‘asymmetry creates the phenomenon’ (‘C’est la dissyme´trie qui cre´e le phe´nome`ne’; Curie, 1894, p. 400). Noting that physical phenomena usually express relations between a cause and an effect (an inﬂuence and a response), P. Curie restated the two above propositions in the following way, now known as Curie laws, although they are not, properly speaking, laws: (i) the asymmetry of the effects must pre-exist in the causes; (ii) the effects may be more symmetric than the causes. The application of the Curie laws enable one to determine the symmetry characteristic of a phenomenon. Let us consider the phenomenon ﬁrst as an effect. If is the symmetry of the phenomenon and C the symmetry of the cause that produces it,

We saw in Section 1.1.1 that physical properties express in general the response of a medium to an impetus. It has been known for a long time that symmetry considerations play an important role in the study of physical phenomena. These considerations are often very fruitful and have led, for instance, to the discovery of piezoelectricity by the Curie brothers in 1880 (Curie & Curie, 1880, 1881). It is not unusual for physical properties to be related to asymmetries. This is the case in electrical polarization, optical activity etc. The ﬁrst to codify this role was the German physicist and crystallographer F. E. Neumann (1795– 1898). In a series of papers (Neumann, 1832, 1833, 1834) he had studied the relations between the orientations of the mechanical, thermal and optical axes on the one hand and that of the crystalline axes on the other. His principle of symmetry was ﬁrst stated in his course at the University of Ko¨nigsberg (1873/1874) and was published in the printed version of his lecture notes (Neumann, 1885). It is now called Neumann’s principle: if a crystal is invariant with respect to certain symmetry elements, any of its physical properties must also be invariant with respect to the same symmetry elements. This principle may be illustrated by considering the optical properties of a crystal. In an anisotropic medium, the index of refraction depends on direction. For a given wave normal, two waves may propagate, with different velocities; this is the double refraction effect. The indices of refraction of the two waves vary with direction and can be found by using the index ellipsoid known as the optical indicatrix (see Section 1.6.3.2). Consider the central section of the ellipsoid perpendicular to the direction of propagation of the wave. It is an ellipse. The indices of the two waves that may propagate along this direction are equal to the semi-axes of that ellipse. There are two directions for which the central section is circular, and therefore two wave directions for which there is no double refraction. These directions are called optic axes, and the medium is said to be biaxial. If the medium is invariant with respect to a threefold, a fourfold or a sixfold axis (as in a trigonal, tetragonal or hexagonal crystal, for instance), its ellipsoid must also be invariant with respect to the same axis, according to Neumann’s principle. As an ellipsoid can only be ordinary or of revolution, the indicatrix of a trigonal, tetragonal or hexagonal crystal is necessarily an ellipsoid of revolution that has only one circular central section and one optic axis. These crystals are said to be uniaxial. In a cubic crystal that has four threefold axes, the indicatrix must have several axes of revolution, it is therefore a sphere, and cubic media behave as isotropic media for properties represented by a tensor of rank 2.

C : Let us now consider the phenomenon as a cause producing a certain effect with symmetry E: E: We can therefore conclude that C E: If we choose among the various possible causes the most symmetric one, and among the various possible effects the one with the lowest symmetry, we can then determine the symmetry that characterizes the phenomenon. As an example, let us determine the symmetry associated with a mechanical force. A force can be considered as the result of a traction effort, the symmetry of which is A1 1M. If considered as a cause, its effect may be the motion of a sphere in a given direction (for example, a spherical ball falling under its own weight). Again, the symmetry is A1 1M. The symmetries associated with the force considered as a cause and as an effect being the same, we may conclude that A1 1M is its characteristic symmetry.

1.1.4.2. Curie laws The example given above shows that the symmetry of the property may possess a higher symmetry than the medium. The property is represented in that case by the indicatrix. The symmetry of an ellipsoid is

1.1.4.3. Symmetries associated with an electric ﬁeld and with magnetic induction (ﬂux density) 1.1.4.3.1. Symmetry of an electric ﬁeld Considered as an effect, an electric ﬁeld may have been produced by two circular coaxial electrodes, the ﬁrst one carrying positive electric charges, the other one negative charges (Fig. 1.1.4.1). The cause possesses an axis of revolution and an inﬁnity

A2 A02 A002 C ¼ mmm for any ellipsoid M M0 M00 (orthorhombic symmetry) A1 1A2 1 C ¼ m for an ellipsoid of revolution m M 1M (cylindrical symmetry) A 1 1 1C ¼1 for a sphere m M (spherical symmetry): [Axes A1 are axes of revolution, or axes of isotropy, introduced by Curie (1884, 1894), cf. International Tables for Crystallography (2005), Vol. A, Table 10.1.4.2.]

Fig. 1.1.4.1. Symmetry of an electric ﬁeld.

11

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES of mirrors parallel to it, A1 1M. Considered as a cause, the electric ﬁeld induces for instance the motion of a spherical electric charge parallel to itself. The associated symmetry is the same in each case, and the symmetry of the electric ﬁeld is identical to that of a force, A1 1M. The electric polarization or the electric displacement have the same symmetry.

to thermal expansion, the distances between these centres of gravity are temperature dependent. A very important case is that of the ferroelectric crystals where the direction of the polarization can be changed under the application of an external electric ﬁeld. From the viewpoint of symmetry, pyroelectricity can be considered as the superposition of two causes, namely the crystal with its symmetry on one hand and the increase of temperature, which is isotropic, on the other. The intersection of the groups of symmetry of the two causes is in this case identical to the group of symmetry of the crystal. The symmetry associated with the effect is that of the electric polarization that is produced, A1 1M. Since the asymmetry of the cause must pre-exist in the causes, the latter may not possess more than one axis of symmetry nor mirrors other than those parallel to the single axis. The only crystal point groups compatible with this condition are

1.1.4.3.2. Symmetry of magnetic induction The determination of the symmetry of magnetic quantities is more delicate. Considered as an effect, magnetic induction may be obtained by passing an electric current in a loop (Fig. 1.1.4.2). The corresponding symmetry is that of a cylinder rotating around its axis, ðA1 =MÞC. Conversely, the variation of the ﬂux of magnetic induction through a loop induces an electric current in the loop. If the magnetic induction is considered as a cause, its effect has the same symmetry. The symmetry associated with the magnetic induction is therefore ðA1 =MÞC. This symmetry is completely different from that of the electric ﬁeld. This difference can be understood by reference to Maxwell’s equations, which relate electric and magnetic quantities: curl E ¼ r ^ E ¼

@B ; @t

curl H ¼ r ^ H ¼

1; 2; 3; 4; 6; m; 2mm; 3m; 4mm; 6mm: There are therefore only ten crystallographic groups that are compatible with the pyroelectric effect. For instance, tourmaline, in which the effect was ﬁrst observed, belongs to 3m.

@D : @t

1.1.4.4.3. Piezoelectricity Piezoelectricity, discovered by the Curie brothers (Curie & Curie, 1880), is the property presented by certain materials that exhibit an electric polarization when submitted to an applied mechanical stress such as a uniaxial compression (see, for instance, Cady, 1964; Ikeda, 1990). The converse effect, namely their changes in shape when they are submitted to an external electric ﬁeld, was predicted by Lippmann (1881) and discovered by J. & P. Curie (Curie & Curie, 1881). The physical interpretation of piezoelectricity is the following: under the action of the applied stress, the centres of gravity of negative and positive charges move to different positions in the unit cell, which produces an electric polarization. From the viewpoint of symmetry, piezoelectricity can be considered as the superposition of two causes, the crystal with its own symmetry and the applied stress. The symmetry associated with a uniaxial compression is that of two equal and opposite forces, namely A1 =M 1A2 =1MC. The effect is an electric polarization, of symmetry A1 1M, which must be higher than or equal to the intersection of the symmetries of the two causes:

It was seen in Section 1.1.3.8.3 that the curl is an axial vector because it is a vector product. Maxwell’s equations thus show that if the electric quantities (E, D) are polar vectors, the magnetic quantities (B, H) are axial vectors and vice versa; the equations of Maxwell are, in effect, perfectly symmetrical on this point. Indeed, one could have been tempted to determine the symmetry of the magnetic ﬁeld by considering interactions between magnets, which would have led to the symmetry A1 1M for the magnetic quantities. However, in the world where we live and where the origin of magnetism is in the spin of the electron, the magnetic ﬁeld is an axial vector of symmetry ðA1 =MÞC while the electric ﬁeld is a polar vector of symmetry A1 1M. 1.1.4.4. Superposition of several causes in the same medium – pyroelectricity and piezolectricity 1.1.4.4.1. Introduction Let us now consider a phenomenon resulting from the superposition of several causes in the same medium. The symmetry of the global cause is the intersection of the groups of symmetry of the various causes: the asymmetries add up (Curie, 1894). This remark can be applied to the determination of the point groups where physical properties such as pyroelectricity or piezoelectricity are possible.

A1 1A2 \ C Scrystal A1 1M; M 1M where Scrystal denotes the symmetry of the crystal. It may be noted that the effect does not possess a centre of symmetry. The crystal point groups compatible with the property of piezoelectricity are therefore among the 21 noncentrosymmetric point groups. More elaborate symmetry considerations show further that group 432 is also not compatible with piezoelectricity. This will be proved in Section 1.1.4.10.4 using the symmetry properties of tensors. There are therefore 20 point groups compatible with piezoelectricity:

1.1.4.4.2. Pyroelectricity Pyroelectricity is the property presented by certain materials that exhibit electric polarization when the temperature is changed uniformly. Actually, this property appears in crystals for which the centres of gravity of the positive and negative charges do not coincide in the unit cell. They present therefore a spontaneous polarization that varies with temperature because, owing

1; 2; m; 222; 2mm; 622; 6mm; 62m 422; 4mm; 42m; 3; 32; 3m; 4; 4; 6; 6; 23; 43m: The intersection of the symmetries of the crystal and of the applied stress depend of course on the orientation of this stress relative to the crystallographic axes. Let us take, for instance, a crystal of quartz, which belongs to group 32 ¼ A3 3A2. The above condition becomes

Fig. 1.1.4.2. Symmetry of magnetic induction.

12

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS A1 1A2 C M 1M

\

If one can assume, as one usually does in physics, that the energy is a ‘good’ function and that the order of the derivatives is of little importance, then one can write

A3 3A2 A1 1M:

If the applied compression is parallel to the threefold axis, the intersection is identical to the symmetry of the crystal, A3 3A2 , which possesses symmetry elements that do not exist in the effect, and piezoelectricity cannot appear. This is of course obvious because the threefold axis is not polar. For all other directions, piezoelectricity may appear.

@2 W @2 W ¼ : @Ek @E j @E j @Ek As one can exchange the role of the dummy indices, one has @2 W=ð@E j @Ek Þ ¼ "kj :

1.1.4.5. Intrinsic symmetry of tensors

Hence one deduces that

1.1.4.5.1. Introduction The symmetry of a tensor representing a physical property or a physical quantity may be due either to its own nature or to the symmetry of the medium. The former case is called intrinsic symmetry. It is a property that can be exhibited both by physical property tensors or by ﬁeld tensors. The latter case is the consequence of Neumann’s principle and will be discussed in Section 1.1.4.6. It applies to physical property tensors.

"jk ¼ "kj : The dielectric constant tensor is therefore symmetric. One notes that the symmetry is conveyed on two indices of the same variance. One could show in a similar way that the tensor representing magnetic susceptibility is symmetric. (3) There are other possible causes for the symmetry of a tensor of rank 2. The strain tensor (Section 1.3.1), which is a ﬁeld tensor, is symmetric because one does not take into account the rotative part of the deformation; the stress tensor, also a ﬁeld tensor (Section 1.3.1), is symmetric because one neglects body torques (couples per unit volume); the thermal conductivity tensor is symmetric because circulating ﬂows do not produce any detectable effects etc.

1.1.4.5.2. Symmetric tensors 1.1.4.5.2.1. Tensors of rank 2 A bilinear form is symmetric if Tðx; yÞ ¼ Tðy; xÞ: Its components satisfy the relations

1.1.4.5.2.2. Tensors of higher rank A tensor of rank higher than 2 may be symmetric with respect to the indices of one or more couples of indices. For instance, by its very nature, the demonstration given in Section 1.1.1.4 shows that the tensors representing principal physical properties are of even rank. If n is the rank of the associated square matrix, the number of independent components is equal to ðn2 þ nÞ=2. In the case of a tensor of rank 4, such as the tensor of elastic constants relating the strain and stress tensors (Section 1.3.3.2.1), the number of components of the tensor is 34 ¼ 81. The associated matrix is a 9 9 one, and the number of independent components is equal to 45.

tij ¼ tji : The associated matrix, T, is therefore equal to its transpose T T : 0 1 0 1 t11 t12 t13 t11 t21 t31 T ¼ @ t21 t22 t23 A ¼ T T ¼ @ t12 t22 t32 A: t31 t32 t33 t13 t23 t33 In a space with n dimensions, the number of independent components is equal to ðn2 nÞ=2 þ n ¼ ðn2 þ nÞ=2: Examples (1) The metric tensor (Section 1.1.2.2) is symmetric because the scalar product is commutative. (2) The tensors representing one of the physical properties associated with the leading diagonal of the matrix of physical properties (Section 1.1.1.4), such as the dielectric constant. Let us take up again the demonstration of this case and consider a capacitor being charged. The variation of the stored energy per unit volume for a variation dD of the displacement is

1.1.4.5.3. Antisymmetric tensors – axial tensors 1.1.4.5.3.1. Tensors of rank 2 A bilinear form is said to be antisymmetric if Tðx; yÞ ¼ Tðy; xÞ: Its components satisfy the relations tij ¼ tji :

dW ¼ E dD;

The associated matrix, T, is therefore also 0 0 t12 0 T ¼ T T ¼ @ t12 t13 t23

where [equation (1.1.3.3)] Di ¼ "ij E j : Since both Di and E j are expressed through contravariant components, the expression for the energy should be written

antisymmetric: 1 t13 t23 A: 0

The number of independent components is equal to ðn2 nÞ=2, where n is the number of dimensions of the space. It is equal to 3 in a three-dimensional space, and one can consider these components as those of a pseudovector or axial vector. It must never be forgotten that under a change of basis the components of an axial vector transform like those of a tensor of rank 2. Every tensor can be decomposed into the sum of two tensors, one symmetric and the other one antisymmetric:

dW ¼ gij E j dDi : If we replace Di by its expression, we obtain dW ¼ gij "ik E j dEk ¼ "jk E j dEk ; where we have introduced the doubly covariant form of the dieletric constant tensor, "jk . Differentiating twice gives

T ¼ S þ A;

2

@W ¼ "jk : @Ek @E j

with S ¼ ðT þ T T Þ=2 and A ¼ ðT T T Þ=2.

13

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Example. As shown in Section 1.1.3.7.2, the components of the vector product of two vectors, x and y,

The twice contracted product t lk ¼ 12 "ijk t ijl

zk ¼ "ijk xi y j ;

is an axial tensor of rank 2 whose components are the independent components of the antisymmetric tensor of rank 3, t ijl .

are really the independent components of an antisymmetric tensor of rank 2. The magnetic quantities, B, H (Section 1.1.4.3.2), the tensor representing the pyromagnetic effect (Section 1.1.1.3) etc. are axial tensors.

Examples (1) Hall constant. The Hall effect is observed in semiconductors. If one takes a semiconductor crystal and applies a magnetic induction B and at the same time imposes a current density j at right angles to it, one observes an electric ﬁeld E at right angles to the other two ﬁelds (see Section 1.8.3.4). The expression for the ﬁeld can be written

1.1.4.5.3.2. Tensors of higher rank If the rank of the tensor is higher than 2, the tensor may be antisymmetric with respect to the indices of one or several couples of indices. (i) Tensors of rank 3 antisymmetric with respect to every couple of indices. A trilinear form Tðx; y; zÞ ¼ tijk xi y j zk is said to be antisymmetric if it satiﬁes the relations 9 Tðx; y; zÞ ¼ Tðy; x; zÞ = ¼ Tðx; z; yÞ ; ¼ Tðz; y; xÞ:

Ei ¼ RH ikl jk Bl ; where RH ikl is the Hall constant, which is a tensor of rank 3. However, because the direction of the current density is imposed by the physical law (the set of vectors B, j, E constitutes a righthanded frame), one has RH ikl ¼ RH kil ;

Tensor tijk has 27 components. It is found that all of them are equal to zero, except

which shows that RH ikl is an antisymmetric (axial) tensor of rank 3. As can be seen from its physical properties, only the components such that i 6¼ k 6¼ l are different from zero. These are

t123 ¼ t231 ¼ t312 ¼ t213 ¼ t132 ¼ t321 :

RH 123 ¼ RH 213 ;

The three-times contracted product with the permutations tensor (Section 1.1.3.7.2), ð1=6Þ"ijk tijk , is a pseudoscalar or axial scalar. It is not a usual scalar: the sign of this product changes when one changes the hand of the reference axes, change of basis represented by the matrix 0 1 1 0 0 @ 0 1 0 A: 0 0 1

Tðx; y; zÞ ¼ Pt123 ; 1 x i j k P ¼ "ijk x y z ¼ y1 z1

2

x y2 z2

RH 312 ;

RH 321 :

(2) Optical rotation. The gyration tensor used to describe the property of optical rotation presented by gyrotropic materials (see Section 1.6.5.4) is an axial tensor of rank 2, which is actually an antisymmetric tensor of rank 3. (3) Acoustic activity. The acoustic gyrotropic tensor describes the rotation of the polarization plane of a transverse acoustic wave propagating along the acoustic axis (see for instance Kumaraswamy & Krishnamurthy, 1980). The elastic constants may be expanded as

Form Tðx; y; zÞ can also be written

where

RH 132 ¼ RH 312 ;

cijkl ð!; kÞ ¼ cijkl ð!Þ þ idijklm ð!Þkm þ . . . ; where dijklm is a ﬁfth-rank tensor. Time-reversal invariance requires that dijklm ¼ djiklm , which shows that it is an antisymmetric (axial) tensor.

x y3 z3 3

1.1.4.5.3.3. Properties of axial tensors The two preceding sections have shown examples of axial tensors of ranks 0 (pseudoscalar), 1 (pseudovector) and 2. They have in common that all their components change sign when the sign of the basis is changed, and this can be taken as the deﬁnition of an axial tensor. Their components are the components of an antisymmetric tensor of higher rank. It is important to bear in mind that in order to obtain their behaviour in a change of basis, one should ﬁrst determine the behaviour of the components of this antisymmetric tensor.

is the triple scalar product of the three vectors x, y, z: P ¼ ðx; y; zÞ ¼ ðx ^ y zÞ: It is also a pseudoscalar. The permutation tensor is not a real tensor of rank 3: if the hand of the axes is changed, the sign of P also changes; P is therefore not a trilinear form. Another example of a pseudoscalar is given by the rotatory power of an optically active medium, which is expressed through the relation (see Section 1.6.5.4) ¼ d;

1.1.4.6. Symmetry of tensors imposed by the crystalline medium

where is the rotation angle of the light wave, d the distance traversed in the material and is a pseudoscalar: if one takes the mirror image of this medium, the sign of the rotation of the light wave also changes. (ii) Tensor of rank 3 antisymmetric with respect to one couple of indices. Let us consider a trilinear form such that

Many papers have been devoted to the derivation of the invariant components of physical property tensors under the inﬂuence of the symmetry elements of the crystallographic point groups: see, for instance, Fumi (1951, 1952a,b,c, 1987), Fumi & Ripamonti (1980a,b), Nowick (1995), Nye (1957, 1985), Sands (1995), Sirotin & Shaskol’skaya (1982), and Wooster (1973). There are three main methods for this derivation: the matrix method (described in Section 1.1.4.6.1), the direct inspection method (described in Section 1.1.4.6.3) and the group-theoretical method (described in Section 1.2.4 and used in the accompanying software, see Section 1.2.7.4).

Tðx; y; zÞ ¼ Tðy; x; zÞ: Its components satisfy the relation t iil ¼ 0;

t ijl ¼ t jil :

14

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS 1.1.4.6.1. Matrix method – application of Neumann’s principle An operation of symmetry turns back the crystalline ediﬁce on itself; it allows the physical properties of the crystal and the tensors representing them to be invariant. An operation of symmetry is equivalent to a change of coordinate system. In a change of system, a tensor becomes

reduction of tensors of even rank is therefore the same in a centred group and in its noncentred subgroups, that is in any of the 11 Laue classes: 1 1 2=m 2; m mmm 222; 2mm 3 3 3m 32; 3m 4 4=m 4; 4=mm 42m; 422; 4mm 6 6=m 6; 6=mm 62m; 622; 6mm m3 23 m3m 432; 432:

0 t ¼ tklij Ai Aj Bk Bl :

If A represents a symmetry operation, it is a unitary matrix: A ¼ BT ¼ B1 : Since the tensor is invariant under the action of the symmetry operator A, one has, according to Neumann’s principle, 0 t ¼ t

If a tensor is invariant with respect to two elements of symmetry, it is invariant with respect to their product. It is then sufﬁcient to make the reduction for the generating elements of the group and (since this concerns a tensor of even rank) for the 11 Laue classes. (ii) Tensors of odd rank, t ij... ¼ ð1Þ2pþ1 t ij... . All the components are equal to zero. The physical properties represented by tensors of rank 3, such as piezoelectricity, piezomagnetism, nonlinear optics, for instance, will therefore not be present in a centrosymmetric crystal.

and, therefore, t ¼ tklij Ai Aj Bk Bl :

ð1:1:4:1Þ

There are therefore a certain number of linear relations between the components of the tensor and the number of independent components is reduced. If there are p components and q relations between the components, there are p q independent components. This number is independent of the system of axes. When applied to each of the 32 point groups, this reduction enables one to ﬁnd the form of the tensor in each case. It depends on the rank of the tensor. In the present chapter, the reduction will be derived for tensors up to the fourth rank and for all crystallographic groups as well as for the isotropic groups. An orthonormal frame will be assumed in all cases, so that co- and contravariance will not be apparent and the positions of indices as subscripts or superscripts will not be meaningful. The Ox3 axis will be chosen parallel to the threefold, fourfold or sixfold axis in the trigonal, tetragonal and hexagonal systems. The accompanying software to the present volume enables the reduction for tensors of any rank to be derived.

1.1.4.6.2.3. General case By replacing the matrix coefﬁcients Aii by their expression, (1.1.4.2) becomes, for a proper rotation, t jk... ¼ t jk... expðirÞ expðisÞð1Þt ¼ t jk... exp iðr sÞ; where r is the number of indices equal to 1, s is the number of indices equal to 2, t is the number of indices equal to 3 and r þ s þ t ¼ p is the rank of the tensor. The component t jk... is not affected by the symmetry operation if ðr sÞ ¼ 2K ;

1.1.4.6.2. The operator A is in diagonal form 1.1.4.6.2.1. Introduction If one takes as the system of axes the eigenvectors of the operator A, the matrix is written in the form 0 1 exp i 0 0 @ 0 exp i 0 A; 0 0 1

where K is an integer, and is equal to zero if ðr sÞ 6¼ 2K : The angle of rotation can be put into the form 2 =q, where q is the order of the axis. The condition for the component not to be zero is then r s ¼ Kq:

where is the rotation angle, Ox3 is taken parallel to the rotation axis and coefﬁcient A3 is equal to +1 or 1 depending on whether the rotation axis is direct or inverse (proper or improper operator). The equations (1.1.4.1) can then be simpliﬁed and reduce to tklij ¼ tklij Aii Ajj Bkk Bll

The condition is fulﬁlled differently depending on the rank of the tensor, p, and the order of the axis, q. Indeed, we have r s p and p ¼ 2, r s 2: the result of the reduction will be the same for any q 3; p ¼ 3, r s 3: the result of the reduction will be the same for any q 4; p ¼ 4, r s 4: the result of the reduction will be the same for any q 5. It follows that: (i) for tensors of rank 2, the reduction will be the same for trigonal (threefold axis), tetragonal (fourfold axis) and hexagonal (sixfold axis) groups; (ii) for tensors of rank 3, the reduction will be the same for tetragonal and hexagonal groups; (iii) for tensors of rank 4, the reduction will be different for trigonal, tetragonal and hexagonal groups. The inconvenience of the diagonalization method is that the vectors and eigenvalues are, in general, complex, so in practice one uses another method. For instance, we may note that equa-

ð1:1:4:2Þ

(without any summation). If the product Aii A jj Bkk Bll (without summation) is equal to unity, equation (1.1.4.2) is trivial and there is signiﬁcance in the component tkl . On the contrary, if it is different from 1, the only solution for (1.1.4.2) is that tklij ¼ 0. One then ﬁnds immediately that certain components of the tensor are zero and that others are unchanged. 1.1.4.6.2.2. Case of a centre of symmetry All the diagonal components are in this case equal to 1. One thus has: (i) Tensors of even rank, t ij... ¼ ð1Þ2p t ij... . The components are not affected by the presence of the centre of symmetry. The

15

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES tion (1.1.4.1) can be written in the case of p ¼ 2 by associating with the tensor a 3 3 matrix T:

1.1.4.7.1. Triclinic system 1: no reduction, the tensor has 9 independent Groups 1, components. The result is represented in the following symbolic way (Nye, 1957, 1985):

T ¼ BTBT ; where B is the symmetry operation. Through identiﬁcation of homologous coefﬁcients in matrices T and BTBT , one obtains relations between components tij that enable the determination of the independent components.

where the sign

1.1.4.6.3. The method of direct inspection The method of ‘direct inspection’, due to Fumi (1952a,b, 1987), is very simple. It is based on the fundamental properties of tensors; the components transform under a change of basis like a product of vector components (Section 1.1.3.2).

*

represents a nonzero component.

1.1.4.7.2. Monoclinic system Groups 2m, 2, m: it is sufﬁcient to consider the twofold axis or the mirror. As the representative matrix is diagonal, the calculation is immediate. Taking the twofold axis to be parallel to Ox3, one has

Examples (1) Let us consider a tensor of rank 3 invariant with respect to a twofold axis parallel to Ox3. The matrix representing this operator is 0 1 1 0 0 @ 0 1 0 A: 0 0 1

t31 ¼ t13 ¼ t32 ¼ t23 ¼ 0: The other components are not affected. The result is represented as

The component tijk behaves under a change of axes like the product of the components xi ; xj ; xk. The components x1 ; x2 ; x3 of a vector become, respectively, x1 , x2 , x3 . To simplify the notation, we shall denote the components of the tensor simply by ijk. If, amongst the indices i, j and k, there is an even number (including the number zero) of indices that are equal to 3, the product xi xj xk will become xi xj xk under the rotation. As the component ‘ijk’ remains invariant and is also equal to its opposite, it must be zero. 14 components will thus be equal to zero:

There are 5 independent components. If the twofold axis is taken along axis Ox2, which is the usual case in crystallography, the table of independent components becomes

111; 122; 133; 211; 222; 133; 112; 121; 212; 221; 323; 331; 332; 313: (2) Let us now consider that the same tensor of rank 3 is invariant with respect to a fourfold axis parallel to Ox3. The matrix representing this operator and its action on a vector of coordinates x1 ; x2 ; x3 is given by 0 1 0 10 1 x2 0 1 0 x1 @ x1 A ¼ @ 1 0 0 [email protected] x2 A: ð1:1:4:3Þ 0 0 1 x3 x3

1.1.4.7.3. Orthorhombic system Groups mmm, 2mm, 222: the reduction is obtained by considering two perpendicular twofold axes, parallel to Ox3 and to Ox2, respectively. One obtains

Coordinate x1 becomes x2, x2 becomes x1 and x3 becomes x3. Component ijk transforms like product xi x j xk according to the rule given above. Since the twofold axis parallel to Ox3 is a subgroup of the fourfold axis, we can start from the corresponding reduction. We ﬁnd 311 123 113 333 132 131 312

() () () () () () ()

322 ð213Þ 223 333 ð231Þ 232 ð321Þ

: : : : : : :

t311 t123 t113 t333 t132 t131 t312

¼ ¼ ¼ ¼ ¼ ¼ ¼

There are 3 independent components. 1.1.4.7.4. Trigonal, tetragonal, hexagonal and cylindrical systems We remarked in Section 1.1.4.6.2.3 that, in the case of tensors of rank 2, the reduction is the same for threefold, fourfold or sixfold axes. It sufﬁces therefore to perform the reduction for the tetragonal groups. That for the other systems follows automatically.

t322 t213 t223 t333 t231 t232 t321 :

6; ðA1 =MÞC, A1 3; 4=m, 4, 4; 6=m, 6, 1.1.4.7.4.1. Groups 3, If we consider a fourfold axis parallel to Ox3 represented by the matrix given in (1.1.4.3), by applying the direct inspection method one ﬁnds

All the other components are equal to zero. It is not possible to apply the method of direct inspection for point group 3. One must in this case use the matrix method described in Section 1.1.4.6.2; once this result is assumed, the method can be applied to all other point groups. 1.1.4.7. Reduction of the components of a tensor of rank 2

where the symbol means that the corresponding component is

The reduction is given for each of the 11 Laue classes.

16

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS numerically equal to that to which it is linked, but of opposite sign. There are 3 independent components.

1.1.4.7.6.2. Monoclinic system (twofold axis parallel to Ox2 )

32, 3m; 4=mm, 422, 4mm, 42m; 1.1.4.7.4.2. Groups 3m, 6=mm, 622, 6mm, 62m; ðA1 =MÞ1ðA2 =MÞC, A1 1A2 The result is obtained by combining the preceding result and that corresponding to a twofold axis normal to the fourfold axis. One ﬁnds

There are 4 independent components. The quadric is still any quadric, but one of its axes coincides with the twofold axis of the monoclinic lattice. Four parameters are required: the lengths of the axes and one angle. 1.1.4.7.6.3. Orthorhombic system

There are 2 independent components. 1.1.4.7.5. Cubic and spherical systems The cubic system is characterized by the presence of threefold axes along the h111i directions. The action of a threefold axis along [111] on the components x1 ; x2 ; x3 of a vector results in a permutation of these components, which become, respectively, x2 ; x3 ; x1 and then x3 ; x1 ; x2 . One deduces that the components of a tensor of rank 2 satisfy the relations

There are 3 independent components. The quadric is any quadric, the axes of which coincide with the crystallographic axes. Only three parameters are required.

t11 ¼ t22 ¼ t33 :

1.1.4.7.6.4. Trigonal, tetragonal and hexagonal systems, isotropic groups

The cubic groups all include as a subgroup the group 23 of which the generating elements are a twofold axis along Ox3 and a threefold axis along [111]. If one combines the corresponding results, one deduces that t12 ¼ t23 ¼ t31 ¼ t13 ¼ t21 ¼ t32 ¼ 0; which can be summarized by

There are 2 independent components. The quadric is of revolution. It is characterized by two parameters: the lengths of its two axes. 1.1.4.7.6.5. Cubic system

There is a single independent component and the medium behaves like a property represented by a tensor of rank 2, like an isotropic medium. 1.1.4.7.6. Symmetric tensors of rank 2 If the tensor is symmetric, the number of independent components is still reduced. One obtains the following, representing the nonzero components for the leading diagonal and for one half of the others.

There is 1 independent component. The associated quadric is a sphere. 1.1.4.8. Reduction of the components of a tensor of rank 3 1.1.4.8.1. Triclinic system 1.1.4.8.1.1. Group 1 All the components are independent. Their number is equal to 27. They are usually represented as a 3 9 matrix which can be subdivided into three 3 3 submatrices: 0 1 111 122 133 123 131 112 132 113 121 B C @ 211 222 233 223 231 212 232 213 221 A: 311 322 333 323 331 312 332 313 321

1.1.4.7.6.1. Triclinic system

There are 6 independent components. It is possible to interpret the number of independent components of a tensor of rank 2 by considering the associated quadric, for instance the optical indicatrix. In the triclinic system, the quadric is any quadric. It is characterized by six parameters: the lengths of the three axes and the orientation of these axes relative to the crystallographic axes.

1.1.4.8.1.2. Group 1 All the components are equal to zero.

17

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.1.4.8.2. Monoclinic system 1.1.4.8.2.1. Group 2 Choosing the twofold axis parallel to Ox3 and applying the direct inspection method, one ﬁnds

There are 7 independent components.

There are 13 independent components. If the twofold axis is parallel to Ox2, one ﬁnds

1.1.4.8.3.3. Group mmm All the components are equal to zero.

1.1.4.8.4. Trigonal system 1.1.4.8.4.1. Group 3 The threefold axis is parallel to Ox3. The matrix method should be used here. One ﬁnds 1.1.4.8.2.2. Group m One obtains the matrix representing the operator m by multiplying by 1 the coefﬁcients of the matrix representing a twofold axis. The result of the reduction will then be exactly complementary: the components of the tensor which include an odd number of 3’s are now equal to zero. One writes the result as follows: There are 9 independent components.

1.1.4.8.4.2. Group 32 with a twofold axis parallel to Ox1 There are 14 independent components. If the mirror axis is normal to Ox2, one ﬁnds

There are 4 independent components. 1.1.4.8.2.3. Group 2=m All the components are equal to zero.

1.1.4.8.4.3. Group 3m with a mirror normal to Ox1

1.1.4.8.3. Orthorhombic system 1.1.4.8.3.1. Group 222 There are three orthonormal twofold axes. The reduction is obtained by combining the results associated with two twofold axes, parallel to Ox3 and Ox2 , respectively. There are 4 independent components.

1.1.4.8.4.4. Groups 3 and 3m All the components are equal to zero.

There are 6 independent components.

1.1.4.8.5. Tetragonal system 1.1.4.8.5.1. Group 4 The method of direct inspection can be applied for a fourfold axis. One ﬁnds

1.1.4.8.3.2. Group mm2 The reduction is obtained by combining the results associated with a twofold axis parallel to Ox3 and with a mirror normal to Ox2 :

18

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS (ii) Mirror perpendicular to Ox1 (the twofold axis is at 45 )

The number of independent components is of course the same, 6.

There are 7 independent components. 1.1.4.8.5.2. Group 422 One combines the reductions for groups 4 and 222:

1.1.4.8.5.7. Group 4=mm All the components are equal to zero.

1.1.4.8.6. Hexagonal and cylindrical systems 1.1.4.8.6.1. Groups 6, A1 , 622, A1 1A2 , 6mm and A1 1M It was shown in Section 1.1.4.6.2.3 that, in the case of tensors of rank 3, the reduction is the same for axes of order 4, 6 or higher. The reduction will then be the same as for the tetragonal system.

There are 3 independent components. 1.1.4.8.5.3. Group 4mm One combines the reductions for groups 4 and 2m:

1.1.4.8.6.2. Group 6 ¼ 3=m One combines the reductions for the groups corresponding to a threefold axis parallel to Ox3 and to a mirror perpendicular to Ox3 : There are 4 independent components. 1.1.4.8.5.4. Group 4=m All the components are equal to zero. There are 2 independent components.

1.1.4.8.5.5. Group 4 The matrix corresponding to axis 4 is 0

0 @1 0

1 0 0

1.1.4.8.6.3. Group 62m One combines the reductions for groups 6 and 2mm:

1

0 0A 1

and the form of the 3 9 matrix is There is 1 independent component.

1.1.4.8.6.4. Groups 6=m, ðA1 =MÞC, ðA1 =MÞ1ðA2 =MÞC All the components are equal to zero.

6=mm

and

There are 6 independent components. 1.1.4.8.5.6. Group 42m One combines either the reductions for groups 4 and 222, or the reductions for groups 4 and 2mm. (i) Twofold axis parallel to Ox1 :

1.1.4.8.7. Cubic and spherical systems 1.1.4.8.7.1. Group 23 One combines the reductions corresponding to a twofold axis parallel to Ox3 and to a threefold axis parallel to [111]:

There are 2 independent components.

There are 6 independent components.

19

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.1.4.8.7.2. Groups 432 and 1A1 =M One combines the reductions corresponding to groups 422 and 23:

1.1.4.9.2. Monoclinic system (groups 2=m, 2, m) The reduction is obtained by the method of direct inspection. For a twofold axis parallel to Ox2, one ﬁnds

There is 1 independent component. 1.1.4.8.7.3. Group 43m One combines the reductions corresponding to groups 42m and 23:

There are 41 independent components. 1.1.4.9.3. Orthorhombic system (groups mmm, 2mm, 222) There is 1 independent component. m3m and 1ðA1 =MÞC 1.1.4.8.7.4. Groups m3, All the components are equal to zero.

1.1.4.9. Reduction of the components of a tensor of rank 4 1) 1.1.4.9.1. Triclinic system (groups 1, There is no reduction; all the components are independent. Their number is equal to 81. They are usually represented as a 9 9 matrix, where components tijkl are replaced by ijkl, for brevity: There are 21 independent components. 1.1.4.9.4. Trigonal system 1.1.4.9.4.1. Groups 3 and 3 The reduction is ﬁrst applied in the system of axes tied to the eigenvectors of the operator representing a threefold axis. The system of axes is then changed to a system of orthonormal axes with Ox3 parallel to the threefold axis:

This matrix can be represented symbolically by

with t1111 t1122 ¼ t1112 þ t1121 ¼ where the 9 9 matrix has been subdivided for clarity in to nine 3 3 submatrices.

t1212 þ t1221 ðt1211 þ t2111 Þ:

There are 27 independent components.

20

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS 32, 3m, with the twofold axis parallel to 1.1.4.9.4.2. Groups 3m, Ox1

1.1.4.9.6. Hexagonal and cylindrical systems 6; ðA1 =MÞC, A1 1.1.4.9.6.1. Groups 6=m, 6,

with

with t1111 t1122 ¼ t1212 þ t1221 t1112 þ t1121 ¼ ðt1211 þ t2111 Þ:

t1111 t1122 ¼ t1212 þ t1221 : There are 14 independent components.

There are 19 independent components. 1.1.4.9.6.2. Groups 6=mm, 622, 6mm, 62m; ðA1 =MÞ1; ðA2 =MÞC, A1 1A2

1.1.4.9.5. Tetragonal system 1.1.4.9.5.1. Groups 4=m, 4, 4

with t1111 t1122 ¼ t1212 þ t1221 : There are 21 independent components. There are 11 independent components. 1.1.4.9.5.2. Groups 4=mm, 422, 4mm, 42m

1.1.4.9.7. Cubic system 1.1.4.9.7.1. Groups 23, 3m

There are 11 independent components.

There are 7 independent components.

21

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 432, 43m 1.1.4.9.7.2. Groups m3m,

1.1.4.9.9.2. Monoclinic system

There are 25 independent coefﬁcients.

There are 4 independent components. The tensor is symmetric. 1.1.4.9.8. Spherical system 1.1.4.9.8.1. Groups 1ðA1 =MÞC and 1A1

1.1.4.9.9.3. Orthorhombic system

with There are 15 independent coefﬁcients.

t1111 t1122 ¼ t1212 þ t1221 : There are 3 independent components. The tensor is symmetric.

1.1.4.9.9.4. Trigonal system (i) Groups 3 and 3

1.1.4.9.9. Symmetric tensors of rank 4 For symmetric tensors such as those representing principal properties, one ﬁnds the following, representing the nonzero components for the leading diagonal and for one half of the others. 1.1.4.9.9.1. Triclinic system

with

t1111 t1122 ¼ t1212 þ t1221 :

There are 15 independent components.

There are 45 independent coefﬁcients.

22

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS 32, 3m (ii) Groups 3m,

1.1.4.9.9.6. Hexagonal and cylindrical systems 6; ðA1 =MÞC; A1 (i) Groups 6=m, 6,

with with

t1111 t1122 ¼ t1212 þ t1221 :

t1111 t1122 ¼ t1212 þ t1221 :

There are 11 independent components.

There are 12 independent components. (ii) Groups 6=mm, 622, 6mm, 62m; ðA1 =MÞ1ðA2 =MÞC, A1 1A2

1.1.4.9.9.5. Tetragonal system (i) Groups 4=m, 4, 4

with t1111 t1122 ¼ t1212 þ t1221 : There are 10 independent components. There are 13 independent components.

1.1.4.9.9.7. Cubic system (i) Groups 23, 3m (ii) Groups 4=mm, 422, 4mm, 42m

with t1111 t1122 ¼ t1212 þ t1221 : There are 9 independent components. There are 5 independent components.

23

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 432, 43m, (ii) Groups m3m, and spherical system: the reduced tensors are already symmetric (see Sections 1.1.4.9.7 and 1.1.4.9.8).

The terms of the leading diagonal correspond to principal normal constraints and the non-diagonal terms to shears (see Section 1.3.2). 1.1.4.10.3. Reduction of the number of independent components of third-rank polar tensors due to the symmetry of the strain and stress tensors Equation (1.1.4.5) can be written P P Pi ¼ dijj Tjj þ ðdijk þ dikj ÞTjk :

1.1.4.10. Reduced form of polar and axial tensors – matrix representation 1.1.4.10.1. Introduction Many tensors representing physical properties or physical quantities appear in relations involving symmetric tensors. Consider, for instance, the strain Sij resulting from the application of an electric ﬁeld E (the piezoelectric effect): Sij ¼ dijk Ek þ Qijkl Ek El ;

j

The sums ðdijk þ dikj Þ for j 6¼ k have a deﬁnite physical meaning, but it is impossible to devise an experiment that permits dijk and dikj to be measured separately. It is therefore usual to set them equal:

ð1:1:4:4Þ

where the ﬁrst-order terms dijk represent the components of the third-rank converse piezoelectric tensor and the second-order terms Qijkl represent the components of the fourth-rank electrostriction tensor. In a similar way, the direct piezoelectric effect corresponds to the appearance of an electric polarization P when a stress Tjk is applied to a crystal: Pi ¼ dijk Tjk :

j6¼k

dijk ¼ dikj :

ð1:1:4:7Þ

It was seen in Section 1.1.4.8.1 that the components of a thirdrank tensor can be represented as a 9 3 matrix which can be subdivided into three 3 3 submatrices: 1 j 2 j 3 :

ð1:1:4:5Þ

Owing to the symmetry properties of the strain and stress tensors (see Sections 1.3.1 and 1.3.2) and of the tensor product Ek El , there occurs a further reduction of the number of independent components of the tensors which are engaged in a contracted product with them, as is shown in Section 1.1.4.10.3 for third-rank tensors and in Section 1.1.4.10.5 for fourth-rank tensors.

Relation (1.1.4.7) shows that submatrices 1 and 2 are identical. One puts, introducing a two-index notation, dijj ¼ di ð ¼ 1; 2; 3Þ dijk þ dikj ðj 6¼ kÞ ¼ di ð ¼ 4; 5; 6Þ: Relation (1.1.4.7) becomes Pi ¼ di T :

1.1.4.10.2. Stress and strain tensors – Voigt matrices The stress and strain tensors are symmetric because body torques and rotations are not taken into account, respectively (see Sections 1.3.1 and 1.3.2). Their components are usually represented using Voigt’s one-index notation. (i) Strain tensor 9 S1 ¼ S11 ; S2 ¼ S22 ; S3 ¼ S33 ; = S5 ¼ S31 þ S13 ; S6 ¼ S12 þ S21 ; S4 ¼ S23 þ S32 ; ; S4 ¼ 2S23 ¼ 2S32 ; S5 ¼ 2S31 ¼ 2S13 ; S6 ¼ 2S12 ¼ 2S21 :

The coefﬁcients di may be written as 0 11 12 13 14 15 @ 21 22 23 24 25 31 32 33 34 35

a 3 6 matrix: 1 16 26 A: 36

This matrix is constituted by two 3 3 submatrices. The left-hand one is identical to the submatrix 1, and the right-hand one is equal to the sum of the two submatrices 2 and 3: 1 j 2þ3 :

ð1:1:4:6Þ

The inverse piezoelectric effect expresses the strain in a crystal submitted to an applied electric ﬁeld:

The Voigt components S form a Voigt matrix: 0 1 S1 S6 S5 @ S2 S4 A: S3

Sij ¼ dijk Ek ; where the matrix associated with the coefﬁcients dijk is a 9 3 matrix which is the transpose of that of the coefﬁcients used in equation (1.1.4.5), as shown in Section 1.1.1.4. The components of the Voigt strain matrix S are then given by S ¼ diik Ek ð ¼ 1; 2; 3Þ S ¼ Sij þ Sji ¼ ðdijk þ djik ÞEk ð ¼ 4; 5; 6Þ:

The terms of the leading diagonal represent the elongations (see Section 1.3.1). It is important to note that the non-diagonal terms, which represent the shears, are here equal to twice the corresponding components of the strain tensor. The components S of the Voigt strain matrix are therefore not the components of a tensor. (ii) Stress tensor T1 ¼ T11 ; T2 ¼ T22 ; T3 ¼ T33 ; T4 ¼ T23 ¼ T32 ; T5 ¼ T31 ¼ T13 ; T6 ¼ T12 ¼ T21 :

This relation can be written simply as S ¼ dk Ek ; where the matrix of the coefﬁcients dk is a 6 3 matrix which is the transpose of the di matrix. There is another set of piezoelectric constants (see Section 1.1.5) which relates the stress, Tij , and the electric ﬁeld, Ek , which are both intensive parameters:

The Voigt components T form a Voigt matrix: 0 1 T 1 T6 T5 @ T2 T4 A : T3

Tij ¼ eijk Ek ;

24

ð1:1:4:8Þ

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS where a new piezoelectric tensor is introduced, eijk . Its components can be represented as a 3 9 matrix: 0 1 1 BC B C B 2 C: B C @A 3

(ii) Group mm2:

Both sides of relation (1.1.4.8) remain unchanged if the indices i and j are interchanged, on account of the symmetry of the stress tensor. This shows that

1.1.4.10.4.4. Trigonal system (i) Group 3:

There are 5 independent components. (iii) Group mmm: all the components are equal to zero.

eijk ¼ ejik : Submatrices 2 and 3 are equal. One introduces here a twoindex notation through the relation ek ¼ eijk , and the ek matrix can be written 1 : 2þ3

where the symbol means that the corresponding component is equal to the opposite of that to which it is linked, means that the component is equal to twice minus the value of the component to which it is linked for dijk and to minus the value of the component to which it is linked for eijk . There are 6 independent components. (ii) Group 32, twofold axis parallel to Ox1 :

The relation between the full and the reduced matrix is therefore different for the dijk and the ekij tensors. This is due to the particular property of the strain Voigt matrix (1.1.4.6), and as a consequence the relations between nonzero components of the reduced matrices are different for certain point groups (3, 32, 3m, 62m). 6, 1.1.4.10.4. Independent components of the matrix associated with a third-rank polar tensor according to the following point groups 1.1.4.10.4.1. Triclinic system (i) Group 1: all the components are independent. There are 18 components. all the components are equal to zero. (ii) Group 1:

with the same conventions. There are 4 independent components. (iii) Group 3m, mirror perpendicular to Ox1 :

with the same conventions. There are 4 independent components. all the components are equal to zero. (iv) Groups 3 and 3m:

1.1.4.10.4.2. Monoclinic system (i) Group 2: twofold axis parallel to Ox2 :

1.1.4.10.4.5. Tetragonal, hexagonal and cylindrical systems (i) Groups 4, 6 and A1 :

There are 8 independent components. (ii) Group m: There are 4 independent components. (ii) Groups 422, 622 and A1 1A2 :

There are 10 independent components. (iii) Group 2=m: all the components are equal to zero. 1.1.4.10.4.3. Orthorhombic system (i) Group 222:

There is 1 independent component. (iii) Groups 4mm, 6mm and A1 1M:

There are 3 independent components.

There are 3 independent components.

25

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES (iv) Groups 4=m, 6=m and ðA1 =MÞC: all the components are equal to zero. (v) Group 4:

1.1.4.10.5. Reduction of the number of independent components of fourth-rank polar tensors due to the symmetry of the strain and stress tensors Let us consider ﬁve examples of fourth-rank tensors: (i) Elastic compliances, sijkl , relating the resulting strain tensor Sij to an applied stress Tij (see Section 1.3.3.2): Sij ¼ sijkl Tkl ;

ð1:1:4:9Þ

where the compliances sijkl are the components of a tensor of rank 4. (ii) Elastic stiffnesses, cijkl (see Section 1.3.3.2):

There are 4 independent components. (vi) Group 6 ¼ 3=m:

Tij ¼ cijkl Skl : (iii) Piezo-optic coefﬁcients, ijkl , relating the variation ij of the dielectric impermeability to an applied stress Tkl (photoelastic effect – see Section 1.6.7):

with the same conventions as for group 3. There are 2 independent components. (vii) Group 42m – twofold axis parallel to Ox1 :

ij ¼ ijkl Tkl : (iv) Elasto-optic coefﬁcients, pijkl , relating the variation ij of the dielectric impermeability to the strain Skl : ij ¼ pijkl Skl :

There are 2 independent components. (viii) Group 42m – mirror perpendicular to Ox1 (twofold axis

at 45 ):

(v) Electrostriction coefﬁcients, Qijkl , which appear in equation (1.1.4.4): Sij ¼ Qijkl Ek El ;

ð1:1:4:10Þ

where only the second-order terms are considered. In each of the equations from (1.1.4.9) to (1.1.4.10), the contracted product of a fourth-rank tensor by a symmetric second-rank tensor is equal to a symmetric second-rank tensor. As in the case of the third-rank tensors, this results in a reduction of the number of independent components, but because of the properties of the strain Voigt matrix, and because two of the tensors are endowed with intrinsic symmetry (the elastic tensors), the reduction is different for each of the ﬁve tensors. The above relations can be written in matrix form:

The number of independent components is of course the same. (ix) Group 62m:

with the same conventions as for group 3. There is 1 independent component. (x) Groups 4=mm, 6=mm and ðA1 =MÞ1ðA2 =MÞC: all the components are equal to zero. where the second-rank tensors are represented by 1 9 column matrices, which can each be subdivided into three 1 3 submatrices and the 9 9 matrix associated with the fourth-rank tensors is subdivided into nine 3 3 submatrices, as shown in Section 1.1.4.9.1. The symmetry of the second-rank tensors means that submatrices 2 and 3 which are associated with them are equal. Let us ﬁrst consider the reduction of the tensor of elastic compliances. As in the case of the piezoelectric tensor, equation (1.1.4.9) can be written P P ð1:1:4:11Þ Sij ¼ sijll Tll þ ðsijkl þ sijlk ÞTkl :

1.1.4.10.4.6. Cubic and spherical systems (i) Groups 23 and 43m:

There is 1 independent component. (ii) Groups 432 and 1A1 : it was seen in Section 1.1.4.8.6 that we have in this case

l

k6¼l

The sums ðsijkl þ sijlk Þ for k 6¼ l have a deﬁnite physical meaning, but it is impossible to devise an experiment permitting sijkl and sijlk to be measured separately. It is therefore usual to set them equal in order to avoid an unnecessary constant:

d123 ¼ d132 : It follows that d14 ¼ 0, all the components are equal to zero. m3m and 1ðA1 =MÞC: all the components (iii) Groups m3, are equal to zero.

sijkl ¼ sijlk :

26

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS (ii) Piezo-optic coefﬁcients, ijkl :

Furthermore, the left-hand term of (1.1.4.11) remains unchanged if we interchange the indices i and j. The terms on the right-hand side therefore also remain unchanged, whatever the value of Tll or Tkl . It follows that sijll ¼ sjill sijkl ¼ sijlk ¼ sjikl ¼ sjilk :

where i ¼ j; i ¼ j; i 6¼ j; i 6¼ j;

Similar relations hold for cijkl , Qijkl , pijkl and ijkl : the submatrices 2 and 3, 4 and 7, 5, 6, 8 and 9, respectively, are equal. Equation (1.4.1.11) can be rewritten, introducing the coefﬁcients of the Voigt strain matrix: P P S ¼ Sii ¼ siill Tll þ ðsiikl þ siilk ÞTkl ð ¼ 1; 2; 3Þ l

S ¼ Sij þ Sji ¼

P

k6¼l

ðsijll þ sjill ÞTll l P þ ðsijkl þ sijlk þ sjikl þ sjilk ÞTkl

k ¼ l; k 6¼ l; k ¼ l; k 6¼ l;

9 ¼ iill > > = ¼ iikl þ iilk ¼ ijkk ¼ jikk > > ; ¼ ijkl þ jikl ¼ ijlk þ jilk :

(iii) Electrostriction coefﬁcients, Qijkl : same relation as for the elastic compliances. 1.1.4.10.6. Independent components of the matrix associated with a fourth-rank tensor according to the following point groups 1 1.1.4.10.6.1. Triclinic system, groups 1,

ð ¼ 4; 5; 6Þ:

k6¼l

We shall now introduce a two-index notation for the elastic compliances, according to the following conventions: 9 i ¼ j; k ¼ l; s ¼ siill > > = i ¼ j; k 6¼ l; s ¼ siikl þ siilk ð1:1:4:12Þ i 6¼ j; k ¼ l; s ¼ sijkk þ sjikk > > ; i 6¼ j; k 6¼ l; s ¼ sijkl þ sjikl þ sijlk þ sjilk : We have thus associated with the fourth-rank tensor a square 6 6 matrix with 36 coefﬁcients:

1.1.4.10.6.2. Monoclinic system Groups 2=m, 2, m, twofold axis parallel to Ox2 :

One can translate relation (1.1.4.12) using the 9 9 matrix representing sijkl by adding term by term the coefﬁcients of submatrices 2 and 3, 4 and 7 and 5, 6, 8 and 9, respectively:

Using the two-index notation, equation (1.1.4.9) becomes S ¼ s T :

ð1:1:4:13Þ

1.1.4.10.6.3. Orthorhombic system Groups mmm, 2mm, 222:

A similar development can be applied to the other fourth-rank tensors ijkl, which will be replaced by 6 6 matrices with 36 coefﬁcients, according to the following rules. (i) Elastic stiffnesses, cijkl and elasto-optic coefﬁcients, pijkl :

where c ¼ cijkl p ¼ pijkl :

27

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.1.4.10.6.4. Trigonal system (i) Groups 3, 3:

with the same conventions. The sign of c14 depends on the orientation of the Ox1 axis.

1.1.4.10.6.5. Tetragonal system (i) Groups 4, 4 and 4=m:

(ii) Groups 422, 4mm, 42m and 4=mm: where is a component numerically equal but opposite in sign to the heavy dot component to which it is linked; is a component equal to twice the heavy dot component to which it is linked; is a component equal to minus twice the heavy dot component to which it is linked; is equal to 1=2ðp11 p12 Þ, ð 11 12 Þ, 2ðQ11 Q12 Þ, 1=2ðc11 c12 Þ and 2ðs11 s12 Þ, respectively. (ii) Groups 32, 3m, 3m:

1.1.4.10.6.6. Hexagonal system (i) Groups 6, 6 and 6=m:

28

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS 1.1.4.10.6.8. Spherical system For all tensors

(ii) Groups 622, 6mm, 62m and 6=mm:

1.1.4.10.7. Reduction of the number of independent components of axial tensors of rank 2 It was shown in Section 1.1.4.5.3.2 that axial tensors of rank 2 are actually tensors of rank 3 antisymmetric with respect to two indices. The matrix of independent components of a tensor such that gijk ¼ gjik is given by 0 @ 121 131

122

232

133 123 223 233

131 231

132 122 232 132

121 123 133

1 A:

231

The second-rank axial tensor gkl associated with this tensor is deﬁned by 1.1.4.10.6.7. Cubic system (i) Groups 23 and 3m:

gkl ¼ 12"ijk gijl : For instance, the piezomagnetic coefﬁcients that give the magnetic moment Mi due to an applied stress T are the components of a second-rank axial tensor, i (see Section 1.5.7.1): Mi ¼ i T :

1.1.4.10.7.1. Independent components according to the following point groups (i) Triclinic system (a) Group 1: (ii) Groups 432, 43m and m3m:

all components are equal to zero. (b) Group 1: (ii) Monoclinic system (a) Group 2:

29

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES (b) Group m:

(v) Cubic and spherical systems (a) Groups 23, 432 and 1A1 :

(c) Group 2=m: all components are equal to zero.

The axial tensor is reduced to a pseudoscalar. 43m, and 1ðA1 =MÞC: all components (b) Groups m3, m3m are equal to zero.

(iii) Orthorhombic system (a) Group 222:

1.1.4.10.7.2. Independent components of symmetric axial tensors according to the following point groups Some axial tensors are also symmetric. For instance, the optical rotatory power of a gyrotropic crystal in a given direction of direction cosines 1; 2 ; 3 is proportional to a quantity G deﬁned by (see Section 1.6.5.4) (b) Group mm2:

G ¼ gij i j ; where the gyration tensor gij is an axial tensor. This expression shows that only the symmetric part of gij is relevant. This leads to a further reduction of the number of independent components: (i) Triclinic system (a) Group 1:

(c) Group mmm: all components are equal to zero. (iv) Trigonal, tetragonal, hexagonal and cylindrical systems (a) Groups 3, 4, 6 and A1 :

all components are equal to zero. (b) Group 1: (ii) Monoclinic system (a) Group 2: (b) Groups 32, 42, 62 and A1 1A2 :

(b) Group m: (c) Groups 3m, 4m, 6m and A1 1M:

(c) Group 2=m: all components are equal to zero. (iii) Orthorhombic system (a) Group 222:

(d) Group 4:

(e) Group 42m: (b) Group mm2:

4=m, 62m, 4=mm and 6=mm: all components (f) Groups 3, 3m, are equal to zero.

(c) Group mmm: all components are equal to zero.

30

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS @G @G @G (iv) Trigonal, tetragonal and hexagonal systems : ; Dn ¼ ; ¼ Skl ¼ (a) Groups 3, 32, 4, 42, 6, 62: @Tkl @En @ Each of these quantities may be expanded by performing a further differentiation in terms of the intensive parameters, Tkl , En and . We have, to the ﬁrst order, @Skl @Skl @Skl dSkl ¼ dT þ dE þ @Tij E; ij @En T; n @ E;T @Dn @Dn @Dn dDn ¼ dTkl þ dEm þ @Tkl E; @Em T; @ E;T @ @ @ d ¼ dTij þ dEm þ : @Tij E; @Em T; @ E;T

(b) Group 4:

(c) Group 42m:

To a ﬁrst approximation, the partial derivatives may be considered as constants, and the above relations may be integrated: 9 E; > Tij þ ðdkln ÞT; En þ ðkl ÞE;T Skl ¼ sklij = E; T; E;T Dn ¼ ðdnkl Þ Tkl þ ð"nm Þ Em þ ðpn Þ > E ; þ ðpm ÞT Em þ ð CE;T =Þ: ¼ ij Tij

62m 3m, 3m, 4=m, 4mm, 4=mm, 6, (d) Groups 3, and 6=mm: all components are equal to zero. (v) Cubic and spherical systems (a) Groups 23, 432 and A1 1A2 :

ð1:1:5:1Þ This set of equations is the equivalent of relation (1.1.1.6) of Section 1.1.1.3, which gives the coefﬁcients of the matrix of physical properties. These coefﬁcients are: E; (i) For the principal properties: sklij : elastic compliances at T; constant temperature and ﬁeld; ð"nm Þ : dielectric constant at constant temperatures and stress; CT;E : heat capacity per unit volume at constant stress and ﬁeld ( is the speciﬁc mass and CT;E is the speciﬁc heat at constant stress and ﬁeld). (ii) For the other properties: ðdkln ÞT; and ðdnkl ÞE; are the components of the piezoelectric effect and of the converse effect. They are represented by 3 9 and 9 3 matrices, respectively. One may notice that

43m, and 1ðA1 =MÞC: all components (b) Groups m3, m3m are equal to zero. In practice, gyrotropic crystals are only found among the enantiomorphic groups: 1, 2, 222, 3, 32, 4, 422, 6, 622, 23, 432. Pasteur (1848a,b) was the ﬁrst to establish the distinction between ‘molecular dissymmetry’ and ‘crystalline dissymetry’.

dkln ¼

@Skl @2 G @2 G @Dn ¼ ¼ ¼ ¼ dnkl ; @En @Tkl @Tkl @En @Tkl @En

which shows again that the components of two properties that are symmetric with respect to the leading diagonal of the matrix of physical properties are equal (Section 1.1.1.4) and that the corresponding matrices are transpose to one another. In a similar way, (a) the matrices ðkl ÞE;T of the thermal expansion and ðij ÞE of the piezocaloriﬁc effect are transpose to one another; (b) the components ðpn ÞT of the pyroelectric and of the electrocaloric effects are equal.

1.1.5. Thermodynamic functions and physical property tensors [The reader may also consult Mason (1966), Nye (1985) or Sirotin & Shaskol’skaya (1982).] 1.1.5.1. Isothermal study The energy of a system is the sum of all the forms of energy: thermal, mechanical, electrical etc. Let us consider a system whose only variables are these three. For a small variation of the associated extensive parameters, the variation of the internal energy is

Remark. The piezoelectric effect, namely the existence of an electric polarization P under an applied stress, is always measured at zero applied electric ﬁeld and at constant temperature. The second equation of (1.1.5.1) becomes under these circumstances

dU ¼ En dDn þ Tkl dSkl þ d; where is the temperature and is the entropy; there is summation over all dummy indices; an orthonormal frame is assumed and variance is not apparent. The mechanical energy of deformation is given by Tkl dSkl (see Section 1.3.2.8). Let us consider the Gibbs free-energy function G deﬁned by

Pn ¼ Dn ¼ ðdnkl Þ Tkl : Remark. Equations (1.1.5.1) are, as has been said, ﬁrst-order approximations because we have assumed the partial derivatives to be constants. Actually, this approximation is not correct, and in many cases it is necessary to take into account the higher-order terms as, for instance, in: (a) nonlinear elasticity (see Sections 1.3.6 and 1.3.7); (b) electrostriction; (c) nonlinear optics (see Chapter 1.7); (d) electro-optic and piezo-optic effects (see Sections 1.6.6 and 1.6.7).

G ¼ U En Dn Tkl Skl : Differentiation of G gives dG ¼ Dn dEn Skl dTkl d: The extensive parameters are therefore partial derivatives of the free energy:

31

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES also called real pyroelectric coefﬁcients, pSn . Let us put Tij ¼ 0 and En ¼ 0 in the ﬁrst equation of (1.1.5.1). For a given variation of temperature, , the observed strain is h iE;T : Skl ¼ kl

1.1.5.2. Other forms of the piezoelectric constants We use here another Gibbs function, the electric Gibbs function, G2 , deﬁned by G2 ¼ U En Dn : Differentiation of G gives

From the second equations of (1.1.5.1) and (1.1.5.2), it follows that

dG2 ¼ Dn dEn þ Tij dSij d:

Dn ¼ pTn Dn ¼ enkl Skl þ pn :

It follows that Tij ¼

@G2 ; @Sij

Dn ¼

@G2 ; @En

¼

@G2 @

Substituting the expression Skl and eliminating Dn , it follows that h iE;T pTn ¼ enkl kl þ pSn : ð1:1:5:3Þ

and a set of relations analogous to (1.1.5.1): Tij ¼ ðcijkl ÞE; Skl Dn ¼ ðenij ÞE; Sij ¼ ð ij ÞE Sij

ðeijn ÞS; En þ ð"nm ÞS; Em þ ðpn ÞS En

9 ð ij ÞE;S > = ð1:1:5:2Þ þ ðpn ÞS > ; E;S þ C =;

This relation shows that part of the pyroelectric effect is actually due to the piezoelectric effect. 1.1.5.4. Adiabatic study Piezoelectric resonators usually operate at a high frequency where there are no heat exchanges, and therefore in an adiabatic regime ð ¼ 0Þ. From the third equation of (1.1.5.1), we obtain a relation between the temperature variation, the applied stress and the electric ﬁeld:

E; are the isothermal elastic stiffwhere the components cijkl nesses at constant ﬁeld and constant temperature, eijn ¼

@Tij @2 G 2 @2 G2 @Dn ¼ ¼ ¼ ¼ enij @En @En @Sij @Sij @En @Sij

are the piezoelectric stress coefﬁcients at constant strain and constant temperature,

ij ¼

ðij ÞE Tij þ ðpm ÞT Em þ

@Tij @2 G2 @2 G 2 @ ¼ ¼ ¼ @ @@Sij @Sij @ @Sij

If we substitute this relation in the two other relations of (1.1.5.1), we obtain two equivalent relations, but in the adiabatic regime: E; Skl ¼ sklij Tij þ ðdklm ÞT; Em E; Dn ¼ dnij Tij þ ð"nm ÞT; Em :

are the temperature-stress constants and pn ¼

CT;E ¼ 0:

@Dn @2 G2 @2 G2 @ ¼ ¼ ¼ @ @@En @En @ @Dn

By comparing these expressions with (1.1.5.1), we obtain the following relations between the adiabatic and the isothermal coefﬁcients:

are the components of the pyroelectric effect at constant strain. The relations between these coefﬁcients and the usual coefﬁcients dkln are easily obtained: (i) At constant temperature and strain: if one puts ¼ 0 and Skl ¼ 0 in the ﬁrst equation of (1.1.5.1) and (1.1.5.2), one obtains, respectively,

ðij ÞE ðkl ÞE CT;E ðp ÞT ðkl ÞE ¼ ðdnij ÞE; n T;E C ðp ÞT ðpm ÞT ¼ ð"mn ÞT; n T;E : C

ðsijkl ÞE; ¼ ðsijkl ÞE;

0 ¼ sklij Tij þ dkln En

ðdnij ÞE;

Tij ¼ eijn En ; ð"mn ÞT;

from which it follows that dkln ¼ sklij eijn

1.1.6. Glossary

at constant temperature and strain. (ii) At constant temperature and stress: if one puts ¼ 0 and Tij ¼ 0, one obtains in a similar way

ei ei xi

Skl ¼ dkln En 0 ¼ cijkl Skl eijn En ;

xi from which it follows that gij

eijn ¼ cijkl dkln

j ...j

ti11 ...ipq

at constant temperature and stress.

AT V

1.1.5.3. Relation between the pyroelectric coefﬁcients at constant stress and at constant strain By combining relations (1.1.5.1) and (1.1.5.2), it is possible to obtain relations between the pyroelectric coefﬁcients at constant stress, pTn , and the pyroelectric coefﬁcients at constant strain, pSn ,

^ @i ji "ijk

32

basis vectors in direct space (covariant) basis vectors in reciprocal space (contravariant) components of a vector in direct space (contravariant) components of a vector in reciprocal space (covariant) components of the metric tensor components of a tensor of rank n, p times covariant and q times contravariant (n ¼ p þ q) transpose of matrix A tensor product outer product vector product partial derivative with respect to xi Kronecker symbol permutation tensor

1.1. INTRODUCTION TO THE PROPERTIES OF TENSORS V p ui Sij S Tij T sijkl s ðsijkl Þ cijkl c E ij

ij U G CE;T E D H B "o " "ij ð"ij Þ e ij pi dijk di di ðdijk Þ eijk Qijkl Q ijkl pijkl p RH ijk

Fumi, F. G. (1952a). Physical properties of crystals: the direct inspection method. Acta Cryst. 5, 44–48. Fumi, F. G. (1952b). The direct-inspection method in systems with a principal axis of symmetry. Acta Cryst. 5, 691–694. Fumi, F. G. (1952c). Third-order elastic coefﬁcients in trigonal and hexagonal crystals. Phys. Rev. 86, 561. Fumi, F. G. (1987). Tables for the third-order elastic tensors in crystals. Acta Cryst. A43, 587–588. Fumi, F. G. & Ripamonti, C. (1980a). Tensor properties and rotational symmetry of crystals. I. A new method for group 3(3z) and its application to general tensors up to rank 8. Acta Cryst. A36, 535–551. Fumi, F. G. & Ripamonti, C. (1980b). Tensor properties and rotational symmetry of crystals. II. Groups with 1-, 2- and 4-fold principal symmetry and trigonal and hexagonal groups different from group 3. Acta Cryst. A36, 551–558. Ikeda, T. (1990). Fundamentals of Piezoelectricity. Oxford University Press. International Tables for Crystallography (2005). Vol. A, Space-Group Symmetry, edited by Th. Hahn. Heidelberg: Springer. International Tables for Crystallography (2008). Vol. B, Reciprocal Space, edited by U. Shmueli. Heidelberg: Springer. Kumaraswamy, K. & Krishnamurthy, N. (1980). The acoustic gyrotropic tensor in crystals. Acta Cryst. A36, 760–762. Lichnerowicz, A. (1947). Alge`bre et analyse line´aires. Paris: Masson. Lippmann, G. (1881). Principe de conservation de l’e´lectricite´. Ann. Chim. Phys. 24, 145–178. Mason, W. P. (1966). Crystal Physics of Interaction Processes. London: Academic Press. Neumann, F. (1832). Theorie der doppelten Strahlenbrechung, abgeleitet den Gleichungen der Mechanik. Poggendorf Ann. Phys. Chem. 25, 418–454. Neumann, F. (1833). Die thermischen, optischen und kristallographischen Axen des Kristallsystems des Gypses. Poggendorf Ann. Phys. Chem. 27, 240–274. ¨ ber das Elastizita¨tsmass kirstallinscher Substanzen Neumann, F. (1834). U der homoe¨drischen Abteilung. Poggendorf Ann. Phys. Chem. 31, 177– 192. Neumann, F. (1885). Vorlesungen u¨ber die Theorie der Elastizita¨t der festen Ko¨rper und des Lichta¨thers, edited by O. E. Meyer. Leipzig: B. G. Teubner-Verlag. Newnham, R. E. (2005). Properties of Materials: Anisotropy, Symmetry, Structure. Oxford University Press. Nowick, A. S. (1995). Crystal Properties via Group Theory. Cambridge University Press. Nye, J. F. (1957). Physical Properties of Crystals, 1st ed. Oxford: Clarendon Press. Nye, J. F. (1985). Physical Properties of Crystals, revised ed. Oxford University Press. Onsager, L. (1931a). Reciprocal relations in irreversible processes. I. Phys. Rev. 37, 405–426. Onsager, L. (1931b). Reciprocal relations in irreversible processes. II. Phys. Rev. 38, 2265–2279. Pasteur, L. (1848a). Recherches sur les relations qui peuvent exister entre la forme cristalline, la composition chimique et le sens de la polarisation rotatoire. Ann. Chim. (Paris), 24, 442–459. Pasteur, L. (1848b). Me´moire sur la relation entre la forme cristalline et la composition chimique, et sur la cause de la polarisation rotatoire. C. R. Acad Sci. 26, 535–538. Pauﬂer, P. (1986). Physikalische Kristallographie. Berlin: AkademieVerlag. Sands, D. E. (1995). Vectors and Tensors in Crystallography. New York: Dover. Schwartz, L. (1975). Les tenseurs. Paris: Hermann. Shuvalov, L. A. (1988). Modern Crystallography IV (Physical Properties of Crystals). Berlin: Springer-Verlag Sirotin, Y. I. & Shaskol’skaya, M. P. (1982). Fundamentals of Crystal Physics. Moscow: Mir. Voigt, W. (1910). Lehrbuch der Kristallphysik. Leipzig: Teubner. 2nd ed. (1929); photorep. (1966). New York: Johnson Reprint Corp. and Leipzig: Teubner. Wooster, W. A. (1973). Tensors and Group Theory for the Physical Properties of Crystals. Oxford: Clarendon Press. Zheludev, I. S. (1986). Space and time inversion in physical crystallography. Acta Cryst. A42, 122–127.

volume pressure components of the displacement vector components of the strain tensor components of the strain Voigt matrix components of the stress tensor components of the stress Voigt matrix elastic compliances reduced elastic compliances adiabatic elastic compliances elastic stiffnesses reduced elastic stiffnesses Poisson’s ratio Young’s modulus temperature entropy thermal expansion temperature-stress constant internal energy Gibbs free energy speciﬁc heat at constant stress and applied electric ﬁeld electric ﬁeld electric displacement magnetic ﬁeld magnetic induction permittivity of vacuum dielectric constant dielectric tensor adiabatic dielectric tensor dielectric susceptibility dielectric impermeability pyroelectric tensor piezoelectric tensor reduced piezoelectric tensor reduced inverse piezoelectric tensor adiabatic piezoelectric tensor piezoelectric tensor at constant strain electrostriction tensor reduced electrostriction tensor piezo-optic tensor reduced piezo-optic tensor elasto-optic tensor reduced elasto-optic tensor Hall constant

References Bhagavantam, S. (1966). Crystal Symmetry and Physical Properties. London: Academic Press. Billings, A. (1969). Tensor Properties of Materials. London/New York: Wiley Interscience. Brillouin, L. (1949). Les tenseurs en me´canique et en e´lasticite´. Paris: Masson & Cie. Cady, W. G. (1964). Piezoelectricity. New York: Dover. Curie, J. & Curie, P. (1880). De´veloppement par pression de l’e´lectricite´ polaire dans les cristaux he´mie`dres a` faces incline´es. C. R. Acad. Sci. 91, 294–295. Curie, J. & Curie, P. (1881). Contractions et dilatations produites par des tensions e´lectriques dans les cristaux he´mie`dres a` faces incline´es. C. R. Acad. Sci. 93, 1137–1140. Curie, P. (1884). Sur les questions d’ordre: re´pe´titions. Bull. Soc. Fr. Mine´ral. 7, 89–110. Curie, P. (1894). Sur la syme´trie dans les phe´nome`nes physiques, syme´trie d’un champ e´lectrique et d’un champ magne´tique. J. Phys. (Paris), 3, 393–415. Fumi, F. G. (1951). Third-order elastic coefﬁcients of crystals. Phys. Rev. 83, 1274–1275.

33

references

International Tables for Crystallography (2013). Vol. D, Chapter 1.2, pp. 34–71.

1.2. Representations of crystallographic groups By T. Janssen 0

1.2.1. Introduction Symmetry arguments play an important role in science. Often one can use them in a heuristic way, but the correct formulation is in terms of group theory. This remark is in fact superﬂuous for crystallographers, who are used to point groups and space groups as they occur in the description of structures. However, besides these structural problems there are many others where group theory may play a role. A central role in this context is played by representation theory, which treats the action of a group on physical quantities, and usually this is done in terms of linear transformations, although nonlinear representations may also occur. To start with an example, consider a spin system, an arrangement of spins on sites with a certain symmetry, for example spacegroup symmetry. The elements of the space group map the sites onto other sites, but at the same time the spins are rotated or transformed otherwise in a well deﬁned fashion. The spins can be seen as elements of a vector space (spin space) and the transformation in this space is an image of the space-group element. In a similar way, all symmetric tensors of rank 2 form a vector space, because one can add them and multiply them by a real factor. A linear change of coordinates changes the vectors, and the transformations in the space of tensors are the image of the coordinate transformations. Probably the most important use of such representations is in quantum mechanics, where transformations in coordinate space are mapped onto linear transformations in the quantum mechanical space of state vectors. To see the relation between groups of transformations and the use of their representations in physics, consider a tensor which transforms under a certain point group. Let us take a symmetric rank 2 tensor Tij in three dimensions. We take as example the point group 222. From Section 1.1.3.2 one knows how such a tensor transforms: it transforms into a tensor Tij0 according to Tij0 ¼

3 P 3 P

Rik Rjm Tkm

a11 B @ a12 a13

a23

a33

1 0

0

a11 B @ a12 a13

a12

0

a22 a23

1 B ¼@ 0 0

0 1 0 a13

0

10

a11

CB 0 [email protected] a12 1 a13 1

a12

0 1 0

10 0 a11 CB 0 [email protected] a12 1 a13

a13

10

1

a22

CB a23 [email protected] 0

a23

a33

a12 a22

10 1 a13 CB a23 [email protected] 0

a23

a33

C a23 A a33

and the solution of 0 a11 @ a12 a13

these equations is 1 0 a11 a12 a13 a22 a23 A ¼ @ 0 a23 a33 0

0

0

0 a22 0

0 1 0

0 1 0

0

1

C 0 A; 1

1 0 C 0 A 1

1 0 0 A: a33

The matrices of rank 2 form a nine-dimensional vector space. The rotation over 180 around the x axis can also be written as 10 1 0 1 0 a11 1 0 0 0 0 0 0 0 0 a11 C B a C B 0 1 0 B 0 0 0 0 0 0 CB a12 C C B 12 C B CB C B C B B a13 C B 0 0 1 0 0 0 0 0 0 CB a13 C CB C B C B CB C B C B 0 1 0 0 0 0 0 CB a21 C B a21 C B 0 0 CB C B C B C B B C 0 0 1 0 0 0 0C RB CB a22 C: B a22 C ¼ B 0 0 CB C B C B 0 0 0 1 0 0 0 CB a23 C B a23 C B 0 0 CB C B C B B a31 C B 0 0 B C 0 0 0 0 1 0 0 C CB a31 C B C B CB C B C B 0 0 0 0 0 1 0 [email protected] a32 A @ a32 A @ 0 0 0 0 0 0 0 0 0 0 1 a33 a33

ð1:2:1:1Þ

for all orthogonal transformations R in the group 222. This action of the point group 222 is obviously a linear one: 0 c1 Tijð1Þ þ c2 Tijð2Þ ¼ c1 Tijð1Þ0 þ c2 Tijð2Þ0 :

This nine-dimensional matrix together with the one corresponding to a rotation along the y axis generate a representation of the group 222 in the nine-dimensional space of three-dimensional rank 2 tensors. The invariant tensors form the subspace (a11 ; 0; 0; 0; a22 ; 0; 0; 0; a33 ). In this simple case, group theory is barely needed. However, in more complex situations, the calculations may become quite cumbersome without group theory. Moreover, group theory may give a wealth of other information, such as selection rules and orthogonality relations, that can be obtained only with much effort without group theory, or in particular representation theory. Tables of tensor properties, and irreducible representations of point and space groups, have been in use for a long time. For point groups see, for example, Butler (1981) and Altmann & Herzig (1994); for space groups, see Miller & Love (1967), Kovalev (1987) and Stokes & Hatch (1988). In the following, we shall discuss the representation theory of crystallographic groups. We shall adopt a slightly abstract language, which has the advantage of conciseness and generality, but we shall consider examples of the most important notions. Another point that could give rise to some problems is the fact that we shall consider in part the theory for crystallographic groups in arbitrary dimension. Of course, physics occurs in three-

The transformations on the tensors really form an image of the group, because if one writes DðRÞT for T 0 , one has for two elements Rð1Þ and Rð2Þ the relation DðRð1Þ Rð2Þ Þ T ¼ DðRð1Þ Þ DðRð2Þ ÞT or ð1:2:1:2Þ

This property is said to deﬁne a (linear) representation. Because of the representation property, it is sufﬁcient to know how the tensor transforms under the generators of a group. In our example, one could be interested in symmetric tensors that are invariant under the group 222. Then it is sufﬁcient to consider the rotations over 180 along the x and y axes. If the point group is a symmetry group of the system, a tensor describing the relation between two physical quantities should remain the same. For invariant tensors one has Copyright © 2013 International Union of Crystallography

1 a13 C a23 A

B ¼ @0

k¼1 m¼1

DðRð1Þ Rð2Þ Þ ¼ DðRð1Þ ÞDðRð2Þ Þ:

0

a12 a22

34

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS n1 n01 a n1 n02 a=2 n2 n01 a=2 þ n2 n02 a: dimensional space, but often it is useful to see what is general and what is special for one, two or three dimensions. In Section 1.2.2, the point groups are discussed, together with their representa- After a basis transformation, pﬃﬃﬃﬃﬃ pﬃﬃﬃ tions. In Section 1.2.3, the same is done for space groups. Tensors e1 ¼ a1 = a; e2 ¼ ða1 þ 2a2 Þ= 3a; for point and space groups are then treated in terms of representation theory in Section 1.2.4. Besides transformations in space, transformations involving time reversal are important as the metric tensor is in standard form (see Section 1.1.2.2): well. They are discussed in Section 1.2.5. Information on crysei ej ¼ ij : tallographic groups and their representations is presented in tabular form in Section 1.2.6. This section can be consulted This means that with respect to the basis e ; e , the three trans1 2 independently. formations become orthogonal matrices. To be able to give a list of all crystallographic point groups in n dimensions it is necessary to state which point groups should be 1.2.2. Point groups considered as different. Two point groups belong to the same 1.2.2.1. Finite point groups in one, two and three dimensions geometric crystal class if they are conjugated subgroups of O(n). 0 the same The crystallographic point groups are treated in Volume A of This means that K OðnÞ and K OðnÞ belong to 0 1 International Tables for Crystallography (2005). Here we just give class if there is an element R 2 OðnÞ such that K ¼ RKR , which implies that there are two orthonormal bases in the vector a brief summary of some important notions. To maintain generspace related by an orthogonal transformation R such that the ality, we consider the case of n-dimensional point groups. 0 Point groups in n dimensions are subgroups of the orthogonal matrices of K for one basis are the same as those for K on the group O(n) in n dimensions. By deﬁnition they leave a point, the second basis. In one-dimensional space, there are only two different point origin, invariant. They are of importance in physics because groups, the ﬁrst consisting of the identity, the second of the physical laws are invariant under such transformations. In this numbers 1. These groups are isomorphic to C1 and C2 , case n = 1, 2 or 3. For crystallography, the crystallographic point groups are the most relevant ones. A crystallographic point group respectively, where Cm is the cyclic group of integers modulo m is a subgroup of O(n) that leaves an n-dimensional lattice (also denoted by Zm ). Both are crystallographic because their 1 1 ‘matrices’ are the integers 1. invariant. A lattice is a collection of points In two-dimensional space, the orthogonal group O(2) is the n P union of the subgroup SO(2), consisting of all orthogonal r ¼ ro þ ni ei ; ni 2 Z; ð1:2:2:1Þ transformations with determinant þ1, and the coset O(2)\SO(2), i¼1 consisting of all orthogonal transformations with determinant where the n vectors ei form a basis of n-dimensional space. In 1. The group SO(2) is Abelian, and therefore all its subgroups The ﬁnite ones are the rotation groups denoted by n other words, the points of the lattice can be obtained by the are Abelian. (n 2 Zþ ). Every element of O(2)\SO(2) is of order two, and action of translations corresponds to a mirror line. Therefore, all the other ﬁnite point n P groups are nmm (n even) or nm (n odd). The rotation groups are t ¼ ni ei ð1:2:2:2Þ isomorphic with the cyclic groups C and the others with the n i¼1 dihedral groups Dn. Only the groups 1, 2, 3, 4, 6, m, 2mm, 3m, on the lattice origin ro . These translations form a lattice transla- 4mm and 6mm leave a lattice invariant and are crystallographic. The isomorphism class of a group can be given by its generators tion group in n-dimensional space, i.e. a discrete subgroup of the and deﬁning relations. For example, the elements of the group group of all translations T(n) in n dimensions, generated by n 4mm can be written as products (with generally more than two linearly independent translations. factors) of the two matrices Because a crystallographic point group leaves a lattice of points invariant, (a) it is a ﬁnite group of linear transformations 1 0 0 1 ; ; B¼ A¼ and (b) on a basis of the lattice it is represented by integer 0 1 1 0 matrices. On the other hand, as will be shown in Section 1.2.2.2, there is for every ﬁnite group of matrices an invariant scalar which satisfy the relations A4 ¼ B2 ¼ ABAB ¼ E, and every product, i.e. a positive deﬁnite metric tensor left invariant by the group whose elements are products of two generating elements group. If one uses this metric tensor for the deﬁnition of the with the same and not more independent relations is isomorphic. scalar product, the matrices represent orthogonal transforma- One calls the relations the deﬁning relations. The set of generations. Moreover, when the matrices are integer, the group of tors and deﬁning relations is not unique. In an extreme case, one matrices can be considered to be a crystallographic point group. can consider all elements of the group as generators, and the In this sense, every ﬁnite group of integer matrices is a crystal- product rules ab ¼ c as the deﬁning relations. lographic point group. Consider as an example the group of For the two-dimensional groups, the generators and deﬁning matrices relations are Cn : one generator A, with An ¼ E; 1 0 0 1 1 1 ; ; ; Dn : two generators A and B, with An ¼ B2 ¼ ðABÞ2 ¼ E, 0 1 1 1 1 0 where E is the unit element. The determination of all ﬁnite point groups in three-dimenwhich leaves invariant the metric tensor sional space is more involved. A derivation can, for example, be found in Janssen (1973). The group O(3) is again the union of a a=2 a1 a1 a1 a2 SO(3) and O(3)\SO(3), and in fact the direct product of SO(3) g¼ ¼ : a=2 a a2 a1 a2 a2 and the group generated by the inversion I ¼ E. One may distinguish between three different classes of ﬁnite point groups: The lattice points n1 a1 þ n2 a2 go over into lattice points and the (a) point groups that belong fully to the rotation group SO(3); transformation leaves the scalar product of two such vectors the (b) point groups that contain the inversion E and are, same if the scalar product of the two vectors n1 a1 þ n2 a2 and consequently, the direct product of a point group of the ﬁrst class n01 a1 þ n02 a2 is deﬁned as and the group generated by E;

35

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES where the matrices 1 ðRÞ form an m-dimensional matrix representation of K. In this situation, the representations DðKÞ and ðKÞ are called reducible. If there is no proper invariant subspace the representation is irreducible. If the representation is a direct sum of subspaces, each carrying an irreducible representation, the representation is called fully reducible or decomposable. In the latter case, a basis in V can be chosen such that the matrices ðRÞ are direct sums of matrices i ðRÞ such that the i ðRÞ form an irreducible matrix representation. If 3 ðRÞ in (1.2.2.4) is zero and 1 and 2 form irreducible matrix representations, is fully reducible. For ﬁnite groups, each reducible representation is fully reducible. That means that if ðKÞ is reducible, there is a matrix S such that ðRÞ ¼ S 1 ðRÞ . . . n ðRÞ S1 1 0 0 ... 0 1 ðRÞ B 0 2 ðRÞ . . . 0 C C 1 B B ¼ SB . .. C .. .. CS : . @ . . A . .

(c) point groups that have elements in common with O(3)\SO(3) but do not contain E; such groups are isomorphic to a group of the ﬁrst class, as one can see if one multiplies all elements with determinant equal to 1 by E. The list of three-dimensional ﬁnite point groups is given in Table 1.2.6.1. All isomorphism classes of two-dimensional point groups occur in three dimensions as well. The isomorphism classes occurring here for the ﬁrst time are: Cn C2 : A, B, with An ¼ B2 ¼ ABA1 B1 ¼ E; Dn C2 : A, B, C with An ¼ B2 ¼ ðABÞ2 ¼ C2 ¼ ACA1 C1 ¼ BCB1 C1 ¼ E; T: A, B, with A3 ¼ B2 ¼ ðABÞ3 ¼ E; O: A, B, with A4 ¼ B3 ¼ ðABÞ2 ¼ E; T C2 : A, B, C, with A3 ¼ B2 ¼ ðABÞ3 ¼ C2 ¼ ACA1 C1 ¼ BCB1 C1 ¼ E; O C2 : A, B, C, with A4 ¼ B3 ¼ ðABÞ2 ¼ C2 ¼ ACA1 C1 ¼ BCB1 C1 ¼ E; 5

3

0

...

0

n ðRÞ

2

ð1:2:2:5Þ

I: A, B, with A ¼ B ¼ ðABÞ ¼ E; I C2 : A, B, C, with A5 ¼ B3 ¼ ðABÞ2 ¼ C2 ¼ ACA1 C1

In this way one may proceed until all matrix representations i ðKÞ are irreducible, i.e. do not have invariant subspaces. Then each representation ðKÞ can be written as a direct sum ðRÞ ¼ S m1 1 ðRÞ . . . ms s ðRÞ S1 ; ð1:2:2:6Þ

¼ BCB1 C1 ¼ E: The crystallographic groups among them are given in Table 1.2.6.2. 1.2.2.2. Representations of ﬁnite groups

where the representations 1 . . . s are all nonequivalent and the multiplicities mi are the numbers of times each irreducible representation occurs. The nonequivalent irreducible representations i for which the multiplicity is not zero are the irreducible components of ðKÞ. We ﬁrst discuss two special representations. The simplest representation in one-dimensional space is obtained by assigning the number 1 to all elements of K. Obviously this is a representation, called the identity or trivial representation. Another is the regular representation. To obtain this, one numbers the elements of K from 1 to the order N of the group (jKj ¼ N). For a given R 2 K there is a one-to-one mapping from K to itself deﬁned by Ri ! Rj RRi . Consider the N N matrix ðRÞ, which has in the ith column zeros except on line j, where the entry is unity. The matrix ðRÞ then has as only entries 0 or 1 and satisﬁes

As stated in Section 1.2.1, elements of point groups act on physical properties (like tensorial properties) and on wave functions as linear operators. These linear operators therefore generally act in a different space than the three-dimensional conﬁguration space. We denote this new space by V and consider a mapping D from the point group K to the group of nonsingular linear operators in V that satisﬁes DðRÞDðR0 Þ ¼ DðRR0 Þ 8 R; R0 2 K:

ð1:2:2:3Þ

In other words D is a homomorphism from K to the group of nonsingular linear transformations GLðVÞ on the vector space V. Such a homomorphism is called a representation of K in V. Here we only consider ﬁnite-dimensional representations. With respect to a basis ei (i ¼ 1; 2; . . . n) the linear transformations are given by matrices ðRÞ. The mapping from K to the group of nonsingular n n matrices GL(n; R) (for a real vector space V) or GL(n; C) (if V is complex) is called an n-dimensional matrix representation of K. If one chooses another basis for V connected to the former one by a nonsingular matrix S, the same group of operators DðKÞ is represented by another matrix group 0 ðKÞ, which is related to ðKÞ by S according to 0 ðRÞ ¼ S1 ðRÞS (8 R 2 K). Two such matrix representations are called equivalent. On the other hand, two such equivalent matrix representations can be considered to describe two different groups of linear operators [DðKÞ and D0 ðKÞ] on the same basis. Then there is a nonsingular linear operator T such that DðRÞT ¼ TD0 ðRÞ (8 R 2 K). In this case, the representations DðKÞ and D0 ðKÞ are also called equivalent. It may happen that a representation DðKÞ in V leaves a subspace W of V invariant. This means that for every vector v 2 W and every element R 2 K one has DðRÞv 2 W. Suppose that this subspace is of dimension m < n. Then one can choose m basis vectors for V inside the invariant subspace. With respect to this basis, the corresponding matrix representation has elements 1 ðRÞ 3 ðRÞ ðRÞ ¼ ; ð1:2:2:4Þ 0 2 ðRÞ

RRi ¼ ðRÞji Rj ;

ði ¼ 1; 2; . . . ; NÞ:

ð1:2:2:7Þ

These matrices ðRÞ form a representation, the regular representation of K of dimension N, as one sees from ðRi Rj ÞRk ¼ Ri

N P

ðRj Þlk Rl ¼

l¼1

¼

N P m¼1

N P N P

ðRj Þlk ðRi Þml Rm

l¼1 m¼1

ðRi ÞðRj Þ

mk

Rm ¼

N P

ðRi Rj Þmk Rm :

m¼1

A representation in a real vector space that leaves a positive deﬁnite metric invariant can be considered on an orthonormal basis for that metric. Then the matrices satisfy ðRÞðRÞT ¼ E [T denotes transposition of the matrix: ðRÞTij ¼ ðRÞji ] and the representation is orthogonal. If V is a complex vector space with positive deﬁnite metric invariant under the representation, the latter gives on an orthonormal basis matrices satisfying ðRÞðRÞy ¼ E

36

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS [ denotes Hermitian conjugation: ðRÞyij ¼ ðRÞ ji ] and the representation is unitary. A real representation of a ﬁnite group is always equivalent with an orthogonal one, a complex representation of a ﬁnite group is always equivalent with a unitary one. As a proof of the latter statement, P consider the standard Hermitian metric on V: f ðx; yÞ ¼ i x i yi . Then the positive deﬁnite form P Fðx; yÞ ¼ ð1=NÞ f ðDðRÞx; DðRÞyÞ ð1:2:2:8Þ y

Proposition. Let M and N be two sets of nonsingular linear transformations in spaces V (dimension n) and W (dimension m), respectively. Suppose that both sets are irreducible (the only invariant subspaces are the full space and the origin). Let S be a linear transformation from V to W such that SM ¼ NS. Then either S is the null operator or S is nonsingular and SMS1 ¼ N. Proof: Consider the image of V under S: ImS V W. That means that Sr 2 ImS V for all r 2 V. This implies that NSr ¼ SMr 2 ImS V. Therefore, ImS V is an invariant subspace of W under N. Because N is irreducible, either ImS V ¼ 0 or ImS V ¼ W. In the ﬁrst case, S is the null operator. In the second case, notice that the kernel of S, the subspace of V mapped on the null vector of W, is an invariant subspace of V under M: if Sr ¼ 0 then NSr ¼ 0. Again, because of the irreducibility, either KerS is the whole of V, and then S is again the null operator, or KerS ¼ 0. In the latter case, S is a one-to-one mapping and therefore nonsingular. Therefore, either S is the null operator or it is an isomorphism between the vector spaces V and W, which are then both of dimension n. With respect to bases in the two spaces, the operator S corresponds to a nonsingular matrix and M ¼ S1 NS. This is a very fundamental theorem. Consequences of the theorem are: (1) If N and M are nonequivalent irreducible representations and SM ¼ NS, then S ¼ 0. (2) If a matrix S is singular and links two irreducible representations of the same dimension, then S ¼ 0. (3) A matrix S that commutes with all matrices of an irreducible complex representation is a multiple of the identity. Suppose that an n n matrix S commutes with all matrices of a complex irreducible representation. S can be singular and is then the null matrix, or it is nonsingular. In the latter case it has an eigenvalue 6¼ 0 and S E commutes with all the matrices. However, S E is singular and therefore the null matrix: S ¼ E. This reasoning is only valid in a complex space, because, generally, the eigenvalues are complex.

R2K

is invariant under the representation. To show this, take an arbitrary element R0 . Then P FðDðR0 Þx; DðR0 ÞyÞ ¼ ð1=NÞ f ðDðR0 RÞx; DðR0 RÞyÞ R2K

¼ Fðx; yÞ:

ð1:2:2:9Þ

With respect to an orthonormal basis for this metric Fðx; yÞ, the matrices corresponding to DðRÞ are unitary. The complex representation can be put into this unitary form by a basis transformation. For a real representation, the argument is fully analogous, and one obtains an orthogonal transformation. From two representations, D1 ðKÞ in V1 and D2 ðKÞ in V2 , one can construct the sum and product representations. The sum representation acts in the direct sum space V1 V2, which has elements (a; b) with a 2 V1 and b 2 V2 . The representation D1 D2 is deﬁned by ðD1 D2 ÞðRÞ ða; bÞ ¼ ðD1 ðRÞa; D2 ðRÞbÞ: ð1:2:2:10Þ The matrices 1 2 ðRÞ are of dimension n1 þ n2 . The product representation acts in the tensor space, which is the space spanned by the vectors ei ej (i ¼ 1; 2; . . . ; dimV1 ; j ¼ 1; 2 . . . ; dimV2 ). The dimension of the tensor space is the product of the dimensions of both spaces. The action is given by ðD1 D2 ÞðRÞ a b ¼ D1 ðRÞa D2 ðRÞb: ð1:2:2:11Þ

1.2.2.3. General tensors Suppose a group K acts linearly on a d-dimensional space V: for any v 2 V one has

For bases ei (i ¼ 1; 2; . . . ; d1 ) for V1 and e0 j (j ¼ 1; 2; . . . ; d2 ) for V2 , a basis for the tensor product of spaces is given by ei e0 j ;

i ¼ 1; . . . ; d1 ; j ¼ 1; 2; . . . ; d2 ;

ð1:2:2:12Þ

Rv 2 V and with respect to this basis the representation of K is given by matrices ð1 2 ÞðRÞik;jl ¼ 1 ðRÞij 2 ðRÞkl :

0 0 B 1 B1 ¼B @0 0 0

1

0

0

1

0 1

0

For a basis ai in V this gives a matrix group ðKÞ via

ð1:2:2:13Þ Rai ¼

As an example of these operations, consider 0 1 0 0 B 1 0 0 1 B 0 1 0 ¼B @0 0 0 0 1 1 0 0 1 0

1 0 0

0 0

0 1

d P

ðRÞji aj ;

R 2 K:

ð1:2:2:14Þ

j¼1

1 0 0C C C; 1A

The matrix group ðKÞ is a matrix representation of the group K. Consider now a linear function f on V. Because d d P P f i ai ¼ i f ðai Þ;

0 1 0 0 C C C: 1 A

i¼1

i¼1

the function is completely determined by its value on the basis vectors ai. A second point is that these linear functions form a vector space because for two functions f1 and f2 the function 1 f1 þ 2 f2 is a well deﬁned linear function. The vector space is called the dual space and is denoted by V . A basis for this space is given by functions f1 ; . . . ; fd such that

0

If two representations D1 ðKÞ and D2 ðKÞ are equivalent, there is an operator S such that SD1 ðRÞ ¼ D2 ðRÞS

8 R 2 K; v 2 V:

fi ðaj Þ ¼ ij ;

8 R 2 K:

because any linear function f can be written as a linear combination of these vectors with as coefﬁcients the value of f on the basis vectors ai :

This relation may also hold between sets of operators that are not necessarily representations. Such an operator S is called an intertwining operator. With this concept we can formulate a theorem that strictly speaking does not deal with representations but with intertwining operators: Schur’s lemma.

f ¼

d P i¼1

37

f ðai Þfi , f ð

d P k¼1

k ak Þ ¼

d P k¼1

k

d P i¼1

f ðai Þfi ðak Þ ¼

d P k¼1

k f ðak Þ:

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

The dðpþqÞ -dimensional space carries a representation of the group K:

Therefore, the space V also has d dimensions. If V has in addition a nonsingular scalar product, there is for each linear function f a vector k such that f ðrÞ ¼ k r;

Rfi1 ;...;ip ;j1 ;...;jq

ð1:2:2:15Þ ¼

and the vectors ki corresponding to the basis functions fi above satisfy ki aj ¼ fi ðaj Þ ¼ ij :

d P

ðRÞji fj $

i¼1

d P

ðRÞji

i¼1

d P

ð1:2:2:16Þ

ð1:2:2:17Þ

ðRÞlk fj ðal Þ ¼ fi ðak Þ ¼ ik ;

from which follows the relation

f ðr; sÞ : f ðr1 þ r2 ; s1 þ s2 Þ ¼ f ðr1 ; s1 Þ þ f ðr1 ; s2 Þ þ f ðr2 ; s1 Þ þ f ðr2 ; s2 Þ:

f ðr; sÞ ¼

P

f ðai ; aj Þfij ðr; sÞ:

ð1:2:2:19Þ

R0 2K

Because 1 ðKÞ and 2 ðKÞ are supposed to be irreducible, it follows from Schur’s lemma that either 1 and 2 are not equivalent and S is the null matrix, or they are equivalent. If they are not equivalent one has PP 1 ðRÞik Mkl 2 ðR1 Þlj : ð1:2:2:23Þ 0 ¼ Sij ¼

ð1:2:2:20Þ

Analogously to the former case, one can determine the transformation properties of the elements of the tensor space V V : Rfij ¼

ðRÞki ðRÞlj fkl :

ðRÞk1 i1 . . . ðRÞkp ip ðRÞl1 j1 . . . fk1 ...lq :

For this matrix one has P 0 S2 ðRÞ ¼ 1 ðR0 ÞM1 2 ðR Þ2 ðRÞ R0 2K P 1 0 ¼ 1 ðRÞ 1 ðRÞ1 ðR0 ÞM1 2 ðR Þ2 ðRÞ R0 2K P 1 0 ¼ 1 ðRÞ 1 ðR1 R0 ÞM1 2 ðR R Þ ¼ 1 ðRÞS:

ij

d P d P

lq ¼1

R2K

Again, such bilinear functions form a vector space of dimension d2 . Any function f ðr; sÞ is ﬁxed by its value on the d2 pairs of basis vectors, and these values are the coefﬁcients of the function on a basis

One has

kp ¼1 l1 ¼1

d P

1.2.2.4. Orthogonality relations Important consequences from symmetry for physical systems are related to orthogonality relations. The vanishing of matrix elements is one example. Consider two irreducible representations 1 ðKÞ and 2 ðKÞ of dimensions d1 and d2 , respectively. Then take an arbitrary d1 d2 matrix M and construct with this a new matrix S: P 1 ðRÞM1 S¼ 2 ðRÞ:

ð1:2:2:18Þ

The matrices ðRÞ form also a representation of K, the contragredient representation. In general, the latter is not equivalent with the former. The elements of the space V are dual vectors. One can generalize the procedure that gave the dual space, and this leads to a more abstract deﬁnition of a tensor. Consider a bilinear function on V.

fij ðak ; al Þ ¼ ik jl :

...

Therefore, the space of (p; q) tensors carries a representation which is the tensor product of the pth tensor power of ðKÞ and the qth tensor power of the contragredient representation ðKÞ. If the (0; 2) tensor f ðr; s) is symmetric in its arguments, the space of such tensors carries the symmetrized tensor product of the representation ðKÞ with itself. Similarly the (anti)symmetric (2; 0) tensors form a space that carries the symmetrized, respectively antisymmetrized, tensor product of ðKÞ with itself. This can be generalized to (p; q) tensors with all kinds of symmetry. One can have a (0; 4) tensor that is symmetric in all its four arguments. Such tensors form a space that not only carries a representation of K, but one of the symmetric group S4 (the permutation group on four letters) as well. We shall come back to such symmetric tensors in Section 1.2.2.7.

l¼1

ðRÞij ¼ 1 ðRÞji :

d P d P

ð1:2:2:22Þ

Then Rfi ¼

...

k1 ¼1

The vectors ki (with i ¼ 1; 2; . . . ; d) form the reciprocal basis (see also Section 1.1.2.4). The transformation properties of the vectors in dual (or reciprocal) space can be derived from those of the vectors in V if one puts ðRf ÞðRrÞ ¼ f ðrÞ:

d P

R2K kl

Because we have taken an arbitrary matrix M, this implies that P 1 ðRÞik 2 ðR1 Þlj ¼ 0 ð1:2:2:24Þ

ð1:2:2:21Þ

k¼1 l¼1

R2K

The space carries the product representation of the contragredient representation with itself. That this is really the same concept of tensor as usually used in physics can be seen from the example of theP dielectric tensor "ij . For an electric ﬁeld E, the energy is given by ij "ij Ei Ej and this is a bilinear function f" ðE; EÞ. The most general situation occurs if one considers all multilinear functions of p vectors and q dual vectors. The function

whenever 1 ðKÞ and 2 ðKÞ are not equivalent. When the two irreducible representations are equivalent we assume them to be identical. Then S commutes with all matrices 1 ðKÞ of an irreducible representation and is thus a multiple of the identity (in case one considers complex representations). Its trace is then d if the dimension of the representation is denoted by d, but on the other hand it is P Tr 1 ðRÞM1 ðR1 Þ ¼ NTrðMÞ: TrðSÞ ¼

f ðr1 ; . . . ; rp ; k1 ; . . . ; kq Þ

R2K

is linear in each of its arguments. Again, the function is determined by its value on the basis vectors ai of V and bj of V . The (p; q)-linear functions form a vector space with basis vectors fi1 ;...;jq given by

Therefore, Sij ¼ ðN=dÞTrðMÞij ¼

PP R2K kl

fi1 ;...;ip ;j1 ;...;jq ðak1 ; . . . ; blq Þ ¼ i1 k1 . . . jq lq :

Hence

38

1 ðRÞik Mkl 1 ðR1 Þlj :

ð1:2:2:25Þ

P

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS 1

1 ðRÞik 1 ðR Þlj ¼ ðN=dÞij kl :

ð1:2:2:26Þ

characters because of the orthogonality relations and the multiplicities and irreducible components are uniquely determined by the formula (1.2.2.30).

R2K

This leads to the following proposition.

Because the character is constant on a conjugacy class, (1.2.2.30) can also be written as

Proposition. If ðKÞ and ðKÞ are irreducible complex representations of the ﬁnite group K one has P ðRÞik ðR1 Þlj ¼ ðN=dÞij kl 0 ; ð1:2:2:27Þ

m ¼ ð1=NÞ

k P

ni ðCi Þ ðCi Þ;

ð1:2:2:31Þ

i¼1

R2K

where Ci denotes the ith conjugacy class (i ¼ 1; 2; . . . k) and ni the number of its elements.

where 0 is zero if the representations are not equivalent, unity if they are identical and undeﬁned if they are equivalent but not identical.

Proposition. The representation DðKÞ is irreducible if and only if

For unitary representations the orthogonality relations can be written as P ðRÞik ðRÞ jl ¼ ðN=dÞij kl 0 : ð1:2:2:28Þ

ð1=NÞ

k P

ni jðCi Þj2 ¼ 1:

i¼1

R2K

Proof: For a representation that is equivalent to the sum of irreducible representations with multiplicities m one has

According to Section 1.2.2.2 for ﬁnite groups K, there is always an equivalent unitary representation.

ð1=NÞ

k P

ni jðCi Þj2 ¼ ð1=NÞ

i¼1

1.2.2.5. Characters

¼

m2 :

ð1:2:2:32Þ

Proof: Consider the regular representation. The value of its character in an element R is given by the number of elements Ri 2 K for which RRi ¼ Ri . Therefore,

0 for R 6¼ E; ðRÞ ¼ N for R ¼ E: The multiplicity formula (1.2.2.30) then gives P m ¼ ð1=NÞ ðRÞ ðRÞ ¼ ð1=NÞðEÞ ðEÞ ¼ d : R2K

Each irreducible representation occurs in the regular representation with a multiplicity equal to its dimension. Therefore, P P N ¼ ðEÞ ¼ m ðEÞ ¼ d2 :

Here one can use the Kronecker delta because characters of equivalent representations are equal, even if they are not identical.

The character of the sum of two representations is the sum of the characters. More generally, the character of the sum of irreducible representations D, each with multiplicity m, is P ðRÞ ¼ m ðRÞ:

Proposition. The number of nonequivalent irreducible representations of a ﬁnite group K is equal to the number of its conjugacy classes. Proof: Take from each equivalence class of irreducible representations of K one unitary representative ðKÞ. The matrix elements ðRÞij are complex functions on the group. The number of these functions is the sum over of d2 and that is equal to the order of the group according to Burnside’s theorem. The number of independent functions on K is, of course, also equal to the order N of the group. If one considers the usual scalar product of functions on the group, P f1 f2 f1 ðRÞf2 ðRÞ;

This gives a formula for the multiplicity of an irreducible component: P PP m ¼ m ¼ ð1=NÞ m ðRÞ ðRÞ R2K

ðRÞ ðRÞ:

P

Proposition. (Burnside’s theorem.) The sum of the squares of the dimensions of all nonequivalent irreducible representations is equal to the order of the group.

R2K

P

m m ¼

If the representation is irreducible, there is exactly one value of for which m ¼ 1, whereas all P other multiplicities vanish. If the representation is reducible, m2 > 1.

Proposition. For two irreducible complex representations of a ﬁnite group K, one has P ðRÞ ðRÞ ¼ N : ð1:2:2:29Þ

¼ ð1=NÞ

ni m m ðCi Þ ðCi Þ

i¼1

Two equivalent representations of a group K are conjugate subgroups in the group of nonsingular linear transformations. Corresponding matrices therefore have the same invariants. It is a remarkable fact that one of these invariants sufﬁces for characterizing the equivalence class of a representation, namely the trace. The character of an element R 2 K in a representation DðKÞ is the trace ðRÞ ¼ TrðDðRÞÞ. It is a complex function on the group: for every R 2 K there is a complex number ðRÞ. The character only depends on the conjugacy class: if two elements R and R0 belong to the same class there is an element T 2 K such that R0 ¼ TRT 1 . Hence ðR0 Þ ¼ TrðDðTRT 1 ÞÞ ¼ TrðDðRÞÞ ¼ ðRÞ. Notice that for the identity element one has DðEÞ ¼ the d-dimensional unit matrix and ðEÞ ¼ d. For the same reason, the character for two equivalent representations is the same. From the orthogonality relations for the matrix elements of two irreducible representations follow those for characters.

P

k P P

ð1:2:2:30Þ

R2K

From the expression for the multiplicities follows:

R2K

Proposition. The representations D1 ðKÞ and D2 ðKÞ are equivalent if and only if their characters are the same: 1 ðRÞ ¼ 2 ðRÞ. Two equivalent representations obviously have the same character. Nonequivalent irreducible representations have different

the scalar product of two of the N functions is P ðRÞij ðRÞkl ¼ ðN=d Þ ik jl R2K

39

ð1:2:2:33Þ

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES k P according to the orthogonality relations. This means that the N ni ðCi Þ ðCi Þ ¼ ; ð1=NÞ functions indeed form an orthogonal basis in the space of all i¼1 functions on the group. In particular, consider a function f ðKÞ k P that is constant on conjugacy classes. This function can be ðCi Þ ðCj Þ ¼ ð1=ni Þij ; ð1=NÞ ¼1 expanded in the basis functions. k P P ni ðCi Þnj ðCj Þ ¼ d cijl nl ðCl Þ: f ðRÞ ¼ fij ðRÞij l¼1 ij

¼

P

fij ð1=NÞ

ij

P

ðTRT 1 Þij

P P

fij ðTÞik ðRÞkl ðT 1 Þlj

ijkl T2K

¼ ð1=NÞ

P

fij ðRÞkl ðN=d Þij kl

ijkl

¼

d PP

ðfii =d Þ ðRÞ:

i¼1

This implies that every class function can be written as a linear combination of the character functions. Therefore, the number of such character functions must be equal to or larger than the number of conjugacy classes. On the other hand, the number of dimensions of the space of class functions is k, the number of conjugacy classes. For the scalar product in this space given by f1 f2

k P

ðni =NÞf1 ðCi Þf2 ðCi Þ

The character table is in agreement with the class multiplication table C1 C1 ¼ C1 C1 C2 ¼ C2 C1 C3 ¼ C3

the character functions are orthogonal: ðni =NÞ ðCi Þ ðCi Þ ¼ ð1=NÞ

i¼1

P

ð1:2:2:37Þ

and the group of matrices is equivalent to an orthogonal group with generators pﬃﬃﬃ 1 1 p 1 0 3 0 0 2 2 ﬃﬃ ﬃ 3 ðAÞ ¼ : ; 3 ðBÞ ¼ 0 1 12 3 12

i¼1

k P

ð1:2:2:36Þ

As an example, consider the permutation group on three letters S3. It consists of six permutations. It is a group that is isomorphic with the point group 32. The character table is a 3 3 array, because there are three conjugacy classes (Ci , i ¼ 1; 2; 3), and consequently three irreducible representations (i , i ¼ 1; 2; 3) (see Table 1.2.2.1). The two one-dimensional representations are equal to their character. A representative representation for the third character is generated by matrices 0 1 1 1 ; 3 ðBÞ ¼ 3 ðAÞ ¼ 1 1 0 1

T2K

¼ ð1=NÞ

ð1:2:2:35Þ

ðRÞ ðRÞ ¼ :

C2 C1 ¼ C2 C2 C2 ¼ 2C1 þ C2 C2 C3 ¼ 2C3

C3 C1 ¼ C3 C3 C2 ¼ 2C3 C3 C3 ¼ 3C1 þ 3C2 :

R2K

ð1:2:2:34Þ 1.2.2.6. The representations for point groups in one, two and three dimensions

There are at most k mutually orthogonal functions, and consequently the number of nonequivalent irreducible characters ðKÞ is exactly equal to the number of conjugacy classes.

For the irreducible representations of the point groups, it is necessary to know something about the structure of these groups. Since the representations of isomorphic groups are the same, one can restrict oneself to representatives of the isomorphism classes. In the following, we give a brief description of the structure of the point groups in spaces up to three dimensions. The character tables are given in Section 1.2.6. For the inﬁnite series of groups (Cn and Dn ), the crystallographic members are given explicitly separately. (i) Cn . Cyclic groups are Abelian. Therefore, each element is a conjugacy class on itself. Irreducible representations are one-dimensional. The representation is determined by its value on a generator. Since An ¼ E, the character ðAÞ of an irreducible representation is an nth root of unity. There are n one-dimensional representations. For the pth irreducible representation, one has ðpÞ ðAÞ ¼ expð2ip=nÞ. (ii) Dn . From the deﬁning relations, it follows that Ap and Ap (p ¼ 1; 2; . . . ; n) form a conjugacy class and that Ap B and Apþ2 B belong to the same class. Therefore, one has to distinguish the

As additional result one has the following proposition. Proposition. The functions ðRÞij with ¼ 1; 2; . . . ; k and i; j ¼ 1; 2; . . . ; d form an orthogonal basis in the space of complex functions on the group K. The characters form an orthogonal basis for the space of all class functions. The characters of a group K can be combined into a square matrix, the character table, with entries ðCi Þ. Besides the orthogonality relations mentioned above, there are also relations connected with class multiplication constants. Consider the conjugacy classes Ci of the group K. Formally one can introduce the sum of all elements of a class: Mi ¼

P

R:

R2Ci

It can be proven that the multiplication of two such class sums is the sum of class sums, where such a class sum may occur more than once: Mi Mj ¼

P

cijk Mk ;

Table 1.2.2.1. Character table for S3 D3

cijk 2 Z:

Elements Symbols

(1) E

ð123Þ A

Class Order

C1 1

C2 3

k

1 2 3

The coefﬁcients cijk are called the class multiplication constants. The elements of the character table then have the following properties.

40

1 1 2

1 1 1

(132) A2

ð23Þ B C3 2 1 1 0

(13) A2 B

(12) AB

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS cases of even n from those of odd n. For odd n, one has a class consisting of E (order 1), (n 1)/2 classes with elements Ap, and one class with all elements Ap B (order 2). For even n, there is a class consisting of E (order 1), one with An=2 , and (n 2Þ/2 classes with Ap . The other elements form two classes of order 2 elements, one with the elements Ap B for p odd, the other with Ap B for p even. The number of one-dimensional irreducible representations is the order of the group (N) divided by the order of the commutator group, which is the group generated by all elements aba1 b1 (a; b 2 K). For n odd this number is 2, for n even it is 4. In addition there are two-dimensional irreducible representations: (n 1)/2 for odd n, n=2 1 for even n. (iii) T; O; I. The conjugacy classes of the tetrahedral, the octahedral and the icosahedral groups T, O and I, respectively, are given in the tables in Section 1.2.6. (iv) K C2 . Because the generator of C2 commutes with all elements of the group, the number of conjugacy classes of the direct product K C2 is twice that for K. If A is the generator of C2 and Ci are the classes of K, then the classes of the direct product are Ci and Ci A. The element A, which commutes with all elements of the direct product, is in an irreducible representation represented by a multiple of the identity. Because A is of order 2, the factor is 1. Therefore, the character table looks like ðKÞ ðKÞ : ðK C2 Þ ¼ ðKÞ ðKÞ

into a complex form and such a transformation does not change the character. Therefore, a better question is: which complex irreducible representations can be brought into real form? Consider a complex irreducible representation with a real character. Then it is equivalent with its complex conjugate via a matrix S: ðRÞ ¼ S ðRÞS1 ;

Here one has to distinguish two different cases. To make the distinction between the two cases one has the following: Proposition. Suppose that ðKÞ is a complex irreducible representation with real character, and S a matrix intertwining ðKÞ and its complex conjugate. Then S satisﬁes either SS ¼ E or SS ¼ E. In the former case, there exists a basis transformation that brings ðKÞ into real form, in the latter case there is no such basis transformation. Proposition. If ðKÞ is a complex irreducible representation with real character ðKÞ, the latter satisﬁes P ðR2 Þ ¼ 1: ð1=NÞ R2K

If the right-hand side is þ1, the representation can be put into real form, if it is 1 it cannot. (Proofs are given in Section 1.2.5.5.) Consequently, a complex irreducible representation ðKÞ is P equivalent with a real one if ðRÞ ¼ ðRÞ and R ðR2 Þ ¼ N. If that is not the case, a real representation containing ðKÞ as irreducible component is the matrix representation ðRÞ þ ðRÞ iððRÞ ðRÞÞ ðRÞ 0 1 : 2 iððRÞ ðRÞÞ ðRÞ þ ðRÞ 0 ðRÞ

The n irreducible representations where A is represented by þE are called gerade representations, the other, where A is represented by E, are called ungerade. In general, if K and H are ﬁnite groups with irreducible representations D1 ðKÞ and D2 ðHÞ, the outer tensor product acts on the tensor product V1 V2 of representation spaces as ðD1 ðRÞ D2 ðR0 ÞÞa b ¼ ðD1 ðRÞaÞ ðD2 ðR0 ÞbÞ; a 2 V1 ; b 2 V2 :

R 2 K:

ð1:2:2:39Þ ð1:2:2:38Þ The basis transformation is given by E E : S¼ iE iE

With the irreducibility criterion, one checks that this is an irreducible representation of K H. Moreover, D1 D2 is equivalent with D10 D20 if and only if ¼ 0 and ¼ 0 . This means that one obtains all nonequivalent irreducible representations of K H from the outer tensor products of the irreducible representations of K and H. If the group H is C2, there are two irreducible representations of C2, both one-dimensional. That means that the tensor product simpliﬁes to a normal product. If H ¼ C2 and D2 ðHÞ is the trivial representation, one has from (1.2.2.38)

The dimension of the physically irreducible representation is 2d, if d is the dimension of the complex irreducible representation ðKÞ. In summary, there are three types of irreducible representation: P (1) First kind: ðKÞ ¼ ðKÞ, R2K ðR2 Þ ¼ þN, dimension of real representation d; P 2 (2) Second kind: ðKÞ ¼ ðKÞ, R2K ðR Þ ¼ N, dimension of real representation 2d; P (3) Third kind: ðRÞ 6¼ ðRÞ , R2K ðR2 Þ ¼ 0, dimension of real representation 2d. Examples of the three cases: (1) The matrices 0 i 1 0 DðAÞ ¼ and DðBÞ ¼ i 0 0 1

Dg ðRÞ ¼ D ðRÞ; Dg ðRAÞ ¼ D ðRÞ; R 2 K Du ðRÞ ¼ D ðRÞ; Du ðRAÞ ¼ D ðRÞ: The letters g and u come from the German gerade (even) and ungerade (odd). They indicate the sign of the operator associated with the generator A of C2 : þ1 for g representations, 1 for u representations. The number of nonequivalent irreducible representations of K C2 is twice that of K. Schur’s lemma and the orthogonality relations and theorems derived above are formulated for complex representations and are, generally, not valid for integer or real representations. Nevertheless, many physical properties can be described using representation theory, but being real quantities they sometimes require a slightly different treatment. Here we shall discuss the relation between the complex representations and physical or real representations. Consider a real matrix representation ðKÞ. If it is reducible over complex numbers, it can be fully reduced. When is an irreducible component itself real? A ﬁrst condition is clearly that its character is real. This is, however, not sufﬁcient. A real representation can by a complex basis transformation be put

generate a group that forms a faithful representation of the dihedral group D4 ¼ 422, for which the character table is given in Table 1.2.6.5. If one uses the same numbering of conjugacy classes, its character is ðCi Þ ¼ 2; 0; 2; 0; 0. It is an irreducible representation (22 þ 22 ¼ N ¼ 8) with real character. The sum of the characters of the squares of the elements is 2 þ 2 ð2Þ þ 2 þ 2 2 þ 2 2 ¼ 8 ¼ N. Therefore, it is equivalent to a real matrix representation, e.g. with 0 1 0 1 D0 ðAÞ ¼ and D0 ðBÞ ¼ : 1 0 1 0

41

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES (2) The matrices

DðAÞ ¼

0 i

i 0

and DðBÞ ¼

0 1

1 0

In many cases in practice, the spaces Vi are all identical and then the dimension of the tensor product V n is simply dn. The tensor product of n identical spaces carries in an obvious way a representation of the permutation group Sn of n elements. A permutation of n elements is always the product of pair exchanges. The action of the permutation (12), that interchanges spaces 1 and 2, is given by

generate a group that is a faithful representation of the quaternion group of order 8. This group has ﬁve classes: E, fA; A3 g, fB; B3 g, fBA; ABg and A2 . The character of the elements is ðRÞ ¼ 2; 0; 0; 0; 2 for the ﬁve classes. Then P ð1=8Þ ðR2 Þ ¼ 1;

P12 ei ej ek . . . ¼ ej ei ek . . . :

Two subspaces are then of particular interest, that of the tensors that are invariant under all elements of Sn and those that get a minus sign under pair exchanges. These spaces are the spaces of fully symmetric and antisymmetric tensors, respectively. If the spaces V1 ; . . . ; Vn carry a representation of a ﬁnite group K, the tensor product space carries the product representation.

R

which means that the representation is essentially complex. A real physically irreducible representation of the group is generated by 1 0 1 0 0 1 0 0 0 0 0 1 B C B 0 0 1 0 C B C and B 1 0 0 0 C; @0 1 0 @ 0 0 0 1 A 0 A 0 0 1 0 1 0 0 0

e1j1 e2j2 . . . n O P ¼ eiji ! 1 ðRÞk1 j1 2 ðRÞk2 j2 . . . e1k1 e2k2 . . . : i¼1

The matrix ðRÞ of the tensor representation is the tensor product of the matrices i ðRÞ. In general, this representation is reducible, even if the representations i are irreducible. The special case of n ¼ 2 has already been discussed in Section 1.2.2.3. From the deﬁnition of the action of R 2 K on vectors in the tensor product space, it is easily seen that the character of R in the tensor product representation is the product of the characters of R in the representations i : n Q ð1:2:2:43Þ ðRÞ ¼ i ðRÞ: i¼1

All complex irreducible representations of the ﬁnite point groups in up to three dimensions with real character can be put into a real form. This is not true for higher dimensions, as we have seen in the example of the quaternion group.

The reduction in irreducible components then occurs with the multiplicity formula. n P Q ðRÞ i ðRÞ: ð1:2:2:44Þ m ¼ ð1=NÞ

1.2.2.7. Tensor representations When V1 ; . . . ; Vn are linear vector spaces, one may construct tensor products of these spaces. There are many examples in physics where this notion plays a role. Take the example of a particle with spin. The wave function of the particle has two components, one in the usual three-dimensional space and one in spin space. The proper way to describe this situation is via the tensor product. In normal space, a basis is formed by spherical harmonics Ylm, in spin space by the states jssz i. Spin–orbit interaction then plays in the ð2l þ 1Þð2s þ 1Þ-dimensional space with basis jlmi jssz i. Another example is a physical tensor, e.g. the dielectric tensor "ij of rank 2. It is a symmetric tensor that transforms under orthogonal transformations exactly like a symmetric bi-vector with components vi wj þ vj wi, where vi and wi (i ¼ 1; 2; 3) are the components of vectors v and w. A basis for the space of symmetric bi-vectors is given by the six vectors (ei ej þ ej ei ) (i j). The space of symmetric rank 2 tensors has the same transformation properties. A basis for the tensor space V1 V2 . . . Vn is given by e1i e2j . . . enk , where i ¼ 1; 2; . . . ; d1 ; j ¼ 1; 2; . . . d2 ; . . . ; k ¼ 1; 2; . . . ; dn . Therefore the dimension of the tensor product is the product of the dimensions of the spaces Vi (see also Section 1.1.3.1.2). The tensor space consists of all linear combinations with real or complex coefﬁcients of the basis vectors. In the summation one has the multilinear property ! d d2 P1 P P c1i e1i

c2j e2j . . . ¼ c1i c2j . . . e1i e2j . . . : j¼1

k1 k2 ...

ð1:2:2:42Þ

and the generated group is a crystallographic group in four dimensions. (3) The complex number expð2i=nÞ generates a representation of the cyclic group Cn. For n > 2 the representation is not equivalent with its complex conjugate. Therefore, it is not a physical representation. The physically irreducible representation that contains this complex irreducible component is generated by cosð2=nÞ sinð2=nÞ expð2i=nÞ 0 ’ : sinð2=nÞ cosð2=nÞ 0 expð2i=nÞ

i¼1

ð1:2:2:41Þ

R2K

i¼1

If the tensor product representation is a real representation, the physically irreducible components can be found by ﬁrst determining the complex irreducible components, and then combining with their complex conjugates the components that cannot be brought into real form. The tensor product of the representation space V with itself has a basis ei ej (i; j ¼ 1; 2; . . . ; d). The permutation (12) transforms this into ej ei. This action of the permutation becomes diagonal if one takes as basis ei ej þ ej ei (1 i j d, spanning the space Vs 2 ) and ei ej ej ei (1 i < j d, spanning the space Va 2 ). If one considers the action of K, one has with respect to the ﬁrst basis ðRÞ ¼ ðRÞ2 if V carries the representation with character ðKÞ. With respect to the second basis, one sees that the character of the permutation P ¼ ð12Þ is given by 12 dðd þ 1Þ 12 dðd 1Þ ¼ d. The action of the element R 2 K on the second basis is P R ei ej ej ei ¼ ð ÞðRÞkl;ij ei ej ej ei : kl

This implies that both Vs 2 and Va 2 are invariant under R. The character in the subspace is P ð1:2:2:45Þ þ ðRÞ ¼ ð ÞðRÞkl;kl k l

for the symmetric subspace and P ðRÞ ¼ ð ÞðRÞkl;kl

ij...

ð1:2:2:40Þ

k 2, the tensor product space does not carry just a symmetric and an antisymmetric subspace, but also higherdimensional representations of the permutation group Sn. The derivation of the character of the fully symmetric and fully antisymmetric subspaces remains rather similar. The formulae for the character of the representation of K carried by the fully symmetric (þ) and fully antisymmetric () subspace, respectively, for n ¼ 1; 2; 3; 4; 5; 6 are

ð14Þð35Þð2Þ ð15Þð34Þð2Þ ð23Þð45Þð1Þ ð24Þð35Þð1Þ ð25Þð34Þð1Þ The sign of all these permutations is even: they are the product of an even number of pair interchanges. The prefactor for the term ðR2 ÞðR2 ÞðRÞ is then þ15=5!. 1.2.2.8. Projective representations It is useful to consider a more general type of representation, one that gives only a homomorphism from a group to linear transformations up to a factor. In quantum mechanics, the relevance of such representations is a consequence of the freedom of the phase of the wave function, but they also occur in classical physics. In particular, we shall need this generalized concept for the determination of representations of crystallographic space groups. A projective representation of a group K is a mapping from K to the group of nonsingular linear transformations of a vector space V such that

1 ðRÞ2 ðR2 Þ 2! 1 n ¼ 3 : ðRÞ ¼ ðRÞ3 3ðR2 ÞðRÞ þ 2ðR3 Þ 3! 1 n ¼ 4 : ðRÞ ¼ ðRÞ4 6ðR2 ÞðRÞ2 þ 3ðR2 Þ2 4! þ 8ðR3 ÞðRÞ 6ðR4 Þ 1 n ¼ 5 : ðRÞ ¼ ðRÞ5 10ðR2 ÞðRÞ3 þ 15ðR2 Þ2 ðRÞ 5! þ 20ðR3 ÞðRÞ2 20ðR3 ÞðR2 Þ 30ðR4 ÞðRÞ þ 24ðR5 Þ 1 n ¼ 6 : ðRÞ ¼ ðRÞ6 15ðR2 ÞðRÞ4 þ 45ðR2 Þ2 ðRÞ2 6! þ 40ðR3 Þ2 15ðR2 Þ3 þ 40ðR3 ÞðRÞ3

n ¼ 2 : ðRÞ ¼

DðRÞDðR0 Þ ¼ !ðR; R0 ÞDðRR0 Þ

8 R; R0 2 K;

where !ðR; R0 Þ is a nonzero real or complex number. The name stems from the fact that the mapping is a homomorphism if one identiﬁes linear transformations that differ by a factor. Then one looks at the transformations of the lines through the origin, and these form a projective space. Other names are multiplier or ray representations. The mapping ! from K K to the real or complex numbers is called the factor system of the projective representation. An ordinary representation is a projective representation with a trivial factor system that has only the value unity. A projective representation that can be identiﬁed with DðHÞ is one with D0 ðRÞ ¼ uðRÞDðRÞ for some real or complex function u on the group. It gives the same transformations of projective space. The projective representations DðHÞ and D0 ðHÞ are called associated. Their factor systems are related by

120ðR3 ÞðR2 ÞðRÞ 90ðR4 ÞðRÞ2 þ 90ðR4 ÞðR2 Þ þ 144ðR5 ÞðRÞ 120ðR6 Þ From this follows immediately the dimension of the two subspaces: 1 n ¼ 2 : ðd2 dÞ 2 1 n ¼ 3 : ðd3 3d2 þ 2dÞ 6 1 n ¼ 4 : ðd4 6d3 þ 11d2 6dÞ 24 1 5 ðd 10d4 þ 35d3 50d2 þ 24dÞ n ¼ 5: 120 1 6 ðd 15d5 þ 85d4 225d3 þ 274d2 120dÞ: n ¼ 6: 720

!0 ðR; R0 Þ ¼

uðRÞuðR0 Þ !ðR; R0 Þ; uðRR0 Þ

ð1:2:2:48Þ

as one can check easily. Two factor systems that are related in this way are also called associated. Not every mapping ! : K K ! complex numbers can be considered as a factor system. There is the following proposition: Proposition. A mapping ! from K K to the complex numbers can occur as factor system for a projective representation if and only if one has

These expressions are based on Young diagrams. The procedure will be exempliﬁed for the case of n ¼ 5. In the expression for occur the partitions of n in groups of integers:

!ðR1 ; R2 Þ!ðR1 R2 ; R3 Þ ¼ !ðR1 ; R2 R3 Þ!ðR2 ; R3 Þ 8 R1 ; R2 ; R3 2 K:

ð1:2:2:49Þ

If one has two mappings !1 and !2 satisfying this relation, the product !ðR; R0 Þ ¼ !1 ðR; R0 Þ!2 ðR; R0 Þ also satisﬁes the relation. Therefore, factor systems form an Abelian multiplicative group. A subgroup is formed by all factor systems that are associated with the trivial one: 5¼ 4þ1¼ 3þ2¼ 3þ1þ1¼ 2þ2þ1¼ 2þ1þ1þ1¼ 1 þ 1 þ 1 þ 1 þ 1. Each partition corresponds with a Young diagram with as many rows as there are terms in the sum, and in each row the corresponding number of boxes. The total number of boxes is n. Each partition corresponds with a term P ðRi1 ÞðRi2 Þ . . . such that j ij ¼ n. Here i1 is the number of boxes in the ﬁrst row etc. The prefactor then is the number of

!ðR; R0 Þ ¼

uðRÞuðR0 Þ uðRR0 Þ

for some function u on the group. These form another Abelian group and the factor group consists of all essentially different factor systems. This factor group is called Schur’s multiplicator group.

43

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES A projective representation is called reducible if there is a proper invariant subspace. It is fully reducible if there is a basis on which the representation matrices form the direct sum of two representations. This is exactly as for ordinary representations. Equivalence of projective representations is slightly more subtle. Two projective representations are called associated if their factor systems are associated. They are weakly equivalent if there is a complex function uðRÞ on the group and a nonsingular linear transformation S such that D2 ðRÞ ¼ uðRÞSD1 ðRÞS1

8 R 2 K:

tion D of R. For two elements r1 and r2 of R there are elements k1 and k2 in K. Deﬁne linear operators Pðki Þ ¼ Dðri Þ. Then k1 k2 corresponds to r1 r2 up to an element a 2 A. This means Pðk1 ÞPðk2 Þ ¼ DðaÞPðk1 k2 Þ: Because a commutes with all elements of R, the operator DðaÞ commutes with all the operators of the irreducible representation DðRÞ. From Schur’s lemma it follows that it is a multiple of the unit operator. Moreover, this multiple depends on k1 and k2 : DðaÞ ¼ !ðk1 ; k2 ÞE. Therefore, an irreducible representation of R gives a projective representation of K. It has been shown by Schur that one obtains all projective representations of K, i.e. one representative from each strong equivalence class for each class of non-associated factor systems, in the way presented if one takes for the group A the multiplicator group. The way to ﬁnd all projective representations of K is then: determine the multiplicator group, determine R, determine the ordinary irreducible representations of R. We shall not go into detail, but only present a way to characterize projective representations (Janssen, 1973). First we consider an example, the group K ¼ 2mm, isomorphic to D2. It can be shown that the multiplicator group is the group of two elements. Therefore, the representation group R has eight elements and one can show that it is isomorphic to D4 or to the quaternion group (in general there is not a unique R). The character table of D4 is given in Table 1.2.2.2. The centre is generated by A2. If the elements of the factor group are e, a, b and ab, then E and A2 correspond to e, A and A3 to a, B and A2 B to b, and AB and A3 B to ab. Because A2 is represented by the unit element for the four one-dimensional representations, each element of the factor group corresponds to a unique element of the representation. PðaÞ can be chosen to be DðAÞ or DðA3 Þ, but because DðA2 Þ ¼ E for the one-dimensional representations these are equal. Therefore, the one-dimensional representations of K ¼ D2 have a trivial factor system. For the two-dimensional representation one may choose 0 1 1 0 ; ; PðaÞ ¼ PðeÞ ¼ 1 0 0 1 1 0 0 1 PðbÞ ¼ ; PðabÞ ¼ : 0 1 1 0

ð1:2:2:50Þ

This implies that their factor systems are associated. Two projective representations are strongly equivalent if their factor systems are identical and there exists a nonsingular linear transformation S such that D2 ðRÞS ¼ SD1 ðRÞ. Therefore, strong equivalence implies weak equivalence, which in turn implies association. The reason for this distinction will soon become clear. For projective representations with identical factor systems there exist orthogonality relations for matrix elements and for characters. It is important to notice that for projective representations the character is generally not a class function, because one can multiply every operator with a separate constant. Proposition. For given factor system ! there is a ﬁnite number r of strong equivalence classes of irreducible projective representations. The dimensions of the nonequivalent irreducible representations satisfy r P d2 ¼ N: ð1:2:2:51Þ ¼1

Proposition. For two irreducible projective matrix representations with the same factor system, the following holds: P 0 ðRÞij 1 ð1:2:2:52Þ ðRÞkl ¼ ðN=d Þ il jk : R2K

Notice that, in general, for projective representations ðR1 Þ 6¼ ðRÞ1 ! Every projective representation of a ﬁnite group is strongly equivalent with a unitary representation, for which one has P ðRÞij ðRÞ ik ¼ ðN=d Þ0 il jk ; ð1:2:2:53Þ

It is easily checked that this forms a projective representation with a nontrivial factor system. One can characterize the projective representation starting from the deﬁning relations a2 ¼ b2 ¼ ðabÞ2 ¼ e. One has PðaÞ2 ¼ E, PðbÞ2 ¼ E, ðPðaÞPðbÞÞ2 ¼ E. It is easily seen that one cannot achieve a trivial factor system by multiplication of the P matrices by suitably chosen factors. Therefore, the factor system is not associated with the trivial one either. This is the general situation. The ordinary representations of R can be partitioned into groups, each group corresponding with one class of associated factor systems, and within each group one ﬁnds representatives of each strong equivalence class. For the example above, there is only one such class for the nontrivial factor system as one sees from d2 ¼ 4 ¼ N ¼ jD2 j. The general procedure then is to characterize a factor system with expressions stemming from deﬁning relations for the group K. Deﬁning relations are expressions (words) in the generators that ﬁx the isomorphism class of the group. They are of the form

R2K

and for the characters P

ðRÞ ðRÞ ¼ N :

ð1:2:2:54Þ

R2K

For projective representations with the same factor system, one can construct the sum representation, which still has the same factor system: ð1 2 ÞðRÞ ¼ 1 ðRÞ 2 ðRÞ. On the other hand, a reducible projective representation can be decomposed into irreducible components with the same factor system and multiplicities P ðRÞ ðRÞ; ð1:2:2:55Þ m ¼ ð1=NÞ R2K

as follows directly from the orthogonality conditions. Projective representations of a group K may be constructed from the ordinary representations of a larger group R. Suppose that R has a subgroup A in the centre, which means that all its elements commute with all elements of R. Suppose furthermore that the factor group R=A is isomorphic with K. Therefore, the order of R is the product of the orders of A and K. Because K is the factor group, each element of R corresponds to a unique element of K and the elements of the subgroup A correspond to the unit element in K. Then consider an irreducible representa-

Table 1.2.2.2. Character table of D4 E 1 2 3 4 5

44

1 1 1 1 2

A, A3 1 1 1 1 0

A2 1 1 1 1 2

B, A2 B 1 1 1 1 0

AB, A3 B 1 1 1 1 0

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS Wi ðA1 ; A2 ; . . . ; Ap Þ ¼ E; i ¼ 1; 2; . . . ; s ð1:2:2:56Þ i 0 0 1 A¼ ; B¼ ; A4 ¼ B2 ¼ ðABÞ2 ¼ E: 0 i 1 0 if the Ai are the generators. For a projective representation the corresponding product This group is isomorphic with D4 , a group with ﬁve irreducible representations: four one-dimensional and one two-dimensional. Wi ðDðA1 Þ; DðA2 Þ; . . . ; DðAp ÞÞ ¼ i E The former are the four ordinary representations of D2 because both E and E are represented by the unit matrix. The twois a multiple of the identity operator. The deﬁning relations are dimensional representation has ðEÞ ¼ ðEÞ and is, therenot unique for a group. Therefore, there is arbitrariness here. The fore, not an ordinary representation for 222. It is an extra complex numbers i that correspond to the deﬁning relations representation for the double group 222d, or a projective repremay be changed by multiplying the operators DðRÞ by factors sentation of 222. Choosing one element from SU(2) for each uðRÞ. This changes the factor system to an associated one. If in a generator of 222 one obtains table the factor systems are given by the numbers i, one can 0 i 0 1 identify the class of a given factor system by calculating the ð2x Þ ¼ ; ð2y Þ ¼ ; corresponding words and solving the problem of ﬁnding the table i 0 1 0 values by taking into account additional factors uðRÞ. For ð2x Þ2 ¼ ð2y Þ2 ¼ E; ðð2x Þð2y ÞÞ2 ¼ E: example, the factor system that gives the values of i for D2 above is associated with one that gives 1;2;3 ¼ 1; 1; 1, if one multiplies The factor system ﬁxed in this way is not associated to a trivial PðaÞ by i. one (otherwise the irreducible representation could not be twodimensional). The extra representation of the double group 1.2.2.9. Double groups and their representations corresponds to a nontrivial projective representation of the point Three-dimensional rotation point groups are subgroups of group itself. SO(3). In quantum mechanics, rotations act according to some To construct the character table of the double group, it is representation of SO(3). Because wave functions can be multi- worthwhile to note that the elements of K d mapped on one class plied by an arbitrary phase factor, in principle projective repre- of K form two classes, except when the class in K consists of 180 sentations play a role here. The projective representations of rotations and there exists for one element of this class another SO(3) can be obtained from the ordinary representations of the 180 rotation in K with its axis perpendicular to that of the former representation group, which is SU(2), the group of all 2 2 element. The example above illustrates this: there are four classes matrices in K ¼ 222 and ﬁve classes in Kd . The identity in K corresponds to E in Kd , and these form two classes. The other pairs A, B a b 2 2 with jaj þ jbj ¼ 1: and AB are mapped each on one class. This is, however, not the b a most general case. uðRÞ only belong to the same class if there is an element S 2 K such that uðRÞuðSÞ ¼ uðSÞuðRÞ. If one brings For example, in spin space for a particle with spin 12, a rotation uðRÞ into diagonal form, one sees that this is only possible if the over ’ along the z axis acts according to diagonal elements are i, i.e. when the rotation angle of R is . In this case one has expði’=2Þ 0 ; 0 expði’=2Þ i 0 i 0 uðSÞ ¼ uðSÞ; 0 i 0 i and in general the representation for a rotation over ’ along an axis n^ is then cosð’=2ÞE þ i sinð’=2Þðr nÞ; ^ 0 expði’Þ ; uðSÞ ¼ expði’Þ 0 where r is a vector with the three Pauli spin matrices as components. Because the matrices for ’ ¼ 2 become E, the which is a twofold rotation with axis perpendicular to the z axis. representation has a nontrivial factor system. As a representation Therefore, in general, if a class in K of 180 rotations does not of SU(2), however, it is an ordinary representation. exist or if there is not a perpendicular 180 rotation, the class in K To each rotation ðR 2 SOð3ÞÞ correspond two elements corresponds to two classes in Kd . UðRÞ 2 SUð2Þ. To a point group K SOð3Þ corresponds a As a second example, we consider the group K ¼ 32 of order subset of SU(2) which is in fact a subgroup, because six. It is generated by a threefold rotation along the z axis and a UðRÞUðR0 Þ ¼ UðRR0 Þ. This group is the double group Kd . It twofold rotation perpendicular to the ﬁrst one. Corresponding contains both E and E, which are both mapped to the unit elements of SU(2) are element of SO(3) under the homomorphism SU(2) ! SO(3). 1 1 pﬃﬃﬃ 0 1 þ 2i 3 0 pﬃﬃﬃ Because E commute with all elements of K d, this group C2 is an 2 : A¼ ; B¼ 1 1 1 0 0 invariant subgroup and the factor group K d =C2 is isomorphic to 2 2i 3 K. Therefore, every representation of K is a representation of Kd, but in general there are other representations as well, the extra The group K d generated by these elements is of order 12 with representations. Notice that the double group of K does not only six classes: E, E, (A; A5 ), (A2 ; A4 ), (B; A2 B; A4 B) and depend on the isomorphism class of K, but also on the geometric (AB; A3 B; A5 B), which are mapped on the three classes of K ¼ 32. Therefore, there are six irreducible representations for class, because the realization as subgroup of O(3) comes in. As an example, we take the group 222 SOð3Þ. The two Kd : four one-dimensional ones and two two-dimensional ones. Two one-dimensional and one two-dimensional representations generators 2x and 2y correspond, respectively, to the matrices are the ordinary representations of K, the other ones are extra 0 1 0 i representations and have ðEÞ ¼ ðEÞ. As projective repre: ; 1 0 i 0 sentations of K ¼ 32, they are associated with ordinary representations: for the one-dimensional ones this is obvious; for the These matrices generate a group of order eight, which can also be two-dimensional one, generated by A and B, one can ﬁnd an presented by associated one ðAÞ ¼ A, ðBÞ ¼ iB such that

45

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 3

2

ðAÞ ¼ ðBÞ ¼ ððAÞðBÞÞ2 ¼ E

Because fEjRag belongs to the lattice translation group for every R 2 K and every lattice translation fEjag, the lattice generated by the vectors ei (i ¼ 1; 2; . . . ; n) is invariant under the point group K. Therefore, the latter is a crystallographic point group. On a basis of the lattice , the point group corresponds to a group ðKÞ of integer matrices. One has the following situation. The space group G has an invariant subgroup A isomorphic to Zn, the factor group G=A is a crystallographic point group K which acts according to the integer representation ðKÞ on A. In mathematical terms, G is an extension of K by A with homomorphism from K to the group of automorphisms of A. The vectors a occurring in the elements fEjag 2 G are called primitive translations. They have integer coefﬁcients with respect to the basis e1 ; . . . ; en. However, not all vectors a in the spacegroup elements are necessarily primitive. One can decompose the space group G according to

and, consequently, this representation has a trivial factor system. This shows that, although 32d has three extra representations, there are no nontrivial projective representations. The characters for the double point groups are given in Table 1.2.6.7. 1.2.3. Space groups 1.2.3.1. Structure of space groups The Euclidean group E(n) in n dimensions is the group of all distance-preserving inhomogeneous linear transformations. In Euclidean space, an element is denoted by g ¼ fRjag

G ¼ A þ g2 A þ g3 A þ . . . þ gN A:

where R 2 OðnÞ and a is an n-dimensional translation. On a point r in n-dimensional space, g acts according to fRjagr ¼ Rr þ a:

To every element R 2 K there is a coset gi A with gi ¼ fRjaðRÞg as representative. Such a representative is unique up to a lattice translation. Instead of aðRÞ, one could as well have aðRÞ þ n as representative for any lattice translation n. For a particular choice, the function aðRÞ from the point group to the group T(n) is called the system of nonprimitive translations or translation vector system. It is a mapping from the point group K to TðnÞ, modulo A. Such a system of nonprimitive translations satisﬁes the relations

ð1:2:3:1Þ

Therefore, jgr1 gr2 j ¼ jr1 r2 j. The group multiplication law is given by fRjagfR0 ja0 g ¼ fRR0 ja þ Ra0 g:

ð1:2:3:2Þ

The elements fEjag form an Abelian subgroup, the group of n-dimensional translations T(n). An n-dimensional space group is a subgroup of E(n) such that its intersection with T(n) is generated by n linearly independent basis translations. This means that this lattice translation subgroup A is isomorphic to the group of n-tuples of integers: each translation in A can be written as n n Q P fEjag ¼ fEjei gni ¼ fEj ni ei g: ð1:2:3:3Þ i¼1

ð1:2:3:4Þ

aðRÞ þ RaðSÞ ¼ aðRSÞ mod A

8 R; S 2 K:

ð1:2:3:5Þ

This follows immediately from the product of two representatives gi . If the lattice translation subgroup A acts on a point r, one obtains the set þ r. One can describe the elements of G as well as combinations of an orthogonal transformation with r as centre and a translation. This can be seen from

i¼1

The lattice translation subgroup A is an invariant subgroup because

fRjag ¼ fEja r þ RrgfRjr Rrg;

gfEjagg1 ¼ fRjbgfEjagfRjbg1 ¼ fEjRag 2 A: The factor group G=A, of the space group G and the lattice translation group A, is isomorphic to the group K formed by all elements R occurring in the elements fRjag 2 G. This group is the point group of the space group G. It is a subgroup of O(n). The unit cell of the space group is a domain in n-dimensional space such that every point in space differs by a lattice translation from some point in the unit cell, and such that between any two points in the unit cell the difference is not a lattice translation. The unit cell is not unique. One choice is the n-dimensional parallelepiped spanned by the n basis vectors. The points in this unit cell have coordinates between 0 (inclusive) and 1. Another choice is not basis dependent: consider all points generated by the lattice translation group from an origin. This produces a lattice of points . Consider now all points that are closer to the origin than to any other lattice point. This domain is a unit cell, if one takes care which part of the boundary belongs to it and which part not, and is called the Wigner–Seitz cell. In mathematics it is called the Voronoi cell or Dirichlet domain (or region). Because the point group leaves the lattice of points invariant, it transforms the Wigner–Seitz cell into itself. This implies that points inside the unit cell may be related by a point-group element. Similarly, space-group elements may connect points inside the unit cell, up to lattice translations. A fundamental region or asymmetric unit is a part of the unit cell such that no points of the fundamental region are connected by a space-group element, and simultaneously that any point in space can be related to a point in the fundamental region by a space-group transformation.

ð1:2:3:6Þ

where now fRjr Rrg leaves the point r invariant. The new system of nonprimitive translations is given by a0 ðRÞ ¼ aðRÞ þ ðR EÞr:

ð1:2:3:7Þ

This is the effect of a change of origin. Therefore, for a space group, the systems of nonprimitive translations are only determined up to a primitive translation and up to a change of origin. It is often convenient to describe a space group on another basis, the conventional lattice basis. This is the basis for a sublattice with the same, or higher, symmetry and with the same number of free parameters. Therefore, the sublattice is also invariant under K and with respect to the conventional basis, which is obtained from the original one via a basis transformation S, the point group has the form conventional ðRÞ ¼ Sprimitive ðRÞS1 ;

ð1:2:3:8Þ

where S is the centring matrix. It is a matrix with determinant equal to the inverse of the number of lattice points of the primitive lattice inside the unit cell of the conventional lattice. As an example, consider the primitive and centred rectangular lattices in two dimensions. Both have symmetry 2mm, and two parameters a and b. The transformation from a basis of the conventional lattice [(2a; 0) and (0; 2b)] to a basis of the primitive lattice [(a; b) and (a; b)] is given by S, and the relations between the generators of the point groups are

46

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS 1 1 1 0 0 1 1 the fundamental region are related by a point-group transfor2 2 ¼S S ; S¼ 1 1 mation from K and that any point in the Brillouin zone can be 0 1 1 0 2 2 obtained from a point in the fundamental region by a point-group 0 1 1 1 0 transformation. S : ¼S 1 0 0 1 1.2.3.3. Irreducible representations of space groups For representations of space groups, we use the same argu1.2.3.2. Irreducible representations of lattice translation groups mentation as for the lattice translation subgroup. Notice that the The lattice translation group A is isomorphic to the group Zn of group AN generated by the vectors fEjNei g is an invariant n-tuples of integers. This is an inﬁnite group and, therefore, the Abelian subgroup of the space group G as well. usual techniques for ﬁnite groups cannot be applied. A way past fRjagfEjNei gfR1 j R1 ag ¼ fEjNRei g 2 AN : this is the following. If ai are the basis vectors of the lattice , the lattice translation group generated by the translations fEjNai g N n forms an Abelian subgroup AN of A. The factor group A=AN is a The factor group G=A is a ﬁnite group of order N times the ﬁnite group isomorphic to the direct product of n cyclic groups of order of the point group K. Representations of this factor group representations of G with the property that all elements of order N. Each representation of this group is a representation of are N A with the property that the elements of AN are represented by A are mapped on the unit operator. We shall consider here only the unit operator. This procedure is in fact that of periodic such space-group representations. Suppose that ðGÞ is an irreducible representation of the space boundary conditions in solid-state physics. In the following, we shall consider only the representations of A that satisfy this group G. Its restriction ðAÞ to the lattice translation subgroup is then reducible, unless it is one-dimensional. Each irreducible condition. The irreducible representations of the direct product of n cyclic representation of A is characterized by a vector k in the Brillouin groups of order N are all one-dimensional. According to Section zone. Therefore, 1.2.2.6 they can be characterized by n integers and read ðfEjagÞ 1 0 expðik1 aÞ 0 0 ... 0 0 n P fpj g C B fEj ni ei g ¼ exp½2iðn1 p1 þ n2 p2 þ . . . þ nn pn Þ=N; 0 expðik2 aÞ 0 ... 0 0 B C

B ¼B B B @

i¼1

ð1:2:3:9Þ because a representation of the cyclic group CN is determined by its value on the basis translations: p ðfEjegÞ ¼ expð2ip=NÞ;

ð1:2:3:10Þ

0

...

...

0

0

0

...

0

expðikn aÞ

0

0

0

0

... 0

0

... 0 ... 0

0 0

... 0

0

1 C C C C: C C A

. . . 0 expðiks aÞE ð1:2:3:15Þ (1.2.3.15)

It can be shown that the dimensions of the unit matrices E are all the same (and equal to d). Then

i¼1

n ¼ s d:

The expression (1.2.3.9) then can be written more concisely if one introduces an n-dimensional vector k: n P k ¼ ð1=NÞ pi bi : ð1:2:3:12Þ

With respect to the basis on which the translation is of this form, every basis vector in the pth block is multiplied by a factor expðikp aÞ. Suppose that fRjug is an element of the space group G. Consider a basis vector v of the representation space that gets a factor expðik aÞ under the translation fEjag. Then one has

i¼1

Then (1.2.3.9) simpliﬁes to fkg ðfEjagÞ ¼ expðik aÞ:

0

0

ðfEjagÞ 0 0 0 expðik1 aÞE B 0 expðik2 aÞE 0 B B ¼B 0 0 expðik 3 aÞE B B 0 0 0 @

These vectors bj span the reciprocal lattice . The scalar product of an arbitrary lattice vector a and a reciprocal-lattice vectors K is then n n n P P P Ka¼ mi bi nj aj ¼ 2 ni mi : ð1:2:3:11Þ j¼1

0

0

Some of the vectors ki may be identical. Therefore, the matrix representation can be written as

There are exactly N n nonequivalent irreducible representations. If ai are basis vectors of the lattice , its dual basis consists of vectors bj deﬁned by

i¼1

C C: C C A

0

ð1:2:3:14Þ (1.2.3.14)

0 p < N:

ai bj ¼ 2ij :

expðik3 aÞ . . .

0

ð1:2:3:13Þ

DðfEjagÞv ¼ expðik aÞv DðfEjagÞDðfRjugÞv ¼ DðfRjugÞDðfEjR1 agÞv

Because 0 pi =N < 1, the vector k belongs to the unit cell of the reciprocal lattice. If one chooses that unit cell as the Voronoi cell for the reciprocal lattice, which in direct space would be the Wigner–Seitz cell, it is called the Brillouin zone. Therefore, representations of the lattice translation subgroup are characterized by a vector in the Brillouin zone. In fact, the vectors k form a mesh inside the Brillouin zone, but this mesh becomes ﬁner if N increases. In the limit of N going to 1, the wavevectors k ﬁll the Brillouin zone. Just like the direct lattice, the reciprocal lattice is invariant under the point group K. The Brillouin zone, or at least its interior, is invariant under K as well. A fundamental domain in the Brillouin zone is a part of the zone such that no two points of

¼ expðiRk aÞDðfRjugÞv; and because DðfRjugÞv also belongs to the representation space there are vectors that transform with the vector Rk as well as vectors that transform with k. This means that for every vector k occurring in a block in (1.2.3.5), there is also a block for each vector Rk as R runs over the point group K. The vectors fRkjR 2 Kg form the star of k. Vectors Rk that differ by a reciprocal-lattice vector (k0 ¼ k þ K with K 2 ) correspond to the same representation and are therefore considered to be the same. Generally, a vector k may be left invariant by a subgroup of the point group K. This point group Kk is the point group of k.

47

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Kk fRjRk k mod g: ð1:2:3:16Þ It can be shown that ðGÞ is irreducible if and only if Dk ðGk Þ is irreducible. From the construction, it is obvious that one may Then there are s point-group elements Ri such that obtain all irreducible representations of G in this way. Moreover, ð1:2:3:17Þ one obtains all representations of G if one takes for the K ¼ Kk [ R2 Kk [ . . . [ Rs Kk construction all stars and for each star all irreducible representations of Gk. and each element Ri corresponds to a vector in the star: So the ﬁnal step is to determine all nonequivalent irreducible ki ¼ Ri k1 ; k1 ¼ k; i ¼ 1; 2; . . . ; s: representations of Gk. Notice that the lattice translation subgroup is a subgroup of Gk. Therefore, Therefore, the blocks in (1.2.3.15) for an irreducible repreDk ðfEjagÞ ¼ expðik aÞE: sentation of the space group G correspond to the s branches of the star of k. They are all of the same dimension d. If the vectors ki in (1.2.3.15) belonged to two or more different stars, the If one makes a choice for the system of nonprimitive translations uðRÞ, every element g ¼ fSjvg 2 Gk can be written uniquely as representation would be reducible. To the point group of k corresponds a subgroup of the space g ¼ fEjagfSjuðSÞg; group G that has Kk as point group. It is called the group of k and is deﬁned by for a lattice translation a. Therefore, one has Gk fg ¼ fRjag 2 GjR 2 Kk g: ð1:2:3:18Þ Dk ðfSjvgÞ ¼ expðik aÞDk ðfSjuðSÞgÞ expfik ½a þ uðSÞgðSÞ ð1:2:3:23Þ

Analogously to (1.2.3.17), one can write G ¼ Gk [ g2 Gk [ . . . [ gs Gk

ð1:2:3:19Þ

if one deﬁnes ðSÞ ¼ exp½ik uðSÞDk ðfSjuðSÞgÞ:

for elements gi ¼ fRi jai g of the space group G. As one sees from (1.2.3.15), there is a subspace of vectors v that get a factor expðik a) for any lattice translation a. If one considers the action of DðgÞ with g 2 Gk , it follows immediately that a vector from this space is transformed into a vector of the same space: the subspace corresponding to a vector k is invariant under Gk . Therefore this space Vk carries a representation of Gk. It can be seen as follows that one may construct the irreducible representation of the whole group G as soon as one knows the representation Dk of Gk in Vk . To that end, consider a basis e1 ; . . . ; ed in Vk . The vectors wi ¼ Dðgi Þe

ði ¼ 1; 2; . . . ; s; ¼ 1; 2; . . . ; dÞ;

It is important to notice that this deﬁnition of does not depend on the choice of the system of nonprimitive translations. If one takes u0 ðSÞ ¼ uðSÞ þ b (b 2 A), the result for ðSÞ is the same. The product of two matrices ðSÞ and ðS0 Þ then becomes ðSÞðS0 Þ ¼ exp ik ½uðSÞ þ uðS0 Þ Dk ðfSS0 juðSÞ þ SuðS0 ÞgÞ ¼ exp ik ½uðS0 Þ SuðS0 Þ ðSS0 Þ: ð1:2:3:25Þ One sees that the matrices ðRÞ form a projective representation of the point group of k. The factor system is given by

ð1:2:3:20Þ

!ðS; S0 Þ ¼ expfik ½uðS0 Þ SuðS0 Þg ¼ exp½iðk S1 Þ uðS0 Þ:

form a basis of the whole representation space. Under a latticetranslation vector a, the vector wi gets a factor expðiki aÞ. On this basis, one can determine the matrix representation ðGÞ. Take an element fRjug 2 G. It belongs to a certain coset gm Gk in the decomposition of G. In addition, the element fRjuggi belongs to a well deﬁned gj Gk . This means that there is an element fSjvg in the group Gk such that fRjuggi ¼ gj fSjvg

i

ði ¼ 1; 2; . . . ; s; fSjvg 2 Gk Þ:

¼ DðfRjugÞDðgi Þe

expfik ½uðS0 Þ SuðS0 Þg ¼ exp½iðk S1 kÞ uðS0 Þ ¼ 1:

¼ Dðgj ÞDðfSjvgÞe d P ¼ Dðgj Þ k ðfSjvgÞ e

A nontrivial factor system !ðS; S0 Þ can therefore only occur for a nonsymmorphic group Gk and for a k on the Brillouin-zone boundary. But even then, it is possible that one may redeﬁne the matrices ðSÞ with an appropriate phase factor such that they form an ordinary representation. This is, for example, always the case if Kk is cyclic, because cyclic groups do not have genuine projective representations. These are always associated with an ordinary representation. If the factor system !ðS; S0 Þ is not associated with a trivial one, one has to ﬁnd the irreducible projective representations with the given factor system. As seen in the previous section, one may do this by using the deﬁning relation for the point group Kk. If these are words Wi ðA1 ; . . . ; Ar Þ in the generators A1 ; . . . ; Ar, the corresponding expressions in the representation

¼1

¼

d P

¼1

¼

k ðfSjvgÞ

s P d P

j

ðfRjugÞj ;i

j :

j¼1 ¼1

This means that the representation matrix ðfRjugÞ can be decomposed into s s blocks of dimension d. In each row of blocks there is exactly one that is not a block of zeros, and the same is true for each column of blocks. Moreover, the only nonzero block in the ith column and in the jth row is Dk ðfSjvgÞ ¼ Dk ðg1 j fRjuggi Þ;

ð1:2:3:21Þ

Wi ðDk ðA1 Þ; . . . ; Dk ðAr ÞÞ ¼ i E

ð1:2:3:22Þ

are multiples of the unit operator. The values of i ﬁx the class of the factor system completely. By multiplying the operators Dk ðAj Þ by proper phase factors, the values of i can be trans-

where i and j are uniquely related by fRjuggi 2 gj Gk :

ð1:2:3:26Þ

Such a factor system may, however, be equivalent to a trivial one. If the space group Gk is symmorphic, one may choose the system of nonprimitive translations to be zero. Consequently, in this case the factor system !ðS; S0 Þ is unity and the matrices ðSÞ form an ordinary representation of the space group Gk. This is also the case if k is not on the Brillouin-zone boundary. If k is inside the Brillouin zone and S 2 Kk , one has Sk ¼ k þ K only for K ¼ 0. So inside the Brillouin zone one has Sk ¼ k for all S 2 Kk . This implies that

Then one can write DðfRjugÞ

ð1:2:3:24Þ

48

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS Table 1.2.3.1. Choices of k in the fundamental domain of Pmmm and the elements of Kk k 000 1 200 0120 0012 012 12 1 1 202 11 220 111 222

00 12 0 0 12 12 12 00 1 2 0 0 12 1 1 22 00 1 2 0 0 12 11 22 0 1 2 0 12 0 12

Wyckoff position a b e c g d f h i k j l m o n p q s r t u v w x y z

Kk mmm mmm mmm mmm mmm mmm mmm mmm 2mm 2mm 2mm 2mm m2m m2m m2m m2m mm2 mm2 mm2 mm2 m11 m11 1m1 1m1 11m 11m 1

Table 1.2.3.2. Strata of irreducible representations of Pmm2 and Pmmm

Elements E E E E E E E E E E E E E E E E E E E E E E E E E E E

mx mx mx mx mx mx mx mx my my my my mx mx mx mx mx mx mx mx mx mx my my mz mz

my my my my my my my my mz mz mz mz mz mz mz mz my my my my

mz mz mz mz mz mz mz mz 2x 2x 2x 2x 2y 2y 2y 2y 2z 2z 2z 2z

1 1 1 1 1 1 1 1

2x 2x 2x 2x 2x 2x 2x 2x

2y 2y 2y 2y 2y 2y 2y 2y

2z 2z 2z 2z 2z 2z 2z 2z

k

Wyckoff position in Pmm2

Wyckoff positions in Pmmm

Kk

00 0 12 1 2 0 11 22 0 12 0 1 2

a b c d e f g h i

a; c; q e; g; r b; d; s f ; h; t i; j; w k; l; x m; n; u o; p; v y; z;

mm2 mm2 mm2 mm2 1m1 1m1 m11 m11 1

sentations are labelled . There are several conventions for the choice of this label, but an irreducible representation of G is always characterized by a pair (k; Þ, where k ﬁxes the star and the irreducible point-group representation. The projective representations of the group of k, i.e. of Kk, can be obtained from the ordinary representations of a larger group. If the factor system !ðR; R0 Þ is of order m [!m ðR; R0 Þ ¼ 1 for all ^ k! is m times the order of R; R0 ], the order of this larger group K Kk . Then the irreducible representations of the space group are labelled by the vector k in the Brillouin zone and an irreducible ^ k!, where ! follows from (1.2.3.26). ordinary representation of K Two stars such that one branch of the ﬁrst one has the same Kk as one branch of the other determine representations that are quite similar. The only difference is the numerical value of the factors expðik aÞ, the form of the representation matrices being the same. Such irreducible representations of the space group are said to belong to the same stratum. Strata are denoted by a symbol for one vector k in the Brillouin zone. For example, the origin, conventionally denoted by , belongs to one stratum that corresponds to the ordinary representations of the point group K. For a simple cubic space group, the point [12; 0; 0] is denoted by X. Its Kk is the tetragonal group 4=mmm. All points [; 0; 0] with 6¼ 0 and 12 < < 12 form one stratum with point group 4mm. This stratum is denoted by etc. The strata can be compared with the Wyckoff positions in direct space. There a Wyckoff position is a manifold in the unit cell for which all points have the same site symmetry, modulo the lattice translations. Here it is a manifold of k vectors with the same symmetry group modulo the reciprocal lattice. The action of Gk does not involve the nonprimitive translations. Therefore, the strata correspond to Wyckoff positions of the corresponding symmorphic space group. The stratum symbols for the various three-dimensional Bravais classes are given in Table 1.2.6.11. As an example, we consider here the orthorhombic space group Pnma. The orthorhombic Brillouin zone has a fundamental domain with volume that is one-eighth of that of the Brillouin zone. The various choices of k in this fundamental domain, together with the corresponding point groups Kk, are given in Table 1.2.3.1. The vectors k correspond to Wyckoff positions of the group Pmmm. In the tables, the vectors k and their corresponding Wyckoff positions are given for the holohedral space groups. In general, the number of different strata is smaller for the other groups. One can still use the same symbols for these groups, or take the symbols for the Wyckoff positions for the groups that are not holohedral. Consider as an example the group Pmm2. Its holohedral space group is Pmmm. The strata of irreducible representations can be labelled by the symbols for Wyckoff positions of Pmm2 as well as those of Pmmm. This is shown in Table 1.2.3.2. The deﬁning relations for the point group mmm are

formed into those tabulated. Then the tables give all irreducible representations for this factor system. In summary, the procedure for ﬁnding all irreducible representations of a space group G is as follows. (1) Consider all stars of k with respect to G. This means that one takes all vectors k in a fundamental region of the Brillouin zone. (2) For each star, one determines the group Kk. (3) For each Kk , one determines the factor system !ðS; S0 Þ. (4) For this factor system, one looks for all nonequivalent irreducible (projective) representations. (5) From the representations Dk ðKk Þ, one determines the representations k ðGk Þ and ðGÞ according to the procedure given above. 1.2.3.4. Characterization of space-group representations The irreducible representations of space groups are characterized by a star of vectors in the Brillouin zone, and by the irreducible, possibly projective, representations of the point group of one point from that star. The stars are sets of vectors in the Brillouin zone related mutually by transformations from the point group K of the space group G modulo reciprocal-lattice vectors. To obtain all stars, it is sufﬁcient to take all vectors in the fundamental domain of the Brillouin zone, i.e. a part of the Brillouin zone such that no vectors in the domain are related by point-group elements (modulo ) and such that every point in the Brillouin zone is related to a vector in the fundamental domain by a point-group operation. From each star one takes one point k and determines the nonequivalent irreducible representations of the point group Kk, the ordinary representations if the group Gk is symmorphic or k is inside the Brillouin zone, or the projective representations with factor system ! [equation (1.2.3.26)] otherwise. These repre-

A2 ¼ B2 ¼ ðABÞ2 ¼ C2 ¼ E;

49

AC ¼ CA;

BC ¼ CB:

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES UðRÞ ¼ E cosð’=2Þ þ ðr nÞ sinð’=2Þ Table 1.2.3.3. Characteristic values of i for the projective irreps of Kk for the point group mmm ð1:2:3:28Þ Representations B2 ðABÞ2 C2 AC ¼ CA BC ¼ CB A2 k

1

2

3

4

5

6

Number

Dimension

000 1 200 0120 0012 012 12 1 1 202 11 220

1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1

1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1

1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1

1 1 1 1 1 1 1 1

1 1 1 1 1 1 1 1

1 1 1 1 1 1 1 1

8 2 2 2 2 8 2 2 4 4 4 4 4 1 1 4 4 1 1 1 2 2 2 2 2 2 1

1 2 2 2 2 1 2 2 1 1 1 1 1 2 2 1 1 2 2 2 1 1 1 1 1 1 1

111 222

00 12 0 0 12 12 12 00 1 2 0 0 12 1 1 22 00 1 2 0 0 12 11 22 0 1 2 0 12 0 12

i ¼ 1; . . . :

In the example one has ðAÞ2 ¼ 1 E ðBÞ2 ¼ 2 E 2 ððAÞðBÞÞ ¼ 3 E ðCÞ2 ¼ 4 E ðAÞðCÞ ¼ 5 ðCÞðAÞ ðBÞðCÞ ¼ 6 ðCÞðBÞ: The values for i characterize the projective representation factor system and are given in Table 1.2.3.3. They are unity for ordinary representations. By putting factors i in front of the representation matrices in the appropriate places, some of the values of i can be changed from 1 to þ1. In this way, one obtains either ordinary representations, which are necessarily one-dimensional for these Abelian groups, or projective representations, which are in this case two-dimensional. This is indicated as well in Table 1.2.3.3. The one-dimensional irreducible representations are ordinary representations of the group Kk. The two-dimensional ones are projective representations, but correspond to ordinary representations of the larger groups isomorphic to D4 C2 and D4 .

ð1:2:3:29Þ

with multiplication rule fUðRÞjagfUðSÞjbg ¼ fUðRÞUðSÞja þ Rbg: ð1:2:3:30Þ

Pk ðfRjagÞ ¼ expðik aÞðRÞ;

ð1:2:3:31Þ

where the projective representation ðKk Þ has the factor system ðRÞðSÞ ¼ !s ðR; SÞ exp½iðk R1 kÞ aðSÞðRSÞ ¼ !ðR; SÞðRSÞ;

ð1:2:3:32Þ

where !s is the spin factor system for Kk and aðSÞ is the nonprimitive translation of the space-group element with orthogonal part S. The factor system ! can be characterized by the deﬁning relations of Kk. If these are the words

1.2.3.5. Double space groups and their representations In Section 1.2.2.9, it was mentioned that the transformation properties of spin-12 particles under rotations are not given by the orthogonal group O(3), but by the covering group SU(2). Hence, the transformation of a spinor ﬁeld under a Euclidean transformation g is given by gðrÞ ¼ UðRÞðR1 ðr aÞÞ

fRjag ! fUðRÞjag

An invariant subgroup of the double space group is the translation group A. The factor group is the double point group K d of the point group K. The representations of the double space groups can be constructed in the same way as those of ordinary space groups. They are characterized by a vector k in the Brillouin zone and a label for an irreducible, generally projective, representation of the (double) point group Kkd of k, which is the double group of Kk. Again, for nonsymmorphic space groups or wavevectors k inside the Brillouin zone, the relevant irreducible representations of Kkd are ordinary representations with a trivial factor system. For an element g of the space group G, there are two elements of the double space group Gd. If one considers an irreducible representation DðGd Þ for the double space group and takes for each g 2 G one of the two corresponding elements in Gd , the resulting set of linear operators forms a projective representation of the space group. It is also characterized by a vector k in the Brillouin zone and a projective representation of the point group (not its double) Kk . This projective representation does not have the same factor system as discussed in Section 1.2.3.3, because the factor system now stems partly from the nonprimitive translations and partly from the fact that a double point group gives a projective representation of the ordinary point group Kk. The projective representations of a space group corresponding to ordinary representations of the double space group again are characterized by the star of a vector k. The projective representation of the group Gk then is given by

For the subgroups, the deﬁning relations follow from these. The corresponding expressions in the representation matrices ðAi Þ for the generators of the point groups give expressions Wileft ðA1 ; . . . ; Ar Þ ¼ i Wiright ðA1 ; . . . ; Ar Þ;

when the rotation R has angle ’ and axis n. When R does not belong to SO(3) one has to take UðR). For an ordinary space group, one can construct the double space group by

Wi ðA1 ; . . . ; Ap Þ ¼ E; then the factor system ! is characterized by the factors i in

8 g ¼ fRjag 2 Eð3Þ; ð1:2:3:27Þ

Wi ððA1 Þ; . . . ; ðAp ÞÞ ¼ i E:

where the SU(2) operator UðRÞ is given by

50

ð1:2:3:33Þ

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS The factors i are the product of the values found from the spin factor system !s and those corresponding to the factor system for an ordinary representation [equation (1.2.3.26)].

the theorems for ﬁnite groups are still valid if one replaces sums over group elements by integration over the group. The group O(3) is the direct product SOð3Þ C2 . Therefore, there are even and odd representations. They have the property D ðRÞ ¼ ðRÞ;

1.2.4. Tensors 1.2.4.1. Transformation properties of tensors

x¼

i ai ! x0 ¼

i¼1

n P

i0 ai ¼

P

Rij j ai ;

‘ ðRÞ ¼

n P

...

j1 ¼1

n P jr ¼1

Ri1 j1 . . . Rir jr Tj1 ...jr :

and the symmetrized and antisymmetrized tensor products are ðDm Dm Þs ¼ ðDm Dm Þa ¼

Rij Fj ðR1 ðr aÞÞ;

fRjag 2 EðnÞ:

m M D2j1 :

ð1:2:4:6Þ

If the components of the tensor Ti1 ...ir are taken with respect to an orthonormal basis, the tensor is called a Cartesian tensor. The orthogonal transformation R then is represented by an orthogonal matrix Rij . Cartesian tensors of higher rank than one are generally no longer irreducible for the group O(n). For example, the rank-two tensors in three dimensions have nine components Tij . Under SO(3), they transform according to the tensor product of two ‘ ¼ 1 representations. Because

ð1:2:4:1Þ

Under a Euclidean transformation, the function transforms according to n P

ð1:2:4:5Þ

j¼1

j¼1

Fi ðrÞ0 ¼

m M D2j ; j¼0

and analogously for pseudotensors (or axial tensors – see Section 1.1.4.5.3). A vector ﬁeld is a vector-valued function in n-dimensional space. Under an orthogonal transformation it transforms according to Rij Fj ðR1 rÞ:

ð1:2:4:4Þ

Dj

j¼j‘mj

j

n P

‘þm M

D‘ Dm ¼

A rank-zero tensor is a scalar, which is invariant under OðnÞ. A pseudovector (or axial vector) has components xi and transforms according to P xi ! x0i ¼ DetðRÞ Rij j

Fi ðrÞ0 ¼

ð1:2:4:3Þ

if R is a rotation with rotation angle ’. From the character it follows that the dimension of the representation D‘ is equal to ð2‘ þ 1Þ. The tensor product of two irreducible representations of SO(3) is generally reducible:

A tensor of rank r under OðnÞ is an object with components Ti1 ...ir (ij ¼ 1; 2; . . . ; n) that transforms as (see Section 1.1.3.2) Ti1 ...ir ! Ti01 ...ir ¼

sinð‘ þ 12Þ’ sin 12 ’

fRij g 2 OðnÞ:

ij

i¼1

R 2 SOð3Þ:

The irreducible representations are labelled by non-negative integers ‘ and have character

A vector is an element of an N-dimensional vector space that transforms under an orthogonal transformation, an element of Oðn), as n P

D ðRÞ ¼ ðRÞ;

D1 D1 ¼ D0 D1 D2 ;

ð1:2:4:2Þ

j¼1

the space of rank 2 Cartesian tensors is the direct sum of three invariant subspaces. This corresponds to the fact that a general rank 2 tensor can be written as the sum of a diagonal tensor, an antisymmetric tensor and a symmetric tensor with trace zero. These three tensors are irreducible tensors, in this case also called spherical tensors, i.e. irreducible tensors for the orthogonal group. An irreducible tensor with respect to the group Oð3Þ transforms, in general, according to some reducible representation of a point group K 2 Oð3Þ. If the group K is a symmetry of the physical system, the tensor should be invariant under K, i.e. it should transform according to the identity representation of K. Consider, for example, a symmetric second-rank tensor under Oð3Þ. This means that it belongs to the space that transforms according to the representation

In a similar way, one has (pseudo)tensor functions under the orthogonal group or the Euclidean group. So it is important to specify under what group an object is a tensor, unless no confusion is possible. The n-dimensional vectors form a vector space that carries a representation of the group O(n). Moreover, it is an irreducible representation space. To stress this fact, one could speak of irreducible tensors and vectors. Vectors are here just rankone tensors. The three-dimensional Euclidean vector space carries in this way an irreducible representation of O(3). Such representations are characterized by an integer l and are ð2l þ 1Þ-dimensional. The usual three-dimensional space is therefore an irreducible l ¼ 1 space for O(3). Since point groups are subgroups of the orthogonal group and space groups are subgroups of the Euclidean group, tensors inherit their transformation properties from their supergroups. As we have seen in Sections 1.2.2.3 and 1.2.2.7, one can also deﬁne tensors in a quite abstract way. Irreducible tensors under a group are then elements of a vector space that carries an irreducible representation of that group. Generally, tensors are elements of a vector space that carries a tensor product representation and (anti)symmetric tensors belong to a space with an (anti)symmetrized tensor product representation. Because the point groups one usually considers in physics are subgroups of O(2) or O(3), it is useful to consider the irreducible representations of these groups. The groups O(2) and O(3) are not ﬁnite, but they are compact, and for compact groups most of

D0 D2 [see (1.2.4.6)]. If the symmetry group of the system is the point group K ¼ 432, the representation D0 ðKÞ D2 ðKÞ has character R:

"

ðRÞ:

6

¼ C3 0

2 2 ¼ C4z

2

and is equivalent to the direct sum

51

¼ C4z 0

¼ C2 2

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1 3 5 : basis such that the representation corresponds to a choice of matrix representation. In particular, if the representation is The multiplicity of 1 is one. Therefore, the space of tensors reducible, it is possible to construct a basis such that the matrix invariant under K is one-dimensional. Consequently, there is only representation is in reduced form. This can be achieved with one parameter left to describe such a symmetric second-rank projection operators. tensor invariant under the cubic group K ¼ 432. Noninvariant Suppose the element R 2 K acts in a space as an operator DðRÞ symmetric second-rank tensors are sums of tensors which trans- such that the representation DðKÞ is equivalent with a matrix form according to the 3 and 5 representations. Here we are representation ðKÞ which has irreducible components ðKÞ. especially interested in invariant tensors. Then choose a vector v in the representation space and construct the d vectors 1.2.4.2. Invariants P vi ¼ ð1=NÞ ðRÞ ji DðRÞv ð1:2:4:7Þ The dimension of the space of tensors of a certain type which R2K are invariant under a point group K is equal to the number of free parameters in such a tensor. This number can be found as the with j ﬁxed. If v does not have a component in the invariant space multiplicity of the identity representation in the tensor space. For of the irreducible representation D , these vectors are all zero, the 32 three-dimensional point groups this number is given in but for a sufﬁciently general vector the d vectors form a basis for Table 1.2.6.9 for general second-rank tensors, symmetric second- the irreducible representation. This property follows from the rank tensors and a number of higher-rank tensors. orthogonality relations. Invariant tensors, i.e. tensors of a certain type left invariant by Using this relation one can write for an invariant symmetric a given group, may be constructed in several ways. The ﬁrst way is second-rank tensor a direct calculation. Take as an example again a second-rank P P symmetric tensor invariant under the cubic group 432. This f ¼ ð1=NÞ DðRÞf 0 ¼ ð1=NÞ ðRÞf 0 ðRÞT means that R2K R2K Rf ¼ f

8 R 2 K;

for an arbitrary symmetric second-rank tensor f 0 . For the group K ¼ 432 this would give a tensor with components fij ¼ aij. Of course, this is a rather impractical method if the order of the group is large. A simple example for a very small group is the construction of the symmetrical and antisymmetrical components of a function: f ðxÞ ¼ ½f ðxÞ f ðxÞ=2.

which is a concise notation for P ðRf Þij ¼ Rik Rjl fkl ¼ fij : kl

The group has two generators. Because each element of K is the product of generators, a tensor is left invariant under a group if it is left invariant by the generators. Therefore, one has in this case for 0 1 a1 a2 a3 f ¼ @ a2 a4 a5 A a3 a5 a6 the equation

1.2.4.3. Clebsch–Gordan coefﬁcients The tensor product of two irreducible representations of a group K is, in general, reducible. If ai is a basis for the irreducible representation (i ¼ 1; . . . ; d ) and bj one for (j ¼ 1; . . . ; d ), a basis for the tensor product space is given by eij ¼ ai bj :

0

0

B @1 0

1

0

1 0

0

1

0

1

On this basis, the matrix representation is, in general, not in reduced form, even if the product representation is reducible. Suppose that P m :

C B C 0 Af @ 1 0 0 A 1 0 0 1 1 1 0 0 0 1 0 1 0 C B C B ¼ @ 0 0 1 Af @ 1 0 0 A ¼ f : 0 1 0 1 0 0 0 0 0

This means that there is a basis

These equations form a system of 12 linear algebraic equations for the coefﬁcients of f with the solution a1 ¼ a4 ¼ a6 ;

‘k

on which the representation is in reduced form. The multiplicity m gives the number of times the irreducible component occurs in the tensor product. The basis transformation is given by X

a bj : ¼ ð1:2:4:8Þ ‘k i j k ‘ i ij

a2 ¼ a3 ¼ a5 ¼ 0:

Up to a factor there is only one 0 a f ¼ @0 0

ð‘ ¼ 1; . . . ; m ; k ¼ 1; . . . ; d Þ;

such tensor: 1 0 0 a 0 A; 0 a

The basis transformation is unitary if one starts with orthonormal bases and has coefﬁcients

ð1:2:4:9Þ i j k ‘

in agreement with the ﬁnding that the space of invariant secondrank symmetric tensors is one-dimensional. An overview of these relations for the 32 point groups can be found in Section 1.1.4 in this volume. This method can always be used for groups with a ﬁnite number of generators. Another method for determining invariant tensors is using projection operators. If a group, for example a point group, acts in some linear vector space, for example the space of tensors of a certain type, this space carries a representation. Then it is possible to construct a

called Clebsch–Gordan coefﬁcients. For the group O(3) they are the original Clebsch–Gordan coefﬁcients; for bases j‘mi and j‘0 m0 i of the (2‘ þ 1)- and (2‘0 þ 1)-dimensional representations D‘ and D‘0 , respectively, of O(3) one has

52

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS

‘

J variables. One can consider the combined operation of T and a j‘mi j‘0 m0 i; jJMi ¼ 0 Euclidean transformation. In other words, we consider the direct m M m m0 m product of the Euclidean group EðdÞ and the time-reversal group ðJ ¼ j‘ ‘0 j; . . . ; ‘ þ ‘0 Þ: ð1:2:4:10Þ of order 2. Elements of this direct product that belong to EðdÞ are called orthochronous, whereas the elements of the coset which The multiplicity here is always zero or unity, which is the reason are combinations of a Euclidean transformation with T are called why one leaves out the number ‘ in the notation. antichronous. We shall start by considering combinations of T If the multiplicity m is unity, the coefﬁcients for given ; ; and orthogonal transformations in the physical d-dimensional are unique up to a common factor for all i; j; k. This is no longer space. Such combinations generate a subgroup of the direct the case if the multiplicity is larger, because then one can make product of OðdÞ and the time-reversal group. linear combinations of the basis vectors belonging to . Anyway, There are three types of such groups. First, one can have a one has to follow certain conventions. In the case of O(3), for group that is already a subgroup of OðdÞ. This group does not example, there are the Condon–Shortley phase conventions. The have time-reversing elements. A second type of group contains degree of freedom of the Clebsch–Gordan coefﬁcients for given the operator T and is, therefore, the direct product of a subgroup matrix representations can be seen as follows. Suppose that of OðdÞ with the time-reversal group. The third type of group there are two basis transformations, S and S0 , in the tensor contains antichronous elements but not T itself. This means that product space which give the same reduced form: the group contains a subgroup of index 2 that belongs to OðdÞ and M 1 01 one coset of this subgroup, all elements of which can be obtained 0 m D : S D D S ¼ S D D S ¼ D ¼ from those of the subgroup by multiplication with one ﬁxed timeð1:2:4:11Þ reversing element which is not T. If one then multiplies all elements of the coset by T, one obtains a group that belongs to Then the matrix S0 S1 commutes with every matrix DðRÞ OðdÞ and is isomorphic to the original group. This is the same (R 2 K). If all multiplicities are zero or unity, it follows from situation as for subgroups of Oð3Þ, which is the direct product Schur’s lemma that S0 S1 is the direct sum of unit matrices of of SOð3Þ with space inversion I. Here also all subgroups of dimension d . If the multiplicities are larger, the matrix S0 S1 is a OðdÞ Z2 are isomorphic to point groups or to the direct product of a point group and Z2 . Magnetic groups can be used to chardirect sum of blocks which are of the form acterize spin arrangements. Because spin inverses sign under time 1 0 11 E 12 E . . . 1m E reversal, a spin arrangement is never invariant under T. ThereB 21 E 22 E . . . 2m E C fore, the point groups of the second type are also called C B C; B .. .. .. .. nonmagnetic point groups. Because time reversal does not play a A @ . . . . role in groups of the ﬁrst type, these are called trivial magnetic m 1 E . . . . . . m m E point groups, whereas the groups of the third type are called nontrivial magnetic point groups. such that Detðij Þ ¼ 1, and the E’s are d -dimensional unit Magnetic point groups are discussed in Chapter 1.5. Orthomatrices. This means that for multiplicity-free (m 1) cases, chronous magnetic point groups (trivial magnetic groups) are the Clebsch–Gordan coefﬁcients are unique up to a common denoted by their symbol as a normal point group. Magnetic point factor for all coefﬁcients involving one value of . groups containing T are denoted by the symbol for the orthoThe Clebsch–Gordan coefﬁcients satisfy the following rules: chronous subgroup, which is a trivial magnetic group, to which

the symbol 10 is added. Magnetic point groups that are neither

trivial nor contain T are isomorphic to a trivial magnetic point ¼ j i k ‘ i j k ‘ group. They are denoted by the symbol of the latter in which all

symbols for antichronous elements are marked with a prime (0 ).

0 is ¼ 0; if D

D does not contain D For example, 1 is the trivial magnetic group generated by I, 11 i j k ‘ 0 the group of four elements generated by I and T, and 1 is the

X

magnetic group of order 2 generated by the product IT.

¼ ii0 jj0

k ‘ 0 0 Two magnetic point groups are called equivalent if they are k ‘ i j i j k‘ conjugated in OðdÞ Z2 by an element in OðdÞ. This means that

X

under the conjugation antichronous elements go to antichronous

¼ kk0 ‘‘0 : elements. The equivalence classes of magnetic point groups are i j k ‘ i j k0 ‘0 ij the magnetic crystal classes. There are 32 classes of trivial crysFor the basis vectors of the invariant space belonging to the tallographic magnetic point groups, 32 classes of direct products with the time-reversal group and 58 classes of nontrivial magnetic identity representation 1 , one has ¼ d ¼ 1. Consequently, crystallographic point groups. They are given in Table 1.2.6.12.

X 1

a bj : ‘ ¼ i j 1 ‘ i X ‘

0

ij

1.2.5.2. Magnetic space groups Magnetic space groups are subgroups of the direct product of the Euclidean group EðdÞ with the time-reversal group (this direct product is sometimes called the Shubnikov group) such that the orthochronous elements together with the products of the antichronous elements and T form a space group in d dimensions. As in the case of magnetic point groups, one can distinguish trivial magnetic groups, which are subgroups of EðdÞ, direct products of a trivial group with the time-reversal group (nonmagnetic) and nontrivial magnetic space groups with antichronous elements but without T. The groups of the third type can be transformed into groups of the ﬁrst type by multiplication of all antichronous elements by T.

1.2.5. Magnetic symmetry 1.2.5.1. Magnetic point groups Until now, the symmetry transformations we have considered affect only spatial variables. In physics, however, time coordinates are also often essential, and time reversal is a very important transformation as well. The time-reversal operation generates a group of order 2 with as elements the unit operator E and the time-reversal operator T. This transformation commutes with transformations of spatial

53

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES The translation subgroup U of a magnetic space group G is the intersection of G and TðdÞ fE; Tg. The factor group G/U is (isomorphic to) a subgroup of OðdÞ fE; Tg. For trivial magnetic space groups, the point group is a subgroup of OðdÞ. For direct products with fE; Tg, the translation group is the direct product of an orthochronous lattice with fE; Tg and the point group is a subgroup of OðdÞ. Magnetic space groups with antichronous elements but without T have either a translation subgroup consisting of orthochronous elements or one with antichronous elements as well. In the ﬁrst case, the point group is a subgroup of OðdÞ fE; Tg and contains antichronous elements; in the second case, one may always choose orthochronous elements for the coset representatives with respect to the translation group, and the point group is a subgroup of OðdÞ. Therefore, nontrivial magnetic space groups without T have either the same lattice or the same point group as the space group of orthochronous elements. Two magnetic space groups are equivalent if they are afﬁne conjugated via a transformation with positive determinant that maps antichronous elements on antichronous elements. Then there are 1651 equivalence classes: 230 classes of trivial groups with only orthochronous elements, 230 classes of direct products with fE; Tg and 1191 classes with nontrivial magnetic groups.

Table 1.2.5.1. Character of the representations corresponding to the electric and magnetic ﬁelds in point groups 222, 20 20 2 and 20 mm0 ni is the number of invariants.

3 3 3

1 1 1

1 1 1

1 1 1

ni

B

0 0 1

3 3 3

ni 1 1 1

1 1 1

1 1 1

0 1 1

1.2.5.4. Time-reversal operators In quantum mechanics, symmetry transformations act on state vectors as unitary or anti-unitary operators. For the Schro¨dinger equation for one particle without spin, @ h- i ðr; tÞ ¼ Hðr; tÞ; @t

ð1:2:5:2Þ

the operator that reverses time is the complex conjugation operator with

ðr; tÞ ¼ ðr; tÞ

ð1:2:5:3Þ

satisfying @ h- i ðr; tÞ ¼ H ðr; tÞ; @t which is the time-reversed equation. This operator is anti-linear [ ð þ Þ ¼ þ ] and has the following commutation relations with the operators r and p for position and momentum:

E 1 10 1 0 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1

r 1 ¼ r;

p 1 ¼ p:

ð1:2:5:4Þ

For a Euclidean transformation g ¼ fRjag, the operation on the state vector is given by the unitary operator

0

0. Here 1 ¼ 11 In general, a vector transforms as the position vector r under but not under 10 . A pseurotations and changes sign under 1, dovector under 1 or (respectively and) 10 gets an additional minus sign. The generalization to tensors is straightforward. n P Q gTi1 ...in ¼ "P "T Rik jk Tj1 ...jn ; ð1:2:5:1Þ j1 ...jn

E

222 20 20 2 20 mm0

of the representations corresponding to the electric and magnetic ﬁelds in two orthorhombic point groups (222, 20 20 2 and 20 mm0 ) are given in Table 1.2.5.1. The number of invariant components is the multiplicity of the trivial representation in the representation to which the tensor belongs. The nonzero invariant ﬁeld components are Bz for 20 20 2, Ex and By for 20 mm0 . These components can be constructed by means of projection-operator techniques, or more simply by solving the linear equations representing the invariance of the tensor under the generators of the point group. For example, the magnetic ﬁeld vector B transforms to (Bx ; By ; Bz ) under my and to (Bx ; By ; Bz ) under m0z , and this gives the result that for 20 mm0 all components are zero except By .

1.2.5.3. Transformation of tensors Vectors and tensors transforming in the same way under Euclidean transformations may behave differently when time reversal is taken into account. As an example, both the electric ﬁeld E and magnetic ﬁeld B transform under a rotation as a position vector. Under time reversal, the former is invariant, but the latter changes sign. Therefore, the magnetic ﬁeld is called a pseudovector ﬁeld under time reversal. Under spatial inversion, the ﬁeld E changes sign, as does a position vector, but the ﬁeld B does not. Therefore, the magnetic ﬁeld is also a pseudovector under central inversion. The electric polarization induced by an electric ﬁeld is given by the electric susceptibility, a magnetic moment induced by a magnetic ﬁeld is given by the magnetic susceptibility and in some crystals a magnetic moment is induced by an electric ﬁeld via the magneto-electric susceptibility. Under the four elements of the group generated by T ¼ 10 and I ¼ 1, the ﬁelds and susceptibility tensors transform according to E B ee mm me

Point group

Tg ðrÞ ¼ ðg1 rÞ ¼ ðR1 ðr aÞÞ:

ð1:2:5:5Þ

The two operators and Tg commute. Therefore, if g is an orthochronous element of the symmetry group, the corresponding operator is Tg, and if gT is an antichronous element the operator is Tg. The operator Tg is also anti-unitary: it is antilinear and conserves the absolute value of the Hermitian scalar product: jh Tg j Tg ij ¼ jhjij. If the particle has a spin, the time-reversal operator has to have the commutation relation

k¼1

where "P and "T are 1, depending on the pseudotensor character with respect to space and time reversal, respectively. Under a rotation [R 2 SOðdÞ], a vector transforms according to a representation characterized by the character ðRÞ of the representation. In two dimensions ¼ 2 cos ’ and in three dimensions ¼ 1 þ 2 cos ’, if ’ is the rotation angle. Under IR the character gets an additional minus sign, under RT it is the same, and under RIT there is again an additional minus sign. For pseudovectors, either under I or T or both, there are the extra factors "P, "T and "P "T , respectively. As an example, the character

S 1 ¼ S

ð1:2:5:6Þ

with the spin operator S. For a spin-12 particle, the spin operators are Si ¼ h- i =2 in terms of the Pauli matrices. Then the timereversal operator is TT ¼ 2 :

54

ð1:2:5:7Þ

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS DðhÞ 0 The operators corresponding to the elements of a magnetic ; MðhÞ ¼ symmetry group are generally (anti-)unitary operators on the 0 Dða1 haÞ state vectors. These operators form a representation of the 0 DðahaÞ magnetic symmetry group. MðahÞ ¼ ; h 2 H; a 2 H 0 DðhÞ 0 Tg Tg0 ¼ Tgg0 : ð1:2:5:8Þ In principle, they even form a projective representation, but as discussed before for particles without spin the factor system is trivial, and for particles with spin one can take as the symmetry group the double group of the symmetry group.

because

Dða1 haÞ ¼ U 1 DðhÞU ð1:2:5:10Þ

The basis transformation T¼

ð1:2:5:11Þ

MðhÞ ! S MðhÞS;

MðahÞ ! S MðahÞS ;

m P

Mða1 haÞ ji Ta j :

1 0

0 U 1

8 h 2 H:

The most general basis transformation S that leaves MðhÞ in the same form is then E E S¼ : ð1:2:5:15Þ E E

ðh 2 HÞ: ð1:2:5:12Þ

Here a is the coset representative of the antichronous elements. The co-representation restricted to the orthochronous subgroup H gives an ordinary representation of H which is not necessarily irreducible even if the co-representation is irreducible. Suppose that 1 . . . m form a basis for the irreducible co-representation of G and that the restriction to H is also irreducible. The elements Ta 1 ; . . . ; Ta m form another basis for the space, and on this basis the representation matrices of H follow from Th Ta i ¼ Ta Ta1 ha i ¼

DðahaÞji ’j :

then gives a new matrix co-representation for G: DðhÞ 0 MðhÞ ! T 1 MðhÞT ¼ ; 0 DðhÞ 0 DðahaÞU 1 MðahÞ ! T 1 MðahÞT ¼ : UDðhÞ 0

transforms the matrices according to 1

P

The two irreducible components for MðHÞ can be either equivalent or non-equivalent. If they are not equivalent the corepresentation is indeed irreducible, because a basis transformation S that leaves the matrices MðhÞ the same is necessarily of the form E E because of Schur’s lemma, and such a matrix cannot bring the matrices Dðah) into a reduced form. In this case, the co-representation MðGÞ is irreducible, in agreement with the starting assumption, and the dimension m is twice the dimension of the representation DðHÞ: m ¼ 2d. If the two irreducible components DðHÞ and Dða1 HaÞ are equivalent, there is a basis transformation U such that

j¼1

1

DðhÞ ji Ta ’j

j

as one veriﬁes easily. Matrices satisfying these relations are called co-representations of the group G. A co-representation is irreducible if there is no proper invariant subspace. If a co-representation is reducible, there is a basis transformation S that brings the matrices into a block form. For co-representations, a basis transformation S with Sji j

P j

Ta hTa ’i ¼ Ta ha’i ¼

The matrices M do not form a matrix representation in the usual sense. They satisfy the relations

m P

DðhÞji ’j ¼

j

k

Si ¼

P

Ta h’i ¼ Ta

1.2.5.5. Co-representations Suppose the magnetic point group G has an orthochronous subgroup H and an antichronous coset H 0 ¼ aH for some antichronous element a. The elements of H are represented by unitary operators, those of H 0 by anti-unitary operators. These operators correspond to matrices in the following way. Suppose j are the elements of a basis of the state vector space. Then P Tg j ¼ MðgÞkj k ; g 2 G: ð1:2:5:9Þ

Mðg1 g2 Þ ¼ Mðg1 ÞMðg2 Þ g1 2 H ¼ Mðg1 ÞM ðg2 Þ g1 2 H 0 ;

ð1:2:5:14Þ

Under this basis transformation, the matrices MðahÞ become S1 MðahÞS ¼

1 M ð Þ

with M11 ¼ UDðhÞ þ DðahaÞU 1 M12 ¼ jj2 DðahaÞU 1 j j2 UDðhÞ

ð1:2:5:13Þ

M21 ¼ jj2 UDðhÞ jj2 DðahaÞU 1

j¼1

M22 ¼ UDðhÞ DðahaÞU 1 :

Because both bases are bases for the same irreducible space, it means that the (ordinary) representations MðHÞ and Mða1 HaÞ are equivalent. If the representation MðHÞ is reducible, there is a basis ’1 ; . . . ; ’d for the irreducible representation DðHÞ. A basis for the whole space then is given by

This is block diagonal if j j2 UU Dða1 haÞU 1 U ¼ jj2 DðahaÞ and analogous expressions for jj2 and jj2 also hold. The transformation matrix U satisﬁes UU ¼ Dða2 Þ, as one can show as follows. From the deﬁnition

’1 ; . . . ; ’d ; Ta ’1 ; . . . ; Ta ’d ;

Dða1 haÞ ¼ U 1 DðhÞU

because the co-representation of G would be reducible if the last d vectors were dependent on the ﬁrst d. On this basis, the matrices for the co-representation become

follow the two relations

55

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 2

2

Dða ha Þ ¼ U

1

Dða1 haÞ ¼ U 1 DðhÞU:

U 1 DðhÞUU

Dða2 ha2 Þ ¼ Dða2 Þ1 DðhÞDða2 Þ:

Then we have P P P ðahahÞ ¼ Dða2 Þik ðU 1 Þkm DðhÞ mn Un‘ DðhÞ‘i h2H h2H ik‘mn P ¼ ðN=dÞ Dða2 Þik ðU 1 Þk‘ Ui‘

2

(Notice that a 2 H.) Because DðHÞ is irreducible, it follows that UU Dða2 Þ is a multiple of the identity: UU ¼ Dða2 Þ. The factor is real because

i;k;‘

Dða2 Þ ¼ U 1 Dða2 ÞU ¼ U 1 UU U=

¼ ðN=dÞ

P

Dða2 Þik ðU UÞik

i;k

and

¼ ðN=dÞ 2

Dða Þ ¼ U U= :

Dða2 Þik Dða2 Þki ¼ N:

i;k

This proves theorem (2). In the special case of a group G in which the time reversal 10 occurs as element, one may choose a ¼ 10. In this case, a2 is the identity and the expressions simplify. Theorem (1) now states that an irreducible d-dimensional representation DðHÞ of an orthochronous group can occur as irreducible component in the restriction of an irreducible m-dimensional co-representation of H fE; 10 g, with

Hence ¼ ¼ 1. The conditions for the transformed matrix MðahÞ to be block diagonal then read j j2 Dða2 ÞDða1 haÞ ¼ jj2 DðahaÞ;

P

ð1:2:5:16Þ

with the corresponding expressions for and . If is equal to 1, these equations do not have a solution. However, when ¼ þ1 there is a solution, which means that the corepresentation is reducible, contrary to the assumption. Therefore, this situation can not occur. One can summarize these considerations in the following theorem.

m ¼ 2d if DðHÞ nonequivalent to DðHÞ m ¼ 2d if DðHÞ ¼ UDðHÞ U 1 and UU ¼ E m ¼ d if DðHÞ ¼ UDðHÞ U 1 and UU ¼ þE;

Theorem 1. If the restriction of an irreducible co-representation to the orthochronous subgroup is reducible, then either the (two) irreducible components are non-equivalent, or they are equivalent and connected by a basis transformation U for which UU ¼ Dða2 Þ. If the restriction MðHÞ is irreducible, it is equivalent to Mða1 HaÞ .

which correspond to, respectively, [cf. theorem (2)] 8 < 0 P ðh2 Þ ¼ N : : h2H þN

ð1:2:5:19Þ

For a spinless particle, the time-reversal operator is the complex conjugation . This generates a co-representation of the group Z2. The symmetry group is the direct product of the point group H and Z2 . Compared to the degeneracy d of a state characterized by the irreducible representation DðHÞ, the degeneracy is double (m ¼ 2d) for the ﬁrst two cases and the same for the third case. When it is a particle with spin 12, the time-reversal operator is 2 , which is of order 4. If one takes for the coset representative a the time reversal, one has Dða2 Þ ¼ E. Therefore, the degeneracy is now doubled in the ﬁrst and third case, and the same for the second. This is Kramer’s degeneracy.

In the former case, the dimension of the co-representation is twice that of the restriction, in the latter case they are equal. Therefore, one has the following corollary. Corollary. A d-dimensional irreducible representation of the orthochronous subgroup H can occur as irreducible component of the restriction of an irreducible co-representation of G with dimension m with m ¼ 2d if DðHÞ nonequivalent to Dða1 HaÞ m ¼ 2d if DðHÞ equivalent to Dða1 HaÞ and UU ¼ Dða2 Þ m ¼ d if DðHÞ equivalent to Dða1 HaÞ and UU ¼ þDða2 Þ:

1.2.6. Tables The three cases from theorem (1) can be distinguished by the following theorem:

In the following, a short description of the tables is given in order to facilitate consultation without reading the introductory theoretical Sections 1.2.2 to 1.2.5. Table 1.2.6.1. Finite point groups in three dimensions. The point groups are grouped by isomorphism class. There are four inﬁnite families and six other isomorphism classes. (Notation: Cn for the cyclic group of order n, Dn for the dihedral group of order 2n, T, O and I the tetrahedral, octahedral and icosahedral groups, respectively). Point groups of the ﬁrst class are subgroups of SO(3), those of the second class contain E, and those of the third class are not subgroups of SO(3), but do not contain E either. The families Cn and Dn are also isomorphism classes of two-dimensional ﬁnite point groups. Table 1.2.6.2. Among the inﬁnite number of ﬁnite threedimensional point groups, 32 are crystallographic. Table 1.2.6.3. Character table for the cyclic groups Cn. The generator is denoted by . The number of elements in the conjugacy classes (ni ) is one for each class. The order is the smallest nonnegative power p for which Ap ¼ E. The n irreducible representations are denoted by i . Table 1.2.6.4. Character tables for the dihedral groups Dn of order 2n. ni is the number of elements in the conjugacy class Ci . The irreducible representations are denoted by i .

Theorem 2. The irreducible representation DðHÞ with character ðHÞ belongs to the respective cases of theorem (1) if 8 < 0 for the first case P ðahahÞ ¼ N for the second case ð1:2:5:17Þ : h2H N for the third case:

The proof of theorem (2) goes as follows. We have P h2H

ðahahÞ ¼

d PP

DðahahÞii P P ¼ Dða2 Þik Dða1 haÞkl DðhÞli ; h2H i¼1 i;k;l

h2H

ð1:2:5:18Þ and this gives zero if DðHÞ and Dða1 HaÞ are non-equivalent, because of the orthogonality relations. If the two representations are equivalent, we take for convenience unitary representations. Then there is a unitary matrix U with

56

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS Table 1.2.6.1. Finite point groups in three dimensions Isomorphism class

First class with determinants > 0

Cn

n

Dn

n22 (n even) n2 (n odd, > 1)

Second class with E

T O I T C2 O C2 I C2

23 432 532

Second class with E

Third class without E

1

m

2=m 3

4 2mm 6 3m

4=m mmm 3m

622 23

A; A1 ; A2 ; A0 ; A00 B; B1 ; B2 ; B3 E T; T1 ; T2 Ag ; Bg etc: Au ; Bu etc:

43m

432 6=mmm m3 m3m

one-dimensional one-dimensional two-dimensional three-dimensional gerade ungerade

The other notation for which the relation with the present notation is indicated is that of Kopsky´, and is used in the accompanying software. The three functions x, y and z transform according to the vector representation of the point group, which is generally reducible. The reduction into irreducible components of this three-dimensional vector representation is indicated. The six bilinear functions x2, xy, xz, y2 , yz, z2 transform according to the symmetrized product of the vector representation. The basis functions of the irreducible components are indicated. Because the basis functions are real, one should consider the physically irreducible representations. Table 1.2.6.6. The point groups of the second class containing E are obtained from those of the ﬁrst class by taking the direct From the point groups, product with the group generated by 1. one obtains nonmagnetic point groups by the direct product with the group generated by the time reversal 10 . The relation between the characters of a point group and its direct products with

1 2 3 4 4 6 6 8 8 8 12 12 12 16 24 24 24 48

6mm, 62m

6=m 4=mmm

12 24 60 24 48 120

groups of the second kind) the sign of the representative of E. This nomenclature is often used by spectroscopists.

Order

4mm, 42m

422

4n

m3 m3m 5 3m

Table 1.2.6.2. Crystallographic point groups in three dimensions

1 2 3 4 222 6 32

2n 2n

43m

Table 1.2.6.5. The character tables for the 32 three-dimensional crystallographic point groups. The groups are grouped by isomorphism class (there are 18 isomorphism classes). For each isomorphism class, the character table is given, including the symbol for the isomorphism class, the number n of elements per conjugacy class and the order of the elements in each such class. The conjugation classes are speciﬁed by representative elements expressed in terms of the generators ; ; . . .. The irreps are denoted by i, where i takes as many values as there are conjugation classes. In each isomorphism class for each point group, given by its international symbol and its Schoenﬂies symbol, identiﬁcation is made between the generators of the abstract group (; ) and the generating orthogonal transformations. Notation: Cnx is a rotation of 2=n along the x axis, x is a reﬂection from a plane perpendicular to the x axis, Snz is a rotation over 2=n along the z axis multiplied by E and v is a reﬂection from a plane through the unique axis. The notation for the irreducible representations can be given as i, but other systems have been used as well. Indicated below are the relations between i and a system that uses a characterization according to the dimension of the representation and (for

C1 C2 C3 C4 D2 C6 D3 C4 C2 D4 D2 C2 D6 T C6 C2 D4 C2 O D6 C2 T C2 O C2

n

n (n odd) n=m (n even) n=mmm (n even, 4) mmm (n ¼ 2) n m (n odd, > 0)

Dn C2

First class

Order

n (n even, > 2) m (n ¼ 2) nmm (n even) n 2m (n even) nm (n odd)

Cn C2

Isomorphism class

Third class without E

Table 1.2.6.4. Irreducible representations for dihedral groups Dn (a) n odd. m ¼ 1; . . . ; ðn 1Þ=2; j ¼ 1; . . . ; ðn 1Þ=2, l.c.d. = largest common divisor. ni Order

" 1 1

j 1 n/l.c.d.(n; j)

... 2 ...

n 2

1 2 2þm

1 1 2

1 1 2 cosð2mj=nÞ

... ... ...

1 1 0

(b) n even. m ¼ 1; . . . ; ðn=2 1Þ; j ¼ 1; . . . ; ðn=2 1Þ, l.c.d. = largest common divisor.

Table 1.2.6.3. Irreducible representations for cyclic groups Cn ! ¼ expð2i=nÞ, l.c.d. = largest common divisor. ni Order

" 1 1

1 n

2 1 n/l.c.d.(n, 2)

3 1 n/l.c.d.(n, 3)

... ... ...

n1 1 n

1 2 .. . n

1 1 1 1

1 ! .. . !1

1 !2 .. . !2

1 !3 .. . !3

... ... .. . ...

1 !1 .. . !

57

ni Order

" 1 1

n=2 1 2

j 2 n/l.c.d.ðn; jÞ

... ... ...

n=2 2

n=2 2

1 2 3 4 4þm

1 1 1 1 2

1 1 ð1Þn=2 ð1Þn=2 ð1Þm 2

1 1 ð1Þj ð1Þj 2cos(2mj=n)

... ... ... ... ...

1 1 1 1 0

1 1 1 1 0

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.2.6.5. Irreducible representations and character tables for the 32 crystallographic point groups in three dimensions (a) C1

(e) C6 [! ¼ expði=3Þ]. C1 n Order

" 1 1

C6 n Order

" 1 1

1 6

1

1

1 2 3 4 5 6

1 1 1 1 1 1

1 ! !2 1 ! !2

1 : A ¼ 1

1 C1

x2 ; y2 ; z2 ; yz; xz; xy

x; y; z

(b) C2

2 1 3 1 !2 ! 1 !2 !

3 1 2 1 1 1 1 1 1

4 1 3

5 1 6

1 ! !2 1 ! !2

1 !2 ! 1 !2 !

Matrices of the real representations:

1 Ci

1 2

1 2

1 1

1 1

1 : A ¼ 1 2 : A00 ¼ 3 1 : Ag ¼ 2 : Au ¼

¼I

2 6

x2 ; y2 ; z2 ; xy yz; xz 2

2

2

2

2

2

x ; y ; z ; xy yz; xz

x; y z

þ 1 1

1 3

1 3

1 2 3

1 1 1

1 ! !2

1 !2 !

6 C6

Matrices of the real two-dimensional representation:

3 S6

¼ S3z

6 C3h

¼ S6z

0 1

0 1

1 1

2 1 1 1 0

1 : A ¼ 1 2 3 : E ¼ 1c þ 1c

¼ C3z

3 C3

1 0

2

¼ C6z

x2 þ y2 ; z2 x2 y2 ; xz; yz; xy

z x; y

3 5

1 0 0 1

1 1 1 0 0 1 1 1

5

1 1 1 0 0 1 1 1

1 0 0 1

4

2

" 1 1

2 3

x ; y ; z ; yz; xz; xy x; y; z

C3 n Order

3

(c) C3 [! ¼ expð2i=3Þ].

"

"

z x; y

0

¼ z

m Cs

" 1 1

1 : A ¼ 1 2 : B ¼ 3

¼ C2z

2 C2

C2 n Order

1 : A ¼ 1 4 : B ¼ 3 2 6 : E1 ¼ 1c þ 1c 3 5 : E2 ¼ 2c þ 2c 1 : Ag ¼ þ 1 4 : Au ¼ 1 2 6 : Eu ¼ 1c þ 1c þ 3 5 : Eg ¼ þ 1c þ 1c

0 1 1 1 1 1 1 0

1 0 0 1

1 0 0 1

0 1 1 1 1 1 1 0

z

x2 þ y2 ; z2

x; y

xz; yz x2 y2 ; xy x2 þ y2 ; z2

z x; y x2 y2 ; xy; xz; yz

1 : A0 ¼ 1 4 : A00 ¼ 3 2 6 : E0 ¼ 2c þ 2c 3 5 : E00 ¼ 1c þ 1c

x2 þ y2 ; z2 z xz; yz x2 y2 ; xy

x; y

(d) C4 C4 n Order

" 1 1

1 4

1 2 3 4

1 1 1 1

1 i 1 i

2 1 2 1 1 1 1

(f) D2

3 1 4

D2 n Order

" 1 1

1 2

1 2

1 2 3 4

1 1 1 1

1 1 1 1

1 1 1 1

222 D2

¼ C2x ¼ C2y ¼ C2z

1 2 3 4

: A1 ¼ 1 : B3 ¼ 3 : B2 ¼ 4 : B1 ¼ 2

mm2 C2v

¼ C2z ¼ x ¼ y

1 2 3 4

: A1 ¼ 1 : A2 ¼ 2 : B2 ¼ 3 : B1 ¼ 4

¼ C2z ¼ z ¼ I

1 2 3 4

: Ag ¼ þ 1 : Au ¼ 1 : Bu ¼ 3 þ : Bg ¼ 3

1 i 1 i

1 2 1 1 1 1

Matrices of the real two-dimensional representation:

2 4

4 C4 4 S4

"

1 0

¼ C4z

¼ S4

0 1

0 1

1 0

2 1 0 0 1

1 : A ¼ 1 3 : B ¼ 3 2 4 : E ¼ 1c þ 1c 1 : A ¼ 1 3 : B ¼ 3 2 4 : E ¼ 1c þ 1c

3

0 1 1 0

x; y

x2 þ y2 ; z2 x2 y2 ; xy yz; xz

z x; y

x2 þ y2 ; z2 x2 y2 ; xy yz; xz

z

2=m C2h

58

x y z z y x

z x; y

x2 ; y2 ; z2 yz xz xz x2 ; y2 ; z2 xy yz xz x2 ; y2 ; z2 ; xy z

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS Table 1.2.6.5 (cont.) (i) D6

(g) D3 D3 n Order

" 1 1

2 3

3 2

1 2 3

1 1 2

1 1 1

1 1 0

Matrices of the two-dimensional representation:

3

32 D3 3m C3v

"

1 0 0 1

0 1 1 1

1 : A1 ¼ 1 2 : A2 ¼ 2 3 : E ¼ 1

¼ C3z ¼ v

1 1 0 1

" 1 1

2 6

1 2 3 4 5 6

1 1 1 1 2 2

1 1 1 1 1 1

z x; y

xz; yz; xy; x2 y2

z

x2 þ y2 ; z2

x; y

xz; yz; xy; x2 y2

"

5

2

3

(h) D4 D4 n Order

" 1 1

2 4

1 2 3 4 5

1 1 1 1 2

1 1 1 1 0

2 1 2

2 2

1 1 1 1 2

1 1 1 1 0

"

2

422 D4

4mm C4v

42m D2d

¼ C4z ¼ C2x

¼ C4z ¼ v

¼ S4z ¼ C2v ¼ d

0 1 1 0

1 0 0 1

2 2 1 1 1 1 0

622 D6

1 2 3 4 5

: A1 ¼ 1 : A2 ¼ 2 : B1 ¼ 3 : B2 ¼ 4 : E ¼ 1

1 2 3 4 5

: A1 ¼ 1 : A2 ¼ 2 : B1 ¼ 3 : B2 ¼ 4 : E ¼ 1

1 2 3 4 5

: A1 ¼ 1 : A2 ¼ 2 : B1 ¼ 3 : B2 ¼ 4 : E ¼ 1

6mm C6v

62m D3h

z

x2 þ y2 ; z2

x; y

x2 y2 xy xz; yz

1 1 1 1 2 2

3 2 1 1 1 1 0 0

0 1

1 1

1 0

0 1

: A1 ¼ 1 : A2 ¼ 2 : B 1 ¼ 3 : B 2 ¼ 4 : E 1 ¼ 1 : E 2 ¼ 2

1 2 3 4 5 6

: A1 ¼ 1 : A2 ¼ 2 : B 1 ¼ 3 : B 2 ¼ 4 : E 1 ¼ 1 : E 2 ¼ 2

1 2 3 4 5 6

: A01 ¼ 1 : A02 ¼ 2 : A001 ¼ 3 : A002 ¼ 4 : E0 ¼ 2 : E00 ¼ 1

¼ C6z ¼ v

¼ S6z ¼ C2v ¼ d

¼ S3z ¼ d

1 2 3 4 5 6

1 0

1 1

1 1

0 1

: : : : : :

A1g ¼ þ 1 A2g ¼ þ 2 A1u ¼ 1 A2u ¼ 2 Eu ¼ 1 þ E g ¼ 1

0 1 1 1

1 0

1 0

1 0

0 1

0 1

3 2 1 1 1 1 0 0

1 1 1 0 0 1

1 1

1 0

x2 y2 xy xz; yz

59

x2 þ y2 ; z2 z

x; y

x2 y2 xy xz; yz

z

x2 þ y2 ; z2

x; y

x2 y2 xy xz; yz x2 þ y2 ; z2

z

x2 y2 xy xz; yz

x; y x2 þ y2 ; z2 z x; y xz:yz; xy; x2 y2

(j) T [! ¼ expð2i=3Þ].

x2 þ y2 ; z2

z x; y

1 0

1 2 3 4 5 6

z

x; y

1 1

¼ C6z ¼ C2x

x2 þ y2 ; z2 x2 y2 xy xz; yz

0 1

3m D3v

1 0

0 1 1 0

3 1 2

6

1 0 0 1

1 0 0 1

1 1 1 1 1 1

Matrices of the two-dimensional representation: 5

2 2 3

Matrices of the two-dimensional representations:

x2 þ y2 ; z2

1 : A1 ¼ 1 2 : A2 ¼ 2 3 : E ¼ 1

¼ C3z ¼ C2x

D6 n Order

T n Order

" 1 1

4 3

2 4 3

3 2

1 2 3 4

1 1 1 3

1 ! !2 0

1 !2 ! 0

1 1 1 1

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.2.6.5 (cont.) Real representations of dimension d > 1: 2 3 1 0 0 1

"

2

1 1 0 1

1 1 0 1

23 T

Other point groups which are of second class and contain E. See Table 1.2.6.6(a).

1 0 0 1

4 0

1

1 0 0 @0 1 0A 0 0 1

0

1 0 1 0 @0 0 1A 1 0 0

0

Isomorphism class

Rotation subgroup

4=m 6=m mmm 4=mmm 6=mmm m3 m3m

C4 Z2 C6 Z2 D2 Z2 D4 Z2 D6 Z2 T Z2 O Z2

4 6 222 422 622 23 432

1 0 0 1 @1 0 0A 0 1 0

and fE; 10 g Table 1.2.6.6. Direct products with fE; 1g

0

1 1 0 0 @ 0 1 0 A 0 0 1

(a) With fE; 1g.

2

1 : A ¼ 1 2 3 : E ¼ 3c þ 3c 4 : T ¼ 1

¼ C3d ¼ C2z

Group

2

2

x þy þz x2 y2 ; x2 z2 xy; xz; yz

x; y; z

K Z2

R2K

g u

ðRÞ ðRÞ

R ðRÞ ðRÞ

C4 Z2 C6 Z2 D2 Z2 D4 Z2 D6 Z2 T Z2 O Z2

cf. cf. cf. cf. cf. cf. cf.

K Z2

R2K

R0

þ

ðRÞ ðRÞ

ðRÞ ðRÞ

10 210 m10 22210 2mm10 410 0 41 4mm10 42210 0 42m1 310 3210 0 31 3m10 6mm10 610 0 61 62210 0 62m1 2310 43210 0 43m1

C1 Z2 C2 Z2 C2 Z2 D2 Z2 D2 Z2 C4 Z2 C4 Z2 D4 Z2 D4 Z2 D4 Z2 C3 Z2 D3 Z2 C6 Z2 D3 Z2 D6 Z2 C6 Z2 C6 Z2 D6 Z2 D6 Z2 T Z2 O Z2 O Z2

cf. 1 cf. 2 cf. m cf. 222 cf. 2mm cf. 4 cf. 4 cf. 4mm cf. 422 cf. 42m cf. 3 cf. 32 cf. 3 cf. 3m cf. 6mm cf. 6 cf. 6 cf. 622 cf. 62m cf. 23 cf. 432 cf. 43m

4=m 6=m mmm 4=mmm 6=mmm m3 m3m

4 6 222 422 622 23 432

(k) O O n Order

" 1 1

8 3

1 2 3 4 5

1 1 2 3 3

1 1 1 0 0

2 3 2

6 4

1 1 2 1 1

(b) With fE; 10 g.

6 2

1 1 0 1 1

1 1 0 1 1

Higher-dimensional representations:

"

3

0 1 1 1

2

432 O

43m Td

1 0 0 1

1 0 0 1

0 1 1 0

¼ S4z ¼ C3d ¼ d

0 0 1 0A 0 1

0

1 0 1 0 0A 1 0

0

1 @ 0 0

1 0 0 1 0 A 0 1

5 0

1 1 0 0 @0 1 0A 0 0 1

0

1 0 0 1 @1 0 0A 0 1 0 0

1 1 0 0 @ 0 1 0 A 0 0 1

0

1 1 0 0 0A 0 1

0

0

1 0 0 0 1A 1 0

0

0 @1 0

1

1 @0 0

0 @1 0

1 0 1 1

¼ C4z ¼ C3d ¼ C2

4 0

1 @ 0 0

1 2 3 4 5

: A1 ¼ 1 : A2 ¼ 2 : E ¼ 3 : T 1 ¼ 1 : T 2 ¼ 2

1 2 3 4 5

: A1 ¼ 1 : A2 ¼ 2 : E ¼ 3 : T 1 ¼ 1 : T 2 ¼ 2

1 0 1 0 @ 1 0 0 A 0 0 1

and fE; 10 g. (c) With fE; 1g

1 1 0 0 @ 0 0 1 A 0 1 0

x2 þ y2 þ z2 x2 y2 ; y2 z2

R2K

gþ uþ g u

ðRÞ ðRÞ ðRÞ ðRÞ 1 0 210 =m 4=m10 6=m10 mmm10 4=mmm10 0 3m1 6=mmm10 m310 0 mð3Þm1

x; y; z xy; xz; yz x2 þ y2 þ z2 x2 y2 ; y2 z2 x; y; z

K Z2 Z2

xy; yz; xz

60

R

R0

R 0

ðRÞ ðRÞ ðRÞ ðRÞ

ðRÞ ðRÞ ðRÞ ðRÞ

ðRÞ ðRÞ ðRÞ ðRÞ

C1 Z2 Z2 C2 Z2 Z2 C4 Z2 Z2 C6 Z2 Z2 D2 Z2 Z2 D4 Z2 Z2 D6 Z2 Z2 D6 Z2 Z2 T Z2 Z2 O Z2 Z2

cf. 1 cf. 2 cf. 4 cf. 6 cf. 222 cf. 422 cf. 3m cf. 622 cf. 23 cf. 432

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS 1 and f1; 10 g are given in Tables 1.2.6.6(a), where and n are the rotation angle and axis of the rotation R, groups generated by 1, (b) and (c), respectively. the matrices uðRÞ form a projective representation: Table 1.2.6.7. The representations of a point group are also uðRÞuðR0 Þ ¼ !s ðR; R0 ÞuðRR0 Þ: representations of their double groups. In addition, there are extra representations which give projective representations of the point groups. For several cases, these are associated with an The factor system !s is the spin factor system. It is determined via ordinary representation. As extra representations, those irre- the generators and deﬁning relations ducible representations of the double point groups that give rise Wi ðA1 ; . . . ; Ap Þ ¼ E to projective representations of the point groups with a factor system that is not associated with the trivial one are given. These do not correspond to ordinary representations of the single of the point group K. Then group. Wi ðuðA1 Þ; . . . ; uðAp ÞÞ ¼ i E; Table 1.2.6.8. If one chooses for each element of a point group one of the two corresponding SUð2Þ elements, the latter form a projective representation of the point group. If one selects for the and the factors ﬁx uniquely the class of the factor system ! . i s rotation R 2 K SOð3Þ the element These factors are given in the table. Because 1 is represented by the unit matrix in spin space, the uðRÞ ¼ E cosð’=2Þ þ iðr nÞ sinð’=2Þ; double groups of two isomorphic point groups obtained from each other by replacing the elements R 2 Oð3Þ\SOð3Þ by R are where ’ is the rotation angle and n the rotation axis, and for the same. R 2 K Oð3Þ\SOð3Þ the element The projective representations with factor system !s may sometimes be associated with one with a trivial factor system. If uðRÞ ¼ E cosð =2Þ þ iðr nÞ sinð =2Þ; this is the case, there are actually no extra representations of the 0

Table 1.2.6.7. Extra representations of double point groups d

222 05

E 2

E 2

A 0

B 0

AB 0

422d 06 07

E 2 2

E 2 2

A2 0 0

A pﬃﬃﬃ p2ﬃﬃﬃ 2

A pﬃﬃﬃ p2ﬃﬃﬃ 2

B 0 0

AB 0 0

622d 08 09 07

E 2 2 2

E 2 2 2

A2 1 1 2

A2 1 1 2

B 0 0 0

A3 0 0 0

A5ﬃﬃﬃ p p3ﬃﬃﬃ 3 0

23d 05 06 07

E 2 2 2

E 2 2 2

A 1 ! !5

A 1 !4 !2

A2 1 !2 !4

A2 1 !5 !

B 0 0 0

432d 06 07 08

E 2 2 4

E 2 2 4

B 1 1 1

B 1 1 1

A2 0 0 0

A ﬃﬃﬃ p pﬃﬃ2ﬃ 2 0

A pﬃﬃﬃ p2ﬃﬃﬃ 2 0

5 A pﬃﬃﬃ p3ﬃﬃﬃ 3 0

A3B 0 0 0

AB 0 0 0

Table 1.2.6.8. Projective spin representations of the 32 crystallographic point groups Double group

Extra representations

A¼E A2 ¼ E

1d

No No

2, m 2=m

A2 ¼ E A2 ¼ B2 ¼ E, ðABÞ2 ¼ E

2d

No

222, 2mm mmm

A2 ¼ B2 ¼ ðABÞ2 ¼ E A2 ¼ B2 ¼ ðABÞ2 ¼ E C2 ¼ E; AC ¼ CA, BC ¼ CB

222d

Yes

4, 4 4=m

A4 ¼ E A4 ¼ B2 ¼ E, AB ¼ BA

4d

No

422, 4mm, 42m 4=mmm

A4 ¼ B2 ¼ ðABÞ2 ¼ E As above, plus C2 ¼ E, AC ¼ CA, BC ¼ CB

422d

Yes

3 3

A3 ¼ E A6 ¼ E

3d

No

32, 3m 3m

A3 ¼ B2 ¼ ðABÞ2 ¼ E A6 ¼ E, B2 ¼ ðABÞ2 ¼ E

32d

No

6, 6 6=m

A6 ¼ E A6 ¼ B2 ¼ E, AB ¼ BA

6d

No

622, 6mm, 62m 6=mmm

A6 ¼ B2 ¼ ðABÞ2 ¼ E As above, plus C2 ¼ E, AC ¼ CA, BC ¼ CB

622d

Yes

23 m3

A3 ¼ B2 ¼ ðABÞ3 ¼ E As above, plus C2 ¼ E, AC ¼ CA, BC ¼ CB

23d

Yes

432, 43m m3m

A4 ¼ B3 ¼ ðABÞ2 ¼ E As above, plus C2 ¼ E, AC ¼ CA, BC ¼ CB

432d

Yes

Point group

Relations giving i

1 1

61

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.2.7. Introduction to the accompanying software Tenvar

double group. If there are extra representations, these are irreducible representations of the double group: see Table 1.2.6.7. Table 1.2.6.9. For the 32 three-dimensional crystallographic point groups, the character of the vector representation and the number of times the identity representation occurs in a number of tensor products of this vector representation are given. This is identical to the number of free parameters in a tensor of the corresponding type. For the direct products K C2, the character is equal to that of K on the rotation subgroup, and its opposite [ðRÞ ¼ ðRÞ] for the coset K. Table 1.2.6.10. The irreducible projective representations of the 32 three-dimensional crystallographic point groups that have a factor system that is not associated to a trivial one. In three (and two) dimensions all factor systems are of order two. Table 1.2.6.11. The special points in the Brillouin zones. Strata of irreducible representations of the space groups are characterized by the wavevector k of such a point and a (possibly projective) irreducible representation of the point group K k. The latter is the intersection of the symmetry group of k (the group of k for the holohedral point group) and the point group of the space group. For each Bravais class the special points for the holohedry are given. These are given by their coordinates with respect to a basis of the reciprocal lattice of the conventional cell. These points correspond to Wyckoff positions in the corresponding dual lattice. The symbols for these Wyckoff positions and their site symmetry are given. A well known notation for the special points is that of Kovalev, as used in his book on representations of space groups. Correspondence with the notation in Kovalev (1987) is given. Table 1.2.6.12. The three-dimensional crystallographic magnetic and nonmagnetic point groups of type I (trivial magnetic, no antichronous elements), type II (nonmagnetic, containing time reversal as an element) and type III (nontrivial magnetic, without time reversal itself, but with antichronous elements).

By M. Ephraı¨m, T. Janssen, A. Janner and A. Thiers 1.2.7.1. Overview The determination of tensors with speciﬁed properties often requires long calculations. In principle the algorithms are simple, but in complicated cases errors can be made. This is therefore a situation in which it is best to rely on computer calculations. For this reason, this volume is accompanied by two software packages. Here we shall give a short introduction to the Tenar package that deals with tensors with speciﬁc symmetry properties in the ﬁrst module, and with characters of representations of point groups in the second module. The latter play a role when determining the number of independent elements of a tensor invariant under a given point group, but they are much more widely applicable. The software package has a graphical interface with windows and buttons. When the program is started, a window opens up in which a choice may be made between the tensor part or the character part of the program. Within each of the two sections of the program, the results of the calculations are given in numbered windows. It is possible to browse through the various pages. Each page may be sent to a separate window (by the command ‘to window’), or to a ﬁle (by the command ‘to ﬁle’). Opened windows may be closed again using a ‘close’ button. Special features of the package are that it is dimension- and rank-independent, and that it performs the calculations in an exact way. The number of dimensions and the rank are only limited by the computer memory and by the time the program needs for higher dimensions and ranks. The calculations are exact in the sense of the computer algebra software. Here this is achieved by performing the calculations with integers and

Table 1.2.6.9. Number of free parameters of some tensors

Group

Character of the vector representation

Multiplicity identity representation in

Isomorphism class

2

2 s

3

2 s

ð 2 s Þs

1 1

C1 C2

3 3, 3

9 9

6 6

27 0

18 0

21 21

2 m 2=m

C2 C2 C2 C2

3, 1 3, 1

5 5 5

4 4 4

13 14 0

8 10 0

13 13 13

222 2mm mmm

D2 D2 D2 C2

3, 1, 1, 1 3, 1, 1, 1

3 3 3

3 3 3

6 7 0

3 5 0

9 9 9

3 3 32 3m 3m

C3 C3 C2 D3 D3 D3 C2

3, 0, 0

3 3 2 2 2

2 2 2 2 2

9 0 4 5 0

6 0 2 4 0

9 9 6 6 6

6 6 6=m 622 6mm 62m 6=mmm

C6 C6 C6 C2 D6 D6 D6 D6 C2

3, 2, 0, 1, 0, 2 3, 2, 0, 1, 0, 2

3 3 3 2 2 2 2

2 2 2 2 2 2 2

7 2 0 3 4 1 0

4 2 0 1 3 1 0

5 5 5 5 5 5 5

4 4 4=m 422 4mm 42m 4=mmm

C4 C4 C4 C2 D4 D4 D4 D4 C2

3, 1, 1, 1 3, 1, 1, 1

3 3 3 2 2 2 2

2 2 2 2 2 2 2

7 6 0 3 4 3 0

4 4 0 1 3 2 0

7 7 7 6 6 6 6

23 m3 432 43m m3m

T T C2 O O O C2

3, 0, 0, 1

1 1 1 1 1

1 1 1 1 1

2 0 1 1 0

1 0 0 1 0

3 3 3 3 3

3, 0, 1 3, 0, 1

3, 2, 0, 1, 1, 1 3, 2, 0, 1, 1, 1 3, 2, 0, 1, 1, 1

3, 1, 1, 1, 1 3, 1, 1, 1, 1 3, 1, 1, 1, 1

3, 0, 1, 1, 1 3, 0, 1, 1, 1

62

2

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS Table 1.2.6.10. Irreducible projective representations of the 32 crystallographic point groups (a) D2 A2 ¼ B2 ¼ E; ðABÞ2 ¼ E Elements

E

A

B

AB

05

2

0

0

0

(b) D4 4

2

2

A ¼ E; B ¼ ðABÞ ¼ E Elements

E

A2

06 07

2 2

0 0

A3 pﬃﬃﬃ i p 2 ﬃﬃﬃ i 2

A pﬃﬃﬃ ipﬃﬃ2ﬃ i 2

B

A2B

AB

A3B

0 0

0 0

0 0

0 0

(c) D6 6

2

2

A ¼ B ¼ E; ðABÞ ¼ E Elements

E

07 08 09

2 2 2

A2

A4

2 1 1

2 1 1

B

A2B

A4B

A3

A

A5

0 0 0

0 0 0

0 0 0

0 0 0

0pﬃﬃﬃ ip3ﬃﬃﬃ i 3

0pﬃﬃﬃ ip3ﬃﬃﬃ i 3

AB

A3B

A5B

0 0 0

0 0 0

0 0 0

(d) T [! ¼ expð2i=3Þ]. 3

3

2

A ¼ E; B ¼ ðABÞ ¼ E Elements

E

A

05 06 07

2 2 2

1 !5 !

Elements

ABA

05 06 07

A2 B

1 !5 !

1 !5 !

A2

BAB

BA

AB

1 !2 !4

1 !2 !4

1 !2 !4

BA2

B

ABA2

A2 BA

0 0 0

0 0 0

0 0 0

1 !5 !

1 !5 !

(e) O 4

2

3

A ¼ E; B ¼ ðABÞ ¼ E Elements

E

B

06 07 08

2 2 4

1 1 1

Elements

BA2 B

AB2 A

1 1 1

1 1 1

ABA3

A2 B2

06 07 08

1 1 1

1 1 1

1 1 1

Elements

A pﬃﬃﬃ ipﬃﬃ2ﬃ i 2 0

A3 pﬃﬃﬃ ipﬃﬃ2ﬃ i 2 0

A3 B pﬃﬃﬃ ipﬃﬃ2ﬃ i 2 0

06 07 08

A2 B

BA2

B2

1 1 1

1 1 1

A2

BA2 B2

B2 A2 B

0 0 0

0 0 0

0 0 0

BA3 pﬃﬃﬃ ip2ﬃﬃﬃ i 2 0

B2 A pﬃﬃﬃ ip2ﬃﬃﬃ i 2 0

AB2 pﬃﬃﬃ ip2ﬃﬃﬃ i 2 0

Elements

A2 B2 A

BA

AB

AB2 A2

AB2 A2 B

B2 AB2

06 07 08

0 0 0

0 0 0

0 0 0

0 0 0

0 0 0

0 0 0

(f) C4 C2 4

2

A ¼ B ¼ E; AB ¼ BA Elements

E

A

09 010

2 2

0 0

A2 2 2

A3

B

AB

A2B

A3B

0 0

0 0

0 0

0 0

0 0

(g) C6 C2 6

2

A ¼ B ¼ E; AB ¼ BA Elements

E

A

A2

A3

A4

A5

B

AB

A2B

A3B

A4B

A5B

013 014 015

2 2 2

0 0 0

2 2!2 2!4

0 0 0

2 2!4 2!4

0 0 0

0 0 0

0 0 0

0 0 0

0 0 0

0 0 0

0 0 0

63

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.2.6.10 (cont.) (h) D2 C2 2

2

2

2

A ¼ E; B ¼ C ¼ ðABÞ ¼ E; AC ¼ CA; BC ¼ CB Elements

E

A

B

AB

09 010

2 2

0 0

0 0

0 0

C 2 2

AC

BC

ABC

0 0

0 0

0 0

A2 ¼ E; B2 ¼ C2 ¼ ðABÞ2 ¼ E; AC ¼ CA; BC ¼ CB Elements

E

A

B

011 012

2 2

0 0

2 2

AB

C

AC

BC

ABC

0 0

0 0

0 0

0 0

0 0

A2 ¼ E; B2 ¼ C2 ¼ ðABÞ2 ¼ E; AC ¼ CA; BC ¼ CB Elements

E

A

B

AB

C

AC

BC

ABC

013 014

2 2

2i 2i

0 0

0 0

0 0

0 0

0 0

0 0

BC

ABC

A2 ¼ E; B2 ¼ C2 ¼ ðABÞ2 ¼ E; AC ¼ CA; BC ¼ CB Elements

E

A

B

AB

C

AC

015 016

2 2

0 0

0 0

0 0

0 0

0 0

2 2

0 0

A2 ¼ E; B2 ¼ C2 ¼ ðABÞ2 ¼ E; AC ¼ CA; BC ¼ CB Elements

E

A

B

AB

C

017 018

2 2

0 0

0 0

0 0

0 0

AC 2i 2i

BC

ABC

0 0

0 0

A2 ¼ E; B2 ¼ C2 ¼ ðABÞ2 ¼ E; AC ¼ CA; BC ¼ CB Elements

E

A

B

019 020

2 2

0 0

0 0

AB 2i 2i

C

AC

BC

ABC

0 0

0 0

0 0

0 0 ABC

A2 ¼ E; B2 ¼ C2 ¼ ðABÞ2 ¼ E; AC ¼ CA; BC ¼ CB Elements

E

A

B

AB

C

AC

BC

021 022

2 2

0 0

0 0

0 0

0 0

0 0

0 0

cyclotomics. Use of arbitrary real numbers would imply a ﬁnite precision. Detailed instructions for the use of the program, together with a guided tour (QuickStart), can be found in the manual for the program.

2i 2i

by generating matrices and is the one under which the (pseudo)tensor is invariant. The second symmetry is the index permutation symmetry. For tensors and pseudotensors up to rank four, all possible symmetries are tabulated after clicking ‘permutation symmetry’. The indices are numbered from 0 to r 1, where r is the rank. The symbol for a tensor symmetric in the indices 2 and 3 is (2 3), and it is [2 3] if the tensor gets a minus sign under permutation. Arbitrary combinations of symmetric and antisymmetric series can be made. For example, (0 1) 2 [3 4] is a rank-ﬁve tensor which is symmetric in the ﬁrst two indices and antisymmetric in the last two indices. The symbol (0 1 2) characterizes a rank-three tensor that is fully symmetric in all indices. For (pseudo)tensors of rank ﬁve and higher, the user needs to specify the permutation symmetry using parentheses in this way. Symmetrization of other pairs is similar. For example, if the rank-three tensor T is symmetric in the ﬁrst and last indices, the symbol for its permutation character is (0 2) 1. Then Txyz ¼ Tzyx . Different settings of the point group may be speciﬁed. The standard setting of a point group as given in International Tables for Crystallography Volume A may be different from the one to be speciﬁed. In this case, the user may perform a basis transformation which transforms the standard setting to the desired setting. This is done via the button ‘basis transformation’. The standard setting is chosen with ‘no transformation’. The transformation from a hexagonal to an orthogonal (Cartesian) basis is performed by selecting ‘hC transformation’. Finally, the tensor or pseudotensor with the speciﬁed point group and permutation symmetry is calculated and displayed in a (numbered) window. The command for this is given by clicking on the button ‘tensor’ or ‘pseudotensor’, respectively. In the window appear the input data, such as the point group, the

1.2.7.2. Tensors The tensor module of Tenar determines the number of independent elements and the relations between the elements of tensors and pseudotensors invariant under a chosen point group and with speciﬁed permutation symmetry of the indices. Although the list of point groups provided in a database is limited to dimensions two and three, the program runs for arbitrary dimensions. Similarly, the choice of index permutation symmetry is limited to rank smaller than or equal to four. This is also not a restriction of the program, which works for arbitrary rank. For higher dimensions and higher ranks, the user needs to provide additional information. The limiting factors are in fact the speed, which becomes low for higher dimensions and/or higher rank, and the available memory, which must be sufﬁcient to store the tensor elements. When the program is started and the tensor part is chosen via a button, a selection box opens. The user can specify dimension and rank in open ﬁelds. A ﬁeld without a coloured border has a formally correct content, but the user should check whether the pregiven numbers correspond to his wishes. In open ﬁelds with a coloured border, additional information must be given. Clicking on the button ‘point group’ results in the opening of a new selection window. A speciﬁc two- or three-dimensional point group may be chosen via geometric crystal classes. This point group may be viewed if wished. The chosen point group is given

64

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS Table 1.2.6.11. Special points in the Brillouin zones in three dimensions (a) Triclinic k a b c d e f g h

000 00 12 0 12 0 1 2 00 11 220 1 1 202 0 12 12 111 222

Kk 1 1 1 1 1 1 1 1

Kk

k Kovalev k8 k7 k6 k5 k4 k3 k2 k1

u v w x y z

0 1 2 0 12 0 12

k a b c d e f g h i j k l m n

000 00 12 1 2 00 0 12 0 0 12 12 1 1 202 11 220 111 222

00 0 12 1 2 0 11 22 0 12

Kk

Kovalev

2=m 2=m 2=m 2=m 2=m 2=m 2=m 2=m 2 2 2 2 m m

k7 k11 k12 k13 k9 k8 k14 k10 k3 k5 k4 k6 k1 k2

k1 k2 k3 k4 k5 k6

a b c d e f g h i j k l m n o p q

000 010 01 12 00 12 11 220 111 222

00 0 12 00 0 12 00 01 11 22 0 0 0 12

Kk

Kovalev

mmm mmm mmm mmm 2=m 2=m 2mm 2mm m2m m2m mm2 mm2 112 m11 1m1 11m 11m

k14 k15 k17 k16 k12 k13 k8 k9 k10 k11 k6 k7 k5 k1 k2 k3 k4

Kk

a b c d e f g h i

000 010 1 2 00 1 2 10 0 12 12 111 222

2=m 2=m 2=m 2=m 1 1

00 1 2 0 0

2 2 m

(d) Orthorhombic P k a b c d e f g h i j k l m n o p q r s t

000 1 2 00 00 12 1 1 202 0 12 0 11 220 0 12 12 111 222

00 0 12 12 0 12 12 00 0 12 1 2 0 1 1 22 00 0 12 1 2 0 11 22

Kk

Kovalev

mmm mmm mmm mmm mmm mmm mmm mmm 2mm 2mm 2mm 2mm m2m m2m m2m m2m mm2 mm2 mm2 mm2

k19 k20 k22 k24 k21 k25 k23 k26 k7 k12 k10 k11 k8 k15 k13 k14 k9 k18 k16 k17

l m n

0 0 0

m11 1m1 11m

k a b c d e f g h i j k l m n o p q r s t

(f) Orthorhombic I

Kovalev k6 k8 k7 k9 k4 k5 k2 k3 k1

Kk 1 1 1 1

Kovalev k10 k11 k12 k13 k1 k2 k3

(h) Tetragonal P

(c) Monoclinic A k

k

111 222 12 12 12 1 11 2 22 11 1 22 2

k

(e) Orthorhombic C k

(b) Monoclinic P

m m11 1m1 1m1 11m 11m

Kovalev

k a b c d e f g h i j k l m n o

000 001 0 12 12 1 12 12 1 1 202 1 1 212 11 220 11 221 111 222

00 00 00 11 22 1 1 22 12 12 0 0 0

Kk

Kovalev

mmm mmm 2=m11 2=m11 12=m1 12=m1 112=m 112=m 222 2mm m2m mm2 112 121 211 m11 1m1 11m

k17 k18 k13 k10 k14 k11 k15 k12 k16 k7 k8 k9 k6 k5 k4 k1 k2 k3

000 00 12 11 220 111 222

0 12 12 0 12 0 00 11 22 0 12 0 12 00 0 12 12 0 12 12 0 12 0 12

Kk

Kovalev

4=mmm 4=mmm 4=mmm 4=mmm mmm mmm 4mm 4mm mm2 2mm 2mm m2m m2m 2mm 2mm 11m 11m m m11 1m1

k17 k19 k18 k20 k16 k15 k13 k14 k12 k10 k11 k8 k9 k6 k7 k1 k2 k5 k3 k4

(i) Tetragonal I k a b c d e f g h i j k l m

000 001 11 220 111 222

00 1 1 202 11 22

0 00 ð1 Þ0 1 1 22 0 ð1 Þ 0

n

Kk

Kovalev

4=mmm 4=mmm mmm 4m2 4mm 12=m1 2mm 2mm 2mm 2mm 121 11m m m 1m1

k14 k15 k13 k12 k10 k11 k9 k7 k7 k8 k5 k2 k3 k4 k1

(g) Orthorhombic F k a b c d e f g h i j

000 100 010 001 00 10 00 10 00 01

Kk

Kovalev

mmm mmm mmm mmm 2mm 2mm m2m m2m mm2 mm2

k14 k15 k16 k17 k4 k5 k6 k7 k8 k9

65

(j) Trigonal R (rhombohedral axes)

111 222

Kk 3m 3m

00 12 11 220 ðÞ0 ðÞ 12

3m 2=m 2=m 2 2 m

k a b c d e f g h

000

Kovalev k7 k8 k6 k4 k5 k2 k2 k1

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.2.6.12. Magnetic point groups

Table 1.2.6.11 (cont.) (k) Hexagonal P k a b c d e f g h i j k l m n o p q

000 00 12 11 330 111 332

00

Kk

Kovalev

6=mmm 6=mmm 6m2 6m2

k16 k17 k13 k15 k11 k12 k14 k10 k9 k5 k7 k6 k8 k3 k4 k1 k2

6mm mmm mmm 3m 2mm 2mm 2mm 2mm 2mm m m m m

1 2 00 1 1 202 11 33 1 2 0

00 0 12 0 12 0 0 12

(l) Cubic P Kk m3m m3m

k a b c d e f g h i j k l m

000 111 222 11 220 00 12

4=mmm 4=mmm 4mm 4mm 3m mm2 2mm 2mm 11m 11m m

00 11 22

1 2 0

0 12 0 12

Kovalev k12 k13 k11 k10 k8 k7 k9 k6 k4 k5 k1 k2 k3

a b c d e f g h i j k

Kk m3m

000 001 111 222 10 12

4=mmm 3m 4m2

00 01 0 ð1 Þ 12

4mm 3m 2mm 2mm 2 11m m

Kovalev k11 k10 k9 k8 k6 k5 k7 k4 k3 k1 k2

k 000 001 111 222 11 220

00 12 12 0 ð1 Þ0 ð1 Þ

Kk

Kovalev

m3m m3m 43m

k11 k10 k10 k9 k8 k7 k6 k4 k9 k1 k2 k3

mmm 4mm 3m 2mm 2mm 2mm 11m m m

Type III

10 0 11

1 0

2 m 2=m

210 m10 210 =m

20 m0 20 =m, 2=m0 , 20 =m0 ,

222 2mm mmm

22210 2mm10 mmm10

20 20 20 mm0 , 2m0 m0 m0 mm, m0 m0 m, m0 m0 m0

4 4 4=m 422 4mm 42m 4=mmm

410 0 41 410 =m 42210 4mm10 0 42m1 4=mmm10

40 4 0 40 =m, 4=m0 , 40 =m0 40 220 , 420 20 40 mm0 , 4m0 m0 0 m0 4 0 20 m, 4 0 2m0 , 42 4=m0 mm, 40 =mm0 m, 40 =m0 m0 m, 4=mm0 m0 , 4=m0 m0 m0

3 3 32 3m 3m

310 0 31 3210 3m10 0 3m1

3 0 320 3m0 0 3 0 m, 3 0 m0 , 3m

6 6 6=m 622 6mm 62m 6=mmm

610 0 61 610 =m 62210 6mm10 0 62m1 6=mmm10

60 6 0 60 =m, 6=m0 , 60 =m0 60 220 , 620 20 60 mm0 , 6m0 m0 0 m0 6 0 20 m, 6 0 2m0 , 62 6=m0 mm, 60 =mm0 m, 60 =m0 m0 m, 6=mm0 m0 , 6=m0 m0 m0

23 m3 432 43m m3m

2310 0 m31 43210 0 43m1 0 m3m1

m0 3 40 320 4 0 3m0 m3m 0 , m0 3m 0 m0 3m,

1.2.7.3. Characters Calculations with characters of representations of point groups can be done in the character module of the program. It is selected in the main window by clicking ‘character’. A selection window opens in which a point group may be selected just as in the tensor module. The point groups are organized according to dimension and geometric crystal class. Selection of a point group leads to the display of the character table if one asks for it by selecting ‘view character table’. The character table consists of a square array of (complex) numbers. The number of rows is the number of nonequivalent irreducible representations and is equal to the number of columns, which is the number of conjugacy classes of the group. For crystallographic groups, the complex numbers that form the entries of the character table are cyclotomic numbers. These are linear combinations with fractions as coefﬁcients of complex numbers of the form expð2in=mÞ: For example, the square root pﬃﬃﬃ of 1 (i) can be written as expð2i1=4Þ: A real number like 2 can be written as pﬃﬃﬃ pﬃﬃﬃ 2 ¼ 12 2ð1 þ i þ 1 iÞ ¼ expð2i 18Þ þ expð2i 78Þ:

(n) Cubic I

a b c d e f g h i j k

Type II

1 1

dimension, the rank, the permutation symmetry and the setting basis transformation, and the calculated data: the number of independent elements (f) and the relations of these elements. They are either zero or expressed in terms of the free parameters a0 ; . . . ; af 1 . The tensor elements are given by sequences x; y; z; . . .. The four elements of a general rank-two tensor in two dimensions are xx, xy, yx, yy, corresponding to T11, T12 , T21 and T22 , respectively.

(m) Cubic F k

Type I

Another example is pﬃﬃﬃ 5 ¼ 1 þ 2 expð2i 15Þ þ 2 expð2i 45Þ:

66

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS However, many entries for the three-dimensional point groups are simply integers. The program provides the following information as rows above the characters of the irreducible representation: (1) Representative elements of the conjugacy classes expressed in terms of the generators a; b; . . . : (2) The number of elements of each class. (3) The order of the elements of the classes: the lowest positive power of an element that equals the identity. Below the character table, the following information is displayed: (1) In the mth row after the square character table, the class to which the ðm þ 1Þth powers of the elements from this column belong is given. If a conjugacy class has elements of order p, then only the p 1 ﬁrst entries are given, because in the column there exists p periodicity. (2) The determinant of the three-dimensional matrix for the element of the point group (or the elements of the conjugacy class). This is the character of an irreducible representation. (3) Finally, the character of the vector representation is given. As an example, the generalized character table for the threedimensional point group 4mm is given in Table 1.2.7.1. The data connected with a character table can be seen by choosing ‘view character table’. The characters of the irreducible representations, the determinant representation and the vector representation are shown in the main window after selection of ‘accept character table’. From the character of these representations, characters of other representations may be calculated. The results are added as rows to the table, which is shown after each calculation. Calculations using rows from the table may have one or more arguments. Operations with one argument will produce, for example, the decomposition into irreducible components, the character of the pth power, the symmetrized or antisymmetrized square, or the character of the corresponding physical (real) representation. Operations with two or more arguments yield products and sums of characters. The arguments of a unitary, binary or multiple operation are selected by clicking on the button in front of the corresponding characters. If the result is a new character (e.g. the product of two characters), it is added as a row to the list of characters. If the result is not a character (e.g. the decomposition into irreducible components), the result is given on the worksheet. Suppose one wants to determine the number of elastic constants for a material with cubic 432 symmetry. After selecting the character table for the group 432, one clicks on the button in front of ‘vector representation’ in the character table. This yields the character of the three-dimensional vector representation of the group. The character of the symmetrized square is obtained by selecting ‘symmetrized square’. This gives the character of a six-dimensional representation. Determining the number of times the trivial representation occurs by selecting ‘decompose’ gives the number of free parameters in the metric tensor, i.e. 1. Clicking on ‘symmetrized square’ for the character of the six-dimensional representation gives the character of a

21-dimensional representation. Decomposition yields the multiplicity 3 for the trivial representation, which means that there are three independent tensor elements for a tensor of symmetry type ðð0 1Þð2 3ÞÞ, which in turn means that there are three elastic constants for the group 432 (see Table 1.2.6.9). For the explicit determination of the independent tensor elements, the tensor module of the program should be used. Of course, many kinds of calculations unrelated to tensors can be carried out using the character module. Examples include the calculation of selection rules in spectroscopy or the splitting of energy levels under a symmetry-breaking perturbation. 1.2.7.4. Algorithms 1.2.7.4.1. Construction of a basis As a basis for a tensor space without permutation symmetry, one may choose one consisting of non-commutative monomials. It has dr elements, where d is the dimension and r is the rank. In two dimensions, these are x; y for r ¼ 1, xx, xy, yx, yy for r ¼ 2 and xxx, xxy, xyx, xyy, yxx, yxy, yyx, yyy for r ¼ 3. Note that xy 6¼ yx. If there is permutation symmetry among the indices i1 ; . . . ; ip, only polynomials xi1 xi2 . . . xr occur in the basis for which i1 i2 . . . ip . Then xi1 xi2 ¼ xi2 xi1 . If there is antisymmetry among these indices, one has the condition i1 < i2 < . . . < ip and xi1 xi2 ¼ xi2 xi1 . Therefore, in two dimensions, the basis for tensors of type (1 3)2 is xxx, xxy, xyx, xyy, yxy, yyy and for those of type [1 3]2 it is xxy, xyy. These bases can be obtained from the general basis by elimination. 1.2.7.4.2. Action of the generators of the point group G on the basis The transformation of the monomial xi xj . . . under the matrix g 2 G is given by the polynomial d d P P gim xm gjn xn . . . ; m¼1

n¼1

which is in principle non-commutative. This polynomial can be written as a sum of the monomials in the basis taking into account the eventual (anti)symmetry of xy and yx. In this way, basis element (a monomial) ei is transformed to gei ¼

d P

MðgÞji ej :

j¼1

To each generator of G corresponds such an action matrix M. The action matrix changes if one considers pseudotensors. In the case of pseudotensors, the previous equation changes to gei ¼ DetðgÞ

d P

MðgÞji ej :

j¼1

The function Det(g) is just a one-dimensional representation of the group G. The determinant is either þ1 or 1.

Table 1.2.7.1. Data connected with the character table for point group 4mm e 1 1

a 2 4

a2 1 2

b 2 2

ab 2 2

1 1 1 1 2

1 1 1 1 0

1 1 1 1 2

1 1 1 1 0

1 1 1 1 0

1

3 2 1

1

1

1

1 1

1 1

1 3

1.2.7.4.3. Diagonalization of the action matrix and determination of the invariant tensor An invariant element of the tensor space under the group G is a vector v that is left invariant under each generator: 0 1 M1 E B M2 E C C B B Cv ¼ v ¼ 0: .. @ A . Ms E

1 1

1 1

If the number of generators is one, ¼ M E. This equation is solved by diagonalization:

67

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1 PQQ v ¼ DQ1 v ¼ 0; n ¼ 2 : ðd2 dÞ 2 1 n ¼ 3 : ðd3 3d2 þ 2dÞ 6 where Dij ¼ di ij. The dimension of the solution space is the 1 number of elements di that are equal to zero. The corresponding n ¼ 4 : ðd4 6d3 þ 11d2 6dÞ 24 rows of Q form a basis for the solution space. (See example 1 5 further on.) ðd 10d4 þ 35d3 50d2 þ 24dÞ n¼5: 120 1 6 1.2.7.4.4. Determination of the vector representation ðd 15d5 þ 85d4 225d3 þ 274d2 120dÞ: n¼6: 720 For a point group G, its isomorphism class and its character table are known. For each conjugacy class, a representative element is given as word A1 A2 . . . where the Ai ’s correspond to The general expression for arbitrary rank can be determined as generators. Replacing the letters by the generating matrices, one follows. (See also Section 1.2.2.7) obtains as product a matrix for which the trace is the character of (1) If n is the rank, the ﬁrst step is to determine all possible the vector representation in the conjugacy class. The characters decompositions of all conjugacy classes being known, the representation can be decomposed into irreducible components by means of n P n ¼ fi i¼1 P m ¼ ð1=jGjÞ ni ðiÞðiÞ; 1

i

with non-negative integers fi satisfying fi fi1 . (2) For each such decomposition m ¼ 1; . . . ntot there is a term

where labels the irreducible representations (the row number in the character table), m the number of times the representation occurs, jGj the order of the group G, ni the number of elements in the ith conjugacy class (given as the second row in the character table), ðiÞ the cyclotomic in the ith row and th column of the character table, and ðiÞ the calculated character in the ith conjugacy class.

p Y Ni Pm ¼ ðfi 1Þ!; fi i¼1 where N1 ¼ n, Ni ¼ Ni1 fi1 ði > 1Þ and p is the number of nonzero integers fi. (3) If there are equal values of fi in the mth decomposition, Pm should be divided by t! for each t-tuple of equal values (fkþ1 ¼ . . . ¼ fkþt ). (4) The sign of the term Pm is þ1 for a symmetrized power and

1.2.7.4.5. Determination of tensor products and their decomposition Given a character (for an irreducible representation from the character table, or for the vector representation, for example), the character of the standard rank n tensor is the nth power of the character and can be decomposed with the multiplicity formula for m given above. Fully symmetrized or antisymmetrized tensor products have characters given by

p Q

ð1Þðfi 1Þ

i¼1

for an antisymmetrized power. (5) The expression for the character of the (anti)symmetrized power then is

1 ðRÞ2 ðR2 Þ 2! 1 n ¼ 3 : ðRÞ ¼ ðRÞ3 3ðR2 ÞðRÞ þ 2ðR3 Þ 3! 1 n ¼ 4 : ðRÞ ¼ ðRÞ4 6ðR2 ÞðRÞ2 þ 3ðR2 Þ2 4! þ 8ðR3 ÞðRÞ 6ðR4 Þ 1 n ¼ 5 : ðRÞ ¼ ðRÞ5 10ðR2 ÞðRÞ3 þ 15ðR2 Þ2 ðRÞ 5! þ 20ðR3 ÞðRÞ2 20ðR3 ÞðR2 Þ 30ðR4 ÞðRÞ þ 24ðR5 Þ 1 ðRÞ6 15ðR2 ÞðRÞ4 þ 45ðR2 Þ2 ðRÞ2 n ¼ 6 : ðRÞ ¼ 6! þ 40ðR3 Þ2 15ðR2 Þ3 þ 40ðR3 ÞðRÞ3

n ¼ 2 : ðRÞ ¼

3

2

4

120ðR ÞðR ÞðRÞ 90ðR ÞðRÞ

ðRÞ ¼ ð1=M!Þ

ntot P

signm Pm

p Q

ðRfi Þ:

i¼1

m¼1

1.2.7.4.6. Invariant tensors Once one has the character of the properly symmetrized tensor, the number of invariants is just m1 , the number of times the trivial representation occurs in the decomposition. Example (1). Dimension 3, rank 3, symmetry type (123), group 3. Basis: xxx, xxy, xxz, xyy, xyz, xzz, yyy, yyz, yzz, zzz. Under 0

0 @0 1

2

þ 90ðR4 ÞðR2 Þ þ 144ðR5 ÞðRÞ 120ðR6 Þ :

1 0 0

1 0 1A 0

the basis elements go to yyy; yyz; yyx; yzz; yzx; yxx; zzz; zzx; zxx; xxx, respectively, and these are equivalent to yyy; yyz; xyy; yzz; xyz; xxy; zzz; xzz; xxz; xxx, respectively. This gives the tendimensional matrix

From this follows immediately the dimension of the subspaces of symmetric and antisymmetric tensors:

68

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS 1 0 0 0 0 0 0 0 0 0 1 the invariant tensor corresponds to the second column of Q, B0 0 0 0 0 1 0 0 0 0C which as a polynomial reads xx þ xy yy. This can be written C B B0 0 0 0 0 0 0 0 1 0C with the tensor Tij as C B B0 0 1 0 0 0 0 0 0 0C P C B 1 12 B0 0 0 0 1 0 0 0 0 0C : xx þ xy yy ¼ Tij xi xj ; Tij ¼ C 12 1 M¼B i;j B 0 0 0 0 0 0 0 1 0 0 C: C B B1 0 0 0 0 0 0 0 0 0C C B This tensor T is invariant under the group. B0 1 0 0 0 0 0 0 0 0C C B @0 0 0 1 0 0 0 0 0 0A Example (3). Dimension 3, rank 2, tensor type (12). Group 0 0 0 0 0 0 1 0 0 0 generated by matrix([[0 1 0][1 0 0][0 0 1]]). The basis xx, xy, xz, yy, yz, zz goes under the generator to yy, xy, yz, xx, xz, zz. Then PðM EÞQ ¼ D, with D diagonal. There are four diagonal The solution of ðM EÞv ¼ 0 is elements of D which are zero, and the invariant tensors corre1 ðxx þ yyÞ þ 2 zz: spond to the corresponding four columns of the matrix Q. The invariant polynomials are The matrix D has two zeros on the diagonal. xxx þ yyy þ zzz; xxy þ xzz þ yyz; xxz þ yzz þ xyy; xyz: Example (4). Dimension 3, rank 3, type (123). Same group as in Example (3). Basis xxx, xxy, xxz, xyy, xyz, xzz, yyy, yyz, yzz, zzz. Example (2). Dimension 2, rank 2, symmetry type (12). Group The solution generated by 1 ðxxz þ yyzÞ þ 2 zzz 0 1 : 1 1 corresponds to a tensor with relations T113 ¼ T223, T111 ¼ T112 ¼ T122 ¼ T123 ¼ T133 ¼ T222 ¼ T233 ¼ 0. Basis xx, xy, yy goes to yy, xy þ yy, xx 2xy þ yy. This gives 0 1 0 0 1 Example (5). Dimension 3, rank 4, type ((12)(34)). Not only M ¼ @ 0 1 2 A: i1 i2 and i3 i4 , but also (i1 i2 Þ, should come lexicographically before (i3 i4 ). Basis xxxx; xxxy; xxxz; xxyy; xxyz; xxzz; xyxy; 1 1 1 xyxz; xyyy; xyyz; xyzz; xzxz; xzyy; xzyz; xzzz; yyyy; yyyz; yyzz; yzyz; yzzz; zzzz. Under the same group as in example (3), there Because are seven invariants. Invariant polynomial: 0 1 0 1 0 1 1 0 0 1 1 1 1 0 0 1 ðxxxx þ yyyyÞ þ 2 ðxxxy xyyyÞ þ 3 xxyy þ 4 xyxy @ 2 1 2 AðM EÞ@ 0 1 0 A ¼ @ 0 0 0 A; þ 5 zzzz þ 6 ðxxzz þ yyzzÞ þ 7 ðxzxz þ yzyzÞ: 1 0 1 0 1 1 0 0 2 0

Table 1.2.7.2. Calculation with characters Generator 0 0 1 @0 0 1 0

1

0 1A 0

Example (1) 0 1 1 1

Example (2) 0 0 1 @1 0 0 0

1

0 0A 1

Example (3) As above Example (4)

As above Example (5)

Composite character

Characters

R

E

A

AA

ðRÞ ðRÞ3 ðR2 Þ ðR2 ÞðRÞ ðR3 Þ 3 1 2 3 6 ððRÞ þ 3ðR ÞðRÞ þ 2ðR ÞÞ

3 27 3 9 3 10

0 0 0 0 3 1

0 0 0 0 3 1

R

E

A

AA

ðRÞ ðRÞ2 ðR2 Þ 2 1 2 2 ððRÞ þ ðR Þ)

2 4 2 3

1 1 1 0

1 1 1 0

R

E

A

AA

AAA

ðRÞ ðRÞ2 ðR2 Þ 2 1 2 2 ððRÞ þ ðR Þ)

3 9 3 6

1 1 1 0

1 1 3 2

1 1 1 0

2D1 þ D2 þ 2D3 þ D4

ðRÞ ðRÞ3 ðR2 Þ ðR2 ÞðRÞ ðR3 Þ 3 1 2 3 6 ððRÞ þ 3ðR ÞðRÞ þ 2ðR ÞÞ

3 27 3 9 3 10

1 1 1 1 1 0

1 1 3 3 1 2

1 1 1 1 1 0

2D1 þ 3D2 þ 2D3 þ 3D4

ðRÞ

3 6 36 6 21

1 0 0 2 1

1 2 4 6 5

1 0 0 2 1

7D1 þ 4D2 þ 6D3 þ 4D4

3 1

1 1

1 1

1 1

D1 þ D2 þ D4 D1

2 1 2 ððRÞ s ðRÞ2 s ðR2 Þ

þ ðR2 Þ)=s ðRÞ

((12)(34)) As above, example (6) As above, example (7)

2 1 2 ððRÞ 3 1 ððRÞ 6

ðR2 Þ) 3ðR2 ÞðRÞ þ 2ðR3 ÞÞ

69

Decomposition

4D1 þ 3D2 þ 3D3

D1 þ D2 þ D3

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES This corresponds to the tensor relations Txxxx ¼ Tyyyy Txxyz ¼ 0

Txxxy ¼ Txyyy Txxzz ¼ Tyyzz

Txxxz ¼ 0 Txyxz ¼ 0

Txyyz ¼ 0

Txyzz ¼ 0

Txzxz ¼ Tyzyz

Txzyy ¼ 0 Tyyyz ¼ 0 0 1 B B 3 B B 6 !B B0 B B @0

Txzyz ¼ 0 Tyzzz ¼ 0

Txzzz ¼ 0

2

3 1

6 6

0 0

0 0

6 0

5 0

0 7

0 0

0

0

0

7

2

0

0

0

xxx xxy xxz xyy xyz xzz yyy yyz yzz zzz

1 2 2 C C C 0 C C: 0 C C C 0 A 4

Example (6). Dimension 3, rank 2, type [12]. The same group as in example (3). Basis xy; xz; yz ! yx; yz; xz, which are equivalent to xy; yz; xz. The transformation in the tensor space is 1 B M ¼ @0

1 0 0 0 C B 1A ! @0

0 0

0 1 0 0 1 1 B C v ¼ @ 0 A xy:

0 1 1

0

1 0 C 1 Av ¼ 0 : 1

0

T¼

0 1

0 0 1 0 0 0 0 0 0 0 0 0 0 0 0 0 0 1 0 0

0 0 0 0 0 1 0 0 0 0 0 0 0 0 0 0 0 0 1 0

1 0 0C C 0C C 0C C 0C C 0C C 0C C 0C C 0C C 1C C: 0C C 0C C 0C C 0C C 0C C 0C C 0C C 0C C 0A 1

After diagonalization, one ﬁnds two nonzero elements on the diagonal:

There is just one invariant antisymmetric polynomial xy ¼ yx corresponding to the tensor

B xxx xxy xxz xyy xyz xzz yyy yyz yzz zzz

Therefore, the action matrix becomes 0 0 0 0 0 0 0 1 B 0 0 0 1 0 0 0 B B 0 0 0 0 0 0 0 B B 0 1 0 0 0 0 0 B B 0 0 0 0 1 0 0 B B 0 0 0 0 0 0 0 B B 1 0 0 0 0 0 0 B B 0 0 1 0 0 0 0 B B 0 0 0 0 0 1 0 B B 0 0 0 0 0 0 0 B B 1 0 0 0 0 0 0 B B 0 1 0 0 0 0 0 B B 0 0 1 0 0 0 0 B B 0 0 0 1 0 0 0 B B 0 0 0 0 1 0 0 B B 0 0 0 0 0 1 0 B B 0 0 0 0 0 0 1 B B 0 0 0 0 0 0 0 B @ 0 0 0 0 0 0 0 0 0 0 0 0 0 0

The latter form is that of an elastic tensor with the usual convention 1 ¼ xx, 2 ¼ yy, 3 ¼ zz, 4 ¼ yz, 5 ¼ xz, 6 ¼ xy.

0

A yyy xyy yyz xxy xyz yzz xxx xxz xzz zzz

zzz ¼ a; xxz ¼ yyz ¼ b; xxx ¼ xxy ¼ xyy ¼ xyz ¼ xzz ¼ yyy ¼ yzz ¼ 0:

1 : 0

1.2.8. Glossary Example (7). Dimension 3, rank 3, type [123]. Basis xyz invariant under the group: xyz ! yxz xyz. The corresponding tensor is the fully antisymmetric rank 3 tensor: Tijk ¼ 1 if ijk is an even permutation of 123, ¼ 1 if ijk is an odd permutation, and ¼ 0 if two or three indices are equal (permutation tensor, see Section 1.1.3.7.2).

Ti1 ...in OðnÞ Z ei g K R Cm SOðnÞ Zþ Dn E I DðKÞ ðKÞ jKj

2 ai

Example (8). Calculation with characters. See Table 1.2.7.2. Example (9). The action matrix for a pseudotensor. Take the group 4=m with generators 0

0 @1 0

1 0 0

1 0 0 A; 1

0

1 @0 0

0 1 0

1 0 0 A: 1

Consider the rank 3 pseudotensor (123). The action matrix is determined from the action of the generators A and B on the basis:

70

tensor of rank n orthogonal group ring of integers basis vectors metric tensor point group orthogonal transformation cyclic group of order m special orthogonal group positive integers dihedral group of order n unit transformation, matrix or element inversion representation of K matrix representation of K order of K sum of spaces or operators tensor product element of basis of space or lattice

1.2. REPRESENTATIONS OF CRYSTALLOGRAPHIC GROUPS V S ðRÞ Ci m N d ni cijk T O I PðKÞ Wi ðA1 ; . . . ; Ap Þ Kd EðnÞ g ¼ fRjag TðnÞ aðRÞ k Gk Kk

! Det(R)

i j k

dual space basis transformation character value of at R conjugacy class irreducible character multiplicity order of K dimension of irreducible representation order of class Ci class multiplication constants tetrahedral group octahedral group icosahedral group projective representation word in generators Aj double group Euclidean group element of EðnÞ translation group in n dimensions lattice reciprocal lattice translation vector system vector in dual space group of k point group of Gk

factor system determinant of R Clebsch–Gordan coefﬁcients

‘ time-reversal operator

References Altmann, S. L. & Herzig, P. (1994). Point-Group Theory Tables. Oxford: Clarendon Press. Butler, P. H. (1981). Point Group Symmetry Applications. New York & London: Plenum Press. International Tables for Crystallography (2005). Vol. A. Space-Group Symmetry, edited by Th. Hahn. Heidelberg: Springer. Janssen, T. (1973). Crystallographic Groups. Amsterdam: NorthHolland. Kovalev, O. V. (1987). Representations of the Crystallographic Space Groups. New York: Gordon and Breach. Miller, S. C. & Love, W. F. (1967). Tables of Irreducible Representations of Space Groups and Co-representations of Magnetic Space Groups. Boulder, Colorado: Pruett Press. Stokes, H. T. & Hatch, D. M. (1988). Isotropy Subgroups of the 230 Crystallographic Space Groups. Singapore: World Scientiﬁc.

71

references

International Tables for Crystallography (2013). Vol. D, Chapter 1.3, pp. 72–99.

1.3. Elastic properties By A. Authier and A. Zarembowitch

The components of the tensor Mij are nonzero, unless, as mentioned earlier, the deformation reduces to a simple translation. Two cases in particular are of interest and will be discussed in turn: (i) The components Mij are constants. In this case, the deformation is homogeneous. (ii) The components Mij are variables but are small compared with unity. This is the practical case to which we shall limit ourselves in considering an inhomogeneous deformation.

1.3.1. Strain tensor 1.3.1.1. Introduction, the notion of strain ﬁeld Let us consider a medium that undergoes a deformation. This means that the various points of the medium are displaced with respect to one another. Geometrical transformations of the medium that reduce to a translation of the medium as a whole will therefore not be considered. We may then suppose that there is an invariant point, O, whose position one can always return to by a suitable translation. A point P, with position vector OP ¼ r, is displaced to the neighbouring point P0 by the deformation deﬁned by

1.3.1.2. Homogeneous deformation If the components Mij are constants, equations (1.3.1.3) can be integrated directly. They become, to a translation, ) ui ¼ Mij xj ð1:3:1:4Þ x0i ¼ Bij xj :

PP0 ¼ uðrÞ: The displacement vector uðrÞ constitutes a vector ﬁeld. It is not a uniform ﬁeld, unless the deformation reduces to a translation of the whole body, which is incompatible with the hypothesis that the medium undergoes a deformation. Let Q be a point that is near P before the deformation (Fig. 1.3.1.1). Then one can write dr ¼ PQ;

1.3.1.2.1. Fundamental property of the homogeneous deformation The fundamental property of the homogeneous deformation results from the fact that equations (1.3.1.4) are linear: a plane before the deformation remains a plane afterwards, a crystal lattice remains a lattice. Thermal expansion is a homogeneous deformation (see Chapter 1.4).

r þ dr ¼ OQ:

After the deformation, Q is displaced to Q0 deﬁned by QQ0 ¼ uðr þ drÞ: In a deformation, it is more interesting in general to analyse the local, or relative, deformation than the absolute displacement. The relative displacement is given by comparing the vectors P0 Q0 ¼ dr0 and PQ. Thus, one has

1.3.1.2.2. Spontaneous strain Some crystals present a twin microstructure that is seen to change when the crystals are gently squeezed. At rest, the domains can have one of two different possible orientations and the inﬂuence of an applied stress is to switch them from one orientation to the other. If one measures the shape of the crystal lattice (the strain of the lattice) as a function of the applied stress, one obtains an elastic hysteresis loop analogous to the magnetic or electric hysteresis loops observed in ferromagnetic or ferroelectric crystals. For this reason, these materials are called ferroelastic (see Chapters 3.1 to 3.3 and Salje, 1990). The strain associated with one of the two possible shapes of the crystal when no stress is applied is called the macroscopic spontaneous strain.

P0 Q0 ¼ P0 P þ PQ þ QQ0 : Let us set dr0 ¼ dr þ uðr þ drÞ uðrÞ

)

du ¼ uðr þ drÞ uðrÞ ¼ dr0 dr:

ð1:3:1:1Þ

Replacing uðr þ drÞ by its expansion up to the ﬁrst term gives 9 @u > > dui ¼ i dxj > = @xj ð1:3:1:2Þ > @u > dx0i ¼ dxi þ i dxj : > ; @xj

1.3.1.2.3. Cubic dilatation Let ei be the basis vectors before deformation. On account of the deformation, they are transformed into the three vectors

If we assume the Einstein convention (see Section 1.1.2.1), there is summation over j in (1.3.1.2) and (1.3.1.3). We shall further assume orthonormal coordinates throughout Chapter 1.3; variance is therefore not apparent and the positions of the indices have no meaning; the Einstein convention then only assumes repetition of a dummy index. The elements dxi and dx0i are the components of dr and dr0 , respectively. Let us put

e0i ¼ Bij ej :

Mij ¼ @ui [email protected] ; Bij ¼ Mij þ ij ; where ij represents the Kronecker symbol; the ij ’s are the components of matrix unity, I. The expressions (1.3.1.2) can also be written using matrices M and B: ) dui ¼ Mij dxj ð1:3:1:3Þ dx0i ¼ Bij dxj : Copyright © 2013 International Union of Crystallography

Fig. 1.3.1.1. Displacement vector, uðrÞ.

72

1.3. ELASTIC PROPERTIES The parallelepiped formed by these three vectors has a volume V0 given by

1.3.1.2.5. Quadric of elongations Let us project the displacement vector uðrÞ on the position vector OP (Fig. 1.3.1.2), and let ur be this projection. The elongation is the quantity deﬁned by ur u r Mij xi xj ¼ 2 ¼ ; r r r2

V 0 ¼ ðe01 ; e02 ; e03 Þ ¼ ðBÞðe1 ; e2 ; e3 Þ ¼ ðBÞV; where ðBÞ is the determinant associated with matrix B, V is the volume before deformation and ðe1 ; e2 ; e3 Þ ¼ ðe1 ^ e2 Þ e3

where x1, x2 , x3 are the components of r. The elongation is the relative variation of the length of the vector r in the deformation. Let A and S be the antisymmetric and symmetric parts of M, respectively:

represents a triple scalar product. The relative variation of the volume is V0 V ¼ ðBÞ 1: V

ð1:3:1:5Þ

A¼

It is what one calls the cubic dilatation. ðBÞ gives directly the volume of the parallelepiped that is formed from the three vectors obtained in the deformation when starting from vectors forming an orthonormal base.

M MT ; 2

S¼

M þ MT : 2

Only the symmetric part of M occurs in the expression of the elongation: ur Sij xi xj ¼ 2 : ð1:3:1:6Þ r r

1.3.1.2.4. Expression of any homogeneous deformation as the product of a pure rotation and a pure deformation (i) Pure rotation: It is isometric. The moduli of the vectors remain unchanged and one direction remains invariant, the axis of rotation. The matrix B is unitary:

The geometrical study of the elongation as a function of the direction of r is facilitated by introducing the quadric associated with M: Sij yi yj ¼ ";

ð1:3:1:7Þ

T

BB ¼ 1:

where " is a constant. This quadric is called the quadric of elongations, Q. S is a symmetric matrix with three real orthogonal eigenvectors and three real eigenvalues, 1 , 2 , 3 . If it is referred to these axes, equation (1.3.1.7) is reduced to

(ii) Pure deformation: This is a deformation in which three orthogonal directions remain invariant. It can be shown that B is a symmetric matrix:

1 ðy1 Þ2 2 ðy2 Þ2 3 ðy3 Þ2 ¼ ":

B ¼ BT :

One can discuss the form of the quadric according to the sign of the eigenvalues i : (i) 1 , 2 , 3 have the same sign, and the sign of ". The quadric is an ellipsoid (Fig. 1.3.1.3a). One chooses " ¼ þ1 or " ¼ 1, depending on the sign of the eigenvalues. (ii) 1 , 2 , 3 are of mixed signs: one of them is of opposite sign to the other two. One takes " ¼ 1. The corresponding quadric is a hyperboloid whose asymptote is the cone

The three invariant directions are those of the eigenvectors of the matrix; it is known in effect that the eigenvectors of a symmetric matrix are real. (iii) Arbitrary deformation: the matrix B, representing an arbitrary deformation, can always be put into the form of the product of a unitary matrix B1 , representing a pure rotation, and a symmetric matrix B2 , representing a pure deformation. Let us put

Sij yi yj ¼ 0:

B ¼ B1 B2

According to the sign of ", the hyperboloid will have one sheet outside the cone or two sheets inside the cone (Fig. 1.3.1.3b). If we wish to be able to consider any direction of the position vector r in space, it is necessary to take into account the two quadrics. In order to follow the variations of the elongation ur =r with the orientation of the position vector, one associates with r a vector y, which is parallel to it and is deﬁned by

and consider the transpose matrix of B: BT ¼ BT2 BT1 ¼ B2 ðB1 Þ1 : The product BT B is equal to BT B ¼ ðB2 Þ2 :

y ¼ r=k;

This shows that we can determine B2 and therefore B1 from B.

r ¼ ky;

where k is a constant. It can be seen that, in accordance with (1.3.1.6) and (1.3.1.7), the expression of the elongation in terms of y is ur =r ¼ "=y2 : Thus, the elongation is inversely proportional to the square of the radius vector of the quadric of elongations parallel to OP. In practice, it is necessary to look for the intersection p of the parallel to OP drawn from the centre O of the quadric of elongations (Fig. 1.3.1.3a): (i) The eigenvalues all have the same sign; the quadric Q is an ellipsoid: the elongation has the same sign in all directions in space, positive for " ¼ þ1 and negative for " ¼ 1. (ii) The eigenvalues have different signs; two quadrics are to be taken into account: the hyperboloids corresponding, respectively, to " ¼ 1. The sign of the elongation is different according to

Fig. 1.3.1.2. Elongation, ur =r.

73

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 0 1 cos sin 0 whether the direction under consideration is outside or inside the B C asymptotic cone and intersects one or the other of the two B ¼ @ sin cos 0 A; hyperboloids. 0 0 1 Equally, one can connect the displacement vector uðrÞ directly 0 1 with the quadric Q. Using the bilinear form cos 1 sin 0 B C M ¼ @ sin cos 1 0 A: f ðyÞ ¼ Mij yi yj ; 0 0 0 Hence we have

the gradient of f ðyÞ, r ðf Þ, has as components

Mij yi yj ¼ ðcos 1Þðy1 y2 Þ ¼ ": i

@f [email protected] ¼ Mij yj ¼ ui :

The quadric Q is a cylinder of revolution having the axis of rotation as axis.

One recognizes the components of the displacement vector u, which is therefore parallel to the normal to the quadric Q at the extremity of the radius vector Op parallel to r. The directions of the principal axes of Q correspond to the extremal values of y, i.e. to the stationary values (maximal or minimal) of the elongation. These values are the principal elongations. If the deformation is a pure rotation

1.3.1.3. Arbitrary but small deformations 1.3.1.3.1. Deﬁnition of the strain tensor If the deformation is small but arbitrary, i.e. if the products of two or more components of Mij can be neglected with respect to unity, one can describe the deformation locally as a homogeneous asymptotic deformation. As was shown in Section 1.3.1.2.4, it can be put in the form of the product of a pure deformation corresponding to the symmetric part of Mij, Sij , and a pure rotation corresponding to the asymmetric part, Aij : 9 @ui @uj > > Sij ¼ Sji ¼ 12 þ > = @xj @xi ð1:3:1:8Þ @uj > > 1 @ui > :; Aij ¼ Aji ¼ 2 @xj @xi Matrix B can be written B ¼ I þ A þ S; where I is the matrix identity. As the coefﬁcients @ui [email protected] of Mij are small, one can neglect the product A S and one has B ¼ ðI þ AÞðI þ SÞ: ðI þ SÞ is a symmetric matrix that represents a pure deformation. ðI þ AÞ is an antisymmetric unitary matrix and, since A is small, ðI þ AÞ1 ¼ ðI AÞ: Thus, ðI þ AÞ represents a rotation. The axis of rotation is parallel to the vector with coordinates 9 @u3 @u2 > 1 ¼ 12 ¼ A32 > þ > > @x2 @x3 > > > = @u3 1 @u1 ¼ A13 2 ¼ 2 þ > @x @x1 > > 3 > > > @u1 1 @u2 ; ¼ A21 ; > 3 ¼ 2 þ @x1 @x2 which is an eigenvector of ðI þ AÞ. The magnitude of the rotation is equal to the modulus of this vector. In general, one is only interested in the pure deformation, i.e. in the form of the deformed object. Thus, one only wishes to know the quantities ðI þ SÞ and the symmetric part of M. It is this symmetric part that is called the deformation tensor or the strain tensor. It is very convenient for applications to use the simpliﬁed notation due to Voigt:

Fig. 1.3.1.3. Quadric of elongations. The displacement vector, uðrÞ, at P in the deformed medium is parallel to the normal to the quadric at the intersection, p, of OP with the quadric. (a) The eigenvalues all have the same sign, the quadric is an ellipsoid. (b) The eigenvalues have mixed signs, the quadric is a hyperboloid with either one sheet (shaded in light grey) or two sheets (shaded in dark grey), depending on the sign of the constant " [see equation (1.3.1.7)]; the cone asymptote is represented in medium grey. For a practical application, see Fig. 1.4.1.1.

@u1 ; @x1 @u @u S4 ¼ 3 þ 2 ; @x2 @x3

S1 ¼

74

@u2 ; @x2 @u @u S5 ¼ 3 þ 1 ; @x1 @x3

S2 ¼

@u3 ; @x3 @u @u S6 ¼ 2 þ 1 : @x1 @x2

S3 ¼

1.3. ELASTIC PROPERTIES ¼ dx02 =dx1 ¼ @u2 [email protected] ; ¼ dx01 =dx2 ¼ @u1 [email protected] :

One may note that S1 ¼ S11 ; S4 ¼ S23 þ S32 ;

S2 ¼ S22 ; S5 ¼ S31 þ S13 ;

The Voigt strain matrix S is of the 0 S1 S6 @ S6 S2 S5 S4

S3 ¼ S33 ; S6 ¼ S12 þ S21 :

One sees that the coefﬁcient S6 of Voigt’s matrix is therefore S6 ¼

form 1 S5 S 4 A: S3

The angle þ is equal to the difference between angles PQ ^ PR before deformation and P00 Q00 ^ P0 R0 after deformation. The nondiagonal terms of the Voigt matrix therefore represent the shears in the planes parallel to Px1, Px2 and Px3 , respectively. To summarize, if one considers a small cube before deformation, it becomes after deformation an arbitrary parallelepiped; the relative elongations of the three sides are given by the diagonal terms of the strain tensor and the variation of the angles by its nondiagonal terms. The cubic dilatation (1.3.1.5) is

1.3.1.3.2. Geometrical interpretation of the coefﬁcients of the strain tensor Let us consider an orthonormal system of axes with centre P. We remove nothing from the generality of the following by limiting ourselves to a planar problem and assuming that point P0 to which P goes in the deformation lies in the plane x1 Px2 (Fig. 1.3.1.4). Let us consider two neighbouring points, Q and R, lying on axes Px1 and Px2 , respectively (PQ ¼ dx1 , PR ¼ dx2 ). In the deformation, they go to points Q0 and R0 deﬁned by 8 0 > < dx1 ¼ dx1 þ ð@u1 [email protected] Þdx1 0 QQ : dx02 ¼ ð@u2 [email protected] Þdx1 > : 0 dx3 ¼ 0 8 0 > < dx1 ¼ ð@u1 [email protected] Þdx2 RR0 :

> :

@u2 @u1 þ ¼ þ : @x1 @x2

ðBÞ 1 ¼ S1 þ S2 þ S3 (taking into account the fact that the coefﬁcients Sij are small). 1.3.1.4. Particular components of the deformation 1.3.1.4.1. Simple elongation Matrix M has only one coefﬁcient, e1 , and reduces to (Fig. 1.3.1.5a) 0 1 e1 0 0 @ 0 0 0 A: 0 0 0

dx02 ¼ dx2 þ ð@u2 [email protected] Þdx2 dx03 ¼ 0:

As the coefﬁcients @ui [email protected] are small, the lengths of P0 Q0 and P R0 are hardly different from PQ and PR, respectively, and the elongations in the directions Px1 and Px2 are 0

0

0

The quadric of elongations is reduced to two parallel pﬃﬃﬃﬃﬃ planes, perpendicular to Ox1, with the equation x1 ¼ 1= jej.

dx01

P Q PQ dx1 @u1 ¼ ¼ ¼ S1 PQ dx1 @x1 P0 R0 PR dx02 dx2 @u2 ¼ ¼ ¼ S2 : PR dx2 @x2 The components S1, S2 , S3 of the principal diagonal of the Voigt matrix can then be interpreted as the elongations in the three directions Px1, Px2 and Px3 . The angles and between PQ and P0 Q0, and PR and P0 R0 , respectively, are given in the same way by

Fig. 1.3.1.4. Geometrical interpretation of the components of the strain tensor. Ox1 , Ox2 , Ox3 : axes before deformation; Ox01 , Ox02 , Ox03 : axes after deformation.

Fig. 1.3.1.5. Special deformations. The state after deformation is represented by a dashed line. (a) Simple elongation; (b) pure shear; (c) simple shear.

75

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.3.1.4.2. Pure shear This is a pure deformation (without rotation) consisting of the superposition of two simple elongations along two perpendicular directions (Fig. 1.3.1.5b) and such that there is no change of volume (the cubic dilatation is zero): 0 1 e1 0 0 @ 0 e1 0 A: 0 0 0 The quadric of elongations is a hyperbolic cylinder. 1.3.1.4.3. Simple shear Matrix Mij has one coefﬁcient 0 0 s @0 0 0 0

Fig. 1.3.2.1. Deﬁnition of stress: it is the limit of R d when the surface element d tends towards zero. R and R0 are the forces to which the two lips of the small surface element cut within the medium are subjected.

only, a shear (Fig. 1.3.1.5c): 1 0 0 A: 0

Now consider a volume V within the solid C and the surface S which surrounds it (Fig. 1.3.2.2). Among the inﬂuences that are exterior to V, we distinguish those that are external to the solid C and those that are internal. The ﬁrst are translated by the body forces, eventually by volume couples. The second are translated by the local contact forces of the part external to V on the internal part; they are represented by a surface density of forces, i.e. by the stresses Tn that depend only on the point Q of the surface S where they are applied and on the orientation of the normal n of this surface at this point. If two surfaces S and S0 are tangents at the same point Q, the same stress acts at the point of contact between them. The equilibrium of the volume V requires: (i) For the resultant of the applied forces and the inertial forces: RRR RR d RRR Tn d þ F d ¼ v d : ð1:3:2:1Þ dt S V V

The matrix is not symmetrical, as it contains a component of rotation. Thus we have 9 x01 ¼ x1 þ sx2 > = x02 ¼ x2 > ; x03 ¼ x3 : One can show that the deformation is a pure shear associated with a rotation around Ox3 . 1.3.2. Stress tensor 1.3.2.1. General conditions of equilibrium of a solid

(ii) For the resultant moment:

Let us consider a solid C, in movement or not, with a mass distribution deﬁned by a speciﬁc mass at each point. There are two types of force that are manifested in the interior of this solid. (i) Body forces (or mass forces), which one can write in the form

RR S

OQ ^ Tn d þ

RRR V

d RRR OP ^ F d ¼ OP ^ v d ; dt V ð1:3:2:2Þ

where Q is a point on the surface S, P a point in the volume V and v the velocity of the volume element d. The equilibrium of the solid C requires that: (i) there are no stresses applied on its surface and (ii) the above conditions are satisﬁed for any volume V within the solid C.

F dm ¼ F d; where d is a volume element and dm a mass element. Gravity forces or inertial forces are examples of body forces. One can also envisage body torques (or volume couples), which can arise, for example, from magnetic or electric actions but which will be seen to be neglected in practice. (ii) Surface forces or stresses. Let us imagine a cut in the solid along a surface element d of normal n (Fig. 1.3.2.1). The two lips of the cut that were in equilibrium are now subjected to equal and opposite forces, R and R0 ¼ R, which will tend to separate or draw together these two lips. One admits that, when the area element d tends towards zero, the ratio R=d tends towards a ﬁnite limit, Tn , which is called stress. It is a force per unit area of surface, homogeneous to a pressure. It will be considered as positive if it is oriented towards the same side of the surface-area element d as the normal n and negative in the other case. The choice of the orientation of n is arbitrary. The pressure in a liquid is deﬁned in a similar way but its magnitude is independent of the orientation of n and its direction is always parallel to n. On the other hand, in a solid the constraint Tn applied to a surface element is not necessarily normal to the latter and the magnitude and the orientation with respect to the normal change when the orientation of n changes. A stress is said to be homogeneous if the force per unit area acting on a surface element of given orientation and given shape is independent of the position of the element in the body. Other stresses are inhomogeneous. Pressure is represented by a scalar, and stress by a rank-two tensor, which will be deﬁned in Section 1.3.2.2.

1.3.2.2. Deﬁnition of the stress tensor Using the condition on the resultant of forces, it is possible to show that the components of the stress Tn can be determined from the knowledge of the orientation of the normal n and of the components of a rank-two tensor. Let P be a point situated inside volume V, Px1 , Px2 and Px3 three orthonormal axes, and consider a plane of arbitrary orientation that cuts the three axes at Q, R

Fig. 1.3.2.2. Stress, Tn , applied to the surface of an internal volume.

76

1.3. ELASTIC PROPERTIES 1.3.2.3. Condition of continuity Let us return to equation (1.3.2.1) expressing the equilibrium condition for the resultant of the forces. By replacing Tn by the expression (1.3.2.4), we get, after projection on the three axes, RR RRR Tij di þ Fj d ¼ 0; S

V

where di ¼ i d and the inertial forces are included in the volume forces. Applying Green’s theorem to the ﬁrst integral, we have RR R R R Tij di ¼ @Tij [email protected] d: S

V

The equilibrium condition now becomes R R R @Tij [email protected] þ Fj d ¼ 0: V

Fig. 1.3.2.3. Equilibrium of a small volume element.

In order that this relation applies to any volume V, the expression under the integral must be equal to zero,

and S, respectively (Fig. 1.3.2.3). The small volume element PQRS is limited by four surfaces to which stresses are applied. The normals to the surfaces PRS, PSQ and PQR will be assumed to be directed towards the interior of the small volume. By contrast, for reasons that will become apparent later, the normal n applied to the surface QRS will be oriented towards the exterior. The corresponding applied forces are thus given in Table 1.3.2.1. The volume PQRS is subjected to ﬁve forces: the forces applied to each surface and the resultant of the volume forces and the inertial forces. The equilibrium of the small volume requires that the resultant of these forces be equal to zero and one can write

@Tij [email protected] þ Fj ¼ 0;

ð1:3:2:5Þ

or, if one includes explicitly the inertial forces, @Tij [email protected] þ Fj ¼ @2 xj [email protected] :

ð1:3:2:6Þ

This is the condition of continuity or of conservation. It expresses how constraints propagate throughout the solid. This is how the cohesion of the solid is ensured. The resolution of any elastic problem requires solving this equation in terms of the particular boundary conditions of that problem.

Tn d þ T1 d1 þ T2 d2 þ T3 d3 þ F d ¼ 0 1.3.2.4. Symmetry of the stress tensor Let us now consider the equilibrium condition (1.3.2.2) relative to the resultant moment. After projection on the three axes, and using the Cartesian expression (1.1.3.4) of the vectorial products, we obtain RR1 R R R 1 2 "ijk ðxi Tlj xj Tli Þdl þ 2 "ijk ðxi Fj xj Fi Þ þ k d ¼ 0:

(including the inertial forces in the volume forces). As long as the surface element d is ﬁnite, however small, it is possible to divide both terms of the equation by it. If one introduces the direction cosines, i , the equation becomes Tn þ T1 d1 þ T2 d2 þ T3 d3 þ F d=d ¼ 0:

S

When d tends to zero, the ratio d=d tends towards zero at the same time and may be neglected. The relation then becomes i

Tn ¼ Ti :

(including the inertial forces in the volume forces). "ijk is the permutation tensor. Applying Green’s theorem to the ﬁrst integral and putting the two terms together gives Z Z Z @ 1 ðx T xj Tli Þ þ ðxi Fj xj Fi Þ þ k d ¼ 0: 2 "ijk @xl i lj

ð1:3:2:3Þ

This relation is called the Cauchy relation, which allows the stress Tn to be expressed as a function of the stresses T1, T2 and T3 that are applied to the three faces perpendicular to the axes, Px1 , Px2 and Px3 . Let us project this relation onto these three axes: Tnj ¼ Tij i :

V

In order that this relation applies to any volume V within the solid C, we must have @ 1 " ðx T x T Þ þ k ¼ 0 j li 2 ijk @xl i lj

ð1:3:2:4Þ

The nine components Tij are, by deﬁnition, the components of the stress tensor. In order to check that they are indeed the components of a tensor, it sufﬁces to make the contracted product of each side of (1.3.2.4) by any vector xi : the left-hand side is a scalar product and the right-hand side a bilinear form. The Tij ’s are therefore the components of a tensor. The index to the far left indicates the face to which the stress is applied (normal to the x1, x2 or x3 axis), while the second one indicates on which axis the stress is projected.

or 1 2 "ijk

1 2 "ijk ½Tij

1 , 2 and 3 are the direction cosines of the normal n to the small surface QRS. Area

Applied stress

Applied force

QRS PRS PSQ PQR

d d1 ¼ 1 d d2 ¼ 2 d d3 ¼ 3 d

Tn T1 T2 T3

Tn Tn Tn Tn

@Tlj @Tli xi þ Fj xj þ Fi þ Tij Tji þ k ¼ 0: @xl @xl

Taking into account the continuity condition (1.3.2.5), this equation reduces to

Table 1.3.2.1. Stresses applied to the faces surrounding a volume element

Face

V

Tji þ k ¼ 0:

A volume couple can occur for instance in the case of a magnetic or an electric ﬁeld acting on a body that locally possesses magnetic or electric moments. In general, apart from very rare cases, one can ignore these volume couples. One can then deduce that the stress tensor is symmetrical:

d d1 d2 d3

77

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Tij Tji ¼ 0: 1.3.2.5. Voigt’s notation – interpretation of the components of the stress tensor This result can be recovered by applying the relation (1.3.2.2) 1.3.2.5.1. Voigt’s notation, reduced form of the stress tensor to a small volume in the form of an elementary parallelepiped, We shall use frequently the notation due to Voigt (1910) in thus illustrating the demonstration using Green’s theorem but order to express the components of the stress tensor: giving insight into the action of the constraints. Consider a rectangular parallelepiped, of sides 2x1, 2x2 and 2x3 , with T2 ¼ T22 ; T3 ¼ T33 ; T1 ¼ T11 ; centre P at the origin of an orthonormal system whose axes Px1, T4 ¼ T23 ¼ T32 ; T5 ¼ T31 ¼ T13 ; T6 ¼ T12 ¼ T21 : Px2 and Px3 are normal to the sides of the parallelepiped (Fig. 1.3.2.4). In order that the resultant moment with respect to a It should be noted that the conventions are different for the Voigt point be zero, it is necessary that the resultant moments with matrices associated with the stress tensor and with the strain respect to three axes concurrent in this point are zero. Let us tensor (Section 1.3.1.3.1). write for instance that the resultant moment with respect to the The Voigt matrix associated with the stress tensor is therefore axis Px3 is zero. We note that the constraints applied to the faces of the form perpendicular to Px3 do not give rise to a moment and neither do 0 1 T1 T6 T5 the components T11, T13 , T22 and T23 of the constraints applied to @ T6 T2 T4 A : the faces normal to Px1 and Px2 (Fig. 1.3.2.4). The components T12 and T21 alone have a nonzero moment. T5 T4 T3 For face 1, the constraint is T12 þ ð@T12 [email protected] Þx1 if T12 is the magnitude of the constraint at P. The force applied at face 1 is 1.3.2.5.2. Interpretation of the components of the stress tensor – @T12 T12 þ x1 4x2 x3 special forms of the stress tensor @x1 (i) Uniaxial stress: let us consider a solid shaped like a parallelepiped whose faces are normal to three orthonormal axes (Fig. and its moment is 1.3.2.5). The terms of the main diagonal of the stress tensor correspond to uniaxial stresses on these faces. If there is a single @T12 T12 þ x1 4x2 x3 x1 : uniaxial stress, the tensor is of the form @x1 0 1 0 0 0 Similarly, the moments of the force on the other faces are @ 0 0 0 A: 0 0 T3 @T Face 10 : T12 þ 12 ðx1 Þ 4x2 x3 ðx1 Þ; @x1 The solid is submitted to two equal and opposite forces, T33 S3 @T21 and T33 S3 , where S3 is the area of the face of the parallelepiped Face 2 : T21 þ x2 Þ 4x1 x3 x2 ; @x2 that is normal to the Ox3 axis (Fig. 1.3.2.5a). The convention used in general is that there is a uniaxial compression if T3 0 and a @T Face 20 : T21 þ 21 ðx2 Þ 4x1 x3 ðx2 Þ: uniaxial traction if T3 0, but the opposite sign convention is @x2 sometimes used, for instance in applications such as piezoelectricity or photoelasticity. Noting further that the moments applied to the faces 1 and 10 (ii) Pure shear stress: the tensor reduces to two equal uniaxial 0 are of the same sense, and that those applied to faces 2 and 2 are constraints of opposite signs (Fig. 1.3.2.5b): of the opposite sense, we can state that the resultant moment is 0 1 T1 0 0 ½T12 T21 8x1 x2 x3 ¼ ½T12 T21 ; @ 0 T1 0 A: 0 0 0 where 8x1 x2 x3 ¼ is the volume of the small parallelepiped. The resultant moment per unit volume, taking into account the couples in volume, is therefore (iii) Hydrostatic pressure: the tensor reduces to three equal T12 T21 þ 3 : uniaxial stresses of the same sign (it is spherical): 0 1 p 0 0 It must equal zero and the relation given above is thus recovered. @ 0 p 0 A; 0 0 p where p is a positive scalar. (iv) Simple shear stress: the tensor reduces to two equal nondiagonal terms (Fig. 1.3.2.5c), for instance T12 ¼ T21 ¼ T6. T12 represents the component parallel to Ox2 of the stress applied to face 1 and T21 represents the component parallel to Ox1 of the stress applied to face 2. These two stresses generate opposite couples that compensate each other. It is important to note that it is impossible to have one nondiagonal term only: its effect would be a couple of rotation of the solid and not a deformation. 1.3.2.6. Boundary conditions If the surface of the solid C is free from all exterior action and is in equilibrium, the stress ﬁeld Tij inside C is zero at the surface. If C is subjected from the outside to a distribution of stresses Tn

Fig. 1.3.2.4. Symmetry of the stress tensor: the moments of the couples applied to a parallelepiped compensate each other.

78

1.3. ELASTIC PROPERTIES

Fig. 1.3.2.6. Normal (m) and shearing (s) stress.

n ¼ ky: The stress applied to a small surface element d normal to n, Tn , is Tn ¼ kr r ðf Þ and the normal stress, , is ¼ i Ti ¼ 1=y2 ; where the i ’s are the direction cosines of n. (iii) Principal normal stresses: the stress tensor is symmetrical and has therefore real eigenvectors. If we represent the tensor with reference to a system of axes parallel to its eigenvectors, it is put in the form 0 1 0 T1 0 @ 0 T2 0 A : 0 0 T3

Fig. 1.3.2.5. Special forms of the stress tensor. (a) Uniaxial stress: the stress tensor has only one component, T33 ; (b) pure shear stress: T22 ¼ T11 ; (c) simple shear stress: T21 ¼ T12 .

(apart from the volume forces mentioned earlier), the stress ﬁeld inside the solid is such that at each point of the surface

T1 , T2 and T3 are the principal normal stresses. The mean normal stress, T, is deﬁned by the relation

Tnj ¼ Tij i ;

T ¼ ðT1 þ T2 þ T3 Þ=3

where the j ’s are the direction cosines of the normal to the surface at the point under consideration.

and is an invariant of the stress tensor.

1.3.2.7. Local properties of the stress tensor (i) Normal stress and shearing stress: let us consider a surface area element d within the solid, the normal n to this element and the stress Tn that is applied to it (Fig. 1.3.2.6). The normal stress, m, is, by deﬁnition, the component of Tn on n,

1.3.2.8. Energy density in a deformed medium

(ii) The stress quadric: let us consider the bilinear form attached to the stress tensor:

Consider a medium that is subjected to a stress ﬁeld Tij . It has sustained a deformation indicated by the deformation tensor S. During this deformation, the forces of contact have performed work and the medium has accumulated a certain elastic energy W. The knowledge of the energy density thus acquired is useful for studying the properties of the elastic constants Let the medium deform from the deformation Sij to the deformation Sij þ Sij under the inﬂuence of the stress ﬁeld and let us evaluate the work of each component of the effort. Consider a small elementary rectangular parallelepiped of sides 2x1, 2x2 , 2x3 (Fig. 1.3.2.8). We shall limit our calculation to the components T11 and T12 , which are applied to the faces 1 and 10 , respectively. In the deformation S, the point P goes to the point P0 , deﬁned by

f ðyÞ ¼ Tij yi yj :

PP0 ¼ uðrÞ:

m ¼ nðTn nÞ and the shearing stress, s, is the projection of Tn on the surface area element, s ¼ n ^ ðTn ^ nÞ ¼ Tn m:

A neighbouring point Q goes to Q0 such that (Fig. 1.3.1.1)

The quadric represented by f ðyÞ ¼ "

PQ ¼ r;

P0 Q0 ¼ r0 :

The coordinates of r0 are given by

is called the stress quadric, where " ¼ 1. It may be an ellipsoid or a hyperboloid. Referred to the principal axes, and using Voigt’s notation, its equation is

x0i ¼ xi þ Sij xj :

y2i Ti ¼ ":

Of sole importance is the relative displacement of Q with respect to P and the displacement that must be taken into account in calculating the forces applied at Q. The coordinates of the relative displacement are

To every direction n of the medium, let us associate the radius vector y of the quadric (Fig. 1.3.2.7) through the relation

79

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.3.2.8. Determination of the energy density in a deformed medium. PP0 represents the displacement of the small parallelepiped during the deformation. The thick arrows represent the forces applied to the faces 1 and 10 .

Fig. 1.3.2.7. The stress quadric: application to the determination of the stress applied to a surface element. The surface of the medium is shaded in light grey and a small surface element, d, is shaded in medium grey. The stress at P is proportional to r ðf Þ at the intersection of OP with the stress quadric.

where E is the elastic stiffness, also called Young’s modulus. The physical mechanism at the origin of elasticity is the deformation of the chemical bonds between atoms, ions or molecules in the solid, which act as so many small springs. The reaction of these springs to an applied stress is actually anharmonic and Hooke’s law is only an approximation: a Taylor expansion up to the ﬁrst term. A rigorous treatment of elasticity requires nonlinear phenomena to be taken into account. This is done in Section 1.3.6. The stress below which the strain is recoverable when the stress is removed, To , is called the elastic limit. (ii) If T > To, the deformation curve is no longer reversible. If one releases the applied stress, the bar assumes a permanent deformation. One says that it has undergone a plastic deformation. The region of the deformation is ultimately limited by rupture (symbolized by an asterisk on Fig. 1.3.3.2). The plastic deformation is due to the formation and to the movement of lattice defects such as dislocations. The material in its initial state, before the application of a stress, is not free in general from defects and it possesses a complicated history of deformations. The proportionality constant between stresses and deformations in the elastic region depends on the interatomic force constants and is an intrinsic property, very little affected by the presence of defects. By contrast, the limit, To , of the elastic region depends to a large extent on the defects in the material and on its history. It is

x0i xi ¼ Sij xj : We shall take as the position of Q the point of application of the forces at face 1, i.e. its centre with coordinates x1 ; 0; 0 (Fig. 1.3.2.8). The area of face 1 is 4x2 x3 and the forces arising from the stresses T11 and T12 are equal to 4x2 x3 T11 and 4x2 x3 T12 , respectively. The relative displacement of Q parallel to the line of action of T11 is x1 S11 and the corresponding displacement along the line of action of T12 is x1 S21. The work of the corresponding forces is therefore for T11 :

4x1 x2 x3 T11 S11

for T12 :

4x1 x2 x3 T11 S21 :

The work of the forces applied to the face 10 is the same (T11 , T12 and x1 change sign simultaneously). The works corresponding to the faces 1 and 10 are thus T11 S11 and T12 S21 for the two stresses, respectively. One ﬁnds an analogous result for each of the other components of the stress tensor and the total work per unit volume is W ¼ Tij Sji :

ð1:3:2:7Þ

1.3.3. Linear elasticity 1.3.3.1. Hooke’s law Let us consider a metallic bar of length lo loaded in pure tension (Fig. 1.3.3.1). Under the action of the uniaxial stress T ¼ F=A (F applied force, A area of the section of the bar), the bar elongates and its length becomes l ¼ lo þ l. Fig. 1.3.3.2 relates the variations of l and of the applied stress T. The curve representing the traction is very schematic and does not correspond to any real case. The following result, however, is common to all concrete situations: (i) If 0 < T < To, the deformation curve is reversible, i.e. if one releases the applied stress the bar resumes its original form. To a ﬁrst approximation, the curve is linear, so that one can write Hooke’s law: l 1 ¼ T; l E

ð1:3:3:1Þ Fig. 1.3.3.1. Bar loaded in pure tension.

80

1.3. ELASTIC PROPERTIES an extrinsic property. For example, the introduction of carbon into iron modiﬁes considerably the extent of the elastic region. The extents of the elastic and plastic regions vary appreciably from one material to another. Fragile materials, for instance, have a much reduced plastic region, with a clear break.

1.3.3.2.2. Matrix notation – reduction of the number of independent components It is convenient to write the relations (1.3.3.2) in matrix form by associating with the stress and strain tensors column matrices 1 9 and with the tensors of the elastic stiffnesses, c, and of the elastic compliances, s, square matrices 9 9 (Section 1.1.4.10.4); these two 9 9 matrices are inverse to one another. The number of independent components of the fourth-rank elastic tensors can be reduced by three types of consideration: (i) Intrinsic symmetry: it was shown in Section 1.1.1.4 that tensors representing principal properties are symmetric. This is the case of the elastic tensors and can be shown directly using expression (1.3.2.7) of the energy stored per unit volume in the medium when we allow it to deform from the state Sij to the state Sij þ Sij under the action of the stress Tij :

1.3.3.2. Elastic constants 1.3.3.2.1. Deﬁnition Young’s modulus is not sufﬁcient to describe the deformation of the bar: its diameter is reduced, in effect, during the elongation. One other coefﬁcient, at least, is therefore necessary. In a general way, let us consider the deformation of a continuous anisotropic medium under the action of a ﬁeld of applied stresses. We will generalize Hooke’s law by writing that at each point there is a linear relation between the components Tij of the stress tensor and the components Sij of the strain tensor: Sij ¼ sijkl Tkl Tij ¼ cijkl Skl :

W ¼ Tij Sji : Applying relation (1.3.3.1), we get

ð1:3:3:2Þ

@[email protected] ¼ cijkl Skl :

The quantities sijkl and cijkl are characteristic of the elastic properties of the medium if it is homogeneous and are independent of the point under consideration. Their tensorial nature can be shown using the demonstration illustrated in Section 1.1.3.4. Let us take the contracted product of the two sides of each of the two equations of (1.3.3.2) by the components xi and yj of any two vectors, x and y:

ð1:3:3:3Þ

Hence, one has by further differentiation @2 W=ð@Sij @Skl Þ ¼ cijkl : Nothing is changed by interchanging the role of the pairs of dummy indices ij and lk:

Sij xi yj ¼ sijkl Tkl xi yj

@2 W=ð@Skl @Sij Þ ¼ cklij :

Tij xi yj ¼ cijkl Skl xi yj :

Since the energy is a state function with a perfect differential, one can interchange the order of the differentiations: the members on the left-hand sides of these two equations are therefore equal; one then deduces

The left-hand sides are bilinear forms since Sij and Tij are secondrank tensors and the right-hand sides are quadrilinear forms, which shows that sijkl and cijkl are the components of fourth-rank tensors, the tensor of elastic compliances (or moduli) and the tensor of elastic stiffnesses (or coefﬁcients), respectively. The number of their components is equal to 81. Equations (1.3.3.2) are Taylor expansions limited to the ﬁrst term. The higher terms involve sixth-rank tensors, sijklmn and cijklmn , with 36 ¼ 729 coefﬁcients, called third-order elastic compliances and stiffnesses and eighth-rank tensors with 38 ¼ 6561 coefﬁcients, called fourth-order elastic compliances and stiffnesses. They will be deﬁned in Section 1.3.6.4. Tables for third-order elastic constants are given in Fumi (1951, 1952, 1987). The accompanying software to this volume enables these tables to be derived for any point group.

cijkl ¼ cklij :

ð1:3:3:4Þ

The tensor of elastic stiffnesses (and also the tensor of elastic compliances) is thus symmetrical. As shown in Section 1.1.4.5.2.2, the number of their independent components is therefore reduced to 45. (ii) Symmetry of the strain and stress tensors: the strain tensor Sij is symmetric by deﬁnition (Section 1.3.1.3.1) because rotations are not taken into account and the stress tensor Tij is symmetric (Section 1.3.2.4) because body torques are neglected. For this reason, summation (1.3.3.2), Sij ¼ sijkl Tkl , can be factorized [equation (1.1.4.11)]: P P

Sij ¼ sijll Tll þ sijkl þ sijlk Tkl : l

k6¼l

This shows that the number of independent components of tensor sijkl is reduced. This effect of the symmetry of the strain and stress tensors was discussed systematically in Section 1.1.4.10.4. It was shown that sijkl ¼ sijlk ¼ sjikl ¼ sjilk cijkl ¼ cijlk ¼ cjikl ¼ cjilk

ð1:3:3:5Þ

and that the number of independent elastic compliances or stiffnesses is reduced to 21. They are replaced by two-index coefﬁcients constituting 6 6 matrices according to Voigt’s notation:

Fig. 1.3.3.2. Schematic stress–strain curve. T: stress; To : elastic limit; l=l: elongation; the asterisk symbolizes the rupture.

81

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 9 compliances c14 ¼ c56 c23 ¼ c44 ; stiffnesses > > > > c13 ¼ c55 ; c25 ¼ c46 i ¼ j; k ¼ l s ¼ siill = c12 ¼ c66 ; c36 ¼ c45 : c ¼ cijkl: i ¼ j; k 6¼ l s ¼ siill þ siilk > > i 6¼ j; k ¼ l s ¼ sijll þ sjill > > ; These are known as the Cauchy relations. The further symmetry s ¼ sijkl þ sjikl þ sijlk þ sjilk i 6¼ j; k 6¼ l that they imply reduces the maximum number of independent ð1:3:3:6Þ constants from 21 to 15. In the spherical system (Section 1.1.4.10.6.8), this number is reduced to 1 (c11 ¼ 3c12 ). Poisson’s Using these notations and Voigt’s notations for the strain and ratio, ¼ s12 =s11 , deﬁned in Section 1.3.3.4.3, is then equal to stress tensors, equations (1.3.3.2) become: 0.25, taking into account the relations between s11 ; s12 and c11 ; c12 given in Section 1.3.3.2.3. In practice, Table 1.3.3.2 shows that in S ¼ s T real crystals is never equal to 0.25, and that Cauchy relations do ð1:3:3:7Þ not apply. T ¼ c S : The extent to which Cauchy relations are fulﬁlled is often used to assess the validity of the assumption of a central-force law. It For instance, the ﬁrst of these two relations is written, once is important to apply such a test only to structures having the developed, as necessary symmetry properties for Cauchy relations to hold. For instance, f.c.c. and b.c.c. metals have the required symmetry (an 10 1 0 1 0 T1 s11 s12 s13 s14 s15 s16 S1 inversion centre at each atomic site), while diamond, silicon and B S2 C B s12 s22 s23 s24 s25 s26 CB T2 C germanium do not. Consequently, any apparent fulﬁlment of CB C B C B B S3 C B s13 s23 s33 s34 s35 s36 CB T3 C the Cauchy relation c12 ¼ c66 , or ’ 0:25, for a diamond-type CB C B C¼B B S4 C B s14 s24 s34 s44 s45 s46 CB T4 C: ð1:3:3:8Þ structure offers no ground for conclusions about the nature of the CB C B C B force ﬁeld. @ S5 A @ s15 s25 s35 s45 s55 s56 [email protected] T5 A S6 s16 s26 s36 s46 s56 s66 T6 1.3.3.2.3. Passage from elastic compliances s to elastic stiffnesses c Matrices s and c are the inverse of each another. It is We have noted already that the matrix c is the inverse of the important to note that they are matrices and not tensors. One matrix s . These matrices can be written for cubic and isotropic cannot apply to them the usual rules of transformation under a materials as follows: change of base since they are only valid for the components of a 1 0 0 0 s11 s12 s12 0 tensor. In cases where the coordinate system is changed, it is Bs necessary to use the components sijkl and cijkl or to establish the 0 0 C C B 12 s11 s12 0 rules of transformation for s and c . C B C B s s s 0 0 0 12 12 11 (iii) Symmetry of the crystal: the reduction of the number of C B s ¼ B 0 0 s44 0 0 C independent components of the matrices s and c was C B 0 C B discussed in Section 1.1.4.10.6. As a summary, Table 1.3.3.1 gives @ 0 0 0 0 s44 0 A the number of independent components for each Laue class. 0 0 0 0 0 s44 (iv) Cauchy relations: in 1828, the French physicist A.-L. 1 0 0 0 c11 c12 c12 0 Cauchy expressed the strain energy of a discrete-particle structure when its potential energy depends only on attractive and Bc 0 0 C C B 12 c11 c12 0 repulsive cohesive forces between pairs of material points (the C B C B c c c 0 0 0 12 12 11 so-called central or point-to-point force law). These forces act C; B c ¼ B along the line joining the points and depend on the distances 0 0 c44 0 0 C C B 0 C B between these points. It can be shown that, if in addition every @ 0 0 0 0 c44 0 A atom is situated at a centre of symmetry, the elastic constants are 0 0 0 0 0 c44 totally symmetric in their four indices. Thus, cijkl ¼ cikjl ¼ ciljk :

where we have, for isotropic materials, s44 ¼ 2ðs11 s12 Þ

This additional symmetry to the symmetries required by the previous considerations implies the following relations between the two-index components:

c44 ¼ 12 ðc11 c12 Þ: We easily ﬁnd that c11 þ c12 ; ðc11 c12 Þðc11 þ 2c12 Þ c12 ; s12 ¼ ðc11 c12 Þðc11 þ 2c12 Þ 1 s44 ¼ ; c44

Table 1.3.3.1. Number of independent components of the elastic compliances and stiffnesses for each Laue class

Laue class 1 1; 2=m; 2; m mmm; 222; 2mm 3 3; 32; 3m 3m; 4=m; 4; 4 4=mmm; 422; 42m; 42m 6=m; 6; 6 6=mmm; 622; 62m; 62m 23 m3; 432; 432 m3m; 1A1 =MC; 1A1

ð1:3:3:9Þ

s11 ¼

No. of independent components 21 13 9 7 6 7 6 5 5 3 3 2

s11 þ s12 ; ðs11 s12 Þðs11 þ 2s12 Þ s12 c12 ¼ ; ðs11 s12 Þðs11 þ 2s12 Þ 1 c44 ¼ : s44 c11 ¼

The coefﬁcient c44 is sometimes called the rigidity modulus. 1.3.3.3. Elastic strain energy Expression (1.3.2.7) of the strain energy stored per unit volume in a medium for a small deformation can be integrated when the medium is strained under a stress Tij according to linear elasticity.

82

1.3. ELASTIC PROPERTIES Applying relation (1.3.3.2), one gets for the density of strain energy W ¼ 12 Tij Sij ¼ 12 cijkl Sij Skl :

In the case of a cubic or isotropic medium, this expression reduces to

ð1:3:3:10Þ

The coefﬁcient of linear compressibility is then equal to one third of the coefﬁcient of volume compressibility. We note that the quadric of elongations is a sphere.

1.3.3.4. Particular elastic constants 1.3.3.4.1. Volume compressibility Let us apply a hydrostatic pressure (Section 1.3.2.5.2). The medium undergoes a relative variation of volume V=V ¼ S1 þ S2 þ S3 (the cubic dilatation, Section 1.3.1.3.2). If one replaces in (1.3.3.8) the stress distribution by a hydrostatic pressure, one obtains for the components of the strain tensor

1.3.3.4.3. Young’s modulus, Poisson’s ratio If the applied stress reduces to a uniaxial stress, T11 ¼ T, the strain tensor is of the form S ¼ s1 T:

S1 ¼ pðs11 þ s12 þ s13 Þ In particular,

S2 ¼ pðs12 þ s22 þ s23 Þ S3 ¼ pðs13 þ s23 þ s13 Þ:

S1 ¼ s11 T;

E ¼ 1=s11 :

1 V ¼ s11 þ s22 þ s33 þ 2ðs12 þ s23 þ s13 Þ: ¼ pV ð1:3:3:11Þ

S2 ¼ S3 ¼ s12 T:

ð1:3:3:12Þ

One deduces from this that s12 is necessarily of opposite sign to s11 and one calls the ratio ¼ s12 =s11 Poisson’s ratio. Putting this value into expression (1.3.3.12) for the coefﬁcient of compressibility in cubic or isotropic materials gives

1.3.3.4.2. Linear compressibility Under the action of a hydrostatic pressure, each vector assumes a different elongation. This elongation is given by equation (1.3.1.6):

1 ¼ 3s11 ð1 2 Þ:

ð1:3:3:14Þ

As the coefﬁcient of compressibility, by deﬁnition, is always positive, we have

ur Sij xi xj ¼ 2 ¼ Sij i j ¼ sijkl Tkl i j ; r r

0 < < 0:5:

where the i ’s are the direction cosines of r. The coefﬁcient of linear compressibility is, by deﬁnition, ð1=pÞður =rÞ. Replacing Tkl by its value pkl , we obtain for the coefﬁcient of linear compressibility

ð1:3:3:13Þ

The elongation of a bar under the action of a uniaxial stress is characterized by S1 and the diminution of the cross section is characterized by S2 and S3 . For a cubic material, the relative diminution of the diameter is

This expression reduces for a cubic or isotropic medium to

¼ 1 ¼ 3ðs11 þ 2s12 Þ:

S2 ¼ s12 T:

We deduce from this that Young’s modulus (equation 1.3.3.1) is

From this, we deduce the volume compressibility, , which is the inverse of the bulk modulus, :

¼ 1

1 ur ¼ s11 þ 2s12 : pr

In practice, Poisson’s ratio is always close to 0.3. It is a dimensionless number. The quantity s44 =2ðs11 s12 Þ represents the departure from isotropy of the material and is the anisotropy factor. It is to be noted that cubic materials are not isotropic for elastic properties. Table 1.3.3.2 gives the values of s11, s12 , s44 , and s44 =2ðs11 s12 Þ for a few cubic materials.

1 ur ¼ sijkl i j : pr

Table 1.3.3.2. Elastic compliances of some cubic materials in (GPa)1 (after Every & McCurdy, 1992) Material

s11

s12

s44

s44 =2ðs11 s12 Þ

Ag Al C (diamond) Cu Fe Ge Mo Ni Pb Si W LiF MgO NaCl GaAs ZnS BaTiO3 Adamantane Almandine (Fe3Al2Si3O12) Spinel (MgAl2O4)

22.9 16.0 1.12 15.0 7.67 9.73 2.63 7.67 93.7 7.73 2.45 11.6 4.01 22.9 11.75 19.7 8.33 240 4.036

9.8 5.8 0.14 6.3 2.83 2.64 0.74 2.93 43.04 2.15 0.69 3.35 0.96 4.8 3.66 7.6 2.68 79 1.093

22.1 35.3 1.83 13.3 8.57 14.9 9.20 8.23 68.0 12.20 6.24 15.8 6.47 78.3 16.8 22.6 9.24 295 10.77

0.428 0.362 0.125 0.42 0.369 0.271 0.273 0.382 0.459 0.279 0.281 0.289 0.239 0.133 0.311 0.386 0.322 0.329 0.271

0.338 0.810 0.726 0.312 0.408 0.602 1.304 0.388 0.249 0.636 0.995 0.528 0.651 1.452 0.545 0.414 0.420 0.462 1.050

5.80

2.05

6.49

0.353

0.413

83

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES (vii) Tetragonal system (groups 422, 42m, 4mm, 4=mmm):

s011 ¼ s11 þ s66 2ðs11 s12 Þ sin2 2=4 sin4 ’ þ s33 cos4 ’ þ ð2s13 þ s44 Þ sin2 2’=4:

1.3.3.4.4. Variation of Young’s modulus with orientation It is interesting to calculate Young’s modulus in any direction. For this it is sufﬁcient to change the axes of the tensor sijkl . If A is the matrix associated with the change of axes, leading to the direction x1 changing to the direction x01 , then Young’s modulus in this new direction is E0 ¼ 1=s011

(viii) Hexagonal system: s011 ¼ s11 sin4 ’ þ s33 cos4 ’ þ ð2s13 þ s44 Þ sin2 2’=4:

with s011 ¼ s01111 ¼ A1i A1j A1k A1l sijkl :

ð1:3:3:15Þ (ix) Cubic system: s011 ¼ s11 þ s44 2ðs11 s12 Þ sin2 ’ cos2 ’ þ sin2 2 sin2 ’=4 :

The matrix coefﬁcients A1i are the direction cosines of Ox01 with respect to the axes Ox1, Ox2 and Ox3 . In spherical coordinates, they are given by (Fig. 1.3.3.3) A11 ¼ cos sin ’;

A12 ¼ sin sin ’;

A13 ¼ cos ’;

This expression reduces to s11 if s44 2ðs11 s12 Þ ¼ 0 and we retrieve the relation between elastic compliances in an isotropic material (Sections 1.1.4.10.4 and 1.3.3.2.3). The representation surface of s11, the inverse of Young’s modulus, is illustrated in Figure 1.3.3.4 for crystals of different symmetries. As predicted by the Neumann principle, the representation surface is invariant with respect to the symmetry elements of the point group of the crystal but, as stated by the Curie laws, its symmetry can be larger. In the examples of Fig. 1.3.3.4, the symmetry of the surface is the same as that of the point group for aluminium (Fig. 1.3.3.4a), tungsten (Fig. 1.3.3.4b) and sodium chloride (Fig. 1.3.3.4c), which have m3m as point group, for tin (Fig. 1.3.3.4e, 4=mmm) and for calcite (Fig. 1.3.3.4f, 3m). But in the case of zinc (Fig. 1.3.3.4d, 6=mmm), the surface is of revolution and has a larger symmetry. It is interesting to compare the differences in shapes of the representation surfaces for the three cubic crystals, depending on the value of the anisotropy factor, which is larger than 1 for aluminium, smaller than 1 for sodium chloride and close to 1 for tungsten (see Table 1.3.3.2). In this latter case, the crystal is pseudo-isotropic and the surface is practically a sphere.

where is the angle between Ox01 and Ox1 , and ’ is the angle between Ox01 and Ox3 . Using the reduction of sijkl for the various crystal classes (Section 1.1.4.9.9), we ﬁnd, in terms of the reduced two-index components, the following. (i) Triclinic system (groups 1, 1): s011 ¼ s11 cos4 þ s22 sin4 þ ð2s12 þ s66 Þ sin2 2=4 þ ðs16 cos þ s26 sin Þ sin 2 sin4 ’

þ 2 ðs25 þ s46 Þ sin þ ðs14 þ s56 Þ cos sin 2=2 þ s15 cos3 þ s24 sin3 cos ’ sin3 ’ þ ð2s23 þ s44 Þ sin2 þ ð2s13 þ s55 Þ cos2 þ ðs36 þ s45 Þ sin 2 sin2 2’=4 þ 2ðs35 cos þ s34 sin Þ cos3 ’ sin ’ þ s33 cos4 ’: (ii) Monoclinic system (groups 2, m, 2=m): s011 ¼ s11 cos4 þ s22 sin4 þ ð2s12 þ s66 Þ sin2 2=4 sin4 ’ þ 2 ðs25 þ s46 Þ sin2 þ s15 cos2 cos ’ sin3 ’ cos þ ð2s23 þ s44 Þ sin2 þ ð2s13 þ s55 Þ cos2 sin2 2’=4

1.3.3.5. Isotropic materials The isotropy relation between elastic compliances and elastic stiffnesses is given in Section 1.3.3.2.3. For reasons of symmetry, the directions of the eigenvectors of the stress and strain tensors are necessarily the same in an isotropic medium. If we take these directions as axes, the two tensors are automatically diagonalized and the second relation (1.3.3.7) becomes

þ 2s35 cos3 ’ sin ’ cos þ s33 cos4 ’: (iii) Orthorhombic system (groups 222, 2mm, mmm): s011 ¼ s11 cos4 þ s22 sin4 þ ð2s12 þ s66 Þ sin2 2=4 sin4 ’ þ ð2s23 þ s44 Þ sin2 þ ð2s13 þ s55 Þ cos2 sin2 2’=4 þ s33 cos4 ’: (iv) Trigonal system (groups 3, 3): s011 ¼ s11 sin4 ’ þ s33 cos4 ’ þ ð2s13 þ s44 Þ sin2 2’=4 þ ðs14 sin 3 s25 cos 3Þ sin 2’ sin2 ’: (v) Trigonal system (groups 32, 3m, 3m): s011 ¼ s11 sin4 ’ þ s33 cos4 ’ þ ð2s13 þ s44 Þ sin2 2’=4 þ s14 sin 3 sin 2’ sin2 ’: 4=m): (vi) Tetragonal system (groups 4, 4;

s011 ¼ s11 þ s66 2ðs11 s12 Þ sin2 2=4 sin4 ’ þ s33 cos4 ’ þ ð2s13 þ s44 Þ sin2 2’=4 þ s16 sin 4 sin4 ’=2:

Fig. 1.3.3.3. Spherical coordinates.

84

1.3. ELASTIC PROPERTIES

Fig. 1.3.3.4. Representation surface of the inverse of Young’s modulus. (a) Al, cubic, anisotropy factor > 1; (b) W, cubic, anisotropy factor ¼ 1; (c) NaCl, cubic, anisotropy factor < 1; (d) Zn, hexagonal; (e) Sn, tetragonal; (f) calcite, trigonal.

T1 ¼ c11 S1 þ c12 ðS2 þ S3 Þ

T1 ¼ 2 S1 þ ðS1 þ S2 þ S3 Þ

T2 ¼ c12 S1 þ c11 S2 þ c12 S3 T3 ¼ c12 ðS1 þ S2 Þ þ c11 S3 :

T2 ¼ 2 S2 þ ðS1 þ S2 þ S3 Þ T3 ¼ 2 S3 þ ðS1 þ S2 þ S3 Þ:

ð1:3:3:16Þ

Two coefﬁcients sufﬁce to deﬁne the elastic properties of an isotropic material, s11 and s12 , c11 and c12 , and , and , etc. Table 1.3.3.3 gives the relations between the more common elastic coefﬁcients.

These relations can equally well be written in the symmetrical form T1 ¼ ðc11 c12 ÞS1 þ c12 ðS1 þ S2 þ S3 Þ T2 ¼ ðc11 c12 ÞS2 þ c12 ðS1 þ S2 þ S3 Þ

1.3.3.6. Equilibrium conditions of elasticity for isotropic media We saw in Section 1.3.2.3 that the condition of equilibrium is

T3 ¼ ðc11 c12 ÞS3 þ c12 ðS1 þ S2 þ S3 Þ:

@Tij [email protected] þ Fj ¼ 0:

If one introduces the Lame´ constants, ¼ ð1=2Þðc11 c12 Þ ¼ c44

If we use the relations of elasticity, equation (1.3.3.2), this condition can be rewritten as a condition on the components of the strain tensor:

¼ c12 ; the equations may be written in the form often used in mechanics:

cijkl

@Skl þ Fi ¼ 0: @xj

Table 1.3.3.3. Relations between elastic coefﬁcients in isotropic media Coefﬁcient

In terms of and

In terms of and

In terms of c11 and c12

c11 c12 c44 ¼ 1=s44 E ¼ 1=s11 s12 ¼ s12 =s11

2 þ ð2 þ 3Þ=ð þ Þ =½2 ð2 þ 3Þ 3=ð2 þ 3Þ =½2ð2 þ 3Þ

2 ð1 Þð1 2 Þ 2 ð1 2 Þ 2 ð1 þ Þ =½2 ð1 þ Þ 3ð1 2 Þ=½2 ð1 þ Þ

c11 c12 ðc11 c12 Þ=2 See Section 1.3.3.2.3 See Section 1.3.3.2.3 3=ðc11 þ 2c12 Þ c11 =ðc11 þ c12 Þ

85

Recalling that Skl ¼

1 2

@uk @ul þ ; @xl @xk

the condition becomes a condition on the displacement vector, uðrÞ:

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 2

cijkl

@ þ Fi ¼ 0: @xl @xj

cijkl

r ¼ r0 þ u; where only u depends on the time and r0 deﬁnes the mean position. Equation (1.3.4.3) is written therefore cijkl

¼ 0:

cijkl uk qj ql ¼ 2 ui :

1.3.4.1. Introduction The elastic properties of materials have been considered in the preceding section in the static state and the elastic constants have been deﬁned in terms of the response of the material to particular static forces. It is effectively the way the elastic constants have been measured in the past, although the measurements could not be very precise. A way of proceeding frequently used now is to excite a mechanical wave in the crystal and measure its propagation velocity or the wavelength associated with a particular frequency. One method consists in sending a train of ultrasonic waves through the crystal; one uses a pulse generator and a piezoelectric transducer glued to the crystal. The elapsed time between the emission of the train of waves and its reception after reﬂection from the rear face of the sample is then measured. Another method involves producing a system of standing waves after reﬂection at the inner surface of the crystal and determining the set of resonance frequencies. The experimental techniques will be described in Section 1.3.4.6. The purpose of the next sections is to establish relations between the wavelength – or the velocity of propagation – and the elastic constants.

With this relation and (1.3.4.2), the system (1.3.4.5) becomes cijkl uk j l ¼ 2 ui :

ð1:3:4:6Þ

ik ¼ cijkl j l

ð1:3:4:7Þ

Putting

in (1.3.4.6), the condition that the Christoffel determinant is zero can be written

ik 2 ik ¼ 0: ð1:3:4:8Þ On account of the intrinsic symmetry of the tensor of elastic stiffnesses, the matrix ik is symmetrical. If we introduce into expression (1.3.4.7) the elastic stiffnesses with two indices [equation (1.3.3.6)], we ﬁnd, for instance, for 11 and 12 11 ¼ c11 ð1 Þ2 þ c66 ð2 Þ2 þ c55 ð3 Þ2 þ 2c16 1 2 þ 2c15 1 3 þ 2c56 2 3 12 ¼ c16 ð1 Þ2 þ c26 ð2 Þ2 þ c45 ð3 Þ2 þ ðc12 þ c66 Þ1 2 þ ðc14 þ c56 Þ1 3 þ ðc46 þ c25 Þ2 3 :

ð1:3:4:1Þ

The expression for the effective value, ceijkl , of the ‘stiffened’ elastic stiffness in the case of piezoelectric crystals is given in Section 2.4.2.2.

where is the frequency and q is the wavevector. The velocity of propagation of the wave is

1.3.4.3. Dynamic elastic stiffnesses Equation (1.3.4.7) may be written P ik ¼ cijkl þ cilkj j l :

ð1:3:4:2Þ

We saw in Section 1.3.3.6 that the equilibrium condition is cijkl

ð1:3:4:5Þ

qi ¼ qi :

1.3.4.2. Equation of propagation of a wave in a material Consider the propagation of a wave in a continuous medium. The elongation of each point will be of the form

V ¼ =q:

ð1:3:4:4Þ

It can be seen that, for a given wavevector, 2 appears as an eigenvalue of the matrix cijkl uk qj ql of which the vibration vector u is an eigenvector. This matrix is called the dynamical matrix, or Christoffel matrix. In order that the system (1.3.4.5) has a solution other than a trivial one, it is necessary that the associated determinant be equal to zero. It is called the Christoffel determinant and it plays a fundamental role in the study of the propagation of elastic waves in crystals. Let 1 ; 2 ; 3 be the direction cosines of the wavevector q. The components of the wavevector are

ð1:3:3:17Þ

1.3.4. Propagation of elastic waves in continuous media – dynamic elasticity

u ¼ u0 expð2 i tÞ expð2 iq rÞ;

@2 u k @2 u ¼ 2i : @xl @xj @t

Replacing u by its value in (1.3.4.1), dividing by 4 2 and using orthonormal coordinates, we get

This equation can ﬁnally be rearranged in one of the three following forms with the aid of Table 1.3.3.3. c12 Þu þ 12 ðc11 þ c12 Þr r ðr r uÞ þ F ¼ 0 u þ ð þ Þr r ðr r uÞ þ F ¼ 0 1 r ðr r uÞ þ F ¼ 0: u þ 1 2

ð1:3:4:3Þ

The position vector of the point under consideration is of the form

In an isotropic orthonormal medium, this equation, projected on the axis Ox1, can be written with the aid of relations (1.3.3.5) and (1.3.3.9): 2 @2 u1 @ u2 @2 u 3 þ c þ c11 12 ð@x1 Þ2 @x1 @x2 @x1 @x3 2 @ u1 @2 u 3 @2 u 1 þ þ þ 12 ðc11 c12 Þ þ Fi ð@x2 Þ2 @x1 @x3 ð@x3 Þ2

1 2 ðc11

@2 u k @2 x ¼ 2i : @xl @xj @t

j6¼l

@2 uk þ Fi ¼ 0: @xl @xj

This shows that in a dynamic process only the sums ½cijkl þ cilkj can be measured and not cijkl and cilkj separately. On the contrary, cijij can be measured directly. In the cubic system therefore, for instance, c1122 is determined from the measurement

Here the only volume forces that we must consider are the inertial forces:

86

1.3. ELASTIC PROPERTIES 0 1 0 0 c11 2 of ½c1122 þ c1221 on the one hand and from that of c1221 on the @ A ¼ 0: other hand. 0 c66 2 0 2 0 0 c44 1.3.4.4. Polarization of the elastic waves The Christoffel determinant has three roots and the Christoffel matrix, being Hermitian with real coefﬁcients, has three real The three solutions are given in Table 1.3.4.5. eigenvalues and three orthogonal eigenvectors. The wavevector q, therefore, encompasses three waves with vibration vectors u1, 1.3.4.5.3. Tetragonal crystals (classes 4mm, 42m, 4=mmm) u2 , u3 which are perpendicular to one another. In the general In tetragonal crystals, there are six independent elastic stiffcase, there is no particular angular relationship between the nesses, c , c , c , c , c and c (Section 1.1.4.10.4). 11 33 12 13 44 66 vibration vectors (or polarization vectors). However, if the latter (i) The wavevector is parallel to [001]. The Christoffel deterare parallel to certain symmetry directions in the crystal, one of minant reduces to the vibration vectors is along this direction. The corresponding wave is called longitudinal. The two other waves have their polarization direction perpendicular to the wavevector and are thus transverse. If one of the polarization vectors is almost Table 1.3.4.1. Velocity of propagation when the wavevector is parallel to [100] parallel to the wavevector, which often happens, then one speaks (cubic crystals) of the vibration as being quasi-longitudinal. Velocity of propagation Polarization vector Nature of the wave pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ c11 = pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c44 = pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c44 = k ¼

1.3.4.5. Relation between velocity of propagation and elastic stiffnesses We shall limit ourselves to cubic, hexagonal and tetragonal crystals and consider particular cases.

[100]

Longitudinal

[010]

Transverse

Any vector normal to [100]

Transverse

Table 1.3.4.2. Velocity of propagation when the wavevector is parallel to [110] (cubic crystals)

1.3.4.5.1. Cubic crystals (i) The wavevector is parallel to [100]. The Christoffel determinant reduces to 0 1 c11 2 0 0 @ A ¼ 0: 0 c44 2 0 2 0 0 c44

Velocity of propagation pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ k ¼ ½c44 þ 12 ðc11 þ c12 Þ= pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ 12 ðc11 c12 Þ= pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c44 =

Polarization vector

Nature of the wave

[110] ½110

Longitudinal Transverse

[001]

Transverse

Table 1.3.4.3. Velocity of propagation when the wavevector is parallel to [111] (cubic crystals)

The three solutions are given in Table 1.3.4.1. These results are valid for a wave propagating in any direction in an isotropic medium. (ii) The wavevector ispparallel ﬃﬃﬃ pﬃﬃﬃto [110]. The direction cosines of the wavevector are 1= 2, 1= 2, 0. The Christoffel determinant assumes the form 01 1 2 1 0 2 ðc11 þ c44 Þ 2 ðc12 þ c44 Þ 1 2 @ 1 ðc12 þ c44 Þ A ¼ 0: 0 2 2 ðc11 þ c44 Þ 2 0 0 c44

Velocity of propagation pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ k ¼ ðc11 þ 2c12 þ 4c44 Þ=3 pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ ðc11 c12 þ c44 Þ=3

Polarization vector

Nature of the wave

[111]

Longitudinal

Any vector normal to [111]

Transverse

Table 1.3.4.4. Velocity of propagation when the wavevector is parallel to [001] (hexagonal crystals) Velocity of propagation pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ k ¼ c33 Þ= pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c44 =

The three solutions are given in Table 1.3.4.2. (iii) The wavevector is parallel to [111]. The Christoffel determinant assumes the form 0 1 c11 þ 2c44 2 c12 þ c44 c12 þ c44 @ c12 þ c44 c11 þ 2c44 Þ 2 c12 þ c44 A ¼ 0: c12 þ c44 c12 þ c44 c44 2

Polarization vector

Nature of the wave

[100]

Longitudinal

Any vector normal to [001]

Transverse

Table 1.3.4.5. Velocity of propagation when the wavevector is parallel to [100] (hexagonal crystals) Velocity of propagation pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ k ¼ c11 = pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c66 = pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c44 =

The solutions are given in Table 1.3.4.3.

Polarization vector

Nature of the wave

[100]

Longitudinal

[010] [001]

Transverse Transverse

Table 1.3.4.6. Velocity of propagation when the wavevector is parallel to [001] (tetragonal crystals)

1.3.4.5.2. Hexagonal crystals In hexagonal crystals, there are ﬁve independent elastic stiffnesses, c11 , c33 , c12 , c13 , c44 and c66 ¼ ðc11 c12 Þ=2 (Section 1.1.4.10.4). (i) The wavevector is parallel to [001]. The Christoffel determinant reduces to 0 1 c44 2 0 0 @ A ¼ 0: 0 c44 2 0 2 0 0 c33

Velocity of propagation pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ k ¼ c33 = pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c44 = pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c44 =

Polarization vector

Nature of the wave

[100]

Longitudinal

[010] [001]

Transverse Transverse

Table 1.3.4.7. Velocity of propagation when the wavevector is parallel to [100] (tetragonal crystals) Velocity of propagation pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ k ¼ c11 = pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c66 = pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ? ¼ c44 =

The solutions are given in Table 1.3.4.4. (ii) The wavevector is parallel to [100]. The Christoffel determinant readily reduces to

87

Polarization vector

Nature of the wave

[100] [010]

Longitudinal Transverse

[001]

Transverse

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1 c44 0 0 (ii) Frequency dependence of the elastic constants. Dynamic @ A ¼ 0: measurements of the elastic constants can be performed at a wide 0 c44 2 0 range of ultrasonic frequencies. Currently used techniques for 0 0 c33 2 investigating a wide range of frequencies are electronic pulseecho techniques in the megahertz frequency range and Brillouin The three solutions are given in Table 1.3.4.6. scattering in the 10 GHz frequency range. To evaluate the (ii) The wavevector is parallel to [100]. The Christoffel deterpossible differences between dynamic elastic constants determinant reduces to mined in different frequency ranges, high-accuracy measure0 1 2 ments of the absolute value of the elastic constants are required. 0 0 c11 From optical resonance techniques in the megahertz frequency 2 2 @ A ¼ 0: 0 0 c66 range and Brillouin scattering in the gigahertz frequency range, it 2 2 0 0 c44 has been shown that the results are the same within 0.1 to 0.2% in the case of simple and stable crystals such as sodium chloride The three solutions are given in Table 1.3.4.7. when the ultrasonic waves can be considered as a ‘passive probe’ (Michard et al., 1971). Larger differences are observed when ultrasonic waves interact with the medium, when they favour or 1.3.4.6. Experimental determination of elastic constants impede structural changes of the material or when they are absorbed for a particular frequency. 1.3.4.6.1. Introduction (iii) Phase velocity and group velocity. When the velocity of As mentioned in Section 1.3.4.1, the elastic constants of a ultrasonic waves is frequency dependent (dispersive medium), material can be obtained by the elastic response of the material to one has to distinguish phase velocity and group velocity. If a particular static forces; however, such measurements are not resonance technique is used, the resonance frequencies correprecise and the most often used approach nowadays consists of determining the velocity of ultrasonic waves propagating along spond to phase-matching conditions and the calculation of different directions of the crystal and calculating the elastic velocity from the resonance frequencies leads to ‘phase velocity’. constants from the Christoffel determinants (1.3.4.8). The If a pulse-echo technique is used, the transit time of an elastic experimental values are often accurate enough to justify the pulse is measured and the interpretation of the measurement is distinction between static and dynamic values of the elastic more complex. In this case, Brillouin (1932) has shown that the constants and between phase and group velocities, and the head and the tail of the pulse travel with the group velocity. careful consideration of the frequency range of the experiments. Differences of a few per cent can be observed between phase and (i) Static and dynamic elastic constants. When one measures the group velocities in dispersive media. elastic response of a material to external static forces, work is done and heat is produced. In general, the external forces are 1.3.4.6.2. Resonance technique applied slowly (quasi-elastic processes) and the solid body The use of the resonance technique is a well established remains in thermal equilibrium with its surroundings, which can be considered as a heat reservoir. In this case, the measured approach for determining the velocity of sound in a gas by elastic constants are isothermal elastic constants as deﬁned in observing nodes and antinodes of a system of standing waves Section 1.1.5.1. On the contrary, when ultrasonic waves propagate produced in the so-called Kund tube. In the case of transparent in a solid body, the compressed regions are slightly hotter than solids, optical means allow us to visualize the standing waves and the expanded regions; the associated temperature gradients give to measure the wavelength directly (Zarembowitch, 1965). An rise to irreversible processes of thermal conduction. However, in easier procedure can be used: let us consider a transparent crystal the megahertz or higher-frequency ranges, the processes of heat in the shape of a parallelepiped (Fig. 1.3.4.1). A piezoelectric exchange between different regions or between the solid and its transducer is glued to the crystal and excited at varying surroundings are slow compared with the period of the ultrasonic frequencies. If the bonding between the transducer and the wave and hence can be considered as isentropic. In this case, the crystal is loose enough, the crystal can be considered as free from measured velocities are isentropic and the elastic stiffnesses stress and the sequence of its resonance frequencies is given by deduced from them are the adiabatic elastic stiffnesses as deﬁned ¼ nV=2l; in Section 1.1.5.4. The differences between isothermal and adiabatic elastic stiffnesses can be calculated from equation (1.1.5.2): where n is an integer, V the phase velocity of the wave in the direction orthogonal to the parallel faces and l the distance Tij ¼ ðcijkl Þ Skl ij between these faces. CS The looseness of the bonding can be checked by the regularity : ¼ kl Skl þ of the arithmetic ratio, V=2l. On account of the elasto-optic coupling, a phase grating is associated with the elastic standingBy combining these two equations, it is possible to obtain wave system and a light beam can be diffracted by this grating. relations between the isothermal elastic stiffnesses, ðcijkl Þ , and The intensity of the diffraction pattern is maximum when resonance occurs. A large number of resonance frequencies can be the adiabatic elastic stiffnesses, ðcijkl Þ : detected, usually more than 100, sometimes 1000 for nonij kl attenuating materials. Consequently, in favourable cases the ; ðcijkl Þ ¼ ðcijkl Þ þ absolute value of the ultrasonic velocity can be determined with cS an uncertainty less than 103 . S where c is the speciﬁc heat at constant strain. This relation shows that adiabatic elastic stiffnesses are larger 1.3.4.6.3. Pulse-echo techniques than isothermal elastic stiffnesses, at least for the terms of the Pulse-echo techniques are valid for transparent and opaque main diagonal of the elastic matrix. In general, the differences between isothermal and adiabatic elastic stiffnesses are less than materials. They are currently used for measuring ultrasonic 1%. An exception to this statement concerns the temperature velocities in solids and can be used in very simple as well as in region near the critical temperature Tc where a phase transition sophisticated versions according to the required precision (McSkimmin, 1964). In the simplest version (Fig. 1.3.4.2), an occurs. 0

2

88

1.3. ELASTIC PROPERTIES is used to control the pulse repetition rate. When the repetition rate is adjusted so that the initiation of a pulse coincides with the return of the ﬁrst echo from the preceding pulses, the change in the signal amplitude indicates superposition. The pulse rate is a measure of the travel time within the specimen. (ii) ‘Sing around method’. The ‘sing around’ method for measuring the velocity of ultrasonic waves involves the use of two piezoelectric transducers, one at each end of the specimen. One transducer receives an impulse from the electronic generator and converts it into an ultrasonic pulse in the specimen. This pulse, after passing through the specimen, is detected by the receiving transducer. The received pulse triggers the electronic generator to initiate a succeeding pulse. The pulse repetition rate is a very sensitive probe for measuring changes of the ultrasonic velocity in the specimen. Relative variations of 107 can be measured, such as temperature or stress dependences of the velocity.

1.3.5. Pressure dependence and temperature dependence of the elastic constants 1.3.5.1. Introduction

Fig. 1.3.4.1. Resonance technique: standing waves excited in a parallelepiped.

In a solid, the elastic constants are temperature and pressure dependent. As examples, the temperature dependence of the elastic stiffnesses of an aluminium single crystal within its stability domain (the melting point is 933 K) and the pressure dependence of the elastic stiffnesses of the ternary compound KZnF3 within its stability domain (the crystal becomes unstable for a hydrostatic pressure of about 20 GPa) are shown in Figs. 1.3.5.1 and 1.3.5.2, respectively. We can observe the following trends, which are general for stable crystals: (i) From 0 K to about D =5, where D is the Debye temperature, the elastic stiffnesses decrease according to a 4 law. From D =5 to the beginning of the instability domain, the dependence is linear with . In addition, ð@cii [email protected]Þp ¼ 0 at 0 K as predicted by the third principle of thermodynamics. (ii) For stable crystals, the pressure dependence of the elastic stiffnesses is linear as long as the applied pressure is small compared to the elastic stiffnesses. As an example, a typical order of magnitude for c11 in crystals is about 100 GPa and, within the experimental uncertainty, the pressure dependence of c11 does not depart from a linear behaviour up to at least 0.2 GPa. These observations can be quantitatively justiﬁed on the basis of an equation of state of a solid:

electronic pulse generator excites the mechanical vibrations of a piezo-electric transducer glued to one of two plane-parallel faces of a specimen. An ultrasonic pulse whose duration is of the order of a microsecond is generated and transmitted through the specimen. After reﬂection at the opposite face, it returns and, when it arrives back at the transducer, it gives rise to an electronic signal, or echo. The whole sequence of such echos is displayed on the screen of an oscilloscope and it is possible to measure from them the time interval for transit. Usually, X-cut quartz crystals or ferroelectric ceramics are used to excite longitudinal waves and Y-cut quartz is used to excite transverse waves. In many cases, a circulator, or gate, is used to protect the receiver from saturation following the main ‘bang’. This method is rough because the beginning and the end of a pulse are not well characterized. Several improvements have therefore been made, mainly based on interferometric techniques (pulse-superposition method, ‘sing around’ method etc.). Nevertheless, if the absolute value of the ultrasonic velocity is not determined with a high accuracy by using pulse-echo techniques, this approach has proved valuable when relative values of ultrasonic velocities are needed, e.g. temperature and pressure dependences of ultrasonic velocities. (i) Pulse-superposition method. A piezoelectric transducer initiates ultrasonic pulses in the specimen. These pulses echo back and forth within the specimen. A continuous-wave oscillator

f ðTij ; Sij ; X; Þ ¼ 0;

Fig. 1.3.4.2. Block diagram of the pulse-echo technique.

89

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.3.5.2. Pressure dependence of the elastic stiffness c11 of a KZnF3 crystal. Reproduced with permission from Ultrasonics Symposium Proc. IEEE (Fischer et al., 1980). Copyright (1980) IEEE.

(c) In the Gru¨neisen model, the frequencies of the oscillators are volume-dependent; this so-called ‘quasiharmonic approximation’ can justify the standard behaviour shown in Figs. 1.3.5.1 and 1.3.5.2. 1.3.5.2. Temperature dependence of the elastic constants Table 1.3.5.1 gives typical values of ð@ ln cij [email protected]Þp for some cubic crystals considered within their stability domain. In column 6, the ‘elastic Debye temperature’ of the crystal, ðD Þel , has been calculated according to the formula

Fig. 1.3.5.1. Temperature dependence of the elastic stiffnesses of an aluminium single crystal (after Every & McCurdy, 1992).

where Tij represents the stress tensor, Sij the strain tensor, X the position of the elementary elements of the solid and the temperature. Different equations of state of solids have been proposed. They correspond to different degrees of approximation that can only be discussed and understood in a microscopic theory of lattice dynamics. The different steps in the development of lattice dynamics, the Einstein model, the Debye model and the Gru¨neisen model, will be presented in Section 2.1.2.7. Concerning the temperature and the pressure dependences of the elastic constants, we may notice that rather sophisticated models are needed to describe correctly the general trends mentioned above: (a) In the Einstein model, where the N atoms of a crystal are considered as 3N independent harmonic oscillators, the temperature increase affects only the amplitude of the oscillations and not the average positions of the atoms; consequently, this model can explain neither the thermal expansion nor the temperature dependence of the elastic constants. In addition, this theory ignores the difference between isothermal and adiabatic elastic constants. Similarly, if the oscillators are harmonic, the stiffness of the ‘springs’ connecting atoms does not depend on the distances between atoms and the model cannot therefore explain the pressure dependence of the elastic constants, which requires anharmonic ‘springs’ or, more accurately, anharmonic potentials. (b) In the Debye model, the 3N oscillators are not independent but they are still harmonic. The result is that here again the elastic constants are pressure and temperature independent.

ðD Þel ¼ hv=kB ð3n=4 Þ1=3 ;

where h is the Planck constant, kB is the Boltzmann constant, v is an average velocity (see for instance De Launay, 1956) and n is the number of atoms per unit volume. It is interesting to compare ðD Þel, the ‘elastic Debye temperature’, with ðD Þcal , the ‘calorimetric Debye temperature’. The deﬁnition of ðD Þcal will be given in Section 2.1.2.7. It results from the attempt at founding a universal description for the thermal properties of solids when the temperature is expressed as a reduced temperature, =ðD Þcal ; ðD Þcal is obtained from calorimetric measurements at low temperature. It is worth noting that accurate values of low-temperature elastic constants and low-temperature calorimetric measurements lead to an excellent agreement between ðD Þel and ðD Þcal [better than 2 or 3 K (De Launay, 1956)]. This agreement demonstrates the validity of the Debye model in the vicinity of 0 K. From Table 1.3.5.1, we can observe that for ionic crystals ð@ ln c11 [email protected]Þp is, in general, greater than ð@ ln c44 [email protected]Þp . This remark is not valid for covalent and metallic crystals. Typical orders of magnitude are given in Table 1.3.5.2. These statements concern only general trends valid for stable crystals. In the case of temperature-induced phase transitions, some elastic constants are softened in the vicinity and sometimes far from the critical temperature. As an example, Fig. 1.3.5.3 shows the temperature dependence of c44 in RbCdF3, CsCdF3 and TlCdF3 single crystals. RbCdF3 and TlCdF3 Table 1.3.5.1. Temperature dependence of the elastic stiffnesses for some cubic crystals undergo structural phase transitions at 124 and 191 K, respectively, while CsCdF3 remains stable in this Temperature ð@ ln c11 [email protected]Þp ð@ ln c44 [email protected]Þp ð@ ln c12 [email protected]Þp el temperature range. The softening of c44 when the Material range (K) (104 K1) (104 K1) (104 K1) (K) temperature decreases starts more than 100 K before the Al 80–300 3.1 4.45 1.3 430 critical temperature, c . In contrast, Fig. 1.3.5.4 shows the Cu 80–300 2.01 3.33 1.24 344 Ag 50–300 2.3 4.0 1.5 226 temperature dependence of c11 in KNiF3, a crystal that Pb 100–300 4.4 1.5 2.8 105 undergoes a para–antiferromagnetic phase transition at Si 80–300 0.81 10.6 1.10 648 246 K; the coupling between the elastic and the magnetic Ge 150–1000 1.2 1.15 1.10 374 energy is weak, consequently c11 decreases abruptly only a ZnS 100–300 1.2 0.65 0.8 347 NaCl 100–300 7.8 2.2 4.7 321 few degrees before the critical temperature. We can KCl 80–300 8.3 2.1 3.6 236 generalize this observation and state that the softening of KBr 80–300 7.6 2.1 7 172 an elastic constant occurs over a large domain of

90

1.3. ELASTIC PROPERTIES

Fig. 1.3.5.5. Temperature dependence of ðc11 c12 Þ=2 in DyVO4, which undergoes a cooperative Jahn–Teller phase transition (after Melcher & Scott, 1972). Fig. 1.3.5.3. Temperature dependence of the elastic constant c44 in RbCdF3, CsCdF3 and TlCdF3 crystals; the crystals of RbCdF3 and TlCdF3 undergo structural phase transitions (after Rousseau et al., 1975).

their experimental determination since they are a unique source of signiﬁcant information in many ﬁelds: (i) In geophysics, a large part of the knowledge we have on the interior of the earth comes from the measurement of the transit time of elastic bursts propagating in the mantle and in the core (in the upper mantle, the average pressure is estimated to be about a few hundred GPa, a value which is comparable to that of the elastic stiffnesses of many materials). (ii) In solid-state physics, the pressure dependence of the elastic constants gives signiﬁcant indications concerning the stability of crystals. For example, Fig. 1.3.5.2 shows the pressure dependence of the elastic constants of KZnF3, a cubic crystal belonging to the perovskite family. As mentioned previously, this crystal is known to be stable over a wide range of temperature and the elastic stiffnesses cij depend linearly on pressure. It may be noted that, consequently, the third-order elastic constants (TOECs) are constant. On the contrary, we observe in Fig. 1.3.5.6 that the pressure dependence of the elastic constants of TlCdF3, a cubic crystal belonging to the same family but which is known to become unstable when the temperature is decreased to 191 K (Fischer, 1982), is nonlinear even at low pressures. In this case, the development of the strain-energy density in terms of strains cannot be stopped after the terms containing the third-order elastic constants; the contributions of the fourth- and ﬁfth-order elastic constants are not negligible. (iii) For practical use in the case of technical materials such as concrete or worked metals, the pressure dependence of the elastic moduli is also required for examining the effect of applied stresses or of an applied hydrostatic pressure, and for studying residual stresses resulting from loading (heating) and unloading (cooling) the materials.

Fig. 1.3.5.4. Temperature dependence of the elastic constant c11 in KNiF3, which undergoes a para–antiferromagnetic phase transition. Reprinted with permission from Appl. Phys. Lett. (Nouet et al., 1972). Copyright (1972) American Institute of Physics.

temperature when this constant is the order parameter or is strongly coupled to the order parameter of the transformation; for instance, in the cooperative Jahn–Teller phase transition in DyVO4, ðc11 c12 Þ=2 is the soft acoustic phonon mode leading to the phase transition and this parameter anticipates the phase transition 300 K before it occurs (Fig. 1.3.5.5). 1.3.5.3. Pressure dependence of the elastic constants As mentioned above, anharmonic potentials are needed to explain the stress dependence of the elastic constants of a crystal. Thus, if the strain-energy density is developed in a polynomial in terms of the strain, only the ﬁrst and the second elastic constants are used in linear elasticity (harmonic potentials), whereas higher-order elastic constants are also needed for nonlinear elasticity (anharmonic potentials). Concerning the pressure dependence of the elastic constants (nonlinear elastic effect), considerable attention has been paid to

Table 1.3.5.2. Order of magnitude of the temperature dependence of the elastic stiffnesses for different types of crystals Type of crystal Ionic Covalent Metallic

ð@ ln c11 [email protected]Þp (K1) 3

10 104 2 104

ð@ ln c44 [email protected]Þp (K1) 3 104 8 105 3 104

Fig. 1.3.5.6. Pressure dependence of the elastic constants ðc11 c12 Þ=2 in TlCdF3. Reproduced with permission from Ultrasonics Symposium Proc. IEEE (Fischer et al., 1980). Copyright (1980) IEEE.

91

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES xi ¼ xi ða1 ; a2 ; a3 Þ; 1.3.6. Nonlinear elasticity 1.3.6.1. Introduction In a solid body, the relation between the stress tensor T and the strain tensor S is usually described by Hooke’s law, which postulates linear relations between the components of T and S (Section 1.3.3.1). Such relations can be summarized by (see equation 1.3.3.2)

where the ai are the independent variables. It follows that @xj @uj dai ¼ þ ij dai : ð1:3:6:6Þ dxj ¼ @ai @ai Let now the particle initially at (a1 , a2 , a3 ) move to (x1 , x2 , x3 ). The square of the initial distance to a neighbouring particle whose initial coordinates were aj þ daj is

Tij ¼ cijkl Skl ;

ds2 ¼ daj daj :

where the cijkl ’s are the elastic stiffnesses. For a solid under ﬁnite strain conditions, Hooke’s law, valid for inﬁnitesimal deformations, does not hold, and the fundamental deﬁnitions for stress and strain must be revisited.

The square of the ﬁnal distance to the same neighbouring particle is ds2 ¼ dxj dxj :

1.3.6.2. Lagrangian and Eulerian descriptions Finite elastic strains may be treated from two different viewpoints using either the Lagrangian (material) or the Eulerian (spatial) descriptions. Let us consider a ﬁxed rectangular Cartesian coordinate system with axes xi (i ¼ 1; 2; 3). Any particular position vector r of components (x1 , x2 , x3 ) denotes a point in space. A point that always moves with the material is called a particle or material point. Let every particle be identiﬁed by its coordinates at some reference time t0. These reference coordinates, referred to the same Cartesian system, will be denoted by (a1 , a2 , a3 ) and the corresponding position vector a. A particular vector a can serve as a name for the particle located at that position at the reference time t0. The vectors r and a both specify a position in a ﬁxed Cartesian frame of reference. At any time, we associate each r with an a by the rule that r is the present position vector of the particle initially at a. This connection between r and a is written symbolically as r ¼ rðt; aÞ

or

xi ¼ xi ðt; a1 ; a2 ; a3 Þ;

ð1:3:6:1Þ

a ¼ rðt0 ; aÞ

or

ai ¼ xi ðt0 ; a1 ; a2 ; a3 Þ:

ð1:3:6:2Þ

In a material description, the strain components Sik are deﬁned by the following equations: dxj dxj daj daj ¼ 2Sik dai dak :

Substituting (1.3.6.6) into (1.3.6.7), it follows that @uj @uj þ ji þ jk dai dak daj daj ¼ 2Sik dai dak : @ai @ak Hence

ai ¼ ai ðt; x1 ; x2 ; x3 Þ;

ð1:3:6:3Þ

r ¼ aðt0 ; rÞ

or

xi ¼ ai ðt0 ; x1 ; x2 ; x3 Þ:

ð1:3:6:4Þ

@uk @ui @uj @uj : þ þ @ai @ak @ai @ak

It is often useful to introduce the Jacobian matrix associated with the transformation (a, x). The components of this matrix are 0 1 11 12 13 J ¼ @ 21 22 23 A; 31 32 33 where ik ¼

where

@uj @xi ¼ þ jk : @ak @ak

From the deﬁnition of matrix J, one has dx ¼ Jda

A spatial description or Eulerian description uses the independent variables (t, x1 , x2 , x3 ), the xi being called spatial coordinates. Now, for the sake of simplicity, we shall work with the Lagrangian formulation exclusively. For more details see, for instance, Thurston (1964) and Wallace (1970, 1972).

and

dx2 da2 ¼ ðdxÞT dx ðdaÞT da ¼ ðdaÞT J T J da;

where ðdaÞT , ðdxÞT and J T are the transpose matrices of da, dx and J, respectively, and is the Kronecker matrix. The Lagrangian strain matrix S may then be written symbolically:

1.3.6.3. Strain and stress tensors The displacement vector from the reference position of a particle to its new position has as components ui ¼ xi ai :

1 2

If the products and squares of the displacement derivatives are neglected, the strain components reduce to the usual form of ‘inﬁnitesimal elasticity’ [see equation (1.3.1.8)]: @ui @uk : þ Sik ¼ 12 @ak @ai

The coordinates ai that identify the particles are called material coordinates. A description that, like (1.3.6.1), uses (t, a1 , a2 , a3 ) as independent variables is called a material or Lagrangian description. The converse of (1.3.6.1) and (1.3.6.2) may be written or

Sik ¼

where

a ¼ aðt; rÞ

ð1:3:6:7Þ

S ¼ 12 ð J T J Þ:

ð1:3:6:8Þ

ð1:3:6:5Þ When ﬁnite strains are concerned, we have to distinguish three states of the medium: the natural state, the initial state and the ﬁnal or present state: The natural state is a state free of stress. The initial state is deduced from the natural state by a homogeneous strain. The ﬁnal state is deduced from the initial state by an arbitrary strain.

The term strain refers to a change in the relative positions of the material points in a body. Let a ﬁnal conﬁguration be described in terms of the reference conﬁguration by setting t equal to a constant in (1.3.6.1). Then t no longer appears as a variable and (1.3.6.1) can be written

92

1.3. ELASTIC PROPERTIES Concerning the stress tensor, as pointed out by Thurston (1964), the stress-deformation relation is complicated in nonlinear elasticity because ‘the strain is often referred to a natural unstressed state, whereas the stress Tij is deﬁned per unit area of the deformed body’. For this reason, the differential of work done by the stress is not equal to the stress components times the differentials of the corresponding strain components. So, following Truesdell & Toupin (1960), we shall introduce a thermodynamic tension tensor tij deﬁned as the ﬁrst derivative of the energy with respect to strain. If the internal energy U per unit mass is considered, the thermodynamic tension refers to an isentropic process. Then @U tij ¼ 0 ; @Sij

Table 1.3.6.1. Number of independent third-order elastic stiffnesses for each Laue class

Laue class 1 1, 2/m, 2, m mmm, 222, 2mm 3 3, 32, 3m 3, 4/m, 4, 4 4/mmm, 422, 42m, 42m 6/m, 6, 6 6/mmm, 622, 62m, 62m 23 m3, 432, 432 m3m, 1ðA1 =MÞC, 1A1

where is the entropy and 0 the volumic mass in the initial state. If the Helmholtz free energy F is considered, the thermodynamic tension refers to an isothermal process. Then @U tij ¼ 0 ; @Sij

Tij ¼ ð1=JÞik jl tkl : 1.3.6.4. Second-order and higher-order elastic stiffnesses Following Brugger (1964), the strain-energy density, or strain energy per unit volume , is assumed to be a polynomial in the strain: 1 1 c SS þ c SS S ; 2! ijkl ij kl 3! ijklmn ij kl mn

l ¼ 12 c112 ; m ¼ c155 ; n ¼ 4c456 : Similarly, the fourth-order stiffnesses form an eighth-rank tensor containing 38 ¼ 6561 components, 126 of which are independent for a triclinic crystal and 11 for isotropic materials (the independent components of a sixth-rank tensor can be obtained for any point group using the accompanying software to this volume). For a solid under ﬁnite strain conditions, the deﬁnition of the elastic compliance tensor has to be reconsidered. In linear elasticity, the second-order elastic compliances sijkl were deﬁned through the relations (1.3.3.2):

ð1:3:6:9Þ

where ¼ 0 UðX; Sij Þ, 0 ¼ 0 UðX; 0Þ, X denotes the conﬁguration of the initial state and the Sij ’s are the Lagrangian ﬁnite strain-tensor components. If the initial energy and the deformation of the body are both zero, the ﬁrst two terms in (1.3.6.9) are zero. Note that cij is a stress and not an intrinsic characteristic of the material. In this expression, the elastic stiffnesses cijkl and cijklmn are the secondand third-order stiffnesses, respectively. Since the strain tensor is symmetric, pairs of subscripts can be interchanged [see equation (1.3.3.4)]:

Sij ¼ sijkl Tkl

cijklmn ¼ cjiklmn ¼ cijlkmn ¼ cjilkmn ¼ cijklnm

sijkl ¼

¼ cjiklnm ¼ cijlknm ¼ cjilknm :

sijkl ¼

@Sij ; @Tkl

@Sij ; @tkl

where

More accurately, the isentropic and the isothermal elastic stiffnesses are deﬁned as the nth partial derivatives of the internal energy and the Helmholtz free energy, respectively. For example, the third-order isentropic and isothermal stiffnesses are, respectively,

tkl ¼ 0

@U : @Skl

1.3.6.5. Expansion of elastic constants for small initial stress

@3 U ; @Sij @Skl @Smn

In most experiments, the initial stress is small compared with the second-order elastic constants (for example, 1 GPa hydrostatic pressure compared with the usual value cijkl = 100 GPa). Consequently, the deformation between the initial (stressed) state and the natural (unstressed) state is small compared with 1. For this reason, it is convenient to expand the elastic constants in the initial state as a power series in the strain about the natural state. To avoid confusion, we introduce new notations: X now represents the coordinates in the natural or unstressed state; X represents the coordinates in the initial or homogeneously

3

c ijklmn ¼ 0

or

while, in nonlinear elasticity, one has

cijkl ¼ cjikl ¼ cijlk ¼ cjilk ;

cijklmn ¼ 0

56 32 20 20 14 16 12 12 10 8 6 3

The third-order stiffnesses form a sixth-rank tensor containing 36 = 729 components, of which 56 are independent for a triclinic crystal and 3 for isotropic materials. The independent components of a sixth-rank tensor can be obtained for any point group using the accompanying software to this volume. They are listed in Table 1.3.6.1 for each Laue class. They can be reduced to threeindex coefﬁcients. Table 1.3.6.2 gives the values of the third-order stiffnesses of some materials. The three independent constants for isotropic materials are often taken as c123, c144 and c456 and denoted respectively by 1, 2 , 3 , the ‘third-order Lame´ constants’. The ‘third-order Murnaghan constants’ (Murnaghan, 1951), denoted by l; m; n, are given in terms of the Brugger constants by the relations

where is the temperature. It will be shown in Section 1.3.7.2 that

¼ 0 þ cij Sij þ

Number of independent components

@F ; @Sij @Skl @Smn

where the internal energy, U, is a function of X, Sij and , and the Helmholtz free energy, F, is a function of X, Sij and . From these deﬁnitions, it follows that the Brugger stiffness coefﬁcients depend on the initial state. When no additional information is given, the initial state is the natural state.

93

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.3.6.2. Third-order elastic stiffnesses of some materials in (GPa)1 (after Every & McCurdy, 1992) (a) Trigonal. Material

c111

c112

c113

c114

c123

c124

c133

c134

c144

c155

c222

c333

c344

c444

Al2O3 CaCO3

3870 579

1090 147

963 193

55 218

289 41

39 10

922 239

131 82

302 69

1160 139

4520 675

3340 498

1090 195

19 33

(b) Tetragonal. Material

c111

c112

c113

c123

c133

c144

c155

c166

c333

c344

c366

c456

KH2PO4 TeO2

538 160

291 600

259 140

258 110

67 180

8 41

35 36

30 640

912 2110

27 54

19 260

8 250

Material

c111

c112

c113

c123

c133

c144

c155

c222

c333

c344

Cd CdS Co Mg Zn

2060 459 6710 663 1760

114 207 1454 178 440

197 182 766 30 270

110 235 429 76 210

268 306 511 86 350

227 27 133 30 10

332 9 1486 58 250

2020 355 5788 864 2410

516 327 6347 726 720

171 69 210 193 440

Material

c111

c112

c123

c144

c155

c456

LiF MgO KBr KCl NaCl Diamond GaAs Ge Si ZnSe Al Cu Au Fe Ni

1920 4900 532 610 866 6260 620 714 795 827 1224 1271 1730 2705 2104

330 95 49 31 37 2260 392 388 445 136 373 814 922 626 1345

40 69 69 9 38 112 62 34 75 511 25 50 233 575 59

100 113 22 19 25 674 8 9 15 222 64 3 13 836 180

325 659 28 35 78 2860 274 303 310 265 368 780 648 531 757

43 147 35 17 18 823 43 48 86 278 27 95 12 721 42

(c) Hexagonal.

(d) Cubic.

strained state; ui ¼ xi Xi are the components of displacement. All letters with superscript bar refer to the natural state; for example, S ij denotes the Lagrangian strain in the natural ¼ UðX; S ij Þ. state; U we Now, in order to relate the properties at X to those at X, need to specify the strain from X to X. Let aij ¼

1.3.6.6. Elastic strain-energy density The elastic strain-energy density has appeared in the literature in various forms. Most of the authors use the Murnaghan constants as long as isotropic solids are concerned. However, most of the literature uses Brugger’s thermodynamic deﬁnition when anisotropic media are under consideration (Brugger, 1964). The elastic strain-energy density for an isotropic medium, including third-order terms but omitting terms independent of strain, may be expressed in terms of three strain invariants, since an isotropic material is invariant with respect to rotation:

@Xi ¼ ij : @X j

Consequently, ¼ @S ij ¼ ami anj : @Smn

where and are the second-order Lame´ constants, l; m; n are the third-order Murnaghan constants, and I1 , I2 , I3 are the three invariants of the Lagrangian strain matrix. These invariants may be written in terms of the strain components as

The second-order elastic constants at X can be expressed in terms of the second- and third-order elastic constants at X: cijkl ¼ 0

I1 ¼ S11 þ S22 þ S33 S11 S12 S22 þ I2 ¼ S21 S22 S32 S11 S12 S13 I3 ¼ S21 S22 S23 : S S S

@2 U @2 U ¼ 0 aim ajn akp alq @Sij @Skl @Smn @S pq

or cijkl

þ 2 l þ 2m ðI1 Þ2 2 I2 þ ðI1 Þ3 2mI1 I2 þ nI3 ; 2 3

0 1 ¼ c þ c mnpqrs Srs þ c mnpqrstu Srs Stu þ aim ajn akp alq : 2! 0 mnpq

31

32

S23 S33 þ S33 S13

S31 S11

33

The elastic strain-energy density for an anisotropic medium (for example a medium belonging to the most symmetrical groups of cubic crystals) is (Green, 1973)

This expression holds for both isentropic and isothermal elastic constants.

94

¼

1 2 c11

1.3. ELASTIC PROPERTIES 2 2 2 which can be written ðS11 Þ þ ðS22 Þ þ ðS33 Þ þ c12 S11 S22 þ S22 S33 þ S33 S11

þ c44 ½ðS12 Þ2 þ ðS21 Þ2 þ ðS23 Þ2 þ ðS32 Þ2 þ ðS31 Þ2 þ ðS13 Þ2 þ c111 ðS11 Þ3 þ ðS22 Þ3 þ ðS33 Þ3 þ c112 ðS11 Þ2 ðS22 þ S33 Þ þ ðS22 Þ2 ðS33 þ S11 Þ þ ðS33 Þ2 ðS11 þ S22 Þ

þ 12 c144 S11 ½ðS23 Þ2 þ ðS32 Þ2 þ S22 ½ðS31 Þ2 þ ðS13 Þ2 þ S33 ½ðS12 Þ2 þ ðS21 Þ2

þ 12 c166 ðS12 Þ2 þ ðS21 Þ2 ðS11 þ S22 Þ þ ðS23 Þ2 þ ðS32 Þ2 ðS22 þ S33 Þ þ ðS13 Þ2 þ ðS31 Þ2 ðS11 þ S33 Þ þ c123 S11 S22 S33 þ c456 S12 S23 S31 þ S21 S32 S13 :

2

0 x00 i ¼ since

@Slm 1

¼ 2 im jl þ il jm : @ij Using now the equation of continuity or conservation of mass: 0 ¼ J ¼ detðaij Þ; and the identity of Euler, Piola and Jacobi: @ 1 @xj ¼ 0; @xj J @Xi we get an expression of Newton’s law of motion:

1.3.7. Nonlinear dynamic elasticity

x00i ¼

1.3.7.1. Introduction In recent years, the measurements of ultrasonic wave velocities as functions of stresses applied to the sample and the measurements of the amplitude of harmonics generated by the passage of an ultrasonic wave throughout the sample are in current use. These experiments and others, such as the interaction of two ultrasonic waves, are interpreted from the same theoretical basis, namely nonlinear dynamical elasticity. A ﬁrst step in the development of nonlinear dynamical elasticity is the derivation of the general equations of motion for elastic waves propagating in a solid under nonlinear elastic conditions. Then, these equations are restricted to elastic waves propagating either in an isotropic or in a cubic medium. The next step is the examination of two important cases: (i) the generation of harmonics when ﬁnite amplitude ultrasonic waves travel throughout an unstressed medium; (ii) the propagation of small amplitude ultrasonic waves when they travel throughout a stressed medium. Finally, the concept of natural velocity is introduced and the experiments that can be used to determine the third- and higherorder elastic constants are described.

d @L @ @L

¼0 þ 0 dt @xi @Xi @ @xi [email protected]

ð1:3:7:1Þ

d @L @ @L þ ¼ 0; dt @x0i @Xi @ij

ð1:3:7:2Þ

Tij ¼

ð1:3:7:4Þ

0 @U @U ¼ ik jl : @Skl J ik jl @Skl

Tij becomes 1 Tij ¼ ik jl tkl J since tkl ¼ 0

@U : @Skl

tkl , the thermodynamic tensor conjugate to the variable Skl =0, is generally denoted as the ‘second Piola–Kirchoff stress tensor’. Using , the strain energy per unit volume, Newton’s law (1.3.7.4) takes the form @ @ @ @ x00i ¼ jk jk or u00i ¼ @Xj @Sik @Xj @Sik and Tij ¼ jk

@ : @Sik

ð1:3:7:5Þ

1.3.7.3. Wave propagation in a nonlinear elastic medium As an example, let us consider the case of a plane ﬁnite amplitude wave propagating along the x1 axis. The displacement components in this case become

or

u1 ¼ u1 ðX1 ; tÞ;

where L is the Lagrangian per unit initial volume and ij ¼ @xi [email protected] are the elements of the Jacobian matrix. For adiabatic motion 0

dTij dTij or u00i ¼ dXj dXj

with

1.3.7.2. Equation of motion for elastic waves For generality, these equations will be derived in the X conﬁguration (initial state). It is convenient to obtain the equations of motion with the aid of Lagrange’s equations. In the absence of body forces, these equations are

L ¼ 12 0 xi2 0 U;

@ @U il jm 0 @Xj @Slm

u2 ¼ u2 ðX1 ; tÞ;

u3 ¼ u3 ðX1 ; tÞ:

Thus, the Jacobian matrix ij reduces to 0 1 11 0 0 J ¼ @ 21 0 0 A: 31 0 0

ð1:3:7:3Þ

where U is the internal energy per unit mass. Combining (1.3.7.2) and (1.3.7.3), it follows that @ @U @Slm 00 2 0 x i ¼ ; @Xj 0 @Slm @ij

The Lagrangian strain matrix is [equation (1.3.6.8)]

S ¼ 12 J T J : The only nonvanishing strain components are, therefore,

95

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES @2 u1 @u1 @2 u1 1 S11 ¼ þ þ 00 ¼ ð þ 2 Þ þ ½3ð þ 2 Þ þ 2ðl þ 2mÞ u " # 1 2 2 2 2 @X1 @X1 @X12 @u1 1 @u1 @u2 @u3 ¼ þ þ þ @u2 @2 u2 @u3 @2 u3 @X1 2 @X1 @X1 @X1 þ ð þ 2 þ mÞ þ @X1 @X12 @X1 @X12 @u S12 ¼ S21 ¼ 12 2 @2 u2 @u1 @2 u2 @u2 @2 u1 00 @X1 þ u2 ¼ 2 þ ð þ 2 þ mÞ @X1 @X1 @X12 @X1 @X12 @u 3 S13 ¼ S31 ¼ 12 @2 u3 @u1 @2 u3 @u3 @2 u1 00 @X1 u3 ¼ 2 þ ð þ 2 þ mÞ : þ @X1 @X1 @X12 @X1 @X12 ð1:3:7:7Þ and the strain invariants reduce to 1 2

211

221

231

I1 ¼ S11 ; I2 ¼ ðS12 S21 þ S13 S31 Þ; I3 ¼ 0: 1.3.7.3.2. Cubic media (most symmetrical groups) In this case, the strain-energy density becomes ¼ 12 c11 ðS11 Þ2 þ c44 ðS12 Þ2 þ ðS21 Þ2 þ ðS31 Þ2 þ ðS13 Þ2 þ c111 ðS11 Þ3 þ 12 c166 S11 ðS12 Þ2 þ ðS21 Þ2 þ ðS31 Þ2 þ ðS13 Þ2 : ð1:3:7:8Þ

1.3.7.3.1. Isotropic media In this case, the strain-energy density becomes ¼ 12 ð þ 2 ÞðS11 Þ2 þ 2 ðS12 S21 þ S13 S31 Þ þ 13 ðl þ 2mÞðS11 Þ3 þ 2mS11 ðS12 S21 þ S13 S31 Þ:

ð1:3:7:6Þ

Differentiating (1.3.7.8) with respect to the strain, one obtains @ ¼ c11 S11 þ 3c111 ðS11 Þ2 þ 12 c166 ½ðS12 Þ2 þ ðS21 Þ2 S11

Differentiating (1.3.7.6) with respect to the strains, we get

þ ðS31 Þ2 þ ðS13 Þ2 Þ

@ ¼ ð þ 2 ÞS11 þ ðl þ 2mÞðS11 Þ2 þ 2mðS12 S21 þ S13 S31 Þ @S11

@ ¼ 2c44 S21 þ c166 S11 S21 S21

@ ¼ 2 S21 þ 2mS11 S21 @S12

@ ¼ 2c44 S31 þ c166 S11 S31 : S31

@ ¼ 2 S31 þ 2mS11 S31 @S13

All other @=Sij ¼ 0. From (1.3.7.5), we derive the stress components:

@ ¼ 2 S12 þ 2mS11 S12 @S21 @ ¼ 2 S13 þ 2mS11 S13 : @S31 All the other @[email protected] ¼ 0. From (1.3.7.5), we derive the stress components: T11 ¼ 1k

T11 ¼ 1k

@ @S1k

T21 ¼ 1k

@ @S2k

T31 ¼ 1k

@ : @S3k

In this particular case, the three components of the equation of motion are

@ @ @ ; T12 ¼ 2k ; T13 ¼ 3k ; @S1k @S1k @S1k

u001 ¼ dT11 =dX1 u002 ¼ dT21 =dX1

@ @ @ T21 ¼ 1k ; T22 ¼ 2k ; T23 ¼ 3k ; @S2k @S2k @S2k

u003 ¼ dT31 =dX1 :

@ @ @ T31 ¼ 1k ; T32 ¼ 2k ; T33 ¼ 3k : @S3k @S3k @S3k

If we retain only terms up to the quadratic order in the displacement gradients, we obtain the following equations of motion:

Note that this tensor is not symmetric. For the particular problem discussed here, the three components of the equation of motion are

@2 u 1 @u1 @2 u1 þ ½3c þ c 11 111 @X12 @X1 @X12 2 @u2 @ u2 @u3 @2 u3 þ ðc11 þ c166 Þ þ @X1 @X12 @X1 @X12 @2 u 2 @u1 @2 u2 @u2 @2 u1 00 u2 ¼ c44 þ ðc11 þ c166 Þ þ @X12 @X1 @X12 @X1 @X12 @2 u 3 @u1 @2 u3 @u3 @2 u1 00 u3 ¼ c44 þ ðc11 þ c166 Þ þ ; @X12 @X1 @X12 @X1 @X12 u001 ¼ c11

u001 ¼ dT11 =dX1 ; u002 ¼ dT21 =dX1 ; u003 ¼ dT31 =dX1 : If we retain only terms up to the quadratic order in the displacement gradients, we obtain the following equations of motion:

which are identical to (1.3.7.7) if we put

96

ð1:3:7:9Þ

c11 ¼ þ 2 ;

c44 ¼ ;

c111

1.3. ELASTIC PROPERTIES ¼ 2ðl þ 2mÞ; c166 ¼ m: where u00 is the initial value for the particle velocity. 1.3.7.5. Small-amplitude waves in a strained medium We now consider the propagation of small-amplitude elastic waves in a homogeneously strained medium. As deﬁned previously, X or a are the coordinates in the natural or unstressed state. X are the coordinates in the initial or homogeneously strained state. ui ¼ xi Xi are the components of displacement from the initial state due to the wave. Starting from (1.3.7.4), we get

1.3.7.4. Harmonic generation The coordinates in the medium free of stress are denoted The notation X is used when we have to discrieither a or X. from the initial conﬁguration minate the natural conﬁguration, X, X. Here, the process that we describe refers to the propagation of an elastic wave in a medium free of stress (natural state) and the coordinates will be denoted ai . Let us ﬁrst examine the case of a pure longitudinal mode, i.e. u1 ¼ u1 ða1 ; tÞ;

Tij ¼

u2 ¼ u3 ¼ 0:

The equations of motion, (1.3.7.7) and (1.3.7.9), reduce to

Its partial derivative is

@Tij 1 @ @U : ¼ 0 il J @Xk @Skl @xj

@2 u @u @2 u u001 ¼ ð þ 2 Þ 21 þ ½3ð þ 2 Þ þ 2ðl þ 2mÞ 1 21 @a1 @a1 @a1 for an isotropic medium or

If we expand the state function about the initial conﬁguration, it follows that

@2 u @u @2 u u001 ¼ c11 21 þ ½3c11 þ c166 1 21 @a1 @a1 @a1

0 UðXk ; Sij Þ ¼ 0 UðXk Þ þ cij Sij þ 12 cijkl Sij Skl þ 16 cijklmn Sij Skl Smn þ . . . :

for a cubic crystal (most symmetrical groups) when a pure longitudinal mode is propagated along [100]. For both cases, we have a one-dimensional problem; (1.3.7.7) and (1.3.7.9) can therefore be written 2

u001 ¼ K2

The linearized stress derivatives become @2 xk @Tij ¼ cjl ik þ cijkl : @xj @Xj @Xl

2

@ u1 @u @ u þ ½3K2 þ K3 1 21 : 2 @a1 @a1 @a1

0 @U : J ik jl @Skl

ð1:3:7:10Þ

If we let Dijkl ¼ cjl ik þ cijkl , the equation of motion in the initial state is

The same equation is also valid when a pure longitudinal mode is propagated along [110] and [111], with the following correspondence:

0 u00i ¼ Djkli

½100 K2 ¼ c11 ; K3 ¼ c111 c þ c12 þ 2c44 c þ 3c112 þ 12c166 ; K3 ¼ 111 ½110 K2 ¼ 11 2 4 c11 þ 2c12 þ 4c44 ; ½111 K2 ¼ 3 c þ 6c112 þ 12c144 þ 24c166 þ 2c123 þ 16c456 : K3 ¼ 111 9

@2 u k : @Xj @Xl

ð1:3:7:13Þ

The coefﬁcients Dijkl do not present the symmetry of the coefﬁcients cijkl except in the natural state where Dijkl and cijkl are equal. The simplest solutions of the equation of motion are plane waves. We now assume plane sinusoidal waves of the form ui ¼ Ai exp½ið!t k XÞ;

Let us assume that K3 K2 ; a perturbation solution to (1.3.7.10) is

ð1:3:7:14Þ

where k is the wavevector. Substitution of (1.3.7.14) into (1.3.7.13) results in

u ¼ u0 þ u1 ;

0 !2 Aj ¼ Dijkl kj kl Ak

where u1 u0 with

or

u0 ¼ A sinðka !tÞ

ð1:3:7:11Þ

1

u ¼ Ba sin 2ðka !tÞ þ Ca cos 2ðka !tÞ:

0 !2 Aj ¼ jk Ak

ð1:3:7:12Þ with jk ¼ Dijkl kj kl . The quantities 0 !2 Aj and A are, respectively, the eigenvalues and eigenvectors of the matrix jk . Since jk is a real symmetric matrix, the eigenvalues are real and the eigenvectors are orthogonal.

If we substitute the trial solutions into (1.3.7.10), we ﬁnd after one iteration the following approximate solution: u ¼ A sinðka !tÞ

ðkAÞ2 ð3K2 þ K3 Þ a cos 2ðka !tÞ; 8c2

1.3.7.6. Experimental determination of third- and higher-order elastic constants The main experimental procedures for determining the thirdand higher-order elastic constants are based on the measurement of stress derivatives of ultrasonic velocities and on harmonic generation experiments. Hydrostatic pressure, which can be accurately measured, has been widely used; however, the measurement of ultrasonic velocities in a solid under hydrostatic pressure cannot lead to the whole set of third-order elastic constants, so uniaxial stress measurements or harmonic generation experiments are then necessary.

which involves second-harmonic generation. If additional iterations are performed, higher harmonic terms will be obtained. A well known property of the ﬁrst-order nonlinear equation (1.3.7.10) is that its solutions exhibit discontinuous behaviour at some point in space and time. It can be seen that such a discontinuity would appear at a distance from the origin given by (Breazeale, 1984) L ¼ 2

ðK2 Þ2 !u00 ; 3K2 þ K3

97

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.3.7.1. Relationships between W 2 , its pressure derivatives and the second- and third-order elastic constants Propagation

Polarization

ð 0 W 2 Þ0

@ð 0 W 2 Þ0 [email protected]

[100] [100] [110] [110] [110] [111] [111]

[100] [010] [110] ½110 [001] [111] ½110

c 11 c 44 ðc 11 þ c 12 þ 2c44 Þ=2 ðc 11 c 12 þ c 44 Þ=3 c 44 ðc 11 þ 2c12 þ 4c44 Þ=3 ðc 11 c 12 þ c 44 Þ=3

1 ð2c11 þ 1111 Þ=3 1 ð 2c44 þ 2323 Þ=3 1 c 11 þ c 12 þ 2c44 þ 0:5 1111 þ 1122 þ 2323 =3 1 c 11 c 11 þ 0:5 1111 1122 =3 1 ð 2c44 þ 2323 Þ=3 1 2c11 þ 4c12 þ 8c14 þ 1111 þ 21122 þ 42323 =9 1 2c11 2c12 þ 2c14 þ 1111 1122 þ 2323 =9

In order to interpret wave-propagation measurements in stressed crystals, Thurston (1964) and Brugger (1964) introduced the concept of natural velocity with the following comments:

, cS D kB U F

‘According to equation of motion, the wave front is a material plane which has unit normal k in the natural state; a wave front moves from the plane k a ¼ 0 to the plane k a ¼ L0 in the time L0 =W. Thus W, the natural velocity, is the wave speed referred to natural dimensions for propagation normal to a plane of natural normal k. In a typical ultrasonic experiment, plane waves are reﬂected between opposite parallel faces of a specimen, the wave fronts being parallel to these faces. One ordinarily measures a repetition frequency F, which is the inverse of the time required for a round trip between the opposite faces.’

References Breazeale, M. A. (1984). Determination of third-order elastic constants from ultrasonic harmonic generation. Physical Acoustics, Vol. 17, edited by R. N. Thurston, pp. 2–75. New York: Academic Press. Brillouin, L. (1932). Propagation des ondes e´lectromagne´tiques dans les milieux mate´riels. Congre`s International d’E´lectricite´, Vol. 2, Section 1, pp. 739–788. Paris: Gauthier-Villars. Brugger, K. (1964). Thermodynamic deﬁnition of higher-order elastic coefﬁcients. Phys. Rev. 133, 1611–1612. De Launay, J. (1956). The theory of speciﬁc heats and lattice vibrations. Solid State Physics, Vol. 2, edited by F. Seitz & D. Turnbull, pp. 219– 303. New York: Academic Press. Every, A. G. & McCurdy, A. K. (1992). Second and higher order elastic constants. In Landolt-Bo¨rnstein, Group III, Condensed Matter, Volume 29, Subvolume A. Berlin/Heidelberg/New York: Springer. Fischer, M. (1982). Third- and fourth-order elastic constants of ﬂuoperovskites CsCdF3, TlCdF3, RbCdF3, RbCaF3. J. Phys. Chem. Solids, 43, 673–682. Fischer, M., Zarembowitch, A. & Breazeale, M. A. (1980). Nonlinear elastic behavior and instabilities in crystals. Ultrasonics Symposium Proc. IEEE, pp. 999–1002. Fumi, F. G. (1951). Third-order elastic coefﬁcients of crystals. Phys. Rev. 83, 1274–1275. Fumi, F. G. (1952). Third-order elastic coefﬁcients in trigonal and hexagonal crystals. Phys. Rev. 86, 561. Fumi, F. G. (1987). Tables for the third-order elastic tensors in crystals. Acta Cryst. A43, 587–588. Green, R. E. (1973). Treatise on Material Science and Technology, Vol. 3. New York: Academic Press. McSkimmin, H. J. (1964). Ultrasonic methods for measuring the mechanical properties of solids and ﬂuids. Physical Acoustics, Vol. IA, edited by W. P. Mason, pp. 271–334. New York: Academic Press. Melcher, R. L. & Scott, B. A. (1972). Soft acoustic modes at the cooperative Jahn–Teller transition in DyVO4 . Phys. Rev. Lett. 28, 607– 610. Michard, F., Zarembowitch, A., Vacher, R. & Boyer, L. (1971). Premier son et son ze´ro dans les nitrates de strontium, barium et plomb. Phonons, edited by M. A. Nusimovici, pp. 321–325. Paris: Flammarion. Murnaghan, F. D. (1951). Finite Deformation in an Elastic Solid. New York: John Wiley and Sons. Nouet, J., Zarembowitch, A., Pisarev, R. V., Ferre´, J. & Lecomte, M. (1972). Determination of TN for KNiF3 through elastic, magneto-optical and heat capacity measurements. Appl. Phys. Lett. 21, 161–162. Rousseau, M., Gesland, J. Y., Julliard, J., Nouet, J., Zarembowitch, J. & Zarembowitch, A. (1975). Crystallographic, elastic and Raman scattering investigations of structural phase transitions in RbCdF3 and TlCdF3. Phys. Rev. 12, 1579–1590. Salje, E. K. H. (1990). Phase Transitions in Ferroelastic and Co-elastic Crystals. Cambridge University Press.

Hence W ¼ 2L0 F: In most experiments, the third-order elastic constants and higher-order elastic constants are deduced from the stress derivatives of 0 W 2. For instance, Table 1.3.7.1 gives the expressions for ð 0 W 2 Þ0 and @ð 0 W 2 Þ0 [email protected] for a cubic crystal. These quantities refer to the natural state free of stress. In this table, p denotes the hydrostatic pressure and the ijkl ’s are the following linear combinations of third-order elastic constants: 1111 ¼ c 111 þ 2c111 1122 ¼ 2c112 þ c 123 2323 ¼ c 144 þ 2c166 :

1.3.8. Glossary ei AT ui Sij S Tij T p m s sijkl s ðsijkl Þ sijklmn cijkl ðcijkl Þ c cijklmn E

Lame´ constants temperature speciﬁc heat at constant strain volumic mass Debye temperature Boltzmann constant internal energy free energy

covariant basis vector transpose of matrix A components of the displacement vector components of the strain tensor components of the strain Voigt matrix components of the stress tensor components of the stress Voigt matrix pressure normal stress shear stress second-order elastic compliances reduced second-order elastic compliances adiabatic second-order elastic compliances third-order elastic compliances second-order elastic stiffnesses adiabatic second-order elastic stiffnesses reduced second-order elastic stiffnesses third-order elastic stiffnesses Poisson’s ratio Young’s modulus bulk modulus (volume compressibility)

98

1.3. ELASTIC PROPERTIES Wallace, D. C. (1970). Thermoelastic theory of stressed crystals and higher-order elastic constants. Solid State Physics, Vol. 25. New York: Academic Press. Wallace, D. C. (1972). Thermodynamics of Crystals. New York: John Wiley and Sons. Zarembowitch, A. (1965). Etude the´orique et de´termination optique des constantes e´lastiques de monocristaux. Bull. Soc. Fr. Mine´ral. Cristallogr. 28, 17–49.

Thurston, R. N. (1964). Wave propagation in ﬂuids and normal solids. Physical Acoustics, Vol. 1A, edited by W. P. Mason, pp. 1–109. New York: Academic Press. Truesdell, C. & Toupin, R. (1960). The classical ﬁeld theories. Handbuch der Physik, Vol. III/1, edited by S. Flu¨gge. Berlin, Go¨ttingen, Heidelberg: Springer-Verlag. Voigt, W. (1910). Lehrbuch der Kristallphysik. 2nd ed. (1929). Leipzig: Teubner. Photoreproduction (1966). New York: Johnson Reprint Corp.

99

references

International Tables for Crystallography (2013). Vol. D, Chapter 1.4, pp. 100–105.

1.4. Thermal expansion By H. Ku¨ppers

1.4.1. Deﬁnition, symmetry and representation surfaces If the temperature T of a solid is raised by an amount T, a deformation takes place that is described by the strain tensor uij : uij ¼ ij T:

ð1:4:1:1Þ

The quantities ij are the coefﬁcients of thermal expansion. They have dimensions of T 1 and are usually given in units of 106 K1 . Since uij is a symmetrical polar tensor of second rank and T is a scalar, ij is a symmetrical polar tensor of second rank ðij ¼ ji Þ. According to the properties of the strain tensor uij (cf. Section 1.3.1.3.2), the ‘volume thermal expansion’, , is given by the (invariant) trace of the ‘linear’ coefﬁcients ij. ¼

1 V ¼ 11 þ 22 þ 33 ¼ trace ðij Þ: V T

ð1:4:1:2Þ

The magnitudes of thermal expansion in different directions, 011 , can be visualized in the following ways: (1) The representation quadric (cf. Section 1.1.3.5.2) ij xi xj ¼ C

ð1:4:1:3Þ

can be transformed to principal axes X1, X2 and X3 with principal values 1, 2 and 3 : 1 X12 þ 2 X22 þ 3 X32 ¼ C: The length of any radius vector leading to the surface of the quadric ðC ¼ 1Þ represents the reciprocal of the square root of thermal expansion along that direction, 011 ¼ a1i a1j ij (akl are the direction cosines of the particular direction). If all i are positive, the quadric ðC ¼ þ1Þ is represented by an pﬃﬃﬃﬃ ellipsoid, whose semiaxes have lengths 1= i. In this case, the square of the reciprocal length of radius vector r, r2 , represents the amount of positive expansion in the particular direction, i.e. a dilation with increasing temperature. If all i are negative, C is set to 1. Then, the quadric is again an ellipsoid, and r2 represents a negative expansion, i.e. a contraction with increasing temperature. If the i have different signs, the quadric is a hyperboloid. The asymptotic cone represents directions along which no thermal expansion occurs ð011 ¼ 0Þ. If one of the i is negative, let us ﬁrst choose C ¼ þ1. Then, the hyperboloid has one (belt-like) sheet (cf. Fig. 1.3.1.3) and the squares of reciprocal lengths of radius vectors leading to points on this sheet represent positive expansions (dilatations) along the particular directions. Along directions where the hyperboloid has no real values, negative expansions occur. To visualize these, C is set to 1. The resulting hyperboloid has two (cap-like) sheets (cf. Fig. 1.3.1.3) and r2 represents the amount of contraction along the particular direction. If two of the i are negative, the situation is complementary to the previous case. (2) A crystal sample having spherical shape (radius = 1 at temperature T) will change shape, after a temperature increase T, to an ellipsoid with principal axes ð1 þ 1 TÞ, ð1 þ 2 TÞ and ð1 þ 3 TÞ. This ‘strain ellipsoid’ is represented by the formula X12 ð1 þ 1 TÞ2

þ

X22 ð1 þ 2 TÞ2

þ

X32 ð1 þ 3 TÞ2

¼ 1:

Copyright © 2013 International Union of Crystallography

Whereas the strain quadric (1.4.1.3) may be a real or imaginary ellipsoid or a hyperboloid, the strain ellipsoid is always a real ellipsoid. (3) The magnitude of thermal expansion in a certain direction (the longitudinal effect), 011 , if plotted as radius vector, yields an oval: ð1 X12 þ 2 X22 þ 3 X32 Þ2 ¼ ðX12 þ X22 þ X32 Þ3 : If spherical coordinates ð’; #Þ are used to specify the direction, the length of r is jrj ¼ 011 ¼ ð1 cos2 ’ þ 2 sin2 ’Þ sin2 # þ 3 cos2 #:

ð1:4:1:4Þ

Sections through this representation surface are called polar diagrams. The three possible graphical representations are shown in Fig. 1.4.1.1. The maximum number of independent components of the tensor ij is six (in the triclinic system). With increasing symmetry, this number decreases as described in Chapter 1.1. Accordingly, the directions and lengths of the principal axes of the representation surfaces are restricted as described in Chapter 1.3 (e.g. in hexagonal, trigonal and tetragonal crystals, the representation surfaces are rotational sheets and the rotation axis is parallel to the n-fold axis). The essential results of these symmetry considerations, as deduced in Chapter 1.1 and relevant for thermal expansion, are compiled in Table 1.4.1.1. The coefﬁcients of thermal expansion depend on temperature. Therefore, the directions of the principal axes of the quadrics in triclinic and monoclinic crystals change with temperature (except the principal axis parallel to the twofold axis in monoclinic crystals). The thermal expansion of a polycrystalline material can be approximately calculated if the ij tensor of the single crystal is known. Assuming that the grains are small and of comparable size, and that the orientations of the crystallites are randomly distributed, the following average of 011 [(1.4.1.4)] can be calculated: Z Z 1 2 0 ¼ sin # d# d’ ¼ 13ð1 þ 2 þ 3 Þ: 4 0 0 11 If the polycrystal consists of different phases, a similar procedure can be performed if the contribution of each phase is considered with an appropriate weight.

Fig. 1.4.1.1. Sections (ac plane) of representation surfaces for a trigonal (or tetragonal or hexagonal) crystal with 11 ¼ 22 ¼ 1 and 33 ¼ þ3 105 K1 (similar to calcite). (a) Quadric, (b) strain ellipsoid (greatly exaggerated), (c) polar diagram. The c axis is the axis of revolution. Sectors with negative expansions are dashed.

100

1.4. THERMAL EXPANSION It should be mentioned that the true situation is more complicated. The grain boundaries of anisotropic polycrystalline solids are subject to considerable stresses because the neighbouring grains have different amounts of expansion or contraction. These stresses may cause local plastic deformation and cracks may open up between or within the grains. These phenomena can lead to a hysteresis behaviour when the sample is heated up or cooled down. Of course, in polycrystals of a cubic crystal species, these problems do not occur. If the polycrystalline sample exhibits a texture, the orientation distribution function (ODF) has to be considered in the averaging process. The resulting overall symmetry of a textured polycrystal is usually 1 m m (see Section 1.1.4.7.4.2), showing the same tensor form as hexagonal crystals (Table 1.4.1.1), or mmm.

Table 1.4.1.1. Shape of the quadric and symmetry restrictions Quadric System

Shape

Direction of principal axes

No. of independent components

Triclinic

General ellipsoid or hyperboloid

No restrictions

6

Monoclinic

One axis parallel to twofold axis (b)

4

Orthorhombic

Parallel to crystallographic axes

3

c axis is revolution axis

2

Trigonal, tetragonal, hexagonal

Revolution ellipsoid or hyperboloid

Nonzero components

1.4.2. Gru¨neisen relation Thermal expansion of a solid is a consequence of the anharmonicity of interatomic forces (see also Section 2.1.2.8). If Cubic, Sphere Arbitrary, not deﬁned 1 the potentials were harmonic, the atoms isotropic media would oscillate (even with large amplitudes) symmetrically about their equilibrium positions and their mean central position would remain unchanged. In order to describe thermal expansion, the anharmonicity is most conveniently accounted for by means of the socalled ‘quasiharmonic approximation’, assuming the lattice vibration frequencies ! to be independent of qt (denoted by an index t running from 1 to N). Each normal temperature but dependent on volume ½ð@[email protected]Þ 6¼ 0. Anhar- mode !s ðqt Þ contributes to the free energy by the amount monicity is taken into account by letting the crystal expand, but it hh!s ðqt Þ is assumed that the atoms vibrate about their new equilibrium : ð1:4:2:3Þ fs;t ¼ !s ðqt Þ þ kT ln 1 exp 2 kT positions harmonically, i.e. lattice dynamics are still treated in the harmonic approximation. The assumption ð@[email protected]Þ ¼ 0, which is made for the harmonic oscillator, is a generalization of the The total free energy amounts, therefore, to postulate that the frequency of a harmonic oscillator does not 3p X N depend on the amplitude of vibration. X fs;t This approach leads, as demonstrated below, to the Gru¨neisen F ¼ s¼1 t¼1 relation, which combines thermal expansion with other material constants and, additionally, gives an approximate description of 3p X N X h h!s ðqt Þ the temperature dependence of thermal expansion (cf. Krishnan ! ðq Þ þ kT ln 1 exp ¼ : ð1:4:2:4Þ et al., 1979; Barron, 1998). 2 s t kT s¼1 t¼1 For isotropic media, the volume expansion ½¼ 3 ¼ 11 þ 22 þ 33 , cf. (1.4.1.2), can be expressed by the therFrom (1.4.2.2) modynamic relation @F 1 @V 1 @V @p @p p ¼ ¼ ¼ ¼ ; ð1:4:2:1Þ @V T V @T p V @p T @T V @T V 3p X N X h @!s expðh- !s =kTÞh- ð@!s [email protected]Þ þ ¼ : ð1:4:2:5Þ being the isothermal compressibility. To obtain the quantity - ! =kTÞ 1 expðh 2 @V s t¼1 s¼1 ð@[email protected]ÞV , the pressure p is deduced from the free energy F, whose differential is dF ¼ S dT p dV, i.e. from The last term can be written as p ¼ ð@[email protected]ÞT : ð1:4:2:2Þ - ð@! [email protected]Þ h @!s s ð1:4:2:6Þ - ! =kTÞ 1 ¼ hnð!s ðqt Þ; TÞ @V ; expðh s In a crystal consisting of N unit cells with p atoms in each unit cell, there are 3p normal modes with frequencies !s (denoted by an index s running from 1 to 3p) and with N allowed wavevectors where nð!s ; TÞ is the Bose–Einstein distribution

101

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1 : ð1:4:2:7Þ behaviour is found to be approximately satisﬁed for many nð!s ; TÞ ¼ compounds, even with different types of interatomic interaction, expðh- !s =kTÞ 1 and takes values roughly between 1 and 2. Even in the case of Differentiation of (1.4.2.5) and (1.4.2.6) with respect to crystals with highly anisotropic elastic and thermal behaviour, the three principal values of the tensor ij [(1.4.2.15)] are comparably temperature at constant volume [see (1.4.2.1)] yields uniform, having values of about 2 (Ku¨ppers, 1974). X X @p @nð!s ; TÞ @!s ðqt Þ Effectively, shows a certain more or less pronounced ¼ [email protected] V @T @V dependence on temperature. The individual s;t are assumed to s t XX be temperature independent. However, being an average over 1 @!s ðqt Þ ð1:4:2:8Þ the whole spectrum of excited modes [cf. (1.4.2.13)], will not ¼ cVs;t !s ðqt Þ @V s t necessarily have the same value at low temperatures (when only low frequencies are excited) as at high temperatures (when all with modes are excited). Two limiting cases can be considered: - ! =kTÞ2 expðh- ! =kTÞ (1) At very high temperatures, all normal modes contribute by @nð! ; TÞ ðh s s s ¼k cVs;t ¼ h- !s ðqt Þ : ð1:4:2:9Þ an equal amount and the overall becomes simply the mean 2 @T ½expðh!s =kTÞ 1 value of all s;t . This quantity, cVs;t (the Einstein function), is the well known contribution of the normal mode !s ðqt Þ to the speciﬁc heat (at constant volume): XX XX @nð!s ; TÞ : ð1:4:2:10Þ cV ¼ cVs;t ¼ h- !s ðqt Þ @T s t s t Equation (1.4.2.8) can be simpliﬁed by the introduction of an ‘individual Gru¨neisen parameter’ s;t for each normal mode !s ðqt Þ: V @!s ðqÞt @½ln !s ðqt Þ : s;t ¼ ¼ !s ðqÞt @V @ðln VÞ Equation (1.4.2.8) then reads [with (1.4.2.1)] @p 1 XX V ¼ c ¼ : @T V V s t s;t s;t

ð1:4:2:12Þ

In this averaging process, the contribution of each normal mode to is weighted in the same way as it contributes to the speciﬁc heat cV [see (1.4.2.10)]. Equations (1.4.2.12) and (1.4.2.13) lead to the Gru¨neisen relation cV : V

(2) At very low temperatures, only the lower frequencies contribute. If only the acoustic branches are considered, can be related to the velocities of elastic waves. In the long-wavelength limit, dispersion is neglected, i.e. jqj is proportional to !: jqt j ¼

ð1:4:2:11Þ

Based on these individual parameters s;t, an average (or overall mode-independent) Gru¨neisen parameter can be deﬁned as PP PP s;t cVs;t s;t cVs;t : ð1:4:2:13Þ ¼ P P V ¼ cV cs;t

¼

ð1:4:2:14Þ

The above derivation was made for isotropic media. For anisotropic media, V=V is replaced by the strain ukl and 1 is replaced by the stiffness tensor cijkl [cf. Chapter 2.1 and equation (2.1.2.75)]. Then the Gru¨neisen parameter turns out to be a second-rank tensor ij : V ð1:4:2:15Þ ij ¼ V cTijkl kl : c

!s ðqt Þ ; vs ð’; #Þ

ð1:4:2:16Þ

where vs ð’; #Þ ðs ¼ 1; 2; 3Þ describes the velocities of the three elastic waves propagating in a direction ð’; #Þ. The density of vibrational states for each acoustic branch in reciprocal space increases with q2 dq. From (1.4.2.16), it follows that the number of normal modes in an increment of solid angle in q space, d ¼ sin # d# d’, within a frequency interval ! to ! þ d!, is proportional to ð!2 d! dÞ=v3. The summation over t can be converted into an integration over ! and , leading to X3 Z ð#; ’Þ d s

s¼1

0 ¼

X3 Z s¼1

v3s ð#; ’Þ : d v3 ð#; ’Þ

The vs ð’; #Þ can be calculatedP if the elastic constants are known. For isotropic solids, the term v3 s can be replaced (as done in 3 Debye’s theory of heat capacity) by ðv3 l þ 2vtr Þ, with vl being the velocity of the longitudinal wave and vtr the velocity of the transverse waves. In metals, the conduction electrons and magnetic interactions yield contributions to the free energy and to the speciﬁc heat. Accordingly, expression (1.4.2.14) can be augmented by introduction of an ‘electronic Gru¨neisen parameter’, e , and a ‘magnetic Gru¨neisen parameter’, m , in addition to the ‘lattice Gru¨neisen parameter’, l , considered so far: ¼ ðl cVl þ e cVe þ m cVm Þ: V

In the Debye approximation, the mode frequencies scale linearly with the cut-off frequency !D. Therefore, with h- !D ¼ kTD , the average isotropic Gru¨neisen parameter is calculated to be D ¼

N 1 XX : 3pN s t s;t 3p

1 ¼

1.4.3. Experimental methods 1.4.3.1. General remarks

V @!D V @TD @ðln TD Þ : ¼ ¼ !D @V TD @V @ðln VÞ

Since, in the Debye theory, TD is independent of temperature, D turns out to be independent of temperature. As and V are only weakly temperature dependent, the thermal expansion should then, according to (1.4.2.14), roughly behave like cV , i.e. should be proportional to T 3 at very low temperatures, and should be approximately constant for T TD (the Dulong–Petit law). This

Although the strain tensor uij and the thermal expansion tensor ij in general contain components with i 6¼ j (shear strains), in practice only longitudinal effects, i.e. relative length changes l=l with temperature changes T, are measured along different directions and the results are later transformed to a common coordinate system. Diffraction methods directly yield this ratio l=l. Other measuring techniques require separate measurements of l and l. The error in the measurement of l can

102

1.4. THERMAL EXPANSION usually be neglected. Thus, the accuracies of l and T limit the accuracy of thermal expansion coefﬁcients. The temperature interval T is determined by two measurements of temperatures T2 > T1 , with T2 T1 ¼ T. To increase the accuracy of the difference T, this interval should be large. The measured thermal expansion l=ðlTÞ is usually assigned to a temperature at the midpoint of the temperature interval, T0 ¼ ðT2 T1 Þ=2. This procedure is only justiﬁed if thermal expansion does not depend on temperature. Since, in fact, thermal expansion depends on temperature, in principle, smaller intervals should be chosen, which, in turn, enlarge the error of T. Here, a compromise has to be made. Sometimes, after completion of a ﬁrst run and after reviewing the preliminary course of ðTÞ, it is necessary to repeat some measurements using smaller temperature intervals in temperature ranges with large curvatures. The more-or-less curved course of ij ðTÞ is usually ﬁtted by polynomials in powers of temperature. Here, those T terms should be selected that are physically meaningful in the particular temperature range. For the low-temperature behaviour of a metal, a polynomial of type ¼ AT þ BT 3 þ CT 5 should be chosen. For minerals at higher temperatures, a polynomial ¼ 0 þ AT þ BT 1 þ CT 2 is used (Saxena & Shen, 1992). Temperature is usually measured by thermocouples and, in the cases of optical or electrical measurements (Sections 1.4.3.3 and 1.4.3.4) and at low temperatures also by platinum resistance thermometers. Above 1100 K, optical pyrometers can be used. In order to measure the thermal expansion of a crystal, at least as many independent measurements are necessary as the tensor has independent components (fourth column in Table 1.4.1.1). It is advisable, however, to carry out more measurements than are necessary. In this case (of redundancy), a ‘best’ set of tensor components is to be determined by least-squares methods as described below. Let us assume the most general case of a triclinic crystal, where m > 6 independent measurements of thermal expansions bk ðk ¼ 1; . . . ; mÞ were performed along m different directions with direction cosines ð1j Þk ðj ¼ 1; 2; 3Þ with respect to the chosen coordinate system. Each measurement bk is related to the six unknown tensor components ij (to be determined) by bk ¼ ð011 Þk ¼ ð1i Þk ð1j Þk ij :

ð1:4:3:1Þ

If the ij are replaced by ð ¼ 1; . . . ; 6Þ, using Voigt’s oneindex notation (Section 1.1.4.10.2), then bk ¼ Ck represents an overdetermined inhomogeneous system of m linear equations for the six unknowns . The coefﬁcients Ck , forming an m 6 matrix, are products containing direction cosines according to (1.4.3.1). The solution is obtained after several matrix calculations which are indicated by the formula (Nye, 1985) n t o bk ¼ ðClt Cl" Þ1 Ck ð; ; "; ¼ 1; . . . ; 6; l; k ¼ 1; . . . ; mÞ; where a superscript ‘t’ means transposed. Instead of determining the tensor components of a triclinic or monoclinic crystal in a direct way, as outlined above, it is also possible to determine ﬁrst the temperature change of the crystallographic unit cell and then, by formulae given e.g. by Schlenker et al. (1978), to deduce the tensor components ij. The direct approach is recommended, however, for reasons of the propagation of errors (Jessen & Ku¨ppers, 1991). The experimental techniques of measuring relative length changes l=l that are most widely used include diffraction, optical interferometry, pushrod dilatometry and electrical capacitance methods. If the specimens available are very small and/or irregular in shape, only diffraction methods can be used. The other methods require single-crystal parallelepipedal samples with at least 5 mm side lengths.

1.4.3.2. Diffraction Thermal expansion expresses itself, on a microscopic scale, by a change of the interplanar spacings of lattice planes. These can be measured by use of diffraction methods from changes of Bragg angles . Differentiation of the Bragg equation 2d sin ¼ , giving d=d ¼ cot , yields the thermal expansions 011 in directions normal to lattice planes (hkl) (i.e. along with h ¼ ha þ kb þ lc ) and, if h has direction cosines aðhklÞ 1j respect to the chosen Cartesian coordinate system, ðhklÞ ¼ aðhklÞ 0ðhklÞ 11 1i a1j ij ¼

1 @dðhklÞ @ ¼ cot : ðhklÞ d @T @T

The coefﬁcient cot permits a tremendous increase of sensitivity and accuracy if ! 90. That means, if possible, high-angle ð > 70 Þ reﬂections should be used for measurement because, for a given d, the changes of Bragg angles jj to be measured increase with ðcot Þ1 ¼ tan . The most important diffraction techniques (X-radiation is preferentially used) are: the rotating-crystal method, the Weissenberg method and diffractometers with counter recording. If small single crystals (> approximately 50 mm) are not available, powder methods (using a Debye–Scherrer ﬁlm camera or powder diffractometer) must be used, although the advantage of the highly accurate back-reﬂections, in general, cannot be used. Experimental aspects of measuring absolute d-values are discussed in detail in Volume C of International Tables for Crystallography (2004), Part 5. Since only relative displacements are to be measured in the present case, many complications connected with the determination of absolute values do not apply for thermal expansion measurements, such as zero-point correction, eccentricity of the mounted sample, refraction, absorption and diffraction proﬁle. 1.4.3.3. Optical methods (interferometry) The basic principle of measuring thermal expansion by interferometry consists of converting sample-length changes into variations of optical path differences of two coherent monochromatic light beams, which are reﬂected from two opposite end faces of the sample (or planes corresponding to them). An He– Ne laser usually serves as a light source. A beam expander produces a parallel beam and interference by two planes, which are slightly inclined to each other, produces fringes of equal thickness. Thermal expansion causes a movement of this fringe pattern, which is detected by photodiodes. The number of fringes passing a reference mark is counted and gives a measure of the relative movement of the two planes. As examples for various realizations of interferometric devices (Hahn, 1998), two basic designs will be described. (i) Fizeau interferometer (Fig. 1.4.3.1). The sample S is covered by a thin plate P2 (with a polished upper surface and a coarsely ground and non-reﬂecting lower surface) and is placed in between a bottom plate P3 and a wedge-shaped plate P1 (wedge angle of about 1 ). The upper surface of P1 reﬂects the incident beam (i) to a reﬂected beam (r) so that it is removed from the interference process. The relevant interference takes place between ray (1) reﬂected by the lower surface of P1 and ray (2) reﬂected by the upper surface of P2. A cylindrical tube T, which deﬁnes the distance between P1 and P3 as well as P2, is usually made of fused silica, a material of low and well known thermal expansion. The measured dilatation is caused, therefore, by the difference between thermal expansion of the sample and a portion of the fused silica tube of equal length. The whole apparatus is mounted in a thermostat. (ii) Michelson interferometer (Fig. 1.4.3.2). The reference mirror M and the beam-splitter B are placed outside the thermostat. The upper face of the sample S is one interference plane and the upper surface of the bottom plate is the other. The

103

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES interference pattern IP is divided into two ﬁelds corresponding to the two ends of the sample. The difference of fringe movements within these two ﬁelds yields the absolute thermal expansion of the sample. 1.4.3.4. Electrical methods 1.4.3.4.1. Inductance changes (pushrod dilatometry) With this method, the expansion of the crystal is transmitted out of the cooled or heated region to an external measuring device by a rod made of a reference material whose thermal expansion is low and well known (usually silica glass) (cf. Gaal, 1998). If this rod is inside a tube of the same material (silica glass), and the specimen is inside as well, then the difference in expansion between the crystal and an equal length of the reference material is measured. Above 1100 K, instead of silica glass, high-purity alumina or single-crystal sapphire or tungsten rods are used. To measure the displacement of the rods, several techniques are used. The most important are: (1) a ferrite core is moved in a coil to change the inductivity of the coil, which is detected by the change of resonance frequency of an electrical circuit having a ﬁxed capacitance; (2) linear-variable-differential transformers. Temperature gradients in the rod and the tube can lead to severe complications. For every determination, the system should be calibrated by certiﬁed materials (White, 1998), such as -Al2O3, Cu, Pt, fused silica, Si, W, Mg or Mo. 1.4.3.4.2. Capacitance methods In a way similar to the interferometric methods, the change of the gap between the lower surface of P1 and the upper surface of P2 (Fig. 1.4.3.1) is used to determine the thermal expansion of the sample. This gap – with electrically conducting surfaces – is used as the capacitance in an electric circuit with a ﬁxed inductance. The change of capacitance leads to a change of resonance frequency, which is measured.

1.4.4. Relation to crystal structure The anharmonicities of the interatomic potentials gain importance with increasing vibration amplitudes of the atoms. Since, at a given temperature, weakly bonded atoms oscillate with larger amplitudes, they contribute to a larger degree to thermal expansion in comparison with stronger bonds. This correlation follows also from the Gru¨neisen relation (1.4.2.14) because (or

Fig. 1.4.3.1. Schematic diagram of a Fizeau interferometer.

) is proportional to the compressibility, which, in turn, is a rough measure of the interatomic and intermolecular forces. This simple consideration allows qualitative predictions of the thermal expansion behaviour of a crystal species if the structure is known: (1) Covalent bonds are associated with very small thermal expansions (diamond, graphite perpendicular to the c axis), whereas van der Waals bonds give rise to large thermal expansions (N2, graphite parallel to the c axis). In accordance with their relatively high elastic stiffness, hydrogen bonds, especially short hydrogen bonds, lead to comparably small thermal expansions. (2) In layer-like structures, the maximum thermal expansion occurs normal to the layers (mica, graphite, pentaerythritol). (3) Thermal expansion decreases when the density of weak bonds decreases: therefore, expansion is greater for crystals with small molecules (many van der Waals contacts per volume) than for their larger homologues (e.g. benzene–naphthalene–anthracene). Buda et al. (1990) have calculated the thermal expansion of silicon by means of ab initio methods. It is to be expected that these methods, which are currently arduous, will be applicable to more complicated structures in the years to come and will gain increasing importance in this ﬁeld (cf. Lazzeri & de Gironcoli, 1998). It is observed rather frequently in anisotropic materials that an enhanced expansion occurs along one direction and a contraction (negative expansion) in directions perpendicular to that direction (e.g. in calcite). The volume expansion, i.e. the trace of ij, is usually positive in these cases, however. If the tensor of elastic constants is known, such negative expansions can mostly be explained by a lateral Poisson contraction caused by the large expansion (Ku¨ppers, 1974). Only a few crystals show negative volume expansion and usually only over a narrow temperature range (e.g. Si and fused silica below about 120 K and quartz above 846 K) (White, 1993). Cubic ZrW2O8 was recently found to exhibit isotropic negative thermal expansion over the complete range of stability of this material (0.5–1050 K) (Mary et al., 1996). This behaviour is explained by the librational motion of practically rigid polyhedra and a shortening of Zr—O—W bonds by transverse vibration of the oxygen atom. By tailoring the chemical content (of TiO2 or

Fig. 1.4.3.2. Schematic diagram of a Michelson interferometer.

104

1.4. THERMAL EXPANSION LiAlSiO4) in a glassy matrix, an expansion coefﬁcient can be achieved that is nearly zero over a desired temperature range. A compilation of numerical values of the tensor components of more than 400 important crystals of different symmetry is given by Krishnan et al. (1979). Phase transitions are accompanied and characterized by discontinuous changes of derivatives of the free energy. Since the thermal expansion is a second-order derivative, discontinuities or changes of slope in the ðTÞ curve are used to detect and to describe phase transitions (cf. Chapter 3.1).

ij uij cV F p S T V

1.4.5. Glossary thermal expansion volume thermal expansion Gru¨neisen parameter isothermal compressibility strain tensor speciﬁc heat at constant volume free energy pressure entropy temperature volume

References Barron, T. H. K. (1998). Generalized theory of thermal expansion of solids. In Thermal expansion of solids, edited by C. Y. Ho, ch. 1. Materials Park, Ohio: ASM International.

Buda, F., Car, R. & Parrinello, M. (1990). Thermal expansion of c-Si via ab initio molecular dynamics. Phys. Rev. B, 41, 1680– 1683. Gaal, P. S. (1998). Pushrod dilatometers. In Thermal expansion of solids, edited by C. Y. Ho, ch. 5. Materials Park, Ohio: ASM International. Hahn, T. A. (1998). Thermal expansion measurements using optical interferometry. In Thermal expansion of solids, edited by C. Y. Ho, ch. 6. Materials Park, Ohio: ASM International. International Tables for Crystallography (2004). Vol. C. Mathematical, physical and chemical tables, 3rd ed., edited by E. Prince. Dordrecht: Kluwer Academic Publishers. Jessen, S. M. & Ku¨ppers, H. (1991). The precision of thermal-expansion tensors of triclinic and monoclinic crystals. J. Appl. Cryst. 24, 239– 242. Krishnan, R. S., Srinivasan, R. & Devanarayanan, S. (1979). Thermal expansion of solids. Oxford: Pergamon. Ku¨ppers, H. (1974). Anisotropy of thermal expansion of ammonium and potassium oxalates. Z. Kristallogr. 140, 393–398. Lazzeri, M. & de Gironcoli, S. (1998). Ab initio study of Be(001) surface thermal expansion. Phys. Rev. Lett. 81, 2096–2099. Mary, T. A., Evans, J. S. O., Vogt, T. & Sleight, A. W. (1996). Negative thermal expansion from 0.3 to 1050 Kelvin in ZrW2O8. Science, 272, 90– 92. Nye, J. F. (1985). Physical properties of crystals. Oxford: Clarendon Press. Saxena, S. K. & Shen, G. (1992). Assessed data on heat capacity, thermal expansion, and compressibility of some oxides and silicates. J. Geophys. Res. 97, 19813–19825. Schlenker, J. L., Gibbs, G. V. & Boisen, M. B. (1978). Strain-tensor components expressed in terms of lattice parameters. Acta Cryst. A34, 52–54. White, G. K. (1993). Solids: thermal expansion and contraction. Contemp. Phys. 34, 193–204. White, G. K. (1998). Thermal expansion reference materials. In Thermal expansion of solids, edited by C. Y. Ho, ch. 11. Materials Park, Ohio: ASM International.

105

references

International Tables for Crystallography (2013). Vol. D, Chapter 1.5, pp. 106–152.

1.5. Magnetic properties By A. S. Borovik-Romanov,† H. Grimmer and M. Kenzelmann

1.5.1. Introduction In the present chapter, we shall give a short review of the structure and some properties of magnetic substances that depend mainly on the symmetry of these substances. Aspects related to the magnetic symmetry receive the most emphasis. The magnetic symmetry takes into account the fact that it is necessary to consider time inversion in addition to the usual spatial transformations in order to describe the invariance of the thermodynamic equilibrium states of a body. The symmetry of magnetic materials depends not only on the mean charge density function ðrÞ, but also on the mean current density jðrÞ and the mean spin density SðrÞ. The symmetry of the function ðrÞ is called the crystallographic or crystallochemical symmetry of a body. If the current density jðrÞ in the crystal is not zero, an orbital magnetic moment is produced. It is obvious that there can be no macroscopic current in a substance which is in R thermodynamic equilibrium and in which the integral j d over the magnetic elementary cell is always equal to zero. The current j, however, may produce a macroscopic nonzero magnetic moment mðrÞ. We shall consider below the function mðrÞ, which determines the space distribution of the total (spin plus orbital) magnetic moment density. The symmetry of the distribution of the magnetic moment density mðrÞ may be considered as the symmetry of the arrangement and orientation of the mean atomic (or ionic) magnetic moments in the crystal (we shall not consider the magnetism of the conduction electrons in this chapter). The ﬁrst part of the chapter is devoted to a brief classiﬁcation of materials according to their magnetic properties. If mðrÞ 0 at every point, the substance is magnetically disordered. There are two types of such substances: diamagnets and paramagnets. Their most important features are brieﬂy outlined in Section 1.5.1.1. If mðrÞ 6¼ 0, the substance possesses a magnetic structure. There are two cases to be considered: (1) The integral of mðrÞ R over the primitive cell is notR zero ( m d 6¼ 0); such a substance is called ferromagnetic. (2) m d ¼ 0; such a substance is called antiferromagnetic. The integration is performed over the magnetic elementary cell, which may differ from the crystallographic one. This crude classiﬁcation is detailed in Section 1.5.1.2. The classiﬁcation of ferromagnets according to the type of the magnetic structure is given in Section 1.5.1.2.1. The concept of the magnetic sublattice is introduced and the ferromagnets are divided into two groups: one-sublattice ferromagnets and multisublattice ferro- and ferrimagnets. Collinear and non-collinear ferromagnets are described. In Section 1.5.1.2.2, the antiferromagnets are classiﬁed by the types of their magnetic structures: collinear, weakly non-collinear and strongly non-collinear antiferromagnets. Incommensurate structures are brieﬂy mentioned in Section 1.5.1.2.3. The study of magnetically ordered crystals has led to a generalization of the theory of crystallographic symmetry. This generalization is based on the fact that mðrÞ changes sign under a speciﬁc transformation R, which is equivalent to time inversion. The invariance of the equation of motion is preserved under R. The symmetry that admits the operation R along with ordinary crystallographic transformations (translations, rotations and reﬂections) is called the magnetic symmetry. Section 1.5.2 is devoted to magnetic symmetry. Different types of magnetic point † Deceased.

Copyright © 2013 International Union of Crystallography

(Section 1.5.2.1) and magnetic space (Section 1.5.2.3) groups are deﬁned. The 22 magnetic Bravais lattices are displayed in Section 1.5.2.2. All magnetic groups (both point and space) are categorized into three types: (1) The groups that possess R as an additional element. The crystals which belong to such space groups satisfy mðrÞ ¼ mðrÞ at every point, hence mðrÞ ¼ 0: Such crystals are found to be paramagnetic or diamagnetic. Crystals with a point group that possesses R as an additional element may also be antiferromagnetic. This is the case if R appears in the space group multiplied by some translations but not as a separate element. (2) The groups that do not possess R at all. (3) The groups that contain the element R only in combination with some other elements (translations, rotations, reﬂections). The latter two types of space groups describe magnetically ordered crystals. The transition from the paramagnetic state to the magnetically ordered state entails a transition from one magnetic group to another. These transitions are considered in Section 1.5.3. Section 1.5.3.1 gives an example of the analysis of such transitions in terms of magnetic symmetry and introduces the concept of ferromagnetic and antiferromagnetic vectors, which characterize the magnetic structures. The phenomenological theory of magnetic transitions is based on the Landau theory of secondorder phase transitions. Section 1.5.3.3 is dedicated to this theory (see also Section 3.1.2). The Landau theory is based on the expansion of the thermodynamic potential into a series of the basic functions of irreducible representations of the space group of the crystal under consideration. It is essential to distinguish the exchange and the relativistic terms in the expansion of the thermodynamic potential (see Section 1.5.3.2). The domain structure of ferromagnets and antiferromagnets is considered in Section 1.5.4, where 180 and T-domains are described. The change from a multidomain structure to a singledomain structure under the action of an applied magnetic ﬁeld explains the magnetization process in ferro- and ferrimagnets. The existence of 180 domains in antiferromagnets was shown in experiments on piezomagnetism and the linear magnetoelectric effect. Non-collinear antiferromagnetic structures (weakly ferromagnetic, non-collinear and non-coplanar antiferromagnetic structures) are described in Section 1.5.5. The existence of these structures is directly connected with the magnetic symmetry. Such a structure arises if the irreducible representation responsible for the phase transition into the ordered state is two- or threedimensional. Correspondingly, the magnetic group allows the coexistence of two or three different ferro- or antiferromagnetic vectors. Besides the magnetic phase transition from the disordered into the ordered state, there exist transitions from one magnetic structure into another. Amongst them, there are reorientation transitions, which are obtained by a rotation of the ferromagnetic or antiferromagnetic vector relative to the crystallographic axis. They are analysed in Section 1.5.6. Sections 1.5.7 and 1.5.8 are devoted to phenomena that can be (and were) predicted only on the basis of magnetic symmetry. These are piezomagnetism (Section 1.5.7) and the magnetoelectric effect (Section 1.5.8). The reciprocal of the piezomagnetic effect (Section 1.5.7.1) is linear magnetostriction (Section 1.5.7.2). The magnetoelectric effect has been investigated far more than piezomagnetism. In addition to the linear magnetoelectric effect (Section 1.5.8.1), effects of higher order (Section 1.5.8.2) have also been observed. In connection with the

106

1.5. MAGNETIC PROPERTIES magnetoelectric effect, ferromagnetic and antiferromagnetic ferroelectrics are also considered (Section 1.5.8.3). Such ‘multiferroic’ crystals have received much attention in recent years. For this reason, Section 1.5.8.3 has been updated by M. Kenzelmann. In Section 1.5.9, the magnetostriction in ferromagnets is discussed. Only fundamental points of this problem are considered. As noted above, only those problems of magnetism that are closely connected with magnetic symmetry are considered in this chapter. However, these problems are only outlined brieﬂy here because of the restricted size of this volume. For the same reason, it is impossible to give an exhaustive list of references. The references given here include selected publications on magnetic symmetry and those describing the ﬁrst experimental work devoted to the properties connected with magnetic symmetry. Because the magnetoelectric effect has recently attracted considerable attention, some references have been added in Section 1.5.8 of this second edition. The Gaussian system of units was used in this chapter in the ﬁrst edition of this book, as was usual for the early work on the topics of this chapter. At present, the majority of publications on magnetism use the legal SI units. Therefore, all equations are now given in both systems in this chapter. Fortunately, many relations do not depend on the choice of units, in most other cases only a small modiﬁcation is sufﬁcient to make the equations valid in both systems; only a few equations have to be written in two forms. In the ﬁgures and tables showing the results of early measurements, the Gaussian units have been kept and the conversion factors are indicated. 1.5.1.1. Magnetically disordered materials A crystal placed in a magnetic ﬁeld H is magnetized. The magnetized state is characterized by two vectors, the magnetization M (the magnetic moment per unit volume) and the magnetic induction B. In Gaussian units the magnetic induction is given by B ¼ H þ 4M:

SIð1:5:1:1Þ

where 0 = 4 107 N A2 is the magnetic constant. It is also known as the vacuum permeability; its dimension can also be written as V s A1 m1 or H m1. The Gaussian units are related to the corresponding SI units as follows: 1 G = 104 tesla (T), 1 Oe = 103/(4) A m1, 1 emu cm3 = 103 A m1. Introducing 0 , where 0 ¼ 0 in SI units and 0 ¼ 1 in Gaussian units, most equations in this chapter can be written in a form that is valid in both systems. Historically, the two ﬁelds H and B have been called the magnetic ﬁeld H and the magnetic induction B. The International Organization for Standards (ISO) recommends ‘magnetic ﬁeld H’ and ‘magnetic ﬂux density B’. We are aware that it would be more appropriate to call B the magnetic ﬁeld strength and H the magnetic excitation (see e.g. Hehl et al., 2009) and to consider the properties that we shall describe as functions of B rather than of H. For easy comparison with published work, we shall stick to the historic approach. Note that except for ferromagnetic crystals, |M| is negligible compared to |H|, so that, instead of an applied ﬁeld H, we have B ¼ 0 H, and vice versa. In magnetically disordered materials, the vectors B and M are linear in the magnetic ﬁeld. Using a Cartesian coordinate system, this can be expressed as

ð1:5:1:2Þ

where ij is the dimensionless magnetic susceptibility per unit volume and ij is the permeability; summations over the repeated indices j are assumed. The susceptibility is frequently referred to one mass unit or to one mole of substance. The mass susceptibility is written as g, the molar susceptibility as mol. The Gaussian units for , g, mol and their SI equivalents are given in Table 1.5.10.1. The Gaussian unit for is 4 times larger than the SI unit. Thus, we obtain SI = 4G. All three vectors H, M and B are axial vectors (see Section 1.1.4.5.3), the symmetry of which is 1=m. Accordingly, the components of these vectors perpendicular to a mirror plane do not change sign on being reﬂected by this plane, whereas the components parallel to the plane do change sign. Consequently, these three vectors are invariant with respect to inversion. The quantities ij and ij are components of second-rank polar tensors. With respect to the principal axes, the tensors become diagonal and both, the magnetic susceptibility and the permeability of a crystal, are characterized by the three values of the principal susceptibilities and principal permeabilities, respectively. The magnetically disordered materials are divided into two types: diamagnets ( < 0) and paramagnets ( > 0). Diamagnetism is a universal property of all materials. It is associated with the tendency of all the electrons to screen the applied external ﬁeld according to the Lenz rule. For materials in which the electron orbits are spherically symmetric, the relation for the diamagnetic susceptibility was calculated by Langevin. For monoatomic substances he obtained, in Gaussian units, ! i¼Z X e2 G 2 r ¼ N Gð1:5:1:3Þ 6mc2 i¼1 i and, in SI units, ! i¼Z e 2 0 X 2 r ; ¼ N 6m i¼1 i SI

Gð1:5:1:1Þ

This equation shows how the units of B, H and M are related in the Gaussian system. The unit for B, the gauss (G), and for H, the oersted (Oe), also coincide in magnitude, whereas the unit for M, usually called emu cm3, is 4 times larger than the gauss and the oersted. In SI units the magnetic induction is given by B ¼ 0 ðH þ MÞ;

Mi ¼ ij Hj and Bi ¼ ij Hj ;

SIð1:5:1:3Þ

where N is the number of atoms per unit volume, Z is the number of electrons per atom, e and m are the charge and the mass of the electron, respectively, and r2i are the mean squares of the radii of the electron orbits. In polyatomic substances, the summation must be done over all types of atoms. In most chemical compounds, the orbits are not spherical and the calculation of the diamagnetic susceptibility becomes more complicated. In metals, the conduction electrons contribute signiﬁcantly to the diamagnetic susceptibility. The diamagnetic susceptibility of most substances is very small (G ’ 106 , SI ’ 105 ) and isotropic. Rare exceptions are bismuth and some organic compounds, in which the diamagnetism is strongly anisotropic. Most paramagnetic materials contain ions (or free atoms) with a partly ﬁlled inner electronic shell. Examples are the transition metals and the rare-earth and actinide elements. Atoms, molecules and point defects possessing an odd number of electrons are also paramagnetic. Ions with a partly ﬁlled inner electronic shell possess orbital L and spin S angular momenta, which determine the total angular momentum J provided the spin–orbit interaction is strong compared with the crystal ﬁeld. The magnetic susceptibility of paramagnets follows the Curie– Weiss law in low magnetic ﬁelds (B B kB T): ¼

N0 p2 2B ; 3kB ðT Þ

ð1:5:1:4Þ

where N is the number of magnetic ions (or atoms) per volume unit, B is the Bohr magneton, p is the effective number of Bohr magnetons, kB is the Boltzmann factor and is the Weiss constant. The Weiss constant is related to the interaction between

107

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES The conduction electrons in metals possess paramagnetism in addition to diamagnetism. The paramagnetic susceptibility of the conduction electrons is small (of the same order of magnitude as the diamagnetic susceptibility) and does not depend on temperature. This is due to the fact that the conduction electrons are governed by Fermi–Dirac statistics. 1.5.1.2. Magnetically ordered materials

Fig. 1.5.1.1. Temperature dependence of 1= at high temperatures for different types of materials: (1) ferromagnet; (2) antiferromagnet; (3) ferrimagnet.

the magnetic moments (mostly exchange interaction) and to the effect of the splitting of electron levels of the paramagnetic ion in the crystalline electric ﬁeld. Many paramagnets that obey the Curie–Weiss law transform into magnetically ordered materials at a temperature Tc, which is of the order of jj. The sign of depends on the sign of the exchange constant Jex [see relation (1.5.1.7)]. For the substances that at low temperatures become ferromagnets, we have > 0, for antiferromagnets < 0, and for ferrimagnets the temperature dependence of is more complicated (see Fig. 1.5.1.1). For those paramagnets that do not go over into an ordered state, is close to zero and equation (1.5.1.4) changes to the Curie law. The value of the effective number of Bohr magnetons p depends strongly on the type of the magnetic ions and their environment. For most rare-earth compounds at room temperature, the number p has the same value as for free ions: p ¼ g½JðJ þ 1Þ1=2 ;

ð1:5:1:5Þ

where g is the Lande´ g-factor or the spectroscopic splitting factor (1 g 2) and J is the quantum number of the total angular momentum. In this case, the paramagnetic susceptibility is practically isotropic. Some anisotropy can arise from the anisotropy of the Weiss constant . The behaviour of the transition-metal ions is very different. In contrast to the rare-earth ions, the electrons of the partly ﬁlled shell in transition metals interact strongly with the electric ﬁeld of the crystal. As a result, their energy levels are split and the orbital moments can be ‘quenched’. This means that relation (1.5.1.5) transforms to pij ¼ ðgeff Þij ½SðS þ 1Þ1=2 :

ð1:5:1:6Þ

Here the value of the effective spin S represents the degeneration of the lowest electronic energy level produced by the splitting in the crystalline ﬁeld; ðgeff Þij differs from the usual Lande´ g-factor. The values of its components lie between 0 and 10–20. The tensor ðgeff Þij becomes diagonal with respect to the principal axes. According to relation (1.5.1.6), the magnetic susceptibility also becomes a tensor. The anisotropy of ðgeff Þij can be studied using electron paramagnetic resonance (EPR) techniques. The Curie–Weiss law describes the behaviour of those paramagnets in which the magnetization results from the competition of two forces. One is connected with the reduction of the magnetic energy by orientation of the magnetic moments of ions in the applied magnetic ﬁeld; the other arises from thermal ﬂuctuations, which resist the tendency of the ﬁeld to orient these moments. At low temperatures and in strong magnetic ﬁelds, the linear dependence of the magnetization versus magnetic ﬁeld breaks down and the magnetization can be saturated in a sufﬁciently strong magnetic ﬁeld. Most of the paramagnetic substances that obey the Curie–Weiss law ultimately develop magnetic order as the temperature is decreased.

1.5.1.2.1. Ferromagnets (including ferrimagnets) As stated above, all magnetically ordered materials that possess a spontaneous magnetization Ms different from zero (a magnetization even in zero magnetic ﬁeld) are called ferromagnets. The simplest type of ferromagnet is shown in Fig. 1.5.1.2(a). This type possesses only one kind of magnetic ion or atom. All their magnetic moments are aligned parallel to each other in the same direction. This magnetic structure is characterized by one vector M. It turns out that there are very few ferromagnets of this type in which only atoms or ions are responsible for the ferromagnetic magnetization (CrBr3, EuO etc.). The overwhelming majority of ferromagnets of this simplest type are metals, in which the magnetization is the sum of the magnetic moments of the localized ions and of the conduction electrons, which are partly polarized. More complicated is the type of ferromagnet which is called a ferrimagnet. This name is derived from the name of the oxides of the elements of the iron group. As an example, Fig. 1.5.1.2(b) schematically represents the magnetic structure of magnetite (Fe3O4). It contains two types of magnetic ions and the number of Fe3+ ions (l1 and l2 ) is twice the number of Fe2+ ions (l3 ). The values of the magnetic moments of these two types of ions differ. The magnetic moments of all Fe2+ ions are aligned in one direction. The Fe3+ ions are divided into two parts: the magnetic moments of one half of these ions are aligned parallel to the magnetic moments of Fe2+ and the magnetic moments of the other half are aligned antiparallel. The array of all magnetic moments of identical ions oriented in one direction is called a magnetic sublattice. The magnetization vector of a given sublattice will be denoted by Mi. Hence the magnetic structure of Fe3O4 consists of three magnetic sublattices. The magnetizations of two of them are aligned in one direction, the magnetization of the third one is oriented in the opposite direction. The net ferromagnetic magnetization is Ms ¼ M1 M2 þ M3 ¼ M3. The special feature of ferrimagnets, as well as of many antiferromagnets, is that they consist of sublattices aligned antiparallel to each other. Such a structure is governed by the nature of the main interaction responsible for the formation of the ordered magnetic structures, the exchange interaction. The energy of the exchange interaction does not depend on the direction of the interacting magnetic moments (or spins S) relative to the crystallographic axes and is represented by the following relation: P ex Uex ¼ Jmn Sm Sn : ð1:5:1:7Þ m;n ex Here Sm, Sn are the spins of magnetic atoms (ions) and Jmn is the exchange constant, which usually decreases fast when the distance between the atoms rises. Therefore, usually only the nearest-neighbour interaction needs to be taken into account. Hence, according to (1.5.1.7), the exchange energy is a minimum for the state in which neighbouring spins are parallel (if J ex > 0) or antiparallel (if J ex < 0). If the nearest-neighbour exchange interaction were the only interaction responsible for the magnetic ordering, only collinear magnetic structures would exist (except in triangle lattices). Together with the exchange interaction, there is also a magnetic dipole interaction between the magnetic moments of the atoms as well as an interaction of the atomic magnetic electrons with the crystalline electric ﬁeld. These interactions are much smaller than the exchange interaction.

108

1.5. MAGNETIC PROPERTIES They are often called relativistic interactions. The relativistic interactions and the exchange interaction between next-nearest atoms bring about the formation of non-collinear magnetic structures. A simple non-collinear structure is the magnetic structure of a weak ferromagnet. It contains identical magnetic ions divided in equal amounts between an even number of sublattices. In the ﬁrst approximation, the magnetizations of these sublattices are antiparallel, as in usual antiferromagnets. In fact, the magnetizations are not strictly antiparallel but are slightly canted, i.e. non-collinear, as shown in Fig. 1.5.1.2(c). There results a ferromagnetic moment MD , which is small compared with the

Fig. 1.5.1.2. Ordered arrangements of magnetic moments li in: (a) an ordinary ferromagnet Ms ¼ Nl1 ; (b) a ferrimagnet Ms ¼ ðN=3Þðl1 þ l2 þ l3 Þ; (c) a weak ferromagnet M ¼ MD ¼ ðN=2Þðl1 þ l2 Þ, L ¼ ðN=2Þðl1 l2 Þ, Lx My ; Mx ¼ Mz ¼ Ly ¼ Lz ¼ 0. N is the number of magnetic ions per volume unit.

sublattice magnetization Mi . The magnetic properties of weak ferromagnets combine the properties of both ferromagnets and antiferromagnets. They will be discussed in detail in Section 1.5.5.1. 1.5.1.2.2. Antiferromagnets As discussed above, the exchange interaction, which is of prime importance in the formation of magnetic order, can lead to a parallel alignment of the neighbouring magnetic moments as well as to an antiparallel one. In the latter case, the simplest magnetic structure is the collinear antiferromagnet, schematically shown in Fig. 1.5.1.3(a). Such an antiferromagnet consists of one or several pairs of magnetic sublattices of identical magnetic ions located in equivalent crystallographic positions. The magnetizations of the sublattices are oriented opposite to each other.

Fig. 1.5.1.3. Ordered arrangements of magnetic moments li in: (a) an ordinary two-sublattice antiferromagnet L ¼ ðN=2Þðl1 l2 Þ; (b) a weakly non-collinear four-sublattice antiferromagnet L1 ðxÞ ¼ ðN=4Þðl1 l2 l3 + l4 Þ, L2 ðyÞ ¼ ðN=4Þðl1 l2 + l3 l4 Þ; (c) a strongly non-collinear threesublattice antiferromagnet L1 ¼ ðN=3Þð3Þ1=2 ðl2 l1 Þ, L2 ¼ ðN=3Þðl1 + l2 l3 Þ. The broken lines show the crystallographic primitive cell and the solid lines the magnetic primitive cell.

109

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES More complicated antiferromagnetic structures also exist: sinusoidal structures, which also consist of layers in which all the magnetic moments are parallel to each other. Fig. 1.5.1.4(c) displays the cycloidal spiral and Figs. 1.5.1.4(d) and (e) display longitudinal and transverse spin density waves, respectively.

1.5.2. Magnetic symmetry

Fig. 1.5.1.4. Helical and sinusoidal magnetic structures. (a) An antiferromagnetic helix; (b) a cone spiral; (c) a cycloidal spiral; (d) a longitudinal spindensity wave; (e) a transverse spin-density wave.

Fig. 1.5.1.3(b) shows a weakly non-collinear antiferromagnet, in which the vectors of magnetization of four equivalent sublattices form a cross with a small tilting angle 2. Such a structure can be considered as an admixture of ‘weak antiferromagnetism’ L1 with easy axis Ox to an ordinary antiferromagnet L2 with easy axis Oy. This weak antiferromagnetism is of the same origin as weak ferromagnetism. Its nature will be discussed in detail in Section 1.5.5.2. The minimum of the exchange interaction energy of three spins located at the corners of a triangle corresponds to a structure in which the angles between two adjacent spins are 120 . Correspondingly, many hexagonal crystals possess a triangular antiferromagnetic structure like the one shown in Fig. 1.5.1.3(c). The sum of the magnetizations of the three sublattices in this structure equals zero. In tetragonal crystals, a 90 antiferromagnetic structure can exist, which consists of four equivalent sublattices with magnetizations oriented along the positive and negative directions of the x and y axes. Finally, in addition to the electronic magnetically ordered substances, there exist nuclear ferro- and antiferromagnets (below 1 mK for some insulators and below 1 mK for metals). 1.5.1.2.3. Helical and sinusoidal magnetic order There are many more complicated non-collinear magnetic structures. Fig. 1.5.1.4(a) shows an antiferromagnetic helical structure. It consists of planes perpendicular to the z axis in which all the magnetic moments are parallel to each other and are perpendicular to z. The polar angle of the direction of the moments changes from plane to plane by some constant . Thus, the magnetization vectors describe a spiral along the axis of the crystal. Such structures were observed in hexagonal rare-earth metals. A speciﬁc feature is that they often are incommensurate structures. This means that 2= is not a rational number and that the period of the magnetic spiral is not a multiple of the period of the lattice. Similar to the antiferromagnetic helix, ferromagnetic helical or spiral structures exist [see Fig. 1.5.1.4(b)] in which the magnetizations of the layers are tilted to the axis at an angle . As a result, the vectors of the magnetization of the layers are arranged on the surface of a cone. The ferromagnetic magnetization is aligned along the z axis. This structure is called a ferromagnetic helix. It usually belongs to the incommensurate magnetic structures.

As discussed in Section 1.5.1, in studies of the symmetry of magnetically ordered crystals one should take into account not only the crystallographic elements of symmetry (rotations, reﬂections and translations) but also the time-inversion element, which causes the reversal of the magnetic moment density vector mðrÞ. Following Landau & Lifshitz (1957), we shall denote this element by R. If combined with any crystallographic symmetry element G we get a product RG, which some authors call the space-time symmetry operator. We shall not use this terminology in the following. To describe the symmetry properties of magnetically ordered crystals, one should use magnetic point and space groups instead of crystallographic ones, see also Section 1.2.5. By investigating the ‘four-dimensional groups of threedimensional space’, Heesch (1930) found not only the 122 groups that now are known as magnetic point groups but also the seven triclinic and 91 monoclinic magnetic space groups. He also recognized that these groups can be used to describe the symmetry of spin arrangements. The present interest in magnetic symmetry was much stimulated by Shubnikov (1951), who considered the symmetry groups of ﬁgures with black and white faces, which he called antisymmetry groups. The change of colour of the faces in antisymmetry (black–white symmetry, see also Section 3.3.5) corresponds to the element R. These antisymmetry classes were derived as magnetic symmetry point groups by Tavger & Zaitsev (1956). Beside antisymmetry, the concept of colour (or generalized) symmetry also was developed, in which the number of colours is not 2 but 3, 4 or 6 (see Belov et al., 1964; Koptsik & Kuzhukeev, 1972). A different generalization to more than two colours was proposed by van der Waerden & Burckhardt (1961). The various approaches have been compared by Schwarzenberger (1984). As the theories of antisymmetry and of magnetic symmetry evolved often independently, different authors denote the operation of time inversion (black–white exchange) by different symbols. Of the four frequently used symbols (R ¼ E0 ¼ 1 ¼ 10 ) we shall use in this article only two: R and 10 . 1.5.2.1. Magnetic point groups Magnetic point groups may contain rotations, reﬂections, the element R and their combinations. A set of such elements that satisﬁes the group properties is called a magnetic point group. It is obvious that there are 32 trivial magnetic point groups; these are the ordinary crystallographic point groups supplemented by the element R. Each of these point groups contains all the elements of the ordinary point group P and also all the elements of this group P multiplied by R. This type of magnetic point group MP1 can be represented by

110

MP1 ¼ P þ RP:

ð1:5:2:1Þ

Table 1.5.2.1. Comparison of different symbols for magnetic point groups Schoenﬂies D4R D4 D4 ðC 4 Þ D4 ðD2 Þ

Hermann–Mauguin 0

4221 422 420 20 40 220

Shubnikov 4:210 4:2 4:20 40 :2

4:21 4:2 4:2 4:2

1.5. MAGNETIC PROPERTIES The second type of magnetic point group, which is also trivial in some sense, contains all the 32 crystallographic point groups without the element R in any form. For this Elements Magnetic type MP2 ¼ P. Thirteen of these point groups allow point group Schoenﬂies Hermann–Mauguin ferromagnetic spontaneous magnetization (ferroD4R ¼ 42210 E; C2 ; 2C4 ; 2U2 ; 2U2a ; 1; 2x ; 2y ; 2z ; 2xy ; 2xy ; 4z ; magnetism, ferrimagnetism, weak ferromagnetism). They a 0 0 0 0 0 0 0 R; RC2 ; 2RC4 ; 2RU2 ; 2RU2 1 ; 2x ; 2y ; 2z ; 2xy ; 2xy ; 4z are listed in Table 1.5.2.4. The remaining 19 point groups D4 ¼ 422 E; C2 ; 2C4 ; 2U2 ; 2U2a 1; 2x ; 2y ; 2z ; 2xy ; 2xy ; 4z D4 ðC 4 Þ ¼ 420 20 E; C2 ; 2C4 ; 2RU2 ; 2RU2a 1; 2z ; 4z ; 20x ; 20y ; 20xy ; 20xy describe antiferromagnets. The groups MP2 are often D4 ðD2 Þ ¼ 40 220 E; C2z ; C2y ; C2x ; 2RU2a ; 2RC4 1; 2x ; 2y ; 2z ; 20xy ; 20xy ; 40z called ‘white’ magnetic point groups. The third type of magnetic point group MP3, ‘black and white’ groups (which are the only nontrivial ones), These groups are sometimes called ‘grey’ magnetic point groups. contains those point groups in which R enters only in combinaAs pointed out above, all dia- and paramagnets belong to this tion with rotations or reﬂections. There are 58 point groups of this type of point group. To this type belong also antiferromagnets type. Eighteen of them describe different types of ferrowith a magnetic space group that contains translations multiplied magnetism (see Table 1.5.2.4) and the others represent antiferromagnets. by R (space groups of type IIIb). Table 1.5.2.2. Comparison of different symbols for the elements of magnetic point groups

Table 1.5.2.3. The 90 magnetic point groups of types 2 and 3 1

2

3

4

5

6

Symbol of magnetic point group M

1 1 1 0

Symmetry operators of group M 1 1; 1 1; 1 0

2 2 m m 2:m 2:m 2:m 2:m

2 20 m m0 2=m 20 =m0 2=m0 20 =m

121 120 1 1m1 1m0 1 1 m2 1 0 1 m2 0 1 2 1 m0 1 0 1 2m 1

1; 2y 1; 20y 1; my 1; m0y 2y ; my 1; 1; 20y ; m0y 1; 1; 1; 2y ; 1 0 ; m0y 1; my ; 1 0 ; 20y

D2 D2 ðC2 Þ C2v C2v ðC2 Þ C2v ðCs Þ D2h D2h ðC 2h Þ D2h ðD2 Þ D2h ðC 2v Þ

2:2 2:2 2m 2m 2m m2 : m m2 : m m2 : m m2 : m

222 20 20 2 mm2 m0 m0 2 20 m0 m mmm mm0 m0 m0 m0 m0 mmm0

222 20 20 2 mm2 m0 m0 2 20 m0 m

1; 2x ; 2y ; 2z 1; 2z ; 20x ; 20y 1; 2z ; mx ; my 1; 2z ; m0x ; m0y 1; mz ; 20x ; m0y 2x ; 2y ; 2z ; mx ; my ; mz 1; 1; 2x ; mx ; 20y ; 20z ; m0y ; m0z 1; 1; 1; 2x ; 2y ; 2z ; 1 0 ; m0x ; m0y ; m0z 1; 2z ; mx ; my ; 1 0 ; 20x ; 20y ; m0z

C4 C4 ðC 2 Þ S4 S4 ðC 2 Þ C4h C4h ðC 2h Þ C4h ðC 4 Þ C4h ðS4 Þ D4 D4 ðD2 Þ D4 ðC4 Þ C4v C4v ðC2v Þ C4v ðC4 Þ D2d D2d ðD2 Þ D2d ðC 2v Þ D2d ðS4 Þ D4h D4h ðD2h Þ D4h ðC 4h Þ D4h ðD4 Þ D4h ðC 4v Þ D4h ðD2d Þ

4 4 4 4 4:m 4:m 4:m 4:m 4:2 4:2 4:2 4m 4m 4m 4m 4m 4m 4m

4 40 4 0 4 4=m 40 =m 4=m0 40 =m0 422 40 220 420 20 4mm 40 mm0 4m0 m0 42m 0 4 2m0 0 4 m20 420 m0 4=mmm 40 =mmm0 4=mm0 m0 4=m0 m0 m0 4=m0 mm 40 =m0 m0 m

4 40 4 0 4

Schoenﬂies C1 Ci Ci ðC 1 Þ

Shubnikov 1 2 2

Monoclinic

C2 C2 ðC 1 Þ Cs Cs ðC1 Þ C2h C2h ðC i Þ C2h ðC 2 Þ C2h ðC s Þ

Orthorhombic

Tetragonal

Hermann–Mauguin Short Full 1 1 1 0

System Triclinic

m4 : m m4 : m m4 : m m4 : m m4 : m m4 : m

2 2 2 mmm 2 20 20 m m0 m0 2 2 2 m0 m0 m0 20 20 2 m m m0

4 m 40 m 4 m0 40 m0

422 40 220 420 20 4mm 40 mm0 4m0 m0 42m 0 4 2m0 0 4 m20 420 m0 4 2 2 mmm 40 2 20 m m m0 4 20 20 m m0 m0 4 2 2 m0 m0 m0 4 20 20 m0 m m 40 2 20 m0 m0 m

111

1; 2z ; 4z 1; 2z ; 40z 1; 2z ; 4 z 0 1; 2z ; 4 z 2z ; mz ; 4z ; 4 z 1; 1; 2z ; mz ; 40z ; 4 0z 1; 1; 0 1; 2z ; 4z ; 1 0 ; m0z ; 4 z 1; 2z ; 4 z ; 1 0 ; m0z ; 40z 1; 2x ; 2y ; 2z ; 2xy ; 2xy ; 4z 1; 2x ; 2y ; 2z ; 20xy ; 20xy ; 40z 1; 2z ; 4z ; 20x ; 20y ; 20xy ; 20xy 1; 2z ; mx ; my ; mxy ; mxy ; 4z 1; 2z ; mx ; my ; m0xy ; m0xy ; 40z 1; 2z ; 4z ; m0x ; m0y ; m0xy ; m0xy 1; 2x ; 2y ; 2z ; mxy ; mxy ; 4 z 0 1; 2x ; 2y ; 2z ; m0xy ; m0xy ; 4 z 0 0 0 1; 2z ; mx ; my ; 2xy ; 2xy ; 4 z 0 0 0 0 1; 2z ; 4z ; 2x ; 2y ; mxy ; mxy 2x ; 2y ; 2z ; 2xy ; 2xy ; mx ; my ; mz ; mxy ; mxy ; 4z ; 4 z 1; 1; 2x ; 2y ; 2z ; mx ; my ; mz ; 20xy ; 20xy ; m0xy ; m0xy ; 40z ; 4 0z 1; 1; 2z ; mz ; 4z ; 4 z ; 20x ; 20y ; 20xy ; 20xy ; m0x ; m0y ; m0xy ; m0xy 1; 1; 0 1; 2x ; 2y ; 2z ; 2xy ; 2xy ; 4z ; 1 0 ; m0x ; m0y ; m0z ; m0xy ; m0xy ; 4 z 0 0 0 0 0 0 0 1; 2z ; mx ; my ; mxy ; mxy ; 4z ; 1 ; 2x ; 2y ; 2xy ; 2xy ; mz ; 4z 1; 2x ; 2y ; 2z ; mxy ; mxy ; 4 z ; 1 0 ; 20xy ; 20xy ; m0x ; m0y ; m0z ; 40z

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.5.2.3 (cont.) 1

2

3

4

5

6

Symbol of magnetic point group M System Trigonal

Hexagonal

Cubic

Hermann–Mauguin Short Full 3 3 0 3

3 3 0 3

Symmetry operators of group M 1; 3z 3z ; 3 z 1; 1; 0 1; 3z ; 1 0 ; 3 z

3:2 3:2 3m 3m 6m 6m 6m 6m

32 320 3m 3m0 3m 0 3m 0 3 m0 0 3 m

321 320 1 3m1 3m0 1 3 m2 1 0 3 m2 0 1 30 20 1 m 0 0 3 2m 1

1; 3ð2? Þ; 3z 1; 3z ; 3ð20? Þ 1; 3ðm? Þ; 3z 1; 3z ; 3ðm0? Þ 3ð2? Þ; 3ðm? Þ; 3z ; 3 z 1; 1; 3z ; 3 z ; 3ð20? Þ; 3ðm0? Þ 1; 1; 0 1; 3ð2? Þ; 3z ; 1 0 ; 3ðm0? Þ; 3 z 0 1; 3ðm? Þ; 3z ; 1 0 ; 3ð20? Þ; 3 z

C6 C6 ðC 3 Þ C3h C3h ðC 3 Þ C6h C6h ðS6 Þ C6h ðC 6 Þ C6h ðC 3h Þ D6 D6 ðD3 Þ D6 ðC6 Þ C6v C6v ðC3v Þ C6v ðC6 Þ D3h D3h ðD3 Þ D3h ðC 3v Þ D3h ðC 3h Þ D6h D6h ðD3d Þ D6h ðC 6h Þ D6h ðD6 Þ D6h ðC 6v Þ D6h ðD3h Þ

6 6 3:m 3:m 6:m 6:m 6:m 6:m 6:2 6:2 6:2 6m 6m 6m m3 : m m3 : m m3 : m m3 : m m6 : m m6 : m m6 : m m6 : m m6 : m m6 : m

6 60 6 0 6

6 60 6 0 6

6=m 60 =m0 6=m0 60 =m 622 60 220 620 20 6mm 60 mm0 6m0 m0 6m2 60 2m0 0 6 m20 0 20 6m 6=mmm 60 =m0 mm0 6=mm0 m0 6=m0 m0 m0 6=m0 mm 60 =mmm0

6 m 60 m0 6 m0 60 m

1; 2z ; 3z ; 6z 1; 3z ; 20z ; 60z 1; mz ; 3z ; 6 z 0 1; 3z ; m0z ; 6 z 2z ; mz ; 3z ; 3 z ; 6z ; 6 z 1; 1; 3z ; 3 z ; 20z ; m0z ; 60z ; 6 0z 1; 1; 0 0 1; 2z ; 3z ; 6z ; 1 0 ; m0z ; 3 z ; 6 z 0 0 0 1; mz ; 3z ; 6z ; 1 ; 2z ; 3z ; 60z

T Th T h ðTÞ O OðTÞ Td T d ðTÞ Oh Oh ðT h Þ Oh ðOÞ Oh ðT d Þ

3=2 6=2 6=2

23 m3 0 m0 3

23 2 m3 2 0 0 3

3=4 3=4 3=4 3=4 6=4 6=4 6=4 6=4

432 40 320 43m 0 4 3m0 m3m 0 m3m 0 m0 3 m0 0 0 m3m

432 40 320 43m 0 4 3m0 4 2 m3m 40 20 m 3 m0 4 0 2 m0 3 m0 40 0 20 0 3

Schoenﬂies C3 S6 S6 ðC 3 Þ D3 D3 ðC3 Þ C3v C3v ðC3 Þ D3d D3d ðS6 Þ D3d ðD3 Þ D3d ðC 3v Þ

Shubnikov 3 6 6

622 60 220 620 20 6mm 60 mm0 6m0 m0 6m2 60 2m0 0 6 m20 0 20 6m 6 2 2 mmm 60 2 20 m0 m m0 6 20 20 m m0 m0 6 2 2 m0 m0 m0 6 20 20 m0 m m 60 20 2 m m m0

m

m

Replacing R by the identity element E in the magnetic point groups of the third type does not change the number of elements in the point group. Thus each group of the third type MP3 is isomorphic to a group P of the second type. The method of derivation of the nontrivial magnetic groups given below was proposed by Indenbom (1959). Let H denote the set of those elements of the group P which enter into the associated magnetic group MP3 not multiplied by R. The set H contains the identity element E, for each element H also its inverse H 1, and for each pair H1 , H2 also its products H1 H2 and H2 H1 . Thus the set H forms a group. It is a subgroup of the crystallographic group P. Let Pi denote an element of ðP HÞ. All these elements enter MP3 in the form of products RPi because RPi ¼ Pi R and R2 ¼ 1. Multiplying the elements of MP3

m

1; 6ð2? Þ; 2z ; 3z ; 6z 1; 3ð2? Þ; 3z ; 3ð20? Þ; 20z ; 60z 1; 2z ; 3z ; 6z ; 6ð20? Þ 1; 2z ; 6ðm? Þ; 3z ; 6z 1; 3ðm? Þ; 3z ; 20z ; 3ðm0? Þ; 60z 1; 2z ; 3z ; 6z ; 6ðm0? Þ 1; 3ð2? Þ; 3ðm? Þ; mz ; 3z ; 6 z 0 1; 3ð2? Þ; 3z ; 3ðm0? Þ; m0z ; 6 z 0 1; 3ðm? Þ; 3z ; 3ð20? Þ; m0z ; 6 z 0 0 1; mz ; 3z ; 6 z ; 3ð2? Þ; 3ðm? Þ 6ð2? Þ; 2z ; 6ðm? Þ; mz ; 3z ; 3 z ; 6z ; 6 z 1; 1; 3ð2? Þ; 3ðm? Þ; 3z ; 3 z ; 3ð20? Þ; 20z ; 3ðm0? Þ; m0z ; 60z ; 6 0z 1; 1; 2z ; mz ; 3z ; 3 z ; 6z ; 6 z ; 6ð20? Þ; 6ðm0? Þ 1; 1; 0 0 1; 6ð2? Þ; 2z ; 3z ; 6z ; 1 0 ; 6ðm0? Þ; m0z ; 3 z ; 6 z 0 0 0 0 0 1, 2z , 6ðm? Þ, 3z , 6z , 1 , 6ð2? Þ, mz , 3z , 6z 0 0 0 0 1, 3ð2? Þ, 3ðm? Þ, mz , 3z , 6z , 1 , 3ð2? Þ, 2z , 3ðm0? Þ, 3 z , 60z 1, 3ð2Þ, 4ð 3Þ 3ð2Þ, 3ðmÞ, 4ð 3Þ, 4ð 3Þ 1, 1, 0 1, 3ð2Þ, 4ð 3Þ, 1 0 , 3ðm0 Þ, 4ð 3 Þ 1, 9ð2Þ, 4ð 3Þ, 3ð 4Þ 1, 3ð2Þ, 4ð 3Þ, 6ð20 Þ, 3ð 40 Þ 1, 3ð2Þ, 6ðmÞ, 4ð 3Þ, 3ð 4Þ 0 1, 3ð2Þ, 4ð 3Þ, 6ðm0 Þ, 3ð 4 Þ 9ð2Þ, 9ðmÞ, 4ð 3Þ, 4ð 3Þ, 3ð 4Þ, 3ð 4Þ 1, 1, 3ð2Þ, 3ðmÞ, 4ð 3Þ, 4ð 3Þ, 6ð20 Þ, 6ðm0 Þ, 3ð 40 Þ, 3ð 4 0 Þ 1, 1, 0 0 1, 9ð2Þ, 4ð 3Þ, 3ð 4Þ, 1 0 , 9ðm0 Þ, 4ð 3 Þ, 3ð 4 Þ 0 0 0 1 , 6ð2 Þ, 3ðm Þ, 4ð 3 0 Þ, 3ð 40 Þ 1, 3ð2Þ, 6ðmÞ, 4ð 3Þ, 3ð 4Þ,

by a ﬁxed element RP1 corresponds to a permutation of the elements of MP3. This permutation maps each element of the subgroup H on an element of MP3 that does not belong to H and vice versa. It follows that one half of the elements of MP3 are elements of ðP HÞ multiplied by R and the other half belong to H. The relation for the magnetic point groups of the third type may therefore be written as MP3 ¼ H þ RðP HÞ ¼ H þ RP1 H:

ð1:5:2:2Þ

H is therefore a subgroup of index 2 of P. The subgroups of index 2 of P can easily be found using the tables of irreducible representations of the point groups. Every real non-unit onedimensional representation of P contains equal numbers of

112

1.5. MAGNETIC PROPERTIES Table 1.5.2.4. List of the magnetic classes in which ferromagnetism is admitted (a) Triclinic Symbol of symmetry class Schoenﬂies Hermann–Mauguin

Allowed direction of Ms

C1 Ci

Any Any

1 1

(b) Monoclinic Symbol of symmetry class Schoenﬂies Hermann–Mauguin

Allowed direction of Ms

C2 C 2 ðC 1 Þ C s ¼ C 1h C s ðC 1 Þ C 2h C 2h ðC i Þ

k2 ? 20 ?m k m0 k2 k m0

2 20 m m0 2=m 20 =m0

(c) Orthorhombic Symbol of symmetry class Schoenﬂies Hermann–Mauguin D2 ðC 2 Þ C 2v ðC 2 Þ C 2v ðC s Þ D2h ðC 2h Þ

220 20 m0 m0 2 m0 m20 mm0 m0

Allowed direction of Ms k2 k2 ?m ?m

(d) Tetragonal Symbol of symmetry class Schoenﬂies Hermann–Mauguin

Allowed direction of Ms

C4 S4 C 4h D4 ðC 4 Þ C 4v ðC 4 Þ D2d ðS4 Þ D4h ðC 4h Þ

k4 k 4 k4 k4 k4 k 4 k4

4 4 4=m 420 20 4m0 m0 0 m0 42 4=mm0 m0

(e) Trigonal Symbol of symmetry class Schoenﬂies Hermann–Mauguin

Allowed direction of Ms

C3 S6 D3 ðC 3 Þ C 3v ðC 3 Þ D3d ðS6 Þ

k3 k3 k3 k3 k3

3 3 320 3m0 0 3m

(f) Hexagonal Symbol of symmetry class Schoenﬂies Hermann–Mauguin

Allowed direction of Ms

C6 C 3h C 6h D6 ðC 6 Þ C 6v ðC 6 Þ D3h ðC 3h Þ D6h ðC 6h Þ

k6 k 6 k6 k6 k6 k 6 k6

6 6 6=m 620 20 6m0 m0 0 20 6m 6=mm0 m0

characters þ1 and 1. In the corresponding magnetic point group MP3, the elements of P with character 1 are multiplied by R and those with character þ1 remain unchanged. The latter form the subgroup H. This rule can be stated as a theorem: every real non-unit one-dimensional representation of a point group of symmetry P produces an isomorphic mapping of this group upon a magnetic group MP3 (Indenbom, 1959). This concept will be developed in Section 1.5.3. Using the Schoenﬂies symbols and the method described above, the point groups of magnetic symmetry (magnetic point

groups) can be denoted by PðHÞ, where P is the symbol of the original crystallographic point group and H is the symbol of that subgroup the elements of which are not multiplied by R. This notation is often used in the physics literature. In the crystallographic literature, the magnetic groups are deﬁned by Hermann–Mauguin or Shubnikov symbols. In this type of designation, the symbols of elements multiplied by R are primed or underlined. The primed symbols are used in most of the recent publications. The Hermann–Mauguin and Shubnikov deﬁnitions differ slightly, as in the case of crystallographic groups. In Table 1.5.2.1, different symbols of magnetic point groups (trivial and nontrivial ones) are compared. This is done for the family that belongs to the crystallographic point group D4 ¼ 422. The symbols of the symmetry elements of these four magnetic point groups are compared in Table 1.5.2.2. Table 1.5.2.3 gives a list of the 90 magnetic point groups belonging to types 2 and 3. The Schoenﬂies, Shubnikov and Hermann–Mauguin symbols of the point groups are given in the table. The entries in the Hermann–Mauguin symbol refer to symmetry directions, as explained in Section 2.2.4 of International Tables for Crystallography, Vol. A (2005). The elements of symmetry of each point group are displayed using the Hermann– Mauguin symbols. The symbol Nð2? Þ denotes N 180 rotations with axes perpendicular to the principal symmetry axis; Nðm? Þ denotes N mirror planes with normals perpendicular to the principal symmetry axis. Similar deﬁnitions hold for the primed symbols Nð20? Þ and Nðm0? Þ. The point groups are arranged in families. The part of the Schoenﬂies symbol before the bracket is the same for each member of a family. Each family begins with a trivial magnetic point group. It contains the same elements as the corresponding crystallographic point group; its Schoenﬂies symbol contains no brackets. For each nontrivial point group, the list of the elements of symmetry begins with the non-primed elements, which belong to a subgroup H of the head of the family G. The number of the primed elements is equal to the number of non-primed ones and the total number of the elements is the same for all point groups of one family. The overall number of the magnetic point groups of all three types is 122. There are two general statements concerning the magnetic point groups. The element RC3 ¼ 30 does not appear in any of the magnetic point groups of type 3. Only trivial magnetic point groups (of both ﬁrst and second type) belong to the families containing the point groups C1 ¼ 1, C 3 ¼ 3 and T ¼ 23. Only 31 magnetic point groups allow ferromagnetism. The different types of ferromagnetism (one-sublattice ferromagnet, ferrimagnet, weak ferromagnet, any magnetic order with nonzero magnetization) cannot be distinguished by their magnetic symmetry. Ferromagnetism is not admitted in any point group of type 1. For the magnetic point groups of the second type, ferromagnetism is not allowed if the point group contains more than one symmetry axis, more than one mirror plane or a mirror plane that is parallel to the axis. The same restrictions are valid for the point groups of type 3 (if the corresponding elements are not multiplied by R). If the point group contains 1 0, ferromagnetic order is also forbidden. There are the following rules for the orientation of the axial vector of ferromagnetic magnetization M: M k N; M ? 20 ; M ? m, M k m0 . These conditions exclude cubic point groups. Table 1.5.2.4 lists those magnetic point groups that admit ferromagnetic order (Tavger, 1958). The allowed direction of the magnetization vector is given for every point group. Ferromagnetic order is allowed in 13 point groups of the second type and 18 point groups of the third type. All 31 point groups of magnetic symmetry allowing ferromagnetism are subgroups of the inﬁnite noncrystallographic group

113

D1h ðC1h Þ ¼

1 20 : m m0

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES magnetic translation group MT is isometric to the crystallographic one G0 that is obtained by replacing R by E in MT . There are trivial magnetic translation groups, in which none of the translation elements is multiplied by R. The magnetic lattices of these groups coincide with crystallographic lattices. Nontrivial magnetic translation groups can be constructed in analogy to relation (1.5.2.2). Zamorzaev (1957) showed that every translation group T has seven subgroups of index 2. If the basic primitive translations of the group T are a1, a2 , a3 , then the basic primitive translations of the seven subgroups H can be chosen as follows (see also Opechowski & Guccione, 1965) H1 : 2a1 ; a2 ; a3 H2 : a1 ; 2a2 ; a3

ð1:5:2:4Þ ð1:5:2:5Þ

Fig. 1.5.2.1. Magnetic lattices of the triclinic system.

H3 : a1 ; a2 ; 2a3 H4 : 2a1 ; a1 þ a2 ; a3

ð1:5:2:6Þ ð1:5:2:7Þ

The transition from a paramagnetic to a ferromagnetic state is always accompanied by a change of the magnetic symmetry.

H5 : 2a2 ; a2 þ a3 ; a1

ð1:5:2:8Þ

H6 : 2a3 ; a3 þ a1 ; a2 H7 : 2a1 ; a1 þ a2 ; a1 þ a3 :

1.5.2.2. Magnetic lattices If the point group of symmetry describes the macroscopic properties of a crystal, its microscopic structure is determined by the space group, which contains the group of translations T as a subgroup. The elements t of T are deﬁned by the following relation: t ¼ n1 a1 þ n2 a2 þ n3 a3 ;

ð1:5:2:3Þ

where a1, a2 , a3 are basic primitive translation vectors and n1 , n2 , n3 are arbitrary integers. The set of points r0 obtained by applying all the translations of the group T to any point r deﬁnes a lattice. All sites of the crystallographic lattice are equivalent. The translation symmetry of magnetically ordered crystals is described by the magnetic lattices and corresponding magnetic translation groups MT . In the magnetic translation groups MT , some of the elements t may be multiplied by R (we shall call them primed translations). The magnetic lattices then have two types of sites, which are not equivalent. One set is obtained by nonprimed translations and the other set by the primed ones. The

ð1:5:2:9Þ ð1:5:2:10Þ

As an example, let us consider the case (1.5.2.5). In this case, the subgroup H consists of the following translations: tðHÞ ¼ n1 a1 þ 2n2 a2 þ n3 a3 :

ð1:5:2:11Þ

Therefore the elements Gi of ðT HÞ [which corresponds to ðP HÞ in relation (1.5.2.2)] must have the following form: tðGi Þ ¼ n1 a1 þ ð2n2 þ 1Þa2 þ n3 a3 :

ð1:5:2:12Þ

The corresponding magnetic translation group consists of the elements (1.5.2.12) multiplied by R and the elements (1.5.2.11). The crystallographic lattices are classiﬁed into Bravais types or Bravais lattices. The magnetic lattices are classiﬁed into Bravais types of magnetic lattices. It turns out that there are 22 nontrivial magnetic Bravais types. Together with the trivial ones, there are 36 magnetic Bravais lattices. Two types of smallest translation-invariant cells are in common use for the description of magnetically ordered structures: the

Fig. 1.5.2.2. Magnetic lattices of the monoclinic system (the y axis is the twofold axis).

114

1.5. MAGNETIC PROPERTIES

Fig. 1.5.2.3. Magnetic lattices of the orthorhombic system.

crystallographic cell obtained if the magnetic order is neglected and the magnetic cell, which takes the magnetic order into account. The list of the basic translations of all the magnetic Bravais lattices was given by Zamorzaev (1957). The diagrams of the magnetic unit cells were obtained by Belov et al. (1957). In Figs. 1.5.2.1–1.5.2.7, the diagrams of the magnetic unit cells of all 36 Bravais types are sketched in such a way that it is clear to

which family the given cell belongs. All the cells of one family are displayed in one row. Such a row begins with the cell of the trivial magnetic lattice. All nontrivial cells of a family change into the trivial one of this family if R is replaced by E (to draw these diagrams we used those published by Opechowski & Guccione, 1965). Open and full circles are used to show the primed and unprimed translations. A line connecting two circles of the same

115

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.5.2.4. Magnetic lattices of the tetragonal system.

type is an unprimed translation; a line connecting two circles of different types is a primed translation. The arrows in the trivial magnetic cell represent the primitive (primed or unprimed) translations for all the magnetic lattices of the family. The arrows in the nontrivial cells are primitive translations of the magnetic unit cell. The magnetic unit cell of a nontrivial magnetic lattice is generated by unprimed translations only. Its volume is twice the volume of the smallest cell generated by all (primed and unprimed) translations. The reason for this is that one of the primitive translations of the magnetic cell is twice a primitive primed translation. The crystallographic cell of many simple collinear or weakly non-collinear structures coincides with the smallest cell generated by the primed and unprimed translations. However, there are also magnetic structures with more compli-

cated transformations from the crystallographic to the magnetic unit cell. The second line after each part of Figs. 1.5.2.1–1.5.2.7 gives, between braces, an extended vector basis of the magnetic translation group (Shubnikov & Koptsik, 1972). The ﬁrst line gives two symbols for each Bravais type: the symbol to the right was introduced by Opechowski & Guccione (1965). The symbol to the left starts with a lower-case letter giving the crystal system followed by a capital letter giving the centring type of the cell deﬁned by the unprimed translations (P: primitive; C, A, B: C-, A-, B-centred; I: body-centred; F: all-face-centred). The subscript, which appears for the nontrivial Bravais types, indicates the translations that are multiplied by time inversion R. Ferromagnetism is allowed only in trivial magnetic Bravais lattices. All nontrivial magnetic lattices represent antiferromagnetic order. There are only two magnetic sublattices in the simplest antiferromagnetic structures; one sublattice consists of the magnetic ions located in the black sites and the other of the

Fig. 1.5.2.5. Magnetic lattices of the rhombohedral system.

Fig. 1.5.2.6. Magnetic lattices of the hexagonal system.

116

1.5. MAGNETIC PROPERTIES groups of type II describe different ferromagnetic crystals; the remaining antiferromagnets. The nontrivial magnetic space groups belong to type III, MG3 . This consists of 1191 groups, in which R enters only in combination with rotations, reﬂections or translations. These groups have the structure described by relation (1.5.2.2). The magnetic space groups of this type are divided into two subtypes. Subtype IIIa contains those magnetic space groups MG3 in which R is not combined with translations. In these groups, the magnetic translation group is trivial. To these space groups correspond magnetic point groups of type MP3. There are 674 magnetic space groups of subtype IIIa; 231 of them admit ferromagnetism, the remaining 443 describe antiferromagnets. In the magnetic space groups of the subtype IIIb, R is combined with translations and the corresponding point groups are of type MP1. They have a nontrivial magnetic Bravais lattice. There are 517 magnetic space groups of this subtype; they describe antiferromagnets. In summary, the 230 magnetic space groups that describe diaand paramagnets are of type I, the 275 that admit spontaneous magnetization are of types II and IIIa; the remaining 1146 magnetic space groups (types II, IIIa and IIIb) describe antiferromagnets. 1.5.2.4. Exchange symmetry

Fig. 1.5.2.7. Magnetic lattices of the cubic system.

ions located in the white sites. All the magnetic moments of one sublattice are oriented in one direction and those of the other sublattice in the opposite direction. However, antiferromagnetism is allowed also in trivial lattices if the (trivial) magnetic cell contains more than one magnetic ion. The magnetic point group must be nontrivial in this case. The situation is more complicated in case of strongly non-collinear structures. In such structures (triangle, 90 etc.), the magnetic lattice can differ from the crystallographic one despite the fact that none of the translations is multiplied by R. The magnetic elementary cell will possess three or four magnetic ions although the crystallographic cell possesses only one. An example of such a situation is shown in Fig. 1.5.1.3(c). There also exist structures in which the magnetic lattice is incommensurate with the crystallographic one. We shall not discuss the problems of such systems in this chapter. 1.5.2.3. Magnetic space groups There are 1651 magnetic space groups MG, which can be divided into three types. Type I, MG1 , consists of the 230 crystallographic space groups to which R is added. Crystals belonging to these trivial magnetic space groups show no magnetic order; they are para- or diamagnetic. Type II, MG2 , consists of the same 230 crystallographic groups which do not include R in any form. In the magnetically ordered crystals that belong to the magnetic space groups of this type, the magnetic unit cell coincides with the classical one. Forty-four

The classiﬁcation of magnetic structures on the basis of the magnetic (point and space) groups is an exact classiﬁcation. However, it neglects the fundamental role of the exchange energy, which is responsible for the magnetic order (see Sections 1.5.1.2 and 1.5.3.2). To describe the symmetry of the magnetically ordered crystals only by the magnetic space groups means the loss of signiﬁcant information concerning those properties of these materials that are connected with the higher symmetry of the exchange forces. Andreev & Marchenko (1976, 1980) have introduced the concept of exchange symmetry. The exchange forces do not depend on the directions of the spins (magnetic moments) of the ions relative to the crystallographic axes and planes. They depend only on the relative directions of the spins. Thus the exchange group Gex contains an inﬁnite number of rotations U of spin space, i.e. rotations of all the spins (magnetic moments) through the same angle about the same axis. The components of the magnetic moment density mðrÞ transform like scalars under all rotations of spin space. The exchange symmetry group Gex contains those combinations of the space transformation elements, the rotations U of spin space and the element R with respect to which the values mðrÞ are invariant. Setting all the elements U and R equal to the identity transformation, we obtain one of the ordinary crystallographic space groups G. This space group deﬁnes the symmetry of the charge density ðrÞ and of all the magnetic scalars in the crystal. However, the vectors mðrÞ may not be invariant with respect to G. The concept of exchange symmetry makes it possible to classify all the magnetic structures (including the incommensurate ones) with the help of not more than three orthogonal magnetic vectors. We shall discuss this in more detail in Section 1.5.3.3. More information about magnetic symmetry can be found in Birss (1964), Cracknell (1975), Gallego et al. (2012), Joshua (1991), Koptsik (1966), Landau & Lifshitz (1957), Opechowski & Guccione (1965), and Sirotin & Shaskol’skaya (1979).

1.5.3. Phase transitions into a magnetically ordered state Most transitions from a paramagnetic into an ordered magnetic state are second-order phase transitions. A crystal with a given crystallographic symmetry can undergo transitions to different ordered states with different magnetic symmetry. In Section 1.5.3.3, we shall give a short review of the theory of magnetic second-order phase transitions. As was shown by Landau (1937),

117

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.5.3.2. Crystallographic structure of transition-metal oxides of the type -Fe2O3.

1.5.3.1. Magnetic structures in rhombohedral crystals

e63d. Fig. 1.5.3.1. Arrangement of the symmetry elements of the group D

such a transition causes a change in the magnetic symmetry. The magnetic symmetry group of the ordered state is a subgroup of the magnetic group of the material in the paramagnetic state. But ﬁrst we shall give a simple qualitative analysis of such transitions. To ﬁnd out what ordered magnetic structures may be obtained in a given material and to which magnetic group they belong, one has to start by considering the crystallographic space group G of the crystal under consideration. It is obvious that a crystal in which the unit cell contains only one magnetic ion can change into a ferromagnetic state only if the magnetic unit cell of the ordered state coincides with the crystallographic one. If a transition into an antiferromagnetic state occurs, then the magnetic cell in the ordered state will be larger than the crystallographic one if the latter contains only one magnetic ion. Such antiferromagnets usually belong to the subtype IIIb described in Section 1.5.2.3. In Section 1.5.3.1, we shall consider crystals that transform into an antiferromagnetic state without change of the unit cell. This is possible only if the unit cell possesses two or more magnetic ions. To ﬁnd the possible magnetic structures in this case, one has to consider those elements of symmetry which interchange the positions of the ions inside the unit cell (especially glide planes and rotation axes). Some of these elements displace the magnetic ion without changing its magnetic moment, and others change the moment of the ion. It is also essential to know the positions of all these elements in the unit cell. All this information is contained in the space group G. If the magnetic ordering occurs without change of the unit cell, the translation group T in the ordered state does not contain primed elements. Therefore, there is no need to consider the whole crystal space group G. It will sufﬁce to consider the cosets of T in G. Such a coset consists of all elements of G that differ only by a translation. From each coset, a representative with minimum translative component is chosen. We denote a set of such representatives by e G; it can be made into a group by deﬁning AB (A; B 2 e G) as the representative of the coset that contains AB. Obviously, e G is then isomorphic to the factor group G=T and therefore to the point group P of G. Once more, we should like to stress that to construct the magnetic structures and the magnetic groups of a given crystal it is not enough to consider only the point group of the crystal. It is necessary to perform the analysis with the help of its space group in the paramagnetic state or of the corresponding group of coset representatives. An example of such an analysis will be given in the following section.

Following Dzyaloshinskii (1957a), we consider crystals To this belonging to the crystallographic space group D63d ¼ R3c. 2+ 2+ group belong -Fe2O3 and the carbonates of Mn , Co and Ni2+. Weak ferromagnetism was ﬁrst observed in these materials. Cr2O3, in which the magnetoelectric effect was discovered, also belongs to this group. The magnetic ordering in these materials occurs without change of the unit cell. e63d. The representatives of the cosets D63d =T form the group D Its symmetry operations are shown in Fig. 1.5.3.1. Directed along the z axis is the threefold axis C3 and the sixfold roto-inversion axis S~ 6. Three twofold axes U2 run through the points at right angles to the z axis. One of these axes is directed along the x axis. Arranged normal to each of the U2 axes are three glide planes ~ d. The y axis is directed along one of these planes. The centre of inversion I~ is located at the point , lying on the z axis halfway between two points . The sign ~ means that the corresponding operation is accompanied by a translation along the z axis through half the period of the crystal (I~ means that the inversion centre is shifted from the point to the point ). In Fig. 1.5.3.1, the elementary period of translation along the z axis is e63d has the marked by tz. Thus the crystallographic group D following elements: ~ 3 ~ d ; 2S~ 6 E; 2C3 ; 3U2 ; I;

~ 3ðc ¼ mÞ; ~ 3~ z g: f1; 3z ; 3ð2? Þ; 1; ð1:5:3:1Þ

In two types of crystals, considered below, the magnetic ions are arranged on the z axis. If we place the magnetic ion at point 1 located between points and (see Fig. 1.5.3.2), then using symmetry operations (1.5.3.1) we obtain three additional positions for other magnetic ions (points 2, 3, 4). Thus, the elementary cell will contain four magnetic ions. This is the structure of oxides of trivalent ions of iron and chromium (Fe2O3, Cr2O3). The structure of these oxides is shown in Fig. 1.5.3.2. If the positions of the magnetic ions coincide with the positions of the inversion centre , we obtain the structure of the carbonates of the transition metals (MnCO3, CoCO3, NiCO3, FeCO3), which is shown in Fig. 1.5.3.3. Evidently, the formation of a magnetic structure in the crystal does not result in the appearance of new elements of symmetry. The magnetic groups of magnetically ordered crystals may lack some elements contained in the crystallographic group and some of the remaining elements may happen to be multiplied by R (primed). Let us ﬁnd the groups of symmetry that correspond to all possible collinear magnetic structures in rhombohedral crystals with four magnetic ions in the elementary cell. We shall

118

1.5. MAGNETIC PROPERTIES Table 1.5.3.1. Two types of symbols for collinear antiferromagnetic and ferromagnetic structures

Fig. 1.5.3.3. Crystallographic structure of transition-metal carbonates of the type MnCO3.

Fig. 1.5.3.4. Four types of magnetic structures of rhombohedral oxides of transition metals. The direction of l is shown conventionally.

assume that the magnetic moments are located at the points of the ion positions 1–4; they will be marked l . The symmetry transformations cannot change the length of the vectors of the magnetic moments but they can change the direction of these vectors and interchange the positions of the sites 1 $ 4, 2 $ 3 and 1 $ 3, 2 $ 4. This interchange of the vectors l1, l2 , l3 , l4 means that these vectors form a basis of a reducible e63d. The following linear combinarepresentation of the group D e63d : tions of l form irreducible representations1 of D l1 ¼ l1 þ l2 l3 l4 l2 ¼ l1 l2 þ l3 l4 l3 ¼ l1 l2 l3 þ l4 m ¼ l1 þ l2 þ l3 þ l4 :

ð1:5:3:2Þ

Vectors l characterize the antiferromagnetic states and are called antiferromagnetic vectors. The ferromagnetic vector m gives the total magnetic moment of the elementary cell. These vectors describe the four possible collinear magnetic structures. Three are antiferromagnetic structures: A1 (l1 6¼ 0, l2 ¼ l3 ¼ m ¼ 0), A2 (l2 6¼ 0, l3 ¼ l1 ¼ m ¼ 0), A3 (l3 6¼ 0, l1 ¼ l2 ¼ m ¼ 0) and one is a ferromagnetic structure, F (m 6¼ 0, l1 ¼ l2 ¼ l3 ¼ 0). All these types are presented schematically in Fig. 1.5.3.4. e63d is mapped on the By omitting its translative part, each element of D This mapping also corresponding element of the point group D3d ¼ 3m. e63d establishes a one-to-one correspondence between the representations of D and those of D3d ¼ 3m. 1

Symbol

Alternative symbol

A1 A2 A3 F

A G C F

In the description of the structures of orthoferrites, other symbols were introduced to deﬁne the linear combinations of l and to denote the antiferromagnetic structures under consideration (see Bertaut, 1963). The two types of symbols are compared in Table 1.5.3.1. It should be borne in mind that in each of these types of magnetic ordering the respective vectors l and m may be directed along any direction. There are 12 types of such structures in which l or m are directed along one of the axes or planes of symmetry. To ﬁnd out to which group of magnetic symmetry each of these structures belongs, one needs to investigate how each element of the crystallographic symmetry transforms the Cartesian components of the four vectors. This is shown in Table e63d. If the component keeps its direction, it 1.5.3.2 for the group D is marked by the þ sign; the sign corresponds to reversal of the component direction. In some cases, the transformation results in a change of the direction of the components li or mi through an angle other than 0 or . This is marked by 0. With the help of Table 1.5.3.2, we can easily describe all the elements of symmetry of the magnetic group that corresponds to each structure (Ai or F i ) with the aid of the following rule. All the elements that yield the þ sign are included in the magnetic group as they stand, while the elements yielding the sign must be multiplied by R; the elements which are marked by the sign 0 are not included in the magnetic group.2 With the aid of this rule, Table 1.5.3.3 of the elements of the magnetic groups for the structures under consideration was compiled. In Table 1.5.3.4, the symbols of the magnetic point groups of all the 12 magnetic structures considered are listed. The crystals with two ions in the elementary cell have only two sublattices and their antiferromagnetic structures belong to the same groups as the structures A3i ¼ Ci. One can see from Tables 1.5.3.3 and 1.5.3.4 that, in accordance with general theory, the magnetic point groups of the crystals under consideration are subgroups of the trivial magnetic point 0, to which they belong in the paramagnetic group D3dR ¼ 3m1 state. In the example considered, the translation group does not change in going from the paramagnetic to the ordered state. Thus the same statement made for the point groups is also true for the space groups. Putting R ¼ E gives a subgroup of the crystallographic group of the crystal. For the magnetic structures with the ferromagnetic or antiferromagnetic vector directed along the z axis, it turns out that the magnetic group is isomorphic to the crystallographic group. This rule is obeyed by all (optically) uniaxial crystals if the transition occurs without change of the elementary cell. (Optically uniaxial are the non-cubic crystals with a point group possessing a threefold, fourfold or sixfold axis.) Tables 1.5.3.3 and 1.5.3.4 show that different types of collinear structures may belong to the same point group (and also to the same space group). For the antiferromagnetic structure A3y and the ferromagnetic F x the group is 2=m, and for the structures A3x and F y it is 20 =m0. Thus the symmetry allows a phase to be simultaneously ferromagnetic and antiferromagnetic. That is not ferrimagnetic order because all the ions in the four sublattices are identical and their numbers are equal. The ferromagnetic vector 2 In Section 1.5.3.3, we shall show that this rule corresponds in the Landau theory of phase transitions to the general law that the magnetically ordered state is described by Li or Mi , which form the basis of one of the irreducible representations of the paramagnetic space group of the crystal.

119

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES e63d in rhombohedral crystals Table 1.5.3.2. Sign variation of the components of antiferromagnetic and ferromagnetic vectors during transformations of the group D with four magnetic ions Elements of symmetry U21 E 2C3

U22

U23

~d2

~ d3

3z

2x

2ð2Þ ?

ð3Þ 2?

I~ 1~

~ d1

1

cx

cð2Þ ?

cð3Þ ?

2S~ 6

3~

l1x l1y l1z

+ + +

0 0 +

+

0 0

0 0

+ +

0 0 +

0 0 +

0 0

l2x l2y l2z

+ + +

0 0 +

+ +

0 0 +

0 0 +

+

0 0

0 0

0 0

l3x l3y l3z

+ + +

0 0 +

+ +

0 0 +

0 0 +

+ + +

+ +

0 0 +

0 0 +

0 0 +

mx my mz

+ + +

0 0 +

+

0 0

0 0

+ + +

+

0 0

0 0

0 0 +

Vector components

m and the antiferromagnetic one l3 are perpendicular and jmj jl3 j. This phenomenon is called weak ferromagnetism and will be discussed in detail in Section 1.5.5.1. Like weak ferromagnetism, the symmetry also allows the coexistence of two orthogonal antiferromagnetic structures A1 and A2 . This gives rise to weakly non-collinear antiferromagnetic structures. The strongly non-collinear structures are described by another set of basis vectors for the irreducible representations of the ~ If the magnetic ions l in the crystal form triangular group G. planes, one gets instead of (1.5.3.2) the relations for the basis vectors (see Fig. 1.5.1.3c): pﬃﬃﬃ l1 ¼ 3ðl2 l1 Þ l2 ¼ l1 þ l2 l3

ð1:5:3:3Þ

m ¼ l1 þ l2 þ l3 :

1.5.3.2. Exchange and magnetic anisotropy energies It is pertinent to compare the different kinds of interactions that are responsible for magnetic ordering. In general, all these interactions are much smaller than the electrostatic interactions between the atoms that determine the chemical bonds in the material. Therefore, if a crystal undergoes a transition into a magnetically ordered state, the deformations of the crystal that give rise to the change of its crystallographic symmetry are comparatively small. It means that most of the non-magnetic properties do not change drastically. As an example, the anisotropic deformation of the crystal that accompanies the transition into the ordered state (see Section 1.5.9.1) is mostly not larger than 104. The formation of the ordered magnetic structures is due mainly to the exchange interaction between the spins S (and corresponding magnetic moments l of the atoms or ions). The expression for the exchange energy can contain the following terms [see formula (1.5.1.7)]:

The exchange interaction decreases rapidly as the distance between the atoms rises. Thus, it is usually sufﬁcient to consider the interaction only between nearest neighbours. The exchange interaction depends only on the relative alignment of the spin moments and does not depend on their alignment relative to the crystal lattice. Therefore, being responsible for the magnetic ordering in the crystal, it cannot deﬁne the direction of the spontaneous magnetization in ferromagnets or of the antiferromagnetic vector. This direction is determined by the spin– orbit and magnetic spin–spin interactions, which are often called relativistic interactions as they are small, of the order of v2 =c2, where v is the velocity of atomic electrons and c is the speed of light. The relativistic interactions are responsible for the magnetic anisotropy energy, which depends on the direction of the magnetic moments of the ions with regard to the crystal lattice. The value of the exchange energy can be represented by the effective exchange ﬁeld He. For a magnetically ordered crystal with a transition temperature of 100 K, He ’ 1000 kOe ’ 108 A m1. Thus, the external magnetic ﬁeld hardly changes the value of the magnetization M or of the antiferromagnetic vector L; they are conserved quantities to a good approximation. The effective anisotropy ﬁeld Ha in cubic crystals is very small: 1–10 Oe ’ 102–103 A m1. In most non-cubic materials, Ha is not larger than 1–10 kOe ’ 105–106 A m1. This means that, by applying an external magnetic ﬁeld, we can change only the direction of M, or sometimes of L, but not their magnitudes. The magnetic anisotropy energy density Ua can be represented as an expansion in the powers of the components of the vectors M or L. The dependence of Ua on the direction of the magnetization is essential. Therefore, one usually considers the expansion of the spontaneous magnetization or antiferromagnetic vector in powers of the unit vector n. The anisotropy energy is invariant under time reversal. Therefore, the general expression for this energy has the form Ua ¼ Kij ni nj þ Kijk‘ ni nj nk n‘ þ Kijk‘mn ni nj nk n‘ nm nn ;

ð1:5:3:5Þ

ð1:5:3:4Þ

where Kij, Kijk‘ , Kijk‘mn are tensors, the components of which have the dimension of an energy density. The forms of the tensors depend on the symmetry of the crystal. There are at most two

Table 1.5.3.3. Magnetic groups of symmetry in rhombohedral oxides of trivalent transition-metal ions

Table 1.5.3.4. Magnetic point groups in rhombohedral oxides of transition metals

S S ; S ½S S :

Type of magnetic structure

Magnetic moments are directed along the axis x

y

z

A1 ¼ A A2 ¼ G A3 ¼ C F¼F

~ ~d R E; U2 ; IR; E; U2 R; I~ R; ~ d E; U2 R; I~ ; ~d R ~ ~d E; U2 ; I;

~ ~d E; U2 R; IR; E; U2 ; I~ R; ~ d R E; U2 ; I~ ; ~d ~ ~ d R E; U2 R; I;

E; E; E; E;

~ 3 ~d ; 2S~ 6 R 2C3 ; 3U2 R; IR; 2C3 ; 3U2 ; I~ R; 3 ~d R; 2S~ 6 R 2C3 ; 3U2 ; I~ ; 3 ~ d ; 2S~ 6 ~ 3 ~d R; 2S~ 6 2C3 ; 3U2 R; I;

120

Type of magnetic structure

Magnetic moments are directed along the axis x

y

z

A1 ¼ A A2 ¼ G A3 ¼ C F¼F

C 2h ðC2 Þ ¼ 2=m0 C 2h ðCs Þ ¼ 20 =m C 2h ðCi Þ ¼ 20 =m0 C 2h ¼ 2=m

C 2h ðC s Þ ¼ 20 =m C 2h ðC 2 Þ ¼ 2=m0 C 2h ¼ 2=m C 2h ðC i Þ ¼ 20 =m0

D3d ðC 3v Þ ¼ 3 0 m D3d ðD3 Þ ¼ 3 0 m0 D3d ¼ 3m 0 D3d ðS6 Þ ¼ 3m

1.5. MAGNETIC PROPERTIES Ua ð6Þ ¼ K1 ðn2x þ n2y Þ þ K2 ðn2x þ n2y Þ2

independent components in Kij . For a uniaxial crystal, the second-order term in the anisotropy energy expansion is determined by one anisotropy constant, K. Instead of using the components of the unit vector n, its direction can be described by two angles: polar and azimuthal ’. Correspondingly, the anisotropy energy for a uniaxial crystal can be written as Ua ¼ Kðn2x þ n2y Þ ¼ K sin2 :

ð1:5:3:6Þ

This relation is equivalent to Ua ¼ Kð1 n2z Þ ¼ K K cos2 :

Ua ð4Þ ¼ K1 ðn2x þ n2y Þ þ K2 ðn2x þ n2y Þ2 þ Kxxyy n2x n2y 4

4

¼ K1 sin2 þ K2 sin4 þ K?00 sin6 cos 6’; ð1:5:3:10Þ where x and ’ have the same meaning as in (1.5.3.9). The symmetry of cubic crystals does not allow any secondorder terms in the expansion of the anisotropy energy. The expression for the anisotropy energy of cubic crystals contains the following invariants: Ua ðcubÞ ¼ K1 ðn2x n2y þ n2x n2z þ n2y n2z Þ þ K2 n2x n2y n2z :

ð1:5:3:7Þ

The direction of the magnetization vector M in a ferromagnet or of the antiferromagnetic vector L in an antiferromagnet is called the direction or the axis of easy magnetization. The crystals in which this axis is aligned with a threefold, fourfold or sixfold axis of the magnetic point group are called easy-axis magnets. The magnetic crystals with the main axis higher than twofold in the paramagnetic state in which, in the ordered state, L (or M) is perpendicular to this axis are often called easy-plane magnets. The anisotropy in this plane is usually extremely small. In this case, the crystal possesses more than one axis of easy magnetization and the crystal is usually in a multidomain state (see Section 1.5.4). If the anisotropy constant K is positive, then the vector n is aligned along the z axis, and such a magnet is an easy-axis one. For an easy-plane magnet, K is negative. It is convenient to use equation (1.5.3.6) for easy-axis magnets and equation (1.5.3.7) for easy-plane magnets. In the latter case, the quantity K is included in the isotropic part of the thermodynamic potential , and (1.5.3.7) becomes Ua ¼ K cos2 . Instead, we shall write Ua ¼ K cos2 in the following, so that K becomes positive for easyplane ferromagnetics as well. Apart from the second-order term, terms of higher order must be taken into account. For tetragonal crystals, the symmetry allows the following invariant terms in the anisotropy energy:

2

þ K?00 12 ½ðnx þ iny Þ6 þ ðnx iny Þ6

ð1:5:3:11Þ

In considering the anisotropy energy, one has to take into account spontaneous magnetostriction and magnetoelastic energy (see Section 1.5.9). This is especially important in cubic crystals. Any collinear cubic magnet (being brought into a single domain state) ceases to possess cubic crystallochemical symmetry as a result of spontaneous magnetostriction. If K1 is positive, the easy axis is aligned along one of the edges of the cube and the crystal becomes tetragonal (like Fe). If K1 is negative, the crystal becomes rhombohedral and can be an easy-axis magnet with vector n parallel to one of the spatial diagonals (like Ni) or an easy-plane magnet with n perpendicular to a spatial diagonal. We shall discuss this topic in more detail in Section 1.5.9.3. The considerations presented above can be applied to all crystals belonging in the paramagnetic state to the tetragonal, trigonal or hexagonal system that become easy-plane magnets in the ordered state. All of them, including the cubic crystals, may possess more than one allowed direction of easy magnetization. In the example considered in the previous section, these directions can be aligned along the three twofold axes for the structures Ax1 ; Ax2 ; Ax3 ; F x and can be parallel to the three mirror planes for Ay1 ; Ay2 ; Ay3 ; F y . It is worth noting that in some applications it is more convenient to use an expansion of the anisotropy energy in terms of surface spherical harmonics. This problem has been considered in detail by Birss (1964). 1.5.3.3. The thermodynamic theory of transitions into a magnetically ordered state

2

¼ K1 sin þ K2 sin þ K? sin sin 2’; ð1:5:3:8Þ the azimuthal angle ’ is measured from the twofold axis x in the basal plane and the constant K? determines the anisotropy in the basal plane. Trigonal symmetry also allows second- and fourth-order invariants: Ua ð3Þ ¼ K1 ðn2x þ n2y Þ þ K2 ðn2x þ n2y Þ2 þ K?0 12 nz ½ðnx þ iny Þ3 þ ðnx iny Þ3 ¼ K1 sin2 þ K2 sin4 þ K?0 cos sin3 cos 3’; ð1:5:3:9Þ where ’ is measured from the x axis, which is chosen parallel to one of the twofold axes. For easy-plane magnets and K?0 > 0, the vector n is directed along one of the twofold axes in the basal plane. If K?0 is negative, then n lies in a vertical mirror plane directed at a small angle to the basal plane. For the complete solution of this problem, the sixth-order term must be taken into account. This term is similar to the one that characterizes the anisotropy of hexagonal crystals. The expression for the latter is of the following form:

According to Landau (1937) (see also Landau & Lifshitz, 1951), a phase transition of the second kind can be described by an order parameter , which varies smoothly in the neighbourhood of the transition temperature Tc. The order parameter ¼ 0 when T Tc and rises continuously as the temperature is decreased below Tc, but the symmetry of the crystal changes suddenly. The order parameter can be a scalar, a vector or a tensor. Consider a crystal with known space group in the paramagnetic state. In this section, we show how the Landau theory allows us to determine the magnetic space groups that are possible after a second-kind phase transition into an ordered state. The application of the Landau theory to the magnetic transitions into different types of antiferromagnets was made by Dzyaloshinskii (1957a,c; 1964). In these cases, the order parameter is the magnetic moment density mðrÞ. To determine the equilibrium form of this function, it is necessary to ﬁnd the minimum of the thermodynamic potential , which is a functional of mðrÞ. Since the transition is continuous and mðrÞ ¼ 0 for T Tc , the value of mðrÞ must be very small in the neighbourhood below the transition point. In this region, the thermodynamic potential will be expanded into a power series of mðrÞ. To ﬁnd the proper form of this expansion, it is convenient to represent mðrÞ as a linear combination of functions that form bases of the irreducible representations of the space group of the paramagnetic phase MG :

121

i

m ðrÞ ¼

P

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES i Mn; ’n; ðrÞ;

ð1:5:3:12Þ

n;

where ’n; ðrÞ are functions that transform under the representation n ( is the number of the function in the representai are tion) and i ¼ x; y; z. In this expansion, the quantities Mn; independent of r and transform with respect to i as the components of an axial vector. The functions ’n; ðrÞ are transformed into combinations of one another by the elements of the group MG . Instead, these elements can be regarded as transforming the i coefﬁcients Mn; and leaving the functions ’n; invariant. In this i case, the quantities Mn; transform according to the direct product of the representation n of MG and the representation formed by the components of the pseudovector. This representation is reducible in the general case. Irreducible representations p; q; . . . can be obtained by forming linear i . Let us denote these combinations by combinations of the Mn; cp; ; cq; ; . . .. These variables can be considered as components of the order parameter, and the thermodynamic potential can be expanded into a power series of cp;. The terms of this expansion must be invariant under the transformations of the magnetic space group of the crystal in the paramagnetic state MG. This group possesses R as a separate element. Therefore the expansion can contain only even terms. For each irreducible representation, there is only one invariant of second order – the sum of the squares. Consequently, retaining only the square terms, the expansion of the thermodynamic potential has the form: P P ð1:5:3:13Þ ðTÞ ¼ 0 ðTÞ þ Ap ðTÞ c2p; : p

To minimize , it is necessary to add the terms of the fourth power. All the coefﬁcients Ap ðTÞ in the relation (1.5.3.13) depend on the temperature. At T Tc all cp; ¼ 0. This solution corresponds to the minimum of if all Ap ðTÞ are positive. The transition into the ordered state occurs if one of the quantities Ap ðTÞ changes its sign. This means that the transition temperature Tc is the temperature at which one of the coefﬁcients Ap ðTc Þ ¼ 0. This coefﬁcient has the form: Ap ðTÞ ¼ ðT Tc Þ:

As an example, let us consider a magnetic transition in UO2. In the paramagnetic state, it is a crystal with a face-centred cubic (for details see Dzyastructure (space group O5h ¼ Fm3m) loshinskii & Man’ko, 1964; Izyumov & Naish, 1979; Izyumov, Naish & Petrov, 1979; Izyumov, Naish & Syromiatnikov, 1979; Barbara et al., 1988). Primitive translations of the crystallographic lattice are (see Fig. 1.5.3.5): a1 ¼ ða=2Þð0; 1; 1Þ;

ð1:5:3:15Þ

where the values of the vectors k are conﬁned to the Brillouin zone in the reciprocal lattice and the function uk ðrÞ is periodic in the real lattice. The irreducible representation deﬁned by the vector k contains the functions with all the vectors k that belong to the same star. The star is the set of the vectors k

obtained by applying all the transformations gi of the corresponding point group to any vector of the star (see also Section 1.2.3.3). If we denote it as k1, then the set of the vectors of the star consists of all inequivalent vectors of the form gi k1 . There are three types of transition we have to consider: (1) the magnetic lattice is commensurate with the crystallographic one and k 6¼ 0; (2) the magnetic lattice is incommensurate with the crystallographic one; (3) k ¼ 0 and the magnetic lattice coincides with the crystallographic lattice. Below we shall discuss in detail only the ﬁrst and the third type of transition. (1) k 6¼ 0. It is found that the ﬁrst type of transition occurs if the arms of the star k are aligned along speciﬁc crystallographic directions and that its vectors are equal to 1/2, 1/3 or 1/4 of some translation in the reciprocal lattice (Lifshitz, 1942). Then, the magnetic structure is described by one of the 22 nontrivial Bravais types of magnetic lattices shown in Figs. 1.5.2.1–1.5.2.7.

a2 ¼ ða=2Þð1; 0; 1Þ;

a3 ¼ ða=2Þð1; 1; 0Þ: ð1:5:3:16Þ

Primitive translations of the reciprocal lattice are:

ð1:5:3:14Þ

Accordingly, the corresponding magnetic structure is deﬁned by the order parameters cp; and belongs to the representation p. The representation of the space group is realized by a set of functions of the following type: ’k ðrÞ ¼ uk ðrÞ expðik rÞ;

Fig. 1.5.3.5. The conventional unit cell of UO2. Only the positions of the magnetic U4+ ions are shown. The vectors a1, a2 , a3 form a basis of a primitive cell of the crystallographic lattice; l1 , l2 , l3 , l4 are the magnetic moments of the ions belonging to the four magnetic lattices.

b1 ¼ ð2=aÞð1; 1; 1Þ;

b2 ¼ ð2=aÞð1; 1; 1Þ;

b3 ¼ ð2=aÞð1; 1; 1Þ:

ð1:5:3:17Þ

Let us assume that there is one magnetic ion in the primitive cell in the position (0, 0, 0) and that the transition takes place over a three-armed star fK10 g (for the deﬁnition of the symbols of the stars see Kovalev, 1987): k1 ¼ ðb1 þ b2 Þ=2 ¼ ð2=aÞð0; 0; 1Þ k2 ¼ ðb1 þ b3 Þ=2 ¼ ð2=aÞð0; 1; 0Þ

ð1:5:3:18Þ

k3 ¼ ðb2 þ b3 Þ=2 ¼ ð2=aÞð1; 0; 0Þ: If l1 is the magnetic moment at the site (0, 0, 0), the value of li ðkj Þ at ti ¼ ða=2Þðhi ; ki ; li Þ may be obtained for each kj with the help of the following relation: li ðkj Þ ¼ l1 exp½iðkj ti Þ:

ð1:5:3:19Þ

From this relation, it follows that li ðkj Þ ¼ l1 for different combinations of ti and kj . The signs of the magnetic moments li at the four sites at the corner and the face centres of the conventional unit cell are displayed in Table 1.5.3.5. Table 1.5.3.5 shows that for each arm of the vector star kj, there exists a linear combination of the four vectors li (i ¼ lattice site) which is a basis of the representation of one of the arms. According to Table 1.5.3.5, these linear combinations have the following forms:

122

1.5. MAGNETIC PROPERTIES Table 1.5.3.5. The signs of li ðkj Þ for four sites ti of the conventional unit cell (the corners of a primitive cell)

k1 k2 k3

t1 a(0; 0; 0)

t2 ða=2Þ(0; 1; 1)

t3 ða=2Þ(1; 0; 1)

t4 ða=2Þ(1; 1; 0)

+ + +

+

+

+

l1 ¼ l1 þ l2 l3 l4 l2 ¼ l1 l2 þ l3 l4 l3 ¼ l1 l2 l3 þ l4 :

ð1:5:3:20Þ

None of the vectors l is a basis of an irreducible representa in the case under tion of the whole space group O5h ¼ Fm3m consideration. The basis functions of the irreducible representation are formed by linear superposition of the basis functions of each arm. One of these representations, 3 , is a superposition of the following components of l : l1x , l2y and l3z . This corresponds to the following orientations of the magnetic moments located in different corners of the primitive unit cell: 1; 1; l2 ½1; 1; 1; l3 ½1; 1; 1; l4 ½1; 1; 1: l1 ½1; ð1:5:3:21Þ Thus the magnetic structure of UO2 consists of four primitive cubic magnetic sublattices Mi inserted into each other. According to (1.5.3.21), the magnetization vectors of these sublattices Mi are aligned along the space diagonals of the cubic lattice. This magnetic structure for UO2 was predicted theoretically by Dzyaloshinskii & Man’ko (1964) (using the representation approach in the way discussed above) and established by neutron scattering by Faber et al. (1975). This example shows that the Landau theory can solve complicated problems of phase transitions where the magnetic lattice does not coincide with the crystallographic one and where the magnetic structure is strongly non-collinear. Here only a qualitative analysis has been given; Section 1.5.3.3.1 and Section 1.5.3.3.2 will be devoted to quantitative solutions connected with phase transitions into an ordered state. As was discussed in Section 1.5.2, Andreev & Marchenko (1976, 1980) introduced the concept of exchange magnetic symmetry. This concept is based on neglecting the relativistic interactions in comparison with the exchange interaction. In such an approach, the orientation of the magnetic moments relative to the crystallographic axis is arbitrary and the crystallographic transformations act on the magnetic moments not as on vectors but as on scalars. In the exchange approximation, three magnetic vectors can be introduced that describe any magnetic structure. These vectors are mutually orthogonal. All magnetic structures can be classiﬁed into four types. (1) Collinear ferromagnets or ferrimagnets are described by one ferromagnetic vector M. (2) Collinear antiferromagnets are described by one antiferromagnetic vector L. (3) Non-collinear ferromagnets are described by one ferromagnetic vector M and one or two antiferromagnetic vectors L. (4) Non-collinear antiferromagnets are

described by two or three antiferromagnetic vectors L. The Andreev and Marchenko approach describes the magnetic structure of UO2 considered above by three antiferromagnetic vectors, which are aligned along [1, 0, 0], [0, 1, 0] and [0, 0, 1], respectively. (2) Incommensurate structures (see also Section 1.10.1). In the second type of transition, k differs slightly from one of the rational values (1/2, 1/3, 1/4). Then the magnetic structure is incommensurate with the crystallographic lattice. Such noncollinear structures are shown in Fig. 1.5.1.4 (antiferromagnetic and ferromagnetic helices). A detailed analysis of this problem is given by Andreev & Marchenko (1976, 1980). (3) k ¼ 0. To the third type belong transitions for which k ¼ 0. In this case, the magnetic primitive cell coincides with the crystallographic one and antiferromagnetic ordering is allowed only if there is more than one magnetic ion in the primitive cell. As stated above, only this type of ordering allows collinear ferromagnetism. Therefore, we shall discuss this type of transition later in more detail. Let us consider the phase transition in a uniaxial crystal with four magnetic ions in the primitive cell, as was done by Dzyaloshinskii (1957a). Now the average density of the magnetic moment mi ðrÞ in (1.5.3.12) is determined by the average values of the magnetic moments of each ion, l1 ; l2 ; l3 ; l4 . In (1.5.3.12), i there is no longer any need to distinguish the coefﬁcients Mn and i the functions ’n; ðrÞ. Their product Mn; ’n; ðrÞ is now replaced by the linear combinations of the components of l1 ; l2 ; l3 ; l4 transforming according to the corresponding irreducible representation of the point group P of the crystal (the space group of which is G). To illustrate this, we shall take for G the group D63d ¼ R3c, which was discussed in Section 1.5.3.1. There we introduced the linear combinations (1.5.3.2) l1 ; l2 , l3 ; m of the vectors l1, l2 , l3 , l4 . The components of these linear combinations are basis functions of the irreducible representations of the corresponding point group D3d ¼ 3m. The characters of the representations of this group are given in Table 1.5.3.6. It follows from this table that all z components of the vectors l and m are transformed according to different one-dimensional representations of D3d (i.e. 1 ; . . . ; 4 ). Following the rule introduced in Section 1.5.2.1 [see relation (1.5.2.2)], we established the magnetic point groups displayed in the last column of Table 1.5.3.6. The symbols for the magnetic structures are given in the corresponding column. The x, y components are transformed by two-dimensional representations: mx ; my and l3x ; l3y are transformed according to the same representation 5 ; a similar situation holds for the pairs l1x ; l1y and l2x ; l2y , which are transformed according to 6. It is obvious that if the magnetic structure possesses x; y components of the magnetic vectors, the magnetic point group (which must be a subgroup of D3d ) will contain only four elements of the group D3d : E, C2 , I, ? . These elements form the point group C 2h ¼ 2=m. The point group C 2h has four one-dimensional representations, which according to relation (1.5.2.2) generate the four magnetic point groups listed in the last column of Table 1.5.3.6. To each of these magnetic point groups corresponds a deﬁnite magnetic structure, which is a

and corresponding magnetic structures Table 1.5.3.6. Characters of the irreducible representations of the group D3d ¼ 3m

Representation 1 2 3 4 5 6

Magnetic vector components l3z mz l1z l2z l3x my mx l3y l1x l2y l2x l1y

Elements of symmetry E

2C3

3U2

I

2S6

3 d

1 1 1 1 2

1 1 1 1 1

1 1 1 1 0

1 1 1 1 2

1 1 1 1 1

1 1 1 1 0

2

1

0

2

1

0

123

Magnetic structure Cz Fz Az Gz Cx F y Cy F x Ax Gy Ay Gx

Magnetic point group D3d ¼ 3m 0 D3d ðS6 Þ ¼ 3m D3d ðC 3v Þ ¼ 3 0 m D3d ðD3 Þ ¼ 3 0 m0 C2h ðCi Þ ¼ 20 =m0 C2h ¼ 2=m C2h ðC2 Þ ¼ 2=m0 C2h ðCs Þ ¼ 20 =m

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES mixture of x and y components of l3 and m or l1 and l2 . The symbols of these structures are also listed in the table (by deﬁnition, the twofold axis is aligned along the x axis). According to the relation (1.5.3.13), the thermodynamic potential contains a sum of quadratic terms of basis functions for each irreducible representation. Thus it contains the following invariants, which correspond to the one-dimensional representations: 2 2 2 þ A02 l2z þ A03 l3z þ B0 m2z : A01 l1z

ð1:5:3:22Þ

The invariants formed with the x, y components of the vectors l1, l2 , l3 , m, which are basis functions of two-dimensional representations, have the following form: 2 A001 ðl1x

þ

2 l1y Þ

þ

2 A002 ðl2x

þ

2 l2y Þ

þ

2 A003 ðl3x

þ

2 l3y Þ

00

þB

ðm2x

þ

m2y Þ:

ð1:5:3:23Þ The thermodynamic potential for any uniaxial crystal possesses such invariants of second order. For crystals belonging to the space group D63d, it is possible to construct additional invariants, which are linear combinations of the mixed products of the x and y components of the pairs of vectors l1, l2 and l3 ; m and are transformed according to the same two-dimensional representations. These invariants have the following form: l1x l2y l1y l2x ;

l3x my l3y mx :

which is determined by minimization of the thermodynamic potential (1.5.3.27). As examples, we shall consider in the next two sections the simplest cases, the uniaxial ferromagnet and the uniaxial antiferromagnet. When doing this, we shall not restrict ourselves to a certain crystallographic structure as in the case above. For the sake of simplicity, it will be assumed that the primitive cell contains only two magnetic ions and therefore there is only one antiferromagnetic vector l. Further, we shall introduce new variables: M ¼ ðN=2Þm;

L ¼ ðN=2Þl;

ð1:5:3:28Þ

where N is the number of magnetic ions per volume unit. 1.5.3.3.1. Uniaxial ferromagnet The temperature of transition from the paramagnetic to the ferromagnetic state is called the Curie temperature. The thermodynamic treatment of the behaviour of uniaxial ferromagnets in the neighbourhood of the Curie temperature TC is given below. In the case of a ferromagnet ðL ¼ 0Þ, the thermodynamic potential (1.5.3.27) near TC including the magnetic energy 0 MH is given by (see 1.5.3.25) ~ ¼ 0 þ ðB=2ÞM2 þ ðb=2ÞðMx2 þ My2 Þ þ ðC=4ÞM4 0 MH;

ð1:5:3:24Þ

ð1:5:3:29Þ

These terms are responsible for ‘weakly non-collinear’ structures; we discuss their properties in Section 1.5.5 and shall not take them into account now. Before writing the whole expression of the thermodynamic potential, let us combine expressions (1.5.3.22) and (1.5.3.23) to separate the exchange terms from the relativistic ones. This can be performed in two ways:

~ is used to designate the thermodynamic potential in where variables p; T; H [instead of ðp; T; MÞ]. The equilibrium value of the magnetization M is found by minimizing the thermo~ dynamic potential . First consider the ferromagnet in the absence of the external ~ ﬁeld ðH ¼ 0Þ. The system of equations @[email protected] ¼ 0 has three solutions:

2 2 2 2 A01 l1z þ A001 ðl1x þ l1y Þ ¼ ðA1 =2Þl21 þ ða1 =2Þl1z 2 A01 l1z

þ

2 A001 ðl1x

þ

2 l1y Þ

¼

ðA1 =2Þl21

þ

2 ða1 =2Þðl1x

or

ðIÞ

2 þ l1y Þ:

ð1:5:3:25Þ Similar rearrangements are performed for l2 , l3 and m. Summing expressions (1.5.3.22) and (1.5.3.23) and taking into account expression (1.5.3.25), we obtain the ﬁnal expression for the thermodynamic potential limited to terms of second order: 1 ¼ 0 þ ðA1 =2Þl21 þ ðA2 =2Þl22 þ ðA3 =2Þl23 þ ðB=2Þm2 2 2 2 þ ða1 =2Þl1z þ ða2 =2Þl2z þ ða3 =2Þl3z þ ðb=2Þm2z :

ð1:5:3:26Þ In this expression, the coefﬁcients of the terms representing the exchange interaction are denoted by capital letters. It is mainly these terms that are responsible for the transition to the ordered state. The much smaller relativistic terms are responsible for the orientation of the vectors l or m. Their coefﬁcients are denoted by small letters. To minimize the potential (1.5.3.26), it is necessary to add terms of the fourth order, which are restricted to the exchange terms. The total expression for the thermodynamic potential will then be P P P ¼ 1 þ 14 C l4 þ 14C0 m4 þ 12 D ðl mÞ2 þ 12 D0 l2 m2 :

ðIIÞ ðIIIÞ

Mx ¼ My ¼ Mz ¼ 0 Bþb Mz ¼ 0; Mx2 þ My2 ¼ M?2 ¼ C B Mx ¼ My ¼ 0; Mz2 ¼ : C

ð1:5:3:30Þ ð1:5:3:31Þ ð1:5:3:32Þ

In the whole range of temperatures T > TC when B > 0, the minimum of the potential is determined by solution (I) (i.e. absence of a spontaneous magnetization). The realization of the second or third state depends on the sign of the coefﬁcient b. If b > 0, then the third state is realized, the magnetization M being directed along the axis. In this case, the transition from the paramagnetic into the ferromagnetic state will take place at TC ¼ T0 (when B ¼ 0). If b < 0, the magnetization is directed perpendicular to the axis. In this case, the Curie temperature is TC ¼ T0 b= (when B þ b ¼ 0). In the absence of a magnetic ﬁeld, the difference between the two values of TC has no physical meaning, since it only means another value of the coefﬁcient B [see (1.5.3.25)]. In a magnetic ﬁeld, both temperatures may be determined experimentally, i.e. when B becomes zero and when B þ b becomes zero. If a magnetic ﬁeld H is applied parallel to the z axis and b > 0, ~ leads to the minimization of the thermodynamic potential H=M ¼ CM 2 þ B:

ð1:5:3:33Þ

ð1:5:3:27Þ As pointed out above, one of the coefﬁcients A or B vanishes at the transition temperature Tc. This coefﬁcient may be expanded in a series of ðT Tc Þ [see (1.5.3.14)]. At T < Tc , a ferro- or antiferromagnetic structure will be realized, the type of

This relation has been veriﬁed in many experiments and the corresponding graphical representations are known in the literature as Arrott–Belov–Kouvel plots (see Kouvel & Fisher, 1964). Putting B ¼ ðT TC Þ according to (1.5.3.14), equations (1.5.3.32) and (1.5.3.33) may be used to derive expressions for the initial magnetic susceptibilities (for H ! 0):

124

1.5. MAGNETIC PROPERTIES 1 ; 2 ðTC TÞ 1 ; 0 ¼

ðT TC Þ 0 ¼

T < TC ;

ð1:5:3:34Þ

T > TC ;

ð1:5:3:35Þ

where ¼ 1. The Landau theory of phase transitions does not take account of ﬂuctuations of the order parameter. It gives qualitative predictions of all the possible magnetic structures that are allowed for a given crystal if it undergoes a second-order transition. The theory also explains which of the coefﬁcients in the expression for the thermodynamic potential is responsible for the corresponding magnetic structure. It describes also quantitative relations for the magnetic properties of the material if 1 ðT TC Þ=TC TC B2 =b3 ;

ð1:5:3:36Þ

where is the coefﬁcient in the term which describes the gradient energy. In this chapter, we shall not discuss the behaviour of the material in the ﬂuctuation region. It should be pointed out that, in this region, in relations (1.5.3.34) and (1.5.3.35) depends on the dimensionality of the structure n and equals 1.24 for n ¼ 1, 1.31 for n ¼ 2 and 1.39 for n ¼ 3. Similar considerations are relevant to the relations (1.5.3.31) and (1.5.3.32), which describe the temperature dependence of spontaneous magnetization. The relations (1.5.3.31) and (1.5.3.32) describe the behaviour of the ferromagnet in the ‘saturated’ state when the applied magnetic ﬁeld is strong enough to destroy the domain structure. The problem of the domains will be discussed later (see Section 1.5.4). The transition from the paramagnetic to the ferromagnetic state is a second-order transition, provided that there is no magnetic ﬁeld. In the presence of a magnetic ﬁeld that is parallel to the easy axis of magnetization, the magnetic symmetry of the crystal is the same (Mz 6¼ 0) both above and below TC. From the point of view of symmetry, no transition occurs in this case. 1.5.3.3.2. Uniaxial antiferromagnet Now let us proceed to the uniaxial antiferromagnet with two ~ for ions in the primitive cell. The thermodynamic potential such an antiferromagnet is given in accordance with (1.5.3.26) and (1.5.3.27) by (Landau, 1933) ~ ¼ 0 þ ðA=2ÞL2 þ ðB=2ÞM2 þ ða=2ÞðL2x þ L2y Þ þ ðb=2ÞðMx2 þ My2 Þ þ ðC=4ÞL4 þ ðD=2ÞðLMÞ2 þ ðD0 =2ÞL2 M2 0 MH:

ðIIÞ

Lx ¼ Ly ¼ Lz ¼ 0

ðIIIÞ

Lz ¼ 0;

Aþa C A 2 Lz ¼ : C

L2x þ L2y ¼ L2? ¼

Lx ¼ Ly ¼ 0;

Formulas (1.5.3.39) and (1.5.3.14) in the form A ¼ ðT Tc Þ yield the expression for the temperature dependence of the sublattice magnetization: L2 ¼ ð =CÞðTN TÞ;

M ¼ ? H ð? k ÞðqHÞq;

ð1:5:3:40Þ

When a < 0, state (II) with Lz ¼ 0 is thermodynamically stable. When a > 0, state (III) is stable and the antiferromagnetic vector is directed along the axis. This means that the term with the coefﬁcient a is responsible for the anisotropy of the uniaxial antiferromagnet. We introduce the effective anisotropy ﬁeld: Ha ¼ aL ¼ 2aM0 ; where M0 is the sublattice magnetization.

ð1:5:3:41Þ

ð1:5:3:43Þ

where q ¼ L=jLj. Thus the magnetization of an antiferromagnet is linear with the magnetic ﬁeld, as for a paramagnet, if the magnetic ﬁeld is not too strong. The main difference is in the anisotropy and temperature dependence of the susceptibility. The parallel susceptibility k decreases when the temperature is lowered, and ? does not depend on temperature (? ¼ 1=B) (see Fig. 1.5.3.6). The coefﬁcient B belongs to the exchange term and deﬁnes the effective exchange ﬁeld He ¼ 12BL ¼ BM0 :

ð1:5:3:44Þ

As seen from Fig. 1.5.3.6, ? > k . Therefore, when the magnetic ﬁeld applied parallel to the axis of a uniaxial antiferromagnet reaches the critical value 2 Hc1 ¼ aL2 =ð? k Þ ’ aBL20 ¼ 2Ha He

ð1:5:3:38Þ ð1:5:3:39Þ

ð1:5:3:42Þ

where TN is the Ne´el temperature. The assertions relating to formulas (1.5.3.34) and (1.5.3.35) concerning the ﬂuctuation region are also valid for the temperature dependence of the sublattice magnetization. ~ with respect to M for The minimization of the potential given L 6¼ 0 when H 6¼ 0 yields the following relation for the magnetization:

ð1:5:3:37Þ

If the magnetic ﬁeld is absent ðH ¼ 0Þ, then M ¼ 0 because B, D and D0 > 0. Then three possible magnetic states are obtained by minimizing the potential with respect to L only: ðIÞ

Fig. 1.5.3.6. Temperature dependence of the mass susceptibility g for a uniaxial antiferromagnet along (k ) and perpendicular (? ) to the axis of antiferromagnetism (see Foner, 1963). g is expressed in Gaussian units; the corresponding SI values are gSI = 4 103 gG.

ð1:5:3:45Þ

(L0 is the value of L at T ¼ 0), a ﬂopping of the sublattices from the direction along the axis to some direction in the plane perpendicular to the axis occurs. In this spin-ﬂop transition (which is a ﬁrst-order transition into a new magnetic structure), the magnetization jumps as shown in Fig. 1.5.3.7. A second-order transition into a saturated paramagnetic state takes place in a much stronger magnetic ﬁeld Hc2 ¼ 2He . This transition is called a spin-ﬂip transition. Fig. 1.5.3.7 shows the magnetic ﬁeld dependence of the magnetization of a uniaxial antiferromagnet. Fig. 1.5.3.8 shows the temperature dependence of both critical ﬁelds. The quantitative behaviour of the critical magnetic ﬁelds in the neighbourhood of TN for both directions of the magnetic ﬁeld (H k Oz and H ? Oz) can be determined from the theory of

125

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.5.3.7. Dependence of the relative magnetization M=Mmax on the magnetic ﬁeld at T ¼ 0. The dashed line corresponds to H ? Oz, the full line to H k Oz. Hc1 is the ﬁeld of spin-ﬂop, Hc2 is the ﬁeld of spin-ﬂip.

second-order phase transitions starting from the thermodynamic ~ and taking into account that L is small and DL2 B potential close to TN . In the presence of the magnetic ﬁeld H ? Oz, L is parallel to Oz, LM ¼ 0, the coefﬁcient A at L2 is replaced by A þ 2D0 H 2 =B2 and the latter is zero at the new transition point. The critical ﬁeld is given by the relation 2 ¼ ð B2 =2D0 ÞðTN TÞ; Hc2

H ? Oz:

ð1:5:3:46Þ

If the ﬁeld is applied parallel to the z axis, then L remains parallel to Oz if H < Hc1 (Hc1 ’ aB2 =D in the neighbourhood of TN ). Therefore, 2 Hc2 ¼

B2 ðT TÞ; 2ðD þ D0 Þ N

H k Oz; H < Hc1 :

ð1:5:3:47Þ

If H > Hc1, L becomes perpendicular to the z axis and the anisotropy term has to be taken into account: 2 Hc2 ¼

B2 ðT T a= Þ; 2D0 N

H k Oz; H > Hc1 :

ð1:5:3:48Þ

Formulas (1.5.3.46)–(1.5.3.48) show that the transition temperature is reduced by applying the magnetic ﬁeld. The displacement of the transition point is directly proportional to the square of the applied ﬁeld. Fig. 1.5.3.9 shows the phase diagram of an antiferromagnet in the neighbourhood of TN . Unlike ferromagnets, antiferromagnets maintain the second-order phase transition when a magnetic ﬁeld is applied because the symmetry

Fig. 1.5.3.8. Magnetic phase diagram for a uniaxial antiferromagnet in a magnetic ﬁeld applied parallel to the axis. (1) The line of spin-ﬂop transition ðHc1 Þ; (2) the line of spin-ﬂip transition ðHc2 Þ; P, paramagnetic phase; AFM, easy-axis antiferromagnetic phase; SF, spin-ﬂop phase; BP, bicritical point.

Fig. 1.5.3.9. Phase diagram for a uniaxial antiferromagnet in the proximity of TN , calculated for MnCl24H2O. Experimental data are taken from Gijsman et al. (1959). The ordinate value 100 corresponds to H = 10 kOe, i.e. B = 10 kG = 1 T.

of the crystal in the antiferromagnetic state differs essentially from that in the paramagnetic state also if the crystal is placed into a magnetic ﬁeld. Formula (1.5.3.43) describes the magnetization process only in easy-axis antiferromagnets. For easy-plane antiferromagnets, the anisotropy in the plane is usually extremely small and the antiferromagnetic vector rotates freely in the basic plane. Therefore, for any direction of the magnetic ﬁeld, the vector L becomes aligned perpendicular to the applied magnetic ﬁeld. Correspondingly the magnetization becomes M ¼ z Hz z^ þ ? H? x^ ;

ð1:5:3:49Þ

where z^ and x^ are unit vectors parallel and perpendicular to the axis. 1.5.4. Domain structure 1.5.4.1. 180 domains Neither symmetry nor energy considerations can determine the alignment of the magnetization vector n in a non-chiral easyaxis magnet (of ferro- or antiferromagnetic type). The vector n may be aligned parallel or antiparallel to the positive direction of the z axis. Therefore, specimens of any magnet are usually split into separate regions, called domains. In each domain of an easyaxis magnet, the vector n has one of its two possible directions. Such domains are called 180 domains. Adjacent domains are separated by a domain wall, in which the magnetic moments are no longer strictly parallel (or antiparallel). As a result of this, both the exchange and the anisotropy energy rise inside the volume of the domain wall. In ferromagnets (and ferrimagnets), the gain in the exchange and anisotropy energy in a multidomain sample is compensated by the loss in the magnetostatic energy. The existence of the domain structure is responsible for the behaviour of a ferromagnet in an applied magnetic ﬁeld. There are two kinds of magnetization processes that one has to distinguish: the displacement of the domain walls and the rotation of the spontaneous

126

1.5. MAGNETIC PROPERTIES

Fig. 1.5.4.1. Magnetization curves of hexagonal cobalt for two main (1 Oe = 103/(4) A m1; crystallographic directions: (1) [0001] and (2) ½1010. 3 3 1 1 emu cm = 10 A m .)

magnetization vector from the easy direction to the direction of the applied magnetic ﬁeld. The magnetization process will ﬁrst be considered without taking the demagnetizing ﬁeld into account. If the magnetic ﬁeld is applied parallel to the axis of an easy-axis ferromagnet, the displacement of the domain wall will completely determine the magnetization process. If the sample contains no impurities and crystal defects, such a displacement must take

Fig. 1.5.4.2. Magnetization curves of two cubic crystals (iron and nickel) for three crystallographic directions. (1 Oe = 103/(4) A m1; 1 emu cm3 = 103 A m1.)

Fig. 1.5.4.3. Schematic display of the magnetization: (a) H along the easy axis; (b) H at an arbitrary angle to the easy axis; (c) H perpendicular to the easy axis.

place in an inﬁnitely small magnetic ﬁeld [see curve (1) in Fig. 1.5.4.1 and Fig. 1.5.4.3a]. If the magnetic ﬁeld is applied perpendicular to the easy axis, the size of the domains does not change but their magnetization vectors rotate. Let us denote the spontaneous magnetization by Ms. Then the sample magnetization M rises linearly with respect to the applied magnetic ﬁeld: M ¼ 0 HMs2 =ð2K1 Þ;

ð1:5:4:1Þ

where K1 is deﬁned by relations (1.5.3.8)–(1.5.3.10). Some nonlinearity in H can arise from the fourth-order term with K2 [see curve (2) in Fig. 1.5.4.1 and Fig. 1.5.4.3c]. When H ¼ 2K1 =ð0 Ms Þ ¼ Hs , the magnetizations of all the domains are rotated by 90 and the magnetization of the sample becomes oriented along the magnetic ﬁeld; its value is saturated and is equal to the spontaneous magnetization Ms . If T 6¼ 0 K, there is an additional rise in magnetization with the magnetic ﬁeld. This rise, which is called true magnetization, is relatively very small at all temperatures except for the temperature region close to the transition temperature. If the magnetic ﬁeld is applied at an arbitrary angle to the easy axis, the magnetization process occurs in two steps [see curves (2) in Fig. 1.5.4.2 and Fig. 1.5.4.3b]. First, as a result of the wall displacement, the magnetization jumps to the value M1 in a small magnetic ﬁeld. Next, the rotation process follows and at Hs the sample becomes saturated [see curves (2) in Fig. 1.5.4.2]. It is essential to take the shape of the sample into account in considering the problem of the magnetization processes in ferromagnets, as the demagnetizing ﬁeld can be up to 4M in Gaussian units, up to M in SI units. In real materials, the displacement process is partly (at low ﬁelds) reversible and partly (at higher ﬁelds) irreversible. Therefore, complicated hysteresis processes arise in magnetizing ferromagnets. The problem of 180 domains in antiferromagnets is not as clear. These domains differ in the sign of the antiferromagnetic vector L. This vector was deﬁned as the difference of the vectors of sublattice magnetizations in a two-sublattice antiferromagnet, i.e. M1 M2 . Thus two such antiferromagnetic domains differ only by the numbering of the sites in the sublattices. Antiferromagnetic 180 domains are also called S-domains. The wall between two S-domains is schematically represented in Fig. 1.5.4.4. The origin of the antiferromagnetic S-domains cannot be explained from the point of view of energy balance as in a ferromagnet. These domains give rise to additional exchange and anisotropy energies which are not compensated by a decrease of any other kind of energy. Thus the S-domain structure is thermodynamically not stable. However, experiments show that S-domains exist in most easy-axis antiferromagnets.

127

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.5.4.4. A 180 domain wall in an antiferromagnet.

The formation of S-domains can be explained by assuming that when the material is cooled down to the Ne´el temperature, antiferromagnetic ordering arises in different independent regions. The direction of the vector L in these regions is accidental. When growing regions with different directions of L meet, the regular alternation of the directions of magnetic moments of the ions is broken on the border between these regions. Domain walls are created on such borders. Such domain structures can be metastable. The existence of S-domains in easy-axis antiferromagnets was ﬁrst proved in experiments in which effects that depend on the sign of L were investigated. These are piezomagnetism, linear magnetostriction and the linear magnetoelectric effect. The sign of these effects depends on the sign of L. We shall discuss this problem in detail in Sections 1.5.7 and 1.5.8. Later, 180 domain walls were observed in neutron scattering experiments (Schlenker & Baruchel, 1978), and the domains themselves in magneto-optical experiments (see Kharchenko et al., 1979; Kharchenko & Gnatchenko, 1981). 1.5.4.2. Twin domains As pointed out in Section 1.5.3, in tetragonal non-easy-axis magnets, in easy-plane hexagonal and trigonal and in cubic magnets there is more than one easy magnetization direction (3, 4 or 6). As a result, domains arise in which vectors Ms or L are directed to each other at 120, 109.5, 90, 70.5 and 60 . Such domains are called twin or T-domains. The formation of magnetic T-domains is accompanied by the formation of crystallographic domains as a result of spontaneous magnetostriction. But mostly this is very small. Each of the T-domains may split into 180 domains. The magnetization process in ferromagnets possessing Tdomains is similar to the previously described magnetization of an easy-axis ferromagnet in a magnetic ﬁeld directed at an oblique angle. First the displacement process allows those 180 domains that are directed unfavourably in each T-domain to disappear, and then the rotation process follows. In easy-plane antiferromagnets, the T-domain structure is destroyed by a small magnetic ﬁeld and the antiferromagnetic vector L in the whole specimen becomes directed perpendicular to the applied magnetic ﬁeld, as was explained in Section 1.5.3. There are four kinds of T-domains in cubic antiferromagnets, in which the vectors L are directed parallel or perpendicular to the four h111i axes. Such a T-domain structure can be destroyed only when the applied magnetic ﬁeld is so strong that the antiferromagnetic order is destroyed at a spin-ﬂip transition.

point group of the ordered state (called the ferroic state) times the number of domains. Aizu found that there are 773 possible combinations of the point-group symmetries of the prototype and the ferroic state, if crystallographically inequivalent orientations of the subgroup in the group of the prototype are distinguished. These 773 combinations are called ferroic species and are characterized by a symbol giving ﬁrst the point group of the prototype, then the letter F, then the point group of the ferroic state and ﬁnally a letter between parentheses if different orientations are possible. As an example, the 20 axis of the ferroic state is parallel to the fourfold axis of the prototype in 42210 F20 ðpÞ and perpendicular to it in 42210 F20 ðsÞ. Let us discuss the ferroic states of rhombohedral transitionmetal oxides given in Table 1.5.3.4. The paramagnetic prototype 0. The four monoclinic ferroic species have has point group 3m1 six domains (‘orientation states’) each, which form three pairs of 180 domains (‘time-conjugate orientation states’). All four species are ‘fully ferroelastic’, i.e. the three pairs show different orientations of the spontaneous strain; two of the four species 0 F20 =m0 and 3m1 0 F2=m) are also ‘fully ferromagnetic’ (3m1 because all six domains have different orientations of the spontaneous magnetization. Switching a domain into another with a different orientation of the spontaneous strain can be achieved by applying mechanical stress. If the domain was spontaneously magnetized, the orientation of the magnetization is changed simultaneously. Similarly, a domain can be switched into another with a different orientation of the spontaneous magnetization by means of a magnetic ﬁeld. If the two spontaneous magnetizations have different directions (not just opposite sign), the direction of the spontaneous strain will change at the same time. Aizu’s concept of ferroic species has been extended by Litvin (2009) from ferroelectric, ferromagnetic (or antiferromagnetic) and ferroelastic domains to the occurrence of domains bearing a toroidal moment, i.e., to ferrotoroidic domains (Van Aken et al., 2007). It is noteworthy that this extension leaves the number of Aizu’s 773 species unchanged. This is plausible, since ferrotoroidic domains are simultaneously either ferromagnetic or purely antiferromagnetic. In both cases the toroidal moment is an inseparable part of the spin structure. Owing to this coupling, toroidic domains can be time-reversed either by a magnetic ﬁeld alone or by electric and magnetic ﬁelds, depending on the tensor form of the linear magnetoelectric effect (Schmid, 2008). The Aizu classiﬁcation is of interest for technological applications because it gives an overall view not only of domain formation but also of the possibilities for domain switching.

1.5.5. Weakly non-collinear magnetic structures As was indicated above (see Tables 1.5.3.3 and 1.5.3.6), certain magnetic space groups allow the coexistence of two different types of magnetic ordering. Some magnetic structures can be described as a superposition of two antiferromagnetic structures with perpendicular antiferromagnetic vectors L. Such structures may be called weakly non-collinear antiferromagnets. There can also be a superposition of an antiferromagnetic structure L with a ferromagnetic one M (with L ? M). This phenomenon is called weak ferromagnetism. We shall demonstrate in this section why one of the magnetic vectors has a much smaller value than the other in such mixed structures. 1.5.5.1. Weak ferromagnetism

1.5.4.3. Ferroic domains Aizu (1970) gave a classiﬁcation of domain formation when a crystal undergoes a transition from an unordered to a magnetically ordered state that has a lower point-group symmetry (see also Section 3.1.1). The unordered state (called the prototype phase) has a grey point group. The number of elements in this group is equal to the product of the number of elements in the

The theory of weak ferromagnetism was developed by Dzyaloshinskii (1957a). He showed that the expansion of the ther~ may contain terms of the following type: modynamic potential Li Mk (i; k ¼ x; y). Such terms are invariant with respect to the transformations of many crystallographic space groups (see Section 1.5.3.3). If there is an antiferromagnetic ordering in the material (Li 6¼ 0) and the thermodynamic potential of the

128

1.5. MAGNETIC PROPERTIES

Fig. 1.5.5.1. Diagrams demonstrating two weakly ferromagnetic structures in rhombohedral crystals with two magnetic ions in the primitive cell (compare with Fig. 1.5.3.1). (a) Magnetic space group P2=c; (b) magnetic space group P20 =c0 .

material contains such a term, the minimum of the potential will be obtained only if Mk 6¼ 0 as well. The term Li Mk is a relativistic one. Therefore this effect must be small. We shall consider as an example the origin of weak ferromagnetism in the two-sublattice antiferromagnets MnCO3, CoCO3 and NiCO3, discussed in Section 1.5.3.1. The following analysis can be applied also to the four-sublattice antiferromagnet -Fe2O3 (assuming L1 ¼ L2 ¼ 0, L3 ¼ L). All these rhombohedral crystals belong to the crystallographic space ~ for these group D63d ¼ R3c. The thermodynamic potential crystals was derived in Section 1.5.3.3. For the case of a twosublattice antiferromagnet, one has to add to the expression (1.5.3.26) the invariant (1.5.3.24): ~ ¼ ðA=2ÞL2 þ ðB=2ÞM2 þ ða=2ÞL2z þ ðb=2ÞMz2 þ dðLx My Ly Mx Þ 0 MH:

anisotropy coefﬁcient a. Such crystals become easy-axis antiferromagnets. Of this type are FeCO3 and the low-temperature modiﬁcation of -Fe2O3. For four-sublattice antiferromagnets, the sequence of the directions of the magnetic moments of the sublattices is also essential. For example, the structures of the types A1 and A2 (see Fig. 1.5.3.4 and Table 1.5.3.3) do not exhibit weak ferromagnetism. The behaviour of weak ferromagnets in magnetic ﬁelds applied perpendicular ðH? Þ and parallel ðHk Þ to the trigonal axis is described by the following relations:

ð1:5:5:1Þ M? ¼ MD þ ? H? ;

The coefﬁcients of the isotropic terms (A and B) are of exchange origin. They are much larger than the coefﬁcients of the relati~ for a ﬁxed value of L2 vistic terms (a; b; d). Minimization of and H ¼ 0 gives two solutions: (1) L k Oz (Lx ¼ Ly ¼ 0, M ¼ 0). FeCO3 and the lowtemperature modiﬁcation of -Fe2O3 possess such purely antiferromagnetic structures. (2) L ? Oz [Mx ¼ ðd=BÞLy , My ¼ ðd=BÞLx , Mz ¼ 0]. This structure exhibits a spontaneous ferromagnetic moment MD ¼ ðMx2 þ My2 Þ1=2 ¼ ðd=BÞL:

Fig. 1.5.5.2. Dependence of magnetization M? and Mk on the magnetic ﬁeld H for the weak ferromagnet MnCO3 at 4.2 K (Borovik-Romanov, 1959a). (H = 1 kOe corresponds to B = 1 kG = 0.1 T; M = 100 emu mol1 = 0.1 A m2 mol1.)

ð1:5:5:2Þ

The magnetic moment MD is smaller than the magnetization of the sublattices (M0 ¼ L=2) in the ratio 2d=B. This phenomenon is therefore called weak ferromagnetism. The vectors MD and L are mutually perpendicular. Their direction in the plane is determined by the sixth-order terms of the anisotropy energy (see Section 1.5.3.2). This anisotropy is extremely small in most materials. The vectors of magnetization of the sublattices M0 are deﬂected by a small angle ’ ’ 2d=B away from the direction of the antiferromagnetic axis L in such weak ferromagnets (see Fig. 1.5.5.1). Weak ferromagnetism was ﬁrst observed in the following trigonal crystals: the high-temperature modiﬁcation of haematite, -Fe2O3 (Townsend Smith, 1916; Ne´el & Pauthenet, 1952), MnCO3 (Borovik-Romanov & Orlova, 1956) and later also in CoCO3, NiCO3 and FeBO3. In accordance with theory, weak ferromagnetism does not occur in trigonal crystals with a positive

Mk ¼ k Hk ;

ð1:5:5:3Þ

k ¼ 1=ðB þ bÞ:

ð1:5:5:4Þ

where ? ¼ 1=B;

An external magnetic ﬁeld can freely rotate the ferromagnetic moment in the basal plane of the easy-plane weak ferromagnets under consideration because their anisotropy in the basal plane is extremely small. During such a rotation, both vectors M and L move simultaneously as a rigid structure. On the other hand, it is impossible to deﬂect the vector MD out of the basal plane, as this is forbidden by symmetry. This is illustrated by the magnetization curves plotted in Fig. 1.5.5.2, which conﬁrm the relations (1.5.5.3). When the weakly ferromagnetic structure is rotated in the basal plane, a change of the magnetic space groups occurs in the following order: P2=c $ P1 $ P20 =c0 $ P1 $ P2=c $ . . .. Each of these symmetry transformations corresponds to a second-order phase transition. Such transitions are allowed because P1 is a subgroup of both groups P2=c and P20 =c0 . NiF2 was one of the ﬁrst weak ferromagnets to be discovered (Matarrese & Stout, 1954). In the paramagnetic state, it is a tetragonal crystal. Its crystallographic space group is D14 4h = P42 =mnm. In the ordered state its magnetic point group is D2h ðC2h Þ ¼ mm0 m0 and the vectors L and M are directed along two twofold axes (one of which is primed) in the plane perpendicular to the former fourfold axis (see Fig. 1.5.5.3a). The invar-

129

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 40 =mmm0 . They are easy-axis antiferromagnets without weak ferromagnetism. The interaction described by the invariant dðLx My Ly Mx Þ in equation (1.5.5.1) is called Dzyaloshinskii–Moriya interaction. It corresponds to the interaction between the spins of neighbouring ions, which can be represented in the form d½Si Sj ;

where the vector d has the components (0; 0; dz ). Terms of such type are allowed by symmetry for crystals that in the paramagnetic state belong to certain space groups of the trigonal, tetragonal and hexagonal systems. In some groups of the tetragonal system, weak ferromagnetism is governed by the term dðLx My þ Ly Mx Þ (as for NiF2) and in the orthorhombic system by ðd1 Li Mk þ d2 Lk Mi Þ; ði; k ¼ x; y; zÞ. In the monoclinic system, the latter sum contains four terms. The weak ferromagnetism in most groups of the hexagonal and cubic systems is governed by invariants of fourth and sixth order of Li ; Mk. For all crystallographic space groups, Turov (1963) determined the form of the invariants of lowest order that allow, for collinear or weakly noncollinear antiferromagnetic structures, a phase transition into a state with weak ferromagnetism. The corresponding list of the numbers of the space groups that allow the transition into an antiferromagnetic state with weak ferromagnetism is given in Table 1.5.5.1. The form of the invariant responsible for weak ferromagnetism is also displayed in the table. Turov (1963) showed that weak ferromagnetism is forbidden for the triclinic system, for the six trigonal groups with point groups C3 ¼ 3 or and the 12 cubic groups with point groups T ¼ 23 or C3i ¼ 3, Th ¼ m3. The microscopic theory of the origin of weak ferromagnetism was given by Moriya (1960a,b, 1963). In this chapter, we have restricted our consideration to the phenomenological approach to this problem. A large number of orthorhombic orthoferrites and orthochromites with the formula RMO3 (where R is a trivalent rareearth ion and M is Fe3+ or Cr3+) have been investigated in many laboratories (cf. Wijn, 1994). Some of them exhibit weak ferromagnetism. The space group of these compounds is D16 2h ¼ Pnma in the paramagnetic state. The primitive cell is the same in the paramagnetic and magnetically ordered states. It contains four magnetic transition-metal ions (see Fig. 1.5.5.4). They determine to a large extent the properties of orthoferrites (outside the region of very low temperatures). For a four-sublattice anti-

Fig. 1.5.5.3. Magnetic structures of ﬂuorides of transition metals. (a) The weak ferromagnet NiF2; (b) the easy-axis antiferromagnets MnF2, FeF2 and CoF2.

iant term responsible for the weak ferromagnetism in tetragonal ﬂuorides has the form dðLx My þ Ly Mx Þ:

ð1:5:5:6Þ

ð1:5:5:5Þ

The anisotropy of the crystals of NiF2 and the relation given above for the invariant lead to the same dependence on the magnetic ﬁeld as for trigonal crystals. However, the anisotropy of the magnetic behaviour in the basal plane is much more complicated than for rhombohedral crystals (see Bazhan & Bazan, 1975). The anisotropy constant K1 is positive for most other ﬂuorides (MnF2, FeF2 and CoF2) and their magnetic structure is described by the magnetic point group D4h ðD2h Þ =

Table 1.5.5.1. The numbers of the crystallographic space groups that allow a phase transition into a weakly ferromagnetic state and the invariants of lowest order that are responsible for weak ferromagnetism Note that the standard numbering of space groups is used in this table, not the one employed by Turov (1963). System

Nos. of the space groups

Invariants

Case No.

Monoclinic

3–15

Mx Ly , Mz Ly , My Lx , My Lz

1

Orthorhombic

16–74

Tetragonal

Trigonal Hexagonal

Cubic

75–88

89–142 149–167

Mx Ly , My Lx

2

My Lz , Mz Ly

3

Mx Lz , Mz Lx

4

Mx Ly þ My Lx , Mx Lx My Ly

5

Mx Ly My Lx

6

Mx Ly þ My Lx

7

Mx Lx My Ly

8

Mx Ly My Lx 3

9; 10 2

168–176

Mz ðLx iLy Þ , ðMx iMy ÞðLx iLy Þ Lz

11

177–194

Mx Ly My Lx

12

iMz ½ðLx þ iLy Þ3 ðLx iLy Þ3 , i½ðMx þ iMy ÞðLx þ iLy Þ2 ðMx iMy ÞðLx iLy Þ2 Lz

13

Mz ½ðLx þ iLy Þ3 þ ðLx iLy Þ3 , ½ðMx þ iMy ÞðLx þ iLy Þ2 þ ðMx iMy ÞðLx iLy Þ2 Lz

14

Mx Lx ðL2y L2z Þ þ My Ly ðL2z L2x Þ þ Mz Lz ðL2x L2y Þ

15

207–230

130

1.5. MAGNETIC PROPERTIES

Fig. 1.5.5.5. Temperature dependence of the susceptibility for CoCO3 (Borovik-Romanov & Ozhogin, 1960). The maximum of mol ? at 18.1 K is ’ 0.08 cm3 mol1 in Gaussian units, ’ 106 m3 mol1 in SI units.

Fig. 1.5.5.4. Magnetic structures of orthoferrites and orthochromites RMO3. (Only the transition-metal ions are shown; the setting Pbnm is used.) (a) Gx F z weakly ferromagnetic state; (b) Gz F x weakly ferromagnetic state.

ferromagnet, there are four possible linear combinations of the sublattice vectors, which deﬁne three types of antiferromagnetic vectors L and one ferromagnetic vector F [see relations (1.5.3.2) and Table 1.5.3.1]. The exchange interaction in these compounds governs magnetic structures, which to a ﬁrst approximation are described by the following antiferromagnetic vector (which is usually denoted by the symbol G): G ¼ L2 ¼ ðN=4Þðl1 l2 þ l3 l4 Þ:

ð1:5:5:7Þ

In the case of orthoferrites, the other two antiferromagnetic vectors L1 and L3 [see relations (1.5.3.2)] are named A and C, respectively. The magnetic structure of the compounds under consideration is usually called the Gi or Gi F k state. Depending on the signs and the values of the anisotropy constants, there are three possible magnetic states: Table 1.5.5.2. Magnetic point groups that allow weak ferromagnetism Schoenﬂies

Hermann–Mauguin

C1 Ci C2 C 2 ðC 1 Þ Cs C s ðC 1 Þ C 2h C 2h ðC i Þ D2 ðC 2 Þ C 2v ðC 2 Þ C 2v ðC s Þ D2h ðC2h Þ

1 1 2 20 m m0 2=m 20 =m0 220 20 m0 m0 2 m0 m20 mm0 m0

ðIÞ

Gx F z

L2x 6¼ 0;

MDz 6¼ 0;

ð1:5:5:8Þ

ðIIÞ ðIIIÞ

Gy Gz F x

L2y 6¼ 0; L2z 6¼ 0;

MD ¼ 0; MDx 6¼ 0:

ð1:5:5:9Þ ð1:5:5:10Þ

The magnetic structures (I) and (III) are weak ferromagnets. They are displayed schematically in Fig. 1.5.5.4. Both are described by the same magnetic point group D2h ðC 2h Þ yet in different orientations: m0 m0 m (i.e. 20x =m0x 20y =m0y 2z =mz ) for structure (I) and mm0 m0 (i.e. 2x =mx 20y =m0y 20z =m0z ) for structure (III). The magnetic point group of structure (II) is D2h ¼ mmm. Weak ferromagnetism is observed in boracites with chemical formula M3B7O13X (where M = Co, Ni and X = Br, Cl, I). These compounds are unique, being simultaneously antiferromagnets, weak ferromagnets and ferroelectrics. Section 1.5.8.3 is devoted to these ferromagnetoelectrics. Concerning the magnetic groups that allow weak ferromagnetism, it should be noted that, as for any ferromagnetism, weak ferromagnetism is allowed only in those space groups that have a trivial magnetic Bravais lattice. There must be at least two magnetic ions in the primitive cell to get antiferromagnetic order. Among the 31 magnetic point groups that admit ferromagnetism (see Table 1.5.2.4), weak ferromagnetism is forbidden in the magnetic groups belonging to the tetragonal, trigonal and hexagonal systems. Twelve magnetic point groups that allow weak ferromagnetism remain. These groups are listed in Table 1.5.5.2. A material that becomes a weak ferromagnet below the Ne´el temperature TN differs from a collinear antiferromagnet in its behaviour above TN . A magnetic ﬁeld applied to such a material above TN gives rise to an ordered antiferromagnetic state with vector L directed perpendicular and magnetization M parallel to the ﬁeld. Thus, as in usual ferromagnets, the magnetic symmetry of a weak ferromagnet in a magnetic ﬁeld is the same above and below TN. As a result, the magnetic susceptibility has a maximum at T ¼ TN [like the relations (1.5.3.34) and (1.5.3.35)]. This is true only if the magnetic ﬁeld is aligned along the easy axis for weak ferromagnetism. Fig. 1.5.5.5 shows the anomalous anisotropy of

131

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.5.6. Reorientation transitions

Fig. 1.5.5.6. A weakly non-collinear magnetic structure corresponding to (1.5.5.12).

the temperature dependence of the magnetic susceptibility in the neighbourhood of TN for weak ferromagnets. Similar anomalies in the neighbourhood of TN are observed in materials with a symmetry allowing a transition into a weakly ferromagnetic state for which the sign of the anisotropy constant causes their transition into purely antiferromagnetic states. 1.5.5.2. Other weakly non-collinear magnetic structures ~ of the form (1.5.5.1) may give A thermodynamic potential rise not only to the weak ferromagnetism considered above but also to the reverse phenomenon. If the coefﬁcient B (instead of A) changes its sign and b > 0, the material will undergo a transition into a slightly canted ferromagnetic structure, in which Ms LD and the expression for LD is LD ¼ ðd=BÞMs? :

ð1:5:5:11Þ

Experimental detection of such structures is a difﬁcult problem and to date no-one has observed such a phenomenon. ~ of a four-sublattice antiThe thermodynamic potential ferromagnet may contain the mixed invariant [see (1.5.3.24)] d1 ðL1x L2y L1y L2x Þ:

ð1:5:5:12Þ

Such a term gives rise to a structure in which all four vectors of sublattice magnetization M form a star, as shown in Fig. 1.5.5.6 (see also Fig. 1.5.1.3b). The angle 2 between the vectors l1 and l3 (or l2 and l4 ) is equal to d1 =A2 if the main antiferromagnetic structure is deﬁned by the vector L2 [see the caption for Fig. 1.5.1.3(b)]. Such a structure may occur in Cr2O3. In most orthoferrites discussed above, such non-collinear structures are observed for all three cases: purely antiferromagnetic (Gy ) and weakly ferromagnetic (Gx F z and Gz F x ). The structure Gy is not coplanar. Apart from the main antiferromagnetic vector G aligned along the y axis, it possesses two other antiferromagnetic vectors: A (aligned along the x axis) and C (aligned along the z axis). The weakly ferromagnetic structure Gx F z has an admixture of the Ay antiferromagnetic structure. The helical (or spiral) structure described in Section 1.5.1.2.3 and depicted in Fig. 1.5.1.4 is also a weakly non-collinear antiferromagnetic structure. As mentioned above, this structure consists of atomic layers in which all the magnetic moments are parallel to each other and parallel to the layer. The magnetizations of neighbouring layers are antiparallel to a ﬁrst approximation; but, more speciﬁcally, there is a small deviation from a strictly antiparallel alignment. The layers are perpendicular to a vector k, which is parallel to the axis of the helix. The two mutually perpendicular antiferromagnetic vectors L are both perpendicular to k. These vectors deﬁne the helical structure by the following relation for the density of the magnetization MðrÞ in the layer with the coordinate r (Dzyaloshinskii, 1964; Andreev & Marchenko, 1980): MðrÞ ¼ L1 sin kr L2 cos kr:

ð1:5:5:13Þ

Most helical structures are incommensurate, which means that the representation deﬁned by the vector k does not satisfy the Lifshitz condition (see Section 1.5.3.3).

In many materials, the anisotropy constants change sign at some temperature below the critical temperature. As a result, the direction of the vector L (or Ms ) changes relative to the crystallographic axes. Correspondingly, the magnetic symmetry of the material also changes. Such phase transitions are called reorientation transitions. Cobalt is a typical ferromagnet and experiences two such reorientation transitions. It is a hexagonal crystal, which at low temperatures behaves as an easy-axis ferromagnet; its magnetic point group is D6h ðC6h Þ ¼ 6=mm0 m0. If the anisotropy energy were described by the relations (1.5.3.6) and (1.5.3.7) with only one anisotropy constant K1 , the change of the sign of this constant would give rise to a ﬁrst-order transition from an easyaxis to an easy-plane ferromagnet. This transition would occur at the temperature Tc at which K1 ðTÞ ¼ 0. In fact, the polar angle that determines the direction of the spontaneous magnetization increases progressively over a ﬁnite temperature interval. The behaviour of during the process of this reorientation may be obtained by minimizing the expression of the anisotropy energy (1.5.3.10), which contains two anisotropy coefﬁcients K1 and K2 . If K2 > 0, the minimum of Ua corresponds to three magnetic phases, which belong to the following magnetic point groups: (1) D6h ðC 6h Þ ¼ 6=mm0 m0 ; for this phase ¼ 0; . It is realized at temperatures T < T1 ¼ 520 K, where K1 > 0. (2) C2h ðCi Þ ¼ 20 =m0 ; for this phase sin ¼ ðK1 =2K2 Þ1=2. It is realized at temperatures T1 ¼ 520 < T < T2 ¼ 580 K, where 2K2 < K1 < 0. (3) D2h ðC 2h Þ ¼ mm0 m0 ; for this phase ¼ =2. It is realized at temperatures T2 ¼ 580 < T < Tc ¼ 690 K, where K1 < 2K2. The low-temperature phase is of the easy-axis type and the high-temperature phase is of the easy-plane type. The intermediate phase is called the angular phase. The two second-order phase transitions occur at temperatures which are the roots of the two equations K1 ðT1 Þ ¼ 0;

K1 ðT2 Þ þ 2K2 ðT2 Þ ¼ 0:

ð1:5:6:1Þ

The chain of these transitions (including the transition to the paramagnetic state at T ¼ TC ) may be represented by the following chain of the corresponding magnetic point groups: D6h ðC6h Þ ¼ 6=mm0 m0

! C 2h ðC i Þ ¼ 20 =m0 ! D2h ðC2h Þ ¼ mm0 m0 ! ðD6h þ RD6h Þ ¼ 6=mmm10 :

In Co and most of the other ferromagnets, the rotation of the spontaneous magnetization described above can be obtained by applying an external magnetic ﬁeld in an appropriate direction. In many antiferromagnets, there occur similar reorientation transitions, which cannot be achieved by means of a magnetic ﬁeld. The ﬁrst reorientation transition in antiferromagnets was observed in haematite (- Fe2O3), which at room temperature is a weak ferromagnet with magnetic structure A3x or A3y (see Tables 1.5.3.3 and 1.5.3.4 in Section 1.5.3.1). Morin (1950) found that the weak ferromagnetism in haematite disappears below TM ’ 260 K. At low temperature, haematite becomes an easyaxis antiferromagnet with the structure A3z. Unlike in cobalt, the transition at TM is a ﬁrst-order transition in haematite. This is so because the anisotropy constant K2 is negative in haematite. As a result, there are only two solutions for the angle that lead to a minimum of the anisotropy energy Ua ð3Þ [(1.5.3.9)], ¼ 0 if K1 > K2 and ¼ =2 if K1 < K2. The transition temperature TM is deﬁned by

132

K1 ðTM Þ þ K2 ðTM Þ ¼ 0:

ð1:5:6:2Þ

1.5. MAGNETIC PROPERTIES

Fig. 1.5.6.1. Schematic representation of the rotation of the vectors G and F (in the xz plane) at a reorientation transition in orthoferrites.

There is the following change in the magnetic space groups at this transition: ð1:5:6:3Þ P2=c 0 TM R3c ! 0 0 ð1:5:6:4Þ P2 =c Which of the two groups is realized at high temperatures depends on the sign of the anisotropy constant K?0 in equation (1.5.3.9). Neither of the high-temperature magnetic space groups is a subgroup of the low-temperature group. Therefore the transition under consideration cannot be a second-order transition. Reorientation transitions have been observed in many orthoferrites and orthochromites. Orthoferrites of Ho, Er, Tm, Nd, Sm and Dy possess the structure Gx F z [see (1.5.5.8)] at room temperature. The ﬁrst ﬁve of them undergo reorientation transitions to the structure Gz F x at lower temperatures. This reorientation occurs gradually, as in Co. Both vectors L and MD rotate simultaneously, as shown in Fig. 1.5.6.1. These vectors remain perpendicular to each other, but the value of MD varies from ðd1 =BÞL for MDz to ðd2 =BÞL for MDx . The coefﬁcients d1 and d2 belong to the terms Lx Mz and Lz Mx , respectively. The following magnetic point groups are observed when these transitions occur: 20x 20y 2z m0x m0y mz

T1

!

20y m0y

T2

!

2x 20y 20z : mx m0y m0z

ð1:5:6:5Þ

Anomalies typical for second-order transitions were observed at the temperatures T1 and T2 . The interval T2 T1 varies from 10 to 100 K. At low temperatures, DyFeO3 is an easy-axis antiferromagnet without weak ferromagnetism – Gy . It belongs to the trivial magnetic point group D2h ¼ mmm. At TM = 40 K, DyFeO3 transforms into a weak ferromagnet Gx F z . This is a ﬁrst-order reorientation transition of the type D2h ¼ mmm

TM

! D2h ðC 2h Þ ¼ m0 m0 m:

ð1:5:6:6Þ

Reorientation transitions in antiferromagnets occur not only as a result of a sign change of the anisotropy constant. They can be governed by the applied magnetic ﬁeld. In Section 1.5.3.3.2, we described the spin-ﬂop ﬁrst-order reorientation transition in an easy-axis antiferromagnet. This transition splits into two secondorder transitions if the magnetic ﬁeld is not strictly parallel to the axis of the crystal. There is a speciﬁc type of reorientation transition, which occurs in antiferromagnets that do not exhibit weak ferromagnetism, but would become weak ferromagnets if the antiferromagnetic vector was directed along another crystallographic direction. As an example, let us consider such a transition in CoF2. It is a tetragonal crystal with crystallographic space group D14 4h ¼ P42 =mnm. Below TN, CoF2 becomes an easyaxis antiferromagnet. The magnetic structure of this crystal is

Fig. 1.5.6.2. Schematic representation of the rotation of the vector L under the action of a magnetic ﬁeld applied to CoF2 perpendicular to the fourfold axis z (reorientation transition) (see Figs. 1.5.5.3a and b).

shown in Fig. 1.5.5.3. Its magnetic point group is D4h ðD2h Þ = 40 =mmm0 . Let us apply the magnetic ﬁeld H parallel to the twofold axis x (see Fig. 1.5.6.2). In a typical antiferromagnet, the ﬁeld stimulates a magnetization M ¼ ? H. The structure D14 4h ¼ P42 =mnm allows weak ferromagnetism if L is perpendicular to the z axis. As a result, if the vector L is deﬂected from the z axis by an angle in the plane yz perpendicular to the x axis, the magnetization will rise according to the relation M ¼ ? ðH þ HD sin Þ;

ð1:5:6:7Þ

where HD ¼ MD =? [see (1.5.5.3) and (1.5.5.4)]. As a result, there is a gain in the magnetic energy, which compensates the loss in the anisotropy energy. The beginning of the deﬂection is a second-order transition. The balance of both energies determines the value of : sin ¼ ðHe =Ha HD ÞH:

ð1:5:6:8Þ

The second second-order transition occurs when becomes equal to =2 at the critical ﬁeld Hc : Hc ¼ HD Ha =He :

ð1:5:6:9Þ

After the reorientation transition, CoF2 has the same magnetic point group as the weak ferromagnet NiF2, i.e. D2h ðC2h Þ ¼ mm0 m0 .

1.5.7. Piezomagnetism As we have seen, the appearance of weak ferromagnetism in antiferromagnets is closely connected with their magnetic symmetry. If the magnetic point group of the antiferromagnetic crystal contains an axis of higher than twofold symmetry, the magnetic structure is purely antiferromagnetic. By applying an external force that disturbs the symmetry of the crystal and destroys the axis of high symmetry, one may create a structure possessing weak ferromagnetism. In the previous section, we considered such reduction of the symmetry with the aid of a magnetic ﬁeld applied perpendicular to the main axis of the crystal. Another possibility for symmetry reduction is to apply an external pressure and to deform the crystal. Thus, in some antiferromagnetic crystals, a ferromagnetic moment may be produced on application of external stress. This phenomenon is called piezomagnetism. To investigate the piezomagnetic effect from the phenomenological point of view, we have to add the terms of the magnetoelastic energy in the expansion of the thermodynamic potential. The magnetoelastic terms of the least degree in the expansion of ~ for a given stable magnetic the thermodynamic potential structure will be of the type Tij Mk Ll (Tij are the components of the elastic stress tensor T). These terms must be invariant relative

133

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES to the crystallographic group of the material under examination. If we consider the potential , which is a function of T, T, H, the terms of the magnetoelastic energy that are responsible for piezomagnetism are of the form Hi Tjk . Thus, for the piezomagnetic crystals the expansion of the thermodynamic potential should be expressed by ðT; T; HÞ ¼ 0 ðT; HÞ ijk Hi Tjk ;

ð1:5:7:1Þ

where summation over the repeated indices i, j, k is implied. If at least one term of this expansion remains invariant under the magnetic symmetry of the given crystal, then the corresponding component ijk will not be zero and hence 0 Mi ¼ @[email protected] ¼ @0 [email protected] þ ijk Tjk :

ð1:5:7:2Þ

Thus, when a stress Tjk is applied, a magnetic moment is produced which is linear with the stress. It follows from expression (1.5.7.1) that the converse of the piezomagnetic effect also exists, i.e. linear magnetostriction: Sjk ¼ @[email protected] ¼ ijk Hi ;

ð1:5:7:3Þ

where Sjk are the components of the deformation tensor. 1.5.7.1. Piezomagnetic effect The possibility of the existence of a piezomagnetic effect was ﬁrst foreseen by Voigt (1928). However, he assumed that it is sufﬁcient to consider only the crystallographic symmetry in order to predict this effect. In reality, the crystals that do not possess a magnetic structure are characterized by the transformation R being contained in the magnetic group as an independent element. The transformation R changes the sign of the magnetic vectors H, L, M. Hence, for such crystals all values of ijk vanish and piezomagnetism is forbidden. The magnetic groups of magnetically ordered crystals (ferromagnets and antiferromagnets) contain R only in combination with other elements of symmetry, or do not contain this transformation at all. Hence the piezomagnetic effect may occur in such crystals. This statement was ﬁrst made by Tavger & Zaitsev (1956). The most interesting manifestation of the piezomagnetic effect is observed in antiferromagnets, as there is no spontaneous magnetization in these materials. From equation (1.5.7.1) it follows that ijk is an axial tensor of third rank. Hence, apart from the restriction that piezomagnetism is forbidden for all para- and diamagnetic materials, it must be absent from the 0 21 magnetic point groups that contain the element Ci R ¼ 1 (see Table 1.5.7.1). The stress tensor Tjk is symmetrical (Tjk ¼ Tkj ); see Section 1.3.2.4. Thus the tensor ijk is symmetrical in its last two indices. This is the reason why piezomagnetism is prohibited for three more magnetic point The remaining 66 and Oh ¼ m3m. groups: O ¼ 432, T d ¼ 43m magnetic point groups were found by Tavger (1958), who also constructed the 16 corresponding forms of the piezomagnetic tensors appropriate to each point group. They are represented in Table 1.5.7.1. (See also Birss & Anderson, 1963; Birss, 1964.) Since the stress tensor Tjk is symmetrical, it has only six independent components. Therefore the notation of its components can be replaced by a matrix notation (Voigt’s notation, see Section 1.3.2.5) in the following manner:

In matrix notation, equation (1.5.7.2) may be written in the form 0 Mi ¼ @ð 0 Þ[email protected] ¼ ijk Tjk ¼ i T ;

ð1:5:7:4Þ

where i ¼ 1; 2; 3 and ¼ 1; 2; 3; 4; 5; 6. These notations are used in Table 1.5.7.1. Notice that ij ¼ ijj for j ¼ 1; 2; 3, i4 ¼ 2i23 , i5 ¼ 2i31 , and i6 ¼ 2i12 . The form of the matrix i depends on the orientation of the axes of the Cartesian coordinate system (CCS) with respect to the symmetry axes of the point group of the crystal under consideration. These symmetry axes may be rotation axes, rotoinversion axes or mirror-plane normals, all possibly combined with time reversal. The usual orientations of the CCS with respect to the symmetry axes can be expressed by the order of the entries in the Hermann–Mauguin symbol. An entry consists (apart from possible primes and bars) of a number N ¼ 1, 2, 3, 4 or 6 or the letter m or N=m (¼ Nm). The conventional rules will be followed: in the monoclinic and orthorhombic crystal systems, the x, y and z axes of the CCS are parallel to the symmetry axes given in the ﬁrst, second and third entries, respectively. In the monoclinic system, there is only one symmetry axis, which is usually chosen parallel to the y axis, and a short Hermann–Mauguin symbol with only one entry is usually used, e.g. 2=m instead of 1 2=m 1. In the trigonal and hexagonal systems, the z, x and y axes are parallel to the symmetry axes given in the ﬁrst, second and third entries, respectively. In the tetragonal system, the z axis is parallel to the symmetry axis given in the ﬁrst entry, and the x and y axes are parallel to the symmetry axes given in the second entry, which appear in two mutually perpendicular directions. In the cubic system, the symmetry axes given in the ﬁrst entry appear in three mutually perpendicular directions; the x, y and z axes of the CCS are chosen parallel to these directions. Alternative orientations of the same point group that give rise to the same form of i have been added between square brackets [] in Table 1.5.7.1. Notice that the Schoenﬂies notation does not allow us to distinguish different orientations of the CCS with respect to the symmetry axes. The forms of i for frequently encountered orientations of the CCS other than those given in Table 1.5.7.1 are (1) 112; 11m; 11 2=m (unique axis z): 2 3 0 0 0 0 14 15 4 0 0 5; 0 0 24 25 31 32 33 0 0 36

Tensor notation Matrix notation T11 T1 T22 T2 T33 T3 T23 ; T32 T4 T31 ; T13 T5 T12 ; T21 T6

134

(2) 1120 ; 11m0 ; 11 20 =m0 (unique axis 2 0 11 12 13 4 21 22 23 0 0 0 0 34

z): 0 0 35

3 16 26 5; 0

(3) 211, m11, 2/m11 (unique axis x): 2 11 12 13 14 0 4 0 0 0 0 25 0 0 0 0 35

3 0 26 5; 36

(4) 20 11; m0 11; 20 =m0 11 (unique axis 2 0 0 0 0 4 21 22 23 24 31 32 33 34

3 16 0 5; 0

x): 15 0 0

1.5. MAGNETIC PROPERTIES Table 1.5.7.1. The forms of the matrix characterizing the piezomagnetic effect Magnetic crystal class Schoenﬂies Hermann–Mauguin

Matrix representation i of the piezomagnetic tensor

C1 Ci

1 1

2

C2 Cs C 2h

2 ð¼ 121Þ m ð¼ 1m1Þ 2=m ð¼ 1 2=m 1Þ (unique axis y)

2

C 2 ðC 1 Þ C s ðC 1 Þ C 2h ðC i Þ

20 ð¼ 120 1Þ m0 ð¼ 1m0 1Þ 20 =m0 ð¼ 1 20 =m0 1Þ (unique axis y)

2

D2 C 2v D2h

222 mm2 ½2mm; m2m mmm

D2 ðC 2 Þ C 2v ðC 2 Þ C 2v ðC s Þ D2h ðC 2h Þ

20 20 2 m0 m0 2 m0 20 m ½20 m0 m m0 m0 m

C4 ; C6 S4 ; C 3h C 4h ; C 6h

4; 6 6 4; 4=m; 6=m

C 4 ðC 2 Þ S4 ðC 2 Þ C 4h ðC 2h Þ

40 4 0 40 =m

D4 ; D6 C 4v ; C6v D2d ; D3h D4h ; D6h

422; 622 4mm; 6mm ½62m ½4m2; 42m 6m2 4=mmm; 6=mmm

D4 ðC 4 Þ; D6 ðC 6 Þ C 4v ðC 4 Þ; C 6v ðC 6 Þ D2d ðS4 Þ; D3h ðC 3h Þ D4h ðC 4h Þ; D6h ðC 6h Þ

420 20 ; 620 20 4m0 m0 ; 6m0 m0 0 20 ½62 0 m0 0 m0 ½4m 0 20 ; 6m 42 4=mm0 m0 ; 6=mm0 m0

D4 ðD2 Þ C 4v ðC 2v Þ D2d ðD2 Þ; D2d ðC 2v Þ D4h ðD2h Þ

40 220 40 mm0 4 0 2m0 ; 4 0 m20 40 =mmm0

C3 S6

3 3

D3 C 3v D3d

32 ð¼ 321Þ 3m ð¼ 3m1Þ ð¼ 3m1Þ 3m

2

D3 ðC 3 Þ C 3v ðC 3 Þ D3d ðS6 Þ

320 ð¼ 320 1Þ 3m0 ð¼ 3m0 1Þ 0 ð¼ 3m 0 1Þ 3m

2

C 6 ðC 3 Þ C 3h ðC 3 Þ C 6h ðS6 Þ

60 6 0 60 =m0

D6 ðD3 Þ C 6v ðC 3v Þ D3h ðD3 Þ; D3h ðC 3v Þ D6h ðD3d Þ

60 220 60 mm0 6 0 2m0 ; 6 0 m20 60 =m0 mm0

T; T h OðTÞ T d ðTÞ Oh ðT h Þ

23; m3 40 320 4 0 3m0 0 m3m

11 4 21 31 0 4 21 0 11 4 0 31

12 22 32

13 23 33

14 24 34

15 25 35

3 16 26 5 36

0 22 0

0 23 0

14 0 34

0 25 0

3 16 0 5 36

12 0 32

13 0 33

0 24 0

15 0 35

3 0 26 5 0

2

14 0 0

0 0 0 40 0 0 0 0 0 2

0 4 0 31

0 0 32

2

0 4 0 31

0 0 33 0 0 33

14 15 0

15 14 0

3 0 05 0

0 0 31

0 0 0

14 15 0

15 14 0

3 0 0 5 36

2

0 0 14 0 0 0 0 0 0

0 40 0 2

0 4 0 31

0 0 31

0 0 33

2

0 0 0 40 0 0 0 0 0 2

11 4 22 31 11 4 0 0

0 0 33

11 0 0

0 0 0

2

0 22 31

11 4 22 0 2

11 4 0 0 2

11 22 0 11 0 0

0 0 0 40 0 0 0 0 0

135

15 0 0

0 15 0 0 14 0

14 15 0 14 0 0

0 0 33

0 15 0 0 0 0

3 0 05 0

3 0 0 5 36

15 14 0

3 222 211 5 0

0 14 0

3 0 211 5 0

15 0 0

3 222 0 5 0

3 0 0 222 0 0 211 5 0 0 0

0 0 0 0 0 0 14 0 0

3 0 05 0

0 14 0

14 0 0

11 22 31

0 4 22 31

3 0 05 0

15 0 0

0 24 0

0 0 31

0 4 0 31 2

3 0 0 5 36

0 25 0

3 0 0 0 211 5 0 0 0 14 0

3 0 0 5 14

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 0 0

0

0

0 0

(5) 22 2 ; 2m m ; mm 2 ½m2 m ; mm0 m0 : 2

11 4 0 0

0

12 0 0

0

13 0 0

0 0 0

0 0 35

3 0 26 5; 0

(6) 20 220 ; m0 2m0 ; 20 mm0 ½m0 m20 ; m0 mm0 : 2

0 4 21 0

0 22 0

0 23 0

0 0 34

0 0 0

3 16 0 5; 0

(7) 40 20 2; 40 m0 m; 4 0 m0 2; 4 0 20 m; 40 =mm0 m: 2

0 4 0 31

0 0 31

0 0 0

0 15 0

15 0 0

3 0 0 5; 0

(8) 60 20 2; 60 m0 m; 6 0 m0 2; 6 0 20 m; 60 =m0 m0 m: 2

0 4 22 0

0 22 0

0 0 0

0 0 0

0 0 0

3 222 0 5; 0

Fig. 1.5.7.1. The dependence of the magnetic moment of CoF2 on the magnetic ﬁeld. (1) Without stress; (2) under the stress Txz = 33.3 MPa (Borovik-Romanov, 1960). (H = 1 kOe corresponds to B = 1 kG = 0.1 T; M = 100 emu mol1 = 0.1 A m2 mol1.)

(9) 312; 31m; 31m: 2

0 4 22 0

0 22 0

0 14 0 0 0 0

0 14 0

~ ¼ ~ 0 þ ðA=2ÞL2 þ ða=2ÞðL2x þ L2y Þ

3

222 0 5; 0

þ ðB=2ÞM2 þ ðb=2ÞðMx2 þ My2 Þ þ dðLx My þ Ly Mx Þ þ 2 1 ðMx Tyz þ My Txz ÞLz þ 2 1 ðLy Tyz þ Lx Txz ÞLz

(10) 3120 ; 31m0 ; 31m0 : 2

11 4 0 31

11 0 31

þ 2 2 Mz Lz Txy þ 2 2 Lx Ly Txy 0 MH: 0 0 33

0 15 0

15 0 0

3 0 211 5: 0

Many connections between the different forms of i given above and in Table 1.5.7.1 have been derived by Kopsky´ (1979a,b) and Grimmer (1991). These connections between the forms that the matrix can assume for the various magnetic or crystallographic point groups hold for all matrices and tensors that describe properties of materials, not just for the special case of piezomagnetism. Dzyaloshinskii (1957b) pointed out a number of antiferromagnets that may display the piezomagnetic effect. These include the ﬂuorides of the transition metals, in which the piezomagnetic effect was ﬁrst observed experimentally (see Fig. 1.5.7.1) (Borovik-Romanov, 1959b). Below we shall discuss the origin of the piezomagnetic effect in ﬂuorides in more detail. The ﬂuorides of transition metals MnF2, CoF2 and FeF2 are tetragonal easy-axis antiferromagnets (see Fig. 1.5.5.3). It is easy ~ up to check that the expansion of the thermodynamic potential to terms that are linear in stress Tij and invariant relative to the transformations of the crystallographic space group D14 4h ¼ P42 =mnm is represented by

ð1:5:7:5Þ

In this expression, the sums (Tij þ Tji ) that appear in the magnetoelastic terms have been replaced by 2Tij , as Tij Tji. The analysis of expression (1.5.7.5) in the absence of stresses proves that ﬂuorides may possess weak ferromagnetism provided that a < 0 (Lz ¼ 0) (see Section 1.5.5.1). Here we shall discuss the easy-axis structure of the ﬂuorides MnF2, CoF2, FeF2 (see Fig. 1.5.5.3b). In the absence of magnetic ﬁelds and stresses only Lz 6¼ 0 for this structure. All other components of the vector L and the magnetization vector M are equal to zero. The magnetic point group is D4h ðD2h Þ ¼ 40 =mmm0. ~ i ; Mj ; Tk‘ Þ [(1.5.7.5)] into the To transform the potential ðL form ðT; T; HÞ [(1.5.7.1)], one has to insert into the magnetoelastic terms the dependence of the components of L and M on the magnetic ﬁeld. The corresponding relations, obtained by minimization of (1.5.7.5) without the magnetoelastic terms, are 0 a H; aðB þ bÞ d2 x 0 a My ¼ H; aðB þ bÞ d2 y Mz ¼ 0 H z ; B

Mx ¼

0 d H; aðB þ bÞ d2 y 0 d Ly ¼ H ; ð1:5:7:6Þ aðB þ bÞ d2 x Lx ¼

Lz ’ constant:

To a ﬁrst approximation, the component Lz does not depend on the magnetic ﬁeld.

136

1.5. MAGNETIC PROPERTIES Inserting the relations (1.5.7.6) for Mi and Li into the magnetoelastic terms of (1.5.7.5), one gets the following expression for the corresponding terms in ðT; Hi ; Tjk Þ: a 1 d 1 ðT; Hi ; Tjk Þ ¼ 0 ðT; Hi Þ þ 0 2Lz T H aðB þ bÞ d2 yz x a 1 d 1

2 T : þ 2Lz T H þ 2L H z aðB þ bÞ d2 xz y B xy z ð1:5:7:7Þ In this case, the expression for the magnetoelastic energy contains only three components of the stress tensor: Tyz , Txz and Txy . Using (1.5.7.4), we get formulas for the three main components of the piezomagnetic effect:

Fig. 1.5.7.2. Linear magnetostriction of CoF2 (Prokhorov & Rudashevskii, 1975). (H = 1 kOe corresponds to B = 1 kG = 0.1 T.)

d 1 a 1 T ¼ 2xyz Tyz ¼ 14 T4 ; aðB þ bÞ d2 yz d 1 a 1 My ¼ 2Lz T ¼ 2yxz Txz ¼ 25 T5 ; aðB þ bÞ d2 xz

Mz ¼ 2Lz 2 Txy ¼ 2zxy Txy ¼ 36 T6 : B

The values of these components are one order of magnitude smaller than for CoF2. The temperature dependence of the components is similar for the piezomagnetic tensor and the sublattice magnetization. This means that the magnetoelastic constants 1 and 2 (as well as the constants B and d) in the relations (1.5.7.7) and (1.5.7.8) depend only slightly on temperature.

Mx ¼ 2Lz

ð1:5:7:8Þ ð1:5:7:9Þ ð1:5:7:10Þ

In all three cases, the piezomagnetic moment is produced in the direction perpendicular to the shear plane. Comparing (1.5.7.8) and (1.5.7.9), we see that 25 ¼ 14 . This is in agreement with the equivalence of the axes x and y in the tetragonal crystals. If the stress is applied in the plane xz (or yz), the vector L turns in the shear plane and a component Lx (or Ly ) is produced: Lx ¼ 2Lz

1 ðB þ bÞ d 1 T : aðB þ bÞ d2 xz

ð1:5:7:11Þ

For Txy stress, no rotation of the vector L occurs. Formulas (1.5.7.8)–(1.5.7.10) show that in accordance with Table 1.5.7.1 the form of the matrix i for the magnetic point group D4h ðD2h Þ ¼ 40 =mmm0 is 2 3 0 0 0 14 0 0 ð1:5:7:12Þ Ki ¼ 4 0 0 0 0 5: 0 14 0 0 0 0 0 36 The relations (1.5.7.8)–(1.5.7.10) show that the components of the piezomagnetic tensor ijk are proportional to the components of the antiferromagnetic vector L. Thus the sign of the piezomagnetic moment depends on the sign of the vector L and the value of the piezomagnetic effect depends on the domain structure of the sample (we are referring to S-domains). The piezomagnetic moment may become equal to zero in a polydomain sample. On the other hand, piezomagnetism may be used to obtain single-domain antiferromagnetic samples by cooling them from the paramagnetic state in a magnetic ﬁeld under suitably oriented external pressure. There are relatively few publications devoted to experimental investigations of the piezomagnetic effect. As mentioned above, the ﬁrst measurements of the values of the components of the tensor ijk were performed on crystals of MnF2 and CoF2 (Borovik-Romanov, 1960). In agreement with theoretical prediction, three components were observed: xyz ¼ yxz and zxy . The largest value obtained for these components was 14 = 21 1010 Oe1 = 26 1012 m A1. The piezomagnetic effect was also observed for two modiﬁcations of -Fe2O3 (Andratskii & Borovik-Romanov, 1966). The magnetic point group of the In low-temperature modiﬁcation of this compound is D3d ¼ 3m. accordance with form (7) given above, the following nonzero components ijk were found for the low-temperature state: xyz ¼ yxz ;

ð1:5:7:13Þ

yyy ¼ yxx ¼ xxy :

ð1:5:7:14Þ

1.5.7.2. Linear magnetostriction From expression (1.5.7.3), it follows that a deformation of the sample may occur in a magnetic ﬁeld. This deformation is linear with respect to the ﬁeld. By its linear dependence, this effect differs essentially from ordinary magnetostriction, which is quadratic in the magnetic ﬁeld. Most substances display such quadratic magnetostriction. The linear magnetostriction may be observed only in those crystals that belong to one of the 66 magnetic point groups that allow piezomagnetism. They are listed in Table 1.5.7.1. The distinctive feature of linear magnetostriction is the dependence of its sign on the sign of the magnetic ﬁeld and on the sign of the antiferromagnetic vector L. The sign of L characterizes the domain state of the specimen. Thus, observation of linear magnetostriction gives information about the domain state. In some materials, it has been observed that a sudden transition from one domain state to the opposite may occur in strong magnetic ﬁelds. Linear magnetostriction (LM) was observed in CoF2 by Borovik-Romanov & Yavelov (1963) in a magnetic ﬁeld applied parallel to the fourfold axis. The relations for the LM in CoF2 can be obtained by differentiating the expression of the thermodynamic potential [(1.5.7.7)]. If the magnetic ﬁeld is applied along the y axis, a deformation Sxz appears: Sxz ¼ @[email protected] ¼ 20 Lz

d 1 a 1 H ¼ 2yxz Hy ¼ 25 H2 : aðB þ bÞ d2 y ð1:5:7:15Þ

A similar formula holds for Syz if the magnetic ﬁeld is applied parallel to the x axis (with 14 , which is equal to 25 ). If the magnetic ﬁeld is applied parallel to the fourfold axis, the Sxy component of the deformation appears: Sxy ¼ @[email protected] ¼ 20 Lz ð 2 =BÞHz ¼ 20 Lz 2 k Hz ¼ 2zxy Hz ¼ 36 H3 :

ð1:5:7:16Þ

If the relations (1.5.7.15) and (1.5.7.16) are compared with (1.5.7.8)–(1.5.7.10), it is apparent that in accordance with theory the components of the tensors of the piezomagnetic effect (PM) and LM are identical. Prokhorov & Rudashevskii (1969, 1975) extended the investigation of LM in CoF2. They discovered that if the applied ﬁeld becomes larger than 20 kOe (Bz > 20 kG = 2 T), a jump in the magnetostriction occurs and it changes its sign (see Fig. 1.5.7.2). This jump is the result of a transition of the magnetic structure

137

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.5.7.2. Experimental data for the piezomagnetic effect (PM) and for linear magnetostriction (LM) a: antiferromagnetic phase; w: weak ferromagnetic phase. Compound

i 1010 (Oe1)

T (K)

PM or LM

Reference†

MnF2 CoF2

14 14 36 36 36 15 15 22 22 22 14 14 14 23

20 20 20 4 6 6 6 78 77 100 78 77 100 292

PM PM PM LM LM LM LM LM PM LM LM PM LM PM

(1) (1) (1) (3) (8) (6) (7) (4) (2) (5) (4) (2) (5) (2)

DyFeO3 YFeO3 YCrO3 -Fe2O3 (a)

-Fe2O3 (w)

’ 0:2 ¼ 21 ¼ 8:2 ¼ 9:8 ¼ 6:0 ¼ 1:7 ’1 ¼ 1:9 ¼ 3:2 ¼ 1:3 ¼ 0:3 ¼ 1:7 ¼ 0:9 ¼ 2:5

The magnetic contribution to the component of the relative permittivity "ij can be represented as a series in the powers of the components of the magnetization and the antiferromagnetic vector. The magnetic birefringence (also called the Cotton– Mouton or Voigt effect) is described by the real symmetrical part of the tensor "ij . In paramagnetic crystals, the magnetization M is proportional to the applied magnetic ﬁeld H, and the series has the form MM M M "ij ¼ QMM ijk‘ Mk M‘ ¼ Qijk‘ kr ‘s Hr Hs ¼ ijrs Hr Hs :

† References: (1) Borovik-Romanov (1959b, 1960); (2) Andratskii & Borovik-Romanov (1966); (3) Prokhorov & Rudashevskii (1969, 1975); (4) Anderson et al. (1964); (5) Levitin & Shchurov (1973); (6) Kadomtseva, Agafonov, Milov et al. (1981); (7) Kadomtseva, Agafonov, Lukina et al. (1981); (8) Zvezdin et al. (1985).

from one domain state (L+) into the opposite state (L). To explain such a transition, one has to take into account the term of third power in the expansion of the magnetic energy (Scott & Anderson, 1966), Um ¼ Ai Hi þ 12ij Hi Hj þ Cijk Hi Hj Hk :

1.5.7.3. Linear magnetic birefringence

The tensor ijrs is symmetric with respect to both the ﬁrst and the second pair of indices. The symmetry of this tensor implies that the diagonal components of the permittivity tensor include magnetic corrections. The modiﬁcation of the diagonal components gives rise to birefringence in cubic crystals and to a change npm of the birefringence in uniaxial and lower-symmetry crystals. It follows from (1.5.7.18) that this birefringence is bilinear in the applied ﬁeld. Bilinear magnetic birefringence can be observed in uniaxial crystals if the magnetic ﬁeld is applied along the x axis perpendicular to the principal z axis. In the simplest case, a difference in the refractive indices nx and ny arises: npm ¼ nx ny ¼

ð1:5:7:17Þ

Cijk is an axial time-antisymmetric tensor, the sign of which depends on the sign of the domain. This term deﬁnes the dependence of the magnetic energy on the sign of the antiferromagnetic domain. To date, CoF2 and MnF2 are unique in that LM and PM occur without rotating the antiferromagnetic vector L if the magnetic ﬁeld is applied along the fourfold axis (or pressure along a h110i axis). In all other cases, these effects are accompanied by a rotation of L and, as a result, the creation of new components Li. To the latter belongs the LM in the low-temperature modiﬁcation of -Fe2O3, which was observed by Anderson et al. (1964) (see also Scott & Anderson, 1966; Levitin & Shchurov, 1973). This compound displays PM, therefore it is obvious that LM will also occur (see Table 1.5.7.1). LM has been observed in some orthoferrites. At low temperatures, the orthoferrite DyFeO3 is a pure antiferromagnet, the vector L of which is aligned along the y axis. Its magnetic point group (D2h ¼ mmm) allows PM and LM. The latter was observed when a magnetic ﬁeld was applied parallel to the z axis by Zvezdin et al. (1985). There it was shown that zxy 6¼ 0 if 0 < H < Hc . At Hc ’ 4 kOe (Bc ’ 4 kG = 0.4 T), there occurs a ﬁrst-order phase transition into a weakly ferromagnetic state with magnetic point group D2h ðC2h Þ ¼ m0 m0 m ðL k Ox; MD k OzÞ. Many orthoferrites and orthochromites that possess weak ferromagnetism belong to the same point group, which possesses an ordinary centre of symmetry. Thus PM and LM are allowed for these phases of orthoferrites. If the magnetic ﬁeld is applied parallel to Ox, they undergo a reorientation transition at which both vectors, L and MD , being orthogonal, rotate in the xz plane. These intermediate angular phases belong to the magnetic point group C 2h ðC i Þ ¼ 20 =m0. LM was observed by Kadomtseva and coworkers (Kadomtseva, Agafonov, Lukina et al., 1981; Kadomtseva, Agafonov, Milov et al., 1981) in two such compounds, YFeO3 and YCrO3. They measured the xxz components of the LM tensor, which are allowed for the D2h ðC 2h Þ ¼ m0 m0 m state. The experimental data obtained to date for PM and LM are summarized in Table 1.5.7.2. The values of the components i can be converted to SI units using 1 Oe1 = 4 103 m A1 = 4 103 T Pa1.

ð1:5:7:18Þ

1 1 ð"xx "yy Þ ¼ ð yyxx ÞHx2 ; 2n0 2n0 xxxx ð1:5:7:19Þ

where n0 is the refractive index for the ordinary beam. Consider now a magnetically ordered crystal which can be characterized by an antiferromagnetic vector L0 and a magnetization vector M0 in the absence of a magnetic ﬁeld. Applying a magnetic ﬁeld with components Hr , we change the direction and L size of L0 and M0 , getting additional components LH k ¼ kr Hr and H M Mk ¼ kr Hr . This is illustrated by the relations (1.5.7.6). Instead of (1.5.7.18) we get ML MM "ij ¼ QLL ijk‘ Lk L‘ þ Qijk‘ Mk L‘ þ Qijk‘ Mk M‘ ML MM ¼ QLL ijk‘ L0k L0‘ þ Qijk‘ M0k L0‘ þ Qijk‘ M0k M0‘ L ML M L MM M þ ½2QLL ijk‘ kr L0‘ þ Qijk‘ ðkr L0‘ þ M0k ‘r Þ þ 2Qijk‘ kr M0‘ Hr :

ð1:5:7:20Þ

The terms in the middle line of (1.5.7.20) show that, in an ordered state, a change in the refractive indices occurs that is proportional to L20 in antiferromagnets and to M02 in ferromagnets. The terms in square brackets show that a linear magnetic birefringence may exist. In the special case of a tetragonal antiferromagnet belonging to the space group D14 4h ¼ P42 =mnm with L0 parallel to the principal axis z, the linear birefringence occurs in the xy plane if the magnetic ﬁeld is applied along the z axis (see Fig. 1.5.5.3). M In this case, M0 ¼ 0, Lkz ¼ 0 for all k, M xz ¼ yz ¼ 0 and M zz ¼ 0 =B [see (1.5.7.6)]. Therefore, the terms in square brackets in (1.5.7.20) differ from zero only for one component of "ij , "xy ¼ QML xyzz L0z 0 Hz =B ¼ qzxy 0 Hz signðL0z Þ:

ð1:5:7:21Þ

As a result, naf ¼ nx0 ny0 ¼

1 1 "xy ¼ q H signðL0z Þ; ð1:5:7:22Þ 2n0 2n0 zxy 0 z

where x0 ; y0 are the optic axes, which in these tetragonal crystals are rotated by =4 relative to the crystallographic axes. Comparing relation (1.5.7.22) with (1.5.7.3), one can see that, like LM, there may be linear magnetic birefringence. The forms of the tensors that describe the two effects are the same. Linear magnetic birefringence has been observed in the uniaxial antiferromagnetic low-temperature modiﬁcation of -Fe2O3

138

1.5. MAGNETIC PROPERTIES Table 1.5.8.1. The forms of the tensor characterizing the linear magnetoelectric effect Magnetic crystal class

Fig. 1.5.7.3. Variation of symmetry of the crystal ﬁeld in the presence of the piezomagnetic effect in CoF2. The unshaded atoms lie at height c=2 above the xy plane (see Fig. 1.5.5.3).

when the magnetic ﬁeld was applied perpendicular to the threefold axis (Le Gall et al., 1977; Merkulov et al., 1981). The most impressive effect was observed in CoF2 when the magnetic ﬁeld was applied along the fourfold axis. The crystal ceased to be optically uniaxial and a difference ðnx0 ny0 Þ / Hz was observed, in accordance with (1.5.7.22). Such linear magnetic birefringence does not exist in the paramagnetic state. Linear birefringence has been observed also in CoCO3 and DyFeO3. For details of these experiments, see Eremenko et al. (1989). These authors also used linear birefringence to make the antiferromagnetic domains visible. A further review of linear magnetic birefringence has been given by Ferre´ & Gehring (1984). Piezomagnetism, linear magnetostriction and linear birefringence in ﬂuorides can be clearly demonstrated qualitatively for one particular geometry. As shown in Fig. 1.5.7.3, the crystallographically equivalent points 1 and 2 are no longer equivalent after a shear deformation applied in the plane xy. During such a deformation, the distances from the magnetic ions to the nearest ﬂuoride ions increase in points 1 and decrease in points 2. As a result, the values of the g-factors for the ions change. Evidently, the changes of the values of the g-factors for different sublattices are opposite in sign. Thus the sublattice magnetizations are no longer equal, and a magnetic moment arises along the direction of sublattice magnetization. On the other hand, if we increase the magnetization of one sublattice and decrease the magnetization of the other by applying a magnetic ﬁeld parallel to the z axis, the interactions with the neighbouring ﬂuoride ions also undergo changes with opposite signs. This gives rise to the magnetostriction. These considerations can be applied only to antiferromagnets with the ﬂuoride structure. In these structures, single-ion anisotropy is responsible for the weak ferromagnetism, not the antisymmetric exchange interaction of the form d½Si Sk .

Hermann–Mauguin

C1 C i ðC 1 Þ

1 0 1

2

C2 C s ðC 1 Þ C 2h ðC 2 Þ

2 ð¼ 121Þ m0 ð¼ 1m0 1Þ 2=m0 ð¼ 1 2=m0 1Þ (unique axis y)

2

Cs C 2 ðC 1 Þ C 2h ðC s Þ

m ð¼ 1m1Þ 20 ð¼ 120 1Þ 20 =m ð¼ 1 20 =m 1Þ (unique axis y)

2

D2 C 2v ðC 2 Þ D2h ðD2 Þ

222 m0 m0 2 ½2m0 m0 ; m0 2m0 m0 m0 m0

2

C 2v D2 ðC 2 Þ C 2v ðC s Þ D2h ðC 2v Þ C 4 ; S4 ðC 2 Þ; C 4h ðC4 Þ C 3 ; S6 ðC 3 Þ C 6 ; C 3h ðC 3 Þ; C 6h ðC 6 Þ

mm2 20 20 2 20 mm0 ½m20 m0 mmm0 0 4; 4 ; 4=m0 0 3; 3 0 6; 6 ; 6=m0

S4 C 4 ðC 2 Þ C 4h ðS4 Þ

4 40 40 =m0

2

D4 ; C 4v ðC 4 Þ D2d ðD2 Þ; D4h ðD4 Þ D3 ; C 3v ðC 3 Þ; D3d ðD3 Þ D6 ; C 6v ðC 6 Þ D3h ðD3 Þ; D6h ðD6 Þ

422; 4m0 m0 0 0 4 2m0 ½4 m0 2; 4=m0 m0 m0 0 32; 3m0 ; 3 m0 0 0 622; 6m m 0 0 6 m0 2 ½6 2m0 ; 6=m0 m0 m0

2

C 4v ; D4 ðC 4 Þ D2d ðC 2v Þ; D4h ðC 4v Þ C 3v ; D3 ðC 3 Þ; D3d ðC 3v Þ C 6v ; D6 ðC 6 Þ D3h ðC 3v Þ; D6h ðC 6v Þ

4mm; 420 20 0 0 4 20 m ½4 m20 ; 4=m0 mm 0 0 3m; 32 ; 3 m 6mm; 620 20 0 0 6 m20 ½6 20 m; 6=m0 mm 0 20 42m; 4m

2

T; T h ðTÞ O; T d ðTÞ; Oh ðOÞ

11 4 21 31

ð1:5:8:1Þ

If (in the absence of a magnetic ﬁeld) an electric ﬁeld E is applied to a crystal with potential (1.5.8.1), a magnetization will be produced:

11 4 0 31 0 4 21 0 11 4 0 0 2

40 220 ; 40 m0 m 40 =m0 m0 m 0

23; m0 3 0 0 432; 4 3m0 ; m0 3 m0

@ ¼ ij Ei : @Hj

12 22 32

3 13 23 5 33

0 22 0

3 13 0 5 33

12 0 32

3 0 23 5 0

0 22 0

3 0 0 5 33

0 4 21 0

12 0 0

3 0 05 0

11 4 12 0

12 11 0

3 0 0 5 33

12 11 0

3 0 05 0

2

11 4 12 0

0 Mj ¼

Curie (1894) stated that materials that develop an electric polarization in a magnetic ﬁeld or a magnetization in an electric ﬁeld may exist. This prediction was given a more precise form by Landau & Lifshitz (1957), who considered the invariants in the expansion of the thermodynamic potential up to linear terms in Hi . For materials belonging to certain magnetic point groups, the thermodynamic potential can be written in the form ¼ 0 ij Ei Hj :

Schoenﬂies

D2d ; D2d ðS4 Þ D4 ðD2 Þ; C 4v ðC 2v Þ D4h ðD2d Þ

1.5.8. Magnetoelectric effect

Matrix representation of the property tensor ij

11 4 0 0

0 4 12 0

2

11 4 0 0 2

11 4 0 0

3 0 0 5 33

0 11 0

12 0 0

3 0 05 0

0 11 0

3 0 05 0

0 11 0

3 0 0 5 11

ð1:5:8:2Þ

Conversely, an electric polarization P arises at zero electric ﬁeld if a magnetic ﬁeld is applied: Pi ¼

@ ¼ ij Hj : @Ei

ð1:5:8:3Þ

This phenomenon is called the magnetoelectric effect. A distinction is made between the linear magnetoelectric effect described above and two types of bilinear magnetoelectric effects. These bilinear effects arise if the thermodynamic potential contains terms of the form Ei Hj Hk or Hi Ej Ek . They will be described in Section 1.5.8.2.

139

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.5.8.1. Linear magnetoelectric effect It is obvious that the linear magnetoelectric effect is forbidden for all dia- and paramagnets, as their magnetic groups possess R as a separate element. The effect is also forbidden if the magnetic space group contains translations multiplied by R, because in these cases the point group also possesses R as a separate element. Since H is an axial vector that changes sign under R and E is a polar vector that is invariant under time inversion, ij is an axial tensor of second rank, the components of which all change sign under time inversion (R). From relation (1.5.8.1), it follows that a magnetic group which allows the magnetoelectric effect cannot possess a centre of symmetry However, it can possess it multiplied by R (Ci R ¼ 1 0 ) (Ci ¼ 1). (see Table 1.5.8.1). There are 21 magnetic point groups that possess a centre of symmetry. The detailed analysis of the properties of the tensor ij shows that among the remaining 69 point groups there are 11 groups for which the linear magnetoelectric effect is also forbidden. These groups C6 ðC 3 Þ ¼ 60 , C 6h ðC 3h Þ ¼ 60 =m, D3h ¼ 6m2, D3h ðC3h Þ are C 3h ¼ 6, 0 20 , D6h ðD3h Þ ¼ 60 =mmm0 , D6 ðD3 Þ ¼ 60 220 , C 6v ðC 3v Þ ¼ 60 m0 m, = 6m OðTÞ ¼ 40 320 and Oh ðT d Þ ¼ m0 3 0 m. T d ¼ 43m, All remaining 58 magnetic point groups in which the linear magnetoelectric effect is possible are listed in Table 1.5.8.1. The 11 forms of tensors that describe this effect are also listed in this table.3 The orientation of the axes of the Cartesian coordinate system (CCS) with respect to the symmetry axes of the crystal is the same as in Table 1.5.7.1. Alternative orientations of the same point group that give rise to the same form of ij have been added between square brackets in Table 1.5.8.1. The tensor has the same form for 32 ð¼ 321Þ and 312, 3m0 1 and 31m0 , 3 0 m0 1 and 3 0 1m0 ; it also has the same form for 3m1 and 31m, 320 1 and 3120 , 3 0 m1 and 3 0 1m. The forms of ij for frequently encountered orientations of the CCS other than those given in Table 1.5.8.1 are (cf. Rivera, 1994, 2009) (1) 112; 11m0 ; 11 2=m0 (unique axis z): 2 3 11 12 0 4 21 22 0 5; 0 0 33 (2) 11m; 1120 ; 11 20 =m (unique axis z): 2 3 0 0 13 4 0 0 23 5; 31 32 0 (3) 211; m0 11; 2=m0 11 (unique axis x): 2 3 0 11 0 4 0 22 23 5; 0 32 33 (4) m11; 20 11; 20 =m11 (unique axis x): 2 3 0 12 13 4 21 0 0 5; 0 31 0 3

Table 1.5.8.1 shows that the tensor ij describing the magnetoelectric effect does not need to be symmetric for 31 of the 58 point groups. Its trace 11 + 22 + 33 is a relativistic pseudoscalar (Hehl et al., 2009). These 31 groups coincide with those that admit a spontaneous toroidal moment (Gorbatsevich & Kopaev, 1994); they were ﬁrst determined by Ascher (1966) as the magnetic point groups admitting spontaneous currents. For recent developments see Schmid (2008) and Spaldin et al. (2008).

(5) 2mm; 220 20 ; m0 m20 ½m0 20 m; m0 mm: 2 3 0 0 0 4 0 0 23 5; 0 32 0 (6) m2m; 20 220 ; mm0 20 ½20 m0 m; mm0 m: 2 3 0 0 13 4 0 0 0 5; 31 0 0 0 m0 ; 40 20 2; 40 mm0 ; 40 =m0 mm0 : (7) 4m2; 42 2 3 0 12 0 4 12 0 0 5: 0 0 0

As mentioned above, the components of the linear magnetoelectric tensor change sign under time inversion. The sign of these components is deﬁned by the sign of the antiferromagnetic vector L, i.e. by the sign of the 180 domains (S-domains). This is like the behaviour of the piezomagnetic effect and, therefore, everything said above about the role of the domains can be applied to the magnetoelectric effect. Dzyaloshinskii (1959) proposed the antiferromagnetic Cr2O3 as the ﬁrst candidate for the observation of the magnetoelectric (ME) effect. He showed that the ME tensor for this compound has three nonzero components: 11 ¼ 22 and 33 . The ME effect in Cr2O3 was discovered experimentally by Astrov (1960) on an unoriented crystal. He veriﬁed that the effect is linear in the applied electric ﬁeld. Folen et al. (1961) and later Astrov (1961) performed measurements on oriented crystals and revealed the anisotropy of the ME effect. In these ﬁrst experiments, the ordinary magnetoelectric effect MEE (the electrically induced magnetization) was investigated by measuring the magnetic moment induced by the applied electric ﬁeld. Later Rado & Folen (1961) observed the converse effect MEH (the electric polarization induced by the magnetic ﬁeld). The temperature dependence of the components of the magnetoelectric tensor in Cr2O3 was studied in detail in both laboratories. In the following years, many compounds that display the linear magnetoelectric effect were discovered. Both the electrically induced and the magnetically induced ME effect were observed. The values of the components of the magnetoelectric tensor range from 106 to 102 in compounds containing the ions of the iron group and from 104 to 102 in rare-earth compounds. Cox (1974) collected values of max of the known magnetoelectrics. Some are listed in Table 1.5.8.2 together with more recent results. Additional information about the experimental data is presented in six conference proceedings. The ﬁrst ﬁve are given as references [4] to [8] in Fiebig (2005), the sixth in Fiebig & Spaldin (2009). The values of ij are given in rationalized Gaussian units, where ij is dimensionless. Some authors follow Dzyaloshinskii (1959) in writing (1.5.8.1) as ¼ 0 ð0ij =4ÞEi Hj , where 0ij are the non-rationalized Gaussian values of the components of the magnetoelectric tensor. If SI units are used, then (1.5.8.1) becomes ¼ 0 SI ij Ei Hj . The connections between the values of the tensor components expressed in these three systems are 4ij ¼ 0ij ¼ 3 108 SI ij :

ð1:5:8:4Þ

1 The units of SI ij are s m . A detailed discussion of the relations between the descriptions of the magnetoelectric effect in different systems of units is given by Rivera (1994).

140

1.5. MAGNETIC PROPERTIES Table 1.5.8.2. A list of some magnetoelectrics max is the maximum observed value of ij expressed in rationalized Gaussian units. Compound

TN or TC (K)

Magnetic point group

max

References†

Fe2TeO6 DyAlO3 GdAlO3 TbAlO3 TbCoO3 Cr2O3

219 3.5 4.0 4.0 3.3 318

4=m0 m0 m0 m0 m0 m0 m0 m0 m0 m0 m0 m0 0 mmm 0 3 m0

3 105 2 103 1 104 1 103 3 105 1 104

Nb2Mn4O9 Nb2Co4O9 Ta2Mn4O9 Ta2Co4O9 LiMnPO4 LiFePO4 LiCoPO4 LiNiPO4 GdVO4 TbPO4 DyPO4 HoPO4 Mn3B7O13I Co3B7O13Cl Co3B7O13Br Co3B7O13I Ni3B7O13I

110 27 104 21 35 50 22 23 2.4 2.2 3.4 1.4 26 12 17 38 61.5

0 3 0 m0 3 0 m0 3 0 m0 3 m0 m0 m0 m0 mmm0 mmm0 mmm0 40 =m0 m0 m 40 =m0 m0 m 40 =m0 m0 m 40 =m0 m0 m m0 m20 m m0 m20 m0 m20 m0

2 106 2 105 1 105 1 104 2 105 1 104 7 104 4 105 3 104 1 102 1 103 2 104 2 106 3 104 2 103 1 103 2 104

Ni3B7O13Cl Cu3B7O13Cl FeGaO3 TbOOH DyOOH ErOOH Gd2CuO4 MnNb2O6 MnGeO3 CoGeO3 CrTiNdO5

9 8.4 305 10.0 7.2 4.1 6.5 4.4 16 31 13

m0 m20 m0 m0 2 m0 m20 2=m0 2=m0 20 =m mmm0 mmm0 mmm0 mmm0 mmm0

2 104 3 106 4 104 4 104 1 104 5 104 1 104 3 106 2 106 1 104 1 105

7–9, 70 11–13 14 12, 15–17 12, 16, 18 45–49, 70, 71, W162 52, 53 52, 53 53 53 55, 56, 58, 60 57, 58 54, 55, R161 54, 55, 61 70 see text 68, 69 72 C204 S204 88C1 90C3 74, 75, 77–79, 90C2 74R2, 91R1 88R1 84–86 114 92, 114 93, 114 W161 101, 102 98–100 70 70, 89

Fig. 1.5.8.1. Temperature dependence of the components k and ? in Cr2O3 (Astrov, 1961). (SI = 4/c s m1.)

The temperature dependences determined for the ME moduli, k and ? , of Cr2O3 are quite different (see Fig. 1.5.8.1). The temperature dependence of ? is similar to that of the order parameter (sublattice magnetization M0 ), which can be explained easily, bearing in mind that the magnetoelectric moduli are proportional to the magnitude of the antiferromagnetic vector ( / Lz ¼ 2M0 ). However, to explain the rather complicated temperature dependence of k, it becomes necessary to assume that the moduli are proportional to the magnetic susceptibility of the crystal so that (Rado, 1961; Rado & Folen, 1962) k ¼ ak k Lz ;

† Numbers refer to references quoted by Cox (1974); codes 88C1, 90C3, 88R1, 90C2, 74R2, 91R1 refer to references quoted by Burzo (1993); and codes W162, R161, C204, S204 and W161 refer to articles in Ferroelectrics, 162, 141, 161, 147, 204, 125, 204, 57 and 161, 133, respectively.

Most magnetoelectrics are oxides containing magnetic ions. The ions of the iron group are contained in corundum-type oxides [magnetic point group D3d ðD3 Þ ¼ 3 0 m0 ], triphyllitetype oxides with different magnetic groups belonging to the orthorhombic crystallographic structure D2h ¼ mmm and other compounds. The rare-earth oxides are represented by the orthorhombic RMO3 structure with R = rare earth, M = Fe3+, Co3+, Al3+ [magnetic point group D2h ðD2 Þ ¼ m0 m0 m0 ], tetragonal zircon-type compounds RMO4 (R = rare earth, M = P, V) [magnetic point group D4h ðD2d Þ ¼ 40 =m0 m0 m], monoclinic oxide hydroxides ROOH [magnetic point groups C2h ðC2 Þ ¼ 2=m0, C 2h ðC s Þ ¼ 20 =m] and other compounds. Of particular interest is TbPO4, which has the highest value for a magnetoelectric tensor component, namely 1.1 102 at 2.2 K, where the point group is 40 /m0 m0 m (Rado & Ferrari, 1973; Rado et al., 1984) and 1.7 102 at 1.5 K, where the point group is 20 /m (Rivera, 2009). There are also some weak ferromagnets and ferrimagnets that exhibit the linear magnetoelectric effect. An example is the weakly ferromagnetic boracite Ni3B7O13I. These orthorhombic compounds will be discussed in Section 1.5.8.3. Another orthorhombic magnetoelectric crystal is ferrimagnetic FeGaO3 (Rado, 1964; see Table 1.5.8.2). It has been shown in experiments with Cr2O3 that in the spinﬂop phase k becomes zero but an off-diagonal component xz arises (Popov et al., 1992). Such behaviour is possible if under the spin-ﬂop transition the magnetic point group of Cr2O3 transforms from D3d ðD3 Þ ¼ 3 0 m0 to C2h ðCs Þ ¼ 1120 =m. For the latter magnetic point group, the ME tensor possesses only transverse components.

? ¼ a ? ? L z ;

ð1:5:8:5Þ

where ak and a? are new constants of the magnetoelectric effect which do not depend on temperature. Formulas (1.5.8.5) provide a good explanation of the observed temperature dependence of . The linear relation between and Lz ¼ 2M0 is also proved by the fact that when studying the ME effect, the domain structure of the sample is revealed. An annealing procedure to prepare a single-domain sample has been developed. To perform this annealing, the sample must be heated well above the Ne´el temperature and then cooled below TN in the presence of electric and magnetic ﬁelds. The directions of these ﬁelds have to agree with the allowed components of the ME tensor. In some compounds, a single-domain state may be obtained by applying simultaneously pulses of both ﬁelds to a multidomain sample at temperatures below TN (see O’Dell, 1970). It was shown in the previous section that the piezomagnetic effect can be explained phenomenologically as weak ferromagnetism caused by the change of the symmetry produced by deformation of the lattice. The electric ﬁeld may act indirectly inducing atomic displacements (similar to the displacements under stress) and as in piezomagnetism may cause the rise of a magnetic moment. Such ideas were proposed by Rado (1964) and expanded by White (1974). The electric ﬁeld may act directly to change the admixture of orbital states in the electron wavefunctions. As a result of such a direct action, there may be a change of different terms in the microscopic spin Hamiltonian. Correspondingly, the following mechanisms are to be distinguished. Changes in the g-tensor can explain the ME effect in DyPO4 (Rado, 1969). The electric-ﬁeldinduced changes in single-ion anisotropy may represent the main mechanism of the ME effect in Cr2O3 (Rado, 1962). Two other mechanisms have to be taken into account: changes in the symmetric and antisymmetric exchange interactions. For details and references see the review article of de Alcantara Bonﬁm & Gehring (1980).

141

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.5.8.2. Nonlinear magnetoelectric effects Along with linear terms in E and H, the thermodynamic potential may also contain invariants of higher order in Ek ; Hi : ¼ 0 ik Ei Hk 12 ijk Ei Hj Hk 12 ijk Hi Ej Ek :

ð1:5:8:6Þ

From this relation, one obtains the following formulas for the electric polarization Pi and the magnetization Mi : Pi ¼ ik Hk þ 12 ijk Hj Hk þ jik Hj Ek ; 0 Mi

¼ ki Ek þ jik Ej Hk þ

1 2 ijk Ej Ek :

ð1:5:8:7Þ ð1:5:8:8Þ

The third term in (1.5.8.7) describes the dependence of the dielectric susceptibility (eik ¼ Pi =Ek ) and, consequently, of the permittivity "ik on the magnetic ﬁeld. Similarly, the second term in (1.5.8.8) points out that the magnetic susceptibility m may contain a term jik Ej , which depends on the electric ﬁeld. The tensors ijk and ijk are symmetric in their last two indices. Symmetry imposes on ijk the same restrictions as on the piezoelectric tensor and on ijk the same restrictions as on the piezomagnetic tensor (see Table 1.5.7.1). Ascher (1968) determined all the magnetic point groups that allow the terms EHH and HEE in the expansion of the thermodynamic potential . These groups are given in Table 1.5.8.3, which has been adapted from a table given by Schmid (1973). It classiﬁes the 122 magnetic point groups according to which types of magnetoelectric effects (EH, EHH or HEE) they admit and whether they admit spontaneous electric polarization (E) or spontaneous magnetization (H). It also classiﬁes the 122 point 10 or 1 0 , as in a table groups according to whether they contain 1, given by Mercier (1974). Ferromagnets, ferrimagnets and weak ferromagnets have a point group characterized by H (the 31 groups of types 4–7 in Table 1.5.8.3); dia- and paramagnets as well as antiferromagnets with a nontrivial magnetic Bravais lattice have a point group containing 10 (the 32 groups of types 1, 13, 17 and 19 in Table 1.5.8.3). The 59 remaining point groups describe antiferromagnets with a trivial Bravais lattice. The 31 point groups characterized by E, the 32 containing 1 and the 59 remaining ones correspond to a similar classiﬁcation of crystals according to their electric properties (see Schmid, 1973).

Table 1.5.8.3 shows that for the 16 magnetic point groups of types 16–19, any kind of magnetoelectric effect is prohibited. These are the 11 grey point groups that contain all three inver the grey group (O þ ROÞ = sions, the white group Oh ¼ m3m, 43210 and the three black–white groups C 6h ðC 3h Þ = 60 =m, D6h ðD3h Þ = 60 =mmm0 and Oh ðT d Þ = m0 3 0 m. Among the 58 magnetic point groups that allow the linear magnetoelectric effect, there are 19 that do not allow the nonlinear effects EHH and HEE (types 10 and 11 in Table 1.5.8.3). The remaining 39 groups are compatible with all three effects, EH, EHH and HEE; 19 of these groups describe ferromagnets (including weak ferromagnets) and ferrimagnets (types 4 and 5 in Table 1.5.8.3). The 21 point groups of types 7, 14 and 15 allow only the except magnetoelectric effect HEE. These groups contain C i ¼ 1, 40 320 . The compounds belonging to these groups possess only one tensor of magnetoelectric susceptibility, the tensor ijk of the nonlinear ME effect. The effect is described by Pi 0 Mi

¼ jik Hj Ek ; ¼

ð1:5:8:9Þ

1 2 ijk Ej Ek :

ð1:5:8:10Þ

The magnetic point group of ferrimagnetic rare-earth garnets 0, which is of type 7. RFe5O12 (R ¼ Gd, Y, Dy) is D3d ðS6 Þ ¼ 3m Therefore, the rare-earth garnets may show a nonlinear ME effect corresponding to relations (1.5.8.9) and (1.5.8.10). This was observed by O’Dell (1967) by means of a pulsed magnetic ﬁeld. As mentioned above, this effect may be considered as the dependence of the permittivity on the magnetic ﬁeld, which was the method used by Cardwell (1969) to investigate this ME effect experimentally. Later Lee et al. (1970) observed the ME effect deﬁned by relation (1.5.8.10). Applying both static electric ﬁelds and alternating ones (at a frequency !), they observed an alternating magnetization at both frequencies ! and 2!. A nonlinear ME effect of the form HEE was also observed in the weakly ferromagnetic orthoferrites TbFeO3 and YbFeO3. Their magnetic point group is D2h ðC2h Þ ¼ m0 m0 m. Moreover, paramagnets that do not possess an inversion centre Ci ¼ 1 may show an ME effect if the point group is not 43210 . They have one of the 20 grey point groups given as types 1 or 13

Table 1.5.8.3. Classiﬁcation of the 122 magnetic point groups according to magnetoelectric types

Type 1 2 3 4 5 6 7

Inversions in the group 10

Permitted terms in thermodynamic potential E E E E

1

8

EH H H H H

0 1

12 13 14 15

1

16 17 18 19

0 1 10 1 10 ; 1 0 1;

10

HEE HEE

EH EH

EHH EHH EHH

HEE HEE HEE HEE

EH

EHH

HEE

EHH

HEE

9 10 11

EHH EHH EHH

EH EH

EHH EHH HEE HEE

Magnetic point groups

Number of magnetic point groups

10 , 210 , m10 , mm210 , 410 , 4mm10 , 310 , 3m10 , 610 , 6mm10 60 , 60 mm0 mm2, 4mm, 40 , 40 mm0 , 3m, 6mm

10 2 6

1, 2, m, 20 , m0 , m0 m20 , m0 m0 2, 4, 4m0 m0 , 3, 3m0 , 6, 6m0 m0 42 0 m0 , 320 , 620 20 20 20 2, 420 20 , 4, 6m 0 20 6, 2=m, 20 =m0 , m0 m0 m, 4=m, 4=mm0 m0 , 3, 3m 0 , 6=m, 1, 0 0 6=mm m 0 0 0 0 0 222,0 4 , 422, 42m, 40 220 , 4 2m0 , 4 20 m, 32, 6 , 622, 6 m0 2, 6 m20 , 23, 4 0 3m0 6m2, 60 220

13 6 2 10

432 0 0 1 , 2=m0 , 20 =m, mmm0 , m00 m00m0 , 4=m ; 40 =m0 , 4=m0 m0 m0 , 0 4=m0 mm, 40 =m0 0 m0 m,0 3 , 3 m0 , 3 m, 6=m0 , 6=m0 m0 m0 , 6=m0 mm, m0 3 , m0 3 m0 43m 0 0 0 0 , 62210 , 6m21 0 , 42210 , 42m1 22210 , 41 , 3210 , 61 , 2310 , 43m1 40 320 60 =m0 , 6=mmm, mmm, 40 =m, 4=mmm, 40 =mmm0 , 3m, m3m 0 60 =m0 m0 m, m3, 0 60 =m, 60 =mmm0 , m0 3 m 0 4321 m3m 0 , 2=m10 , mmm10 , 4=m10 , 4=mmm10 , 31 0 , 3m1 0 , 6=m10 , 11 0 , m3m1 0 6=mmm10 , m31

1 18

19

1 10 1 10

11

142

31

49

31

14

73

2

3 1 1 11

11 16

122

1.5. MAGNETIC PROPERTIES in Table 1.5.8.3. Bloembergen (1962) pointed out that all these paramagnets are piezoelectric crystals. He called the ME effect in these substances the paramagnetoelectric (PME) effect. It is deﬁned by the nonzero components of the tensor ijk : Pi ¼ 12 ijk Hj Hk ; 0 Mi ¼ jik Ej Hk :

ð1:5:8:11Þ ð1:5:8:12Þ

The PME effect was discovered by Hou & Bloembergen (1965) in NiSO46H2O, which belongs to the crystallographic point group D4 ¼ 422. The only nonvanishing components of the third-rank tensor are xyz ¼ xzy ¼ yzx ¼ yxz ¼ ( 14 ¼ 25 ¼ 2

in matrix notation), so that P ¼ ðHy Hz ; Hx Hz ; 0Þ and 0 M ¼ (Ey Hz , Ex Hz , Ex Hy Ey Hx ). Both effects were observed: the polarization P by applying static (Hz ) and alternating (Hx or Hy ) magnetic ﬁelds and the magnetization M by applying a static magnetic ﬁeld Hz and an alternating electric ﬁeld in the plane xy. As a function of temperature, the PME effect shows a peak at 3.0 K and changes sign at 1.38 K. The coefﬁcient of the PME effect at 4.2 K is

ð4:2 KÞ ¼ 2:2 109 cgs units ¼ 1:16 1018 s A1 :

ð1:5:8:13Þ

The theory developed by Hou and Bloembergen explains the PME effect by linear variation with the applied electric ﬁeld of the crystal-ﬁeld-splitting parameter D of the spin Hamiltonian. Most white and black–white magnetic point groups that do not either by itself or multiplied by contain the inversion (C i ¼ 1), R ¼ 10 , admit all three types of ME effect: the linear (EH) and two higher-order (EHH and HEE) effects. There are many magnetically ordered compounds in which the nonlinear ME effect has been observed. Some of them are listed by Schmid (1973); more recent references are given in Schmid (1994a). In principle, many ME effects of higher order may exist. As an example, let us consider the piezomagnetoelectric effect. This is a combination of piezomagnetism (or piezoelectricity) and the ME effect. The thermodynamic potential must contain invariants of the form ¼ 0 ijk‘ Ei Hj Tk‘ :

ð1:5:8:14Þ

The problem of the piezomagnetoelectric effect was considered by Rado (1962), Lyubimov (1965) and in detail by Grimmer (1992). All 69 white and black–white magnetic point groups that possess neither C i ¼ 1 nor R ¼ 10 admit the piezomagnetoelectric effect. (These are the groups of types 2–6, 8–12, 14 and 16 in Table 1.5.8.3.) The tensor ijk‘ , which describes the piezomagnetoelectric effect, is a tensor of rank 4, symmetric in the last two indices and invariant under space-time inversion. This effect has not been observed so far (Rivera & Schmid, 1994). Grimmer (1992) analysed in which antiferromagnets it could be observed. 1.5.8.3. Multiferroics4 Initially, Schmid deﬁned multiferroics as materials with two or three primary ferroics coexisting in the same phase, such as ferromagnetism, ferroelectricity or ferroelasticity (Schmid, 1994b). The term primary ferroics was deﬁned in a thermodynamic classiﬁcation, distinguishing primary, secondary and tertiary ferroics (Newnham, 1974; Newnham & Cross, 1976). For magnetoelectric multiferroics, however, it has become customary to loosen this deﬁnition. Magnetoelectric multiferroics are now considered materials with coexisting magnetic (ferro- or antiferromagnetic) and ferroelectric order. They can be divided into two classes: multiferroics where the origins of ferroelectricity 4

Updated by M. Kenzelmann.

Table 1.5.8.4. List of the magnetic point groups of the ferromagnetoelectrics Symbol of symmetry group Schoenﬂies Hermann–Mauguin

Allowed direction of P M

C1 C2 C 2 ðC1 Þ C s ¼ C 1h C s ðC 1 Þ C 2v ðC 2 Þ C 2v ðC s Þ C4 C 4v ðC 4 Þ C3 C 3v ðC 3 Þ C6 C 6v ðC 6 Þ

Any k2 k 20 km k m0 k2 k 20 k4 k4 k3 k3 k6 k6

1 2 20 m m0 m0 m0 2 m0 m20 4 4m0 m0 3 3m0 6 6m0 m0

Any k2 ? 20 ?m k m0 k2 ?m k4 k4 k3 k3 k6 k6

and magnetic order are independent, and multiferroics where ferroelectricity is induced by magnetic or orbital order. For the case of magnetically commensurate ferromagnetic ferroelectrics, Neronova & Belov (1959) pointed out that there are ten magnetic point groups that admit the simultaneous existence of spontaneous ferroelectric polarization P and magnetic polarization M, which they called ferromagnetoelectrics. Neronova and Belov considered only structures with parallel alignment of P and M (or L). There are three more groups that allow the coexistence of ferroelectric and ferromagnetic order, in which P and M are perpendicular to each other. Shuvalov & Belov (1962) published a list of the 13 magnetic groups that admit the coexistence of ferromagnetic and ferroelectric order. These are the groups of type 4 in Table 1.5.8.3; they are given with more details in Table 1.5.8.4. Notice that P and M must be parallel in eight point groups, they may be parallel in 1 and m0 , and they must be perpendicular in 20 , m and m0 m20 (see also Ascher, 1970). The magnetic point groups listed in Table 1.5.8.4 admit not only ferromagnetism (and ferrimagnetism) but the ﬁrst seven also admit antiferromagnetism with weak ferromagnetism. Ferroelectric pure antiferromagnets of type IIIa may also exist. They must belong to one of the following eight magnetic point groups (types 2 and 3 in Table 1.5.8.3): C2v = mm2; C4v = 4mm; C4(C2) = 40 ; C4v(C2v) = 40 mm0 ; C3v = 3m; C6v = 6mm; C6(C3) = 60 ; C6v(C3v) = 60 mm0 . Table 1.5.8.3 shows that the linear magnetoelectric effect is admitted by all ferroelectric ferromagnets and all ferroelectric antiferromagnets of type IIIa except 60 and 60 mm0 . The ﬁrst experimental evidence to indicate that complex perovskites may become ferromagnetoelectric was observed by the Smolenskii group (see Smolenskii et al., 1958). They investigated the temperature dependence of the magnetic susceptibility of the ferroelectric perovskites Pb(Mn1/2Nb1/2)O3 and Pb(Fe1/2Nb1/2)O3. The temperature dependence at T > 77 K followed the Curie–Weiss law with a very large antiferromagnetic Weiss constant. Later, Astrov et al. (1968) proved that these compounds undergo a transition into a weakly ferromagnetic state at Ne´el temperatures TN = 11 and 9 K, respectively. The single crystals of boracites synthesized by Schmid (1965) raised wide interest as examples of ferromagnetic ferroelectrics. The boracites have the chemical formula M3B7O13X (where M = Cu2+, Ni2+, Co2+, Fe2+, Mn2+, Cr2+ and X = F, Cl, Br, I, OH, NO 3 ). Many of them are ferroelectrics and weak ferromagnets at low temperatures. This was ﬁrst shown for Ni3B7O13I (see Ascher et al., 1966). The symmetries of all the boracites are cubic at high 0 temperatures and their magnetic point group is 43m1 . As the temperature is lowered, most become ferroelectrics with the magnetic point group mm210. At still lower temperatures, the spins of the magnetic ions in the boracites go into an antiferromagnetic state with weak ferromagnetism. For some of the boracites the ferromagnetic/ferroelectric phase belongs to the group m0 m20 , and for others to m0 m0 2, m0 , m or 1. In accordance with Table 1.5.8.4, the spontaneous polarization P is oriented

143

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.5.8.5. Irreducible representations of the group Gk for TbMnO3 (Kenzelmann et al., 2005) 1 2 3 4

Fig. 1.5.8.2. The hysteresis loop of the linear magnetoelectric effect in ferroelectric and weakly ferromagnetic Ni3B7O13I at 46 K (Ascher et al., 1966). H = 1 kOe corresponds to B = 1 kG = 0.1 T.

perpendicular to the weak ferromagnetic moment MD for the groups m0 m20 and m. Boracites feature a complicated behaviour in external magnetic and electric ﬁelds, which depends strongly on the history of the samples. Changing the direction of the electric polarization by an electric ﬁeld also changes the direction of the ferromagnetic vector (as well as the direction of the antiferromagnetic vector) and vice versa. As an example, Fig. 1.5.8.2 shows the results of measurements on Ni–I boracite with spontaneous polarization along [001] and A magnetic ﬁeld spontaneous magnetization initially along [1 10]. was applied along [110] and the polarization induced along [001] was measured. If the applied ﬁeld H was increased beyond 6 kOe (B = 6 kG = 0.6 T), the induced polarization changed sign because the spontaneous magnetization had been reversed. The applied magnetic ﬁeld was reversed to obtain the rest of the hysteresis loop describing the MEk response. If the spontaneous polarization is reversed, e.g. by applying an electric ﬁeld, the spontaneous magnetization will rotate simultaneously by 90 around the polarization axis. Applying magnetic ﬁelds as described above will no longer produce a measurable polarization. If, however, the crystal is rotated by 90 around the polarization axis before repeating the experiment, a hysteresis loop similar to Fig. 1.5.8.2, but turned upside down, will be obtained (cf. Schmid, 1967). The similarity of the jumps in the curves of linear magnetostriction (see Fig. 1.5.7.2) and magnetoelectric effect in Ni-I boracite is noteworthy. More details on multiferroic boracites are given in Schmid (1994b). Materials can be multiferroic when magnetic order occurs in a ferroelectric material. An important example of this type of multiferroic is BiFeO3, where ferroelectricity arises from the lone-pair activity of the Bi ion. Early on, BiFeO3 was shown to be an antiferromagnet below TN = 643 K using neutron scattering (Kiselev et al., 1962; Michel et al., 1969) and magnetic measurements (Smolenskii et al., 1962; see also Venevtsev et al., 1987). BiFeO3 also possesses a spontaneous ferroelectric polarization. The magnetic point group above TN is 3m10 , and it was suggested that below TN , the magnetic point group is 3m. However, it was shown that the magnetic structure is incommensurately spatially modulated (Sosnovska et al., 1982). Ferroelectric monodomain crystals were used to study the relationship between the direction of the ferroelectric polarization and the magnetic structure (Lebeugle et al., 2008). It was found that the easy-axis plane, in which the magnetic moments are ordered, depends on the direction of the ferroelectric polarization. The antiferromagnetic structure can thus be changed by the application of electric ﬁelds. Another important example of multiferroicity where magnetic order appears in a ferroelectric material is YMnO3. Here, ferroelectricity arises from a complex rotation of the oxygen

1

2y

mz

mx

1 1 1 1

1 1 1 1

1 1 1 1

1 1 1 1

environment of the transition-metal ions (Bertaut et al., 1964). YMnO3 becomes ferroelectric at Tc = 193 K (with paramagnetic point group 6mm10 ) and antiferromagnetic at TN = 77 K. The antiferromagnetic ordering was also proved by investigating the Mo¨ssbauer effect (Chappert, 1965). The most recent neutron measurements, using neutron polarimetry, suggest that the magnetic space group is P60 3 (Brown & Chatterji, 2006). The symmetries of both antiferromagnetic ferroelectrics, BiFeO3 and YMnO3, do not allow weak ferromagnetism according to Table 1.5.5.2, and indeed experimentally no spontaneous ferromagnetic moment has been found in the bulk. In another important class of multiferroics, ferroelectricity is generated by spontaneous magnetic order. Some of the ﬁrst studies of these kinds of materials were done in the late 1970s on Cr2BeO4 (Newnham et al., 1978). It had already been shown that the magnetic structure is a cycloidal spiral at low temperatures (Cox et al., 1969). Pyroelectric measurements showed that Cr2BeO4 is ferroelectric below TN = 28 K, and it was noted that the magnetic structure breaks all symmetry elements of the space groups. In 2003, it was shown that TbMnO3 features ferroelectricity below Tc = 27 K (Kimura et al., 2003). TbMnO3 adopts antiferromagnetic order below TN = 42 K, and the ferroelectric onset coincides with a second magnetic transition, which was thought to be a lock-in transition to a commensurate structure. No ferromagnetic order is observed in TbMnO3. Neutron diffraction showed that the magnetic structure remains incommensurate at all temperatures, and that the onset of ferroelectricity coincides with the onset of cycloidal magnetic order (Kenzelmann et al., 2005). The cycloidal order is described by two irreducible representations of the group Gk of those elements of mmm that leave the magnetic modulation vector k = (0, q, 0) invariant. Harris introduced a trilinear coupling theory that clariﬁed the relation between the symmetry of the magnetic structure and ferroelectricity (Kenzelmann et al., 2005; Harris, 2007). Ferroelectricity in TbMnO3 directly emerges from the magnetic symmetry breaking that creates a polar axis along which ferroelectric polarization is observed. In the case of TbMnO3, the trilinear coupling between the magnetic and ferroelectric order takes the form H ¼ Vijk Mi ðkÞMj ðkÞPk :

ð1:5:8:15Þ

Here Vijk is a coupling term that couples the incommensurate order parameters Mi and Mj with the ferroelectric polarization Pk. Such a coupling term conserves translational symmetry and has to be invariant under all symmetry elements of the space group. If Mi and Mj belong to the same one-dimensional irreducible representation, Pk has to be invariant under all symmetry elements of the space group and, consequently, has to vanish. If, however Mi and Mj belong to two different one-dimensional irreducible representations, this allows for a nonzero ferroelectric polarization Pk. For temperatures between Tc = 27 K and TN = 41 K, the magnetic structure is described only by one irreducible representation, namely 3 (as deﬁned in Table 1.5.8.5). As a result, there can be no ferroelectric polarization. Below Tc , however, the magnetic structure is described by two irreducible representations, 2 and 3. Since the coupling term H has to be invariant under all symmetry elements of the space group, the ferroelectric polarization has to transform as the product of 2

144

1.5. MAGNETIC PROPERTIES and 3, which is 4. Therefore, the ferroelectric polarization is only allowed along the c axis, as is experimentally observed. Magnetically induced ferroelectricity is also possible for commensurate structures. Examples include some of the phases in the RMn2O5 series (Hur et al., 2004, Chapon et al., 2006), and the ‘up-up-down-down’ spin ordering in the MnO2 planes (called E-type ordering) in the orthorhombic RMnO3 series (Lorenz et al., 2007), where R = a rare-earth metal. The E-type magnetic structure is a good example of how a single two-dimensional irreducible representation can induce ferroelectricity. There are also magnetically induced ferromagnetic ferroelectrics, where ferroelectricity arises from antiferromagnetic order, and weak ferromagnetism is present due to uniform canting of the magnetic moments. Here examples include CoCr2O4 (Yamaski et al., 2006) and Mn2GeO4 (White et al., 2012). Since 2003, a growing number of magnetically induced ferroelectrics have been discovered. Reviews of their symmetry properties have been given by Harris (2007) and Radaelli & Chapon (2007). This phenomenon has been observed for various different transition-metal ions, and for very different crystal structures. They all have in common the fact that ferroelectricity emerges with magnetic order or with a change of an already existing magnetic order. Competing magnetic interactions and low-dimensional magnetic topologies appear to be beneﬁcial for magnetically induced ferroelectricity. The size of the ferroelectric polarization is orders of magnitude smaller than observed in BiFeO3 and YMnO3.

Magnetostriction is observed experimentally as a change l of the linear dimension along a direction speciﬁed by a unit vector b ¼ ð 1 ; 2 ; 3 Þ: P

¼ l=l ¼ Sij i j ; ð1:5:9:2Þ ij

where Sij are the deformation components, which are functions of the components of the unit vector n aligned in the direction of the magnetization. Only the symmetric part of the deformation tensor Sij has been taken into account, because the antisymmetric part represents a rotation of the crystal as a whole. The magnetostriction that arises in an applied magnetic ﬁeld will be discussed in Section 1.5.9.2; Section 1.5.9.1 is devoted to the spontaneous magnetostriction. 1.5.9.1. Spontaneous magnetostriction In this section, we shall assume that the crystal under consideration undergoes a phase transition from the paramagnetic state into a magnetically ordered state. The latter is a single-domain state with the magnetization (or the antiferromagnetic vector) aligned along the vector n. As was mentioned above, to solve the problem of the spontaneous magnetostriction we have to minimize the sum of magnetoelastic and elastic energy. Like the anisotropy energy, the anisotropic part of the magnetoelastic energy can be represented as a series in the components of the unit vector n: 0 Ume ¼ Qk‘mn Sk‘ nm nn þ Qk‘mnop Sk‘ nm nn no np þ . . . ¼ Vk‘ Sk‘ :

ð1:5:9:3Þ

1.5.9. Magnetostriction The transition to an ordered magnetic state is accompanied by a spontaneous distortion of the lattice, which is denoted spontaneous magnetostriction. The lattice distortion may be speciﬁed by the deformation (strain) components Sij. The undeformed state is deﬁned as the crystal structure that would be realized if the crystal remained in the paramagnetic state at the given temperature. This means that it is necessary to separate the magnetostrictive deformation from the ordinary thermal expansion of the crystal. This can be done by measurements of the magnetostriction in external magnetic ﬁelds applied in different directions (see Section 1.5.9.2). The magnetostriction arises because the ﬁrst derivatives of the exchange and relativistic energies responsible for the magnetic order do not vanish at Sij ¼ 0. Thus these energies depend linearly on the deformations around Sij ¼ 0. That part of the magnetic energy which depends on the deformations (and consequently on the stresses) is called the magnetoelastic energy, Ume . To ﬁnd the equilibrium values of the spontaneous magnetostriction, one also has to take the elastic energy into account. The magnetoelastic energy includes both an exchange and a relativistic part. In some ferromagnets that are cubic in the paramagnetic phase, the exchange interaction does not lower the cubic symmetry. Thus the exchange part of Ume satisﬁes the relations @Ume [email protected] ¼ B00 and @Ume [email protected] ¼ 0

ði 6¼ jÞ:

ð1:5:9:1Þ

Such a form of the magnetoelastic energy gives rise to an isotropic spontaneous magnetostriction or volume change (volume striction) which does not depend on the direction of magnetization. In what follows, we shall analyse mainly the anisotropic magnetostriction. The spontaneous magnetostriction deformations are so small (about 105) for some ferro- and antiferromagnets that they cannot be observed by the usual X-ray techniques. However, in materials with ions possessing strong spin–orbit interactions (like Co2+), it may be as large as 104. The magnetostriction in rareearth metals and their compounds with iron and cobalt are especially large (up to 103).

As for every magnetically ordered crystal, this relation contains only even powers of the magnetization unit vector. The components of the tensors Q are called magnetostrictive or magnetoelastic coefﬁcients. They are proportional to even powers of the magnetization M (Qk‘mn / M 2 and Qk‘mnop / M4 ). The symmetry of the tensors Qk‘mn and Qk‘mnop is deﬁned by the crystallographic point group of the initial paramagnetic phase of the crystal. It is convenient to consider the magnetoelastic energy as part of a general expansion of the free energy of a crystal into a series with respect to the deformation (as the magnetostrictive deformations are small): 0 0 V ¼ V 0 þ Vk‘ Sk‘ þ 12Vk‘mn Sk‘ Smn þ . . . ;

ð1:5:9:4Þ

where all the expansion coefﬁcients V 0 are functions of the components of the magnetization unit vector n. The superscripts zero indicate that the expansion coefﬁcients have been calculated relative to the undistorted lattice. Such a state in which, at a given temperature, there is no magnetic interaction to distort the crystal is not realizable practically. It will be shown below that the 0 values of the coefﬁcients Vk‘ may be obtained experimentally by observing the magnetostriction in a magnetic ﬁeld (see Section 1.5.9.2). The ﬁrst term in (1.5.9.4) is the anisotropy energy at zero deformation Ua0 : 0 0 V 0 ¼ Ua0 ¼ Kij0 ni nj þ Kijk‘ ni nj nk n‘ þ Kijk‘mn ni nj nk n‘ nm nn :

ð1:5:9:5Þ This expression has to be compared with the expression for the anisotropy at zero stress introduced in Section 1.5.3.2 [see (1.5.3.5)]. It is obvious that symmetry imposes the same restrictions on the tensors K in both expressions for the anisotropy. Later, we shall discuss these two relations for the anisotropy in more detail. The second term in (1.5.9.4) is the magnetoelastic energy density, which is displayed in equation (1.5.9.3) and represents the energy of anisotropic deformation.

145

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.5.9.1. Correspondence between matrix indices , A and tensor indices of the tensors describing spontaneous magnetostriction

ij

A

k‘mn

1 2 3 4 5 6

11 22 33 23, 32 31, 13 12, 21

01 02 03 04 05 06 07

1111 2222 3333 2233, 2323, 2332, 3223, 3232, 3322 3311, 3131, 3113, 1331, 1313, 1133 1122, 1212, 1221, 2112, 2121, 2211 1123, 1132, 1213, 1231, 1312, 1321, 2113, 2131, 2311, 3112, 3121, 3211 2231, 2213, 2321, 2312, 2123, 2132, 3221, 3212, 3122, 1223, 1232, 1322 3312, 3321, 3132, 3123, 3231, 3213, 1332, 1323, 1233, 2331, 2313, 2133 2223, 2232, 2322, 3222 3331, 3313, 3133, 1333 1112, 1121, 1211, 2111 3332, 3323, 3233, 2333 1113, 1131, 1311, 3111 2221, 2212, 2122, 1222

08 09 10 11 12 13 14 15

The third term in (1.5.9.4) is quadratic in Sk‘ and can be considered as an additional contribution to the elastic energy arising from the distortion of the lattice by spontaneous magnetostriction. This term is small compared with the main part of the elastic energy, and the effect it produces is called a morphic effect and is usually neglected. The equilibrium deformation components Sij may be found by minimization of the sum of the magnetoelastic and elastic energies. The latter, Uel , is given by Uel ¼ 12 cijk‘ Sij Sk‘ ;

ð1:5:9:6Þ

matrix N , where ; ¼ 1; . . . ; 6. The correspondence between the numbers 1 to 6 and pairs ij or k‘ is given in Table 1.5.9.1. The tensors N ijk‘ and N ijk‘mn must satisfy the symmetry of the paramagnetic state of the crystal under consideration. In the case of cubic crystals with fourfold axes (paramagnetic point groups 0 0 ), the two matrices N and NA possess 43210 , 43m1 or m3m1 instead of the 36 and 90 independent components only 3 and 6, i.e. N11 , N12 , N44 and N101 , N102 , N104 , N105 , N407 , N410 , respectively. The exact form of the two matrices will be given in the following. (a) Cubic crystals. 0 If the point group of the paramagnetic crystal is 43210, 43m1 or 0 , it follows from the Neumann principle that the only m3m1 nonvanishing components of N are N11 ¼ N22 ¼ N33, N12 ¼ N23 ¼ N31 ¼ N21 ¼ N32 ¼ N13 and N44 ¼ N55 ¼ N66 . Similarly, the only nonvanishing components of NA are N101 ¼ N202 ¼ N303, N102 ¼ N203 ¼ N301 ¼ N103 ¼ N201 ¼ N302 , N104 ¼ N205 ¼ N306 , N105 ¼ N206 ¼ N304 ¼ N106 ¼ N204 ¼ N305 , N407 ¼ N508 ¼ N609 , N410 ¼ N511 ¼ N612 ¼ N413 ¼ N514 ¼ N615 . The spontaneous magnetostriction (1.5.9.11) can then be written as

0 ¼ h0 þ h1 Sðn21 21 Þ þ 2h2 Sðn1 n2 1 2 Þ þ h3 Sðn21 n22 Þ þ h4 Sðn41 21 þ 23n21 n22 Þ þ 2h5 Sðn1 n2 n23 1 2 Þ: ð1:5:9:12Þ Here an operator S() has been introduced, which denotes the sum of the three quantities obtained by cyclic permutation of the sufﬁxes in the expression within the brackets. For example, Sðn21 n2 n3 2 3 Þ ¼ n21 n2 n3 2 3 þ n22 n3 n1 3 1 þ n23 n1 n2 1 2 . The coefﬁcients hi are related in the following way to the components of the matrices N and NA and the spontaneous magnetization Ms :

where cijk‘ are the elastic stiffnesses. The minimization leads to @ðUel þ Ume Þ[email protected] ¼

cijk‘ Sk‘

þ

Vij0

¼ 0:

h0 ¼ N12 Ms2 þ N102 Ms4 ;

ð1:5:9:7Þ

h1 ¼ ðN11 N12 ÞMs2 6ðN104 N105 ÞMs4 ; h2 ¼ 2N44 Ms2 þ 4N410 Ms4 ; h3 ¼ ½23ðN101 þ 2N102 Þ þ 2ðN104 þ 2N105 ÞMs4 ;

We shall replace the elastic stiffnesses cijk‘ in this equation by the elastic compliances sijk‘, taking into account that Hooke’s law can be written in two forms (see Section 1.3.3): Tij ¼ cijk‘ Sk‘ or Sij ¼ sijk‘ Tk‘ :

ð1:5:9:8Þ

Thus the relation for the equilibrium components of the strain Sij becomes Sij

¼

0 sijk‘ Vk‘ :

h4 ¼ ½N101 N102 þ 6ðN104 N105 ÞMs4 ; h5 ¼ 4ð3N407 N410 ÞMs4 :

ð1:5:9:9Þ

Combining the relations (1.5.9.9) and (1.5.9.3), we get the following equation for the magnetostrictive strain components Sij as a function of the magnitude Ms and direction n ¼ Ms =Ms of the magnetization Ms :

(b) Hexagonal crystals. The equation for the spontaneous magnetostriction of a crystal that, in its paramagnetic state, has a point group 62210, 6mm10 , 0 6m21 or 6=mmm10 , is of the following form [if we restrict ourselves to the quadratic terms in (1.5.9.11)]:

0 ¼ h0 þ h1 n23 23 þ h2 ðn21 21 þ n22 22 Þ þ h3 ðn21 22 þ n22 21 Þ þ 2h4 n1 n2 1 2 þ 2h5 n3 3 ðn1 1 þ n2 2 Þ þ h6 23 :

Sij ¼ sijk‘ ðQk‘mn nm nn þ Qk‘mnop nm nn no np þ . . .Þ ¼

Ms2 Nijk‘ nk n‘

þ

Ms4 Nijk‘mn nk n‘ nm nn

ð1:5:9:14Þ

þ ...: ð1:5:9:10Þ

The coefﬁcients hi are related to the components N and the spontaneous magnetization as follows: h0 ¼ N13 Ms2

Let us denote the spontaneous magnetostriction by 0 (b deﬁnes the direction of the magnetostriction relative to the crystallographic axes). According to (1.5.9.2), we obtain

0 ¼ Ms2 Nijk‘ i j nk n‘ þ Ms4 Nijk‘mn i j nk n‘ nm nn :

ð1:5:9:13Þ

h1 ¼ ðN33 N31 ÞMs2 h2 ¼ ðN11 N13 ÞMs2 h3 ¼ ðN12 N13 ÞMs2

ð1:5:9:11Þ

Relation (1.5.9.11) shows that N ijk‘mn can be chosen as symmetric in its ﬁrst two indices and symmetric in its last four indices. It can therefore be represented by a 6 15 matrix NA , where ¼ 1; . . . ; 6 and A ¼ 01; . . . ; 15. Table 1.5.9.1 lists the pairs ij that correspond to and the quadruples k‘mn that correspond to A. Similarly, N ijk‘ can be chosen as symmetric in its ﬁrst two and in its last two indices. It can therefore be represented by a 6 6

h4 ¼ ðN11 N12 ÞMs2 h5 ¼ 2N44 Ms2 h6 ¼ ðN31 N13 ÞMs2

ð1:5:9:15Þ

As mentioned above, the values of the magnetostrictive coefﬁcients hi and the spontaneous magnetostriction 0 may be obtained from measurements of magnetostriction in a magnetic ﬁeld. The latter will be discussed in the next section.

146

1.5. MAGNETIC PROPERTIES Table 1.5.9.2. Magnetostriction data for ferromagnets with prototype 0 symmetry m3m1 Compound

100 106

111 106

References†

Fe Ni Fe3O4 YIG (T = 300 K) DyIG (T = 300 K) DyIG (T = 4.2 K)

20.7 45.9 20 1.4 12.5 1400

21.2 24.3 78 2.4 5.9 550

(1) (1) (2) (3) (3) (4)

† References: (1) Lee (1955); (2) Bickford et al. (1955); (3) Iida (1967); (4) Clark et al. (1966).

Fig. 1.5.9.1. Diagram explaining the occurrence of magnetostrictive strains in the demagnetized and saturated states of a cube-shaped crystal with a cubic prototype.

Notice that there is some disagreement between our results (1.5.9.12)–(1.5.9.13) and the corresponding results of Mason (1951, 1952), and similarly between (1.5.9.14)–(1.5.9.15) and the results of Mason (1954). 1.5.9.2. Magnetostriction in an external magnetic ﬁeld There are three reasons for the magnetostriction arising in a magnetic ﬁeld: (a) the transfer of the crystal into a single-domain state if the magnetic ﬁeld is directed along one of the easy axes; (b) the deﬂection of the magnetization (or antiferromagnetic vector) by the magnetic ﬁeld from the easy axis in a singledomain crystal; (c) the change of the magnetization in a sufﬁciently strong magnetic ﬁeld. Let us begin with case (a) and consider a crystal with cubic symmetry in the paramagnetic state (i.e. with a cubic prototype). We calculate the magnetostriction that occurs when the applied magnetic ﬁeld transforms the crystal from the demagnetized multidomain state into the saturated single-domain state. This transformation is shown schematically in Fig. 1.5.9.1. Each domain in the demagnetized state is distorted by spontaneous magnetostriction. The number of domains in the sample is usually much larger than shown in the ﬁgure. Thus a sample of a crystal with a cubic prototype which in the paramagnetic state has the form of a cube will retain this form in the ordered state. Its linear dimension will be changed as a result of magnetostriction. Averaging these strains over all the domains, one gets the spontaneous magnetostrictive change of the linear dimension of the sample, which is equal for any direction x, y or z: ðlÞdem =l0 ¼ dem ¼ 0 ðnk Þ;

ð1:5:9:16Þ

where nk deﬁnes the directions parallel to all the easy axes of the crystal. For crystals with a cubic prototype, there are two principal ordered states: with the easy axis along the h111i directions as in nickel or along the h100i directions as in iron. Averaging the strains of all eight possible easy-axis directions of the domains in the h111i-type ferromagnet we obtain from (1.5.9.12) the following expression for the spontaneous magnetostriction of the demagnetized crystal:

dem ¼ h0 þ 13ðh1 þ h3 þ h4 Þ:

2 2 2 2 1 1

sat

¼ h1 ½Sðn1 1 Þ 3 þ 2h2 Sðn1 n2 1 2 Þ þ h3 ½Sðn1 n2 Þ 3

þ h4 ½Sðn41 21 þ 23n21 n22 Þ 13 þ 2h5 Sðn21 n2 n3 2 3 Þ; ð1:5:9:19Þ

h100i type: 2 2 2 2 1

sat

¼ h1 ½Sðn1 1 Þ 3 þ 2h2 Sðn1 n2 1 2 Þ þ h3 Sðn1 n2 Þ

þ h4 ½Sðn41 21 þ 23n21 n22 Þ 13 þ 2h5 Sðn21 n2 n3 2 3 Þ: ð1:5:9:20Þ Both types of crystals with a cubic prototype are described by a two-constant equation if the terms of fourth power are neglected. This equation was obtained by Akulov (1928) in the form 2 2 2 2 2 2 3 1

sat

¼ 2 100 ðn1 1 þ n2 2 þ n3 3 3Þ

þ 3 111 ðn1 n2 1 2 þ n2 n3 2 3 þ n3 n1 3 1 Þ; ð1:5:9:21Þ where the constants 100 and 111 correspond to the magnetostrictive deformation of a ‘cubic’ ferromagnet along the direction of the magnetic ﬁeld that is applied along the directions h100i and h111i, respectively. Let us denote by Q1 and Q2 the following equal coefﬁcients in the equation for the magnetoelastic energy (1.5.9.3): Q1 ¼ Qxxxx ¼ Qyyyy ¼ Qzzzz ;

Q2 ¼ Qxyxy ¼ Qyzyz ¼ Qzxzx : ð1:5:9:22Þ

According to (1.5.9.9), the coefﬁcients 100 and 111 may be written as the following fractions of Qi and the elastic stiffnesses c :

100 ¼

Q1 ; c12 c11

111 ¼

1 Q2 : 3 c44

ð1:5:9:23Þ

ð1:5:9:17Þ

In the case of the h100i-type ferromagnet, the averaging over the six groups of domains leads to

dem ¼ h0 þ 13ðh1 þ h4 Þ:

tostriction (1.5.9.12) the expressions (1.5.9.17) and (1.5.9.18) for the demagnetized sample, Becker & Do¨ring (1939) obtained the equations that describe the anisotropy of the magnetostriction caused by saturation magnetization of the h111i and h100i types of magnetic crystals: h111i type:

ð1:5:9:18Þ

In the saturated state, the sample loses its cubic form. It becomes longer parallel to the magnetic ﬁeld and thinner perpendicular to it. By deﬁnition, the demagnetized state is taken as a reference state for the magnetostriction in the magnetic ﬁeld. Subtracting from the general relation for spontaneous magne-

If the magnetic ﬁeld transforms the crystal from the demagnetized to the saturated state and if the linear dimension of the sample along the magnetic ﬁeld increases, then its dimension perpendicular to the ﬁeld will decrease (see Fig. 1.5.9.1). It follows from relation (1.5.9.21) that the magnetostriction perpendicular to the magnetic ﬁeld is ? 1 1

? 100 ¼ 2 100 and 111 ¼ 2 111 :

ð1:5:9:24Þ

Some data for magnetostriction of ferromagnets with proto 0 are presented in Table 1.5.9.2. type symmetry m3m1

147

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.5.10.1. Conversion of non-rationalized (except for ) Gaussian units to SI units Symbol

Quantity

Gaussian unit and its SI equivalent

B H M g mol

Magnetic induction Magnetic ﬁeld Magnetization (= magnetic moment per unit volume) Linear magnetoelectric tensor (rationalized units) Piezomagnetic tensor Magnetic volume susceptibility Magnetic mass susceptibility Magnetic molar susceptibility

1 gauss (G) = 104 tesla (T) 1 oersted (Oe) = 103/(4) A m1 1 emu cm3 = 103 A m1 1 (dimensionless units) = 4 108/3 s m1 1 Oe1 = 4 103 m A1 = 4 103 T Pa1 1 (dimensionless units) = 4 (dimensionless units) 1 cm3 g1 = 4 103 m3 kg1 1 cm3 mol1 = 4 106 m3 mol1

In a uniaxial crystal, the magnetostriction in the magnetic ﬁeld arises mainly as a result of the rotation of the magnetization vector from the direction of the easy axis to the direction of the applied ﬁeld. The magnetostriction in the magnetic ﬁeld of an easy-axis hexagonal ferromagnet can be obtained from the relation for the spontaneous magnetostriction (1.5.9.14). In the demagnetized state, such a ferromagnet possesses only two types of antiparallel domains, in which the magnetization is aligned parallel or antiparallel to the hexagonal axis (nz ¼ 1, nx ¼ ny ¼ 0). Thus the magnetostriction of the demagnetized state is described by

dem ¼ h0 þ ðh1 þ h6 Þ 23 :

ð1:5:9:25Þ

The saturation magnetostriction can be calculated for different directions of the applied magnetic ﬁeld using the equations (1.5.9.14), (1.5.9.15) and (1.5.9.25). If the magnetic ﬁeld is applied along the x axis (nx ¼ 1, ny ¼ nz ¼ 0), the saturation magnetostrictions for three directions of the vector b: sat

¼ A ; B ; C are

1.5.9.3. The difference between the magnetic anisotropies at zero strain and zero stress The spontaneous magnetostriction makes a contribution to the magnetic anisotropy (especially in crystals with a cubic prototype). Therefore, to ﬁnd the full expression for the anisotropy energy, one has to sum up the magnetic Ua0 [see (1.5.9.5)], the magnetoelastic Ume [see (1.5.9.3)] and the elastic Uel [see (1.5.9.6)] energies. At zero strain (Sij ¼ 0), only Ua0 6¼ 0. At zero stress Ua0 þ Ume þ Uel ¼ Ua0 þ Vij0 Sij þ 12 cijk‘ Sij Sk‘ ¼ Ua0 þ 12Vij0 Sij :

ð1:5:9:29Þ

Here we used the modiﬁed equation (1.5.9.7): 1 2 cijk‘ Sij Sk‘

¼ 12Vij0 Sij :

ð1:5:9:30Þ

Substituting the values for the spontaneous magnetostriction, the ﬁnal equation for the anisotropy energy measured at atmospheric pressure may be written as Ua ¼ Ua0 þ 12Vij0 Sij 0 0 ¼ ðKij0 þ Kij0 Þni nj þ ðKijk‘ þ Kijk‘ Þni nj nk n‘

b k Ox A ¼ h2 ; b k Oy B ¼ h3 ;

0 0 þ ðKijk‘mn þ Kijk‘mn Þni nj nk n‘ nm nn þ . . . :

ð1:5:9:31Þ

C ¼ h1 :

b k Oz

ð1:5:9:26Þ

If the magnetic ﬁeld is applied at an angle of 45 to the hexagonal axis along the [101] direction, the saturation magnetostriction along the magnetic ﬁeld is described by

D ¼

sat 101

¼

1 4ðh2

h1 þ 2h5 Þ:

ð1:5:9:27Þ

Using the constants A, B , C and D introduced above, the general relation for the magnetostriction caused by magnetization to saturation can be presented in the form

þ B ½ð1 n23 Þð1 23 Þ ðn1 1 þ n2 2 Þ2

ð1:5:9:32Þ

The coefﬁcients K10 and K20 may be expressed in terms of the saturation magnetostriction constants h0 ; . . . ; h5 [see (1.5.9.12)] and the elastic stiffnesses c : K10 ¼ c11 ½h0 ð2h4 3h3 Þ þ h1 ðh1 h3 þ 3h4 Þ h4 ðh3 2h4 Þ þ c12 ½2h0 ð2h4 3h3 Þ ðh1 þ h4 Þðh1 þ 2h3 Þ 12 c44 h22 ; ð1:5:9:33Þ

12 c44 ð6h2 þ h5 Þh5 : ð1:5:9:28Þ

A typical hexagonal ferromagnet is cobalt. The magnetostriction constants introduced above have the following values for Co at room temperature:

A ¼ 45 106 ;

B ¼ 95 106 ;

Ua ¼ ðK10 þ K10 ÞSðn21 n22 Þ þ ðK20 þ K20 Þn21 n22 n23 :

K20 ¼ c11 ½3h4 ðh1 þ h3 Þ þ ðh4 h3 Þð4h4 3h3 Þ þ c12 ½3h4 ðh1 þ h3 Þ þ h3 ð5h4 6h3 Þ

2

sat

¼ A ½ðn1 1 þ n2 2 Þ ðn1 1 þ n2 2 Þn3 3

þ C ½ð1 n23 Þ 23 ðn1 1 þ n2 2 Þn3 3 þ 4 D ðn1 1 þ n2 2 Þn3 3 :

As an example, for the ferromagnets with a cubic prototype this equation may be written as

C ¼ þ110 106 ;

D ¼ 100 106 :

A more sophisticated treatment of the symmetry of the magnetostriction constants is given in the monograph of Birss (1964) and in Zalessky (1981).

ð1:5:9:34Þ

For cubic crystals, Ki0 and Ki0 are of the same magnitude. As an example, for Ni one has K10 = 80 000 erg cm3 = 8000 J m3 and K10 = 139 000 erg cm3 = 13 900 J m3. 1.5.10. Connection between Gaussian and SI units Numerical values of magnetic quantities are given in the tables and ﬁgures in this chapter in Gaussian units together with information on how the corresponding values in SI units are obtained. As a summary, Table 1.5.10.1 gives for each such quantity the corresponding Gaussian unit and its value expressed in SI units. More details on the transformation between Gaussian and SI units are given e.g. in the Appendix of Jackson (1999).

148

1.5. MAGNETIC PROPERTIES Professor Stephen Lovesey, Dr Jean-Pierre Rivera and Professor Hans Schmid for suggesting numerous improvements to the manuscript. In preparing this second edition, Hans Grimmer has also proﬁtted from useful hints from Professor Friedrich W. Hehl.

1.5.11. Glossary ij

ijk ijk n "ij

ijk i ij l B ijk‘ ðrÞ eij ij , m ij B c cijk‘ d e E g H jðrÞ J Jex k kB li Li L mðrÞ m M N p P r SðrÞ S sijk‘ Sij Tij T Tc TC TN U Ua Uel Ume v Z

(linear) magnetoelectric tensor nonlinear magnetoelectric tensor EHH nonlinear magnetoelectric tensor HEE Weiss constant magnetic birefringence permittivity constant describing magnetostriction tensor describing the piezomagnetic effect matrix describing the piezomagnetic effect permeability magnetic moment Bohr magneton piezomagnetoelectric tensor charge density thermodynamic potential dielectric susceptibility magnetic susceptibility magnetic induction speed of light elastic stiffness volume element charge of the electron electric ﬁeld Lande´ g-factor magnetic ﬁeld current density total angular momentum exchange constant position vector in reciprocal space Boltzmann factor sum of the magnetic moments in a unit cell, in which some of the moments are taken with opposite sign antiferromagnetic vector orbital angular momentum (Section 1.5.1.1), antiferromagnetic vector (remainder of this chapter) magnetic moment density sum of the magnetic moments in a unit cell magnetization (= magnetic moment per unit volume = ferromagnetic vector) No. of atoms per unit volume effective number of Bohr magnetons (Section 1.5.1), pressure (remainder of this chapter) electric polarization position vector in space spin density spin angular momentum (of an atom or ion) elastic compliance strain tensor stress tensor temperature phase transition temperature Curie temperature Ne´el temperature energy anisotropy energy elastic energy magnetoelastic energy velocity atomic number (= number of electrons per atom)

References

The authors express their gratitude to Dr Elena Zhdanova for her great support in the preparation of the ﬁgures, and to

Aizu, K. (1970). Possible species of ferromagnetic, ferroelectric and ferroelastic crystals. Phys. Rev. B, 2, 754–772. ¨ ber die Magnetostriktion der Eisenkristalle. Z. Phys. Akulov, N. (1928). U 52, 389–405. Alcantara Bonﬁm, O. F. de & Gehring, G. A. (1980). Magnetoelectric effect in antiferromagnetic crystals. Adv. Phys. 29, 731–769. Anderson, J. C., Birss, R. R. & Scott, R. A. M. (1964). Linear magnetostriction in hematite. In Proc. Int. Conf. Magnetism, Nottingham, pp. 597–599. London: Institute of Physics and the Physical Society. Andratskii, V. P. & Borovik-Romanov, A. S. (1966). Piezomagnetic effect in -Fe2O3. (In Russian.) Zh. Eksp. Teor. Fiz. 51, 1030–1036. [English translation: Sov. Phys. JETP, 24 (1967), 687–691.] Andreev, A. F. & Marchenko, V. I. (1976). Macroscopic theory of spin waves. (In Russian.) Zh. Eksp. Teor. Fiz. 70, 1522–1538. (English translation: Sov. Phys. JETP, 43, 794–803.) Andreev, A. F. & Marchenko, V. I. (1980). Symmetry and the macroscopic dynamics of magnetic materials. (In Russian.) Usp. Fiz. Nauk, 130, 39–63. (English translation: Sov. Phys. Usp. 23, 21–34.) Ascher, E. (1966). Some properties of spontaneous currents. Helv. Phys. Acta, 39, 40–48. Ascher, E. (1968). Higher-order magneto-electric effects. Philos. Mag. 17, 149–157. Ascher, E. (1970). The interactions between magnetization and polarization: phenomenological symmetry considerations on boracites. J. Phys. Soc. Jpn, 28 Suppl., 7–14. Ascher, E., Rieder, H., Schmid, H. & Sto¨ssel, H. (1966). Some properties of ferromagnetoelectric nickel–iodine boracite, Ni3B7O13I. J. Appl. Phys. 37, 1404–1405. Astrov, D. N. (1960). The magnetoelectric effect in antiferromagnetics. (In Russian.) Zh. Eksp. Teor. Fiz. 38, 984–985. (English translation: Sov. Phys. JETP, 11, 708–709.) Astrov, D. N. (1961). Magnetoelectric effect in chromium oxide. (In Russian.) Zh. Eksp. Teor. Fiz. 40, 1035–1041. (English translation: Sov. Phys. JETP, 13, 729–733.) Astrov, D. N., Al’shin, B. I., Zorin, R. V. & Drobyshev, L. A. (1968). Spontaneous magnetoelectric effect. (In Russian.) Zh. Eksp. Teor. Fiz. 55, 2122–2127. [English translation: Sov. Phys. JETP, 28 (1969), 1123– 1125.] Barbara, B., Gignoux, D. & Vettier, C. (1988). Lectures on Modern Magnetism. Beijing: Science Press. Bazhan, A. N. & Bazan, Ch. (1975). Weak ferromagnetism in CoF2 and NiF2. (In Russian.) Zh. Eksp. Teor. Fiz. 69, 1768–1781. (English translation: Sov. Phys. JETP, 42, 898–904.) Becker, R. & Do¨ring, W. (1939). Ferromagnetismus. Berlin: Springer. Belov, N. V., Belova, E. N. & Tarkhova, T. N. (1964). Polychromatic plane groups. In Shubnikov & Belov (1964). Colored Symmetry, edited by W. T. Holser, pp. 228–237. Oxford: Pergamon. Belov, N. V., Neronova, N. N. & Smirnova, T. S. (1957). Shubnikov groups. (In Russian.) Kristallograﬁya, 2, 315–325. (English translation: Sov. Phys. Crystallogr. 2, 311–322.) Bertaut, E. F. (1963). Spin conﬁgurations of ionic structures: theory and practice. In Magnetism, Vol. III, edited by G. T. Rado & H. Suhl, pp. 149–209. New York: Academic Press. Bertaut, E. F., Mercier, M. & Pauthenet, R. (1964). Ordre magne´tique et proprie´te´s magne´tiques de MnYO3. J. Phys. 25, 550–557. Bickford, L. R. Jr, Pappis, J. & Stull, J. L. (1955). Magnetostriction and permeability of magnetite and cobalt-substituted magnetite. Phys. Rev. 99, 1210–1214. Birss, R. R. (1964). Symmetry and Magnetism. Amsterdam: NorthHolland. Birss, R. R. & Anderson, J. C. (1963). Linear magnetostriction in antiferromagnetics. Proc. Phys. Soc. 81, 1139–1140. Bloembergen, N. (1962). In Proc. Int. Conf. High Magnetic Fields, edited by B. Lax, p. 454. New York: John Wiley. Borovik-Romanov, A. S. (1959a). Investigation of weak ferromagnetism in the MnCO3 single crystal. (In Russian.) Zh. Eksp. Teor. Fiz. 36, 766– 781. (English translation: Sov. Phys. JETP, 9, 539–549.)

149

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Borovik-Romanov, A. S. (1959b). Piezomagnetism in the antiferromagnetic ﬂuorides of cobalt and manganese. (In Russian.) Zh. Eksp. Teor. Fiz. 36, 1954–1955. (English translation: Sov. Phys. JETP, 9, 1390– 1391.) Borovik-Romanov, A. S. (1960). Piezomagnetism in the antiferromagnetic ﬂuorides of cobalt and manganese. (In Russian.) Zh. Eksp. Teor. Fiz. 38, 1088–1098. (English translation: Sov. Phys. JETP, 11, 786– 793.) Borovik-Romanov, A. S. & Orlova, M. P. (1956). Magnetic properties of cobalt and manganese carbonates. (In Russian.) Zh. Eksp. Teor. Fiz. 31, 579–582. [English translation: Sov. Phys. JETP, 4 (1957), 531–534.] Borovik-Romanov, A. S. & Ozhogin, V. I. (1960). Weak ferromagnetism in an antiferromagnetic CoCO3 single crystal. (In Russian.) Zh. Eksp. Teor. Fiz. 39, 27–36. (English translation: Sov. Phys. JETP, 12, 18–24.) Borovik-Romanov, A. S. & Yavelov, B. E. (1963). Linear magnetostriction in antiferromagnetic CoF2. In Proc. 3rd Regional Conf. Prague, 81–83. Brown, P. J. & Chatterji, T. (2006). Neutron diffraction and polarimetric study of the magnetic and crystal structures of HoMnO3 and YMnO3. J. Phys. Condens. Matter, 18, 10085–10096. Burzo, E. (1993). Magnetic properties of non-metallic inorganic compounds based on transition elements. Boron containing oxides. Landolt-Bo¨rnstein III 27 h, Berlin: Springer. Cardwell, M. J. (1969). Measurements of the magnetic ﬁeld dependent electric susceptibility of yttrium iron garnet. Phil. Mag. 20, 1087– 1089. Chapon, L. C., Radaelli, P. G., Blake, G. R., Park, S. & Cheong, S. W. (2006). Ferroelectricity induced by acentric spin-density waves in YMn2O5. Phys. Rev. Lett. 96, 097601. Chappert, J. (1965). Etude par effet Mo¨ssbauer de la substitution partielle par le fer du mangane`se dans les manganites de terres rares. Phys. Lett. 18, 229–230. Clark, A. E., DeSavage, B. F., Tsuya, N. & Kawakami, S. (1966). Magnetostriction of dysprosium, holmium, and erbium iron garnets. J. Appl. Phys. 37, 1324–1326. Cox, D. E. (1974). Spin ordering in magnetoelectrics. Int. J. Magn. 6, 67– 75. [Reprinted in Freeman & Schmid (1975), pp. 111–119.] Cox, D. E., Frazer, B. C., Newnham, R. E. & Santoro, R. P. (1969). Neutron diffraction investigation of the spiral magnetic structure in Cr2BeO4. J. Appl. Phys. 40, 1124–1125. Cracknell, A. P. (1975). Magnetism in Crystalline Materials. Oxford: Pergamon. Curie, P. (1894). Sur la syme´trie dans les phe´nome`nes physiques, syme´trie d’un champ e´lectrique et d’un champ magne´tique. J. Phys., 3rd series III, 393–415. Dzyaloshinskii, I. E. (1957a). Thermodynamic theory of ‘weak’ ferromagnetism in antiferromagnetic substances. (In Russian.) Zh. Eksp. Teor. Fiz. 32, 1547–1562. (English translation: Sov. Phys. JETP, 5, 1259–1272.) Dzyaloshinskii, I. E. (1957b). The problem of piezomagnetism. (In Russian.) Zh. Eksp. Teor. Fiz. 33, 807–808. [English translation: Sov. Phys. JETP, 6 (1958), 621–622.] Dzyaloshinskii, I. E. (1957c). The magnetic structure of ﬂuorides of the transition metals. (In Russian.) Zh. Eksp. Teor. Fiz. 33, 1454–1456. [English translation: Sov. Phys. JETP, 6 (1958), 1120–1122.] Dzyaloshinskii, I. E. (1959). On the magneto-electrical effect in antiferromagnets. (In Russian.) Zh. Eksp. Teor. Fiz. 37, 881–882. [English translation: Sov. Phys. JETP, 10 (1960), 628–629.] Dzyaloshinskii, I. E. (1964). Theory of helicoidal structures in antiferromagnets. (In Russian.) Zh. Eksp. Teor. Fiz. 46, 1420–1437, 47, 336–348 and 992–1002. [English translation: Sov. Phys. JETP, 19, 960–971, 20 (1965), 223–231 and 665–671.] Dzyaloshinskii, I. E. & Man’ko, V. I. (1964). Nonlinear effects in antiferromagnets. ‘Latent’ antiferromagnetism. (In Russian.) Zh. Eksp. Teor. Fiz. 46, 1352–1359. (English translation: Sov. Phys. JETP, 19, 915–919.) Eremenko, V. V., Kharchenko, N. F., Litvinenko, Yu. G. & Naumenko, V. M. (1989). Magneto-optics and spectroscopy of antiferromagnets. (In Russian.) Kiev: Naukova Dumka. [English translation (1992): New York: Springer.] Faber, J., Lander, G. H. & Cooper, B. R. (1975). Neutron-diffraction study of UO2: observation of an internal distortion. Phys. Rev. Lett. 35, 1770– 1773. Ferre´, J. & Gehring, G. A. (1984). Linear optical birefringence of magnetic crystals. Rep. Prog. Phys. 47, 513–611.

Fiebig, M. (2005). Revival of the magnetoelectric effect. J. Phys. D Appl. Phys. 38, R123–R152. Fiebig, M. & Spaldin, N. A. (2009). Topical issue on Magnetic Interaction Phenomena in Crystals. Eur. Phys. J. B, 71, Issue 3, 293–427. Folen, V. J., Rado, G. T. & Stalder, E. W. (1961). Anisotropy of the magnetoelectric effect in Cr2O3. Phys. Rev. Lett. 6, 607–608. Foner, S. (1963). Antiferromagnetic and ferrimagnetic resonance. In Magnetism, Vol. I, edited by G. T. Rado & H. Suhl, pp. 383–447. New York: Academic Press. Freeman, A. J. & Schmid, H. (1975). Magnetoelectric Interaction Phenomena in Crystals. London: Gordon and Breach. Gallego, S. V., Tasci, E. S., de la Flor, G., Perez-Mato, J. M. & Aroyo, M. I. (2012). Magnetic symmetry in the Bilbao Crystallographic Server: a computer program to provide systematic absences of magnetic neutron diffraction. J. Appl. Cryst. 45, 1236–1247. Gijsman, H. M., Poulis, N. J. & Van den Handel, J. (1959). Magnetic susceptibilities and phase transitions of two antiferromagnetic manganese salts. Physica, 25, 954–968. Gorbatsevich, A. A. & Kopaev, Yu. V. (1994). Toroidal order in crystals. Ferroelectrics, 161, 321–334. Grimmer, H. (1991). General connections for the form of the property tensors in the 122 Shubnikov point groups. Acta Cryst. A47, 226– 232. Grimmer, H. (1992). The piezomagnetoelectric effect. Acta Cryst. A48, 266–271. Harris, A. B. (2007). Landau analysis of the symmetry of the magnetic structure and magnetoelectric interaction in multiferroics. Phys. Rev. B, 76, 054447. ¨ ber die vierdimensionalen Gruppen des dreidimenHeesch, H. (1930). U sionalen Raumes. Z. Kristallogr. 73, 325–345. Hehl, F. W., Obukhov, Y. N., Rivera, J.-P. & Schmid, H. (2009). Magnetoelectric Cr2O3 and relativity theory. Eur. Phys. J. B, 71, 321– 329. Hou, S. L. & Bloembergen, N. (1965). Paramagnetoelectric effects in NiSO46H2O. Phys. Rev. A, 138, 1218–1226. Hur, N., Park, S., Sharma, P. A., Ahn, J. S., Guha, S. & Cheong, S. W. (2004). Electric polarization reversal and memory in a multiferroic material induced by magnetic ﬁelds. Nature (London), 429, 392–395. Iida, S. (1967). Magnetostriction constants of rare earth iron garnets. J. Phys. Soc. Jpn, 22, 1201–1209. Indenbom, V. L. (1959). Relation of the antisymmetry and color symmetry groups to one-dimensional representations of the ordinary symmetry groups. Isomorphism of the Shubnikov and space groups. (In Russian.) Kristallograﬁya, 4, 619–621. [English translation: Sov. Phys. Crystallogr. 4 (1960), 578–580.] International Tables for Crystallography (2005). Vol. A. Space-Group Symmetry, edited by Th. Hahn. Heidelberg: Springer. Izyumov, Yu. A. & Naish, V. E. (1979). Symmetry analysis in neutron diffraction studies of magnetic structures. J. Magn. Magn. Mater. 12, 239–248. Izyumov, Yu. A., Naish, V. E. & Petrov, S. B. (1979). Symmetry analysis in neutron diffraction studies of magnetic structures. J. Magn. Magn. Mater. 13, 267–274, 275–282. Izyumov, Yu. A., Naish, V. E. & Syromiatnikov, V. N. (1979). Symmetry analysis in neutron diffraction studies of magnetic structures. J. Magn. Magn. Mater. 12, 249–261. Jackson, J. D. (1999). Classical Electrodynamics, 3rd ed. New York: Wiley. Joshua, S. J. (1991). Symmetry Principles and Magnetic Symmetry in Solid State Physics. Graduate Student Series in Physics. Bristol: Hilger. Kadomtseva, A. M., Agafonov, A. P., Lukina, M. M., Milov, V. N., Moskvin, A. S. & Semenov, V. A. (1981). Characteristic magnetoelastic properties of yttrium orthochromite. (In Russian.) Fiz. Tverd. Tela, 23, 3554–3557. (English translation: Sov. Phys. Solid State, 23, 2065–2067.) Kadomtseva, A. M., Agafonov, A. P., Milov, V. N., Moskvin, A. S. & Semenov, V. A. (1981). Direct observation of symmetry change induced in orthoferrite crystals by an external magnetic ﬁeld. (In Russian.) Pis’ma Zh. Eksp. Teor. Fiz. 33, 400–403. (English translation: JETP Lett. 33, 383–386.) Kenzelmann, M., Harris, A. B., Jonas, S., Broholm, C., Schefer, J., Kim, S. B., Zhang, C. L., Cheong, S. W., Vajk, O. P. & Lynn, J. W. (2005). Magnetic inversion symmetry breaking and ferroelectricity in TbMnO3. Phys. Rev. Lett. 95, 087206. Kharchenko, N. F., Eremenko, V. V. & Belyi, L. I. (1979). Visual observation of 180-degree antiferromagnetic domains. (In Russian.)

150

1.5. MAGNETIC PROPERTIES Pis’ma Zh. Eksp. Teor. Fiz. 29, 432–435. (English translation: JETP Lett. 29, 392–395.) Kharchenko, N. F. & Gnatchenko, S. L. (1981). Linear magnetooptic effect and visual observation of antiferromagnetic domains in an orthorhombic crystal of DyFeO3. (In Russian.) Fiz. Nizk. Temp. 7, 475–493. (English translation: Sov. J. Low Temp. Phys. 7, 234–243.) Khomskii, D. (2009). Classifying multiferroics: Mechanisms and effects. Physics, 2, 20. Kimura, T., Goto, T., Shintani, H., Ishizaka, K., Arima, T. & Tokura, Y. (2003). Magnetic control of ferroelectric polarization. Nature (London), 426, 55–58. Kiselev, S. V., Ozerov, R. P. & Zhdanov, G. S. (1962). Detection of magnetic order in ferroelectric BiFeO3 by neutron diffraction. (In Russian.) Dokl. Akad. Nauk SSSR, 145, 1255–1258. [English translation: Sov. Phys. Dokl. 7 (1963), 742–744.] Kopsky´, V. (1979a). Tensorial covariants for the 32 crystal point groups. Acta Cryst. A35, 83–95. Kopsky´, V. (1979b). A simpliﬁed calculation and tabulation of tensorial covariants for magnetic point groups belonging to the same Laue class. Acta Cryst. A35, 95–101. Koptsik, V. A. (1966). Shubnikov Groups. (In Russian.) Moscow: Izd. MGU. Koptsik, J. N. & Kuzhukeev, Zh.-N. M. (1972). Derivation of the three-, four- and six-color Belov space groups from tables of irreducible representations. (In Russian.) Kristallograﬁya, 17, 705–711. [English translation: Sov. Phys. Crystallogr. 17 (1973), 622–627.] Kouvel, J. S. & Fisher, M. E. (1964). Detailed magnetic behavior of nickel near its Curie point. Phys. Rev. A, 136, 1626–1632. Kovalev, O. V. (1987). Representations of the Crystallographic Space Groups, 2nd ed. (In Russian.) Moscow: Nauka. [English translation (1993): New York: Gordon and Breach.] Landau, L. D. (1933). Eine mo¨gliche Erkla¨rung der Feldabha¨ngigkeit der Suszeptibilita¨t bei niedrigen Temperaturen. Phys. Z. Sowjet. 4, 675–679. Landau, L. D. (1937). Zur Theorie der Phasenumwandlungen. I. Phys. Z. Sowjet. 11, 26–47. Landau, L. D. & Lifshitz, E. M. (1951). Statistical Physics. (In Russian.) Moscow: Gostekhizdat. [English translation (1958): London: Pergamon.] Landau, L. D. & Lifshitz, E. M. (1957). Electrodynamics of Continuous Media. (In Russian.) Moscow: Gostekhizdat. [English translation (1960): London: Pergamon.] Le Gall, H., Leycuras, C., Minella, D., Rudashevskii, E. G. & Merkulov, V. S. (1977). Anomalous evolution of the magnetic and magnetooptical properties of hematite at temperature near and lower than the Morin phase transition. Physica B, 86–88, 1223–1225. Lebeugle, D., Colson, D., Forget, A., Viret, M., Bataille, A. M. & Gukasov, A. (2008). Electric-ﬁeld-induced spin ﬂop in BiFeO3 single crystals at room temperature. Phys. Rev. Lett. 100, 227602. Lee, E. W. (1955). Magnetostriction and magnetomechanical effects. Rep. Prog. Phys. 18, 184–229. Lee, G., Mercier, M. & Bauer, P. (1970). Mesures magne´toe´lectriques sur les grenats de Y, de Gd et de Dy aux basses tempe´ratures. In Les e´le´ments des terres rares, Vol. II, pp. 389–399. Paris: Editions du CNRS. Levitin, R. Z. & Shchurov, V. A. (1973). In Physics and Chemistry of Ferrites, pp. 162–194. (In Russian.) Moscow: Izd. Mosk. Gos. Univ. Lifshitz, E. M. (1942). On the theory of phase transitions of the second order. J. Phys. (Moscow), 6, 61–74. Litvin, D. B. (2009). Tensor distinction of domains in ferroic crystals. Eur. Phys. J. B, 71, 315–320. Lorenz, B., Wang, Y. Q. & Chu, C. W. (2007). Ferroelectricity in perovskite HoMnO3 and YMnO3. Phys. Rev. B, 76, 104405. Lyubimov, V. N. (1965). The interaction of polarization and magnetization in crystals. (In Russian.) Kristallograﬁya, 10, 520–524. [English translation: Sov. Phys. Crystallogr. 10 (1966), 433–436.] Mason, W. P. (1951). A phenomenological derivation of the ﬁrst- and second-order magnetostriction and morphic effects for a nickel crystal. Phys. Rev. 82, 715–723. Mason, W. P. (1952). A phenomenological derivation of the ﬁrst- and second-order magnetostriction and morphic effects for a nickel crystal. Erratum. Phys. Rev. 85, 1065. Mason, W. P. (1954). Derivation of magnetostriction and anisotropic energies for hexagonal, tetragonal, and orthorhombic crystals. Phys. Rev. 96, 302–310. Matarrese, L. M. & Stout, J. W. (1954). Magnetic anisotropy of NiF2. Phys. Rev. 94, 1792–1793.

Mercier, R. (1974). Magnetoelectric behaviour in garnets. Int. J. Magn. 6, 77–88. [Reprinted in Freeman & Schmid (1975), pp. 99–110.] Merkulov, V. S., Rudashevskii, E. G., Le Gall, H. & Leycuras, C. (1981). Linear magnetic birefringence of hematite in the vicinity of the Morin temperature. (In Russian.) Zh. Eksp. Teor. Fiz. 80, 161–170. (English translation: Sov. Phys. JETP, 53, 81–85.) Michel, Ch., Moreau, J.-M., Achenbach, G. D., Gerson, R. & James, W. J. (1969). The atomic structure of BiFeO3. Solid State Commun. 7, 701– 704. Morin, F. J. (1950). Magnetic susceptibility of -Fe2O3 and -Fe2O3 with added titanium. Phys. Rev. 78, 819–820. Moriya, T. (1960a). Theory of magnetism of NiF2. Phys. Rev. 117, 635– 647. Moriya, T. (1960b). Anisotropic superexchange interaction and weak ferromagnetism. Phys. Rev. 120, 91–98. Moriya, T. (1963). Weak ferromagnetism. In Magnetism, Vol. I, edited by G. T. Rado & H. Suhl, pp. 85–125. New York: Academic Press. Ne´el, L. & Pauthenet, R. (1952). E´tude thermomagne´tique d’un monocristal de Fe2O3. C. R. Acad. Sci. 234, 2172–2174. Neronova, N. N. & Belov, N. V. (1959). Ferromagnetic and ferroelectric space groups. (In Russian.) Kristallograﬁya, 4, 807–812. (English translation: Sov. Phys. Crystallogr. 4, 769–774.) Newnham, R. E. (1974). Domains in minerals. Am. Mineral. 59, 906–918. Newnham, R. E. & Cross, L. E. (1976). Secondary ferroics and domaindivided piezoelectrics. Ferroelectrics, 10, 269–276. Newnham, R. E., Kramer, J. J., Schulze, W. A. & Cross, L. E. (1978). Magnetoferroelectricity in Cr2BeO4. J. Appl. Phys. 49, 6088–6091. O’Dell, T. H. (1967). An induced magneto-electric effect in yttrium iron garnet. Philos. Mag. 16, 487–494. O’Dell, T. H. (1970). The electrodynamics of magneto-electric media. Amsterdam: North-Holland. Opechowski, W. & Guccione, R. (1965). Magnetic symmetry. In Magnetism, Vol. IIA, edited by G. T. Rado & H. Suhl, pp. 105–165. New York: Academic Press. Popov, Yu. F., Kazei, Z. A. & Kadomtseva, A. M. (1992). Linear magnetoelectric effect in Cr2O3 in strong magnetic ﬁelds. (In Russian.) Pis’ma Zh. Eksp. Teor. Fiz. 55, 238–241. (English translation: JETP Lett. 55, 234–238.) Prokhorov, A. S. & Rudashevskii, E. G. (1969). Magnetostriction of antiferromagnetic cobalt ﬂuoride. (In Russian.) Pis’ma Zh. Eksp. Teor. Fiz. 10, 175–179. (English translation: JETP Lett. 10, 110–113.) Prokhorov, A. S. & Rudashevskii, E. G. (1975). Magnetoelastic interactions and the single-domain antiferromagnetic state in cobalt ﬂuoride. (In Russian.) Kratk. Soobshch. Fiz. 11, 3–6. (English translation: Sov. Phys. Lebedev Inst. Rep. 11, 1–4.) Radaelli, P. G. & Chapon, L. C. (2007). Symmetry constraints on the electrical polarization in multiferroic materials. Phys. Rev. B, 76, 054428. Rado, G. T. (1961). Mechanism of the magnetoelectric effect in an antiferromagnet. Phys. Rev. Lett. 6, 609–610. Rado, G. T. (1962). Statistical theory of magnetoelectric effects in antiferromagnets. Phys. Rev. 128, 2546–2556. Rado, G. T. (1964). Observation and possible mechanisms of magnetoelectric effects in a ferromagnet. Phys. Rev. Lett. 13, 335–337. Rado, G. T. (1969). Magnetoelectric evidence for the attainability of timereversed antiferromagnetic conﬁgurations by metamagnetic transitions in DyPO4. Phys. Rev. Lett. 23, 644–647, 946. Rado, G. T. & Ferrari, J. M. (1973). Magnetoelectric effects in TbPO4. AIP Conf. Proc. 10, 1417. Rado, G. T., Ferrari, J. M. & Maisch, W. G. (1984). Magnetoelectric susceptibility and magnetic symmetry of magnetoelectrically annealed TbPO4. Phys. Rev. B, 29, 4041–4048. Rado, G. T. & Folen, V. J. (1961). Observation of the magnetically induced magnetoelectric effect and evidence for antiferromagnetic domains. Phys. Rev. Lett. 7, 310–311. Rado, G. T. & Folen, V. J. (1962). Magnetoelectric effects in antiferromagnetics. J. Appl. Phys. 33 Suppl., 1126–1132. Rivera, J.-P. (1994). On deﬁnitions, units, measurements, tensor forms of the linear magnetoelectric effect and on a new dynamic method applied to Cr–Cl boracite. Ferroelectrics, 161, 165–180. Rivera, J.-P. (2009). A short review of the magnetoelectric effect and related experimental techniques on single phase (multi-) ferroics. Eur. Phys. J. B, 71, 299–313. Rivera, J.-P. & Schmid, H. (1994). Search for the piezomagnetoelectric effect in LiCoPO4. Ferroelectrics, 161, 91–97.

151

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Schlenker, M. & Baruchel, J. (1978). Neutron techniques for the observation of ferro- and antiferromagnetic domains. J. Appl. Phys. 49, 1996–2001. Schmid, H. (1965). Die Synthese von Boraziten mit Hilfe chemischer Transportreaktionen. J. Phys. Chem. Solids, 26, 973–988. Schmid, H. (1967). Twinning and sector growth in nickel boracites grown by transport reactions. (In Russian.) Rost Krist. 7, 32–65. (English translation: Growth Cryst. USSR, 7, 25–52.) Schmid, H. (1973). On a magnetoelectric classiﬁcation of materials. Int. J. Magn. 4, 337–361. [Reprinted in Freeman & Schmid (1975) pp. 121– 146.] Schmid, H. (1994a). Introduction to the proceedings of the 2nd international conference on magnetoelectric interaction phenomena in crystals, MEIPIC-2. Ferroelectrics, 161, 1–28. Schmid, H. (1994b). Multi-ferroic magnetoelectrics. Ferroelectrics, 162, 317–338. Schmid, H. (2008). Some symmetry aspects of ferroics and single phase multiferroics. J. Phys. Condens. Matter, 20, 434201. Schwarzenberger, R. L. E. (1984). Colour symmetry. Bull. London Math. Soc. 16, 209–240. Scott, R. A. M. & Anderson, J. C. (1966). Indirect observation of antiferromagnetic domains by linear magnetostriction. J. Appl. Phys. 37, 234–237. Shubnikov, A. V. (1951). Symmetry and antisymmetry of ﬁnite ﬁgures. (In Russian.) Moscow: Acad. Sci. USSR. [English translation in Shubnikov & Belov (1964) pp. 3–172 and 249–252.] Shubnikov, A. V. & Belov, N. V. (1964). Colored Symmetry, edited by W. T. Holser. Oxford: Pergamon. Shubnikov, A. V. & Koptsik, V. A. (1972). Symmetry in Science and Art. (In Russian.) Moscow: Nauka. [English translation (1974): New York: Plenum.] Shuvalov, L. A. & Belov, N. V. (1962). The symmetry of crystals in which ferromagnetic and ferroelectric properties appear simultaneously. (In Russian.) Kristallograﬁya, 7, 192–194. (English translation: Sov. Phys. Crystallogr. 7, 150–151.) Sirotin, Y. I. & Shaskol’skaya, M. P. (1979). Fundamentals of Crystal Physics. (In Russian.) Moscow: Nauka. [English translation (1982): Moscow: Mir.] Smolenskii, G. A., Agranovskaia, A. I., Popov, S. N. & Isupov, V. A. (1958). New ferroelectrics of complex composition. (In Russian.) Zh. Tekh. Fiz. 28, 2152–2153. (English translation: Sov. Phys. Tech. Phys. 3, 1981–1982.) Smolenskii, G. A., Yudin, V. M., Sher, E. S. & Stolypin, Yu. E. (1962). Antiferromagnetic properties of some perovskites. (In Russian.) Zh. Eksp. Teor. Fiz. 43, 877–880. [English translation: Sov. Phys. JETP, 16 (1963), 622–624.] Sosnovska, I., Peterlin-Neumaier, T. & Steichele, E. (1982). Spiral magnetic ordering in bismuth ferrite. J. Phys. C, 15, 4835–4846.

Spaldin, N. A., Fiebig, M. & Mostovoy, M. (2008). The toroidal moment in condensed-matter physics and its relation to the magnetoelectric effect. J. Phys. Condens. Matter, 20, 434203. Tavger, B. A. (1958). The symmetry of ferromagnetics and antiferromagnetics. (In Russian.) Kristallograﬁya, 3, 339–341. (English translation: Sov. Phys. Crystallogr. 3, 341–343.) Tavger, B. A. & Zaitsev, V. M. (1956). Magnetic symmetry of crystals. (In Russian.) Zh. Eksp. Teor. Fiz. 30, 564–568. (English translation: Sov. Phys. JETP, 3, 430–436.) Townsend Smith, T. (1916). The magnetic properties of hematite. Phys. Rev. 8, 721–737. Turov, E. A. (1963). Physical Properties of Magnetically Ordered Crystals. (In Russian.) Moscow: Akad. Nauk SSSR. [English translation (1965): New York: Academic Press.] Van Aken, B. B., Rivera, J. P., Schmid, H. & Fiebig, M. (2007). Observation of ferrotoroidic domains. Nature (London), 449, 702– 705. Venevtsev, Yu. N., Gagulin, V. V. & Zhitomirsky, I. D. (1987). Material science aspects of seignette-magnetism problem. Ferroelectrics, 73, 221– 248. Voigt, W. (1928). Lehrbuch der Kristallphysik. Leipzig: Teubner. Waerden, B. L. van der & Burckhardt, J. J. (1961). Farbgruppen. Z. Kristallogr. 115, 231–234. White, J. S., Honda, T., Kimura, K., Kimura, T., Niedermayer, C., Zaharko, O., Poole, A., Roessli, B. & Kenzelmann, M. (2012). Coupling of magnetic and ferroelectric hysteresis by a multicomponent magnetic structure in Mn2GeO4. Phys. Rev. Lett. 108, 077204. White, R. L. (1974). Microscopic origins of piezomagnetism and magnetoelectricity. Int. J. Magn. 6, 243–245. [Reprinted in Freeman & Schmid (1975), pp. 41–43.] Wijn, H. P. J. (1994). Magnetic properties of non-metallic inorganic compounds based on transition elements. Perovskites. II. Oxides with corundum, ilmenite and amorphous structures. Landolt-Bo¨rnstein III, 27, f3, Berlin: Springer. Yamasaki, Y., Miyasaka, S., Kaneko, Y., He, J. P., Arima, T. & Tokura, Y. (2006). Magnetic reversal of ferroelectric polarization in a multiferroic spinel oxide. Phys. Rev. Lett. 96, 207204. Zalessky, A. V. (1981). Magnetic properties of crystals. In Modern Crystallography, Vol. IV, edited by L. A. Shuvalov. (In Russian.) Moscow: Nauka. [English translation (1988): Berlin: Springer.] Zamorzaev, A. M. (1957). Generalization of Fedorov groups. (In Russian.) Kristallograﬁya, 2, 15–20. (English translation: Sov. Phys. Crystallogr. 2, 10–15.) Zvezdin, A. K., Zorin, I. A., Kadomtseva, A. M., Krynetskii, I. B., Moskvin, A. S. & Mukhin, A. A. (1985). Linear magnetostriction and antiferromagnetic domain structure in dysprosium orthoferrite. (In Russian.) Zh. Eksp. Teor. Fiz. 88, 1098–1102. (English translation: Sov. Phys. JETP, 61, 645–647.)

152

references

International Tables for Crystallography (2013). Vol. D, Chapter 1.6, pp. 153–180.

1.6. Classical linear crystal optics By A. M. Glazer and K. G. Cox†

1.6.1. Introduction The ﬁeld of classical crystal optics is an old one, and in the last century, in particular, it was the main subject of interest in the study of crystallography. Since the advent of X-ray diffraction, however, crystal optics tended to fall out of widespread use, except perhaps in mineralogy, where it has persisted as an important technique for the classiﬁcation and identiﬁcation of mineral specimens. In more recent times, however, with the growth in optical communications technologies, there has been a revival of interest in the optical properties of crystals, both linear and nonlinear. There are many good books dealing with classical crystal optics, which the reader is urged to consult (Hartshorne & Stuart, 1970; Wahlstrom, 1959; Bloss, 1961). In addition, large collections of optical data on crystals exist (Groth, 1906–1919; Winchell, 1931, 1939, 1951, 1954, 1965; Kerr, 1959). In this chapter, both linear and nonlinear optical effects will be introduced brieﬂy in a generalized way. Then the classical derivation of the refractive index surface for a crystal will be derived. This leads on to a discussion on the practical means by which conventional crystal optics can be used in the study of crystalline materials, particularly in connection with mineralogical study, although the techniques described apply equally well to other types of crystals. Finally, some detailed explanations of certain linear optical tensors will be given.

1.6.2. Generalized optical, electro-optic and magneto-optic effects When light of a particular cyclic frequency ! is incident on a crystal of the appropriate symmetry, in general an electrical polarization P may be generated within the crystal. This can be expressed in terms of a power series with respect to the electric vector of the light wave (Nussbaum & Phillips, 1976; Butcher & Cotter, 1990; Kaminow, 1974): P P ¼ "o ðiÞ Ei ¼ "o ð1Þ E þ ð2Þ E2 þ ð3Þ E3 þ . . . ; ð1:6:2:1Þ

Here, the superscripts refer to the frequencies of the relevant ﬁeld terms and the susceptibilities are expressed as tensor components. Each term in this expansion gives rise to a speciﬁc effect that may or may not be observed, depending on the crystal symmetry and the size of the susceptibility coefﬁcients. Note a possible confusion: in the notation ðiÞ , i is equal to one less than its rank. It is important to understand that these terms describe various properties, both linear and nonlinear. Those terms that describe the effect purely of optical frequencies propagating through the crystal give rise to linear and nonlinear optics. In the former case, the input and output frequencies are the same, whereas in the latter case, the output frequency results from sums or differences of the input frequencies. Furthermore, it is apparent that nonlinear optics depends on the intensity of the input ﬁeld, and so is an effect that is induced by the strong optical ﬁeld. If the input electrical ﬁelds are static (the term ‘static’ is used here to mean zero or low frequency compared with that of light), the resulting effects are either linear or nonlinear electrical effects, in which case they are of no interest here. There is, however, an important class of effects in which both static and optical ﬁelds are involved: linear and nonlinear electro-optic effects. Here, the use of the terms linear and nonlinear is open to confusion, depending on whether it is the electrical part or the optical part to which reference is made (see for example below in the discussion of the linear electro-optic effect). Similar considerations apply to applied magnetic ﬁelds to give linear and nonlinear magneto-optic effects and to applied stresses, the photoelastic effects. Table 1.6.2.1 lists the most important effects according to the terms in this series. The susceptibilities are written in the form ð!1 ; !2 ; !3 ; . . .Þ to indicate the frequency !1 of the output electric ﬁeld, followed after the semicolon by the input frequencies !1 ; !2 ; . . ..

where the ðiÞ are susceptibilities of order i. Those working in the ﬁeld of electro-optics tend to use this notation as a matter of course. The susceptibility ð1Þ is a linear term, whereas the higherorder susceptibilities describe nonlinear behaviour. However, it is convenient to generalize this concept to take into account other ﬁelds (e.g. electrical, magnetic and stress ﬁelds) that can be imposed on the crystal, not necessarily due to the incident light. The resulting polarization can be considered to arise from many different so-called electro-optic, magneto-optic and photoelastic (elasto-optic) effects, expressed as a series expansion of Pi in terms of susceptibilities ijk‘... and the applied ﬁelds E, B and T. This can be written in the following way:

Table 1.6.2.1. Summary of linear and nonlinear optical properties Type of polarization term

Susceptibility

Effect

P0i "o ij E!j

ð0; 0Þ ð!; !Þ

"o ij‘ r‘ E!j "o ijk E!j 1 E!k 2

ð!; !Þ ð0; 0; 0Þ ð!; !; 0Þ

Spontaneous polarization Dielectric polarization, refractive index, linear birefringence Optical rotation (gyration) Quadratic electric effect Linear electro-optic effect or Pockels effect Sum/difference frequency generation, two-wave mixing Second harmonic generation (SHG) Optical rectiﬁcation Parametric ampliﬁcation

ð!1 !2 ; !1 ; !2 Þ ð!; !=2; !=2Þ ð0; !=2; !=2Þ ð!3 ; !1 ; !2 Þ "o ijk‘ E!j 1 E!k 2 E!‘ 3

ð!; !=2; !=2; 0Þ

Pi ¼ P0i þ "o ij E!j þ "o ij‘ r‘ E!j þ "o ijk E!j 1 E!k 2 !

!

!

!

ð!; 0; 0Þ

!

þ "o ijk‘ Ej 1 Ek 2 E‘ 3 þ "o ijk Ej 1 Bk 2

ð!1 ; !2 ; !3 ; !4 Þ

!2 þ "o ijk‘ E!j 1 B!k 2 B!‘ 3 þ "o ijk‘ E!j 1 Tk‘ þ ...:

ð1:6:2:2Þ † The sudden death of Keith Cox is deeply regretted. He died in a sailing accident on 27 August 1998 in Scotland at the age of 65.

Copyright © 2013 International Union of Crystallography

153

"o ijk E!j 1 B!k 2 "o ijk‘ E!j 1 B!k 2 B!‘ 3

ð!; !; 0Þ ð!; !; 0; 0Þ

!2 "o ijk‘ E!j 1 Tk‘

ð!; !; 0Þ ð!1 !2 ; !1 ; !2 Þ

Quadratic electro-optic effect or Kerr effect Electric-ﬁeld induced second harmonic generation (EFISH) Four-wave mixing Faraday rotation Quadratic magneto-optic effect or Cotton–Mouton effect Linear elasto-optic effect or photoelastic effect Linear acousto-optic effect

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES 1.6.2.1. Spontaneous polarization P0i A spontaneous polarization of a crystal can be created in some polar crystals after a strong static electric ﬁeld is ﬁrst applied and then removed. Subsequent application of an electric ﬁeld in the opposite direction can then reverse the sense of the spontaneous polarization. By analogy with the well known similar phenomenon of ferromagnetism, such crystals are known as ferroelectrics (Jona & Shirane, 1962; Lines & Glass, 1979). This effect is therefore not an optical effect, but is included here for the sake of completeness. For a crystal to be a ferroelectric, it cannot have a centre of symmetry. 1.6.2.2. Dielectric polarization "o ij E!j Application of an electric ﬁeld E of frequency ! to a crystal results in a polarization response whose size depends on the dielectric susceptibility ð1Þ. This is a second-rank tensor that is applicable to all materials, and is often quoted in terms of the dielectric constant " ¼ "o ð1 þ Þ. For electric ﬁelds at optical frequencies, the dielectric constant is equal to the square of the refractive index for light propagating in a certain direction and in a particular polarization state. This effect can only be termed optical if the frequency of the electric ﬁeld lies at optical frequencies. There is no difference between input and output frequencies, and so the susceptibility is written in the form ij ð!; !Þ. Because there is no change in frequency, this is a linear optical effect. 1.6.2.3. Optical rotation (gyration) "o ij‘ r‘ E!j This is the phenomenon often known as optical activity (Born & Wolf, 1993; Agranovich & Ginzburg, 1984) in which planepolarized light of frequency ! passing through a medium has its polarization rotated through an angle depending on the path length through the medium. It is seen most easily along uniaxial directions in crystals with the appropriate symmetry. Centrosymmetric crystals cannot show optical rotation. Because no change in frequency occurs, it can be considered to be a linear optical effect. !

!

1.6.2.4. Quadratic electric effect "o ijk Ej 1 Ek 2 If !1 ¼ !2 ¼ 0, i.e. the susceptibility is ijk ð0; 0; 0Þ, the resulting polarization is given by P0i ¼ "o ijk E0j E0k : This is therefore a polarization induced in the crystal by a strong static electric ﬁeld. It is a nonlinear electrical effect, and so it is not an optical property. 1.6.2.5. Linear electro-optic effect "o ijk E!j 1 E!k 2 If !1 ¼ ! and !2 ¼ 0, i.e. ijk ð!; !; 0Þ, this contribution becomes P!i ¼ "o ijk E!j E0k

1.6.2.6. Sum/difference frequency generation (two-wave mixing) ! ! "o ijk Ej 1 Ek 2 It can happen that when two different light ﬁelds of frequencies !1 and !1 , such as can be obtained from two lasers, propagate through a crystal, the resulting output frequency can be the sum or difference of the two incident frequencies, through the susceptibility ijk ð!1 !2 ; !1 ; !2 Þ. A particular case is of interest: suppose !1 ¼ !2 ¼ !=2 i.e. ijk ð!; !=2; !=2Þ, to get !=2 P!i ¼ "o ijk E!=2 j Ek :

Here, the light, on passing through the crystal, interacts with itself to produce a doubling of the frequency. This important effect is known as second harmonic generation or SHG and is used for generating different laser frequencies starting from a fundamental frequency. The observation of SHG is also often a good indicator of the lack of a centre of inversion in a crystal. As two optical ﬁelds are involved, the incident ﬁeld inducing the second one, this is a true nonlinear optical effect. Another effect can be envisaged in which the susceptibility is ijk ð0; !=2; !=2Þ, i.e. there is a cancellation of the two incident frequencies to produce a polarization in the crystal. This is called optical rectiﬁcation. Parametric ampliﬁcation is an effect caused when an incident beam at frequency !1 is incident on a nonlinear optical crystal at the same time as an intense pump beam frequency !2, where !2 > !1 . The !1 wave is then ampliﬁed accompanied by an ‘idler’ wave of frequency !3 ¼ !2 !1. !

!

!

1.6.2.7. Quadratic electro-optic effect "o ijk‘ Ej 1 Ek 2 E‘ 3 This effect, known also as the Kerr effect, results from setting !1 ¼ !, !2 ¼ !3 ¼ 0, i.e. the susceptibility is ijk‘ ð!; !; 0; 0Þ, thus: P!i ¼ "o ijk‘ E!j E0k E0‘ : Like the linear electro-optic effect described above, a static electric ﬁeld applied to the medium causes a change in the refractive indices, which then affects the polarization of the transmitted light. The difference here is that the Kerr effect is displayed by all transparent media, including liquids. In an otherwise optically isotropic system, application of a strong static ﬁeld makes the system optically anisotropic: this change from isotropic to anisotropic can be used to produce a fast optical shutter. Because the light frequency is unchanged, this can be termed a linear optical effect, but on the other hand, because it depends on the square of the static electric ﬁeld, it is a nonlinear electrical effect. 1.6.2.8. Electric-ﬁeld induced second harmonic generation "o ijk‘ E!j 1 E!k 2 E!‘ 3 If !1 ¼ !2 ¼ !=2 and !3 ¼ 0, i.e. the susceptibility is ijk‘ ð!; !=2; !=2; 0Þ, the resulting polarization is !=2 0 P!i ¼ "o ijk‘ E!=2 j Ek E‘ :

and corresponds to the situation where light of frequency ! passes into the crystal at the same time as a static electric ﬁeld is applied. The effect, sometimes known as the Pockels effect, is to change the polarization state of the incident light, effectively by altering the refractive indices of the crystal. This physical property is governed by the third-rank electro-optic susceptibility ð2Þ, components ijk, which follow the same symmetry constraints as the piezoelectric tensor. Crystals therefore must lack a centre of symmetry for this effect to be observable. Although this can be classiﬁed as a nonlinear effect, because more than one incident ﬁeld is involved, it is customary to call it a linear electro-optic effect, as only a single electrical ﬁeld is used, and moreover there is no change in the frequency of the incident light.

A second-harmonic response is obtained, but this time induced by a static electric ﬁeld. This is called electric-ﬁeld-induced SHG or EFISH. It is a nonlinear optical effect that is created by a linear electric effect. 1.6.2.9. Four-wave mixing "o ijk‘ E!j 1 E!k 2 E!‘ 3 One use of a third-order nonlinear optical susceptibility is in the important area of four-wave mixing. In this case, the complex amplitude of the induced polarization at the frequency !1 ¼ !2 þ !3 !4 is given by

154

4 P!i 1 ¼ "o ijk‘ ð!1 ; !2 ; !3 ; !4 ÞE!j 2 E!k 3 E! ‘ :

1.6. CLASSICAL LINEAR CRYSTAL OPTICS Thus if a nonlinear crystal is pumped by two counter-propagating beams of frequency !1 ¼ !2 ¼ !, and another beam !4 ¼ ! is input at some angle, a fourth beam !3 ¼ ! results whose complex amplitude will be the complex conjugate of the !4 beam. Thus four-wave mixing is an important arrangement for producing phase conjugation. 1.6.2.10. Faraday rotation "o ijk E!j 1 B!k 2 Application of a static magnetic ﬁeld to certain crystals through which light of frequency ! passes causes a change in polarization state via P!i

¼

"o ijk E!j B0k :

The effect is to rotate the plane of polarization of the incident light, the size of the effect depending not only on the length of the medium traversed, but also on the size of the applied magnetic ﬁeld. An interesting difference from ordinary optical rotation is that on reﬂecting the light beam back through the medium, the plane of polarization is further rotated rather than cancelled: this property has been used in making optical isolators. !

!

!

1.6.2.11. Quadratic magneto-optic effect "o ijk‘ Ej 1 Bk 2 B‘ 3 By analogy with the quadratic electro-optic effect, application of a strong static magnetic ﬁeld can modulate the polarization state of the incident light via

magnetic ﬁeld outside the crystal to that inside (a good description of Ewald’s work on this can be read in the book P. P. Ewald and his Dynamical Theory of X-ray Diffraction, published by the International Union of Crystallography, Oxford Science Publications, 1992). For the purposes needed here, it is sufﬁcient to apply Maxwell’s equations to a bulk anisotropic continuum crystal, thus taking a macroscopic approach. The treatment here follows that given by Nussbaum & Phillips (1976). Consider the relationship between the dielectric displacement D and an electric ﬁeld E which in tensor terms is given by Di ¼ "o "ij Ej ;

where "o is the vacuum dielectric permittivity and "ij is a secondrank tensor, the relative dielectric tensor. Correspondingly, there is an induced polarization P related to E via Pk ¼ "o k‘ E‘ ;

!2 1.6.2.12. Linear photoelastic effect "o ijk‘ E!j 1 Tk‘

Also known as the piezo-optic effect (or elasto-optic effect), this is usually observed through ijk‘ ð!; !; 0Þ, i.e. the applied stress is static. Thus the application of a force to an elasto-optic material results in a change in birefringence. This effect can be seen not only in crystals, but also in isotropic materials such as glass or transparent plastics. By observation of a stressed material between crossed polars, the resulting strains can be seen as coloured fringes, a useful way of examining engineering structures.

curl H ¼ @[email protected] curl E ¼ @[email protected];

!2 P!i 1 !2 ¼ "o ijk‘ E!j 1 Tk‘ :

A beam of light of frequency !1 passing through the crystal can then be diffracted by the refractive index modulation, and so such a crystal is a useful device for converting sound waves into an optical signal for long-distance transmission along optical ﬁbres. As !1 !2, the frequency of the input light is only very slightly altered by the sound wave, and for most purposes can be neglected.

ð1:6:3:3Þ ð1:6:3:4Þ

where B and H are the magnetic induction and magnetic ﬁeld intensity, respectively. It is customary at this point to assume that the crystal is non-magnetic, so that B ¼ o H, where o is the vacuum magnetic permeability. If plane-wave solutions of the form E ¼ Eo exp½iðk r !tÞ H ¼ Ho exp½iðk r !tÞ

ð1:6:3:5Þ ð1:6:3:6Þ

D ¼ Do exp½iðk r !tÞ

ð1:6:3:7Þ

are substituted into equations (1.6.3.3) and (1.6.3.4), the following results are obtained:

!2 1.6.2.13. Linear acousto-optic effect "o ijk‘ E!j 1 Tk‘

In the acousto-optic effect, the applied stress is at an acoustic frequency !2, i.e. the relevant susceptibility is ijk‘ ð!1 !2 ; !1 ; !2 Þ. Thus a sound wave passing through an acousto-optic crystal modulates the refractive index via

ð1:6:3:2Þ

where k‘ is another second-rank tensor, called the dielectric susceptibility tensor. Note that the restriction to a linear relationship between D and E (or P and E) conﬁnes the theory to the region of linear optics. Addition of higher-order terms (see above) gives nonlinear optics. (Nonlinear optics is discussed in Chapter 1.7.)

P!i ¼ "o ijk‘ E!j B0k B0‘ : This effect is also known as the Cotton–Mouton effect.

ð1:6:3:1Þ

k H ¼ !D

ð1:6:3:8Þ

k E ¼ !B:

ð1:6:3:9Þ

These equations taken together imply that D, H and k are vectors that are mutually orthogonal to one another: note that in general E and D need not be parallel. Similarly B (and hence H), E and k are mutually orthogonal. Now, on substituting (1.6.3.9) into (1.6.3.8), 1 k ðk EÞ ¼ D: o ! 2

ð1:6:3:10Þ

Deﬁning the propagation vector (or wave normal) s by c ð1:6:3:11Þ s ¼ k ¼ n^s; ! where s^ is the unit vector in the direction of s and n is the refractive index for light propagating in this direction, equation (1.6.3.10) then becomes

1.6.3. Linear optics 1.6.3.1. The fundamental equation of crystal optics It is necessary, in order to understand fully the propagation of light through a general anisotropic crystal, to address the question of the way in which an electromagnetic wave is affected by its passage through a regular array of atoms or molecules. A full analysis of this problem at a microscopical level is complicated and was treated, for example, by Ewald (1916), who showed through consideration of a ‘half-crystal’ how to link the electro-

1 s ðs EÞ ¼ D: o c2

ð1:6:3:12Þ

Via the vector identity A ðB CÞ ¼ ðA CÞB ðA BÞC, this result can be transformed to

155

ðs sÞE þ ðs EÞs ¼ o c2 D:

ð1:6:3:13Þ

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.6.3.1. The optical indicatrix.

s sP is equal to n2 and s E can be expressed simply in tensor form as j sj Ej. Now, with equation (1.6.3.1), the fundamental equation of linear crystal optics is found: P ð"ihj þ si sj ÞEj ¼ n2 IEi ; ð1:6:3:14Þ

Fig. 1.6.3.2. Positive and negative uniaxial indicatrix.

as the other. This latter solution can be rewritten as 1 cos2 sin2 ¼ þ 2 ; n22 n2o ne

j

ð1:6:3:21Þ

where I is the unit matrix. 1.6.3.2. The optical indicatrix Equation (1.6.3.14) is the relevant starting point for the derivation of the way in which light propagates in an anisotropic medium. To solve it in a particular case, treat it as an eigenvector– eigenvalue problem: the Ei are the eigenvectors and n2 the eigenvalues. For example, take the case of a uniaxial crystal. The dielectric tensor is then given by 0 1 "11 0 0 @ 0 "11 0 A: ð1:6:3:15Þ 0 0 "33 Assume that light propagates along a direction in the x2 x3 plane, at an angle to the x3 axis. Then, using (1.6.3.11), it is seen that s1 ¼ 0 s2 ¼ n sin s3 ¼ n cos and

0

0 s i sj ¼ @ 0 0

0 n2 sin2 n2 sin cos

1 0 n2 sin cos A: n2 cos

ð1:6:3:16Þ

ð1:6:3:17Þ

Substituting into equation (1.6.3.14) yields 0 10 1 0 0 "11 E1 B CB C 2 2 2 @ 0 "11 þ n sin n sin cos [email protected] E2 A 0 n2 sin cos "33 þ n2 cos E3 0 2 10 1 E1 0 0 n B CB C ð1:6:3:18Þ ¼ @ 0 n2 0 A @ E 2 A : 0

0

n2

E3

Solving this for the eigenvalues n gives n21 ¼ "11

ð1:6:3:19Þ

1 cos2 sin2 ¼ þ n22 "11 "33

ð1:6:3:20Þ

as one solution and

showing how the observed refractive index n2 varies between the limits set by no and ne , called the ordinary and extraordinary refractive index, respectively (sometimes these are denoted by ! and ", respectively). Equation (1.6.3.21) can be thought of as the equation of a uniaxial ellipsoid (circular cross section) with the lengths of the semi-axes given by no and ne . This is illustrated in Fig. 1.6.3.1, where OZ is the direction of propagation of the light ray at an angle to x3. Perpendicular to OZ, an elliptical cross section is cut from the uniaxial ellipsoid with semi-axes OA equal to no and OB given by (1.6.3.21): the directions OA and OB also correspond to the eigenvectors of equation (1.6.3.4). Direction OA is therefore the direction of the electric polarization transverse to the propagation direction, so that the refractive index measured for light polarized along OA is given by the value no. For light polarized along OB, the refractive index would be given by equation (1.6.3.7). When OZ is aligned along x3 , a circular cross section of radius no is obtained, indicating that for light travelling along OZ and with any polarization the crystal would appear to be optically isotropic. The ellipsoid described here is commonly known as the optical indicatrix, in this case a uniaxial indicatrix. Two cases are recognized (Fig. 1.6.3.2). When no < ne , the indicatrix is a prolate ellipsoid and is deﬁned to be positive; when no > ne , it is oblate and deﬁned to be negative. Note that when no ¼ ne the indicatrix is a sphere, indicating that the refractive index is the same for light travelling in any direction, i.e. the crystal is optically isotropic. The quantity n ¼ ne no is called the linear birefringence (often simply called birefringence). In general, then, for light travelling in any direction through a uniaxial crystal, there will be two rays, the ordinary and the extraordinary, polarized perpendicular to each other and travelling with different velocities. This splitting of a ray of light into two rays in the crystal is also known as double refraction. The origin of the birefringence in terms of the underlying crystal structure has been the subject of many investigations. It is obvious that birefringence is a form of optical anisotropy (the indicatrix is not spherical) and so it must be linked to anisotropy in the crystal structure. Perhaps the most famous early study of this link, which is still worth reading, is that of Bragg (1924), who showed that it was possible to calculate rough values for the refractive indices, and hence birefringence, of calcite and aragonite. His theory relied upon the summation of polarizability contributions from the Ca2+ and O2 ions. Returning now to the theory of the indicatrix, more general solution of the fundamental equation (1.6.3.14) leads to a triaxial

156

1.6. CLASSICAL LINEAR CRYSTAL OPTICS 1.6.4. Practical observation of crystals

Fig. 1.6.3.3. Biaxial indicatrix, showing the two optic axes and corresponding circular cross sections.

ellipsoid, i.e. one in which all three semi-axes are different from one another (Fig. 1.6.3.3). It is conventional to label the three axes according to the size of the refractive index by n > n > n (or simply > > ). In such an ellipsoid, there are always two special directions lying in the – plane, known as the optic axial plane, and perpendicular to which there are circular cross sections (shown shaded) of radius . Thus these two directions are optic axes down which the crystal appears to be optically isotropic, with a measured refractive index for light of any polarization. For this reason, crystals with this type of indicatrix are known as biaxial. When the angle between the optic axes, denoted conventionally as 2V, is acute about the axis, the crystal is positive biaxial, and when it is acute about the crystal is negative biaxial. Note that as 2V becomes smaller, the biaxial indicatrix becomes closer to a uniaxial indicatrix (positive or negative). In all general directions the crystal is optically anisotropic. Thus, for light along x3 , the measured refractive indices will be and for light polarized along x1 and x2 , respectively; for light along x2 , and are measured for light polarized along x1 and x3 , respectively; and along x1 , and are measured for light polarized along x2 and x3 , respectively. There are therefore three different linear birefringences to measure: –, – and –. The different indicatrices are oriented in the crystal according to symmetry considerations (Table 1.6.3.1), and so their observation can form valuable and reliable indicators of the crystal system. 1.6.3.3. The dielectric impermeability tensor It has been seen how the refractive indices can be described in a crystal in terms of an ellipsoid, known as the indicatrix. Thus for orthogonal axes chosen to coincide with the ellipsoid axes, one can write x21 x22 x23 þ þ ¼ 1; n21 n22 n23

ð1:6:3:22Þ

where n1 ¼ ð"11 Þ1=2, n2 ¼ ð"22 Þ1=2 and n3 ¼ ð"33 Þ1=2 . One can write this equation alternatively as 11 x21

þ

22 x22

þ

33 x23

¼ 1;

1.6.4.1. The polarizing microscope There are countless applications of polarizing microscopy. One of the largest ﬁelds of use is in mineralogy and petrology, where the requirement is to identify naturally occurring minerals, the optical properties of which have already been determined elsewhere. Medical applications of a similar sort exist, for instance in the identiﬁcation of the minerals present in bladder or kidney stones. The chemist or materials scientist who has synthesised a crystalline material may also wish to identify it from known properties, or it may be a new substance that needs to be described. For other purposes it might, for example, be necessary to determine the orientation (relative to crystallographic axes) of mineral specimens, e.g. in the cutting of synthetic corundum for the manufacture of watch jewels. This section explains the point of view of an observer who wishes to record and measure optical properties, for whatever reason. Although much of what follows is discussed in terms of mineral crystals, it is equally valid for crystals in general, whether organic or inorganic. The polarizing microscope incorporates ﬁve major features not found in ordinary microscopes. These are: (i) A polarizer, normally a sheet of Polaroid, which is part of the microscope substage assembly. This produces plane-polarized light before the light reaches the specimen. In some microscopes, the polarizer can be rotated, though applications of this technique are rare. In the commonly used petrological microscope, the vibration direction of the polarizer is set in what is called the E–W direction, that is, as the user of the microscope sees the ﬁeld of view, the vibration direction is from side to side. (ii) An extra, high-power condenser situated in the substage immediately below the specimen. The condenser is switched in and out of the optical path as required. (iii) A rotating stage, circular in plan and graduated in degrees. For a number of purposes, specimens can be rotated through known angles. (iv) An analyser, a second polarizing device, situated in the microscope tube above the specimen. Its vibration direction is set at right angles to that of the polarizer, i.e. usually N–S. Like the condenser, this can be inserted into the optical path as needed. (v) A Bertrand lens, also in the microscope tube and insertable as required, which has the function of transferring images from the back (upper) focal plane of the objective to the front (lower) focal plane of the eyepiece. The Bertrand lens and the extra substage condenser are used together to convert the microscope from the orthoscopic to the conoscopic conﬁguration (see later). In addition, polarizing microscopes have slotted tubes that allow the insertion of a variety of extra devices generally known as accessory plates. Most common amongst these are the sensitive-tint plate (or 1 plate) and the quartz wedge. Objective lenses of various magnifying powers are mounted in a rotating turret. Apart from magniﬁcation (typically ca 5 for low power, and 40 or more for high power), the numerical aperture (n.a.) of a lens is an important feature. This is deﬁned as the diameter divided by the focal length. This is a measure of the angle of the cone of light that can enter the objective. In the

ð1:6:3:23Þ

where the ii ¼ 1="ii are the relative dielectric impermeabilities. For the indicatrix in any general orientation with respect to the coordinate axes 11 x21 þ 22 x22 þ 33 x23 þ 212 x1 x2 þ 223 x2 x3 þ 231 x3 x1 ¼ 1: ð1:6:3:24Þ Thus the dielectric impermeability tensor is described by a second-rank tensor, related inversely to the dielectric tensor.

157

Table 1.6.3.1. Symmetry constraints on the optical indicatrix Crystal system

Indicatrix

Orientation constraints

Cubic

Isotropic (sphere)

None

Tetragonal Trigonal Hexagonal

Uniaxial

Circular cross section perpendicular to c

Orthorhombic

Biaxial

All indicatrix axes aligned along a, b and c

Monoclinic

Biaxial

One indicatrix axis aligned along b (second setting)

Triclinic

Biaxial

None

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.6.4.1. A thin section of a rock containing the minerals aegirine (elongated crystals) and eudyalite (the matrix) viewed in plane-polarized light in two positions at right angles to each other [(a) and (b)]. Aegirine shows pleochroism from grass-green to yellow–green (compare speciﬁc crystals in the two photographs). Eudyalite shows pleochroism from pink to almost colourless.

conoscopic use of the microscope (see Section 1.6.4.11), this angle is required to be as large as possible so that the properties of rays travelling through the crystal in a variety of directions can be observed. Numerical apertures of more than ca 0.9 can not be achieved with ‘dry’ objectives, but higher values are obtained by inserting a drop of immersion oil between the specimen and the lens. Eyepieces in polarizing microscopes are set in a short tube, at the lower end of which is mounted a set of cross wires, which lie in the front focal plane of the lens. When the microscope is properly focused, a real image of the specimen, created by the objective, is made to coincide with the cross wires. The cross wires are conventionally oriented vertically (N–S) and horizontally (E–W) in the ﬁeld of view, and coincide with the vibration directions of the polarizer and analyser. 1.6.4.2. Specimen preparation Specimens for examination with the polarizing microscope are usually of two different sorts: collections of small crystals or grains (and individual crystals), and thin sections cut from larger solid samples. In the ﬁrst category, the material is often crushed to a ﬁne sand, scattered on a microscope slide, a drop of immersion oil is applied, and a cover slip is placed on top. For special applications, an individual crystal may, for example, be mounted on the end of a glass ﬁbre, and similarly examined under immersion oil. The thin-section technique is more widely used in petrology. Here a rock sample is cut into a section of standard thickness (0.03 mm) and mounted on a glass slide, using a resinous mounting material, formerly Canada Balsam but now synthetic. Small single crystals can also be used by mounting them on a spindle stage, or similar device, which allows one to orient the crystal in the microscope. 1.6.4.3. The indicatrix as an aid to practical microscopy It is convenient for the microscopist to imagine the indicatrix sitting inside the crystal under observation. The indicatrix ellipsoid is ﬁxed with respect to the crystallographic axes, according to different crystal systems (Table 1.6.3.1). The radial dimensions of the ellipsoid, in whatever direction, are a measure of the refractive index of a ray vibrating in that direction. Hence, because ray directions are approximately parallel to the microscope axis, a planar section across the indicatrix at right angles to the axis approximately contains the vibration directions of the ray. Such a section is in general an ellipse, the magnitudes of the major and minor axes of which represent the relative refractive indices, and the directions of which represent the vibration directions of the two transmitted rays. In all cases, the ray with the greater refractive index is known as the slow ray and the other as the fast ray. In uniaxial crystals the ordinary ray may be

slow or fast, depending on the optic sign. This mental image of the indicatrix acts as the microscopist’s guide in the practical operations that follow. 1.6.4.4. Vibration directions For the microscopist, the overriding feature of the behaviour of light transmitted through crystals is double refraction. Many of the observations that can be made with the polarizing microscope depend on the ability to distinguish the individual properties of the two rays. In general, they have different refractive indices, and in coloured crystals they may show different absorptions (i.e. the rays show different colours after transmission, the phenomenon known as pleochroism – see Fig. 1.6.4.1). When the microscope is used for observations in plane-polarized light, the polarizer is inserted into the optical path but the analyser is not. The light before entering the crystal is polarized E–W. On entry, in the general case where the vibration directions of the crystal happen to lie in a random orientation relative to the vibration direction of the polarizer, the light is transmitted as two rays resolved into the two vibration directions of the specimen. These reach the observer’s eye unchanged, and the effects observed are an average of what each ray would individually demonstrate. Two cases can be used to illustrate this fundamental concept. The mineral calcite (CaCO3) is always given as an example of extreme double refraction. In sections cut parallel to the c crystallographic axis, the two rays have refractive indices of 1.486 and 1.658, and this is the maximum difference they can show. Crystals in other orientations always show a smaller difference. The numerical difference between the two refractive indices, when we have identiﬁed the maximum difference, is what is quoted as the birefringence of the mineral, and for calcite it is unusually large (0.172) by the standards of other commonly occurring minerals (cf. quartz = 0.009). Birefringence is an important quantitative optical property, because in thin sections it is easily measurable. It is also useful to refer to the birefringence of individual grains, but this should not be confused with the use of the same term, based on maximum birefringence, as a diagnostic optical property of the material concerned. Consider a calcite crystal lying with its c axis in the plane of the microscope slide. The vibration directions are parallel and at right angles to the crystallographic axis. On rotation of the stage, the c axis may be brought into parallelism with the vibration direction of the polarizer, in which case all the light is transmitted using only one of the vibration directions, which in this case has a refractive index of 1.486. On turning the stage through a right angle, all the effects seen are completely due to the other ray, with a refractive index of 1.658. The mounting medium in standard thin-section preparations has a refractive index of ca 1.54.

158

1.6. CLASSICAL LINEAR CRYSTAL OPTICS Hence, in the ﬁrst position there is quite a large contrast between the refractive index of the crystal grain and the mounting medium, and in the other it is considerably smaller. Calcite is usually a highly transparent and virtually colourless substance, and whether the observer can even see the crystals depends on the refractive index difference between it and the mounting medium. In the ﬁrst case, it is highly visible and in the second case it is harder to see. It is of course the roughness of the surface of the thin section, or the angularities of the form of the crushed crystal, which create small refractions, if there is a refractiveindex contrast between it and the mounting medium, and thus make the crystal visible. The general property is known as relief. High relief means highly visible in this sense. Calcite shows such extreme changes in relief on rotation of the stage that the phenomenon is known as twinkling. Relief is not a measurable property, but to the experienced microscopist it is a subtle and useful guide to identiﬁcation. As a second example consider the mineral biotite, which shows extremely strong pleochroism. Biotite is for practical purposes a hexagonal mineral having a platy form dominated by a strong cleavage on (001.1). In thin sections, biotite crystals cut across the cleavage, i.e. parallel to the direction [00.1], are typically very dark brown in plane-polarized light when the cleavage lies parallel to the polarizer direction. When turned through 90 , the same crystals are only a very pale brown, pale yellow, or almost colourless. The colour contrast, a consequence of the different absorbing properties of the two rays, is striking. Examples of pleochroism are shown in Fig. 1.6.4.1. From these examples it should be clear that the different rays show different things. However, the microscopist needs to be certain that the observations made refer exactly to one ray or the other. When the analyser is inserted into the optical path, most crystals (excluding those of the cubic system, and crystallites lying in special orientations) will show polarization colours, a consequence of the interference between the two rays once they are recombined vibrating in the analyser plane. Details will be discussed below, but for the present purpose it is the extinction position that is of importance. On rotation, a crystal viewed with both analyser and polarizer in position (a conﬁguration known as crossed Nicols, after the Nicol prism, the forerunner of Polaroid) will transmit no light in two positions at right angles to each other. This happens when the vibration direction of a transmitted ray coincides with that of the polarizer. In this case, all the light transmitted through the crystal vibrates in a single direction, at right angles to the vibration direction of the analyser, and it is consequently unable to reach the observer. Thus, for all observations of the effects of a particular ray, crossing the polars (inserting the analyser), turning the stage to an extinction position, and then uncrossing the polars (removing the analyser) leaves the specimen showing the pure effects of whichever ray vibrates in the same direction as the polarizer. Much that follows depends on this simple operation.

1.6.4.5. Measuring refractive indices Refractive indices measured carefully can be extremely useful aids in crystal identiﬁcation, as well as being of importance as physical properties of interest. Apart from distinguishing crystalline species that may look similar under the microscope but have widely different refractive indices, the precise composition of crystalline materials belonging to important solid-solution series (e.g. the plagioclase feldspars or the olivines, in geological applications) can also be determined. The direct measurement of refractive indices is often made by the examination of crystal grains mounted in an immersion oil, using the so-called Becke line test. This is observed in planepolarized light with the substage diaphragm closed down to produce a narrow beam of essentially parallel rays. A medium-

power lens is usually suitable. When the oil has a refractive index different from that of the crystal, the Becke line appears as a bright rim of light around the edge of the crystal. However, as the microscope tube is racked up and down slightly (i.e. the position of focus is changed), the Becke line moves in or out relative to the crystal edge. As the position of focus is lowered the line moves towards the medium with the lower refractive index, e.g. if the oil has a higher refractive index than the crystal, lowering the focus (racking down) causes the Becke line to contract into the crystal. It is of course important to set the specimen in an extinction position before making the observation. If the oil has a refractive index between those of the two rays passing through the crystal, then the behaviour of the Becke line will reverse if the crystal is rotated to the other extinction position. In cases where there is a very large contrast between the crystal and the surrounding medium, a line as such may not be observed, but rather the specimen may appear to glow with concentrated light. The equivalent of Becke line movement is then the expansion or contraction of the light pool with changing focus. The general objective of the observations is eventually to achieve an exact match between the immersion medium and the crystal. This is done by choosing different oils, or mixtures of oils, in sequence, the refractive indices of which are measured by a suitable refractometer. Ideally monochromatic or near-monochromatic light (e.g. the Na doublet with ¼ ca 590 nm) is used, in which case the Becke line simply disappears when the crystal and the oil match. In white light however, because of dispersion by the oil, a match is shown by the presence of two faint Becke lines, one red and one greenish blue, which migrate in opposite directions as the focus is changed. The general strategy of refractive-index determination is perfectly straightforward for cubic crystals, but requires the separate determination of values of ne and no in uniaxial crystals, and n , n and n in biaxial crystals. The most general case is that of the biaxial crystal. If a large number of crystal grains in the mount are examined, a number of cases may be distinguished. (i) All grains have both refractive indices higher than the oil. The oil has a refractive index below n. (ii) All grains have both refractive indices below that of the oil. The oil has a refractive index above n . (iii) Some grains have both refractive indices above that of the oil, while others have one above and one below. The oil has a refractive index between n and n . (iv) Conversely, some grains have both refractive indices below the oil, while others have one above and one below. The oil has a refractive index between n and n . Uniaxial crystals present a simpler series of cases, in which the crystal may show both refractive indices higher than the oil (i.e. the refractive index of the oil is less than that of the fast ray), both lower than the oil, or one higher and one lower. Systematic application of the above techniques leads to the determination of all the refractive indices required, and constitutes one of the most powerful methods of crystal identiﬁcation or description. However, it is useful to make an additional check using the fact that, in anisotropic crystals, any specimen that fails to show polarization colours between crossed polars (i.e. remains dark in all stage positions) must lie with an optic axis parallel to the microscope axis. Such a crystal directly shows no (uniaxial crystals) or n (biaxial crystals). Furthermore, crystal grains showing maximum birefringence (see below) can be checked to see if they give a centred ﬂash ﬁgure (see later), and if they do, their two vibration directions will show ne and no , or n and n , that is, the optic axis or axes lie in the plane of the microscope slide. In larger crystalline specimens, several other techniques are available for measuring the refractive index. Perhaps the simplest and also the most convenient is to cut the crystal into a prism, and use minimum-deviation measurements on a spectrometer table. In addition, large plates can be inserted directly into a commer-

159

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES cial refractometer, in order to measure the refractive index directly.

where z is the thickness of the section. The time difference between the two rays is then

1.6.4.6. Determination of linear birefringence

t1 t2 ¼

The numerical determination of linear birefringence gives less information than a full set of refractive-index measurements, but is nevertheless highly useful in crystal identiﬁcation, particularly in mineralogical and petrological applications where the thin section is the norm. It is also a most sensitive indicator of changes in the crystal structure at a phase transformation or as a function of temperature, pressure etc. Refractive-index determination is tedious, but birefringence determination is quick and easy. Double refraction generates polarization colours when crystals are viewed between crossed polars, except where the crystal is by chance in an extinction position, or cut normal to an optic axis. The colours result from the interference of the two transmitted rays when they are combined into one vibration direction in the analyser. Polarization colours are best observed with the substage diaphragm moderately closed down, so that the transmitted light corresponds to a roughly parallel bundle of rays (if the diaphragm is wide open, and the supplementary condenser is inserted, the resultant rays are far from parallel, and the polarization colours will immediately be seen to degrade in the direction of whitening). Considering a section showing two refractive indices, n1 and n2 , the time difference required for a ray to traverse the section is

ðn1 n2 Þz ; c

ð1:6:4:2Þ

which is referred to as the retardation. Multiplication by c gives the relative retardation or optical path difference, R, where R ¼ cðt1 t2 Þ ¼ ðn1 n2 Þz:

ð1:6:4:3Þ

R is usually expressed in nm (formerly mm). The possibilities of interference clearly depend on R, but also on wavelength. For complete destructive interference, because of the way the transmitted rays are resolved into the vibration direction of the analyser (see Fig. 1.6.4.2), R must either be zero (as in cubic crystals, and sections normal to optic axes in anisotropic crystals) or a whole number of wavelengths. Thus as R changes, either with thickness, orientation of the crystals or with variation in birefringence in different substances, a variety of colours are produced, essentially formed from white light with various wavelengths subtracted. There is a good discussion of this point in Wahlstrom (1959). Fig. 1.6.4.3 shows the effect of increasing R on a variety of visible-light wavelengths. When R is zero, no light is transmitted since all wavelengths show total destructive interference. As R increases a little, all wavelengths continue to show interference, and the polarization colours are essentially greys, which decrease nz ð1:6:4:1Þ in darkness until the middle of the ﬁrst order where the grey is t¼ ; very pale, almost white. Most wavelengths at this stage are c showing relatively strong transmission. With increasing R, the region is reached where the shortest wavelengths of the visible light spectrum (violet) are beginning to approach a phase difference of 1. The transmitted light then takes on ﬁrst a yellow tinge and then bright orange, as violet light (at R 400 nm) and then blue are completely removed. Next, the removal of green light (R 500 nm) results in the transmitted light being red and at R 560 nm the top of the ﬁrstorder colours is reached with the removal of yellow light. The resultant polarization Fig. 1.6.4.2. Successive sections across the optical path of the microscope. (a) Above the polarizer, colour is a distinctive magenta colour beneath the crystal. Polarized light vibrates E–W. (b) Within the crystal. Transmitted light is resolved into known as sensitive tint. The accessory the two vibration directions of the crystal ( 1 and 2 ). (c) Above the analyser. The two transmitted rays plate known as the ‘sensitive-tint’ or ‘1’ are resolved into the N–S direction. Amplitudes are shown, but phase difference is not. plate is made to have R = 560 nm. Its use will be explained below, but meanwhile note that the polarization colour is socalled because with only very slight changes in R it becomes obviously red (falling R) or blue (rising R). Between R = 560 nm and R = 1120 nm, the second-order colours are produced, and are similar in appearance to the colours of the rainbow (blue, green, yellow, orange and red in sequence), as orange, red, violet, blue, and green are successively cut out. The third-order colours (R = 1120–1680 nm) are essentially a repeat of the second-order, but there is a subtle change of quality about them, as they take on slightly garish hues compared with rainbow colours (the red at the top of the order has for example a distinct air of ‘shocking pink’ or even lipstick about it). This effect is a consequence of the increasing chances that two Fig. 1.6.4.3. Plot of retardation, R, versus wavelength, showing how polarization colours are formed. wavelengths will be cut out simulta-

160

1.6. CLASSICAL LINEAR CRYSTAL OPTICS 1.6.4.7. Identiﬁcation of polarization colours

Fig. 1.6.4.4. A quartz wedge between crossed Nicols. The thin end is on the left. The colours shown vary between about the middle of the ﬁrst order up to high ﬁfth order.

neously (see Fig. 1.6.4.3), e.g. while ﬁrst-order red results from the removal of green, second-order red results from the removal of both violet and yellow. With increasing R, the distinction of colours within each order becomes weaker as the number of wavelengths simultaneously removed increases. Colours are diluted towards grey or white, so that from the ﬁfth order upwards the range is little more than an alternation of pale pinkish and pale greenish tints. Eventually, at higher orders the polarization colours become a more-or-less uniform dull white. Fig. 1.6.4.4 shows the colours produced by a quartz crystal cut into a wedge shape.

Birefringence can be determined quantitatively if the polarization colour can be correctly identiﬁed, and the section is of known thickness (see Fig. 1.6.4.6). It is of course necessary to distinguish between the birefringence of an individual grain, which will depend on orientation (see Fig. 1.6.4.5a), and the maximum birefringence (highest polarization colour) shown by the crystals concerned. It is the latter that is diagnostic, and in general it will be necessary to examine as many grains as possible to determine it. The grey colours of the lower part of the ﬁrst-order colours are unique and immediately identiﬁable, but all other colours are at least superﬁcially ambiguous. Even ﬁrst-order white may be confused with a high-order white. There are essentially two methods of determining the order of an ambiguous colour, the ﬁrst of which, fringe counting, is discussed here. Other methods depending on the use of the quartz wedge and sensitive-tint plate will be considered later. 1.6.4.8. Fringe counting In a well made thin section, most crystals show a uniform polarization colour because of uniform orientation and thickness. Crystal edges, however, frequently taper off to near-zero thickness. In this case, the edge acts as a natural wedge of variable R and displays a series of fringes corresponding to the orders within the complete spectrum of interference colours, from ﬁrst-order grey up to the main colour shown by the body of the crystal (Figs. 1.6.4.5b and c). Using a moderately high power objective, it is often easy to identify the individual bands and thus count up to the order concerned. The colour band red–sensitive tint–blue

Fig. 1.6.4.5. (a) Photomicrograph between crossed polars of a thin section of rock containing large olivine crystals set in a ﬁne-grained matrix. The olivine crystals show a variety of polarization colours (ﬁrst-order to high second-order) depending on their orientation. (b) Thin section between crossed polars of a rock containing a large pyroxene crystal, intergrown with other phases marginally. The edges of the crystal are wedge-like, and therefore thinner than the main body. The ﬁrst-order white to orange colours make a prominent fringe on the right, grading inwards to sensitive tint and then to blue. The main body of the crystal is thus determined as second-order blue. (c) A similar section to that in (a) (centre of photograph) but here the second-order blue fringe is narrow and is succeeded by a second-order yellow fringe. Hence the main body of the crystal must be showing second-order pink.

161

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES marking the ﬁrst/second-order change is particularly easy to spot because of its generally dark colour. The method is also usable when the crystal grain has a sloping contact with a different crystal, and is especially easy when the latter has signiﬁcantly lower birefringence. In this case, there are effectively two superimposed wedges (leading to some interesting addition or subtraction effects on R), but counting the fringes in ascending order will lead correctly to the identiﬁcation of the polarization colour of the high-birefringence grain.

When this effect is seen, it shows that the slow direction of the crystal lies NE–SW. In the converse case, the observed polarization colour also changes, and, if the original colour is at least as high as secondorder, will move down the scale by one complete order, e.g. second-order orange (R = 950 nm) changes to ﬁrst-order yellow/ orange (R = 390 nm). If the original colour is, however, within the ﬁrst order (i.e. R < 560 nm), the new colour is still a consequence of subtracting 580 nm from R, but it is the absolute value of the new R (not the sign) which is relevant. For example, if the original colour is a ﬁrst-order grey (R = 100 nm), the new colour corresponds to R = 460 nm, i.e. ﬁrst-order orange. As a rapid mental 1.6.4.9. Fast and slow vibration directions aid, it is useful to think of the original colour falling to the bottom Before discussing other methods of identifying polarization of the scale (R = 0) and then ‘bouncing’ back up until a change of colours, it is necessary to explain the use of the sensitive-tint plate one order has been reached, e.g. a ﬁrst-order white, in the middle and the quartz wedge. Both devices consist of a crystal mounted of the ﬁrst order, hardly changes (half an order down followed by in an elongated holder that can be inserted into a slot in the half an order up); ﬁrst-order red changes to ﬁrst-order grey (a fall microscope tube set at 45 to the vibration directions of the of 90% of an order, followed by a rise of 10%). If there is any doubt about the identiﬁcation of the new colour, polarizer and analyser. The vibration directions of the plates themselves are normally oriented so that the slow ray vibrates the crystal should be rotated through 90 and the second new colour examined. A comparison of the two options available, NE–SW and the fast ray NW–SE. The sensitive-tint (or 1) plate is made from a cleavage sheet before and after rotation, rarely leaves any doubt about which is of the white mica, muscovite, and has a thickness such that R = the higher colour (i.e. the slow-parallel-to-slow case). In all cases, 560 nm. To determine fast and slow directions in an unknown whether or not the original colour is in the ﬁrst order, one of the specimen, the crystal grain is set to an extinction position and two new colours is higher than the other. The sensitive-tint plate is so-called because it allows investithen rotated 45 in either direction. Thus its own vibration directions lie in diagonal positions, and when the tint plate is gation of crystals showing very low birefringence (e.g. dark greys inserted, the vibration directions of plate and grain are parallel to with R 50 nm or less). In the parallel position, the new colour each other. There are two possible cases depending whether the will lie just on the blue side of sensitive tint, and in the crossed fast and slow directions coincide or not, i.e. slow vibration position, just on the red side. These two colours are very easy to direction of plate parallel to the slow direction of the crystal (and distinguish even though they represent only a small change in R. From the above, it should be clear what an important aid the fast parallel to fast) or slow direction of plate parallel to the fast sensitive-tint plate can be in the actual identiﬁcation of an direction of the crystal. In the ﬁrst case, the relative retardation is increased by 560 nm unknown polarization colour, whether it be the body colour of and the observed polarization colour jumps up the scale by one the crystal or something observed in a set of grain-margin fringes. complete order as the plate is inserted. Thus, for example, ﬁrst- There are always two other colours that can be generated using order white (R = 230 nm) changes to second-order yellow/green the plate, and their relationship to the original colour is known in (R = 790 nm), second-order blue changes to third-order blue etc. terms of R change, so that there are altogether three colours providing information. The quartz wedge (Fig. 1.6.4.6) is an elongated wedge-shaped plate of progressively increasing thickness, usually cut parallel to the c axis so that the slow vibration direction is parallel to the length of the wedge. In this form it is inserted into a NE–SW slot so that the slow direction has this orientation. Some microscopes are, however, ﬁtted with a NW–SE slot, and are provided with wedges (and sensitive-tint plates) that are ‘length fast’ rather than ‘length slow’. The optical effects are of course the same in both cases, but it is always a good idea to examine an accessory plate for its vibration directions (marked by the manufacturer) to be on the safe side. The wedge varies in thickness from almost zero to about 0.2 mm, and typically shows a range of polarization colours from dark ﬁrst-order grey up to the fourth order or so, as it is progressively inserted into the slot. The wedge can thus be used to change the polarization colour of an observed crystal by any Fig. 1.6.4.6. Polarization colours versus thickness. The lines radiating from the origin are of equal desired amount of R within the available birefringence (numerical values are given at the top and the right-hand side of the ﬁgure). The diagram range (roughly 0–2500 nm). By using the may be used to determine thickness if birefringence is known, or birefringence if thickness is known. For example, the diagonal line for birefringence = 0.009 (e.g. quartz) intersects the standard thin-section two vibration directions of the crystal, thickness (0.03 mm) on ﬁrst-order white. This is the polarization colour shown by quartz in a standard these changes can be made additive or subtractive at will. In its simplest possible thin section.

162

1.6. CLASSICAL LINEAR CRYSTAL OPTICS application, the crystal is set so that slow is against fast and the wedge is inserted until the crystal shows as close to zero birefringence as possible, i.e. the relative retardations of the wedge and the crystal are equal and opposite (this is called compensation). Next, the specimen is removed, the colour shown by the wedge noted, and the wedge is slowly pulled out, counting the orders as they go past. This is an accurate and simple alternative method of determining polarization colours. The accessory plates are useful in identifying the order of polarization colours, but their most frequent application is in determining which of the vibration directions shown by a crystal is fast and which is slow. For example, in a specimen of a biaxial crystal lying with the optic axial plane in the plane of the slide, the slow ray represents and the fast ray . To determine which is which, the vibration directions are set in the 45 position and the tint plate is inserted. If the polarization colour goes up by an order, then the slow direction of the plate is parallel to the slow direction of the crystal. Conversely, if the colour goes down by an order, or goes up by less than a complete order (when the original R < 560 nm), fast in the crystal is parallel to slow in the plate.

1.6.4.10. Other methods of measuring birefringence While the use of compensating plates is convenient, more precise techniques have been developed for the measurement of linear birefringence, both in an absolute and in a relative sense. The main methods of making absolute measurements use commercially available compensators mounted on a microscope. The main types are used with a polarizing microscope with crossed polars: (i) Babinet compensator: This is mounted instead of the eyepiece of the microscope, and uses two quartz wedges sliding in opposite directions to each other. The wedges are so designed that when they fully overlap, but without a birefringent specimen in the microscope, a black compensation band is seen in the centre of the ﬁeld of view. Then when the specimen is placed on the microscope stage in one of the two possible 45 positions, the compensation band is shifted. When in the correct 45 position, as found by trial, the lower wedge is then screwed out to recentre the compensation band, and the distance moved is read from an internal scale. This distance is calibrated in terms of relative retardation. (ii) Berek and Ehringhaus compensators: These use a rotating birefringent crystal to change their effective retardation in order to compensate against the retardation of the specimen. The Berek compensator uses a calcite plate 0.01 mm thick, whereas the Ehringhaus compensator has compound compensating plates of either quartz or calcite, made of two sections of equal thickness cut parallel to the optic axes and cemented above one another at right angles. The compensator is inserted in the slot used for accessory plates with the specimen in one of the two 45 positions. Then by tilting the compensator plate, the apparent retardations are varied until the combined retardation matches that of the specimen, thus giving rise to the compensation band appearing in the centre of the ﬁeld of view. The angle of tilt can then be converted to relative rotation by the use of suitable tables provided by the manufacturer. In order to measure birefringence in a relative sense, the following techniques have been devised. All are capable of phenomenal precision in measuring changes in birefringence, in some instances to one part in 107. (i) Se´narmont compensator: A =4 plate is inserted above the specimen, with one of its principal vibration directions, say the slow direction, parallel to the vibration direction of the polarizer. The analyser is rotatable with a divided circle so that the angle of rotation can be measured. It can be shown that the phase shift of the light is given in terms of the angle through which the analyser is turned to achieve extinction by

¼

2 nz ¼ 2:

Thus if the birefringence, or more correctly the relative retardation, of the specimen is changed, say by altering the temperature, one can follow the change simply by monitoring the angle . This can be done either manually, or electronically using a phase meter attached to a photomultiplier to measure the intensity as a function of the angle of the analyser, which is rotated at some frequency by a motor. (ii) Intensity between crossed polars: In this case the specimen is placed in the 45 position between crossed polars and the intensity of the light through the system is measured by a photomultiplier and presented typically on a recorder. On changing the retardation of the specimen, say by heating, this intensity changes according to I ¼ Io sin2 =2: Thus on heating a set of sin2 fringes is drawn out, and by counting the fringes exact measurements of can be made. This technique is of great sensitivity, but suffers from the fact that the specimen must be maintained throughout in the 45 position. (iii) Rotating analyser: In this system (Wood & Glazer, 1980), a =4 plate is inserted below the substage but above the polarizer in order to produce circularly polarized light. On passing through a birefringent crystal specimen, this is generally converted to elliptical polarization. This then passes through a Polaroid analyser set to rotate about the axis of the light at a predetermined frequency !. The resulting intensity is then given by I ¼ ðIo =2Þ½1 þ sinð2!t 2’Þ sin ; where ’ is the angle between the analyser at any time and an allowed vibration direction of the specimen. Thus by measuring the light intensity with a photomultiplier and then by using, say, phase-sensitive detection to examine the signal at 2!, a plot of sin can be made as the specimen’s retardation is changed. The fact that circularly polarized light is incident on the specimen means that it is not necessary to align the specimen to any particular angle. Recently, a new type of optical microscope (Glazer et al., 1996) has been developed using this principle, in which false colour images representing Io , ’ and j sin j can be formed (Fig. 1.6.4.7). 1.6.4.11. Interference ﬁgures Interference ﬁgures provide one of the most powerful tools for obtaining information about a crystal. The simplest applications allow the division of crystals into uniaxial and biaxial classes, hence constraining the crystal system. Within these classes, crystals are easily divided into the subclasses of positive and negative. More advanced techniques enable the orientation of the indicatrix relative to crystallographic features to be fully established. Interference ﬁgures are obtained when the microscope is used in its conoscopic conﬁguration. This means that light is made to pass through the specimen in as wide a range of directions as possible. A powerful substage condenser is inserted to produce a wide cone of incident light and the substage diaphragm is set wide open. A diffusing screen makes a good substitute for the condenser, as it also produces light with a variety of ray directions. However, some brightness is inevitably lost. In either case, a high-power objective with a large numerical aperture is used to collect the light above the specimen, and the polarizer and analyser are crossed. The distinction between conoscopic and orthoscopic (parallellight) applications of the microscope is important. For observations of birefringence, the orthoscopic arrangement is required so that optical path lengths through the crystal are constant. The

163

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.6.4.7. Three birefringence images of industrial diamond viewed along [111] taken with the rotating analyser system. (a) I0 ; (b) j sin j; (c) orientation ’ of slow axis with respect to horizontal.

images observed in plane-polarized light rely on scattering from point sources within the specimen, and do not depend strictly on whether the conﬁguration is conoscopic or orthoscopic. Nevertheless, relief and the Becke line are much more clearly observable in orthoscopic use. The principle of conoscopic use is quite different. Here, the image is formed in the back focal plane of the objective. Any group of parallel rays passing through the specimen is brought to a focus in this plane, at a speciﬁc point depending on the direction of transmission. Hence every point in the image corresponds to a different transmission direction (see Fig. 1.6.4.8). Moreover, the visible effects are entirely caused by interference, and there is no image of the details of the specimen itself. That image is of course also present, towards the top of the tube at or near the cross wires, but the two are not simultaneously visible. The conoscopic image may be viewed simply by removing the eyepiece and looking down the tube, where it appears as a small but bright circle. More commonly however, the Bertrand lens is inserted in the tube, which has the effect of transferring the conoscopic image from the back focal plane of the objective to the front focal plane of the eyepiece, where it coincides with the cross wires and may be examined as usual.

Fig. 1.6.4.8. Formation of the interference ﬁgure. The microscope axis lies vertically in the plane of the paper. A bundle of rays travelling through the crystal parallel to the microscope axis (dashed lines) is brought to a focus at A in the back focal plane of the objective. This is the centre of the interference ﬁgure. A bundle of oblique rays (solid lines) is brought to a focus at B, towards the edge of the ﬁgure.

It is useful to think of the conoscopic image as analogous to the gnomonic projection as used in crystallography. The geometrical principles are the same, as each direction through the crystal is projected directly through the centre of the lens into the back focal plane. 1.6.4.12. Uniaxial ﬁgures To understand the formation of an interference ﬁgure, consider a simple example, a specimen of calcite cut at right angles to the c crystallographic axis. Calcite is uniaxial negative, with the optic axis parallel to c. The rays that have passed most obliquely through the specimen are focused around the edge of the ﬁgure, while the centre is occupied by rays that have travelled parallel to the optic axis (see Fig. 1.6.4.8). The birefringence within the image clearly must increase from nil in the centre to some higher value at the edges, because the rays here have had longer path lengths through the crystal. Furthermore, the image must have radial symmetry, so that the ﬁrst most obvious feature of the ﬁgure is a series of coloured rings, corresponding in outward sequence to the successive orders. The number of rings visible will of course depend on the thickness of the sample, and when birefringence is low enough no rings will be obvious because all colours lie well within the ﬁrst order (Figs. 1.6.4.9a and b). Fig. 1.6.4.10(a) illustrates, by reference to the indicatrix, the way in which the vibration directions of the o and e rays are disposed. Fig. 1.6.4.10(b) shows the disposition of vibration directions in the ﬁgure. Note that o rays always vibrate tangentially and e rays radially. The o-ray vibration directions lie in the plane of the ﬁgure, but e-ray vibration directions become progressively more inclined to the plane of the ﬁgure towards the edge. The shaded cross on the ﬁgure illustrates the position of dark ‘brushes’ known as isogyres (Fig. 1.6.4.10b). These develop wherever vibration directions lie N–S or E–W, hence corresponding to the vibration directions of the analyser and polarizer. As the stage is rotated, as long as the optic axis is truly parallel to the microscope axis, the ﬁgure will not change. This is an example of a centred uniaxial optic axis ﬁgure, and such a ﬁgure identiﬁes the crystal as belonging to the tetragonal, trigonal or hexagonal systems (see Fig. 1.6.4.11a). From the point of crystal identiﬁcation, one can also determine whether the ﬁgure coincides with the uniaxial positive ðne > no ) or uniaxial negative (ne < no ) cases. Inserting the sensitive-tint plate will move the coloured ring up or down the birefringence scale by a complete order. Fig. 1.6.4.11(c) shows the centred optic axis ﬁgure for calcite, which is optically negative. The insertion of a tint plate with its slow vibration direction lying NE–SW lowers the colours in the NE and SW quadrants of the ﬁgure, and raises

164

1.6. CLASSICAL LINEAR CRYSTAL OPTICS

Fig. 1.6.4.9. (a) Centred uniaxial optic axis ﬁgure of a crystal with low birefringence. The isogyres are diffuse and the polarization colours in the quadrants are likely to be ﬁrst-order grey. (b) As above, but for a crystal with high birefringence. The isogyres are narrower, and circular rings of polarization colours are seen, progressing outwards from ﬁrst order to higher orders. (c) Off-centre uniaxial optic axis ﬁgure in the straight position (extinction position of crystal). (d) The same rotated to 45 . The curved arrow shows the rotation of the ﬁgure as the stage is turned clockwise. Arrows inside the ﬁeld of view show directions of motions of isogyres. If the optic axis lies outside the ﬁeld of view, such ﬁgures are difﬁcult to interpret and may easily be confused with an off-centre biaxial optic axis ﬁgure when 2V is small to moderate.

those in the other quadrants (Fig. 1.6.4.11b). The simplest general rule is to look at the dark ﬁrst-order grey in the original ﬁgure, lying immediately adjacent to the optic axis, i.e. the centre of the cross formed by the isogyres (Figs. 1.6.4.11b and c). If the crystal is optically negative, this colour changes to ﬁrst-order yellow in the NE quadrant, if positive to blue. When the crystal has low birefringence, these colours may occupy the whole quadrant.

An off-centre uniaxial optic axis ﬁgure is obtained when the optic axis is inclined to the microscope axis by an amount which is small enough for it still to be visible within the ﬁgure (roughly within 25 of the microscope axis, using a normal high-power objective). Such ﬁgures show an isogyre cross with attendant rings, but the centre of the cross does not lie in the centre of the ﬁgure, and as the stage is rotated the centre of the cross moves round the ﬁgure in a circle (Figs. 1.6.4.9c and d). The isogyres remain NS and EW throughout. If the ﬁgure is so off-centre that the centre of the cross is not visible, the behaviour of the ﬁgure becomes difﬁcult to interpret, and may easily be confused with some sorts of off-centre biaxial ﬁgures (see below). In the extreme case, when the optic axis lies in the plane of the slide, a quite different ﬁgure, known as a ﬂash ﬁgure, is obtained. This is similar to many of the ﬁgures obtained from biaxial crystals, and will be considered further below. 1.6.4.13. Biaxial ﬁgures

Fig. 1.6.4.10. (a) Vibration directions of an oblique ray passing through calcite, viewed relative to the indicatrix. OA is the optic axis, normal to the circular cross section of indicatrix, r is the ray direction, e and o are, respectively, the vibration directions of the extraordinary and ordinary rays in the plane of the elliptical cross section of the indicatrix normal to r. (b) Vibration directions as seen in the ﬁgure. The tangential set represents the o rays, the radial set represents e rays. The isogyres are also shown.

(i) Acute bisectrix ﬁgures: Biaxial ﬁgures may be introduced by considering a crystal with a small 2V angle, oriented so that the acute bisectrix is parallel to the microscope axis. The conoscopic ﬁgure will have much in common with the uniaxial case already discussed (and indeed will become identical as 2V tends to zero), and some form of bilateral rather than radial symmetry is to be expected. Vibration directions within the ﬁgure can be deduced by consideration of the Biot–Fresnel construction. Given that the form of the indicatrix is known, this is used to determine vibration directions in any orientation required. A general case presented in the form of a stereographic projection is given in Fig. 1.6.4.12(a). It is ﬁrst necessary to know the positions of the optic axes and the position of a ray direction. Two planes are constructed, each containing one optic axis and the ray direction. Two additional planes are constructed, each containing the microscope axis and bisecting the angles between the ﬁrst two planes. The plane in which the vibration directions lie is plotted normal to the ray direction, and the two vibration directions in this plane are ﬁxed by the intersections of this plane with the two additional planes. This is also a very powerful construction to use in conjunction with orthoscopic methods. If crystallographic features, e.g. traces of cleavage planes, crystallographic axes, twin planes etc. (twinning is discussed in Chapter 3.3) are added to the stereogram, it becomes possible to determine the predicted angles between vibration directions and crystallographic features. One of the most fundamental aims of polarizing microscopy is the determination of the complete orientation of the indicatrix relative to crystallographic directions. Familiarity with the Biot– Fresnel construction is a substantial aid.

165

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Returning to the interference ﬁgure, a modiﬁed version of the Biot–Fresnel construction is illustrated in Fig. 1.6.4.12(b). Since the interference ﬁgure is analogous to a gnomonic rather than a stereographic projection, the various constructional planes required are straight lines. The vibration directions for the complete ﬁgure are given in Fig. 1.6.4.12(c). Considering ﬁrst the isogyres (brushes), if the optic axial plane lies N–S, as in Fig. 1.6.4.13(a), clearly the isogyres form a cross, as in the uniaxial case. There is a small difference, however. Because the vibration directions curve round more rapidly near the optic axial plane, the N–S isogyre is sharper than the E–W, which is relatively broadened and less dark. If the slide is rotated so that the optic axial plane lies NE–SW, inspection of the vibration directions in Fig. 1.6.4.13(b) shows that the isogyres must part in the direction shown. Rotation of the stage through a full 180 will thus show two positions at which the brushes cross – once when the optic axial plane lies N–S, the other when it lies E–W – and two positions of maximum separation of the isogyres – when the optic axial plane lies NE– SW and NW–SE (see Fig. 1.6.4.14a). The position of the broader, more diffuse, brush will alternate. The amount by which the two

isogyres are separated in the 45 position depends on the size of 2V. Since the ﬁeld of view is usually about 60 , when 2V is 60 the isogyres will retreat right to the edge of the ﬁeld of view in the 45 position, and then come back as rotation continues. When 2V > 60 , the brushes will entirely leave the ﬁeld of view for part of the rotation (Fig. 1.6.4.14c). Approximate estimates of 2V can be made on this basis. As in the uniaxial case, coloured fringes are also part of the ﬁgure, and are most obvious when birefringence is high (Fig. 1.6.4.14a and Fig. 1.6.4.15a). The outermost fringes have an elliptical form, but towards the centre of the ﬁgure they are distorted into a dumbbell-like or ﬁgure-of-eight form. This arises

Fig. 1.6.4.12. (a) The Biot–Fresnel construction illustrated on the stereographic projection. (b) Method of determining vibration directions in a biaxial acute bisectrix ﬁgure using the Biot–Fresnel construction and a gnomonic projection. (c) Complete vibration directions of a ﬁgure similar to the above. As noted in the text, the directions shown are components resolved into the plane of the ﬁgure, and the true vibration directions are in general somewhat inclined.

Fig. 1.6.4.11. (a) Centred optic axis ﬁgure of quartz (uniaxial). The birefringence is low, resulting in a diffuse cross and quadrant colours in the lower half of the ﬁrst order. (b) The same ﬁgure with the sensitive-tint plate inserted (slow vibration direction NE–SW). The isogyres take on the sensitive-tint colour. Compensation takes place in the NE and SW quadrants (slow directions of crystal and plate parallel to each other) resulting in second-order blue, that is, one whole order above the original. In the other quadrants, the colours also apparently rise, but are restricted to yellow (high ﬁrst-order). Thus the crystal is optically positive, that is, e rays (radial) are slow and o rays (tangential) are fast. (c) Centred optic axis ﬁgure of calcite with sensitive-tint plate (slow direction lying NE–SW) inserted. The birefringence is very high so there are many coloured rings. In the top right quadrant, the colour immediately adjacent to the cross is ﬁrst-order yellow, whereas in the top left it is second-order blue. Calcite is hence optically negative. It can be observed that all the coloured rings in the top right and bottom left quadrants are an order lower than their counterparts in the top left and bottom right.

Fig. 1.6.4.13. (a) Illustration of the formation of crossed isogyres when the optic axial plane of a biaxial ﬁgure lies N–S. The shaded lines illustrate the zones in which vibration directions are N–S and E–W, leading to the formation of the isogyres. Along the E–W line, the zone across which vibration directions depart little from N–S and E–W is broad, hence this isogyre is wider than the N–S isogyre. (b) Illustration of the formation of separated curved isogyres when the same crystal is in the 45 position (optic axial plane NE–SW).

166

1.6. CLASSICAL LINEAR CRYSTAL OPTICS

Fig. 1.6.4.14. (a) Drawing of biaxial optic axis ﬁgures set in the 45 position with the optic axial plane set NW–SE. 2V, represented by the angle O1–O2, is about 40 (cf. total ﬁeld of view of ca 60 ). The distribution of coloured fringes is represented, with near-circular areas of ﬁrst-order colours around the optic axes, progressing outwards to higher orders (see also Fig. 1.6.4.15a). (b) The same ﬁgure in the straight position (optic axial plane N–S). Note that the isogyre along the optic axial plane is sharper than the E–W isogyre. (c) Representation of a biaxial ﬁgure in the 45 position when 2V > 60 . The isogyres leave the ﬁeld completely.

because the areas of minimum birefringence must lie adjacent to the optic axes, and birefringence, although generally increasing outwards, must also increase towards a point midway between the optic axes. This effect is slight when birefringence is low, but is prominent when birefringence is high, in which case each optic axis is surrounded by its own set of almost-circular fringes, set within the general elliptical array. Optic sign can be determined from the acute bisectrix biaxial ﬁgure in a way analogous to the uniaxial case. The stage is rotated to the 45 position, i.e. with maximum separation of the isogyres, and the analogues of the uniaxial quadrants are identiﬁed. The difference here is that in one of the 45 positions the NE and SW quadrants join through the space between the optic axes, and in the other the NW and SE quadrants are connected. The sensitivetint plate is employed just as in the uniaxial case, and the same rules apply to change of colour (Fig. 1.6.4.15a and b). For example, suppose that the stage is turned so that the NE and SW quadrants are separated from each other. Optically positive crystals show second-order blue close to the isogyre within the quadrant (on the concave side of the isogyre), while ﬁrst-order yellow appears on the convex side, which is part of the combined NW and SE quadrants. Optically negative crystals show the reverse.

Slightly off-centre acute bisectrix ﬁgures are easy to interpret if 2V is low, but as the degree of off-centring increases, and as 2V increases, it is obvious that interpretational difﬁculties will rapidly increase, and recourse must be made to the optic axis ﬁgure. (ii) Optic axis ﬁgures: Although the acute bisectrix ﬁgure forms the most convenient introduction to the subject, it is in practice quite difﬁcult to ﬁnd a suitable section without trial and error. In monoclinic and triclinic crystals, for example, the acute bisectrix section is not in general identiﬁable by reference to crystallographic features (cleavage, faces etc.), nor by any special optical properties observable under orthoscopic conditions. As in the uniaxial case, however, the optic axis section is identiﬁable by its low-to-nil birefringence. The optic axis ﬁgure is the workhorse of the microscopist. The essential feature of this ﬁgure is that, as the stage is rotated, one of the optic axes is positioned permanently in the centre of the ﬁeld of view, while the other rotates around it. One of the isogyres is always visible. When 2V is small, on rotation of the stage the ﬁgure simply looks like a wobbly version of the acute bisectrix ﬁgure. Both isogyres are visible, and determination of optic sign, using the sensitive-tint plate, is as described above. As 2V increases, however, the second isogyre leaves the ﬁeld during part of the rotation, and the point where the isogyres cross, when the optic axial plane lies N–S or E–W, moves towards the edge of the ﬁeld of view. Eventually, with further increase of 2V, the second isogyre does not enter the ﬁeld of view at all, and the ﬁgure consists of a single brush rotating about the optic axis. The brush changes from straight, when it lies N–S or E–W, to curved, when the crystal is in the 45 position, and the degree of curvature decreases with rising 2V. When 2V = 90 , the brush remains straight in all positions. With experience, the Fig. 1.6.4.15. (a) Acute bisectrix ﬁgure of a biaxial crystal with 2V ’ 40 . The optic axial plane is oriented maximum curvature of the isogyre NW–SE. First-order colours are conﬁned to the two circular ‘eyes’ or melatopes around the optic axes, can be used for rough estimation of with sensitive tint itself making a ﬁgure-of-eight shape (‘dumbbell’). At the edge of the ﬁgure in the NE 2V. and SW directions the coloured fringes reach third-order pink. (b) The same ﬁgure with the sensitive-tint Optic sign is readily determined from plate inserted (slow direction NE–SW). The isogyres have taken on the sensitive-tint colour. Between the any sort of optic axis ﬁgure by setting the optic axes (e.g. the centre of the ﬁgure), the original sensitive-tint dumbbell has become black, and to the crystal in the 45 position and using the NW and SE of the centre all the fringes have dropped by one order. Conversely, in the extreme NW and SE directions all fringes have gained an order. The little patches of yellow lying just inside the optic axes, curvature of the isogyre to identify the and the accompanying blue patches just outside, indicate by analogy with the uniaxial ﬁgure that the various ‘quadrants’ as described above. This of course is not possible when crystal is optically negative.

167

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

2V = 90 , and such crystals are described as optically neutral. A further piece of useful information is derivable from optic axis (and acute bisectrix) ﬁgures, i.e. the direction of the optic axial plane, that is, the line joining the two optic axes. Even if the second isogyre is never visible, the position of the second optic axis, outside the ﬁeld of view, is easily judged. By reverting to orthoscopic observation without moving the specimen, it is easy to see how the optic axial plane relates to crystallographic features such as faces, cleavages or twin planes. (iii) Other biaxial ﬁgures: Several special ﬁgures are occasionally useful, and their behaviour is readily explained by comparison with the acute bisectrix ﬁgure. The obtuse bisectrix ﬁgure behaves like the acute bisectrix ﬁgure, but as if 2V were very large. The isogyres form a diffuse cross in the centre of the ﬁeld, and then, on rotation, rapidly depart from the ﬁeld, either via the NE and SW quadrants or via the NW and SE. As rotation approaches 90 , they re-enter the ﬁeld of view from the other direction. When 2V approaches 90 , there is of course very little difference between the acute and obtuse bisectrix ﬁgures, and to determine which is which it is necessary to measure the speed at which isogyres leave the ﬁeld of view during rotation (for a given rotation the obtuse bisectrix isogyres move further). The optic normal ﬁgure (often known as a ﬂash ﬁgure because of the extreme speed of isogyre movement) is formed when the optic axial plane lies in the plane of the slide. Its behaviour on rotation of the stage is an extremely rapidly moving version of the obtuse bisectrix ﬁgure. The isogyres are very broad and diffuse, and when the cross is formed there is little more than a momentary darkening of the whole ﬁeld of view. The brushes vanish completely from the ﬁeld with only a very small rotation from this position. Often it requires careful inspection even to be certain that the cross splits into two brushes that vanish diagonally from the ﬁeld. The optic normal ﬁgure is useful in orientation studies and, as mentioned above, grain mounts of orthorhombic crystals may naturally give rise to suitably oriented crystals. In thin sections, the ﬁgure is useful to conﬁrm that grains apparently showing maximum birefringence do in fact lie with their optic axial planes normal to the microscope axis. When only a small number of grains are available, this check is important. In the most general sense, this exercise illustrates that all ﬁgures are variations on a single theme, in which the vibration direction diagram of Fig. 1.6.4.12(c) can be thought of as being viewed from different distances (delimiting the size of the area viewed) and different directions (i.e. where the centre of the ﬁeld of view is, relative to the centre of the diagram). For, example, the ﬁgure shown represents a centred uniaxial optic axis ﬁgure if viewed from inﬁnite distance in a direction corresponding to the centre of the diagram. On the other hand, if viewed from close up in the same direction (so that the ﬁeld of view is thought of as a rather small circle in the middle of the diagram), the ﬁgure becomes analogous to the acute bisectrix ﬁgure of a crystal with a large 2V, the obtuse bisectrix ﬁgure, or even the uniaxial ﬂash ﬁgure (but see below), with increasing distance of the viewpoint. Off-centre ﬁgures can be equally well explained by placing the viewpoint non-centrally. Only the uniaxial ﬂash ﬁgure and the biaxial optic normal ﬁgure seem, at ﬁrst sight, to defy exact interpretation, because the optic axes, lying in the plane of the ﬁgure, seem to require to be plotted at inﬁnity in the plane of the paper. This then requires that the map of the vibration directions consists of two linear sets at a right angle to each other. No explanation of the rapid separation of the diffuse isogyres accompanying a small rotation from the extinction position is forthcoming. Rather, a simple extinction of the whole ﬁeld is predicted at every 90 . In fact, the vibration directions seen in such ﬁgures still retain the ‘barrel-shaped’ conﬁguration seen in Fig. 1.6.4.12(c), though degrees of curvature can be very small. This arises because the

true vibration directions of, for example, the e rays in the uniaxial case, do not lie in the plane of the ﬁgure (except at the centre). A curved surface is required for the true description of the vibration directions. We have up to this point regarded the diagram as ﬂat, but in fact the vibration directions, as we view them, become distorted into the barrel shape.

1.6.4.14. Orientation studies The full skills of the microscopist are required in the production of an accurate description of the optical orientation of a sample, that is the relationship of the indicatrix to the crystallographic axes. It is best to start by determining the crystal system. Completely isotropic crystals are cubic, uniaxial crystals are tetragonal, trigonal or hexagonal, while biaxial crystals are orthorhombic, monoclinic or triclinic. Crystallographic features such as edges, faces, crystal outlines, shapes, cleavages and twin planes give the additional information required to subdivide the uniaxial and biaxial classes. In uniaxial cases, a grain giving a centred optic axis ﬁgure is required. If the crystals look square, or have cleavages and/or twin planes intersecting at right angles, then the system is most likely to be tetragonal. Features disposed as equilateral triangles indicate triclinic, and hexagonal arrangements may indicate triclinic or hexagonal. The cases are often impossible to distinguish. Orthorhombic crystals are usually fairly easy to identify because, although biaxial, they still show parallelism between many optical and crystallographic properties. For example, vibration directions commonly lie parallel to the traces of cleavage planes or crystal outlines (so-called straight extinction). Alternatively, vibration directions may bisect the angles between such features (symmetrical extinction). Furthermore, crystals with obviously special orientations can be identiﬁed, e.g. a section showing two sharply deﬁned cleavages (i.e. lying at right angles to the plane of the slide) perhaps at right angles to each other, or producing a diamond pattern, is obviously cut normal to an important crystallographic direction, perhaps containing two of the crystallographic axes. The interference ﬁgure of such a section should be examined carefully as it is likely to be a centred version of the acute bisectrix, obtuse bisectrix or ﬂash ﬁgure. Monoclinic crystals are extremely common, and, while biaxial, do not generally show the parallelism of optical and crystallographic features typical of the orthorhombic system. There is no general recipe for success in determining the optical orientation of such crystals, other than systematic observation of crystals in different orientations. The most important observations are the relationships between extinction positions and crystallographic features, and the nature of the interference ﬁgures. All monoclinic crystals have one plane that, if at right angles to the slide, shows symmetrical or straight extinction. This plane is observed when the twofold symmetry axis lies in the plane of the slide. In crystals that show two cleavages, their intersection is also likely to mark a crystallographic axis. From consideration of such features it is often possible to identify a crucial special section, that lying perpendicular to the twofold axis. This is an important section, because two crystallographic axes now lie in the plane of the slide and their directions may be indicated by cleavage traces, crystal edges etc. Determination of the angles between vibration directions and supposed crystallographic axis directions then gives the important angle (e.g. n , c) which expresses the tilt of the indicatrix within the plane normal to the twofold axis. If everything fails, and no relationship can be found between crystallographic and optical directions, the crystal is probably triclinic, and it is not possible to say very much about its orientation using the ﬂat-stage microscope. Recourse must then be had

168

1.6. CLASSICAL LINEAR CRYSTAL OPTICS to the universal stage, a device that allows rotation of the slide in three dimensions. This is rarely done these days. Orientation studies are completed by assigning speciﬁc axes of the indicatrix to speciﬁc crystallographic axes. The identiﬁcation of the principal axes of the indicatrix is easy. For example, in uniaxial cases, sections showing maximum birefringence contain the unique crystallographic axis, which is parallel to the ne direction. Knowledge of the optic sign shows which of the two vibration directions coincides with ne , on the basis of being fast or slow. In biaxial cases, the maximum birefringence section has n and n lying in the plane of the slide, and of these n corresponds of course to the slow ray. In biaxial crystals, the identiﬁcation of the optic axial plane direction in a ﬁgure enables immediate identiﬁcation of the n direction, which is normal to it. 1.6.4.15. Absorption colours Many crystalline substances are coloured in transmitted light under the microscope, as a result of the absorption of certain visible-light wave bands. Though there may be much variability between one sample of a substance and another, colour is nevertheless often a great aid in identiﬁcation. Absorption, like other optical phenomena, is capable of showing marked anisotropy, the phenomenon known as pleochroism. Pleochroism is usually obvious in both grain mounts and thin sections, because grains change colour when rotated in plane-polarized light. The effect can be subtle (e.g. the mineral hypersthene is almost colourless in thin sections but often shows pleochroism from a very faint pink to a very faint green), or very marked (e.g. dark brown to colourless or pale yellow in the mineral biotite). The full description of pleochroism involves the assigning of different colours to speciﬁc axes of the indicatrix. Uniaxial crystals are dichroic, that is, two colours describe the effects. Sections showing centred optic axis ﬁgures do not exhibit pleochroism, showing only the pure absorption colours of light vibrating normal to the optic axis (no ). In biotite for example (which is for practical purposes uniaxial), this colour is usually dark brown. Maximum birefringence sections, or those showing centred ﬂash ﬁgures in grain mounts, show maximum pleochroism, one vibration direction exhibiting the no absorption already noted, and the other the pure effects of absorption on ne (in the case of biotite, colourless to pale yellow). Random sections show less pleochroism, and colours that are combinations of the pure end members. Biaxial crystals can be notably trichroic, and colours are readily assigned by looking at maximum birefringence (ﬂash ﬁgure) sections to obtain n (fast ray) and n (slow ray) absorptions, and optic axis sections to obtain that for n . The other notable thing about absorption colours is that they can occasionally severely mask polarization colours. Once this is appreciated, the use of the sensitive-tint plate is often sufﬁcient to identify the latter. 1.6.4.16. Dispersion Dispersion, that is to say variation of refractive index depending on wavelength, is a common phenomenon in crystals, and occasionally an important aid in identiﬁcation. In extreme cases, it results in the production of highly anomalous polarization colours, often browns, blue greys or brownish purples, or bright colours which just look slightly unusual compared with normal second- or third-order colours. Anomalous colours are highly diagnostic of certain substances (e.g. the minerals chlorite, zoisite and epidote). Dispersion also results in a lack of deﬁnition of extinction positions, because in biaxial crystals there may effectively be differently oriented indicatrices for different wavelengths. In extreme cases, it may be impossible to locate the extinction position with any accuracy. As an example of a milder case, the very common mineral plagioclase (triclinic) shows subtle, though

highly characteristic, features between crossed polars in sections cut approximately normal to the b crystallographic axis. The normal polarization colours seen in between the extinction positions are pure ﬁrst-order greys and whites, but as a grain is rotated slowly through an extinction position the colours darken and take on a bluish (cold) tinge before going black, and then lighten again with a yellowish (warm) tinge. This is the result of a slight mismatch of the orientations of the indicatrices for long and short wavelengths. Such dispersion is also often obvious (at least, when looked for) in the interference ﬁgures of biaxial crystals. Isogyres become edged with ‘cold’ (i.e. bluish) and ‘warm’ (tending to red or orange) fringes on opposite sides, indicating that optic axes for different wavelengths have slightly different positions. Dispersion is a difﬁcult phenomenon to investigate fully with the polarizing microscope. In cubic crystals, it can only be studied systematically by the determination of refractive indices using a number of monochromatic light sources of different wavelengths. Uniaxial crystals can show anomalous polarization colours, but they do not show fringes in interference ﬁgures, nor vagueness in extinction position, because the indicatrices for different wavelengths all have the same orientation. Like cubic crystals, however, the dispersion can be investigated by monochromatic light studies of refractive index. Biaxial crystals present the most complex cases. Not only can the shape of the indicatrix vary with wavelength (i.e. the relative values of the principal refractive indices), but so can orientation relative to the crystallographic axes. There are even substances known (admittedly with small 2V) in which the optic axial plane for red light is at right angles to the optic axial plane for violet light. The phenomenon is known as ‘crossed axial plane dispersion’, a real challenge for the microscopist.

1.6.5. Optical rotation 1.6.5.1. Introduction Optical rotation or gyration, as it is sometimes known, was ﬁrst recorded by Arago in 1811. Since then, a great deal of work has been done to try to explain this phenomenon, and at the present time it is one of the few physical properties of a crystal that can be successfully understood in terms of the underlying crystal structure (Glazer & Stadnicka, 1986). Lowry (1935) has given a good historical account of the subject. Optical rotation is the phenomenon observed in some crystals (and in some solutions of, usually, organic compounds) of the rotation of plane-polarized light on passing through the crystal. If the rotation, as seen by the observer, is to the left or counterclockwise it is known as laevorotation; if to the right or clockwise it is known as dextrorotation. A crystal that shows this effect is sometimes called optically active or gyrotropic. It is therefore clear that, from a symmetry point of view, optical rotation can only occur in a crystal in which one direction is not equivalent to its opposite, i.e. there are no inversion symmetry operations that can change chirality. One of the earliest theories to explain the origin of optical rotation was given by Fresnel. This was based on the idea that a plane-polarized wave can be equally described by two opposing circularly polarized waves propagating along the same direction. In Fig. 1.6.5.1(a), the polarization vector OA is simply given by the vector sum of OB and OC, polarization vectors at some instant of time belonging to a right-circular and a left-circular wave, respectively. Here it is assumed that the light propagates in a direction towards the viewer. If the light now passes through a gyrotropic material, one of the circularly polarized waves will be slowed down with respect to the other (this corresponds to having a small difference in refractive indices for the two waves). Thus on emerging from the crystal, there will be a phase difference between the circular waves, so that on recombining, the resulting

169

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES

Fig. 1.6.5.1. Fresnel’s explanation of optical rotation.

plane of linear polarization OA will have rotated through an angle ’. This is shown in Fig. 1.6.5.1(b), where the right-circular (clockwise) component travels faster than the left-circular (anticlockwise) component. Because of this, in a given time, the electric vector for the right-circular wave, observed in a ﬁxed plane perpendicular to the line of sight, will have rotated through a larger angle clockwise than the electric vector for the leftcircular wave will have rotated anticlockwise. The result is a net rotation to the right, i.e. dextrorotation, of the vector OA. The left and right-circular refractive indices, nL and nR , are inversely related to the velocities of the waves, and so Fig. 1.6.5.1(b) corresponds to the case where nL > nR. Thus this theory shows that a positive value of nL nR deﬁnes dextrorotation and that optical rotation is in fact a form of circular birefringence. Fig. 1.6.5.2 illustrates in a more generalized way the nature of the birefringences possible in a crystal. Formally, the refractive index of a medium can be written in terms of real and imaginary components: n ¼ n0 þ in00 ;

ð1:6:5:1Þ

the imaginary component referring to the absorption of the light (the real and imaginary terms are related as usual by the Kramers–Kronig relationship). Similarly, the linear and circular birefringences can also be written in real and imaginary terms: nlinear ¼ ðn1 n2 Þ0 þ iðn1 n2 Þ00 ncircular ¼ ðnL nR Þ0 þ iðnL nR Þ00 :

ð1:6:5:2Þ

The real linear birefringence (a) shows a resonance, changing sign, at a particular wavelength. Its variation with wavelength is known as birefringent dispersion. The imaginary component (b) peaks at this wavelength and corresponds to the difference in absorption between linear polarization states. This is called linear dichroism (LD) and is determined by quantum-mechanical selection rules resulting from matrix elements of the type ^ 0 i, where p^ is the electric dipole operator. The circular h1 jpj components follow similar behaviour. The real circular birefringence (c) corresponds to the optical rotation and its change with wavelength is known as optical rotatory dispersion (ORD). The imaginary circular birefringence (d) corresponds to the difference in absorption of opposite circularly polarized states. This is called circular dichroism (CD) and is determined by the matrix ^ 0 i, where ^ is the polarizability elements of the type h1 jj operator. Since ^ is an even function, whereas p^ is an odd function, the selection rules for LD and CD are different, and each type of spectrum gives different information. The link between optical rotation and crystal structure has been the subject of a great deal of work from the 18th century to date. Experimental methods for determining absolute chirality (Glazer & Stadnicka, 1989) of crystals only became routine in the late 1940s with the use of the X-ray anomalous dispersion effect,

Fig. 1.6.5.2. Real and imaginary birefringence as a function of wavelength: (a) real linear; (b) imaginary linear; (c) real circular; (d) imaginary circular.

which made it possible to determine the absolute sense of the chiral nature of a crystal and then to link this to the sense of optical rotation. However, despite the preponderance of a great many complex theories, until recently, experimental evidence to support these theories has been fragmentary. It was shown by Glazer & Stadnicka (1986) that, at least for inorganic crystals, the problem lay in mistakes in the experiments or publications describing the experiments, rather than in the underlying theories. Once these errors are taken into account, it is possible to ﬁnd a direct link between the chiral nature of the structure and the optical rotation, which appears to work in almost all cases. It has even been possible to produce a computer program OPTACT (Devarajan & Glazer, 1986; Glazer, 2002), using a polarizability theory based on earlier work by Born (1933), that is capable of calculating both the sign and magnitude of the effect with reasonable precision in many cases. OPTACT also calculates the refractive indices with good reliability. 1.6.5.2. The dielectric tensor and spatial dispersion The relevant polarization term to consider here is P!i ¼ !0 ij‘ r‘ E!j :

ð1:6:5:3Þ

The important part of this expression is the use of the ﬁeld gradient, which implies a variation of the electric ﬁeld across the unit cell of the crystal rather than the assumption that E is everywhere constant. This variation in E is known as spatial dispersion (Agranovich & Ginzburg, 1984). Assume propagation of a plane wave given by E ¼ Eo expðik rÞ through an optically active crystal. Substituting into the expression for the polarization gives P!i ¼ i!0 ij‘ E!j k‘ :

ð1:6:5:4Þ

This term can now be treated as a perturbation to the dielectric tensor "ij ð!Þ to form the effective dielectric tensor "ij ð!; kÞ:

170

"ij ð!; kÞ ¼ "ij ð!Þ þ iij‘ k‘ ;

ð1:6:5:5Þ

1.6. CLASSICAL LINEAR CRYSTAL OPTICS where ij‘ has been written for the susceptibility ij‘ in order to distinguish it from the use of elsewhere. Note that this can be expressed more generally as a power-series expansion in the vector k (Agranovich & Ginzburg, 1984) to allow for a generalization to include all possible spatial dispersion effects: "ij ð!; kÞ ¼ "ij ð!Þ þ iij‘ ð!Þk‘ þ ij‘m ð!Þk‘ km ;

ð1:6:5:6Þ

where the susceptibilities are in general themselves dependent on frequency.

The operation G E can also be represented by the product of an antisymmetric tensor ½G with the vector E: 1 10 1 0 0 G12 E2 þ G13 E3 E1 0 G12 G13 C CB C B B 0 G23 [email protected] E2 A ¼ @ G23 E3 G12 E1 A @ G12 G13 G23 0 E3 G13 E1 G23 E2 0 1 G3 E2 þ G2 E3 B C ¼ @ G1 E3 þ G3 E1 A; G2 E1 þ G1 E2

1.6.5.3. Symmetry of effective dielectric tensor To determine the symmetry constraints on the effective dielectric tensor, it should be recognized that the application of a real electric ﬁeld E must lead to a real dielectric displacement D. This therefore implies that one can write

where G1 ¼ G23 ¼ G32, G2 ¼ G13 ¼ G31 and G3 ¼ G12 ¼ G21 . If s^ is the unit vector in the propagation direction, then

"ij ð!; kÞ ¼ "ij ð! ; k Þ

G ¼ G^s

ð1:6:5:15Þ

ð1:6:5:16Þ

and G represents the magnitude of the gyration vector. Thus,

or

"ij ð! ; k Þ ¼

"ij ð!; kÞ:

s^ G ¼ s^ G^s ¼ G^s s^ ¼ G:

ð1:6:5:7Þ

ð1:6:5:17Þ

Furthermore, in the absence of any absorptive processes, "ij must be Hermitian, that is

Consequently, if one knows the direction of propagation inside the crystal, the coefﬁcient G can be calculated via

"ij ð!; kÞ ¼ "ji ð!; kÞ:

G ¼ s^1 G1 þ s^2 G2 þ s^3 G3

ð1:6:5:8Þ

This is fulﬁlled by the following symmetry constraints for the leading terms in the effective dielectric tensor: "ij ð!Þ ¼ "ji ð!Þ;

ij‘ ð!Þ ¼ ji‘ ð!Þ;

In a gyrotropic crystal, there must be at least one direction that is not equivalent to its opposite, and so such a crystal cannot have a centre of symmetry. (Only a noncentrosymmetric crystal can be gyrotropic. However, it is true to say that all nongyrotropic crystals must be centrosymmetric.) Therefore, for a non-gyrotropic crystal, "ij ð!; kÞ ¼ "ij ð!; kÞ:

ð1:6:5:10Þ

It follows therefore in such a case that ij‘ ð!Þ ¼ 0:

ð1:6:5:11Þ

It is obvious then that the susceptibility ij‘ ð!Þ has the required symmetry for gyration and that it forms an antisymmetric tensor of rank 3 (see Section 1.1.4.5.3 for the properties of antisymmetric tensors). 1.6.5.4. Gyration tensor It is convenient to rewrite the effective dielectric expression in the following way (just keeping the ﬁrst two terms): "ij ð!; kÞ ¼ "ij ð!Þ þ i^eijm gm‘ kl ;

ð1:6:5:12Þ

where e^ ijm is a unit antisymmetric pseudotensor of rank 3 or permutation tensor (^e123 ¼ 1, e^ 213 ¼ 1, e^ 112 ¼ 0 etc.; e^ ijm is not affected by mirror reﬂection) and gm‘ represents a pseudotensor (i.e. axial tensor) of rank 2. One can then write further "ij ð!; kÞ ¼ "ij ð!Þ þ i^eijm Gm ;

and then the optical rotatory power is deﬁned as ¼

ij‘m ð!Þ ¼ ji‘m ð!Þ: ð1:6:5:9Þ

ð1:6:5:13Þ

where Gm ¼ gm‘ k‘ is a component of a pseudovector (i.e. axial vector), known as the gyration vector. The formula for the dielectric displacement can then be expressed in the form Di ¼ "o "ij ð!; kÞEj ¼ "o "ij ð!ÞEj iðG EÞi : ð1:6:5:14Þ

ð1:6:5:18Þ

G ; n

ð1:6:5:19Þ

where is the angle of rotation in degrees per millimetre. According to the way in which the sign of G has been deﬁned here, a positive value of means dextrorotation and a negative value means laevorotation. There is a possibility of confusion here in terminology with respect to the term ‘gyration tensor’. It is seen that there exists an antisymmetric tensor ½G: this is sometimes referred to as the gyration tensor. However, returning to equation (1.6.5.12), it is the pseudotensor given by gm‘ that is more often described as the gyration tensor. The difference between them is really one of emphasis. The ½G tensor refers to the polarization directions of the wave, whereas the g tensor is referred to the direction of wave propagation. Thus, for example, G23 refers to a wave whose polarization lies in the x2 x3 plane, and so propagates in the x1 direction, according to the axial gyration vector component G1 . The gyration is equally described by the tensor component g11 . Being an axial tensor, g11 corresponds to a wave travelling along x1 , along which direction one observes a rotation in the x2 x3 plane. Although g is in general an antisymmetric tensor, since it is only the scalar products gm‘ s^m s^‘ that are important in determining the rotation of the plane of polarization, the components of D, and hence the refractive index behaviour, are independent of the antisymmetric part of gm‘. It is thus possible to construct a table of tensor invariances for the symmetric part of the gyration tensor with regard to the possible symmetry classes of a crystal (Table 1.6.5.1). For a discussion of the importance of the antisymmetric terms, see Agranovich & Ginzburg (1984). 1.6.5.5. Optical rotation along the optic axis of a uniaxial crystal Consider a uniaxial crystal such as quartz, crystallizing in point group 32. In this case, the only dielectric tensor terms (for the effect of symmetry, see Section 1.1.4.10) are "11 ¼ "22 6¼ "33, with the off-diagonal terms equal to zero. The equations for the dielectric displacements along the three coordinate axes x1, x2 and x3 are then given, according to equations (1.6.5.14) and (1.6.5.15), by

171

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.6.5.1. Symmetry constraints (see Section 1.1.4.10) on the gyration tensor gij All gij components are zero for the centrosymmetric point groups plus 4mm, 43m, 3m, 6mm, 6 and 6m2. Triclinic

Monoclinic Point group 2 (2 k x2 )

Point group 1 0

g12 g22 g23

g11 @ g12 g13

Orthorhombic

1

0

g11 @ 0 g13

g13 g23 A g33

0 g22 0

Point group m (m ? x2 ) 0

1

0 @ g12 0

g13 0 A g33

Point group 2 (2 k x3 ) 0

g11 @ g12 0

g12 g22 0

Tetragonal

g11 @ 0 0

0 g11 0

0

1

0

1 0 0 A g33

@

g13

g11 @ g12 0

0 0 A g33

g12 g11 0

0 0A 0

0

g11 @ 0 0

0 g11 0

Point group 42m 0

g11 @ 0 0

0 g11 0

n2

ð1:6:5:20Þ

which gives ð1:6:5:24Þ

This results in two eigenvalue solutions, n1 and n2 , from which one has

and thus

0 @ g12 0

g12 0 0

1 0 0A 0

Cubic and isotropic Point groups 432, 23 0

g11 @ 0 0

0 g11 0

1 0 0 A g11

0 g11 0

ð1:6:5:25Þ

1 0 0 A g11

G12 G ¼ 3: n n

ð1:6:5:26Þ

The optical rotatory power (1.6.5.19) is then given by ¼

G3 ðn2 n1 Þ : ¼ n

ð1:6:5:27Þ

Note that in order to be consistent with the deﬁnition of rotatory power used here, n2 > n1 for a dextrorotatory solution. This implies that n2 should be identiﬁed with nL and n1 with nR . To check this, ﬁnd the eigenvectors corresponding to the two solutions (1.6.5.24). For n21 ¼ "11 G3 , the following matrix is found from (1.6.5.21): G3 iG3 ¼ 0; ð1:6:5:28Þ iG3 G3

ð1:6:5:22Þ

can be ignored, as one normally deals with a transverse electric ﬁeld in the normal case of propagating light. For a non-trivial solution, then, "11 n2 iG12 ¼ 0; ð1:6:5:23Þ iG "11 n2 12

ðn1 n2 Þðn1 þ n2 Þ ¼ 2G12 ¼ 2G3

0

1 g13 g23 A 0

n1 n2 ¼

As usual, the longitudinal solution given by

n2 ¼ "11 G12 :

0 0 A g33

1 0 0 A g33

0 g22 0

Point group mm2

g11 @ 0 0

E3

iG13 E1 þ iG23 E2 þ "33 E3 ¼ 0

1

g11 @ 0 0

0

If the light is taken to propagate along x3 , the optic axis, the fundamental optics equation (1.6.3.14) is expressed as 0 10 1 "11 iG12 iG13 E1 B CB C "11 iG23 [email protected] E2 A @ iG12 iG13 iG23 "33 þ n2 E3 0 2 10 1 E1 n 0 0 B CB C 2 ð1:6:5:21Þ ¼@ 0 n 0 [email protected] E2 A: 0

0 g23

Point group 222 0

Isotropic, no centre of symmetry

1 0 0A 0

D1 ¼ "o "11 E1 i"o G12 E2 þ G13 E3 D2 ¼ "o "22 E2 i"o G23 E3 G21 E1 D3 ¼ "o "33 E3 i"o G31 E1 G32 E2 :

0

0

Point groups 3, 32, 6, 622 1

0 g23 A 0

Point group m (m ? x3 )

Trigonal and hexagonal Point group 4

Point groups 4, 422 0

g12 0 g23

1

giving the Jones matrix 1 ð1=2 Þ ¼ 0: i 1=2

ð1:6:5:29Þ

This corresponds to a right-circularly polarized wave. It should be noted that there is confusion in the optics textbooks over the Jones matrices for circular polarizations. Jones (1948) writes a right-circular wave as 1 ; i but this is for a deﬁnition of right-circularly polarized light as that for which an instantaneous picture of the space distribution of its electric vector describes a right spiral. The modern usage is to deﬁne the sense of circular polarization through the time variation of the electric vector in a given plane as seen by an observer

172

1.6. CLASSICAL LINEAR CRYSTAL OPTICS looking towards the source of the light. This reverses the deﬁnition given by Jones. For n22 ¼ "11 þ G3 , the following matrix is found: G3 iG3 ¼ 0; ð1:6:5:30Þ iG3 G3 giving

Fig. 1.6.5.3. The principle of superposition.

1 ð1=21=2 Þ ¼ 0: i

0

ð1:6:5:31Þ

This corresponds to a left-circularly polarized wave. Therefore it is proved that the optical rotation arises from a competition between two circularly polarized waves and that in equation (1.6.5.26) n1 ¼ nR and n2 ¼ nL , the refractive indices for rightand left-circularly polarized light, respectively. Note that Fresnel’s original idea of counter-rotating circular polarizations ﬁts nicely with the eigenvectors rigorously determined in (1.6.5.29) and (1.6.5.31). Thus ðnL nR Þ : ¼

s^1 ¼ 0;

s^2 ¼ 0;

s^3 ¼ 1

ð1:6:5:33Þ

iG12

B @ iG12 iG13 0 2 n B ¼@ 0

0 n2

0

0

iG13

10

E1

1

CB C iG23 [email protected] E2 A E3 "33 10 1 E1 0 CB C 0 [email protected] E2 A: E3 n2

"11 iG23

Solving for the non-trivial transverse solutions "11 n2 iG23 ¼0 iG "33 n2 23

ð1:6:5:32Þ

Finally, for light propagating along x3 in quartz, one can write the direction of the wave normal as

"11 n2

ð1:6:5:36Þ

ð1:6:5:37Þ

and then n4 n2 ð"11 þ "33 Þ þ "11 "33 G223 ¼ 0:

ð1:6:5:38Þ

Finding the roots of this equation considered as a quadratic in n2 , the following birefringence is obtained: 1=2 ð1:6:5:39Þ n1 n2 ¼ ðno ne Þ2 þðG223 =n 2 Þ :

and then the gyration vector is given by G ¼ gi3 s^i s^3 ¼ g13 þ g23 þ g33 ¼ g33

ð1:6:5:34Þ

as g12 ¼ g23 ¼ 0 in point group 32. Thus from (1.6.5.26) it is seen that g33 ¼ G3 ¼ G12 ;

ð1:6:5:35Þ

thus linking one of the components of the gyration tensor gm‘ with a component of the gyration vector G and a tensor component of ½G.

The eigenvectors for the two solutions n1 and n2 can easily be shown to correspond to elliptical polarizations. Notice that in equation (1.6.5.39), two refractive-index solutions are obtained whose difference depends on two terms, one with respect to the linear birefringence no ne and the other to the circular birefringence represented by the gyration component G23 ¼ G1 . The refractive-index difference n1 n2 gives rise to a phase shift between the two elliptically polarized components of the light, given by ¼ ð2=Þðn1 n2 Þ;

ð1:6:5:40Þ

from which 2 ¼ ð42 =2 Þ ðno ne Þ2 þ ðG223 =n 2 Þ

1.6.5.6. Optical rotation perpendicular to the optic axis of a uniaxial crystal

¼ 2 þ ð2 Þ2 ;

ð1:6:5:41Þ

4

The magnitude of circular birefringence is typically about 10 times smaller than that of linear birefringence. For this reason, optical rotation has usually been observed only in directions where the linear birefringence is absent, such as in optic axial directions. However, it has been clear for some time that optical rotation also exists in other directions and that with specialized techniques it is even possible to measure it. The techniques (Moxon & Renshaw, 1990; Moxon et al., 1991) are complex and require very precise measuring capabilities, and therefore are generally not commonly available. Probably the best known case where optical rotation has been measured in a linearly birefringent section is that of quartz. It has been seen that it is easy to measure the rotation along the optic axial direction, since this is the direction along which the crystal looks isotropic. Szivessy & Mu¨nster (1934) measured the rotation in a direction perpendicular to the optic axis and found that its magnitude was smaller and opposite in sign to that along the optic axis of the same crystal. To see the relationship between the linear and circular birefringences, consider light travelling along x1 in quartz. The fundamental equation (1.6.3.14) then becomes

where

¼

2 G23 G1 ðn ne Þ and ¼ ¼ : o n n

ð1:6:5:42Þ

is the phase difference when there is no optical rotation and 2 is the phase difference corresponding to a normal optical rotation when there is no linear birefringence. (1.6.5.41) shows that the linear and circular terms simply add, and this is known as the principle of superposition. This reveals that an elliptical polarization is created by the simple vector addition of a linearly polarized wave to a circularly polarized wave, as indicated in Fig. 1.6.5.3. From this, the ellipticity of the polarization is given by

173

¼ tanð12Þ;

ð1:6:5:43Þ

2 :

ð1:6:5:44Þ

where tan ¼

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.6.6.1. Symmetry constraints (see Section 1.1.4.10) on the linear electro-optic tensor rij (contracted notation) Triclinic

Monoclinic

0

r11 B r21 B B r31 B B r41 B @ r51 r61

1

r12 r22 r32 r42 r52 r62

Orthorhombic Point group m (m ? x2 )

Point group 2 (2 k x2 )

Point group 1

0

0 B 0 B B 0 B B r41 B @ 0 r61

r13 r23 C C r33 C C r43 C C r53 A r63

1

r12 r22 r32 0 r52 0

0

r11 B r21 B B r31 B B 0 B @ r51 0

0 0 C C 0 C C r43 C C 0 A r63

0 B 0 B B 0 B B r41 B @ r51 0

1 r13 r23 C C r33 C C 0 C C 0 A r63

0 0 0 r42 r52 0

Tetragonal

0 B 0 B B 0 B B r41 B @ r51 0

0 B 0 B B 0 B B r41 B @ 0

0 B 0 B B 0 B B r41 B @ 0 0

r13 r23 C C r33 C C 0 C C r53 A 0

r11 B r21 B B r31 B B 0 B @ 0 r61

r12 r22 r32 0 0 r62

0 0 0 0 r52 0

1 0 0 C C 0 C C 0 C C 0 A r63

Point group mm2

1 0 0 C C 0 C C r43 C C r53 A 0

0

1

0

0 B 0 B B 0 B B 0 B @ r51 0

0 0 0 r42 0 0

1 r13 r23 C C r33 C C 0 C C 0 A 0

Trigonal 1

0 0 0 r51 r41 0

0

r13 r13 C C r33 C C 0 C C 0 A 0

0 B 0 B B 0 B B r41 B @ r51 0

Point group 42m 0

0

Point group 4

Point group 4 0

0 0 0 r42 0 r62

0

Point group m (m ? x3 )

Point group 2 (2 k x3 ) 0

Point group 222

1

r41 0

0 0 0 r51 r41 0

0

0 B 0 B B 0 B B r41 B @ 0 0

0

0 0 0 0 r41 0

r22 r22 0 r51 r41 r11

r11 B r11 B B 0 B B r41 B @ r51 r22

r13 r13 C C 0 C C 0 C C 0 A r63

Point group 32 r11 B r11 B B 0 B B r41 B @ 0 0

r13 r13 C C r33 C C 0 C C 0 A 0

Point group 3m1 (m ? x1 )

Point group 422

1 0 0 C C 0 C C 0 C C 0 A r63

0 0 0

Point group 3 1

0

1 0 0C C 0C C 0C C 0A 0

B B B B B B @

r22 r22 0 r51 0 0

0 0 0 0 r51 r22

0 0 0 0 r41 r11

1 0 0C C 0C C 0C C 0A 0

Point group 31m (m ? x2 ) 0

1 r13 r13 C C r33 C C 0 C C 0 A 0

0 0 0 r51 0 r11

r11 B r11 B B 0 B B 0 B @ r51 0

1 r13 r13 C C r33 C C 0 C C 0 A 0

Point group 4mm 0

0 B 0 B B 0 B B 0 B @ r51 0

0 0 0 r51 0 0

1 r13 r13 C C r33 C C 0 C C 0 A 0

Hexagonal

Cubic

Point group 6 0

0 B 0 B B 0 B B r41 B @ r51 0

0 0 0 r51 r41 0

1 r13 r13 C C r33 C C 0 C C 0 A 0

Point group 6 0

r11 B r11 B B 0 B B 0 B @ 0 r22

r22 r22 0 0 0 r11

1 0 0C C 0C C 0C C 0A 0

Point group 6mm 0

0 B 0 B B 0 B B 0 B @ r51 0

0 0 0 r51 0 0

1 r13 r13 C C r33 C C 0 C C 0 A 0

Point group 6m2 (m ? x1 ) 0

0 B 0 B B 0 B B 0 B @ 0 r22

r22 r22 0 0 0 0

Point group 622 0

0 B 0 B B 0 B B r41 B @ 0 0

0 0 0 0 r41 0

1 0 0C C 0C C 0C C 0A 0

Point group 62m (m ? x2 )

1 0 0C C 0C C 0C C 0A 0

0

r11 B r11 B B 0 B B 0 B @ 0 0

174

0 0 0 0 0 r11

1 0 0C C 0C C 0C C 0A 0

Point groups 43m, 23 0

0 B 0 B B 0 B B r41 B @ 0 0

0 0 0 0 r41 0

1 0 0 C C 0 C C 0 C C 0 A r41

Point group 432 0

0 B0 B B0 B B0 B @0 0

0 0 0 0 0 0

1 0 0C C 0C C 0C C 0A 0

1.6. CLASSICAL LINEAR CRYSTAL OPTICS Thus

1.6.6.2. Example of LiNbO3 tan ¼

G1 g11 ¼ : n ðno ne Þ n ðno ne Þ

ð1:6:5:45Þ

Generally speaking, the ellipticity is extremely small and difﬁcult to measure (Moxon & Renshaw, 1990). In right-handed quartz (right-handed with respect to optical rotation observed along the c axis), no = 1.544, ne = 1.553, g11 = g22 = 5.82 105 ˚ . Since the c and g33 = 12.96 105 measured at = 5100 A axis is also the optic axis, = 0 for the (0001) plane, and thus = 1 for this section [equations (1.6.5.44) and (1.6.5.43)]. This value of

= 1 means that the two waves are circular (see Section 1.6.5.5), i.e. there is no linear birefringence, only a pure rotation. In this direction, the gyration g33 means a rotation of = 29.5 mm1 [using equation (1.6.5.27)]. In a direction normal to the optic axis, from equation (1.6.5.40) one ﬁnds = 13.3 mm1. However, in this direction, the crystal appears linearly birefringent with = 110.88 mm1 [equation (1.6.5.42)]. Thus the ellipticity = 0.00209, as calculated from equations (1.6.5.44) and (1.6.5.43). In other words, the two waves are very slightly elliptical, and the sense of rotation of the two ellipses is reversed. Because of the change in sign of the gyration coefﬁcients, it is found that at an angle of 56 100 down from the optic axis = 0, meaning that waves travelling along this direction show no optical rotation, only linear birefringence. 1.6.6. Linear electro-optic effect The linear electro-optic effect, given by P!i ¼ "o ijk E!j E0k, is conventionally expressed in terms of the change in dielectric impermeability caused by imposition of a static electric ﬁeld on the crystal. Thus one may write the linear electro-optic effect as ij ¼ rijk E0k ;

In order to understand how tensors can be used in calculating the optical changes induced by an applied electric ﬁeld, it is instructive to take a particular example and work out the change in refractive index for a given electric ﬁeld. LiNbO3 is the most widely used electro-optic material in industry and so this forms a useful example for calculation purposes. This material crystallizes in point group 3m, for which the electro-optic tensor has the form (for the effect of symmetry, see Section 1.1.4.10) (with x1 perpendicular to m) 1 0 0 r22 r13 B 0 r22 r13 C C B B 0 0 r33 C C; B ð1:6:6:2Þ B 0 r51 0 C C B @ r51 0 0 A 0 0 r22 with r13 = 9.6, r22 = 6.8, r33 = 30.9 and r51 = 32.5 1012 mV1, under the normal measuring conditions where the crystal is unclamped. Calculation using dielectric impermeability tensor. Suppose, for example, a static electric ﬁeld E03 is imposed along the x3 axis. One can then write 1 0 1 1 0 0 0 r22 r13 1 r13 E03 B 2 C B 0 0 1 B r13 E03 C r22 r13 C C B C C 0 B B 0C B 3 C B 0 B 0 r33 C C¼B [email protected] 0 A ¼ B r33 E3 C: ð1:6:6:3Þ B B 4 C B 0 B 0 C r51 0 C C B C C E03 B B @ 5 A @ r51 @ 0 A 0 0 A 6 0 0 r22 0 Thus

ð1:6:6:1Þ

where the coefﬁcients rijk form the so-called linear electro-optic tensor. These have identical symmetry with the piezoelectric tensor and so obey the same rules (see Table 1.6.6.1). Like the piezoelectric tensor, there is a maximum of 18 independent coefﬁcients (triclinic case) (see Section 1.1.4.10.3). However, unlike in piezoelectricity, in using the Voigt contracted notation there are two major differences: (1) In writing the electro-optic tensor components as rij, the ﬁrst sufﬁx refers to the column number and the second sufﬁx is the row number. (2) There are no factors of 1/2 or 2. Typical values of linear electro-optic coefﬁcients are around 1012 mV1. 1.6.6.1. Primary and secondary effects In considering the electro-optic effect, it is necessary to bear in mind that, in addition to the primary effect of changing the refractive index, the applied electric ﬁeld may also cause a strain in the crystal via the converse piezoelectric effect, and this can then change the refractive index, as a secondary effect, through the elasto-optic effect. Both these effects, which are of comparable magnitude in practice, will occur if the crystal is free. However, if the crystal is mechanically clamped, it is not possible to induce any strain, and in this case therefore only the primary electro-optic effect is seen. In practice, the free and clamped behaviour can be investigated by measuring the linear birefringence when applying electric ﬁelds of varying frequencies. When the electric ﬁeld is static or of low frequency, the effect is measured at constant stress, so that both primary and secondary effects are measured together. For electric ﬁelds at frequencies above the natural mechanical resonance of the crystal, the strains are very small, and in this case only the primary effect is measured.

1 ¼ r13 E0 ¼ 2 3 ¼ r33 E0 4 ¼ 5 ¼ 6 ¼ 0:

ð1:6:6:4Þ

Since the original indicatrix of LiNbO3 before application of the ﬁeld is uniaxial, 1 1 ¼ 2 ¼ 2 no 1 3 ¼ 2 ; ð1:6:6:5Þ ne and so differentiating, the following are obtained: 2 1 ¼ 2 ¼ 3 no no 2 3 ¼ 3 ne : ne

ð1:6:6:6Þ

Thus, the induced changes in refractive index are given by n1 ¼ n2 ¼ n3 ¼

n3o r E0 2 13 3

n3e r E0 : 2 33 3

ð1:6:6:7Þ

It can be seen from this that the effect is simply to change the refractive indices by deforming the indicatrix, but maintain the uniaxial symmetry of the crystal. Note that if light is now propagated along, say, x1 , the observed linear birefringence is given by

175

ðne no Þ 12ðn3e r33 n3o r13 ÞE03 :

ð1:6:6:8Þ

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES be considered with the static ﬁeld along x3 are 113 ¼ 223 and 333 . Equation (1.6.3.14) can then be written as 0 10 1 E1 0 0 "1 þ "o 13 E03 þ n2 B CB C 0 0 "1 þ "o 13 E3 0 @ [email protected] E2 A 0 E3 0 0 "3 þ "o 33 E3 0 2 10 1 E1 n 0 0 B CB C ¼ @ 0 n2 0 [email protected] E2 A; ð1:6:6:12Þ 0

0

n2

E3

where for simplicity the Voigt notation has been used. The ﬁrst line of the matrix equation gives ð"1 þ "o 13 E03 þ n2 ÞE1 ¼ n2 E1 :

ð1:6:6:13Þ

Since only a transverse electric ﬁeld is relevant for an optical wave (plasma waves are not considered here), it can be assumed that the longitudinal ﬁeld E1 ¼ 0. The remaining two equations can be solved by forming the determinantal equation "1 þ "o 13 E03 n2 0 ¼ 0; ð1:6:6:14Þ 0 "3 þ "o 33 E03 n2 which leads to the results Fig. 1.6.6.1. (a) Symmetry elements of point group 3m. (b) Symmetry elements after ﬁeld applied along x2 . (c) Effect on circular section of uniaxial indicatrix.

If, on the other hand, the electric ﬁeld i.e. within the mirror plane, one ﬁnds

E02

ð2Þ

ð1:6:6:9Þ

ð3Þ

and since n1 ’ no and n2 ’ ne , n1 no ¼

1

0 4 A 3

ð1:6:6:10Þ

r22 E02 r22 þ

ð1:6:6:16Þ

ðn1 no Þðn1 þ no Þ ¼ "o 13 E03 and ðn2 ne Þðn2 þ ne Þ ¼ "o 33 E03 ; ð1:6:6:17Þ

containing these terms gives three eigenvalue solutions for the changes in dielectric impermeabilities: ðr222

n21 ¼ n2o þ "o 13 E03 and n22 ¼ n2e þ "o 33 E03 ; and so

4 ¼ þr51 E02 3 ¼ 5 ¼ 6 ¼ 0:

ð1Þ

ð1:6:6:15Þ

Thus

is applied along x2 ,

1 ¼ r22 E02 2 ¼ þr22 E02

Diagonalization of the matrix 0 1 0 @ 0 2 0 4

n21 ¼ "1 þ "o 13 E03 and n22 ¼ "3 þ "o 33 E03 :

"o 13 E03 " E0 and n2 ne ¼ o 33 3 : 2no 2ne

ð1:6:6:18Þ

Subtracting these two results, the induced birefringence is found: "o 13 0 1 "o 33 E3 : ð1:6:6:19Þ ðne no Þ 2 ne no Comparing with the equation (1.6.6.8) calculated for the linear electro-optic coefﬁcients, ð1:6:6:20Þ ðne no Þ 12 n3e r33 n3o r13 E03 ;

4r251 Þ1=2

þ E02 2 r22 ðr222 þ 4r251 Þ1=2 0 E2 : 2 ð1:6:6:11Þ

On calculating the eigenfunctions, it is found that solution (1) lies along x1 , thus representing a change in the value of the indicatrix axis in this direction. Solutions (2) and (3) give the other two axes of the indicatrix: these are different in length, but mutually perpendicular, and lie in the x2 x3 plane. Thus a biaxial indicatrix is formed with one refractive index ﬁxed along x1 and the other two in the plane perpendicular. The effect of having the electric ﬁeld imposed within the mirror plane is thus to remove the threefold axis in point group 3m and to form the point subgroup m (Fig. 1.6.6.1). Relationship between linear electro-optic coefﬁcients rijk and the susceptibility tensor ð2Þ ijk . It is instructive to repeat the above calculation using the normal susceptibility tensor and equation (1.6.3.14). Consider, again, a static electric ﬁeld along x3 and light propagating along x1 . As before, the only coefﬁcients that need to

one ﬁnds the following relationships between the linear electrooptic coefﬁcients and the susceptibilities ð2Þ : " " ð1:6:6:21Þ r13 ¼ o 413 and r33 ¼ o 433 : no ne

1.6.7. The linear photoelastic effect 1.6.7.1. Introduction The linear photoelastic (or piezo-optic) effect (Narasimhamurty, 1981) is given by P!i ¼ "o ijk‘ E!j S0k‘, and, like the electrooptic effect, it can be discussed in terms of the change in dielectric impermeability caused by a static (or low-frequency) ﬁeld, in this case a stress, applied to the crystal. This can be written in the form

176

0 : ij ¼ ijk‘ Tk‘

ð1:6:7:1Þ

1.6. CLASSICAL LINEAR CRYSTAL OPTICS The coefﬁcients ijk‘ form a fourth-rank tensor known as the linear piezo-optic tensor. Typically, the piezo-optic coefﬁcients are of the order of 1012 m2 N1. It is, however, more usual to express the effect as an elasto-optic effect by making use of the relationship between stress and strain (see Section 1.3.3.2), thus Tk‘ ¼ ck‘mn Smn ;

ð1:6:7:2Þ

where the ck‘mn are the elastic stiffness coefﬁcients. Therefore equation (1.6.7.2) can be rewritten in the form ij ¼ ijk‘ ck‘mn Smn ¼ pijmn Smn

ð1:6:7:3Þ

or, in contracted notation, i ¼ pij Sj ;

ð1:6:7:4Þ

where, for convenience, the superscript 0 has been dropped, the elastic strain being considered as essentially static or of low frequency compared with the natural mechanical resonances of the crystal. The pijmn are coefﬁcients that form the linear elastooptic (or strain-optic) tensor (Table 1.6.7.1). Note that these coefﬁcients are dimensionless, and typically of order 101, showing that the change to the optical indicatrix is roughly onetenth of the strain. The elasto-optic effect can arise in several ways. The most obvious way is through application of an external stress, applied to the surfaces of the crystal. However, strains, and hence changes to the refractive indices, can arise in a crystal through other ways that are less obvious. Thus, it is a common ﬁnding that crystals can be twinned, and thus the boundary between twin domains, which corresponds to a mismatch between the crystal structures either side of the domain boundary, will exhibit a strain. Such a crystal, when viewed between crossed polars under a microscope will produce birefringence colours that will highlight the contrast between the domains. This is known as strain birefringence. Similarly, when a crystal undergoes a phase transition involving a change in crystal system, a so-called ferroelastic transition, there will be a change in strain owing to the difference in unit-cell shapes. Hence there will be a corresponding change in the optical indicatrix. Often the phase transition is one going from a high-temperature optically isotropic section to a lowtemperature optically anisotropic section. In this case, the hightemperature section has no internal strain, but the lowtemperature phase acquires a strain, which is often called the spontaneous strain (by analogy with the term spontaneous polarization in ferroelectrics). 1.6.7.2. Spontaneous strain in BaTiO3 As an example of the calculation of the relationship between spontaneous strain and linear birefringence, consider the hightemperature phase transition of the well known perovskite BaTiO3. This substance undergoes a transition at around 403 K phase to the roomon cooling from its high-temperature Pm3m temperature P4mm phase. The P4mm phase is both ferroelectric and ferroelastic. In this tetragonal phase, there is a small distortion of the unit cell along [001] and a contraction along h100i compared with the unit cell of the high-temperature cubic phase, and so the room-temperature phase can be expected to have a uniaxial optical indicatrix. phase is (Table 1.6.7.1) The elasto-optic tensor for the m3m 1 0 p11 p12 p12 0 0 0 B p12 p11 p12 0 0 0 C C B B p12 p12 p11 0 0 0 C C: B ð1:6:7:5Þ B 0 0 0 p44 0 0 C C B @ 0 0 0 0 p44 0 A 0 0 0 0 0 p44

Fig. 1.6.7.1. (a) Symmetry elements of point group 43m. (b) Symmetry elements after strain applied along [110]. (c) Effect on spherical indicatrix.

Consider the low-temperature tetragonal phase to arise as a small distortion of this cubic phase, with a spontaneous strain Ss3 given by the lattice parameters of the tetragonal phase: Ss3 ¼ ½ðc aÞ=a:

ð1:6:7:6Þ

Therefore, the equations (1.6.7.4) for the dielectric impermeability in terms of the spontaneous strain component are given in matrix form as 1 0 p11 1 B C B p B 2 C B 12 C B B B 3 C B p12 C B B B C ¼ B 0 B 4C B C B B @ 5 A @ 0 0

6

p12 p11

p12 p12

0 0

0 0

p12

p11

0

0

0 0

0 0

p44 0

0 p44

0 0 1 p12 Ss3 B p Ss C B 12 3 C C B B p11 Ss3 C C B ¼B C B 0 C C B @ 0 A

0

0

0

0

10 1 0 0 C B 0 CB 0 C C CB C 0 CB Ss3 C CB C B C 0 C CB 0 C CB C 0 [email protected] 0 A p44

0

ð1:6:7:7Þ

0 so that 1 ¼ 2 ¼ p12 Ss3 3 ¼ p11 Ss3 4 ¼ 5 ¼ 6 ¼ 0:

ð1:6:7:8Þ

By analogy with equations (1.6.6.5) and (1.6.6.6), the induced changes in refractive index are then

177

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Table 1.6.7.1. Symmetry constraints on the linear elasto-optic (strain-optic) tensor pij (contracted notation) (see Section 1.1.4.10.6) Triclinic

Orthorhombic Point group 1

0

p11 B p21 B B p31 B B p41 B @ p51 p61

p12 p22 p32 p42 p52 p62

p13 p23 p33 p43 p53 p63

p14 p24 p34 p44 p54 p64

Tetragonal

p15 p25 p35 p45 p55 p65

1 p16 p26 C C p36 C C p46 C C p56 A p66

0

p11 B p21 B B p31 B B 0 B @ 0 0

p12 p22 p32 0 0 0

p13 p23 p33 0 0 0

0 0 0 p44 0

0 0 0 0 p55 0

1 0 0 C C 0 C C 0 C C 0 A p66

Point groups 2; m; 2=m ð2 k x2 Þ p11 B p21 B B p31 B B 0 B @ p51 0

p12 p22 p32 0 p52 0

p13 p23 p33 0 p53 0

0 0 0 p44 0 p64

p15 p25 p35 0 p55 0

10

0 0 C C 0 C C p46 C C 0 A p66

p11 B p21 B B p31 B B 0 B @ 0 p61

p12 p22 p32 0 0 p62

p13 p23 p33 0 0 p63

0 0 0 p44 p54 0

0 0 0 p45 p55 0

p12 p11 p31 0 0 p61

p13 p13 p33 0 0 0

0 0 0 p44 p45

p11 p12 p31 0 0 p16

p11 B p12 B B p31 B B 0 B @ 0 0

p11 B p12 B B p31 B B 0 B @ 0 0

p16 p26 C C p36 C C 0 C C 0 A p66

p12 p11 p31 0 0 0

p13 p13 p33 0 0 0

0 0 0 p44 0 0

1 p16 p16 C C 0 C C 0 C C 0 A p66

0 0 0 p45 p44 0

0

p11 B p12 B B p31 B B p41 B @ p51 p16

p12 p11 p31 p41 p51 p16

p12 p11 p31 0 0 p16

p13 p13 p33 0 0 0

0 0 0 p44 p45 0

0 0 0 p45 p44 0

1 0

p16 C p16 C C 0 C C 0 C A 0 1 2 ðp11 p12 Þ

p11 B p21 B B p12 B B 0 B @ 0 0

p12 p11 p31 0 0 0

p13 p13 p33 0 0 0

0 0 0 p44 0 0

0 0 0 0 p44 0

1 0 C 0 C C 0 C C 0 C A 0 1 ðp p Þ 11 12 2

n1 ¼ n2 ¼ n3 ¼

p12 p11 p21 0 0 0

p21 p12 p11 0 0 0

0 0 0 p44 0 0

0

p11 B p12 B B p12 B B 0 B @ 0 0

p12 p11 p12 0 0 0

p12 p12 p11 0 0 0

0 0 0 p44 0 0

ð1:6:7:9Þ

where ncub is the refractive index of the cubic phase. Thus the birefringence in the tetragonal phase as seen by light travelling along x1 is given by n3 n2 ¼

n3cub ðp11 p12 ÞSs3 : 2

1 0 0 C C 0 C C 0 C C 0 A p66

p14 p14 0 p44 p45 p15

p15 p15 0 p45 p44 p14

1 p16 C p16 C C 0 C C p51 C A p41 1 2 ðp11 p12 Þ

32 Point groups 3m; 3m; 0

p11 B p12 B B p31 B B p41 B @ 0 0

p12 p11 p31 p41 0 0

p13 p13 p33 0 0 0

p14 p14 0 p44 0 0

0 0 0 0 p44 p14

1 0 C 0 C C 0 C C 0 C A p41 1 ðp p Þ 11 12 2

0 0 0 0 p44 0

1

0 0 C C 0 C C 0 C C 0 A p44

0

p11 B p12 B B p12 B B 0 B @ 0 0

p12 p11 p12 0 0 0

p12 p13 p11 0 0 0

0 0 0 1 2 ðp11 p12 Þ 0 0

0 0 0 0 1 2 ðp11 p12 Þ 0

1 0 C 0 C C 0 C C 0 C A 0 1 2 ðp11 p12 Þ

Point groups 43m; 432; m3m

n3cub p Ss 2 12 3

n3cub p Ss ; 2 11 3

0 0 0 0 p44 0

p13 p13 p33 0 0 0

Isotropic 23 Point groups m3;

Point groups 6mm; 6m2; 622; 6=mmm 0

0

1

Cubic 6=m Point groups 6; 6;

B B B B B B @

p11 B p12 B B p31 B B 0 B @ 0 p61

Point groups 2; m; 2=m ð2 k x3 Þ

Hexagonal 0

0

Point groups 3; 3

Point groups 4mm; 42m; 422; 4=mmm

Monoclinic

0

Trigonal

4=m Point groups 4; 4;

Point groups 222, mm2, mmm

ð1:6:7:10Þ

Thus a direct connection is made between the birefringence of the tetragonal phase of BaTiO3 and its lattice parameters via the spontaneous strain. As in the case of the linear electro-optic effect, the calculation can be repeated using equation (1.6.3.14) with the susceptibilities 11 and 12 to yield the relationship c " c " ð1:6:7:11Þ p11 ¼ 1111 4o 11 ; p12 ¼ 1122 4o 12 : no no

0 0 0 0 p44 0

1 0 0 C C 0 C C 0 C C 0 A p44

wave of frequency !2 is given by P!i ¼ ijk‘ E!j 2 S!k‘1, where ! ¼ !1 !2 . However, since the sound-wave frequency is very small compared with that of the light, to all intents and purposes the change in frequency of the light ﬁeld can be ignored. The effect then of the sound wave is to produce within an acoustooptic crystal a spatially modulated change in refractive index: a beam of light can then be diffracted by this spatial modulation, the resulting optical diffraction pattern thus changing with the changing sound signal. Acousto-optic materials therefore can be used as transducers for converting sound signals into optical signals for transmission down optical ﬁbres in communications systems. Consider, for instance, a sound wave propagating along the [110] direction in gallium arsenide (GaAs), which crystallizes in point group 43m. Suppose that this sound wave is longitudinally polarized. With respect to the cube axes, this corresponds to an oscillatory shear strain S12 sinð!t kÞ, where is a distance along the [110] direction (Fig. 1.6.7.1). Then one can write ij ¼ pij12 S12 sinð!t kÞ

ð1:6:7:12Þ

or in contracted notation

1.6.7.3. The acousto-optic effect The acousto-optic effect (Sapriel, 1976) is really a variant of the elasto-optic effect, in that the strain ﬁeld is created by the passage of a sound wave through the crystal. If this wave has frequency !1, the resulting polarization in the presence of a light

i ¼ pi6 S6 sinð!t kÞ:

ð1:6:7:13Þ

From Table 1.6.7.1, it seen that the change in dielectric impermeability tensor is

178

1.6. CLASSICAL LINEAR CRYSTAL 6 ¼ p66 S6 sinð!t kÞ ¼ p44 S6 sinð!t kÞ ð1:6:7:14Þ ijk‘ since all other components are zero. This means that the original rijk spherical indicatrix of the cubic crystal has been distorted to form s^ a biaxial indicatrix whose axes oscillate in length according to Sij T ij n3 v n1 ¼ ncub þ cub p44 S6 sinð!t kÞ 2 V n3cub ! p44 S6 sinð!t kÞ n2 ¼ ncub 2 xi n3 ¼ ncub ; ð1:6:7:15Þ thus forming an optical grating of spatial periodicity given by the k term. In gallium arsenide, at a wavelength of light equal to 1.15 mm, p11 ¼ 0:165, p12 ¼ 0:140 and p44 ¼ 0:072. It is convenient to deﬁne a ﬁgure of merit for acousto-optic materials (Yariv & Yeh, 1983) given by n6 p2 M¼ 3 ; dv

ð1:6:7:16Þ

where v is the velocity of the sound wave and d is the density of the solid. For gallium arsenide, d = 5340 kg m3, and for a sound wave propagating as above v = 5.15 m s1. At the wavelength = 1.15 mm, n = 3.37, and so it is found that M = 104. In practice, ﬁgures of merits can range from less than 0.001 up to as high as 4400 in the case of Te, and so the value for gallium arsenide makes it potentially useful as an acousto-optic material for infrared signals. 1.6.8. Glossary , , ^ Bi c ck‘mn ijk... d Di e^ ijm Ei gij , Gij G ij‘ H ij "o "ij

k o n n , n , n no ne i Pi pijk‘ p^

refractive indices of biaxial indicatrix, < < polarizability operator ith component of magnetic induction velocity of light k‘mnth component of elastic stiffness tensor ijk . . . th component of generalized susceptibility density ith component of dielectric displacement phase difference of light unit antisymmetric pseudotensor of rank 3 ith component of electric ﬁeld ijth component of gyration tensor gyration vector third-rank optical gyration susceptibility magnetic ﬁeld intensity ijth component of dielectric impermeability tensor permittivity of free space ijth component of dielectric tensor ellipticity of wave wavevector of light propagating in crystal (jkj ¼ 2=) wavelength of light vacuum magnetic permeability refractive index of light refractive indices for biaxial indicatrix, n < n < n ordinary refractive index extraordinary refractive index wavefunction of state i ith component of electric polarization ijk‘th component of elasto-optic (strain-optic) tensor electric dipole operator

OPTICS optical rotatory power ijk‘th component of linear piezo-optic tensor ijkth component of linear electro-optic tensor unit vector in the direction of s, the wave normal ijth component of strain tensor ijth component of stress tensor velocity of sound half the angle between optic axes cyclic frequency direction of ith Cartesian axis, i = 1, 2, 3

References Agranovich, V. M. & Ginzburg, V. C. (1984). Crystal optics with spatial dispersion, and excitons. Berlin: Springer. Bloss, F. D. (1961). An introduction to the methods of optical crystallography. New York: Holt, Rinehart and Winston. Born, M. (1933). Dynamische Gittertheorie der Kristalle. In Handbuch der Physik, 24, 623–794. Born, M. & Wolf, E. (1993). Principles of optics. Sixth corrected edition. Oxford: Pergamon Press. Reissued (1999) by Cambridge University Press. Bragg, W. L. (1924). The refractive indices of calcite and aragonite. Proc. R. Soc. London Ser. A, 105, 370. Butcher, P. N. & Cotter, D. (1990). The elements of nonlinear optics. Cambridge University Press. Devarajan, V. & Glazer, A. M. (1986). Theory and computation of optical rotatory power in inorganic crystals. Acta Cryst. A42, 560–569. Ewald, P. P. (1916). Zur Begru¨ndung der Kristalloptik. Ann. Phys. (Leipzig), 49, 1–38, 117–143. Glazer, A. M. (2002). WINOPTACT: a computer program to calculate optical rotatory power and refractive indices from crystal structure data. J. Appl. Cryst. 35, 652. Glazer, A. M., Lewis, J. G. & Kaminsky, W. (1996). An automatic optical imaging system for birefringent media. Proc. R. Soc. London Ser. A, 452, 2751–2765. Glazer, A. M. & Stadnicka, K. (1986). On the origin of optical activity in crystal structures. J. Appl. Cryst. 19, 108–122. Glazer, A. M. & Stadnicka, K. (1989). On the use of the term ‘absolute’ in crystallography. Acta Cryst. A45, 234–238. Groth, P. (1906–1919). Chemische Kristallographie. Vols. I-V. Leipzig: Engelmann. Hartshorne, N. H. & Stuart, A. (1970). Crystals and the polarising microscope. London: Arnold. Jona, F. & Shirane, G. (1962). Ferroelectric crystals. Oxford: Pergamon. Jones, R. C. (1948). A new calculus for the treatment of optical systems. VII. Properties of N-matrices. J. Opt. Soc. Am. 38, 671–685. Kaminow, I. P. (1974). An introduction to electro-optic devices. New York: Academic Press. Kerr, P. F. (1959). Optical mineralogy. New York: McGraw-Hill. Lines, M. E. & Glass, A. M. (1979). Principles and applications of ferroelectrics and related materials. Oxford: Clarendon. Lowry, T. M. (1935). Optical rotatory power. London: Longmans. Moxon, J. R. L. & Renshaw, A. R. (1990). The simultaneous measurement of optical activity and circular dichroism in birefringent linearly dichroic crystal sections: I. Introduction and description of the method. J. Phys. Condens. Matter, 2, 6807–6836. Moxon, J. R. L., Renshaw, A. R. & Tebbutt, I. J. (1991). The simultaneous measurement of optical activity and circular dichroism in birefringent linearly dichroic crystal sections: II. Description of the apparatus and results for quartz, nickel sulphate hexahydrate and benzil. J. Phys. D Appl. Phys. 24, 1187–1192. Narasimhamurty, T. S. (1981). Photoelastic and electro-optic properties of crystals. New York: Plenum. Nussbaum, A. & Phillips, R. A. (1976). Contemporary optics for scientists and engineers. New Jersey: Prentice Hall. Sapriel, J. (1976). Acousto-optics. Chichester: Wiley. ¨ ber die Pru¨fung der Gitteroptik bei Szivessy, G. & Mu¨nster, C. (1934). U aktiven Kristallen. Ann. Phys. (Leipzig), 20, 703–736.

179

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES Wahlstrom, E. E. (1959). Optical crystallography. New York: Wiley. Winchell, A. N. (1931). Microscopic characters of artiﬁcial inorganic solid substances or artiﬁcial minerals. New York: Wiley. [New edition (1964). New York: Academic Press.] Winchell, A. N. (1939). Elements of optical mineralogy, Part III. New York: Wiley. Winchell, A. N. (1951). Elements of optical mineralogy, Part II. New York: Wiley.

Winchell, A. N. (1954). The optical properties of organic compounds. New York: Academic Press. Winchell, A. N. (1965). Optical properties of minerals. A determinative table. New York: Academic Press. Wood, I. G. & Glazer, A. M. (1980). Ferroelastic phase transition in BiVO4. I. Birefringence measurements using the rotating-analyser method. J. Appl. Cryst. 13, 217–223. Yariv, A. & Yeh, P. (1983). Optical waves in crystals. New York: Wiley.

180

references

International Tables for Crystallography (2013). Vol. D, Chapter 1.7, pp. 181–222.

1.7. Nonlinear optical properties By B. Boulanger and J. Zyss

1.7.1. Introduction The ﬁrst nonlinear optical phenomenon was observed by Franken et al. (1961): ultraviolet radiation at 0.3471 mm was detected at the exit of a quartz crystal illuminated with a ruby laser beam at 0.6942 mm. This was the ﬁrst demonstration of second harmonic generation at optical wavelengths. A coherent light of a few W cm2 is necessary for the observation of nonlinear optical interactions, which thus requires the use of laser beams. The basis of nonlinear optics, including quantum-mechanical perturbation theory and Maxwell equations, is given in the paper published by Armstrong et al. (1962). It would take too long here to give a complete historical account of nonlinear optics, because it involves an impressive range of different aspects, from theory to applications, from physics to chemistry, from microscopic to macroscopic aspects, from quantum mechanics of materials to classical and quantum electrodynamics, from gases to solids, from mineral to organic compounds, from bulk to surface, from waveguides to ﬁbres and so on. Among the main nonlinear optical effects are harmonic generation, parametric wave mixing, stimulated Raman scattering, self-focusing, multiphoton absorption, optical bistability, phase conjugation and optical solitons. This chapter deals mainly with harmonic generation and parametric interactions in anisotropic crystals, which stand out as one of the most important ﬁelds in nonlinear optics and certainly one of its oldest and most rigorously treated topics. Indeed, there is a great deal of interest in the development of solid-state laser sources, be they tunable or not, in the ultraviolet, visible and infrared ranges. Spectroscopy, telecommunications, telemetry and optical storage are some of the numerous applications. The electric ﬁeld of light interacts with the electric ﬁeld of matter by inducing a dipole due to the displacement of the electron density away from its equilibrium position. The induced dipole moment is termed polarization and is a vector: it is related to the applied electric ﬁeld via the dielectric susceptibility tensor. For ﬁelds with small to moderate amplitude, the polarization remains linearly proportional to the ﬁeld magnitude and deﬁnes the linear optical properties. For increasing ﬁeld amplitudes, the polarization is a nonlinear function of the applied electric ﬁeld and gives rise to nonlinear optical effects. The polarization is properly modelled by a Taylor power series of the applied electric ﬁeld if its strength does not exceed the atomic electric ﬁeld (108– 109 V cm1) and if the frequency of the electric ﬁeld is far away from the resonance frequencies of matter. Our purpose lies within this framework because it encompasses the most frequently encountered cases, in which laser intensities remain in the kW to MW per cm2 range, that is to say with electric ﬁelds from 103 to 104 V cm1. The electric ﬁeld products appearing in the Taylor series express the interactions of different optical waves. Indeed, a wave at the circular frequency ! can be radiated by the second-order polarization induced by two waves at !a and !b such as ! ¼ !a !b : these interactions correspond to sumfrequency generation (! ¼ !a þ !b ), with the particular cases of second harmonic generation (2!a ¼ !a þ !a ) and indirect third harmonic generation (3!a ¼ !a þ 2!a ); the other three-wave process is difference-frequency generation, including optical parametric ampliﬁcation and optical parametric oscillation. In the same way, the third-order polarization. governs four-wave mixing: direct third harmonic generation (3!a ¼ !a þ !a þ !a ) Copyright © 2013 International Union of Crystallography

and more generally sum- and difference-frequency generations (! ¼ !a !b !c ). Here, we do not consider optical interactions at the microscopic level, and we ignore the way in which the atomic or molecular dielectric susceptibility determines the macroscopic optical properties. Microscopic solid-state considerations and the relations between microscopic and macroscopic optical properties, particularly successful in the realm of organic crystals, play a considerable role in materials engineering and optimization. This important topic, known as molecular and crystalline engineering, lies beyond the scope of this chapter. Therefore, all the phenomena studied here are connected to the macroscopic ﬁrst-, second- and third-order dielectric susceptibility tensors (1), (2) and (3), respectively; we give these tensors for all the crystal point groups. We shall mainly emphasize propagation aspects, on the basis of Maxwell equations which are expressed for each Fourier component of the optical ﬁeld in the nonlinear crystal. The reader will then follow how the linear optical properties come to play a pivotal role in the nonlinear optical interactions. Indeed, an efﬁcient quadratic or cubic interaction requires not only a high magnitude of (2) or (3), respectively, but also speciﬁc conditions governed by (1): existence of phase matching between the induced nonlinear polarization and the radiated wave; suitable symmetry of the ﬁeld tensor, which is deﬁned by the tensor product of the electric ﬁeld vectors of the interacting waves; and small or nil double refraction angles. Quadratic and cubic processes cannot be considered as fully independent in the context of cascading. Signiﬁcant phase shifts driven by a sequence of sum- and difference-frequency generation processes attached to a ð2Þ ð2Þ contracted tensor expression have been reported (Bosshard, 2000). These results point out the relevance of polar structures to cubic phenomena in both inorganic and organic structures, thus somewhat blurring the borders between quadratic and cubic NLO. We analyse in detail second harmonic generation, which is the prototypical interaction of frequency conversion. We also present indirect and direct third harmonic generations, sum-frequency generation and difference-frequency generation, with the speciﬁc cases of optical parametric ampliﬁcation and optical parametric oscillation. An overview of the methods of measurement of the nonlinear optical properties is provided, and the chapter concludes with a comparison of the main mineral and organic crystals showing nonlinear optical properties. 1.7.2. Origin and symmetry of optical nonlinearities 1.7.2.1. Induced polarization and susceptibility The macroscopic electronic polarization of a unit volume of the material system is classically expanded in a Taylor power series of the applied electric ﬁeld E, according to Bloembergen (1965): P ¼ P0 þ "o ðð1Þ E þ ð2Þ E2 þ . . . þ ðnÞ En þ . . .Þ; ð1:7:2:1Þ where (n) is a tensor of rank n þ 1, En is a shorthand abbreviation for the nth order tensor product E E . . . E ¼ n E and the dot stands for the contraction of the last n indices of the

181

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES (n)

n

tensor with the full E tensor. More details on tensor algebra can be found in Chapter 1.1 and in Schwartz (1981). A more compact expression for (1.7.2.1) is P ¼ P0 þ P1 ðtÞ þ P2 ðtÞ þ . . . þ Pn ðtÞ þ . . . ;

ð1:7:2:2Þ

where P0 represents the static polarization and Pn represents the nth order polarization. The properties of the linear and nonlinear responses will be assumed in the following to comply with time invariance and locality. In other words, time displacement of the applied ﬁelds will lead to a corresponding time displacement of the induced polarizations and the polarization effects are assumed to occur at the site of the polarizing ﬁeld with no remote interactions. In the following, we shall refer to the classical formalism and related notations developed in Butcher (1965) and Butcher & Cotter (1990). Tensorial expressions will be formulated within the Cartesian formalism and subsequent multiple lower index notation. The alternative irreducible tensor representation, as initially implemented in the domain of nonlinear optics by Jerphagnon et al. (1978) and more recently revived by Brasselet & Zyss (1998) in the realm of molecular-engineering studies, is particularly advantageous for connecting the nonlinear hyperpolarizabilities of microscopic (e.g. molecular) building blocks of molecular materials to the macroscopic (e.g. crystalline) susceptibility level. Such considerations fall beyond the scope of the present chapter, which concentrates mainly on the crystalline level, regardless of the microscopic origin of phenomena. 1.7.2.1.1. Linear and nonlinear responses 1.7.2.1.1.1. Linear response Let us ﬁrst consider the ﬁrst-order linear response in (1.7.2.1) and (1.7.2.2): the most general possible linear relation between P(t) and E(t) is þ1 R

Pð1Þ ðtÞ ¼ "o

d T ð1Þ ðt; Þ EðÞ;

ð1:7:2:3Þ

1

where T(1) is a rank-two tensor, or in Cartesian index notation Pð1Þ ðtÞ ¼ "o

þ1 R

ð1Þ d T ðt; ÞE ðÞ:

ð1:7:2:4Þ

1

¼ "o ¼ "o

þ1 R 1 þ1 R 1 þ1 R

1.7.2.1.1.2. Quadratic response The most general expression for P(2)(t) which is quadratic in E(t) is Pð2Þ ðtÞ ¼ "o

or in Cartesian notation þ1 R þ1 R

Pð2Þ ðtÞ ¼ "o

It can easily be proved by decomposition of T(2) into symmetric and antisymmetric parts and permutation of dummy variables (, 1) and (, 2), that T(2) can be reduced to its symmetric part, satisfying ð2Þ ð2Þ T ðt; 1 ; 2 Þ ¼ T ðt; 2 ; 1 Þ:

ð1:7:2:5Þ

hence T ð1Þ ðt þ t0 ; Þ ¼ T ð1Þ ðt; t0 Þ or, setting t ¼ 0 and t0 ¼ t, ð1:7:2:6Þ

T ð2Þ ðt; 1 ; 2 Þ ¼ Rð2Þ ðt 1 ; t 2 Þ; ð1:7:2:11Þ þ1 þ1 R R Pð2Þ ðtÞ ¼ "o d1 d2 Rð2Þ ðt 1 ; t 2 Þ Eð1 Þ Eð2 Þ; Pð2Þ ðtÞ ¼ "o

1 1 þ1 R þ1 R

¼ "o

þ1 R 1 þ1 R

d Rð1Þ ðt ÞEðÞ d Rð1Þ ðÞEðt Þ:

d1 d2 Rð2Þ ð1 ; 2 Þ Eðt 1 Þ Eðt 2 Þ:

1 1

ð1:7:2:12Þ Causality demands that R(2)( 1, 2) cancels for either 1 or 2 negative while R(2) is real. Intrinsic permutation symmetry implies that R(2)( 1, 2) is invariant by interchange of (, 1) and (, 2) pairs. 1.7.2.1.1.3. Higher-order response The nth order polarization can be expressed in terms of the (n þ 1)-rank tensor T ðnÞ ðt; 1 ; 2 ; . . . ; n Þ as þ1 R

d1

þ1 R

d2 . . .

1

þ1 R

dn T ðnÞ ðt; 1 ; 2 ; . . . ; n Þ

1

ð1:7:2:7Þ

1

R(1) can be viewed as the tensorial analogue of the linear impulse function in electric circuit theory. The causality principle imposes that R(1)() should vanish for < 0 so that P(1)(t) at time t will

ð1:7:2:13Þ

For similar reasons to those previously stated, it is sufﬁcient to consider the symmetric part of T(n) with respect to the n! permutations of the n pairs (1, 1), (2, 2) . . . (n, n). The T(n) tensor will then exhibit intrinsic permutation symmetry at the nth order. Time-invariance considerations will then allow the introduction of the (n þ 1)th-rank real tensor R(n), which generalizes the previously introduced R operators: PðnÞ ðtÞ ¼ "o

þ1 R 1

where R(1) is a rank-two tensor referred to as the linear polarization response function, which depends only on the time difference t . Substitution in (1.7.2.5) leads to

ð1:7:2:10Þ

From time invariance

Eð1 Þ Eð2 Þ . . . Eðn Þ:

1

Pð1Þ ðtÞ ¼ "o

ð2Þ d1 d2 T ðt; 1 ; 2 ÞE ð1 ÞE ð2 Þ: ð1:7:2:9Þ

1 1

1

d T ð1Þ ðt; þ t0 Þ EðÞ

T ð1Þ ðt; Þ ¼ T ð1Þ ð0; tÞ ¼ Rð1Þ ðt Þ;

d1 d2 T ð2Þ ðt; 1 ; 2 Þ Eð1 Þ Eð2 Þ ð1:7:2:8Þ

d T ð1Þ ðt þ t0 ; Þ EðÞ

d 0 T ð1Þ ðt; 0 t0 Þ Eð 0 Þ;

þ1 R þ1 R 1 1

PðnÞ ðtÞ ¼ "o

Applying the time-invariance assumption to (1.7.2.4) leads to Pð1Þ ðt þ t0 Þ ¼ "o

depend only on polarizing ﬁeld values before t. R(1), P(1) and E are real functions of time.

d1

þ1 R 1

d2 . . .

þ1 R 1

ðnÞ dn R ð1 ; 2 ; . . . n Þ 1 2 ...n

E1 ðt 1 ÞE2 ðt 2 Þ . . . En ðt n Þ:

ð1:7:2:14Þ

R(n) cancels when one of the i’s is negative and is invariant under any of the n! permutations of the (i, i) pairs. 1.7.2.1.2. Linear and nonlinear susceptibilities Whereas the polarization response has been expressed so far in the time domain, in which causality and time invariance are most naturally expressed, Fourier transformation into the frequency domain permits further simpliﬁcation of the equations given above and the introduction of the susceptibility tensors according to the following derivation.

182

1.7. NONLINEAR OPTICAL PROPERTIES The direct and inverse Fourier transforms of the ﬁeld are deﬁned as þ1 R

EðtÞ ¼

d! Eð!Þ expði!tÞ

ðnÞ ð! ; !1 ; !2 ; . . . ; !n Þ þ1 þ1 þ1 n R P R R d1 d2 . . . dn RðnÞ ð1 ; 2 ; . . . ; n Þ exp i !j j ¼ 1

ð1:7:2:15Þ

1

j¼1

1

ð1:7:2:21Þ

1 þ1 R

Eð!Þ ¼ ð1=2Þ

dt EðtÞ expði!tÞ;

ð1:7:2:16Þ

1

where Eð!Þ ¼ Eð!Þ as E(t) is real.

and ! ¼ !1 þ !2 þ . . . þ !n . All frequencies must lie in the upper half complex plane and reality of (n) imposes ðnÞ ð! ; !1 ; !2 ; . . . ; !n Þ ¼ ðnÞ ð! ; !1 ; !2 ; . . . ; !n Þ: ð1:7:2:22Þ

1.7.2.1.2.1. Linear susceptibility By substitution of (1.7.2.15) in (1.7.2.7), Pð1Þ ðtÞ ¼ "o Pð1Þ ðtÞ ¼ "o

þ1 R 1 þ1 R

þ1 R

d!

Intrinsic permutation symmetry implies that ðnÞ 1 2 ...n ð! ; !1 ; !2 ; . . . ; !n Þ is invariant with respect to the n! permutations of the (i, !i) pairs.

d Rð1Þ ðÞ Eð!Þ exp½i!ðt Þ

1

d! ð1Þ ð! ; !ÞEð!Þ expði! tÞ;

1

ð1:7:2:17Þ where ð1Þ ð! ; !Þ ¼

þ1 R

d Rð1Þ ðÞ expði!Þ:

1

In these equations, ! ¼ ! to satisfy the energy conservation condition that will be generalized in the following. In order to ensure convergence of (1), ! has to be taken in the upper half plane of the complex plane. The reality of R(1) implies that ð1Þ ð! ; !Þ ¼ ð1Þ ð! ; ! Þ.

1.7.2.1.3. Superposition of monochromatic waves Optical ﬁelds are often superpositions of monochromatic waves which, due to spectral discretization, will introduce considerable simpliﬁcations in previous expressions such as (1.7.2.20) relating the induced polarization to a continuous spectral distribution of polarizing ﬁeld amplitudes. The Fourier transform of the induced polarization is given by PðnÞ ð!Þ ¼ ð1=2Þ

þ1 R

d!1

1

þ1 R 1

d!2

þ1 R

d1

1

þ1 R

d!1

1

1

PðnÞ ð!Þ ¼ "o

d!2 ð2Þ ð! ; !1 ; !2 Þ Eð!1 Þ Eð!2 Þ

þ1 R

d1

þ1 R

1

þ1 R

d!n ðnÞ ð! ; !1 ; !2 ; . . . !n Þ

1

Eð!1 ÞEð!2 Þ . . . Eð!n Þð! ! Þ:

ð1:7:2:25Þ

!0

d2 Rð2Þ ð1 ; 2 Þ

The optical intensity for a wave at frequency !0 is related to the squared ﬁeld amplitude by

1

and ! ¼ !1 þ !2 . Frequencies !1 and !2 must be in the upper half of the complex plane to ensure convergence. Reality of R(2) implies ð2Þ ð! ; !1 ; !2 Þ ¼ ð2Þ ð! ; !1 ; !2 Þ. ð2Þ ð! ; !1 ; !2 Þ is invariant under the interchange of the (, !1) and (, !2) pairs.

d!2 . . .

þ1 R

I!0 ¼ "o cnð!0 ÞhE2 ðtÞit ¼ 12 "o cnð!0 ÞjE!0 j2 :

ð1:7:2:28Þ

The averaging as represented above by brackets is performed over a time cycle and nð!0 Þ is the index of refraction at frequency !0 . 1.7.2.1.4. Conventions for nonlinear susceptibilities 1.7.2.1.4.1. Classical convention Insertion of (1.7.2.26) in (1.7.2.25) together with permutation symmetry provides P P PðnÞ Kð! ; !1 ; !2 ; . . . ; !n Þ ð! Þ ¼ "o

1.7.2.1.2.3. nth-order susceptibility Substitution of (1.7.2.15) in (1.7.2.14) provides

1

d!2 . . .

with E!0 ¼ E!0 . By Fourier transformation of (1.7.2.26) P Eð!Þ ¼ ð1=2Þ ½E!0 ð! !0 Þ þ E!0 ð! þ !0 Þ: ð1:7:2:27Þ

exp½ið!1 1 þ !2 2 Þ

1

þ1 R

!0

1

þ1 R

d!1

ð1:7:2:19Þ

ð2Þ ð! ; !1 ; !2 Þ ¼

d!1

ð1:7:2:24Þ

In practical cases where the applied ﬁeld is a superposition of monochromatic waves P EðtÞ ¼ ð1=2Þ ½E!0 expði!0 tÞ þ E!0 expði!0 tÞ ð1:7:2:26Þ

with

þ1 R

þ1 R 1

1

expði! tÞ

PðnÞ ðtÞ ¼ "o

dt exp½ið! ! Þt ¼ ð! ! Þ

leads to

d2 Rð2Þ ð1 ; 2 Þ

or Pð2Þ ðtÞ ¼ "o

þ1 R 1

ð1:7:2:18Þ

þ1 R

ð1:7:2:23Þ

Replacing P(n)(t) by its expression as from (1.7.2.20) and applying the well known identity ð1=2Þ

Eð!1 Þ Eð!2 Þ expfi½!1 ðt 1 Þ þ !2 ðt 2 Þg

þ1 R

dt PðnÞ ðtÞ expði!tÞ:

1

1.7.2.1.2.2. Second-order susceptibility Substitution of (1.7.2.15) in (1.7.2.12) yields Pð2Þ ðtÞ ¼ "o

þ1 R

d!n ðnÞ ð! ; !1 ; !2 ; . . . !n Þ

1

Eð!1 Þ Eð!2 Þ . . . Eð!n Þ expði! tÞ

1 2 ...n !

ð1:7:2:20Þ

ðnÞ 1 2 ...n ð! ; !1 ; !2 ; . . . ; !n Þ E1 ð!1 ÞE2 ð!2 Þ . . . En ð!n Þ;

where

183

ð1:7:2:29Þ

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES P ðnÞ Table 1.7.2.1. The most common nonlinear effects and the corresponding 1 ...n ð! ; !1 ; . . . ; !n Þ PðnÞ ð! Þ ¼ "o susceptibility tensors in the frequency domain

1 ;...;n

Process

Order n

! ; !1 ; !2 ; . . . ; !n

K

Linear absorption Optical rectiﬁcation Linear electro-optic effect Second harmonic generation Three-wave mixing D.c. Kerr effect D.c. induced second harmonic generation Third harmonic generation Four-wave mixing Coherent anti-Stokes Raman scattering Intensity-dependent refractive index nth harmonic generation

1 2 2 2 2 3 3

!; ! 0; !; ! !; !; 0 2!; !; ! !3 ; !1 ; !2 !; !; 0; 0 2!; !; !; 0

1 1/2 2 1/2 1 3 3/2

3 3 3

3!; !; !; ! !4 ; !1 ; !2 ; !3 !as ; !p ; !p ; !s

1/4 3/2 3/4

3

!; !; !; !

3/4

n

n!; !; !; . . . ; !

21n

E 1 ð!1 Þ . . . En ð!n Þ;

where þ and refer to the eigen polarization modes. According to (1.7.2.33), the nth harmonic generation induced polarization is expressed as P ðnÞ 1 ...n ðn!; !; . . . ; !Þ PðnÞ ðn!Þ ¼ "o 1 ;...;n

E 1 ð!1 Þ . . . En ð!n Þ:

þ Pð2Þ y ð2!Þ ¼ "o ½yxz ð2!; !; !ÞEx ð!ÞEz ð!Þ

ð1:7:2:31Þ

Table 1.7.2.1 summarizes the most common classical nonlinear phenomena, following the notations deﬁned above. Then, according to Table 1.7.2.1, the nth harmonic generation induced nonlinear polarization is written P n1 ðnÞ Pð2Þ 2 1 2 ...n ðn!; !; !; . . . ; !Þ ðn!Þ ¼ "o 1 2 ...n

E1 ð!ÞE2 ð!Þ . . . En ð!Þ:

þ yzx ð2!; !; !ÞEþ z ð!ÞEx ð!Þ:

ð1:7:2:35Þ

ð1:7:2:30Þ

where p is the number of distinct permutations of !1 ; !2 ; . . . ; !n, n is the order of the nonlinear process, m is the number of d.c. ﬁelds (e.g. corresponding to ! ¼ 0) within the n frequencies and s ¼ 0 when ! ¼ 0, otherwise s ¼ 1. For example, in the absence of a d.c. ﬁeld and when the !i’s are different, K ¼ 2sn n!. The K factor allows the avoidance of discontinuous jumps in magnitude of the ðnÞ 1 2 ...n elements when some frequencies are equal or tend to zero, which is not the case for the other conventions (Shen, 1984). The induced nonlinear polarization is often expressed in terms of a tensor d(n) by replacing (n) in (1.7.2.29) by ðnÞ ¼ 2smþn dðnÞ :

ð1:7:2:34Þ

For example, in the particular case of SHG where the two waves at ! have different directions of polarization E+(!) and E(!) and where the only nonzero ð2Þ yij coefﬁcients are yxz and yzx , (1.7.2.34) gives

where the summation over ! stands for all distinguishable permutation of !1 ; !2 ; . . . ; !n, K being a numerical factor given by Kð! ; !1 ; !2 ; . . . ; !n Þ ¼ 2sþmn p;

ð1:7:2:33Þ

ð1:7:2:32Þ

The Ei are the components of the total electric ﬁeld E(!). 1.7.2.1.4.2. Convention used in this chapter The K convention described above is often used, but may lead to errors in cases where two of the interacting waves have the same frequency but different polarization states. Indeed, as demonstrated in Chapter 1.6 and recalled in Section 1.7.3, a direction of propagation in an anisotropic crystal allows in the general case two different directions of polarization of the electric ﬁeld vector, written E+ and E. Then any nonlinear coupling in this medium occurs necessarily between these eigen modes at the frequencies concerned. Because of the possible non-degeneracy with respect to the direction of polarization of the electric ﬁelds at the same frequency, it is suitable to consider a harmonic generation process, second harmonic generation (SHG) or third harmonic generation (THG) for example, like any other non-degenerated interaction. We do so for the rest of this chapter. Then all terms derived from the permutation of the ﬁelds with the same frequency are taken into account in the expression of the induced nonlinear polarization and the K factor in equation (1.7.2.29) disappears: hence, in the general case, the induced nonlinear polarization is written

The two ﬁeld component products are equal only if the two eigen modes are the same, i.e. þ or . According to (1.7.2.33) and (1.7.2.34), we note that ðnÞ ðnÞ 1 ...n ð! ; !1 ; . . . ; !n Þ changes smoothly to 1 ...n ðn!; !; . . . ; !Þ when all the !1 ; . . . !n approach continuously the same value !. 1.7.2.2. Symmetry properties 1.7.2.2.1. Intrinsic permutation symmetry 1.7.2.2.1.1. ABDP and Kleinman symmetries Intrinsic permutation symmetry, as already discussed, imposes the condition that the nth order susceptibility ðnÞ 1 2 ...n ð! ; !1 ; !2 ; . . . ; !n Þ be invariant under the n! permutations of the (i ; !i ) pairs as a result of time invariance and causality. Furthermore, the overall permutation symmetry, i.e. the invariance over the ðn þ 1Þ! permutations of the (i ; !i ) and (; ! ) pairs, may be valid when all the optical frequencies occuring in the susceptibility and combinations of these appearing in the denominators of quantum expressions are far removed from the transitions, making the medium transparent at these frequencies. This property is termed ABDP symmetry, from the initials of the authors of the pioneering article by Armstrong et al. (1962). Let us consider as an application the quantum expression of the quadratic susceptibility (with damping factors neglected), the derivation of which being beyond the scope of this chapter, but which can be found in nonlinear optics treatises dealing with microscopic interactions, such as in Boyd (1992): ð2Þ ð! ; !1 ; !2 Þ X Ne3 rab rbc rca ;

o ðaÞ ¼ 2 - 2 ST ðba !1 !2 Þðca !1 Þ "h o

abc

ð1:7:2:36Þ where N is the number of microscopic units (e.g. molecules in the case of organic crystals) per unit volume, a, b and c are the eigen states of the system, ba and ca are transition energies, rab is the component of the transition dipole connecting states a and b, and o ðaÞ is the population of level a as given by the corresponding diagonal term of the density operator. ST is the summation operator over the six permutations of the (; ! ), (; !1 ), (; !2 ). Provided all frequencies at the denominator are much smaller than the transition frequencies ba and ca, the optical frequencies !, !1 , !2 can be permuted without signiﬁcant variation of the susceptibility. It follows correspondingly that the susceptibility is invariant with respect to the

184

1.7. NONLINEAR OPTICAL PROPERTIES permutation of Cartesian indices appearing only in the numerator of (1.7.2.36), regardless of frequency. This property, which can be generalized to higher-order susceptibilities, is known as Kleinman symmetry. Its validity can help reduce the number of non-vanishing terms in the susceptibility, as will be shown later. 1.7.2.2.1.2. Manley–Rowe relations An important consequence of overall permutation symmetry is the Manley–Rowe power relations, which account for energy exchange between electromagnetic waves in a purely reactive (e.g. non-dissipative) medium. Calling Wi the power input at frequency !i into a unit volume of a dielectric polarizable medium, dP ðtÞ ; ð1:7:2:37Þ Wi ¼ EðtÞ dt where the averaging is performed over a cycle and EðtÞ ¼ Re½E!i expðj!i tÞ PðtÞ ¼ Re½P!i expðj!i tÞ:

ð1:7:2:38Þ

The following expressions can be derived straightforwardly: Wi ¼ 12 !i ReðiE!i P!i Þ ¼ 12 !i ImðE!i P!i Þ:

ð1:7:2:39Þ

Introducing the quadratic induced polarization P(2), Manley– Rowe relations for sum-frequency generation state W1 W2 W ¼ ¼ 3: ð1:7:2:40Þ !1 !2 !3

contracted tensor notation with the following contraction convention: for : x ! 1 y ! 2 z ! 3 for m: xxx ! 1 yyy ! 2 zzz ! 3 xzz ! 6

yz ¼ zy ! 4

xy ¼ yx ! 6:

þ ¼ "o 25 ð2!; !; !Þ½eþ x ð!ÞE ð!Þez ð!ÞE ð!Þ þ þ eþ z ð!ÞE ð!Þex ð!ÞE ð!Þ:

xyz ! 0:

Table 1.7.2.2. Nonzero (2) coefﬁcients and equalities between them in the general case Symmetry class

(2) nonzero elements

Triclinic C1 (1)

All 27 elements are independent and nonzero

Monoclinic C2 (2) (twofold axis parallel to z) Cs (m) (mirror perpendicular to z)

xyz, xzy, xxz, xzx, yyz, yzy, yxz, yzx, zxx, zyy, zzz, zxy, zyx xxx, xyy, xzz, xxy, xyx, yxx, yyy, yzz, yxy, yyx, zyz, zzy, zxz, zzx

Orthorhombic C2v (mm2) (twofold axis parallel to z) D2 (222) Tetragonal C4 (4) S4 (4) D4 (422) C4v (4mm) D2d (42m) Hexagonal C6 (6) C3h (6) D6 (622) C6v (6mm) (mirror D3h (62m) perpendicular to x) Trigonal C3 (3)

The 27 elements of ð2Þ ð2!; !; !Þ are then reduced to 18 in the m contracted tensor notation (see Section 1.1.4.10). For example, (1.7.2.35) can be written Pð2Þ y ð2!Þ

xxy ! 9

1.7.2.2.2. Implications of spatial symmetry on the susceptibility tensors Centrosymmetry is the most detrimental crystalline symmetry constraint that will fully cancel all odd-rank tensors such as the d(2) [or (2)] susceptibilities. Intermediate situations, corresponding to noncentrosymmetric crystalline point groups, will reduce the number of nonzero coefﬁcients without fully depleting the tensors. Tables 1.7.2.2 to 1.7.2.5 detail, for each crystal point group, the remaining nonzero (2) and (3) coefﬁcients and the eventual connections between them. (2) and (3) are expressed in the principal axes x, y and z of the second-rank (1) tensor. (x; y; z) is usually called the optical frame; it is linked to the crystal-

1.7.2.2.1.3. Contracted notation for susceptibility tensors ð2Þ The tensors ð2!; !; !Þ or dð2Þ ð2!; !; !Þ are invariant with respect to (, ) permutation as a consequence of the intrinsic permutation symmetry. Independently, it is not possible ð2Þ to distinguish the coefﬁcients ijk ð2!; !; !Þ and ð2Þ ikj ð2!; !; !Þ by SHG experiments, even if the two fundamental waves have different directions of polarization. Therefore, these third-rank tensors can be represented in contracted form as 3 6 matrices m ð2!; !; !Þ and dm ð2!; !; !Þ, where the sufﬁx m runs over the six possible (, ) Cartesian index pairs according to the classical convention of contraction:

xz ¼ zx ! 5

xyy ! 8

yyz ! 5

If Kleinman symmetry holds, the contracted tensor can be further extended beyond SHG and THG to any other processes where all the frequencies are different.

Since !1 þ !2 ¼ !3, (1.7.2.40) leads to an energy conservation condition, namely W3 þ W1 þ W2 ¼ 0, which expresses that the power generated at !3 is equal to the sum of the powers lost at !1 and !2. A quantum mechanical interpretation of these expressions in terms of photon fusion or splitting can be given, remembering that Wi =h- !i is precisely the number of photons generated or annihilated per unit volume in unit time in the course of the nonlinear interactions.

for : x ! 1 y ! 2 z ! 3 for m: xx ! 1 yy ! 2 zz ! 3

xxz ! 7

yzz ! 4

ð1:7:2:41Þ

The same considerations can be applied to THG. Then the 81 ð3Þ ð3!; !; !; !Þ can be reduced to 30 in the m elements of

185

xzx, xxz, yyz, yzy, zxx, zyy, zzz xyz, xzy, yzx, yxz, zxy, zyx

xyz ¼ yxz, xzy ¼ yzx, xzx ¼ yzy, xxz ¼ yyz, zxx ¼ zyy, zzz, zxy ¼ zyx xyz ¼ yxz, xzy ¼ yzx, xzx ¼ yzy, xxz ¼ yyz, zxx ¼ zyy, zxy ¼ zyx xyz ¼ yxz, xzy ¼ yzx, zxy ¼ zyx xzx ¼ yzy, xxz ¼ yyz, zxx ¼ zyy, zzz xyz ¼ yxz, xzy ¼ yzx, zxy ¼ zyx xyz ¼ yxz, xzy ¼ yzx, xzx ¼ yzy, xxz ¼ yyz, zxx ¼ zyy, zzz, zxy ¼ zyx xxx ¼ xyy ¼ yxy ¼ yyx, yyy ¼ yxx ¼ xyx ¼ xxy xyz ¼ yxz, xzy ¼ yzx, zxy ¼ zyx xzx ¼ yzy, xxz ¼ yyz, zxx ¼ zyy, zzz yyy ¼ yxx ¼ xxy ¼ xyx

C3v (3m) (mirror perpendicular to x)

xxx ¼ xyy ¼ yyx ¼ yxy, xyz ¼ yxz, xzy ¼ yzx, xzx ¼ yzy, xxz ¼ yyz, yyy ¼ yxx ¼ xxy ¼ xyx, zxx ¼ zyy, zzz, zxy ¼ zyx xxx ¼ xyy ¼ yyx ¼ yxy, xyz ¼ yxz, xzy ¼ yzx, zxy ¼ zyx yyy ¼ yxx ¼ xxy ¼ xyx, xzx ¼ yzy, xxz ¼ yyz, zxx ¼ zyy; zzz

Cubic T (23), Td (43m) O (432)

xyz ¼ xzy ¼ yzx ¼ yxz ¼ zxy ¼ zyx xyz ¼ xzy ¼ yzx ¼ yxz ¼ zxy ¼ zyx

D3 (32)

1. TENSORIAL ASPECTS OF PHYSICAL PROPERTIES lographical frame by the standard conventions given in Chapter 1.6. 1.7.3. Propagation phenomena 1.7.3.1. Crystalline linear optical properties We summarize here the main linear optical properties that govern the nonlinear propagation phenomena. The reader may refer to Chapter 1.6 for the basic equations. 1.7.3.1.1. Index surface and electric ﬁeld vectors The relations between the different ﬁeld vectors relative to a propagating electromagnetic wave are obtained from the constitutive relations of the medium and from Maxwell equations. In the case of a non-magnetic and non-conducting medium, Maxwell equations lead to the following wave propagation equation for the Fourier component at the circular frequency ! deﬁned by (1.7.2.15) and (1.7.2.16) (Butcher & Cotter, 1990): rxrxEð!Þ ¼ ð!2 =c2 ÞEð!Þ þ !2 0 Pð!Þ;

ð1:7:3:1Þ

where ! ¼ 2c= , is the wavelength and c is the velocity of light in a vacuum; 0 is the free-space permeability, E(!) is the electric ﬁeld vector and P(!) is the polarization vector. Table 1.7.2.3. Nonzero (2) coefﬁcients and equalities between them under the Kleinman symmetry assumption Symmetry class Triclinic C1 (1)

Monoclinic C2 (2) (twofold axis parallel to z) Cs (m) (mirror perpendicular to z) Orthorhombic C2v (mm2) (twofold axis parallel to z) D2 (222) Tetragonal C4 (4) S4 (4) D4 (422) C4v (4mm) D2d (42m) Hexagonal C6 (6) C3h (6) D6 (622) C6v (6mm) D3h (62m) (mirror perpendicular to x) Trigonal C3 (3)

Fig. 1.7.3.1. Field vectors of a plane wave propagating in an anisotropic medium. (X; Y; Z) is the wave frame. Z is along the direction of propagation, X and Y are contained in + and respectively, by an arbitrary convention.

In the linear regime, Pð!Þ ¼ "0 ð1Þ ð!ÞEð!Þ, where "0 is the free-space permittivity and (1)(!) is the ﬁrst-order electric susceptibility tensor. Then (1.7.3.1) becomes rxrxEð!Þ ¼ ð!2 =c2 Þ"ð!ÞEð!Þ:

Independent nonzero (2) elements under Kleinman symmetry xxx, xyy ¼ yxy ¼ yyx, xzz ¼ zxz ¼ zzx, xyz ¼ xzy ¼ yxz ¼ yzx ¼ zxy ¼ zyx, xxz ¼ xzx ¼ zxx, xxy ¼ xyx ¼ yxx, yyy, yzz ¼ zyz ¼ zzy, yyz ¼ yzy ¼ zyy, zzz

xyz ¼ xzy ¼ yxz ¼ yzx ¼ zxy ¼ zyx, xxz ¼ xzx ¼ zxx, yyz ¼ yzy ¼ zyy, zzz xxx, xyy ¼ yxy ¼ yyx, xzz ¼ zxz ¼ zzx, xxy ¼ xyx ¼ yxx, yyy, yzz ¼ zyz ¼ zzy

xzx ¼ xxz ¼ zxx, yyz ¼ yzy ¼ zyy, zzz xyz ¼ xzy ¼ yzx ¼ yxz ¼ zxy ¼ zyx xzx ¼ xxz ¼ zxx ¼ yzy ¼ yyz ¼ zyy, zzz xyz ¼ xzy ¼ yzx ¼ yzx ¼ zxy ¼ zyx, xzx ¼ xxz ¼ zxx ¼ yzy ¼ yyz ¼ zyy All elements are nil xzx ¼ xxz ¼ zxx ¼ yyz ¼ yzy ¼ zyy, zzz xyz ¼ xzy ¼ yzx ¼ yxz ¼ zxy ¼ zyx

xzx ¼ xxz ¼ zxx ¼ yyz ¼ yzy ¼ zyy, zzz xxx ¼ xyy ¼ yxy ¼ yyx, yyy ¼ yxx ¼ xyx ¼ xxy All elements are nil xzx ¼ xxz ¼ zxx ¼ yyz ¼ yzy ¼ zyy, zzz yyy ¼ yxx ¼ xxy ¼ xyx

case, "ð!Þ ¼ 1 þ ð1Þ ð!Þ is the dielectric tensor. In 0 the general 00 ð1Þ ð!Þ is a complex quantity i.e. ð1Þ ¼ ð1Þ þ ið1Þ . For the following, we consider a medium for which the losses are small 0 00 (ð1Þ ð1Þ ); it is one of the necessary characteristics of an efﬁcient nonlinear medium. In this case, the dielectric tensor is 0 real: " ¼ 1 þ ð1Þ . The plane wave is a solution of equation (1.7.3.2): Eð!; X; Y; ZÞ ¼ eð!ÞEð!; X; Y; ZÞ exp½ikð!ÞZ:

D3 (32) C3v (3m) (mirror perpendicular to x) Cubic T (23), Td (43m) O (432)

xyz ¼ xzy ¼ yzx ¼ yxz ¼ zxy ¼ zyx All elements are nil

ð1:7:3:3Þ

(X; Y; Z) is the orthonormal frame linked to the wave, where Z is along the direction of propagation. We consider a linearly polarized wave so that the unit vector e of the electric ﬁeld is real (e ¼ e ), contained in the XZ or YZ planes. Eð!; X; Y; ZÞ ¼ Að!; X; Y; ZÞ exp½ið!; ZÞ is the scalar complex amplitude of the electric ﬁeld where ð!; ZÞ is the phase, and E ð!; X; Y; ZÞ ¼ Eð!; X; Y; ZÞ. In the linear regime, the amplitude of the electric ﬁeld varies with Z only if there is absorption. k is the modulus of the wavevector, real in a lossless medium: þkZ corresponds to forward propagation along Z, and kZ to backward propagation. We consider that the plane wave propagates in an anisotropic medium, so there are two possible wavevectors, k+ and k, for a given direction of propagation of unit vector u: k ð!; ; ’Þ ¼ ð!=cÞn ð!; ; ’Þuð ; ’Þ:

xxx ¼ xyy ¼ yyx ¼ yxy, xzx ¼ xxz ¼ zxx ¼ yyz ¼ yzy ¼ zyy, yyy ¼ yxx ¼ xxy ¼ xyx, zzz xxx ¼ xyy ¼ yyx ¼ yxy yyy ¼ yxx ¼ xxy ¼ xyx, xzx ¼ xxz ¼ zxx ¼ yyz ¼ yzy ¼ zyy, zzz

ð1:7:3:2Þ

ð1:7:3:4Þ

( ; ’) are the spherical coordinates of the direction of the unit wavevector u in the optical frame; (x; y; z) is the optical frame deﬁned in Section 1.7.2. The spherical coordinates are related to the Cartesian coordinates (ux ; uy ; uz ) by ux ¼ cos ’ sin

186

uy ¼ sin ’ sin

uz ¼ cos :

ð1:7:3:5Þ

1.7. NONLINEAR OPTICAL PROPERTIES The refractive indices n ð!; ; ’Þ ¼ ½" ð!; ; ’Þ1=2, ðnþ > n Þ, real in the case of a lossless medium, are the two solutions of the Fresnel equation (Yao & Fahlen, 1984): 1=2 2 n ¼ B ðB2 4CÞ1=2 B ¼ u2x ðb þ cÞ u2y ða þ cÞ u2z ða þ bÞ

C ¼ u2x bc þ u2y ac þ u2z ab a ¼ n2 x ð!Þ;

b ¼ n2 y ð!Þ;

c ¼ n2 z ð!Þ: ð1:7:3:6Þ

nx(!), ny(!) and nz(!) are the principal refractive indices of the index ellipsoid at the circular frequency !. Equation (1.7.3.6) describes a double-sheeted three-dimensional surface: for a direction of propagation u the distances from the origin of the optical frame to the sheets (+) and () correspond to the roots n+ and n. This surface is called the index surface or the wavevector surface. The quantity (nþ n ) or (n nþ ) is the birefringency. The waves (+) and () have the phase velocities c=nþ and c=n , respectively. Equation (1.7.3.6) and its dispersion in frequency are often used in nonlinear optics, in particular for the calculation of the phase-matching directions which will be deﬁned later. In the regions of transparency of the crystal, the frequency law is well described by a Sellmeier equation, which is the case for normal dispersion where the refractive indices increase with frequency (Hadni, 1967): n ð!i Þ < n ð!j Þ for !i < !j :

ð1:7:3:7Þ

If !i or !j are near an absorption peak, even weak, n(!i) can be greater than n(!j); this is called abnormal dispersion. The dielectric displacements D, the electric ﬁelds E, the energy ﬂux given by the Poynting vector S ¼ E H and the collinear wavevectors k are coplanar and deﬁne the orthogonal vibration planes (Shuvalov, 1981). Because of anisotropy, k and S , and hence D and E , are non-collinear in the general case as shown in Fig. 1.7.3.1: the walk-off angles, also termed double-refraction angles, ¼ arccosðd e Þ ¼ arccosðu s Þ are different in the general case; d , e , u and s are the unit vectors associated with D , E , k and S , respectively. We shall see later that the efﬁciency of a nonlinear interaction is strongly conditioned by k, E and , which only depend on (1)(!), that is to say on the linear optical properties. The directions S+ and S are the directions normal to the sheets (+) and () of the index surface at the points n+ and n. For a plane wave, the time-average Poynting vector is (Yariv & Yeh, 2002) 1 S ð!Þ ¼ Re E ð!Þ H ð!Þ 2 k ð!Þ 1 E ð!Þ2 cos2 ð!Þ: ¼2 0 ! ð1:7:3:8Þ - !N , which is a power per unit area kS k is the energy ﬂow I ¼ h i.e. the intensity, where h! is the energy of the photon and N are the photons ﬂows. (!) is the angle between S and u; it is detailed later on. The unit electric ﬁeld vectors e+ and eare calculated from the propagation equation projected on the three axes of the optical

Table 1.7.2.4. Nonzero (3) coefﬁcients and equalities between them in the general case Symmetry class

(3) nonzero elements

Triclinic C1 (1), Ci (1)

All 81 elements are independent and nonzero

Monoclinic Cs (m), C2 (2), C2h m2 (twofold axis parallel to z)

xxxx, xyyy, xyzz, xzyz, xzzy, xxzz, xzxz, xzzx, xxyy, xyxy, xyyx, xxxy, xxyx, xyxx, yxxx, yyyy, yyzz, yzyz, yzzy, yxzz, yzxz, yzzx, yxyy, yyxy, yyyx, yxxy, yxyx, yyxx, zzzz, zyyz, zyzy, zzyy, zxxz, zxzx, zzxx, zxyz, zxzy, zyxz, zzxy, zyzx, zzyx

Orthorhombic C2v (mm2), D2 (222), D2h (mmm) (twofold axis parallel to z) Tetragonal C4 (4), C4h 4 S4 (4), m C4v (4mm), D2d (42m), D4 (422), D4h m4 mm Hexagonal C6 (6), C6h 6 C3h (6), m C6v (6mm), D3h (62m), D6 (622), D6h m6 mm Trigonal C3 (3), C3i (3)

C3v (3m), D3 (32), D3d (3m) (mirror perpendicular to x) (twofold axis parallel to x) Cubic T (23), Th (m3) O (432), Oh (m3m) Td (43m),

xxxx, xxzz, xzxz, xzzx, xxyy, xyxy, xyyx, yyyy, yyzz, yzyz, yzzy, yxxy, yxyx, yyxx, zzzz, zyyz, zyzy, zzyy, zxxz, zxzx, zzxx

xxxx ¼ yyyy, xyyy ¼ yxxx, xyzz ¼ yxzz, xzyz ¼ yzxz, xzzy ¼ yzzx, xxzz ¼ yyzz, xzxz ¼ yzyz, xzzx ¼ yzzy, xxyy ¼ yyxx, xyxy ¼ yxyx, xyyx ¼ yxxy, xxxy ¼ yyyx, xxyx ¼ yyxy, xyxx ¼ yxyy, zzzz, zyyz ¼ zxxz, zyzy ¼ zxzx, zzyy ¼ zzxx, zxyz ¼ zyxz, zxzy ¼ zyzx, zzxy ¼ zzyx xxxx ¼ yyyy, xxzz ¼ yyzz, xzxz ¼ yzyz, xzzx ¼ yzzy, xxyy ¼ yyxx, xyxy ¼ yxyx, xyyx ¼ yxxy, zzzz, zyyz ¼ zxxz, zyzy ¼ zxzx, zzyy ¼ zzxx

xxxx ¼ yyyy ¼ xxyy þ xyxy þ xyyx, xyyy ¼ xxxy þ xxyx þ xyxx ¼ yxxx, xyzz ¼ yxzz, xzyz ¼ yzxz, xzzy ¼ yzzx, xxzz ¼ yyzz, xzxz ¼ yzyz, xzzx ¼ yzzy, xxyy ¼ yyxx, xyxy ¼ yxyx, xyyx ¼ yxxy, xxxy ¼ yyyx, xxyx ¼ yyxy, xyxx ¼ yxyy, zzzz, zyyz ¼ zxxz, zyzy ¼ zxzx, zzyy ¼ zzxx, zxyz ¼ zyxz, zxzy ¼ zyzx, zzxy ¼ zzy